KINETICS IN MATERIALS SCIENCE AND ENGINEERING KINETICS IN MATERIALS SCIENCE AND ENGINEERING Dennis W. Readey University Emeritus Professor Colorado School of Mines, Golden, USA Boca Raton London New York CRC Press is an imprint of the Taylor & Francis Group, an informa business Cover Image: Courtesy of Jaehyung Lee. From “Vapor Phase Sintering of Hematite in HCl” (PhD Thesis. The Ohio State University, 1984). CRC Press Taylor & Francis Group 6000 Broken Sound Parkway NW, Suite 300 Boca Raton, FL 33487-2742 © 2017 by Taylor & Francis Group, LLC CRC Press is an imprint of Taylor & Francis Group, an Informa business No claim to original U.S. Government works Printed on acid-free paper Version Date: 20160830 International Standard Book Number-13: 978-1-4822-3566-1 (Pack - Book and Ebook) This book contains information obtained from authentic and highly regarded sources. Reasonable efforts have been made to publish reliable data and information, but the author and publisher cannot assume responsibility for the validity of all materials or the consequences of their use. The authors and publishers have attempted to trace the copyright holders of all material reproduced in this publication and apologize to copyright holders if permission to publish in this form has not been obtained. If any copyright material has not been acknowledged please write and let us know so we may rectify in any future reprint. Except as permitted under U.S. Copyright Law, no part of this book may be reprinted, reproduced, transmitted, or utilized in any form by any electronic, mechanical, or other means, now known or hereafter invented, including photocopying, microfilming, and recording, or in any information storage or retrieval system, without written permission from the publishers. For permission to photocopy or use material electronically from this work, please access www.copyright.com (http://www.copyright.com/) or contact the Copyright Clearance Center, Inc. (CCC), 222 Rosewood Drive, Danvers, MA 01923, 978-750-8400. CCC is a not-for-profit organization that provides licenses and registration for a variety of users. For organizations that have been granted a photocopy license by the CCC, a separate system of payment has been arranged. Trademark Notice: Product or corporate names may be trademarks or registered trademarks, and are used only for identification and explanation without intent to infringe. Library of Congress Cataloging-in-Publication Data Names: Readey, D. W., author. Title: Kinetics in materials science and engineering / Dennis W. Readey. Description: Boca Raton, FL : CRC Press, Taylor & Francis Group, [2016] | Includes bibliographical references and index. Identifiers: LCCN 2016018601| ISBN 9781482235661 (alk. paper) | ISBN 1482235668 (alk. paper) Subjects: LCSH: Materials science. | Chemical processes. | Dynamics. | Diffusion. Classification: LCC TA403.6 .R376 2016 | DDC 620.1/12--dc23 LC record available at https://lccn.loc.gov/2016018601 Visit the Taylor & Francis Web site at http://www.taylorandfrancis.com and the CRC Press Web site at http://www.crcpress.com To my wife Suzann for her encouragement and patience Contents Preface . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . ix For the Instructor . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . xiii For the Student . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . xvii Acknowledgments . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . xxi Author . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . xxiii Section i — introduction to Kinetics Chapter 1. Kinetics and Materials Science and Engineering . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3 Section ii — Reaction Kinetics Chapter 2. Introduction to Kinetic Processes in Materials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 41 Chapter 3. Second-Order and Multistep Reactions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 61 Chapter 4. Temperature Dependence of the Reaction Rate Constant . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .95 Chapter 5. Heterogeneous Reactions: Gas–Solid Reactions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 111 Section iii — Phase transformations Chapter 6. Thermodynamics of Surfaces and Interfaces and Some Consequences . . . . . . . . . . . . . . . . . . . . .153 Chapter 7. Phase Transitions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .195 vii viii Kinetics in Materials Science and Engineering Section iV — Diffusion with a constant Diffusion coefficient Chapter 8. Fundamentals of Diffusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .257 Chapter 9. Atomistics of Diffusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .275 Chapter 10. Steady-State Diffusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .333 Chapter 11. Solutions to Fick’s Second Law: Infinite and Semi-Infinite Boundary Conditions . . . . . . . . . . . . .381 Chapter 12. Diffusion with Finite Boundary Conditions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 413 Section V — Fluxes, Forces, and interdiffusion Chapter 13. Fluxes, Forces, and Diffusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .447 Chapter 14. Interdiffusion and Metals . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .479 Chapter 15. Interdiffusion in Compounds . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .519 Chapter 16. Spinodal Decomposition Revisited . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .563 Appendix I: List of Symbols . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .591 Appendix II: Constants . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .599 Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .601 Preface T his book is intended to be an undergraduate text for junior- and senior-level students majoring in materials science and engineering (MSE). Most MSE undergraduate programs have a one-semester kinetics course in their curricula that has taken the place of a classical physical chemistry course and one or more courses on materials processing. This book is not intended to be a reference work that summarizes and evaluates all of the reactions and phase transformations of importance in MSE, although some unique topics are presented. Given the breadth of the field today—metals, ceramics, electronic materials, polymers, biomaterials, and composites—it is not feasible to cover all of kinetics. Nevertheless, the book does cover considerably more material than can be covered in a one-semester course and includes approaches and topics that are rarely found elsewhere that might be useful to graduate students, researchers, and industrial practitioners. One goal of this book is to incorporate important concepts that all students in MSE should be exposed to at some point in their careers based on the author’s personal experience as a student, researcher, practicing engineer, and instructor over a number of years. The primary goal is to develop simple mathematical models, involving process variables such as temperature, pressure, composition, and time, to provide a fundamental model-based understanding of commercially important materials processes critical to the development, fabrication, and application of materials. In doing so, at the expense of additional equations, most of the mathematical steps necessary to develop a model are explicitly presented so the student, or reader, can follow the text without the absolute necessity of an instructor for interpretation and insertion of the missing steps—frequently the case in many textbooks. This, of course, means more pages to cover a given topic. WHY THIS BOOK There are several reasons why this book was written. First, there is limited textual material for the junior/ senior-level general courses in MSE. There are many introduction to materials, or similarly named, textbooks. Most of these texts do not cover the different types of materials equitably, usually reflecting the author’s understandable partiality to a specific material type based on his or her own experience and interests. Unapologetically, some partiality will be found here as well. More importantly, virtually none of introductory texts present kinetics in sufficient depth to be of use in an upper level course. Also, many texts approach important kinetic topics with a black box or “…it can be shown that…” methodology. For example, most introductory texts have sections on solid state diffusion and they tell you that carbon diffuses into steel, and its concentration, C, as a function of distance, x, and time, t, is given by x C = Cs erfc 4Dt ix x Kinetics in Materials Science and Engineering where: CS is the surface concentration D is the diffusion coefficient It is hard to imagine a more opaque black box than “erfc(y)”: What is it? Where does it come from? An MSE student should know where it comes from before completing an undergraduate program. This book shows explicitly how to get this result with no more than introductory calculus and serves as an example of one of the several kinetic concepts an undergraduate MSE student should be exposed to before entering the materials profession as a research scientist or practicing engineer. Second, MSE programs today incorporate instruction on metals, ceramics, polymers, electronic materials, biomaterials, and composites, all with varying degrees of emphasis. Yet, as discussed in the Chapter 1, most of these programs were, at one point in their history, focused only on metals and called metallurgy or metallurgical engineering. Today, materials are often separated into hard materials and soft materials, the latter including polymers and biomaterials. Biomaterials can be further subdivided into bioreplacement materials—scaffolds and implants—and the study of actual biological materials processes such as bone growth. In one of the author’s teaching experiences, with about 100 MSE students taking the kinetics course, over 50% were interested in soft materials. Fifty years ago, all of the students in this particular program would have been interested only in metals, but not today. This change in interests illustrates the need for exposure to a new and broader range of kinetic processes involving all types of materials used today. Third, most kinetic processes in materials usually have several possible steps operating in series or in parallel controlled either by material transport (diffusion) or by an actual chemical reaction; for example, the deposition of silicon films from a gas. For hard materials, reactions usually take place at elevated temperatures and are often diffusion controlled. In contrast, reactions in soft materials occur at low temperatures, and a chemical reaction is usually more important. With the growing importance and interest in soft materials—with a significant interest overlap with chemistry, physics, chemical, and bioengineering— inclusion of chemical reaction kinetics in an MSE course is crucial. This text tries to accomplish this as well as brief digression into nuclear chemistry as an example of ideal kinetics. This typically serves as a first exposure to nuclear chemistry to over 80% of the students in spite of its importance. Every MSE major needs some exposure to nuclear reactions given the importance of materials in nuclear power, nuclear waste disposal, nuclear medicine, and other uses of isotopes. Finally, for virtually all of the kinetic models developed, where possible, examples of real industrial processes are presented to demonstrate the applicability of the models. HOW THIS BOOK DEVELOPED This book is a textbook on the modeling of kinetic processes for undergraduates majoring in MSE and similar programs. It grew from notes acquired over 30 years of teaching such a course in materials programs at three different academic institutions, each having different student primary interests and faculty research specialties: ceramics, metals, and polymers. The objective is to provide material for a one-semester course (probably two) on kinetics based on the backgrounds expected of juniors and seniors (and some graduate students) in undergraduate programs. This is not a book on computational materials science. Computational materials science is an important and growing field in materials research but typically involves the use of mathematical or computational techniques that better serve graduate students. This book is also not an extensive review of the original literature. In fact, every effort is made to summarize material that already exists in some form in another text or publication. Similarly, this is not a physics or chemistry text. In reality, some of the approximations made to models will make physicists, chemists, mathematicians, and probably even some materials scientists, cringe! Nevertheless, where approximations appear, they are intended to make the development of a kinetic model more transparent so that the final— and correct—result is not lost in the details. No single text exists that treats kinetic topics for materials at an introductory, junior–senior level and accomplishes two important goals: (1) goes more deeply into a Preface topic than an introductory materials text does and (2) equitably covers all materials. Although there are many excellent books on chemical kinetics, details of diffusion mechanisms, and solutions to diffusion equations at an advanced level, they are usually focused on a single class of material: metals, ceramics, polymers, semiconductors,* and so on. Today, a student needs exposure to all materials with the emphasis on areas of commonality. That is why MSE exists: commonality in the processing, structure, and properties among materials. In this book, an effort is made to include topics and examples for both hard and soft materials because each MSE program has different student and faculty interests. However, for soft materials such as polymers, it is more challenging to easily find commonality with the kinetics of processing of hard materials. The reason for this is probably twofold. First, the useful temperature range for polymers is only a few hundred degrees centigrade, whereas hard materials processing covers a range of over 3000°C. Second, the microstructure of hard materials can be varied greatly, largely controlled by kinetic processes at elevated temperatures, the main factor determining properties. This is why steels are heat-treated! In contrast, it is the chemistry, length, and entanglement or cross-linking of polymer molecules that have the largest influence on polymer properties. The greater parts of such topics are more appropriate to a chemistry course. THE TARGET AUDIENCE Today, there are about 60–70 accredited undergraduate MSE programs that graduate about 1200 students a year. In addition, there are many chemistry, physics, and engineering programs that have a strong materials orientation or undergraduate option. In the author’s experience, many MSE graduate students do not have an MSE undergraduate background and take an undergraduate course, such as kinetics, to become more familiar with MSE topics and terminology. Also, both undergraduate and graduate students from other departments frequently take such a course to gain information about various topics; for example, nuclear engineers need to understand diffusion of neutrons in reactors. The book is not primarily intended as a reference for a practicing engineer or researcher but certainly should be useful to them as a refresher on specific topical areas and introduction to other topics not usually found elsewhere. Please also refer to the sections “For the Instructor” and “For the Student” following this preface. This book assumes that a student has had a chemical thermodynamics course and an introductory materials course as prerequisites. A mathematical background no higher than a second or third calculus course is all that is required, and a prior course differential equations is not necessary. HOW THE BOOK IS ORGANIZED The general organization of this book is to present essentially classical chemical reaction kinetics first. Then nucleation and growth phase transitions are presented with control by a chemical reaction rather than by diffusion or transport. Prior to this, a chapter on the surface energy and its effects is offered first because not all students have seen surface energy effects in thermodynamics or chemistry courses. Then diffusion with a constant diffusion coefficient is presented. In the “Table of Contents,” the atomistics of diffusion are listed before the solutions to the equations of diffusion. However, this material can be presented the other way around without any loss in continuity. The last section focuses on interdiffusion and more complex geometries. The final chapter is on the kinetics of spinodal decomposition presented with a * Including semiconductors as a type of material is really comparing apples and oranges because semiconduction—implying that a material is neither metallic nor insulating—is possible in many different materials other than those used to make integrated circuits and light-emitting diodes. Semiconduction really implies a range of values for the conductivity and not a type of material. For example, ionic semiconductors are critical for battery and fuel cell applications even though they conduct ions and not electrons. To generalize, there are really only two classes of materials, metals and others. Metals have free electrons at absolute zero kelvin—the metallic bond—and all other materials require energy to create free electrons by knocking them out of chemical bonds. If this does not take much energy, the material is a semiconductor: if it takes a lot of energy it is an insulator. xi xii Kinetics in Materials Science and Engineering different approach but hopefully a more transparent one for an undergraduate student. So, the organization of the book is, progressing from simpler concepts to more complex ones, as follows: 1. 2. 3. 4. 5. Introduction to Materials Kinetics Reaction Kinetics Phase Transformations Diffusion with a Constant Diffusion Coefficient Fluxes and Forces and Interdiffusion SUMMARIZING THE MAIN FEATURES OF THIS BOOK The book is intended to be a junior- to senior-level text for majors in MSE. As such, its main features are as follows: ª ª ª ª ª ª ª ª ª ª ª ª Goes beyond the introductory level for MSE students Covers topics of interest in all subfields of materials: metals, polymers, and so on Addresses kinetics of reactions important for soft materials such as polymers and biomaterials Gives real examples of industrial processes and materials used wherever possible Discusses both the atomistic and macroscopic aspects of diffusion in solids, liquids, and gases Focuses on understanding rather than mathematical rigor, still yielding correct results Avoids black boxes or equations that magically appear Explicitly presents intermediate steps in solving equations, allowing for self-study Presents all topics with real materials processes in which the results are—or should be—applied in actual industrial practice Includes problems for each chapter with the intent of not being practice for the student but providing the opportunity to quantify the results of the chapter Discusses real processes in a way that shows how the various different serial or parallel steps can be controlled to give different results for the same overall process Addresses unique topics such as similarity variable solutions to the partial differential equations of diffusion; simple derivation of the Boltzmann distribution; correct point defect chemistry including the Kröger–Vink notation; the glass transition as a relaxation process; the Kirkendall effect both in metals and compounds; compound formation; a more direct approach to spinodal decomposition Dennis W. Readey For the Instructor T his book assumes that students have taken courses on introduction to materials, chemical thermodynamics, and one, two, or three courses in calculus but not differential equations or a higher level engineering mathematics course. Since most students come out of a first thermodynamics course with less than a strong grasp of the topic, thermodynamics and phase equilibria are emphasized wherever possible. Most kinetic models presume an understanding of the thermodynamics of the process. The thermodynamics are explicitly discussed to reinforce the students’ understanding of both kinetics and thermodynamics. Many topics involve solving ordinary or partial differential equations. However, a course on differential equations is not a prerequisite because most of the equations can be easily solved, usually by separation of variables, so a second calculus course is sufficient. Nevertheless, at the junior level, many students have either taken, or are taking, differential equations and should be familiar with most of the mathematical manipulations with the possible exception of solutions of partial differential equations. But here again, the relevant equations are solved with no requirements beyond those in a second calculus course. The emphasis is on understanding where equations come from rather than on mathematically rigorous derivations—although simple algebraic manipulation to develop a model is often considered a derivation to many students. As a result, a plausibility argument is sometimes used to obtain an expression or solve an equation; a procedure quite unsatisfactory to a mathematician or physicist, although the final result can be correct. There are many equations in the text. The reason for this is simply to provide all of the individual steps going from a starting equation to the desired result, so the student (or instructor) does not need several sheets of paper to do the calculations between the beginning and end of a model. This has the advantage that a student can follow the development step by step: nothing is hidden. If the algebra or calculus involves too many steps, they are included in an appendix to not impede the flow of the discussion. Students should have had a course on chemical thermodynamics including phase diagrams and Gibbs energy-composition diagrams. There is a brief review in Chapter 1 of the essentials of thermodynamics that are important in later chapters in this book. Examples of Gibbs energy-composition diagrams and the relation to phase diagrams are given in Chapter 1. A chapter on surfaces is included and a lot of details on the correct way to do point defect chemistry in solids are also presented. These topics may have been covered in a prior thermodynamics course but often they are not, yet are crucial for understanding kinetic processes in materials. Also, it is assumed that most students have not had courses on heat transfer or fluid dynamics as most MSE programs do not require these. However, programs whose focus is on extractive or chemical processing might consider these topics essential in a kinetics course, but they are not covered in detail here. This book is on the modeling of kinetic processes important in MSE. In the distant past when MSE programs were mainly metallurgical or ceramic engineering, each program would provide courses very xiii xiv Kinetics in Materials Science and Engineering specific to the discipline such as heat treatment of steels or powder processing. The combined influences of decreases in program credit hours mandated by universities and MSE program inclusion of all materials have either eliminated such specific courses or relegated them to areas of specialization within a program. There is a great deal of commonality among materials linking structure and properties. However, the processing of each type of material—metals, ceramics, polymers, biomaterials, and semiconductors—has its own unique focus, yet most of these courses disappeared when MSE programs came into existence. It has fallen to courses such as kinetics to be sufficiently broad to fill this lack of processing fundamentals dedicated to individual materials. However, it is challenging to make a course such as kinetics, whose focus is processing, sufficiently inclusive to satisfy the details required for each material. Therefore, principles that apply to all or most materials are emphasized but with the caveat that the temperature ranges—and the importance of temperature—for the processing and performance of metals, ceramics, and semiconductor materials are much larger than for polymers and biomaterials. The main reason for this is that most kinetic processes involved in microstructural changes in hard materials are controlled by diffusion rather than a chemical reaction. In contrast, for polymers and biomaterials, reactions, of necessity, must occur at low temperatures and are controlled by the atomic details of the reaction process. Each of these two areas, diffusion and reaction chemistry, can easily fill more than a semester’s worth of kinetics individually, so not all details of each can be easily covered in a single course. Nevertheless, attempts are made to cover kinetic processes that are important for the processing of materials both at high and low temperatures. The primary goal is to develop models for various kinetic processes so that the rates of reactions can be explicitly written as a function of the process variables; for example, rate = f (temperature, time, pressure, concentration, etc.) where the rate is determined by the rate-controlling step, which is one of many possible steps in the overall process. In most cases, the rate equations developed are macroscopic in that the relationship between a variable such as temperature and the underlying detailed atomistic mechanism may not be obvious. This is simply because the details of the atomic mechanism are not completely known, that there are just too many possible mechanisms to investigate in detail, or the level of detail—quantum mechanics for example—is beyond the typical background of MSE students at this level. Nevertheless, the goal is to develop fundamentals-based models that can be—and are—used for the control of real materials processing and the understanding of real materials behavior. The one exception to the more macroscopic approach is the development of atomistic or molecular models of diffusion* in solids, gases, and liquids. For example, it is shown that the diffusion coefficient in solids, D, in Fick’s first law, J = −D(dC /dx), where J = flux and Units(J) = mol/cm2-s† and C = concentration with Units(C) = mol/cm3, depends on temperature as D = D0exp(−Q/RT), where D0 and Q come from for diffusion in different materials. In introductory materials texts, solutions to Fick’s second law, ∂C /∂t = D(∂ 2C /∂x 2 ), such as diffusion into a solid with a fixed surface concentration C = CSerfc x 4Dt are presented, and students are urged to make calculations of concentration as a function of time and distance with this black box without showing where the black box comes from. For many students, black boxes impede further learning. A major justification for this book is to go beyond introductory texts and to show where expressions such as this come from, that is, how to solve the partial differential equation of Fick’s second law. To do this with complete mathematical rigor frequently goes beyond the mathematical experience and maturity of students in junior–senior classes. Here, mathematical rigor and exact expressions are often sacrificed for more transparent approaches that use plausibility arguments, lead to correct solutions, and, hopefully, a better understanding of the fundamental concepts. Several areas of kinetics important to materials processing are not included. Some of these are: solidification, sintering, grain growth, grain boundary grooving, polymer swelling, interface instability, electron exchange and electrochemical kinetics, and broader coverage of point defect chemistry. There are several reasons for this. One is that some of the topics are too specific to one type of material than for others: solidification and metals; sintering and ceramics; point defect chemistry and electronic materials; and ( ) * Note that diffusion is defined as the spontaneous intermingling or mixing of atoms, ions, molecules, or particles due to random thermal motion. † Note that Units(Q) is used in this book to denote the units of Q. For the Instructor swelling and polymers. Another reason is that some topics are best left to graduate courses such as interface instability. Not everything in this book can be covered in a single semester even with the exclusion of these additional topics: choices had to be made. Nevertheless, a few topics such as some nuclear chemistry and ionic conductivity are included simply because MSE students today are probably not exposed to these topics elsewhere but are essential to an undergraduate’s education. In reality, major parts of Chapters 2 through 12 can be reasonably completed in a typical semester. The introductory chapter (Chapter 1), Chapter 6 on surfaces, and the discussions of nuclear chemistry and point defect chemistry could be shortened or not covered at all if covered in other courses. Similarly, parts of Chapters 13 through 16 can be included depending on students’ backgrounds and the intent of the course. Based on the experience of teaching materials kinetics over many years, there is sufficient material to cover two semesters if all the chapters were to be covered completely. Of course, the sequence of presentation of the various topics certainly does not have to follow the order in the “Table of Contents.” For example, atomistics of diffusion is listed before solutions to diffusion equations. However, the information can be presented in the opposite order just as well without loss in continuity. xv For the Student T his book does not focus on materials science exclusively with the assumption that all engineering students will become materials graduate students, so a deeper background is needed. In most MSE programs, only about half the undergraduates go into graduate programs—and many of these are not in MSE—the rest take jobs in industry with the bachelor’s degree being the terminal degree, at least for now. As a result, in this book, engineering or practical applications are emphasized where possible with the philosophy that the development of model-based kinetic processes are those actually used to make or understand real materials and processes. If an engineer knows why variables affect a process in a certain way, then when the process is not working right, the engineer can adjust the variables to make the process perform the way it was designed, eliminating expensive and time-consuming trial and error procedures. Modeling of kinetic processes involves mathematics, mostly algebra and a little calculus. The intent here is to provide the correct solutions to kinetic problems without relying on students’ mathematical exposure beyond the second or third semester of calculus. Although kinetics requires the solution of differential equations, most of these can be solved by integration techniques learned in elementary calculus precluding the need for a formal background in differential equations. Also, black boxes, such as “…it can be shown that…,” and other impediments to understanding are largely eliminated. Integrations and intermediate algebraic manipulations are performed step-by-step so that a student can follow the development of a model without the need for working out the intermediate steps with a pencil and paper. Unfortunately, this leads to more lines of equations in the text, but going from one equation to the next requires only a small and easily identified algebraic or calculus step. There are several things unique about this book. For example, the solution to kinetic processes that go to equilibrium and involve second or higher order forward or back reactions is typically not seen in texts where reaction kinetics are covered. Similarly, the solution for series reactions is usually just given and not modeled. Doing this requires a little more advanced differential equation solving, so it is presented as part of an appendix. The correct way to do point defect chemistry is presented, although most texts and published papers do it incorrectly often because the simpler, albeit incorrect, methodology has been passed down from one generation of academics to the next over the past 50 years! Yet the correct version is, in fact, more straightforward once charged species are accounted for and charge neutrality is maintained in the analysis. A free-volume model of the glass transition is presented that shows that it involves a double exponential with temperature and explains the relative sharpness of the transition. A model for interdiffusion in compounds demonstrates the possibility, although small, for a Kirkendall effect during interdiffusion of compounds that is not available in many other texts. Formation of ternary compounds by diffusion is presented in detail, and the model follows directly from the electrical charge neutrality required of the ion xvii xviii Kinetics in Materials Science and Engineering fluxes. Finally, the approach to modeling kinetics of spinodal decomposition is different from the methods generally used and, hopefully, is more direct and plausible to the average undergraduate. MATHEMATICS This book is on developing quantitative models of kinetic processes in MSE.* Since this book is intended as a textbook for a course on kinetics for juniors or seniors in MSE programs, it is assumed that the students will have had two or three semesters of calculus but may or may not have had a course on differential equations. The starting point for a model of a kinetic process is the rate at which a given process takes place, for example, moles per second, dn/dt. However, what is usually the goal of the model is the amount—the number of moles, n—as a function of time and other process variables such as composition, temperature, pressure, and perhaps other parameters. This implies integration of the rate equation or solving the differential equation, dn/dt. The solutions to both linear and relevant partial differential equations are obtained in this book. But fear not! For most of the differential equations of interest, the variables can be separated, so techniques learned in elementary calculus can be used to integrate both sides of the equation to get the desired result. There are a couple of exceptions to this general principle, but these are relegated to appendices in order to not disrupt the flow of model development. These are not major compromises because even some of the more rigorous developments are still approximations as not all structure and properties of real materials can be easily modeled: this is a main motivation of computational materials science. For example, the atomistic aspects of diffusion coefficients for gases can be easily and accurately modeled assuming that the atoms are hard spheres. But things get more complicated when the molecules are not spheres, have dipole moments, and so on—typical of real gases. Furthermore, in most cases, particularly for solids, even though the fundamental principles are understood, the uncertainty in the empirically measured values—D0 and Q in the diffusion coefficient, for example—far exceeds the limits of the model approximations! Therefore, developing an understanding of the fundamentals—both macroscopic and microscopic—and their relationships is the goal of this book rather than detailed theoretical models that explain everything exactly. Nevertheless, every effort is made to focus on phenomena of broad application to all classes of materials. UNITS, GRAPHS, AND PLOTS SI units are the preferred units in science today, and they are used in this book where appropriate. However, in many cases, they are not. The use of meters and kilograms rather than centimeters and grams frequently gives numbers that are cumbersome, unfamiliar, and of little use. For example, the densities of most polymers are in the range of 1 g/cm3. To say that the density of a polyethylene is 103 kg/m3 seems unrealistic unless you are working with cubic meters of material. Certainly in the laboratory and in most technological applications, the quantities dealt with are grams and cm3 rather than 103 kg and m3. Exceptions exist when dealing with commodity products such as corn, steel ingots, output of cement kilns, or production facilities for raw polyethylene. Then tonnes (a metric ton = 1000 kg) and cubic meters might be appropriate. Therefore, in this book, SI and CGS units (and sometimes English units) are used arbitrarily depending on what the circumstances warrant. Nevertheless, it is important to be able to recognize what units are required for a given parameter in an equation or formula to make its units consistent with all the other terms in the equation. The ability to be able to do dimensional analysis is crucial. In the 1970s, the United States after years of effort—going back to the founding of the country—made a serious effort to adopt the metric system.† However, it gave up trying in 1982 when the United States Metric Board was abolished by President Reagan after a great deal of popular resistance against the change to a metric system. This led to the rejoicing of many newspapers and commentators on the benefits of our way of doing things, the American Way! However, with the growth of globalization since the 1970s, * It is worthwhile to note that the development of a mathematical model is not “a derivation.” Derivations are things that mathematicians do! † Marciano, John Bemelmans. 2014. Whatever Happened to the Metric System? New York: Bloomsbury. For the Student metric measurements and components have universally appeared so that your toolbox needs sets of both metric and English wrenches. Certainly, there are many industries in the United States that still operate their ovens and furnaces in degrees Fahrenheit, their pressure vessels in pounds per square inch, and use dimensions in mils,* inches, or feet. So a scientist or engineer needs to be able to quickly, and correctly, convert between English and metric units. This ability is emphasized in several of the exercises at the end of each chapter and in the text to highlight this reality. However, today, conversion is easy: all you have to do is ask your cellphone, tablet, or computer to make the conversion for you. He, she, or it will tell you that one bushel = 0.03524 m3, important for farmers because corn and soybeans are sold by the bushel and crop yields are given in bushels/acre and one acre = 4046.86 m2. Also, cement, for which it might make sense to report the density in kg/m3, in the United States is sold by the cubic yard, or more concisely by the yard. One cubic yard = 0.7646 m3. Since about one-half of BS MSE graduates go into industry, they need to be able to quickly convert between different units and no apology is given for not strictly adhering to SI units in this book. Many of the calculated graphs and plots include the calculated data points in the graphs. The reason for this is threefold. First, it shows the independent variable values that were used to calculate the graphs. Second, the density of these points along a plot gives some indication of the number of points needed to provide a smooth plot over the data range of interest. Third, and perhaps most important, it gives the student some idea of how a graph should be constructed in terms of proportion, type fonts, line widths, and so on. Before the days of computer-generated graphs, most engineering students were required to take a course in engineering drawing or descriptive geometry and be able to generate detailed drawings with multiple views and dimensions from which parts were fabricated in the machine shop and joined on the floor of a factory. In such courses, there were strict rules about line widths, line styles, text fonts—very limited since they were hand-drawn—and their sizes relative to locations on the drawing. So a student became familiar with the generally accepted graphical methods to display technical information. This is no longer the case: courses in engineering graphics are not required and students are frequently not exposed to readily available computer graphing software. In the exercises at the end of most of the chapters in this book, there are requirements for plotting data to give practice in generating publication quality illustrations that computer graphing software can provide. Hand-drawn curves in the digital age are not acceptable for future engineers and scientists. For most of the graphs in this book, the data points were first calculated with spreadsheet software—frequently having powerful computation capability—and then data transferred to graphics software for plotting. * 1 mil = 0.001 in. xix Acknowledgments I thank my son, Dr. Michael Readey, for taking time to proofread the final draft of the manuscript for this book while he spent his days as the president of a renewable energy technology company and evenings teaching engineering management at the University of Colorado, Boulder, where he is now a full-time professor. His careful reading has corrected many of my mistakes and any remaining errors are still mine. Also, his background in materials science and engineering gave him the ability to make many useful changes and suggestions to improve the clarity and accuracy of the text. I also thank Luna Han and Judith Simon at Taylor & Francis for their patience during the time it actually took to complete this book: about twice as long as anticipated. Finally, the publisher and I acknowledge and thank the reviewers of the original manuscript for their constructive suggestions during the development process that have helped to improve the final text. xxi Author Dennis W. Readey is university emeritus professor of metallurgical and materials engineering at the Colorado School of Mines, Golden CO where he served as the H. F. Coors distinguished professor of ceramic engineering and director of the Colorado Center for Advanced Ceramics for 17 years. Prior to that, he served as chairman of the Department of Ceramic Engineering at Ohio State University Columbus, OH. He has been performing research on kinetic processes in materials for almost 50 years and teaching the subject for over 30 years. Before entering academia, he was a program manager in the Division of Physical Research of what is now the Department of Energy, where he was responsible for funding materials research in universities and national laboratories. Earlier, he was also a group leader in the Research Division of the Raytheon Company and in the Materials Division of Argonne National Laboratory. For the last eight years he has been an adjunct professor in MSE at the University of Illinois, Urbana–Champaign. He had been active in the Accreditation Board for Engineering and Technology (ABET) for a number of years representing TMS (The Mining, Minerals, and Materials Society) and served on several government committees including the Space Sciences Board and the National Materials Advisory Board of the National Academy of Sciences. He is a member of several professional societies and is a fellow of ASM International (formerly the American Society of Metals) and a fellow, distinguished life member, and pastpresident of the American Ceramic Society. Dr. Readey’s research has involved gaseous and aqueous corrosion of ceramics, the effect of atmospheres on sintering, the properties of porous ceramics, processing and properties of ceramic–metal composites, and the electronic properties of compounds, particularly transparent conducting oxides and microwave and infrared materials. He advised 29 PhD and 42 MS degree theses, which generated about 120 publications and 13 patents. He received a BS degree in metallurgical engineering from the University of Notre Dame, Notre Dame, IN, and a ScD degree in ceramic engineering from MIT, Cambridge, MA. xxiii Section I Introduction to Kinetics Chapter 1 Kinetics and Materials Science and Engineering 1 3 1 Kinetics and Materials Science and Engineering 1.1 Introduction 1.2 Materials Science and Engineering 1.3 Historical Development of MSE as a Discipline 1.4 Impact of MSE 1.5 Microstructure 1.6 Thermodynamics Review 1.6.1 A Difficult Subject 1.6.2 History of Thermodynamics 1.6.2.1 Relation to MSE 1.6.2.2 Why Thermodynamics Is Difficult 1.6.2.3 Significant Events in the Development of Thermodynamics 1.7 Review of Thermodynamic Concepts 1.7.1 Purpose 1.7.2 Four Laws of Thermodynamics 1.7.3 First Law of Thermodynamics 1.7.4 Second Law of Thermodynamics 1.7.5 Helmholtz and Gibbs Energies 1.7.6 Reactions and Equilibrium Constants 1.7.6.1 Equilibrium 1.7.6.2 Standard States and Equilibrium Constants 1.7.6.3 Gibbs Energy as a Function of Temperature 3 4 4 6 8 8 9 9 10 10 10 11 13 13 13 14 16 17 18 18 18 20 4 Chapter 1. Kinetics and Materials Science and Engineering 1.7.7 Multicomponent Systems 1.7.7.1 Introduction 1.7.7.2 Partial Molar Quantities 1.7.7.3 Chemical Potential and Partial Molar Gibbs Energy 1.7.7.4 Gibbs–Duhem Relation 1.7.7.5 Solutions 1.7.8 Phase Rule and Phase Diagrams 1.7.8.1 Phase Rule 1.7.8.2 Phase Diagrams 1.7.8.3 Single Component System 1.7.8.4 Two-Component System 1.7.8.5 Phase Diagrams and Gibbs Energy-Composition Diagrams 1.8 Chapter Summary Appendix Exercises References 1.1 22 22 22 24 25 25 26 26 27 27 28 29 32 32 35 37 INTRODUCTION This book is about kinetic processes in materials, and as such, it deals with how fast reactions such as phase transitions occur in materials and is intended as a text for junior-senior level students in undergraduate materials science and engineering (MSE) programs. Included in the scope of materials kinetics are shape changes driven by surface energies and compositional changes driven by concentration gradients. The first question is, “Where does kinetics—and the kinetics topics covered in this book—fit into the broad field of MSE?” Introducing a little modern history of MSE is useful in answering this question, so the first part of this chapter deals with some MSE history. Before approaching the kinetics of a process, the thermodynamics of the system undergoing change needs to be understood since it is the thermodynamics that drives the direction of the process. It is assumed that readers of this book will have had at least an introductory course in thermodynamics. However, rarely does anyone get a firm grasp on thermodynamic concepts the first time exposed to them. Therefore, the second part of this introductory chapter is a summary of some important thermodynamic principles. Clearly, not everything included in a first course on chemical thermodynamics can be presented in detail here, since there would not be room to discuss kinetics if it were. Therefore, only several of the principles used in later models of kinetic processes are briefly summarized. 1.2 MATERIALS SCIENCE AND ENGINEERING Frequently, textbooks give the impression that a field of science or engineering suddenly appeared as presented in the text. Of course, this is a completely false impression. Since the field of MSE is relatively new as a separate academic discipline, it is instructive to take some time to review what the field is about, how it got here, and what its main goals are. This is particularly true of MSE because of the breadth of its scope and diversity of its ancestral history. MSE consists of understanding the relationships between the processing, structure, and properties of materials (Figure 1.1). Many MSE practitioners add performance as the fourth corner of a materials tetrahedron, but this makes the relationships hard to draw in two dimensions—properties really determine performance anyway, and it usually the goal of the materials engineer to provide a material 1.2 Materials Science and Engineering Materials science and engineering Structure • Atomic • Electronic • Crystal • Microstructure - Phases - Distribution - Size Processing • Raw materials • Compounding • Shaping • Heat treatment • Finishing Properties • Mechanical • Thermal • Chemical • Electrical • Dielectric • Magnetic • Optical FIGURE 1.1 Illustration of the relationships between the three key areas of materials science and engineering: processing, structure, and properties. Kinetics focuses more on the processing part of these relationships but also includes chemical properties such as corrosion, dissolution, and oxidation. with a specific set of properties to achieve the required performance of a complex system such as jet turbine or an integrated circuit. More will be said about this later. Some items listed under structure in Figure 1.1 need more clarification. The atomic part of structure here really means the composition of the material in terms of what atoms or ions are present and their relative amounts. The electronic structure includes both the type and strength of chemical bonding in a material since they both play important roles in determining properties, such as electrical conductivity. The crystal structure, or lack of one, has large effects on most of the properties of interest. Finally, the microstructure is one of three concepts central to MSE that justify its existence as a separate discipline. The other two are crystal structure and phase equilibria (Cahn 2001). Included in the microstructure are the phases present: how many, their compositions, crystal structures—or lack thereof, that is, glasses—their distribution and sizes. For example, small amounts (a few percent) of low melting point second phases segregated to, and covering, the grain boundaries of materials that are mainly crystalline—metals, inorganic compounds, and polymers—can significantly alter the properties of these materials. In contrast, if the second phase were isolated into discontinuous pockets in a material, it may have little or no effect on properties. The science part of MSE has to do with understanding the fundamental principles involved in the relationships between processing, structure, and properties and the engineering part is applying these principles to make something useful. For example, Figure 1.2 is focused on a ceramic material—a ceramic being defined as “something useful made from one or more Compounded powder Controlled microstructure 2 μm 10 μm 2 μm Heat treatment, densification FIGURE 1.2 Relationship between the starting material, heat-treatment (densification), and the final microstructure. The example is yttrium iron garnet, Y3Fe5O12, a single-phase magnetic material containing several chemical additives to control the final magnetic properties for microwave applications. 5 6 Chapter 1. Kinetics and Materials Science and Engineering inorganic compounds”—simply as an illustration. Figure 1.2 shows the typical processing of a ceramic material beginning with powder particles that are formed into some shape. The part is then fired or heat-treated at some high temperature, so that the surface energy associated with the small particles (top left) drives mass transport by diffusion that bonds the particles together (center), produces shrinkage, and eliminates most of the porosity (which starts at about 45 volume percent) to form a dense polycrystalline material (top right). This is a photomicrograph of a magnetic ceramic based on yttrium iron garnet (YIG), Y3Fe5O12 . This is an important material in microwave applications because it is both an electrical insulator, thus transparent to microwave radiation, and magnetic, so the microwaves can interact with the magnetization of the material. By changing the magnetization, the index of refraction to microwaves is changed, which allows the electrical engineer to make interesting devices such as an electronically scanned radar. This particular material is actually a single phase solid solution oxide alloy with a composition Y3-x-zGd x Dy zFe5-m-n-pAl m Mn n InpO12 . Each of the five additives to YIG gives a different adjustment to the magnetic properties appropriate for the application. Not only does the composition have to be precisely controlled to ensure a single phase solid solution, but so does the microstructure (top right). The average grain size of this material needs to be about 12 μm and the porosity—black spots at grain boundaries—less than 1% by volume. In addition, there can be no other phases present, as these would degrade the desired properties. A proper choice of the starting powders (composition and particle size), firing temperature (~1400°C), firing atmosphere (oxygen-rich), and time must be made and controlled in order to obtain the desired material. One of the critical steps in the processing of this material is the calcination or reaction step that involves heating mixed oxides, Y2O3, Gd 2O3, Dy2O3, Fe2O3, Al 2O3, Mn 2O3, and In 2O3, causing them to react by solid state diffusion to form the solid solution alloy. This is done at several hundred degrees below the sintering temperature (~1200°C in this case) so that diffusion can occur but the small powder particles do not sinter into a hard dense mass. After calcination, the reacted powder is pulverized to break up any agglomerates and reduce the particle size—0.1– 1.0 μm—suitable for subsequent solid-state sintering and densification. In general, calcination is a heat treatment process in which a reaction occurs to produce a new solid and is modeled in some detail in Chapter 15. 1.3 HISTORICAL DEVELOPMENT OF MSE AS A DISCIPLINE Metallurgical engineering grew out of mining engineering as an academic discipline when the need arose to have people trained in the extraction of metals from their ores. In 1894, ceramic engineering also emerged as a separate academic discipline from mining engineering. Here, the motive was to apply the principles of chemistry and physics to the manufacturing of ceramic products, which at that time were limited to commodity materials such as paving bricks, roof tiles, refractory bricks, sanitary ware, table ware, and glass. It was not until about the 1930s did ceramic engineering encompass more enabling* materials such as electronic and optical materials. In addition, at the end of the nineteenth century, physical metallurgy began to emerge with efforts to understand the correlations between the composition and microstructure and the mechanical properties of steel. This led to a rapid increase in the number of metallurgical engineering degree programs to provide metallurgical engineers for the metal-user industries as well as the extractive industry. Although the production of synthetic rubber around 1914 may well have been the start of polymer engineering, it was not until around World War II did the production of synthetic polymer materials become important. Interestingly, a great deal of this work was perceived to be chemistry and education in polymers was almost exclusively relegated to chemistry and chemical engineering departments at universities before the past few decades (Morawetz 1985; Cahn 2001). * A commodity material such as a building brick is essentially the end product. In contrast, an enabling material is one that is a critical component of a larger, more complex system, such as the magnetic radar material. ist m In the early 1950s, there were about 80 metallurgy or metallurgical engineering degree programs and about 15 ceramic engineering programs, and maybe one polymer engineering program. In the late 1950s, it was realized by engineers and scientists working in the various materials areas that there was great commonality among their disciplines, particularly the relationships between structure and properties of materials. This ultimately led to the formation of the first MSE graduate program at Northwestern in 1959. By 1970, almost a third of the some 80 metallurgical engineering programs had changed their names—if not their programs—to include materials in one form or another. Today, there are about 60 accredited materials programs* and only a four metallurgical and two ceramic engineering programs remaining. There are five accredited programs in polymers and none are named simply polymer engineering. These polymer programs have names such as plastics and polymer engineering, polymer science and engineering, and polymer and fiber engineering. These mergers and changes in department focus did not always occur smoothly. But two events encouraged integrating the different disciplines into single, yet multidisciplinary, MSE programs. However, neither of these was focused on undergraduate programs but primarily graduate programs and research. The first was the establishment of the Materials Research Laboratories (MRLs) by the then Atomic Energy Commission† and later transferred to the National Science Foundation in 1972. The second was the Committee on the Survey of Materials Science and Engineering (COSMAT) report (COSMAT 1974) whose purpose was to determine the nature and scope of materials science and engineering and to encourage interdisciplinary and multidisciplinary research and education. Today, MSE can be considered to be the intersection of four major disciplines: physics, chemistry, chemical engineering, and mechanical engineering, as shown in Figure 1.3. One might argue with this particular selection and certainly other disciplines can be included. The reality is “…the profession has become so broad and merged at the edges with other disciplines is that it is hard to define.” (Weertman 2007, 18) Indeed, there are many graduate programs and research activities in some MSE and other academic departments at universities where there are no undergraduate programs. On the other hand, there are both materials undergraduate options and accredited programs in many non-MSE academic departments. Although there is a strong commonality among materials between structure and properties, there are significant differences between the processing and resulting structure for the different materials: metals and ceramics typically requiring much higher temperatures than polymers, for example. As a result of these mergers and broadening of the scope of materials, the materials-specific processing: casting and heat treatment for metals; fine powders, high temperatures and sintering for ceramics; and chemistry and glass transitions for polymers get less coverage than they did in materials-specific degree programs. In addition, with increased availability of electron microscopy and the more recent development of nanomaterials, it was clear that the structure–property relationships between man-made materials and those produced in nature, biomaterials, were not too different. As a result, today’s field of MSE is a broad one encompassing metals, ceramPh ics, polymers, electronic materials, biomaterials, and composites. ys ics Interestingly, some metallurgists recognized similarities between the structures of biological materials and metals and their properties almost a century ago (Goerens 1908). 7 ry Historical Development of MSE as a Discipline Ch e 1.3 en Che gi m ne ica er l in g MSE * † Most of these are “materials engineering and science” programs but also includes “metallurgical and materials engineering,” “ceramic and materials engineering,” and other combination of descriptors. Now the U.S. Department of Energy. M en ech gi an ne ic er al in g FIGURE 1.3 The intersection between physics, chemistry, chemical engineering, and mechanical engineering to delineate the fuzzy boundaries of materials science and engineering. 8 Chapter 1. Kinetics and Materials Science and Engineering 1.4 IMPACT OF MSE Materials engineers and scientists have the most critical position in science and industry since … everything has to be made out of something. It is the availability and properties of existing materials that frequently limits advances in technology. This was one of the motivating factors for the establishment of the MRLs in the late 1950s, slow materials development was perceived to be limiting technology (Cahn 2002). For example, it is very easy for a mechanical engineer or aeronautical engineering to design a turbine engine that would increase the thrust and performance of a modern jet aircraft by several tens of percent. However, this would require raising the operating temperature of the gas turbine well above the typical 1000°C–1100°C range now encountered by the turbine blades to maybe as high as 1500°C. As another example, an article (Chang 2014, D6) discussing the history of the undeveloped X-30 “Aero-Space Plane” initially proposed in 1986 to fly at the edge of space at up to 23 times the speed of sound, states, “For the X-30 to succeed, infant ideas would have had to have been developed into robust, reliable technologies— materials that could survive intense temperatures, air breathing engines that could fly faster and higher” (italics added). Unfortunately, even today there are no materials that will reliably perform at such high temperatures. A large government research program tried to develop silicon nitride, Si3N4, as a turbine material that could, in principle, operate at that temperature since there are no fundamental material properties preventing it. However, being a ceramic, silicon nitride is brittle, with no plastic deformation before breaking, and design engineers are still learning how to design with materials that are not ductile like metals. Rather than try to design an entirely new engine that might be able to take advantage of the high temperature capability of silicon nitride, the focus was to design a ceramic component as a direct replacement for metal turbine blades. This puts the ceramic part at a big disadvantage because of the differences in processing and properties compared to metals. For these and other reasons, metals are still being used as turbine blades in jet engines. Nevertheless, there is a now a much better understanding of brittle failure and there remains considerable technological and commercial interest in ceramic-matrix composites that have both high-temperature capability and excellent mechanical properties. Similar comments could be made about nuclear power. Engineers can design a nuclear plant to work at higher powers levels, but the temperature limitations of existing fuel and other materials critical for safe operation do not permit it. Modern microelectronic devices are made from silicon, not because silicon is the best material from a semiconductor properties standpoint—germanium and gallium arsenide are superior—but rather the fact that the native oxide on silicon, amorphous SiO2, can easily be grown and has superior insulating properties to the native oxides on Ge or GaAs. Yet, as devices such as FETs—field effect transistors—become smaller and the SiO2 gate oxide becomes so thin—a nanometer—that it no longer has the good insulating properties of bulk SiO2, other materials, such as HfO2, hafnium oxide, are being used. As a result, the feasibility of applying other semiconductor materials becomes more attractive. There is considerable activity with electric motors replacing the internal combustion engines in automobiles reducing the U.S. and world’s dependence on the certainly finite supply of fossil fuels with the additional beneficial result of decreasing heat-trapping gases such as CO2. However, for this to happen, new batteries with high energy storage capacities must be developed. This is one of the most intense areas of materials R&D that exists today: for it is the properties of the anodes, cathodes, and electrolytes—all materials—that determine the energy capacity and performance of electrochemical cells. Here again, it will be the development of new materials that will make widespread electric propulsion a reality. One article (Moss 2015) suggests that it will be materials engineers and scientists developing new materials that will save the world from various disasters such as global warming! 1.5 MICROSTRUCTURE A comment about the term microstructure is appropriate since it one of the key elements of MSE. The relationship between microstructure—structure that can be seen in a microscope—and properties has been a well-established part of MSE for over a 100 years, and one it is one of the three core 1.6 Thermodynamics Review areas of phase equilibria, crystal structure, and microstructure that distinguish MSE from other fields of science and engineering (Cahn 2002). The historical development of the microstructural investigation of metals has been well documented by Smith (1988). The importance of composition on strength dominated the development of metals, primarily iron and steels, during the late nineteenth century. Since iron and steel were important structural materials, strength was their most important property and remains so for most applications of metals. This ultimately led to the investigation of microstructure by Sorby (Smith 1988) and its relationship to composition and properties. Interestingly, Sorby first studied the microstructure of rocks in transmitted light using thin sections. When he studied metals, he again used thin, mounted samples but examined them in reflected light. Mineralogists quickly adopted Sorby’s thin section technique for rocks, while the metallurgists adopted his techniques more slowly (Smith 1988, Preface, v). It is worth noting that the term microstructure originally had nothing to do with the scale of what was being observed in the microscope. Initially, Sorby called what he could see in the optical microscope microscopical structures (Smith 1988). By 1900, the term had been shortened to microstructure, and was in common use by metallurgists (Goerens 1908; Sauveur 1912), and continued to be used in that way for over a 100 years. It was the correlation between composition (carbon content), heat treatment time and temperature, and microstructure with the strength of steels that was the birth of modern MSE. Today, in materials science, the use of the term microstructure, nanostructure, and mesostructure are used by many to refer to the size of the features in a material. In addition, some polymer scientists refer to the configuration of atoms along a polymer chain as the chain’s microstructure (Sperling 2006). This is very confusing, and hopefully discouraged, since many polymers have both crystalline and glassy phases present in varying amounts and sizes that would be described as the polymer’s microstructure applying the term’s generally accepted meaning. Here, microstructure is used in the broader context of what can be seen with a microscope regardless of the size of the features or the type of microscope being used to observe them. 1.6 1.6.1 THERMODYNAMICS REVIEW A Difficult Subject It is assumed that students taking a course on materials kinetics would have completed a course in chemical thermodynamics and have been exposed to the topics that are summarized here. An elementary knowledge of chemical thermodynamics is a prerequisite for understanding much of the kinetics that will follow. However, the reality is that nobody is really comfortable with his or her understanding of thermodynamics after going through only a one-semester course on the subject. Considerably more exposure to many of the topics and terminology of thermodynamics is required before a level of confidence is attained. In fact, Arnold Sommerfeld (1868–1951), the famous German physicist, supposedly replied in the 1940s to the question “Why didn’t he publish a book on thermodynamics?” (Keszei 2012, Preface, v)* Thermodynamics is a funny subject. The first time you go through it, you don’t understand it all. The second time you go through it, you think you understand it, except for one or two small points. The third time you go through it, you know you don’t understand it, but by that time you are so used to it, it doesn’t bother you any more (sic). Sommerfeld was more than your average scientist. He expanded Bohr’s theory of the atom to explain spectral lines as well as performed research on X-ray diffraction and crystallography. Although he never won a Nobel Prize himself, he was advisor to the largest number of Noble Prize recipients even to this day. Four of students went on to win Nobel Prizes: Hans Bethe, Werner Heisenberg, Wolfgang Pauli, and Peter Debye. Three of his postgraduate students also won Noble Prizes: Linus * Searching on the Internet for the first sentence in this quote generates a large number of hits. Curiously, however, the quote appears in only a few texts devoted to physical chemistry or thermodynamics such as the one quoted. 9 10 Chapter 1. Kinetics and Materials Science and Engineering Pauling, Isidor Rabi, and Max von Laue. In addition, many of his students became famous by making significant contributions to physics during their careers (Millar et al. 2002). So, if someone as talented as Sommerfeld had some trouble understanding thermodynamics after his first few exposures to it, it is not surprising that most people have difficulties. In modeling the kinetics of reactions important in MSE, the thermodynamics of the system must be understood. So, a short refresher on some fundamental thermodynamic concepts is a worthwhile use of time. After all, kinetics typically deals with systems going from a high energy state to a lower one and evaluating the energies of these different states is the goal of thermodynamics. Whereas the goal of kinetics is to determine how fast systems go from high to lower energy states usually by either a reaction-controlled or a transport (diffusion)-controlled process. While the thermodynamics of system is crucial for understanding diffusion-controlled processes, it is important in reaction-controlled kinetics as well. Certainly, an extensive review of thermodynamics is neither possible nor attempted here. Selected thermodynamic topics reviewed are those used in many of the kinetic models developed later. 1.6.2 HiStory of tHermoDynAmicS 1.6.2.1 Relation to MSE The history of how thermodynamics was developed is of particular interest to MSE since both fields had the same motivation: steam engines. Furthermore, the modern field of MSE and its dependence on phase equilibria and phase diagrams was made possible when chemical thermodynamics was developed toward the end of the nineteenth century, primarily by J. Willard Gibbs, a great American scientist. As noted earlier, the properties of steel only became understandable when phase equilibria were applied to interpretation of the microstructure and its relation to the properties of iron-carbon alloys. 1.6.2.2 Why Thermodynamics Is Difficult Similar to MSE, the subject of thermodynamics really got its start after the invention of the steam engine in the late 1700s. The field expanded and grew initially by trying to determine the efficiencies of such engines to get the most work out of burning fuel. Thermodynamics was largely developed throughout the 1800s mainly by manipulating differentials of macroscopic quantities such as internal energy, U, temperature, pressure, and volume. In addition new quantities were developed and given strange-sounding names such as entropy, S, and enthalpy, H (Laidler 1993). The macroscopic equations of thermodynamics were essentially complete before there was general understanding and acceptance of the atomic and molecular structure of matter. As a result, concepts such as the energy content of a substance, U, are rather abstract, and were developed to try to determine how much work could be done by a system given a certain amount of energy input. Today, it is understood that the energy content of a solid, liquid, or gas depends on the vibrations, rotations, and translations of atoms or molecules in a given system. Empirically, the concept of the entropy grew out measurements of work done and heat input and the requirement to balance the total energy equations. Today, it is understood that entropy reflects the randomness of a system. When a crystalline solid sublimes to a gas, the entropy of the system increases because the gas atoms are much more randomly arranged compared to the ordered positions of atoms in solids. This was a major topic of controversy. It was not until about 1877 when Boltzmann published his relationship between entropy and probability: S = k B ln W where: W is the number of ways atoms may be distributed over energy states kB is Boltzmann’s constant. This made the connection between macroscopic thermodynamic quantities and atomic or molecular structure of a material much clearer. When he proposed this relation, he did not state what the value of the constant was other than it was a constant of proportionality. Boltzmann was sufficiently proud of 1.6 this result that it is inscribed on his tomb (Figure 1.4) (Lindley 2001). Today, the relationships between macroscopic thermodynamic quantities and atoms and molecules are well understood. This makes terms such as internal energy and entropy, and the equations relating them, much easier to understand, removing some of the mystery from thermodynamics (Kjellander 2016). Adding to the complexity of thermodynamic definitions and calculations are the different systems of units used in various countries, mainly the English and the metric systems. In recent years, in efforts to standardize notation, units and, definitions of terms, international bodies such as the International Union of Pure and Applied Chemistry (IUPAC) have suggested standards that require changing some long-used terms and definitions. As a result, there are differences in notation between older and newer references and even differences in contemporary references depending on who has accepted the changes and who has not. In addition, different fields focus on different energies (previously called free energies, and still called free energies by some): chemists use the Gibbs energy, G, and physicists prefer the Helmholtz energy, A, both of which were free energies—the energy available to do work—until the end of the twentieth century. 1.6.2.3 Significant Events in the Development of Thermodynamics Thermodynamics Review 11 FIGURE 1.4 Boltzmann’s grave in the Central Cemetery, Vienna, Austria, bearing the inscription of Boltzmann’s law: S = k lnW. (https://commons. wikimedia.org/wiki/File:Zentralfriedhof_Vienna_-_ Boltzmann.JPG) During the development of thermodynamics, there were contributions from French, German, and English scientists. However, sometimes nationalism got in the way of acceptance of the contributions of a colleague from another country (Laidler 1993, 106). Today we think of thermodynamics as a rather stolid and established discipline, with little scope for controversy and it comes as a surprise that in the latter part of the nineteenth century there were fundamental and acrimonious disagreements about it, with harsh words written on both sides. Furthermore, because many scientists were working on similar topics at the same time, it is often difficult to discern who was responsible for a given discovery. For example, Clausius is often given credit for the concept of entropy. However, talking about who made contributions to the concept, Lindley (2004, 111) points out that Subsequently Rankine, Clausius, and Thomson all made contributions to the statement of a second law, both in its physical conception and in the mathematical demonstration of its universality. Clausius in the end christened the child and most often gets the credit. As a result, one might conclude that the significance of a discovery or publication in thermodynamics may be more of an observer’s personal choice than an absolute reality. Therefore, here are some personal choices: Lord Rumford (Benjamin Thompson) Lord Rumford is worthy of being singled out because he was ahead of his time in thermodynamic thinking plus his life story is an extremely fascinating one. Benjamin Thompson was born in Massachusetts in 1753; he was a royalist and British spy during the American Revolution and subsequently went to England when the British lost. There he became an officer in the British army, was knighted, and did some research on gunpowder that led to his election to the Royal Society. Largely through self-promotion and influential contacts, he reappeared in Bavaria where he was made a count and he chose the name Mumford, which was the original name of the town he lived in, Concord New Hampshire, when he left the United States. This was a period when even the difference between heat and temperature were not clearly differentiated and the exact nature of heat was a mystery. After observing the heat generated by boring some 12 Chapter 1. Kinetics and Materials Science and Engineering cannons in the Munich arsenal in 1797, he did some experiments on the relationship between heat and work. He concluded in 1798 that 5.60 J—in today’s units—were equivalent to one calorie of heat (Brown 1999). The accepted value today is 4.184 J/cal (IUPAC 2014). This was only one of his many scientific and engineering pursuits but the one that had the greatest impact on thermodynamics. In 1880, John Tyndall, a renowned scientist of his time, wrote, “When the history of the dynamical theory of heat is completely written, the man, who in opposition to the scientific belief of his time, could experiment, and reason upon experiment, as Rumford did, may count on a foremost place.” (Tyndall 1880, 46; Brown 1999, 94) However, it was over 50 years later before others tried to improve on his determination on the equivalence of heat and work. James Prescott Joule James Prescott Joule is interesting because he essentially did his research as a private citizen, not in a university or industrial research laboratory, and his measurements were the conclusive results that a skeptical scientific world needed to agree on the equivalence between energy and heat. Furthermore, his name lives on in the joule unit of energy. James Prescott Joule was born in England in 1818, son of a wealthy brewing family. This wealth allowed him to begin his research early in life, which he later continued when he ran the beer company. He too did research on the equivalence between work and heat, perhaps to improve the efficiency of the brewing process. In any event, he tried several approaches to heating water by both mechanical and electrical means. In the electrical case, he ran current through a resistor generating I2R heating—and developed this relationship—that is to this day called joule heating. Most significantly, he was able to rotate a paddle wheel driven by a falling weight and found the mechanical equivalent of heat, which he published in 1845. Since he was not an academic, he could not get his results published by the Royal Society but had to publish elsewhere. He was a very careful experimentalist and continued to refine his experiments for greater accuracy. He published additional papers on the mechanical equivalent of one calorie of heat with the final result in 1878 with 772.55 ft-lb of work needed to raise the temperature of a pound of water 1°F at 60°F and sea level (4.144 J/cal a little short of the accepted value today). See Appendix for the conversion calculation). This final value is inscribed on Joule’s headstone (Figure 1.5) in the cemetery in Sale England where he spent his entire life (Brown 1999). FIGURE 1.5 Grave of James Prescott Joule with the inscription for his mechanical equivalent of heat: 772.55 ft-lbs equivalent to 1 calorie. (Photo by Glaukon in the public domain. https://commons.wikimedia. org/wiki/File:James_Prescott_Joule-gravestone.JPG) 1.7 Review of Thermodynamic Concepts 13 Josiah Willard Gibbs Josiah Willard Gibbs (1839–1903, Figure 1.6) was an American scientist who, in 1863, received a PhD in engineering from Yale University, only the second PhD awarded in the United States up to that time (Millar et al. 2002). He was appointed professor of mathematical physics at Yale in 1871 and spent the rest of his bachelor life there. During the 1870s, he essentially single-handedly developed the field of chemical thermodynamics, including the concept of the Gibbs energy—important because it depends on the easily controlled variables of temperature and pressure—the Gibbs phase rule, and phase diagrams (Laidler 1993). He is considered by some to be one of the greatest American scientists of all time. He remains probably the greates theoretical scientist born in the USA (Millar et al. 2002, 142). “What was the nature of his mind? And the greatness? What was that? What places Gibbs with Newton and Einstein?” (Rukeyser 1942, 7) Unfortunately, he published his ideas and results in rather obscure journals; his writing style was incomprehensible to most other scien- FIGURE 1.6 Josiah Willard Gibbs before tists. As a result, the importance of much of his work was not realized 1903. (Photograph in the public domain since it was published before January 1, 1923. https:// until several years after, during which time others had come to similar commons.wikimedia.org/wiki/File:Josiah_ conclusions. Gibbs and his phase diagrams, of course, enabled met- Willard_Gibbs_-from_MMS-.jpg) allurgists to understand the relationships between composition, heat treatment, microstructure, and the properties of steel in the early twentieth century. This knowledge of steels permitted the development of boilers that did not explode and bridges that did not collapse bringing full circle the original intent of thermodynamics: increasing the efficiency of steam engines to giving birth to the field of MSE. 1.7 1.7.1 REVIEW OF THERMODYNAMIC CONCEPTS PurPoSe The goal here is not to justify the various thermodynamic relationships but mainly to review the important conclusions of thermodynamics developed in thermodynamics courses. Most books on physical chemistry cover chemical thermodynamics in detail. In addition, there are several texts devoted to chemical thermodynamics applied to materials (Darken and Gurry 1953; Ragone 1995; DeHoff 2006; Gaskell 2008). The emphasis here is on those relationships that are primarily used in the modeling of kinetic processes that follows. 1.7.2 four lAwS of tHermoDynAmicS The laws of thermodynamics are essentially empirical laws that have been determined by experiment over the last few hundred years. They are as follows: 1. The first law of thermodynamics states that the energy of the universe is conserved during some kind of process. 2. The second law of thermodynamics states that the entropy of the universe increases during a process. 3. The third law of thermodynamics states that there is an absolute zero of temperature and the entropy of all materials is the same at absolute zero. 4. The zeroth law of thermodynamics, defined by some, is: if three bodies A, B, and C are in equilibrium, then A is equilibrium with B, B is in equilibrium with C, and A is in equilibrium with C. 14 Chapter 1. Kinetics and Materials Science and Engineering 1.7.3 firSt lAw of tHermoDynAmicS The first law of thermodynamics, which is rather intuitive, is simply as follows: a small increase in the internal energy of a system, dU, is given by the sum of the heat input, δq, and the work done on the system, δw, the units of all three of them are joules (J). That is, dU = δq + δw. (1.1) Stating it another way, the first law is simply the conservation of energy. Equation 1.1 can also be written as U 2 − U1 = ∆U = ∆q + ∆w ΔU is the difference in internal energy going from state 1 to state 2; it is referred to as state function in that regardless of how the system got from state 1 to state 2, it will have the same set of thermodynamic properties, that is, internal energy. Today, it is known that the internal energy of a system is essentially the vibrational and translational motions of the atoms or molecules that make up the system. But what is a system? A system can be defined as a region of space with boundaries and has thermodynamic properties as shown in Figure 1.7. Now, the internal energy of a system is a state function since its value only depends on the values of the state variables that affect the system, such as pressure, temperature, and composition. That is, if changes are made to state variables and then they are returned to their original values, the internal energy, a state function, is the same as before the variables were changed as illustrated in Figure 1.8. The work done on a system can be of several types: 1. 2. 3. 4. Pressure volume work, PdV, where P is the pressure and dV is the volume change. Mechanical work, Fdl where F is the force and dl is the displacement. Surface work, γdA, where γ is the surface energy and dA is the increase in area. Others, including magnetic work, polarization work, and electrical conduction. It is conventional to write the first law considering only mechanical work, PdV—remember that thermodynamics was developed to understand steam engines—as dU = δq − PdV Heat System • Isolated • Adiabatic • Open Work (1.2) Moles State variables • • • • • P, pressure T, temperature V, volume X, composition ..., other System boundaries • Rigid • T-insulating • Permeable Surroundings (rest of universe) FIGURE 1.7 A thermodynamic system and its surroundings. If the boundaries of the system are rigid, thermally insulating, and impermeable, then the system is isolated. If the boundaries are thermally insulating, then the system is adiabatic. If both matter and heat can pass through the boundaries then the system is open. 1.7 where PdV is now pressure-volume work done by the system with an expansion dV. Note that PdV is the product of an intensive variable, P, and an extensive variable, V.* Such pairs of intensive and extensive variables occur frequently in thermodynamics are termed conjugate variables. Integrating both sides of Equation 1.2 at constant pressure gives† Review of Thermodynamic Concepts V(P,T) 1 V 4 T 2 ∆U = q P − P∆V 3 or the differences in the quantities between two states is P1 P3 ∆U + P∆V = ( U 2 + PV2 ) − ( U1 + PV2 ) = q P and the enthalpy, or heat content, is defined as H = U + PV so ∆H = q p . Similarly, integrating Equation 1.2 under constant volume conditions gives ∆U = q V.‡ Now, the heat capacity at constant volume per mole is CV = q V ∆U = ∆T ∆T (1.3) dU CV = dT V P q P ∆H = ∆T ∆T dH CP = . dT P (1.4) Note that for one mole of an ideal gas, its state function is PV = RT, so for an ideal gas H = U + PV = U + RT or dH = dU + RdT so dH dU = +R dT dT (1.5) CP = CV + R demonstrating that heat capacities and constant volume and constant pressure are not the same. The ideal gas is a rather extreme case and for most solids there is only a small difference between the constant volume and constant pressure heat capacities. In most tables of data, CP values are given because it is much easier to measure them at constant pressure, one bar, than at constant volume. The relationships between CP and CV can be determined for solid and liquids as well from * † ‡ T3 T1 FIGURE 1.8 Schematic representation of a state function V(P, T) that is a function of the state variables P and T. Starting at any point 1, if the system goes through paths P1 → P2 , T1 → T3 , P3 → P2 , and T3 → T1, or any path back to its original P1 and T1 the volume will be the same as the starting volume. where the last term is the molar heat capacity at constant volume. Similarly, the molar heat capacity at constant pressure is given by CP = 15 An extensive variable is one whose value depends on how much is present. On the contrary the value of an intensive variable does not. Both U and V are extensive variables and can be integrated to get the total internal energy and volume. If one mole is being considered, then the quantities of interest are molar quantities and are indicated with an overhead bar; that is, U, H, etc. 16 Chapter 1. Kinetics and Materials Science and Engineering a combination of properties by manipulation of various thermodynamic quantities, but this goes beyond this review and can be found in the literature (Darken and Gurry 1953). 1.7.4 SeconD lAw of tHermoDynAmicS The second law of thermodynamics can be most easily stated that for a reversible process, the entropy, S, is a state-function (only depends in the initial and final states of a system, e.g., P and T like U and H) given by dS = dq rev T (1.6) where q rev is the amount of heat transferred in a reversible process, one that is essentially in equilibrium throughout the process (Gaskell 2008). For an isothermal process, such as melting, at constant pressure, ∆Sm = ∆H m T where ∆H m is the enthalpy involved in melting. When the concept of entropy was developed in the mid-1800s it was considered that it was the amount of heat in a system that was not available to do useful work. Today, it is better understood that it has to do with the increase in disorder among the atoms or molecules making up a system. For example, melting takes heat so ∆Sm > 0 as it must be for all spontaneous processes such as melting where the order among the atoms or molecules is much less in the liquid than the very-ordered crystalline solid. So the entropy is a quantitative measure of the disorder of the system or the number of possible states as given by Boltzmann’s law, S = k b ln W. (1.7) Therefore, the first law can be written dU = TdS − PdV or in its integrated form, U = TS − PV. Entropy or Gibbs energy S, entropy Equilibrium Stated another way, for any spontaneous process, the entropy of the universe must increase. At equilibrium, a system has its maximum entropy and dS = 0 as illustrated in Figure 1.9. For example, assume that the system in Figure 1.7 is one mole of copper at an initial temperature of 300 K, which is placed in a large furnace, the surroundings, at a temperature of 500 K and a constant pressure of one bar. Heat will be transferred to the mole of copper from the surroundings until the copper reaches the temperature of the furnace. The amount of heat necessary to heat the copper is given by dS = 0 dG = 0 500 ∆Q = ∆H = G, Gibbs energy Extent of a process FIGURE 1.9 Schematic showing the relationship between the entropy and Gibbs energy of a system. For a spontaneous process, the entropy always increases while the Gibbs energy decreases. At equilibrium, the entropy is a maximum while the Gibbs energy is a minimum. Therefore, at equilibrium, dS = 0 and dG = 0. ∫ C dT P 300 where the overhead bar indicates molar quantities. Assume that CP is constant and equal to 3R, as will be seen later, or CP = 24.942 J mol ⋅ K so ∆Q = CP ∆T = 24.942 × 200 = 4988.4 J mol . The surroundings is considered to be sufficiently large, so that its temperature does not change with this transfer of heat, so the entropy change of the surroundings is ∆Ssurr = −∆Q T = −4988.4 500 = −9.9768 J mol ⋅ K and is negative because heat is lost to the system. On the other hand, the entropy change of the copper is 1.7 500 ∆Ssys = ∫ 300 Review of Thermodynamic Concepts CP 500 dT = 24.942 ln = 12.741 J mol ⋅ K T 300 so the entropy change of the universe is ∆Suniverse = ∆Ssurr + ∆Ssys = −9.9768 + 12.741 = 2.764 J K the mol is dropped since one mole of copper is being heated. As predicted, the entropy change for this irreversible process is positive. It is irreversible because heat will not flow back into the surroundings from the copper lowering its temperature. Heat always flows from a high temperature to a low temperature until the temperatures are the same and the system and surroundings, in this case, are in thermal equilibrium—their temperatures are equal. 1.7.5 HelmHoltz AnD GibbS enerGieS In order to calculate the amount of work done by systems at constant volume and constant pressure, two additional state functions are defined. The Helmholtz energy, A, given by A = U − TS (1.8) which is the amount of internal energy available to do work and was called the Helmholtz free energy. The second is the Gibbs energy * given by G = H − TS = U + PV − TS. (1.9) For chemical thermodynamics, the Gibbs function is most useful. Since the first law for a reversible process is dU = TdS − PdV and taking the total differential of Equation 1.9 dG = dU + PdV + VdP − SdT − TdS (1.10) and inserting the first law dG = dU + PdV + VdP − SdT − TdS dG = ( TdS − PdV ) + PdV + VdP − SdT − TdS (1.11) dG = VdP − SdT where in the last equation, the change in the Gibbs energy depends on changes in pressure and/or temperature, which are easily fixed and controllable experimental variables and the main reason for introducing the Gibbs function in the first place. On the other hand, doing the same with the Helmholtz energy, the change in energy depends on the change in volume, which is a harder variable to control. At equilibrium, the entropy is a maximum and dS = 0. What is the comparable situation for the Gibbs energy at equilibrium? Again, dSuniverse = dSsys + dSsurr (1.12) and dU = TdS − PdV or dS = dU PdV + . T T (1.13) But, dU sys = −dU surr and dVsys = −dVsurr so with Equations 1.12 and 1.13, the entropy change is * For most of the twentieth century, A and G were called the Helmholtz free energy and Gibbs free energy, respectively. In the 1990s, IUPAC recommended that these be shortened to the Helmholtz energy or function and the Gibbs energy or function. 17 18 Chapter 1. Kinetics and Materials Science and Engineering dSuniverse = dSsys − dU sys PdVsys − ≥0 T T (1.14) from the second law. Multiplying Equation 1.14 by (–T) changes the inequality so −TdSsys + dU sys + PdVsys ≤ 0. But from Equation 1.11, this is dG sys − VsysdP + SsysdT ≤ 0. Therefore, at constant temperature and pressure, dG T , P ≤ 0. (1.15) So, the second law requires that the Gibbs energy be a minimum at equilibrium as shown in Figure 1.9; it is just opposite to the variation in entropy and has its minimum at equilibrium but, like entropy, dG = 0 at equilibrium. 1.7.6 reActionS AnD equilibrium conStAntS 1.7.6.1 Equilibrium Of great importance in kinetics is “What is the equilibrium or lowest Gibbs energy state of a system?” since kinetics models the route to achieving this lowest energy state. Figure 1.10 shows a ball on a track at various heights above some reference level with different potential energies relative to the reference level.* This also serves as a model of the Gibbs energy as a function of the extent of a reaction. Clearly, in the metastable position, the ball (system) will lower its energy by moving to the metastable equilibrium position unless it gained enough kinetic energy to go over the barrier of unstable equilibrium. If it just has enough kinetic energy, the ball may find itself at the unstable equilibrium position where it stops but a slight fluctuation in energy will push it either back to the metastable position or move it forward to the stable equilibrium, the lowest energy state the ball (system) can achieve. 1.7.6.2 Standard States and Equilibrium Constants What is really of interest is to what extent a reaction will occur. Take the simple reaction of the formation of water vapor by the reaction of hydrogen and oxygen at some constant elevated temperature where all three are gases exist in equilibrium. The reaction is H 2 (g) + 1 2 O2 (g) = H 2O(g). Energy Unstable (1.16) For a constant temperature, Equation 1.11 becomes for an ideal gas Unstable equilibrium dG = VdP dG = Metastable equilibrium Stable equilibrium (1.17) where n = number of moles for each of the gases. Integrating this from some standard state Position FIGURE 1.10 Schematic showing different kinds of equilibrium for a ball rolling a track with hills and valleys. In this case, the energy is the potential energy and the stable equilibrium position is the lowest point on the track. nRT dP = nRTd ( ln P ) P p G = G o + nRT ln o P * (1.18) Energies are relative. For example, the ball in Figure 1.9 may reach its lowest potential energy on the track but both the ball and track are moving through space at a very high velocity due to the rotations of earth on its axis and in its orbit. 1.7 Review of Thermodynamic Concepts where Go is the Gibbs energy of the gas in its standard state, Po: the pure gas at one bar pressure* and whatever temperature is being considered.† The pressure of the gas in a reaction is written with a lowercase P to indicate that it is a partial pressure of a specific gas in a molecular mixture of other gases. Gibbs showed that the change in energies for the reaction in Equation 1.16 could be written ∆G = G ( H 2O ) − G ( H 2 ) − 1 2G ( O2 ) (1.19) p H 2 O /P o ∆G = G ( H 2O ) − G ( H 2 ) − 1 2G ( O2 ) + RT ln p /Po p /Po O2 H2 o o o ( p H 2 O /P o ∆G = ∆G + RT ln p /Po p /Po O2 H2 o ( 1/ 2 . ) 1/ 2 ) (1.20) At equilibrium, ∆G = 0 so ∆G o = −RT ln K e (1.21) where Ke is the equilibrium constant and is the term in the brackets in Equation 1.20. Note that the equilibrium constant has no units! Example: Hydrogen-water Gas Mixtures Hydrogen–water vapor gas mixtures are frequently used to get fixed and low oxygen pressure in various kinds of experiments and processes. For example, consider a gas of almost pure hydrogen, so that pH2 ≅ 1 bar that has a dew point of about −20°C (easily achievable in practice with a variety of techniques), which corresponds to a pH2 O ≅ 10 −3 bar (Roine 2002). At 500°C, the Gibbs energy for the reaction in Equation 1.19 is ∆Go = −205.014kJ corresponding to an equilibrium constant of K e = 7.113 × 1013 (Roine 2002). So, pO2 can be calculated from Equations 1.20 and 1.21; that is, 2 pO2 pH2 O 10 −3 = = Po pH2 K e (1) 7.113 × 1013 ( ) 2 pO2 = 1.97 × 10 −34 bar. It is common to refer to the pressure of a gas relative to its standard state pressure as its activity, a, so that if a gas is in its standard state of one bar, then its activity is a = 1.0. In the above example, the activity of oxygen is a O2 = 1.97 × 10 −34 . To handle condensed phases, solids and liquids, their standard states are defined as the pure material at one bar pressure and at whatever temperature is being considered. Therefore, the activities of pure solids and liquids in their standard states is also a = 1.0. So from Equation 1.18, in general, for one mole G = G o + RT ln a. * † (1.22) It used to be a pressure of one atmosphere for everyone but the standard state pressure has been redefined by international convention. But there is not much difference between the two: 1 atm = 1.01325 bar. Note the difference between the two terms: standard state and standard conditions of temperature and pressure. Standard conditions are one bar pressure and 25°C, whereas the standard state is the pure material at one bar pressure at whatever temperature is of interest. 19 20 Chapter 1. Kinetics and Materials Science and Engineering Example: Thermodynamic Activity of Water in a Sodium Chloride Solution At 25°C, the vapor pressure of H2O in equilibrium with pure water is pH2 O = 0.031699 bar (Roine 2002). That is, H 2 O(l) H 2 O(g); K e = 0.031699 so pH2 O = Ke. a H2 O Since the activity of pure H2O is one, the pressure of water vapor over pure H2O is 0.031699 bar. However, over a saturated solution of NaCl in water, the vapor pressure of water is 0.0236 bar (Haynes 2013). Therefore, the thermodynamic activity of water in the solution is a= H 2 O,so ln 1.7.6.3 pH2 O,so ln 0.023855 = = 0.7526. Ke 0.031699 Gibbs Energy as a Function of Temperature Equation 1.9 gives the Gibbs energy as G = H − TS. As a result, Go = H o − TSo and, likewise, ∆Go = ∆H o − T∆So. From Equation 1.4, at constant pressure, the enthalpy of a mole of a substance can be obtained by integrating the heat capacity over some temperature region T ∫ o H oT = H 298 .15 + CPdT (1.23) 298.15 where the enthalpy is the heat content per mole—hence the bar over H—if the heat capacity, CP, has units of J/mol-K as it usually does. Similarly, the expression for the entropy can be written as T o STo = S298 .15 + ∫ 298.15 CP dT. T (1.24) For a reaction such as Ti(s) + O2 (g) → TiO2 (s), the Gibbs energy as a function of temperature is o ∆G oTiO2 = G oTiO2 − G oTi − G oO2 = ∆H oTiO2 − T∆STiO 2. (1.25) Thermodynamic data are determined by experiment and are tabulated and given in various forms o (Roine 2002). The data tabulated are values of H o298.15 and S298 .15 as well as the heat capacities as a function of temperature. The heat capacities, also empirically measured, are usually given in the following form: CP = A + B × 10 −3 T + C 10 −5 + D × 10 −6 T 2 J mol ⋅ K T2 (1.26) and the values of A, B, C, and D are tabulated usually over a finite temperature region. For a given element or compound, these values probably are different over different temperature ranges. Therefore, the enthalpy, entropy, and Gibbs energy can, in principle, be calculated at any temperature of interest and the equilibrium constant for a reaction calculated. However, given the temperature dependence for heat capacities above, the calculations are rather tedious even with a spreadsheet program. Thankfully, software is available that carries out these calculations (Roine 2002). Figure 1.11 shows the enthalpy for rutile TiO2 by reacting titanium with oxygen. The curvature in these plots indicates that the heat capacities of either the reactants or product or both are not constant over this rather limited temperature range. Any phase changes over the temperature range of interest with either the products or reactants will introduce discontinuities to the thermodynamic quantities, G, H, and S at the temperature of the phase transition since each transition adds (subtracts) a finite amount of heat. Figure 1.12 shows the enthalpy of formation of MgO from 1.7 Review of Thermodynamic Concepts 5 ° ΔHT° – ΔH298.15K (kJ/mole) 4 3 2 1 0 ΔHT° (kJ/mole) −940 Ti(s) + O2(g) → TiO2(s) −942 −944 0 100 200 300 500 400 Temperature (°C) FIGURE 1.11 The bottom part of this figure shows the change in enthalpy for the reaction of titanium with T o + ∫298 ∆CP dT where the ∆CP is the oxygen to form titanium dioxide (rutile) as a function of temperature: ∆H298 difference between the molar heat capacities of the products and reactants. And the top curve just shows the change in enthalpy due to the difference in heat capacities. Since the plots are not straight lines, this implies that ∆CP is not a constant but a function of temperature. −595 MgO Mg(s,l) + 1/2 O2(g) ΔHT° (kJ/mole) −600 −605 Tmp (Mg) −610 −615 0 100 200 300 400 500 600 700 800 900 1000 Temperature (°C) FIGURE 1.12 A plot of the enthalpy versus temperature for the reaction of magnesium with oxygen to form magnesium oxide. In this case, there is an increase in enthalpy of the magnesium at its melting point of 650°C due to its enthalpy of fusion, ∆Hf . This makes the enthalpy of the reaction more negative and results in a discontinuity of enthalpy versus temperature at this solid–liquid phase transition. 21 22 Chapter 1. Kinetics and Materials Science and Engineering magnesium and oxygen as a function of temperature. There is a discontinuity at the melting point of magnesium since heat is added to the magnesium reactant at its melting point and the enthalpy of reaction for MgO is the difference between the enthalpy of MgO and that of magnesium and oxygen. Consequently, the enthalpy of the MgO product becomes more negative at the point where the enthalpy of one of the reactants, magnesium, becomes more positive. 1.7.7 multicomPonent SyStemS 1.7.7.1 Introduction All four of the above examples, namely the hydrogen, oxygen, water vapor system; the water-NaCl solution; the reaction to form TiO2; and that to form MgO, are all multicomponent systems in that they contain more than one element or chemical species. More often than not, MSE deals with multicomponent systems with two or more components. In what follows, for the sake of simplicity and concreteness, only two-component systems are considered. All results are easily extended to more than two components. With more than one component in a system, there needs to be a convenient way of expressing how each component makes changes when added to a mixture or a solution* of the components. 1.7.7.2 Partial Molar Quantities† Consider the total volume of a binary solution or mixture of two components, A and B, the partial molar volume of component A is defined by ∂V VA = ∂n A T,P ,nB (1.27) where VA is the change in volume of a multicomponent system with the addition on one mole of component A, at constant temperature, pressure, and moles of component B. There is, of course, a similar expression for component B. Therefore, the total volume of a two-component system consisting of n A moles of A and nB moles of B is V = n A VA + n BVB . (1.28) Dividing by the total number of moles, n, where n = n A + n B Equation 1.28 becomes V = X A VA + X BVB (1.29) where: V is the molar volume of the mixture or solution and the mole fraction Xi is simply X i = n i ( n A + n B ) . For a mechanical mixture or an ideal solution, Vi = Vio where Vi = Vio is the molar volume of component i in its pure or standard state. Example: Molar Volumes of an Ideal Mixture of Water and Sand For water at 25°C, with a molecular weight of 18 g/mol and density of 1 g/cm3, the molar volume is VHo 2O = * † M 18 g mol ≅ ≅ 18cm 3 mol . 1 g cm 3 ρ A mixture here means that the components are interdispersed on a macroscopic scale in which each of the components can be physically separated (with a tweezers or screen) from one another. Examples would be sand and salt or water and oil. A solution consists of the components mixed on the atomic or molecular level such as a solid solution of zinc and copper, brass, or sodium chloride dissolved in water and the components can only be separated at the atomic or molecular level. Some of the literature on thermodynamics refers to these as partial molal quantities, but this terminology is not accepted by the International Union of Pure and Applied Chemistry (IUPAC 2014), and its use does not help to make thermodynamics less confusing. Molar volume, V (cm3/mol) 1.7 – V(X1) – dV (X ) dX 1 – V –B VB0 1–X1 – VA Review of Thermodynamic Concepts – Videal – V – VA0 0 X1 Mole fraction B, X 1 FIGURE 1.13 A schematic plot of molar volume as a function of composition for two situations. The first consists of simple mechanical mixing of the two components A and B resulting in the dashed straight line between their molar volumes in their standard, pure states: VAo and VBo. The second situation is when they form a solution and the molar volume follows the solid curve. The molar volumes of each constituent are determined from the intersection of a tangent line at a given composition, X1, and the two vertical axes. As a result, the partial molar volumes of A and B at this composition are given by VB = V ( X1 ) + (1− X1)(dV /dX ) ( X1 ) and VA = V ( X1 ) − X1(dV /dX ) ( X1 ) as can be seen graphically in the figure. and for SiO2 sand grains o VSiO 2 = M 60.085g mol ≅ ≅ 25.8cm 3 mol 2.334 g cm 3 ρ Therefore, a mixture of sand grains and water would follow the Videal straight line in Figure 1.13 and at a composition of X = 0.5 the total volume occupied would be* V = 0.5 × 18 + 0.5 × 25.8 = 21.9cm 3 mol . For a solution that does not follow ideal behavior, Figure 1.13 also shows a curve of V versus mole fraction. The partial molar values of the two components, A and B, are then given by the intercept of the tangent line dV/dX at X1 at the two vertical axes, VA and VB, as shown in Figure 1.13. From Figure 1.13, graphically, at composition X1, VB = V ( X1 ) + (1 − X1 ) dV ( X1 ) dX (1.30) and VA = V ( X1 ) − X1 dV ( X1 ) . dX (1.31) Example: Molar Volumes of Methanol-Water Solution With data taken from the literature (Haynes 2013) the molar volume of water-methanol solutions is plotted in Figure 1.14. The partial molar volumes of water and methanol were calculated with * This calculation ignores the fact that sand grains by themselves would pack like cannon balls and would have about 45% pore volume in between them which the water could fill, so that the apparent volume of the mixture in a calibrated vessel would appear less than this. Nevertheless, this is the total volume occupied by the water and sand mixture including the volume in the pore space occupied by water. 23 Chapter 1. Kinetics and Materials Science and Engineering 40 Vmethanol Vmethanol 35 Molar volume (cm3/mol) 24 Vsolution 30 (dV/dX)x1 1 – x1 25 20 Vwater Vwater 15 0.0 0.2 0.4 x1 0.6 0.8 1.0 Mole fraction methanol, X FIGURE 1.14 Calculated molar volumes and partial molar volumes with data taken from the literature (Haynes 2013) for water-methanol solutions. The system is almost ideal although, as the plot shows, the partial molar volumes of water and methanol are not constant. As described in Figure 1.13, the partial molar volumes calculated at X1 X= = 0.4576 are Vwater = 17.35cm3 mol and Vmethanol = 39.14cm3 mol as shown methanol in the figure. Equations 1.30 and 1.31 on a spreadsheet program and shown in Figure 1.14. Note that the system is almost ideal—a straight line—but clearly the partial molar volumes of both water and methanol are not constant as is necessary for an ideal solution. At the composition X1 = 0.4576 mole fraction methanol, the values of Vwater and Vmethanol calculated with Equations 1.30 and 1.31 are Vwater = 17.35cm 3 mol and Vmethanol = 39.14 cm 3 mol as shown in Figure 1.14 at the intersections of the tangent line at X1 and the two vertical axes. 1.7.7.3 Chemical Potential and Partial Molar Gibbs Energy If a system has more than one chemical component, say two,* A and B then the thermodynamic functions need to include the effects of composition since it would be expected that different components would have different internal energies. So the first law can be rewritten as, dU = TdS − pdV + µ A dn A + µ Bdn B (1.32) where the chemical potentials, μi, are defined as ∂U µA = ∂n A S,V,µB (1.33) with a similar expression for component B and the ni are the number of moles of components A and B. Now, as an exact differential, the Gibbs energy can be written as ∂G ∂G ∂G dG = dP + dT + ∂P ∂T ∂n A ∂G dn A + ∂n dn B B (1.34) and the partial molar Gibbs energy is defined as, ∂G GA = ∂n A T , P, nB * Only two-component systems are considered but, again, certainly more components are possible. (1.35) 1.7 Review of Thermodynamic Concepts and similarly for component B. Therefore, from Equation 1.11 and these definitions, Equation 1.34 becomes dG = VdP − SdT + G A dn A + G Bdn B . (1.36) Substituting Equation 1.32 into Equation 1.10 now gives, dG = VdP − SdT + µ A dn A + µ Bdn B . (1.37) so the partial molar Gibbs energies and the chemical potentials must be equal; that is, ∂G GA = = µA ∂n A T,P ,nB (1.38) with a similar expression for the chemical potential of component B. A system is in chemical equilibrium when the chemical potential of each component is uniform throughout the system. 1.7.7.4 Gibbs–Duhem Relation At constant temperature and pressure Equation 1.37 becomes dG = µ A dn A + µ Bdn B (1.39) and integrating over the extensive variables n A and nB gives G = µA n A + µBn B . (1.40) Taking the complete differential of Equation 1.40 and subtracting Equation 1.39, the result is 0 = n A dµ A + n Bdµ B (1.41) 0 = X A dµ A + X B d µ B . (1.42) and dividing by n = n A + n B This is the Gibbs–Duhem equation and is used frequently in many of the models developed later. 1.7.7.5 Solutions Equation 1.22 is G = G o + RT ln a (1.43) since the units of G are clearly J/mol. In general, if two components A and B form a solution, then the Gibbs energy of mixing can be written as ∆G mix = ( n A G A + n BG B ) − ( n A G oA + n BG oB ) = n A RT ln a A + n BRT ln a B (1.44) where the terms within the first set of parentheses are the Gibbs energies in the solution state and the second set are the Gibbs energies of the components in their unmixed state. An ideal solution is one that follows Raoult’s law, a i = X i, that is, the activity equals the mole fraction. So the Gibbs energy of mixing of an ideal solution of two components A and B is given by ∆G mix ,id = n A RT ln X A + n BRT ln X B (1.45) and dividing by n = n A + n B gives ∆G mix ,id = RT ( X A ln X A + X B ln X B ) . (1.46) 25 26 Chapter 1. Kinetics and Materials Science and Engineering From Equation 1.11, at constant pressure dG = −S dT P Therefore, ∆Smix ,id = −R ( X A ln X A + X B ln X B ) (1.47) which is exactly the same result obtained with the statistical approach with S = k B ln W in Appendix A.3, Equation A.6. Note, however, if two compounds such as Al2O3 and Cr2O3 form an ideal liquid or solid solution, then the cations are distributed over 2NA lattice sites and the ideal entropy of mixing is just twice that given in Equation 1.47, namely, Smix,id = −2R ( X Al2O3 ln X Al2O3 + X Cr2O3 ln X Cr2O3 ) as shown in Appendix A.3, Equation A.8. For a nonideal solution, of course, the mole fractions must be replaced by activities and there may be a ∆H mix as well. In general, if solutions are not ideal, then the activities may be represented as a i = γ i X i where γi is the activity coefficient for component i, and it can vary with the composition. Example: Activity Coefficient of NaCl in a NaCl-H2O Solution In Section 1.7.6.2 it was found that the activity of water in a saturated sodium chloride solution at 25°C was a H2 O = 0.7526. At 25°C, a saturated aqueous solution of sodium chloride is 6.248 molal; that is, there are 6.248 moles of NaCl per 1000 g of solution (Roine 2002). The molecular weight of NaCl is 58.443 g/mol. The number of grams of NaCl in the 1000 g of saturated solution is m NaCl = 6.248mol × 58.443g/mol = 365.15g so the number of moles of water in the saturated solutions is n H2 O = (1000 − 365.15)g 18.015g mol = 35.240 mol. Therefore, the mole fraction of H2O in the saturated solution is X H2 O = 35.240 ( 35.240 + 6.248 ) = 0.8494. As a result, the activity coefficient for water in a saturated solution of NaCl at 25°C is γ H2 O = 0.7526 = 0.8860. 0.8494 Now the mole fraction of NaCl is X NaCl = 6.248 ( 6.248 + 35.240 ) = 0.1506 which checks since X H2 O + X NaCl = 1.0000 . But the activity of NaCl must be a NaCl = 1.0 since it is a saturated solution; that is, it is equilibrium with pure NaCl that has an activity of 1.0. Therefore, the activity coefficient of sodium chloride in the saturated solution is, γ NaCl = 1.0 = 6.640. 0.1506 1.7.8 PHASe rule AnD PHASe DiAGrAmS 1.7.8.1 Phase Rule Gibbs derived the phase rule, where the number of phases present plus the number of degrees. of freedom is equal to the number of components plus 2, or more simply: Phases + Freedom = Ccomponents + 2..* This is the mathematical result of unknowns ( F) = variables (C + 2) − equations ( P) * A useful mnemonic for remembering the phase rule is Police Force = Cops + 2. 1.7 Review of Thermodynamic Concepts the last term comes from the fact that the chemical potentials must be equal in all of the phases in equilibrium, so there are P equations with the chemical potentials. The number of variables is the number of chemical components, C, plus temperature and pressure, for the extra 2. It should be noted that a phase can be defined as a physically and/or chemically distinct, mechanically separable region of matter. The key phrase here is mechanically separable. For example, a mixture of salt and sand particles consists of two chemically distinct regions, NaCl and SiO2 . They are also physically distinct in that the salt particles may be small cubes where the sand grains are probably somewhat larger and less uniform. They certainly are mechanically separable since, if the mixture were sieved, the smaller salt particles might pass through the screen while the larger sand grains would not. If worse came to worse, the sand grains could be separated from the salt particles with a magnifying glass and a small pair of tweezers. On the other hand, if the salt were dissolved in water, the salt ions and the water molecules are mixed at the molecular level and a magnifying glass and a pair of tweezers will not be of much use. Another example might be ice in equilibrium with water at one bar and 273.15 K, the two phases are chemically the same but physically distinct: one is a solid and one is a liquid, and they certainly are mechanically separable, just knock over the glass! 1.7.8.2 Phase Diagrams Phase diagrams are extremely useful because they visually display a large amount of thermodynamic information. For a one-component, unary, system, the axes of the two dimensional diagram are pressure and temperature. For a two-component, binary, system the pressure is held fixed, usually one bar, and the temperature and composition are the axes of the diagram. For a three-component, ternary, system the pressure is also fixed and a composition triangle forms the base, with the percentages of the three components along the axes, and the temperature is plotted vertically to give a three-dimensional diagram. Useful thermodynamic data are obtained from planar, isothermal sections parallel to the base of the diagram. Additional details of ternary diagrams are not covered here since they are not used in this book. For systems containing more than three components, the diagrams become more complex and considerably less visually useful in displaying thermodynamic data so they are ignored here. 1.7.8.3 Single Component System A schematic of the phase diagram for the H2O system is given in Figure 1.15. Consider a point someplace in the middle of the liquid phase region. In this case, C = 1 (H2O), P = 1 (liquid), therefore Critical point Pressure (atm) 218 Solid 1 Liquid Normal boiling point, 100°C Normal freezing point, 0°C Vapor 0.006 Triple point 0.01 100 Temperature (°C) 374 FIGURE 1.15 P-T phase diagram for pure H2O that shows the triple point, the melting and boiling points at 1 atm pressure, and the critical temperature and pressure where the gas and liquid are no longer distinguishable. The negative slope of the solid–liquid equilibrium is due to the larger volume of ice at any given temperature than that of water. This is discussed in detail in the text. 27 28 Chapter 1. Kinetics and Materials Science and Engineering the degrees of freedom, F, must be F = 3 − 1 = 2. That is, there are two degrees of freedom in that the temperature and pressure can be varied independently and a point stays within the single phase liquid field. The same is true in both the vapor or the solid phase regions as well. However, along the equilibrium lines between the phases, for example, solid–liquid, then P = 2 and F = 1. Neither the pressure nor temperature can be varied independently and stay on the equilibrium curve between the two phases: if the temperature changes, so must the pressure as given by the curve between the phases. Finally, at the triple point, all three phases are in equilibrium, so F = 0, the three phases can exist in equilibrium at only a single value of temperature and pressure. Note that there is also a critical point where the gas and the liquid phases merge to become a single phase. This is not too surprising since, as will be seen, the only real difference between a liquid and a gas is the packing density of the atoms or molecules, the number per unit volume. Note that for the ice–water transition, the temperature of the transition goes to lower temperatures as the pressure increases. This is not surprising since ice is one of few the solids that has a greater volume in the solid state than in the liquid state due to the directional hydrogen bonding in solid H2O making the solid structure more open than in the liquid. Silicon with its directed covalent bonding behaves the same way. This behavior can be made quantitative by applying Equation 1.11 to the equilibrium between ice and water: dG L = dG S VLdP − SLdT = VSdP − SSdT ( VL − VS ) dP = SL − SS dT. ( ) Rearranging the last equation gives dP ( SL − SS ) ∆H m = = dT ( VL − VS ) Tm ( VL − VS ) (1.48) this is a form of Clausius–Clapeyron equation. Taking values from the literature (Roine 2002), VL = M 18.015 −6 3 3 −6 3 = × 10 m cm = 18.06 × 10 m mol ρL 0.997 VS = M 18.015 −6 3 3 −6 3 = × 10 m cm = 19.65 × 10 m mol ρS 0.917 and ∆H m = 6.07 kJ mol and at Tm = 273.15 K, dP ∆H m 6079 × 106 = = = −139.8 bar K dT Tm ( VL − VS ) 273.15 (18.08 − 19.65 ) so the slope dP dT is negative as shown in Figure 1.15. 1.7.8.4 Two-Component System Consider the two-component phase diagram for A and B in Figure 1.16, a simple eutectic system with some terminal solid solutions at both A and B. Usually, such phase diagrams refer to a constant pressure of one bar. Therefore, with the pressure variable constant, the phase rule becomes F = C − P +1. For point 1 in a single phase field, here the liquid phase, F = 3 − 1 = 2 degrees of freedom. As was the case in a single phase field for the one component system, both temperature and composition can be varied independently and a point remains in the single phase field. At point 2 in the liquid + alpha solid solution two-phase field, there is only 1 degree of freedom. The compositions of the two phases in equilibrium are given by the ends of the tie-line intersecting the liquidus 1.7 Review of Thermodynamic Concepts T1 Liquid Temperature T2 Point 1 Point 2 Solidus Liquid + α T3 α T4 Liquidus Liquid + β β Solvus Point 3 α+β T5 20 A 40 60 Mole % B 80 B FIGURE 1.16 Binary phase diagram of two components A and B that exhibits a eutectic and point 3 and terminal solid solutions alpha, α, and beta, β. The Gibbs energy-composition plots in Figure 1.18a–e are constructed at the temperatures labeled 1–5. Gibbs energy (G0, G*) G0 = GA0 + XB (G0B – GA0) Physical mixture G0B Temperature T GA0 G* = G – G0 = 0 0 Solution RT ln aB X1 RT ln aA A 20 40 60 Mole % B 80 B FIGURE 1.17 Schematic diagram showing how a new function G* can be calculated that removes the standard state part of the equation for mixing two components A and B. Plotting G* = G − Go versus composition is often convenient since the tangent intercepts at the two vertical axis give µ A − µ oA and µB − µBo . and solidus lines* and are fixed at a given temperature (Figure 1.16). If the temperature is raised or lowered, the tie-line moves and the compositions of the two phases in equilibrium changes. At point 3, the eutectic point, F = 3 − 3 = 0, there are no degrees of freedom. This is a point fixed in temperature and composition and is called an invariant point in the phase diagram. Note that going horizontally across a binary phase diagram at a constant temperature, say T3, the phase regions follow the pattern: one-phase, two-phase, one-phase, two-phase, and so on. 1.7.8.5 Phase Diagrams and Gibbs Energy-Composition Diagrams One of the most useful things about phase diagrams is that there is a one-to-one correspondence between them and the molar Gibbs energies of the phases that in the diagram. Consider the Gibbs energy versus composition diagram in Figure 1.17. The upper straight line represents the Gibbs energy * The liquidus is the line separating the liquid phase region from the liquid + solid region. The solidus is the line separating the two-phase liquid plus solid region and the solid region. The solvus is the line separating the two solid phase region from the single-phase solid region. The names for these lines were given in the late 1800s when a Latin sounding name was assumed to lend more scientific credibility to something. 29 Chapter 1. Kinetics and Materials Science and Engineering of two components A and B that only form a mechanical mixture such as sand and water, salt and pepper, or a polymer and a solid filler material. In these cases, there is no reaction between the two phases, and there is simple linear relation between any molar quantity of A and B, G in the figure, namely, ( G = G oA + X B G oB − G oA ) (1.49) where the molar Gibbs energies of A and B remain in their standard states. It is sometimes useful, however, to remove this part involving the standard states when working with Gibbs energycomposition diagrams, so that it is easier to evaluate the role of solutions. Therefore, if Equation 1.49 is relabeled G o and a new Gibbs function G* is defined as G * = G − G o . Then when the two components do not form a solution, G* = 0 for all XB, the horizontal dashed line in Figure 1.17. If A and B do form a solution, as shown in the bottom curve of Figure 1.17, then the intersection of the tangent line at a point X1 with the two vertical axes gives RT ln a A and RT ln a B, which can be useful, where a A and aB are the thermodynamic activities of A and B, respectively. Example: Gibbs Energy-Composition Diagrams for the Simple Eutectic System of Figure 1.16. From the phase diagram in Figure 1.16, the Gibbs energy, G*, composition diagrams can be constructed. At T1, the system is liquid for any composition. Therefore, Figure 1.18a shows the G*-composition diagram for this temperature. The liquid has the lowest Gibbs energy of the three α β Gibbs energy (G*) Temperature T1 Liquid GB – GB° = R T InaB GA – GA° = RT In aA (a) Phases present = Liquid 20 A 40 60 Mole % B 80 B β Gibbs energy (G*) 30 Temperature T2 α 1 2 α α + liquid Liquid Phases present Liquid (b) A 20 40 60 Mole % B 80 B FIGURE 1.18 (a) Gibbs energy-composition diagram constructed from the phase diagram in Figure 1.16 at T1. (b) Gibbs energy-composition diagram constructed from the phase diagram in Figure 1.16 at T2. (Continued) 1.7 Gibbs energy (G*) 4 Liquid 1 3 2 Phases present α + liquid α 20 A (c) β Temperature T3 α Review of Thermodynamic Concepts Liquid 40 60 Mole % B β + liquid β 80 B Temperature T4 Gibbs energy (G*) 2 1 3 Phases present 20 A β α + β + liquid α (d) β Liquid α 40 60 Mole % B 80 B Temperature T5 Gibbs energy (G*) Liquid β α 2 1 Phases present α (e) A α+β 20 40 β 60 Mole % B 80 B FIGURE 1.18 (Continued) (c) Gibbs energy-composition diagram constructed from the phase diagram in Figure 1.16 at T3. (d) Gibbs energy-composition diagram constructed from the phase diagram in Figure 1.16 at T4. (e) Gibbs energy-composition diagram constructed from the phase diagram in Figure 1.16 at T5. phases (liquid, solid alpha, and solid beta) so it is the stable phase at all compositions with the tangent line at some composition giving the G* for A and B at the intersection of the two vertical axes. At T2, Figure 1.18b, the α phase has a lower energy than the liquid over a finite region. A common tangent line to the two phases, α and liquid, at points 1 and 2, respectively, gives the G* values for A and B again at the intersection of the tangent line with the two vertical axes. Of course, if these two phases are in equilibrium, then the Gibbs energies of both A and B must be the same in both phases; hence, the common tangent. However, between the contacts, points 1 and 2 of the common 31 32 Chapter 1. Kinetics and Materials Science and Engineering tangent with the two phases, a mixture of two phases with compositions given by the tangent points has a lower energy, the tangent line, than either of the two phases in equilibrium. Therefore, these two tangent points determine the composition range of a two-phase region at this temperature in Figure 1.16. For compositions to the left of the tangent point 1 on the α phase, the α phase has the lowest Gibbs energy and so this tangent point determines the maximum composition of single phase alpha on the phase diagram in Figure 1.16. At T3, Figure 1.18c, two tangent lines can be drawn: one intersecting the alpha and liquid phases at points 1 and 2, and one intersecting the liquid and beta phases at points 3 and 4. As at T2, G* is lower for the two-phase mixtures of alpha + liquid (points 1 and 2) and liquid + beta (points 3 and 4) between these common tangent points on the tangent lines. Again, the extensions of the tangent lines to the vertical axes give the activities (actually RT ln a) of A and B for the compositions of the three phases at the tangent points. Again, to the left of the α + liquid, two-phase region (point 1) the single phase α has the lowest energy and is the stable phase. Similarly, for compositions to the right of point 4, tangent to the beta phase, beta has the lowest energy and is the stable phase. At T4, a single tangent line intersects all three phases at points 1, 2, and 3. This is the invariant eutectic temperature where the three phases are in equilibrium so all three must have the same G*A and G*B where the tangent line intersects the left and right vertical axes, respectively. To the left of point 1, alpha has the lowest Gibbs energy and is the stable phase while to the right of point 3, beta has the lowest energy and is the stable phase. Finally, at T5, both solid phases are lower in energy than the liquid as given by the tangent line between them intersecting at points 1 and 2. Between points 1 and 2, the tangent has the lowest energy so these two points give the limits of the two-phase α + β region. To the left of point 1, α has the lowest energy and is the stable phase while to the right of point 2, β has the lowest Gibbs energy and is the stable phase. Conversely, the phase diagram shown in Figure 1.16 could be constructed from the Gibbs energycomposition diagrams in Figure 1.18. This example demonstrates the very close relationship between Gibbs energy-composition diagrams and phase diagrams. It is possible to create either from the other. Understanding this relationship is invaluable in being able to use phase diagrams to initiate development of kinetic models for the rates of reactions and phase transitions. 1.8 CHAPTER SUMMARY The purpose of this introductory chapter was twofold. First, a student is presented a topic and too often, along with it, the impression that out of the cloud, disciplines such as MSE or thermodynamics suddenly appeared in their present state. Of course, nothing could be further from the truth. It took thermodynamics over 100 years to reach a rather mature state and MSE almost as long. Therefore, a brief history of each is presented to show that these fields took time to get to their present state. Furthermore, the common root of both disciplines, steam engines, is emphasized. This culminated in the chemical thermodynamics and phase diagrams of Gibbs that gave the metallurgist at the beginning of the twentieth century the tools needed to understand the effect of composition and heat treatment on the properties of steel. Second, a brief review of important topics in thermodynamics is presented since the thermodynamics of a system underlies the development of kinetic models of reactions and phase transformations, the subject of this book. APPENDIX A.1 joule’S mecHAnicAl equivAlent of HeAt As early as 1824, the calorie was defined as the amount of heat needed to raise the temperature of 1 kg of water 1°C. This is now designated as the kilogram-calorie or calorie. During the 1800s, there was confusion between this and the definition of the gram-calorie or the amount of heat needed to raise 1 g of water 1°C. The difference between the two is now recognized and during Joule’s measurements, he was probably not concerned with either since they were terms used in France, while Appendix in his England, the unit of heat was the British thermal unit, the amount of heat necessary to raise 1 lb of water 1°F! Today, the energy unit is a joule, so the goal is to convert Joule’s measurement of the energy equivalent of heat into joules and compare that to a calorie. His best measurement of the equivalence of work and heat was 722.55 ft-lb/BTU. There are 2.2046 lb/kg. Therefore, carrying out the conversion step by step: 1 ft = 1 ft × 12 ( in. ft ) × 2.54 ( cm in.) × 1 lb = 1 lb × 1 = 0.3048 m 100 ( cm m ) 1 = 0.4525 kg. 2.2046 lb kg Therefore, 1 ft ⋅ lb = 0.3048 m × 0.4525 kg × 9.8 m s2 = 1.35164 J where 9.8 m/s2 is the acceleration of gravity necessary to change mass into a force. So 772.55 ft-lb are 772.55 ft ⋅ lb × 1.35164 J ft ⋅ lb = 1.04421J ×103 is the amount of heat to raise the temperature of 1 lb of water 1°F. Therefore, the number of joules required to heat 1 g of water 1°C is 1.04421× 103 ( J lb ⋅°F ) × 2.2046 ( lb kg ) × 1 9 × ( °F °C ) = 4.144 ( J g ⋅°C ) = 1 calorie 1000 ( g kg ) 5 Since the amount of heat necessary to raise 1 g of water depends on the starting temperature, the IUPAC has determined, based on more recent measurements, that the value of the thermodynamic calorie is 1 calorie = 4.184J. So James Prescott Joule’s measurement in his laboratory, almost 150 years ago, was off by only about 1% from the currently accepted value. A.2 StirlinG’S APProximAtion A.2.1 Plausibility Argument Stirling’s approximation is ln ( N !) ≅ N ln N − N (A.1) which is made plausible from the following very non rigorous approach: ln ( N !) = ln (1× 2 × 3 × 4 × N ) = ln 1 + ln 2 + ln N = N ∑ ln n (A.2) 1 and approximating the sum with an integral (here N and n are just integers and dummy variables) N ∑ 1 N ∫ N ln n ≅ ln n dn = n ln n − n 1 1 = N ln N − N + 1 ≅ N ln N − N (A.3) 33 34 Chapter 1. Kinetics and Materials Science and Engineering ln (N !) ≅ N ln N − N (A.4) Substituting the integral for the sum certainly seems valid if N is large. The integral is evaluated by integration by parts where the value of the integral at the lower limit is just 1 which can be ignored compared to any reasonably large value of N. A.2.2 How Good Is Stirling’s Approximation? For example, even for N = 100, N! = 9.3 × 10157 so ln N! = 363.7 while N ln N − N = 100 × ln 100 − 100 = 360.5 or a difference of about 0.9%. Therefore, for the large numbers involved in solids, N ≅ 1022 cc −1 Stirling’s approximation is certainly good enough! A.3 StAtiSticAl APProAcH to tHe entroPy of mixinG A.3.1 Molar Entropy of Mixing of Two Crystalline Elements The entropy of mixing of an ideal solution can be modeled from Boltzmann’s equation for the entropy S = k B ln W where W, in this case, is the number of ways a total number of N atoms consisting of a atoms, Na, and N b b atoms can be distributed among N lattice sites, where N = N a + N b . Therefore, W= N! Na ! N b ! (A.5) is the number of ways that the a and b atoms can be arranged over the N total sites. Taking the natural logarithm of both sides of Equation A.5 ln W = ln N ! − ln N a ! − ln N b !. And with the application of Stirling’s approximation this becomes, ln W = N ln N − N − N a ln N a + N a − N b ln N b + N b N ln W = − N a ln a N Nb − N b ln N and if N = NA, Avogadro’s number, one mole of atoms, then N N N N ln W = − N A a ln a − N A b ln b NA NA NA N so the entropy becomes, Smix ,id = − k B N A ( X a ln X a + X a ln X a ) Smix ,id = −R ( X a ln X a + X a ln X a ) (A.6) where Xa and Xb are the mole fractions of a and b, respectively. This is the same as Equation 1.47 in the text obtained through a strictly thermodynamic path. For a 50–50 solution, Smix,id = −R ln 0.5 = −5.762 J mol ⋅ K . A.3.2 Molar Entropy of Mixing of Two Compounds NiO and MgO form almost an ideal solid solution. Therefore, the ideal molar entropy of mixing of these two compounds is also given by Equation A.6 since the two cations are distributed over a Exercises total of NA lattice sites. However, what is not always appreciated is that the molar entropy of mixing is different if the two compounds are Al2O3 and Cr2O3 that also form an almost ideal solid solution. In this case, the total number of sites that the aluminum and chromium ions are distributed over is not NA but 2NA since there are two cations for each mole of the two constituent compounds. Therefore, now 2N A = N Al + N Cr and W= ( 2 N A )! (A.7) N Al ! N Cr ! and taking the natural logarithm of both sides of the equation ln W = ln ( 2 N A !) − ln ( N Al !) − ln ( N Cr !) and applying Stirling’s approximation ln W ≅ 2 N A ln ( 2 N A ) − 2 N A − N Al ln N Al + N Al − N Cr ln N Cr + N Cr ln W ≅ ( N Al + N Cr ) ln ( 2 N A ) − N Al ln N Al − N Cr ln N Cr N N ln W ≅ − N Al ln Al − N Cr ln Al N 2 A 2N A 2N A ln W ≅ − N Al 2N A 2N A ln X Al2 O3 − N Cr 2 N A ln X Cr2 O3 ln W ≅ −2 N A ( X Al2 O3 ln X Al2 O3 + X Cr2 O3 ln X Cr2 O3 ) . Therefore, the molar entropy of mixing is Smix ,id = −2R ( X Al2 O3 ln X Al2 O3 + X Cr2 O3 ln X Cr2 O3 ) (A.8) just twice that for the molar entropy of mixing for a solution of elements. So, for a 50–50 solid or liquid solution, Smix ,id = −2R ln 0.5 = −11.526 J mol ⋅ K . Obviously, if the solution consisted of Al2O3 and Cr2S3—but not very likely—then there are 5 NA sites over which the cations and anions can be distributed and the molar entropy would be Smix ,id = −5R ( X Al2 O3 ln X Al2 O3 + X Cr2S3 ln X Cr2S3 ) . EXERCISES 1.1 The value of the gas constant, R, is R = 8.314 J/mol-K. However, it is often more convenient to have it in different units. Convert R to the following units: a. cal/mol-K b. liter-atm/mol-K c. cm3-atm/mol-K d. m3-MPa/mol-K e. in3-psi/mol-°F f. cm3-torr/mol-°F 1.2 On the other hand, when dealing with energies of atoms or molecules rather than moles, it is frequently more convenient to use Boltzmann’s constant, kB = R/NA where NA is Avogadro’s number. a. Calculate Boltzmann’s constant in J/K b. Calculate Boltzmann’s constant erg/°F 35 36 Chapter 1. Kinetics and Materials Science and Engineering 1.3 Physicists like to use energies of atoms and molecules in terms of electron volts (eV) which is the energy necessary to move an electron across a potential of 1 V. a. Calculate the value of an eV in J. b. Calculate the value of 1.7 eV/atom in J/mole. c. Calculate a value of Boltzmann’s constant in eV rather than Joules. 1.4 Dichlorosilane, SiH2Cl2, can be used to make high purity silicon for integrated circuit processing via the following reaction: SiH2Cl2(g) = Si(s) + 2 HCl(g) The Gibbs energies at 1400 K for dichlorosilane and HCl are, respectively, ΔGo(SiH2Cl2) = −183,410 J/mol and ΔGo(HCl) = −102,822 J/mol. a. Calculate the value of the equilibrium constant at 1400 K. b. Calculate the equilibrium partial pressures of dichlorosilane and HCl over silicon at 1400 K if the starting pressures are p(SiH2Cl2) = 0.01 atm and p(HCl) = 0. 1.5 Gas mixtures of methane, CH4 and H2 are frequently used in surface hardening of steels to increase the carbon content at the surface. The Gibbs energy for the reaction at 700°C is given by (Roine 2002): C(s) + 2H 2 (g) CH 4 (g); ∆G o700 °C = 16.312 kJ mol a. It is desired that the surface of the steel in this atmosphere contain 1.0 w/o C. If the atomic weight of carbon is 12.01 g/mol and that of iron 55.85 g/mol, calculate the mole fraction of carbon in 1 w/o steel. b. If the mole fraction is the same as the activity of carbon, calculate the necessary pressure (bar) of methane in the gas to achieve this surface concentration if the pressure of hydrogen is fixed at one bar. 1.6 The molar heat capacity of solid copper is given by (Kubaschewski et al. 1993) CP = A + B × 10 −3 T + C 10 −5 + D × 10 −6 T 2 J mol ⋅ K T2 where A = 30.29, B = −10.71, C = −3.22, and D = 9.47 and Units (T) = K. a. Calculate and plot the molar heat capacity of solid copper from 0°C to 1000°C at 100° intervals. o b. Calculate and plot ∆H oT − ∆H 273 .15 of solid copper from 0°C to 1000°C at 100° intervals. c. Do the same for the entropy. 1.7 The melting point of copper is about Tm = 1083°C, its density at 20°C is ρ = 8.96 g/cm 3, its atomic weight is M = 63.55 g/mol, its heat of fusion is 13.02 kJ/mol, and its linear thermal expansion coefficient is α = 17.0 × 10 −6 K−1 (Brandes and Brook 1992). a. Calculate the density of solid copper at its melting point. Assume that the volume expansion coefficient ≅ 3α. b. The density of liquid copper at the melting point is ρ = 8.00 g/cm3. Calculate the slope of the P-T line between solid and liquid copper at 1 atm. 1.8 The melting point of silicon is about Tm = 1410°C, its density at 20°C is ρ = 2.34 g/cm3, its atomic weight is M = 28.09 g/mol, its heat of fusion is 50.66 kJ/mol, and its linear thermal expansion coefficient is α = 7.6 × 10−6 K−1 (Brandes and Brook 1992). a. Calculate the density of solid silicon at its melting point. Assume that the volume expansion coefficient ≅ 3α. b. The density of liquid silicon at the melting point is ρ = 2.51 g/cm3. Calculate the slope of the P-T line between solid and liquid silicon at 1 atm. References T1 Temperature T2 Liquid T3 T4 A 20 40 AB 60 80 B Mole % B FIGURE E.1 Phase diagram that shows an intermetallic compound AB and no terminal solid solutions at components A and B. 1.9 From Boltzmann’s relation S = k B ln W show that the ideal molar entropy of mixing of aluminum sulfide (Al2S3) and aluminum selenide (Al2Se3) is given by Smix,id = −3R ( X Al2S3 ln X Al2S3 + X Al2Se3 ln X Al2Se3 ) 1.10 The phase diagram in Figure E.1 is similar to that for many III-V compounds that have useful electronic properties allowing them to be used for light-emitting diodes (LEDs) and other applications. a. Label all of the phase fields in the diagram. b. Sketch the Gibbs energy-composition plots for temperatures T1 to T4 each on a separate plot. c. If the Gibbs energy of formation of the compound AB is −120 kJ/mol at T4, calculate the thermodynamic activity of B in AB at the 40 m/o B overall composition. d. Do the same for A in AB at the 60 m/o B overall composition. REFERENCES Brown, G. I. 1999. Count Rumford. Stroud, Gloucestershire: Sutton Publishing. Cahn, R. W. 2001. The Coming of Materials Science. London: Pergamon. Chang, K. 2014. Time Travel. New York Times, October 24, 2014. Committee on the Survey of Materials Science and Engineering (COSMAT). 1974. Materials and Man’s Needs. Washington, DC: National Academy of Sciences. Darken, L. S. and R. W. Gurry. 1953. Physical Chemistry of Metals. New York: McGraw-Hill Book. DeHoff, R. 2006. Thermodynamics in Materials Science, 2nd ed. Boca Raton, FL: Taylor & Francis Group. Gaskell, D. R. 2008. Introduction to the Thermodynamics of Materials, 5th ed. New York: Taylor & Francis Group. Goerens, P. 1908. Introduction to Metallography, translated by F. Ibbotson. London: Longmans, Green. Haynes, W. M., Editor-in-Chief. 2013. CRC Handbook of Chemistry and Physics, 94th ed. Boca Raton, FL: CRC Press. International Union of Pure and Applied Chemistry (IUPAC). 2014. Compendium of Chemical Terminology. Gold Book. goldbook.iupac.org. Keszei, E. 2012. Chemical Thermodynamics. Berlin, Germany: Springer-Verlag. Kjellander, R. 2016. Thermodynamics Kept Simple. Boca Raton, FL: CRC Press. Kubaschewski, O., C. B. Alcock, and P. J. Spencer. 1993. Materials Thermochemistry, 6th. ed. Oxford: Pergamon Press. Laidler, K. J. 1993. The World of Physical Chemistry. Oxford: Oxford University Press. 37 38 Chapter 1. Kinetics and Materials Science and Engineering Lindley, D. 2001. Boltzmann’s Atom. New York: The Free Press. Lindley, D. 2004. Degrees Kelvin. Washington, DC: John Henry Press. Millar, D., I. Millar, J. Millar, and M. Millar. 2002. The Cambridge Dictionary of Scientists, 2nd ed. Cambridge: Cambridge University Press. Morawetz, H. 1985. Polymers, The Origins and Growth of a Science. New York: Wiley. Moss, S. 2015. Materials Scientists to the Rescue. MRS Bull. 40(3): 296. Ragone, D. V. 1995. Thermodynamics of Materials, Vols. I and II. New York: Wiley. Roine, A. 2002. Outokumpu HSC Chemistry for Windows, Ver. 5.11, thermodynamic software program, Outokumpu Research Oy, Pori, Finland. Rukeyser, M. 1942. Willard Gibbs. Woodbridge, CT: Ox Bow Press. Sauveur, A. 1912. The Metallography of Iron and Steet. Cambridge, MA: Sauveur and Boylston. Smith, C. S. S. 1988. A History of Metallography, Cambridge, MA: MIT Press. Sperling, L. H. 2006. Introduction to Physical Polymer Science, 4th ed. New York: Wiley. Tyndall, J. 1880. Heat: A Mode of Motion. London: Longmans, Green. Weertman, J. 2007. The Evolution of the Materials Science Profession and Professional over the Past 50 Years. JOM. 59(2): 18–19. Wheeler, L. P. 1951. Josiah Willard Gibbs. Woodbridge, CT: Ox Bow Press. Section II Reaction Kinetics Chapter 2 Introduction to Kinetic Processes in Materials Chapter 3 Second-Order and Multistep Reactions Chapter 4 Temperature Dependence of the Reaction Rate Constant Chapter 5 Heterogeneous Reactions 39 41 61 95 111 2 Introduction to Kinetic Processes in Materials 2.1 2.2 2.3 2.4 2.5 2.6 Introduction: Material Transport and Reaction Rates 2.1.1 Example: Deposition of Silicon from the Gas 2.1.2 Example: Dissolution Rates of NaCl and Al2O3, Contrast Diffusion and Reaction Control 2.1.3 Conclusions from Examples Homogeneous and Heterogeneous Reactions Homogeneous Reaction Rates 2.3.1 Why Study? 2.3.2 Reaction Order 2.3.3 Units and Symbols Zero-Order Reaction First-Order Reaction 2.5.1 Integrated Equation 2.5.2 Fraction Reacted 2.5.3 The Half-Life of a Reaction 2.5.4 Relaxation Time 2.5.5 Example of First-Order Reaction: COCl2 Decomposition Radioactive Decay and Related Nuclear Reactions 2.6.1 Ideal First-Order Reaction 2.6.2 Uranium Isotopes 2.6.3 Radioisotope Power Sources 41 42 42 43 45 45 47 47 47 48 50 50 50 51 51 51 52 52 52 53 54 42 Chapter 2. Introduction to Kinetic Processes in Materials 2.6.4 Nuclear Reactors and Fission Products 2.6.5 Radiocarbon Dating 2.7 Importance of First-Order Reactions in Materials 2.8 Chapter Summary Exercises References 2.1 54 55 57 58 58 60 INTRODUCTION: MATERIAL TRANSPORT AND REACTION RATES A major consideration in presenting kinetics in materials science and engineering (MSE) is what topics should be covered and to what depth? Certainly, mass transport—diffusion—is an important topic for all materials. Indeed, the second half of this book is devoted to diffusion: the spontaneous intermingling or mixing of atoms, ions, molecules, or particles due to random thermal motion. The macroscopic diffusion equations, how they are solved, and their relation to kinetic processes are important and general areas for all materials and are central to developing model-based process control. However, many texts only cover kinetic processes involving phase changes in the solid state and ignore transport in liquids and gases—fluids—or between liquids and gases, and solids and gases. The solutions to the macroscopic diffusion equations are not always applied to material processes involving solids with liquids or gases. Furthermore, often only the atomistic mechanisms of diffusion in solids are discussed, and those in liquids and gases are not. MSE is much broader than this, and, in many cases, the interactions between solids, gases, and liquids are of critical importance in materials processing and the development of structure and properties. Therefore, this chapter introduces the classical concepts of macroscopic reaction kinetics by defining reaction rates, their temperature dependence, the order of a reaction, and other terminology such as fraction reacted, half-life, and relaxation time. In this chapter, only zero- and first-order reactions are covered with a significant discussion about nuclear reactions and decay because they are ideal first-order reactions and introduce some nuclear chemistry and physics important to materials. The following two examples illustrate the importance in understanding reaction kinetics in MSE. 2.1.1 ExamplE: DEposition of silicon from thE Gas A singularly important example is the chemical vapor deposition (CVD) of silicon (Si) thin films from a Si-containing gas for semiconductor and photovoltaic device applications. CVD is the formation of a solid on some suitable solid substrate by the reaction of gases only. There are several Si-containing gases that are used to deposit Si. One process is SiHCl3 ( g ) + H 2 ( g ) Si(s) + 3 HCl ( g ) illustrated in Figure 2.1. In this case, the reactant gases—trichlorosilane (SiHCl3) and hydrogen— must first be transported to the surface of the solid substrate before the reaction can take place. Usually, this happens by a gas phase diffusion process. Then the reactants must actually react at the surface to deposit the Si. Such surface reactions can involve many individual reaction steps (as will be seen later in this chapter) before the reaction is complete. Finally, the product gas, HCl, must be transported away from the surface, again by diffusion. This process illustrates the broader range of kinetic processes that today’s materials scientists and engineers need to be familiar with. Older texts on materials frequently discuss only diffusion in the solid state because only kinetic processes in solids were considered important. The situation has changed, and the very important technological 2.1 Introduction: Material Transport and Reaction Rates SiHCl3 + H2 Diffusion Gas Surface reaction 3 HCl Diffusion Si film Substrate FIGURE 2.1 Schematic showing the deposition of a silicon film on a substrate by chemical vapor deposition from trichlorosilane (SiHCl3) in a hydrogen carrier gas. The three series steps are as follows: (1) transport of the reactant gases to the surface, (2) the actual reaction at the surface, and (3) transport or diffusion of the product gases away from the surface. The slowest of the three steps controls the overall kinetics of the deposition. process in MSE of Si deposition illustrates that diffusion in the gas phase and reaction kinetics need to be part of MSE education today. The process variables under a materials engineer’s control that determine the rate of Si deposition are the various gas pressures, gas flow rates, and temperatures. Reactant diffusion to the surface, followed by a surface reaction, finally followed by product diffusion away from the surface are three kinetic steps in series. As will be demonstrated later, the slowest step in the sequence determines the overall rate of a series sequential step process. Usually, at low temperatures, the surface reaction rate is the slowest step and limits the rate of deposition. In contrast, at high temperatures, diffusion is slower and limits the rate of deposition. Therefore, in order to develop a rational model of this process, it is essential to understand both the kinetics of diffusion in the gas and the kinetics of surface and other reactions. The first part of this book focuses on what could be called “classical kinetics” that might be taught in a physical chemistry course. But most MSE students do not take physical chemistry as a separate course today, so there is a need to expose the student to the terminology and concepts of classical reaction kinetics. This chapter is the first of several chapters that attempts to do this. 2.1.2 ExamplE: Dissolution ratEs of nacl anD al2o3, contrast Diffusion anD rEaction control The kinetics of dissolution of solids in aqueous or other solutions, an area certainly important in the processing and/or performance of all materials—metals, ceramics, polymers, and biomaterials—illustrates the effect of the relative speed of these two series processes: reaction and transport. For example, sodium chloride (NaCl) is thermodynamically quite soluble in water and dissolves by the reaction: NaCl(s) Na + (solution) + Cl − (solution); ∆ G°(0°C) = −7.84 kJ/mole which gives for the equilibrium constant (Roine 2002): ∆ G° Na + Cl − − = K e (0° C) = e RT = 31.53 a NaCl (where [Na+] and [Cl−] are concentrations in mol/kg-soln, that is, molal concentrations). If the solid is pure NaCl, its thermodynamic activity is a NaCl = 1, so the equilibrium concentrations of Na+ and Cl− are [ Na + ]e = [Cl − ]e = 31.53 = 5.62 mol/kg-soln at 0°C. The NaCl-H 2O phase diagram with data taken from a variety of sources is sketched in Figure 2.2, showing the solubility of NaCl in H 2O as a function of temperature, and the depression of the freezing point of water down to 43 Temperature (°C) Chapter 2. Introduction to Kinetic Processes in Materials Liquid Liquid + solid NaCl Tmp = 801°C 0 −21 Ice + liquid Ice + solid NaCl 26.6 w/o 10.05 m/o 4.5 mol/kg-soln H2O Sodium chloride–water phase diagram based on data from a number of sources. − − − + Solvated Na+ and Cl− ions − + − + + Cl− − + − Water molecules + NaCl crystal Surface − + + − − − − − + Na+ + − + + − + − − + + + + FIGURE 2.2 NaCl w/o NaCl + 44 − Solution FIGURE 2.3 The dissolution of a sodium chloride crystal in water with the solvation energy of the water molecules with the Na+ and Cl− ions providing the necessary free energy for dissolution. The rate of dissolution of NaCl is generally controlled by liquid diffusion of the solvated ions away from the surface. the eutectic temperature of −21.1°C at 26.6 w/o (w/o = weight percent), or 10.05 m/o (m/o = mole percent), or 4.5 mol/kg-soln. Figure 2.3 schematically shows the sequential reaction and diffusion steps. In this case, the Na+ and Cl− ions give up their nearest neighbor anion and cations in the solid surface for the polar H 2O molecules in solution. The enthalpy for the reaction at 0°C is actually positive, 8.132 kJ/mol, because the solvation energy of the ions is less than the energy of the ions in the crystal. But it is the high increase in entropy, 58.462 J/mol-K, going from the ordered solid to the disordered liquid, ∆G = ∆H − T∆S = 8.132 × 103 − 273.15 × 58.462 = −7.837 kJ mol that produces the high solubility (Roine 2002). This reaction step is followed by the diffusion of the solvated ions away from the surface. For the dissolution of NaCl in water, the rate of dissolution is controlled by diffusion in the liquid, which is easily demonstrated by stirring the solution— essentially decreasing the diffusion distance—which increases the rate of dissolution. Experience shows that salt (NaCl) dissolves quite rapidly in water, at least at room temperature and above. In contrast, the dissolution or corrosion of Al2O3 in acidic solutions occurs by the following reaction: Al 2O3 (s) + 6H + (solution) → 2Al +3 (solution) + 3H 2O (solution); ∆G °(30 ° C ) = −101.5 kJ mol with an equilibrium constant of (Roine 2002) 2 Al +3 a 3H2 O = K e (30 ° C) = 3.09 × 1017. 6 H + a Al2 O3 The thermodynamic activities of water and alumina are 1.0 (not exactly true for the water but close enough for estimation purposes). If the solution is acidic, so that [H+] ≅ 1 mol/kg-soln (pH ≅ 0), this 2.2 Homogeneous and Heterogeneous Reactions would make the equilibrium concentration of [Al+3] (or Al2O3) on the order of 108 molal, which is clearly ridiculous because the molar concentration of pure water is only [ H 2O ] = 1000 1000 = = 55.6 mol /kg 18 M and that of pure Al2O3, [ Al2O3 ] = 1000 = 9.9 mol kg . 102 Nevertheless, it is obvious that, thermodynamically, Al2O3 is quite soluble in acidic solutions. However, the dissolution of Al2O3 in acids occurs so exceedingly slowly that, for all practical purposes, Al2O3 does not dissolve in acids! Why not? Diffusion of the ions in the solution to and from the surface of the solid should occur at about the same rate as the diffusion of the ions that controls the rate of dissolution of NaCl because diffusion coefficients in most liquids are about the same (DL ≈ 10−5 cm2/s)—as will be shown later. However, for Al2O3, the rate of dissolution is controlled by the rate of the surface chemical reaction between the H+ ions in the solution and the aluminum and oxygen ions at the surface of the alumina. This reaction rate is vanishingly small in spite of the fact that the thermodynamics for the dissolution are quite favorable. Here, stirring does not help because the reaction at the alumina surface controls the dissolution rate under all conditions and decreasing the distance that the ions diffuse by stirring does not affect the dissolution rate. 2.1.3 conclusions from ExamplEs These examples of two identical processes for two solids—dissolution in an aqueous solution—illustrate the importance of the combined effects of the relative rates of the surface chemical reaction and diffusion in the liquid. They demonstrate the necessity of studying both chemical reaction kinetics and diffusion processes to understand more broadly the “phase transformation kinetics” of solids. These examples also illustrate two other important points: (1) the thermodynamics of the process must be known before the kinetics can be studied and (2) for reactions in series, sequential steps—in these examples, a surface reaction followed by liquid diffusion—it is the slower of the two steps that controls the overall rate of the dissolution reaction. Therefore, it is essential to investigate both chemical reaction kinetics— particularly at solid surfaces and interfaces—and the macroscopic and atomistic aspects of diffusion in solids, liquids, and gases in order to develop a firm grasp of kinetic processes in materials. 2.2 HOMOGENEOUS AND HETEROGENEOUS REACTIONS There are some differences between “classical” chemical kinetics and kinetics of material processes. For example, chemical kinetics can be defined as (Laidler and Meiser 1999) “that branch of physical chemistry that deals with the rates of reaction and with the factors on which the rate depends: time, temperature, pressure, composition, etc.” With materials, the kinetics are sometimes referred to as kinetics of phase transformations (Porter et al. 2009) because the concern is not only with the rate of a reaction but with the rates of change in a crystal or glass structure, the number of phases, the phase assemblage (microstructure), and the size and/or shape of the material. In all cases, the driving force for the reaction is a reduction or minimization of the Gibbs energy of the system. For solids, the Gibbs energy can take the form of the actual energy for a reaction, an energy difference because of compositional differences, or differences due to stress or surface curvature—surface energy. The goal is to understand how the controllable variables affect the kinetics of a materials process to develop a fundamentals-based model that predicts how the process will respond to changes in the variables. For example, the rates of many solid-state reactions depend exponentially on temperature and linearly on time. With a quantitative model of the system, it is possible to predict which would be economically better to take a commercial process to completion: increase the reaction time, increase the pressure, or increase the reaction temperature. 45 Chapter 2. Introduction to Kinetic Processes in Materials Temperature (°C) 46 1453 Liquid Liquid + solid 1083 Cu Solid solution w/o nickel Ni Temperature (°C) FIGURE 2.4 The copper–nickel phase diagram showing essentially ideal behavior with complete solid solubility. (After Brandes and Brook 1992.) Frequently, classical chemical kinetics is concerned primarily with homogeneous reactions defined as reactions in which the reactants and products are all in the same phase, that is, no phase change or transformation. For example, ª H 2 ( g ) + I 2 ( g ) 2 HI ( g ), reactants and products in the same gas phase ª Fe +2 (solution) + Cl 2 (solution) Fe +3 (solution) + 2 Cl − (solution) in the same liquid phase x Ni(s) + (1 − x) Cu(s) → Ni xCu1‒x(s), because Cu and Ni form a continuous series of solid solutions, same solid phase (Figure 2.4) and similarly x/2 Cr2O3(s) + (1 − x/2) Al2O3(s) → Crx Al2−xO3(s) ª ª 2275 Liquid because Cr2O3 and Al2O3 also form a continuous solid solution as well (Figure 2.5).* Whether it is acceptable to call these last two homogeneous 2050 Solid solution “reactions” is just a question of how far to stretch the concept of a “reaction.” In these latter two cases, there is merely a compositional change, but it is driven by the entropy of mixing of the two end-member compositions— pure Ni and Cu and pure Al2O3 and Cr2O3—and, at the temperatures where w/o Cr2O3 Al2O3 Cr2O3 these reactions occur, they are certainly controlled by solid-state diffusion. FIGURE 2.5 The Al2O3–Cr2O3 phase diagram showHomogeneous reactions in fluids—gases and liquids—are the kinds of reacing essentially ideal behavior with complete solid tions that chemists and chemical engineers primarily deal with. solubility. (After Levin et al. 1964.) In contrast, in materials kinetics, heterogeneous reactions are more common. A heterogeneous reaction is one in which more than one phase is involved in the reaction. The previous examples of CVD of Si and dissolution of NaCl and Al2O3 are examples of heterogeneous reactions. Another familiar example is the oxidation of a metal (Ni) or a nonmetal (silicon carbide (SiC), polyethylene). In the oxidation of a metal such as nickel (or silicon, iron, etc.), olid +s Liquid Ni(s) + 1 O2 (g) NiO(s) 2 three phases are involved: solid Ni, gaseous oxygen, and solid NiO. Figure 2.6 schematically shows this oxidation and the series and parallel kinetic steps that must take place for the oxidation to occur. Oxygen must be (1) transported through the gas phase to the NiO–gas interface where it (2) can react with (3) Ni ions diffusing through the NiO layer to the NiO–gas interface. Another possibility, oxygen molecules are (1) transported to the NiO–gas interface where they (2) separate into oxygen atoms, (3) pick up two electrons to become O−2 ions that then (4) diffuse through the NiO layer to (5) react with the Ni at the NiO–Ni interface. In the first option there are three steps in series and in the second option there are five steps in series. For series steps, the slowest reaction step controls the overall rate. In reality, the slowO2 est step in oxidation is usually the diffusion of either the cation (Ni+2) or the anion (O−2) through the oxide layer that controls the overall rate or reaction, O NiO Ni oxidation in this case. However, the diffusion of nickel out and the diffusion of oxygen in are parallel steps, and the faster of the two controls the rate.† In Ni reality, in the oxidation of nickel—and many metals—it is the diffusion of the cation that is faster and controls the rate of oxidation: at least at elevated temperatures. Oxidation kinetics will be examined more closely later. FIGURE 2.6 Schematic representation of the oxidation of nickel with the formation of nickel oxide on the surface. This represents a heterogeneous reaction because three phases are involved: gas, NiO, and Ni. In addition, the figure shows that the NiO may be formed by Ni2+ ions diffusing out to the NiO–O2 interface or O2− ions diffusing in toward the Ni–NiO interface. * † A few percent of chromium oxide in aluminum oxide is “ruby” if the aluminum oxide is a single crystal. Another parallel step is the diffusion of electrons, which is usually quite fast and does not produce mass transfer for the reaction but is necessary for charge flux balance as will be seen later. 2.3 H2 Gas Carbon concentration Homogeneous Reaction Rates C0 C(x,t) Time Gas CH4 Cf 0 Distance L Steel sheet FIGURE 2.7 Decarburization of a steel sheet of thickness “L” in a hydrogen atmosphere by diffusion of carbon to the surface of the steel sheet to form CH4 in the gas phase. By controlling the [H2]/[CH4] in the gas, the carbon content (thermodynamic activity) can be set to a specific value. The C(x,t) are shown with C0 (the concentration at zero time) and Cf (the final concentration as time goes to infinity). Another example of a heterogeneous reaction is the degassing or decarburizing a steel sheet— which has the identical kinetic model as removal of a solvent from a polymer sheet or drying a cast ceramic tape shown in Figure 2.7. In this case, the reaction is C ( Fe ) + 2H 2 ( g ) CH 4 ( g ) and there are two phases involved, the steel sheet and the gas phase. The reverse of this reaction is carburization—increasing the carbon content—of a steel sheet. Both processes lead to the same model only with different initial carbon contents and gas compositions. 2.3 HOMOGENEOUS REACTION RATES 2.3.1 Why stuDy? Homogeneous fluid reactions are studied mainly by chemists and chemical engineers because many chemical processes of interest to them, such as combustion, occur in a single phase (Laidler and Meiser 1999). These reactions are explored here in order to provide a concrete platform for some common kinetic terminology that can be applied to heterogeneous reactions as well. Consider the following homogeneous gas reaction—one that has been well studied because the kinetics are sufficiently slow so that the reaction can be monitored with modest equipment over easily accessible time periods—hours rather than nanoseconds (Laidler and Meiser 1999): H 2 ( g ) + I 2 ( g ) 2HI ( g ) . The reaction rate is usually defined by the change in concentration or pressure of either one of the reactants or one of the products: d [ H2 ] d [I2 ] 1 d [ HI ] = =− 2 dt dt dt (2.1) where again “[]” denotes “concentration” (mol/cm3, mol/L, mol/m3, etc.). Because these rates are related by the stoichiometry of the reaction, any one of them can be used to measure the rate of reaction. 2.3.2 rEaction orDEr For the gas phase formation of hydrogen iodide (HI), it would not be surprising that the rate of reaction depends on the frequency of collisions between hydrogen and iodine molecules in the gas. As a result, the rate intuitively depends on the concentration, the number of molecules per 47 48 Chapter 2. Introduction to Kinetic Processes in Materials unit volume, of each of these reactants. In this particular reaction, this is a good assumption and fits the reality. However, a word of caution: It is generally true that the dependence of the reaction rate on the concentrations of the reactants is not obvious simply by inspecting the reaction equation. As will be seen, even simple reactions can involve multiple steps that are not reflected in the stoichiometric reaction equation, and it is one of these steps that will control the rate. Referring again to the reaction above, the rate of reaction can be given by Rate = d [H2 ] α β = −k [ H2 ] [I2 ] dt (2.2) where: α + β is the (overall) order of the reaction, where α and β are just numbers and are, but not always, integers α is the order with respect to [H 2] β is the order with respect to [I2]. Usually, the main interest is the concentration of either the products or reactants as a function of time, temperature, etc. and not their rate of appearance or disappearance. Therefore, differential rate equations, such as Equation 2.2, are usually integrated. So the order of the reaction leads to different expressions for the concentrations as a function of the experimental variables, time and concentrations. Zero-, first-, and second-order reactions are examined more closely simply because many elementary reactions follow one of these types of reactions. The reaction rate constant, k, typically has the form of an Arrhenius equation: k = k 0e − Q RT where: Q = the activation energy in kJ/mol k0 = the pre-exponential (the units of k0 depend on the order of the reaction) R = gas constant = 8.314 J/mol-K T = absolute temperature in kelvin (Svante Arrhenius). This exponential temperature dependence of reaction rate constants ensures that the rate of a reaction is a strong function of temperature. The basis for this exponential dependence on temperature and the justification for the activation energy are explored in detail in Chapter 4. To generalize, simplify, and also make the notation more transparent, assume that there are two gases A and B that react as A(g) B(g) with a rate of reaction given by Rate = d [A ] α = −k [A ] dt (2.3) where α is the order of the reaction (with respect to the reactant A). If α = 0, the reaction is zero order; if α = 1, the reaction is first order; and if α = 2, the reaction is second order, etc. As mentioned above, what is usually of interest, is the integrated form of the rate expression to give the concentration of A, [A], as a function of time. 2.3.3 units anD symbols Of course, either gas pressures or concentrations can be used as they are proportional to each other, because of PV = nRT for an ideal gas (all gases in this book are considered to be ideal). So, for some gas A at a pressure P(A), 2.3 n [A ] = V = Homogeneous Reaction Rates P(A) , RT where the units of concentration depend on the units of pressure and those of R. In this book, the format Units(x) is used to signify the units of whatever symbol is inside the parentheses, ().* So, for the Units(R): Units ( R ) = N⋅m N m3 Pa ⋅ m 3 J = = 2 = mol ⋅ K mol ⋅ K m mol ⋅ K mol ⋅ K so that if the pressure is in pascals, then the Units([A]) = mol/m3. However, often, Units (P) = atmospheres (or bars) and sometimes, for convenience, Units([A]) in mol/cm 3 or mol/L are more useful. So, Units(R) = 8.314 3 8.314 Pa m 3 1 atm cm 3 Pa m 3 6 cm = × 10 . × = 82 05 mol K 1.01325 × 105 Pa /atm m 3 mol K mole K or Units( R ) = 8.314 L atm L 8.314 Pa m 3 Pa m 3 1 = × 103 3 × = 0.08205 5 mol K 1.01325 × 10 Pa /atm m mol K mole K are the other two commonly used units for R. Because 1 bar = 105 Pa and 1 atm = 760 torr = 760 mm of Hg, a number of other possible values for Units(R) could be calculated. Note that 1 atm = h( Hg) × ρ( Hg) × g 1 atm = 76.0 cm × 13.6 g /cm 3 × 980 cm s2 × 1 atm = 1.013 × 105 (10 4 )( cm 2 m 2 1 m / 102 cm ) 1000 g kg N = 1.013 bar m2 Also, it should be pointed out that R 8.314 J /mol ⋅ K = 1.38 × 10 −23 J /atom ⋅ K = k B = N A 6.022 × 1023 atoms/mol or Boltzmann’s constant (frequently given by just k, but here kB is used). For example, putting numbers into some of the above expressions, for example, expressing [A] in mol/cm3, [A] = n/V = P/RT, P = 1 atm, and R = 82.04 cm3-atm/mol-K, then at 30°C, [A] = 4.02 × 10 −5 mol/cm 3. Multiplying this by Avogadro’s number, NA = 6.022 × 1023 atoms or molecules per mole, gives η = 2.4 × 1019 molecules/cm3 in a gas at room temperature and 1 atm pressure.† It is interesting to contrast the number of atoms/cm3 in a gas to the number of atoms—or ions or molecules—in a solid or liquid. For example, the density, ρ, of Al2O3 is ρ = 4.00 g/cm3 and its molecular weight is 100.96 g/mol (Haynes 2013), so its molar volume is V( Al 2O3 ) = M 101.96 = = 25.49 cm 3 /mol. ρ 4.00 The number of Al2O3 “molecules” or “formula units” per unit volume is given by η ( Al 2O3 ) = * † 4.00 ρ NA = × 6.022 × 1023 = 2.36 × 1022 cm −3 101.96 M “Units(x)” is used to designate the “units of x” while “[x]” designates the “concentration of x.” The Greek letter eta, η, is used for number concentrations in this book, or number density, simply because n and N are used to represent so many other quantities and η at least looks like an n. The units of η are, Units(η) = atoms/cm3 or atoms/m3. Of course, the number of molecules per unit volume is proportional to the pressure for an ideal gas. 49 50 Chapter 2. Introduction to Kinetic Processes in Materials so the number of oxygen ions per cm 3, η(O) = 3 η(Al 2O3) = 7.09 × 1022/cm 3 and the number of aluminum ions per cm 3, η(Al) = 2 η(Al 2O3) = 4.72 × 1022/cm 3. Note that for virtually all condensed phases—solids and liquids—the number of atoms, ions, or molecules per cm 3 is always something times 1022 . So the number density in condensed phases is about three orders of magnitude higher than the number density in gases at room temperature and 1 atm pressure. The number density in condensed phases does not vary much with temperature and reasonable pressures. In contrast, of course, the number density in gases varies significantly with pressure and temperature. 2.4 ZERO-ORDER REACTION Going back to Equation 2.3, for a zero-order reaction, α = 0, so d[A ] = −k dt (2.4) so Units(k) = mol/cm3 s, if the concentration of A is in moles per cm3. This is readily integrated to give [ A ] = − kt + C where C is just an integration constant. When t = 0, [A] = [A]0, the starting concentration of A, which, after substitution, gives the simple linear relation [A] = [A]0 − kt (2.5) and the reaction goes to completion ([A] = 0) when t = [A]0/k as shown in Figure 2.8. [A]0 2.5 [A] 0 [A]0/k Time FIGURE 2.8 The concentration of reactant A, [A], as a function of time for a zero-order reaction with a reaction rate constant k and an initial concentration at zero time of [A]0. [B] [A]0 [A] FIRST-ORDER REACTION 2.5.1 intEGratED Equation First-order reactions are particularly important because they occur frequently in MSE. For the A B reaction in Section 2.3.2, for a first-order reaction, the differential equation that needs to be solved is d [ B] d[A ] = −k [A ] = − . dt dt Note that the units for k are Units(k) = s−1 and are different from those for the zero-order reaction. Integrating, ln [ A ] = − kt + C or or [B] [A] 0 0 Time FIGURE 2.9 The concentrations of reactant A, [A], and product B, [B], for the first-order reaction A → B as a function of time with initial concentrations of [A]0 and zero for A and B, respectively. (2.6) [ A ] = Ce− kt where C is a constant. At t = 0, [A] = [A]0 = C, which leads to [ A ] = [ A ]0 e− kt . (2.7) The concentrations of both A and B are plotted as a function of time in Figure 2.9. An easy way to obtain k from experimental data is, of course, to plot the concentration of A on a semilog plot as shown in 2.5 2.5.2 fraction rEactED A few commonly used terms need defining. The fraction reacted can be calculated for any order reaction. In the specific case of a first-order reaction, call the fraction unreacted, f U, then f U = (amount of reactant remaining)/ (initial amount of reactant) or fU = [A ] [ A ]0 = e − kt (2.8) log10[A]0 Slope = −k/2.303 0 Time FIGURE 2.10 Concentration of the reactant A, [A] on a semilog plot versus time for a first-order reaction. From the slope, the value of the reaction constant k can be determined. [A]0 is again the initial concentration of A. and the fraction reacted, f R, is fR = 1 − fU = 1 − [A ] [ A ]0 = 1 − e − kt (2.9) or fR = [ A ]0 − [ A ] = 1 − e− kt . [ A ]0 2.5.3 thE half-lifE of a rEaction Another expression relating to the extent of a reaction is the half-life or t1/2 , which is the amount of time for one-half of the original reactant disappear or react, or the time necessary for the reaction to go half way to completion. The half-life is very important in nuclear decay reactions because they are all first-order reactions and characterized by their half-lives, which gives an indication of how intensively radioactive they are. For a first-order reaction, the time for [A] = [A]0/2 is the half-life, or [A ] [ A ]0 = 0.5 = e − kt1/2 (2.10) where t1/2 is the half-life of the reaction. Therefore − kt1 2 = ln 0.5 = −0.693, so t1/ 2 = 0.693/k . For example, if k = 10−3 s−1, then t1/2 = 693 s. 2.5.4 rElaxation timE One final term requiring definition is the relaxation time, τ, or the time for the reaction to proceed to 1/e = 1/2.718 = 0.37 of its final value—zero for Equation 2.7. That is [A]/[A]0 = e−1, which implies that kτ = 1 or τ = 1/k. For example, if k = 10−3 s, then τ = 103 s and [ A ] = [ A ]0 = e− t / τ . * 51 log10[A] Figure 2.10. Note that the plot log10[A] versus time is a straight line with a slope of −k/2.303.* (Note that if x = 10log10 x, then ln x = log10 x × ln 10. Because e = 2.718, 10 = 2.7182.303, so ln 10 = 2.303 and ln x = 2.303 log10x and log10x = ln x/2.303.) First-Order Reaction (2.11) Note: Never, never, ever make a semilog plot with natural logarithm values on the vertical axis if the results are going to be presented to someone else such as in a publication, report, or paper. The reason for this is that everyone is familiar with quantities to the base 10, but few can translate quantities to the base e into base 10 values. For example, if one of the points is on the vertical axis at −6 on a log10 plot, then the value at this point is 10 −6, or one part per million. Everyone has a reasonable idea of what 10−6 means. However, if this were a natural logarithm plot, then the −6 would be e−6 = 2.718−6 = ????, whatever this is! However, the penalty that you have to pay for plotting an exponential function as log10 on a semilog plot is that the slope is not –k as it would be on natural logarithm plot but –k/(ln 10) = –k/2.303. 52 Chapter 2. Introduction to Kinetic Processes in Materials 2.5.5 ExamplE of first-orDEr rEaction: cocl2 DEcomposition Carbonyl chloride, COCl2, phosgene, was introduced during the First World War as a poison gas but today is used in large quantities in the production of certain polymers. COCl2 gas undergoes decomposition—at elevated temperatures—by the following reaction: COCl2 ( g ) CO ( g ) + Cl 2 ( g ) . The equilibrium constant, Ke, is given by Ke = p ( CO ) p ( Cl 2 ) p ( COCl 2 ) and Ke = 217 at 1200 K (Roine 2002). At this temperature, thermodynamics indicates that essentially all of the COCl2 is decomposed at equilibrium. How far the reaction goes to completion can be estimated by assuming that p(CO) = p(Cl2) ≅ 1 bar, so p(COCl2) ≅ 1/217 = 4.6 × 10−3 bar, or about 99.5% of the COCl2 is decomposed. At this point, the kinetics become interesting.* This is a first-order reaction with a first-order reaction constant (NIST Kinetics Database): k = k0 e − Q RT = 1.45 × 1014 e − 345 kJ/mol RT s −1. (2.12) At 1200 K, Equation 2.12 gives k = 1.45 × 1014 exp(−(345, 000/(8.314 ×1200))) s−1 = 0.139 s−1, which gives a half-life of t1/2 = 0.693/0.139 = 4.99 s, and a relaxation time of τ = 1/k = 7.19 s, a fairly rapid reaction. In contrast, COCl2 is pretty stable at low temperatures and at 300 K, (NIST-JANAF Thermochemical Tables; NIST Kinetics Database) p ( Cl 2 ) p ( CO ) = K e = 1.12 × 10 −12. p ( COCl 2 ) (2.13) For example, if at the start of the reaction, pure COCl2 is enclosed in a fixed volume at 300 K at one bar pressure and is allowed to go to equilibrium, the pressure of COCl2 does not change much because of the small equilibrium constant, Equation 2.13, and the amount of Cl2 and CO can be estimated from pe (CO) = pe (Cl 2 ) = (1.1210 −12 )1/ 2 ≅ 1 × 10 −6 bar, or only about one part per million (ppm) of the COCl2 decomposes. This is a sufficiently small amount that it would be doubtful if there were much interest in the kinetics of decomposition. Making it even less interesting, the first-order reaction constant is calculated to be k = 1.45 × 1014 exp( − 345,000/(8.314 × 1200)) s −1 = 1.23 × 10 −46 s −1 ! Not only does it not decompose very much, but it would take a long time for even this small amount of decomposition (1 year ≅ 3 × 107 s, and the age of the universe is only 13.8 billion years or 4.14 × 1017 s).† 2.6 RADIOACTIVE DECAY AND RELATED NUCLEAR REACTIONS 2.6.1 iDEal first-orDEr rEaction Radioactive decay is the prime example of a first-order reaction because the number of disintegrations per unit time, dm*/dt, (Units(dm*/dt) = becquerel (Bq), 1 Bq = one disintegration per second), is directly proportional to the amount of radioactive material present, m*, that is, * † The NIST Kinetics Database provides a great deal of information on gas reaction kinetics, whereas the Thermochemical Tables are a primary source of thermodynamic data for gases, liquids, and solids. These thermodynamic data are also included in many available software packages (HSC Chemistry Software) that utilize the NIST data and other data sources to calculate a variety of thermodynamic properties for a large number of compounds and thermodynamic data for many reactions. However, it should be pointed out that the database suggests that the parameters in the reaction rate constant, k0 and Q, are only valid between 1400 and 2000 K, both of which are above the temperatures used in this example. So the extrapolation of the given data down to the temperatures of interest may not give very accurate results. Nevertheless, these are the best data available, so there is little choice but to use them: a situation frequently faced by a materials scientist or engineer. Also note the very large value of Q (345 kJ) that produces the very strong temperature dependence of the reaction rate constant. 2.6 Radioactive Decay and Related Nuclear Reactions dm*/dt = −km*. Furthermore, radioactive decay and other nuclear reactions are extremely important in MSE considering the critical role that radioactive materials play in nuclear power generation, nuclear waste disposal, and the use of radioactive isotopes to study reactions and transport in materials. Therefore, a short discussion of some important nuclear reactions and nuclear chemistry is germane to the overall theme of materials kinetics as well as examples of ideal first-order reactions. 2.6.2 uranium isotopEs 4 The first example is the decay of 238 92 U by the emission of an alpha particle, a helium nucleus, 2 He, 234 * 238 along with 4.25 MeV (million electron volts of energy) to 92Th. U is the most common isotope of uranium found in uranium ore deposits and represents 99.3% of natural uranium with 235U, the fissionable isotope—the one that can be split by neutrons while generating large amounts of energy— present at about 0.7%. The half-life of 4.51 billion years is shown for the decay to 234Th over the arrow. The 234Th is also radioactive and undergoes several disintegrations, eventually decaying to one of the stable lead isotopes such as 208 82 Pb. 238 92 9 .51×10 year U 4 → 23490Th + 42 He + 4.25 MeV Th → eventually to Pb. 234 90 Uranium 235 also undergoes alpha particle decay with a half-life of about 700 million years: 8 .0×10 year 4 U 7 → 231 90Th + 2 He + 4.68 MeV Th → eventually to Pb . 235 92 231 90 Uranium is usually “enriched” to about 5% 235 92 U so that a nuclear chain reaction obtained by fission can be sustained in a nuclear reactor—“reactor grade uranium.” For a nuclear weapon, the enrichment needs to be much higher, greater than 85%—“weapons grade uranium.” This enrichment in the past was accomplished with UF6 gas in very large—several kilometers on a side—gaseous diffusion plants, in which the 235UF6 and 238UF6 were separated by the small difference in their gaseous diffusion rates that depend on 1/M1/2, where M is the molecular weight—as is discussed in Chapters 8 and 9. Such plants were hard to hide from satellite observation because they were so large—diffusion distances had to be long to separate gases whose diffusion coefficients varied by only about 0.4%. However, today the enrichment can be done with high-speed centrifuges in a much smaller and harder to detect facility. Hence, the concern when a country announces an enrichment program: What is the level of enrichment it intends, reactor grade, or weapons grade? On the other hand, an unannounced program is even more insidious, because it may go undetected. The 238U left over is called “depleted uranium” and because of its high density—19.05 g/cm3—it is used for armor piercing projectiles. It can be placed in a reactor to produce fissionable 239Pu that can also be used in a reactor or a weapon. In a reactor, 238U undergoes the following reaction and decay sequence to produce 239Pu, a man-made element: .4 minute − U 23 → 239 93 Np + β + 1.28 MeV 238 92 U + 01 n → 239 93 .35 day − → 239 Np 2 94 Pu + β + 0.723 MeV. 239 92 A β− particle is a high-energy electron resulting from the decay of a neutron into a proton, which carries most of the energy of the reaction. 239Pu also undergoes radioactive decay with emission of an alpha particle similar to 238U, * 239 94 , 000 year 4 Pu 24 → 235 92 U + 2 He + 5.2 MeV 235 92 U → eventually to Pb. 1 eV = 1 electron volt = energy to move the charge on one electron across a potential of 1 volt = 1.602 × 10−19 C × 1 V = 1.602 10−19 J since 1 V = 1 J/C and for 1 mole = 1eV × NA = 1.602 × 10−19 × 6.022 × 1023 = 96,472 J/mol ≅ 100 kJ/mol on the order of the energy of an atomic bond. Physicists like to deal in eV per atomic reaction event, although chemists more commonly use kJ/mol when talking about moles of reactants and products. Materials people use whatever suits the situation best. 53 54 Chapter 2. Introduction to Kinetic Processes in Materials Even with an apparently long half-life of 24,000 years, the rate of energy generated in the disintegration of 239Pu, makes a piece of pure plutonium metal actually warm to the touch. 2.6.3 raDioisotopE poWEr sourcEs On the other hand, this heating can be useful and another radioactive isotope of plutonium, 238Pu, is used as a radioisotope heat source because the half-life is short enough to provide sufficient power to reach temperatures in excess of 1000°C from the reaction: 238 94 year Pu 86 → 42 He + 234 92 U + 5.59 MeV Such heat sources are made from PuO2 spheres or cylinders encased in a welded iridium or platinum–rhodium shell and used for satellite—particularly military—and deep space probes where solar panels do not provide enough power, Figure 2.11 (radioisotope power systems). Several of the modular units shown in Figure 2.11 are used, in order to supply the necessary power for a satellite. Each of the iridium-encased PuO2 modules contain about 34 Ci* of 238 94 Pu, that generates about 1 W of heat. This heat is used to generate electricity with thermoelectric elements (thermocouples) and the entire subassembly is called a radioisotope thermoelectric generator (RTG) or radioactive power source. The United States has launched many satellites with these power sources, with powers ranging from a few hundred watts, to a few kilowatts with some containing tens of pounds of plutonium. The New Horizons mission to Pluto in 2015 used a radioisotope power system. Supposedly, the PuO2 will not get dispersed into the environment even if the satellite were to be aborted because of the iridium encapsulation. There have been a few accidents, but purportedly no radioactive 238Pu was released to the environment (Radioisotope Power Systems). The concern with plutonium is that, because the isotopes have significant decay rates and emit energetic alpha particles, only small concentrated amounts—micrograms—can do considerable tissue damage, particularly in the lungs, that potentially lead to cancer. 2.6.4 nuclEar rEactors anD fission proDucts The other concern with plutonium is that it can be separated chemically from the uranium and fission products in nuclear reactor fuel—a much simpler process than the physical processes necessary for uranium enrichment—providing the operating personnel can be protected from the extremely high level of radiation from partially used nuclear fuel. Also, the process can be carried out in small facilities that can be easily hidden, if the intent is to use the plutonium for something other than reactor fuel. It only takes a few 100 cm3 of 239Pu to make a nuclear weapon! As a result, the United States decided in the 1970s that it would not pursue nuclear fuel reprocessing to recover fissionable Iridium metal cladding Plutonium-238 dioxide fuel pellet (heat source) Fuel clads in fueled position Aeroshell Carbon fiber sleeve Graphite impact shell FIGURE 2.11 General purpose heat source module showing how the iridium-clad 238 94 PuO 2 pellet heat sources are inserted into various carbon parts to form the module. NASA photograph (Radioisotope Power Systems). The original color photograph was color inverted, converted to grayscale, and contrast-enhanced with Photoshop®. * Note, 1 Ci = 1 Curie = 3.7 × 1010 disintegrations/s = 3.7 × 1010Bq, which is roughly the number of disintegrations per second from a gram of radium, the element that was discovered by Marie and Pierre Curie and the unit was named after them. 2.6 Radioactive Decay and Related Nuclear Reactions plutonium, unused 235U and 238U from nuclear power reactors for fear of proliferation of nuclear weapons, because of the availability of 239Pu. However, from an energy generation perspective, with the geological abundance of 238U, that can be converted into 239Pu, there is virtually an unlimited supply of energy from the nuclear power potential in the uranium ore. The potential for energy from nuclear reactions comes from the fission process of the uranium and plutonium isotopes that can easily fission. Both 235U and 239Pu are fissionable materials in that when bombarded with neutrons their nuclei split into two isotopes of similar, but not equal, atomic weights, plus more neutrons, plus a large amount of energy, which is the basis for nuclear power generation: 235 92 with a similar reaction for such as 90Sr, 131I, and 127Cs: 239 143 1 U + 01 n → 90 38 Sr + 54 Xe + 3 0 n + 205 MeV Pu. In both cases, several radioactive fission products are produced, 90 38 .1 year Sr 28 → 9039Y + β− + 0.546 MeV hour − Y 64 → 90 40 Zr + β + 2.95 MeV 90 39 90 Zr is a stable isotope, meaning that it does not undergo further radioactive decay; 131 53 .07 day − I 8 → 131 54 Xe + β + 0.97 MeV 127 55 hour + Cs 62 → 127 54 Xe + β + 2.1 MeV 127 54 .4 day Xe 36 → 127 53 I + γ + 0.44 MeV and 131Xe is a stable isotope; Here, the 127I is stable and the last reaction occurs by an “electron capture” process in which an orbital electron enters the nucleus dropping the number of protons from 54 to 53. The β+ is a high-energy positron—antielectron. These radioactive fission products are unwelcome additions to the human body because iodine concentrates in the thyroid and strontium in bones, and their high-energy emissions lead to broken chemical bonds, cell damage, and, potentially, cancer. 2.6.5 raDiocarbon DatinG A useful example of radioactive decay and a first-order reaction is the dating of objects from the decay of carbon-14 (Taylor 2000; “Radiocarbon Dating”). Willard Libby did the first work on radiocarbon dating in 1949 when he was a professor at the University of Chicago, research for which he received the Nobel Prize in Physics in 1960 (Willard Libby). The natural abundances of carbon isotopes are 12 6 C 98.89% 13 6 C 1.11% 14 6 C 1× 10 −12. The concentration of 146 C is estimated from literature data (Taylor 2000). Here 12C and 13C are stable, whereas 14C decays as 14 6 year C 5730 → 147 N + β− + 0.156 MeV (2.14) and so its concentration can be measured by counting the beta particle radiation. Given a sample of carbon, by counting the rate of disintegration, the concentration of 14C, [14C], can be determined. Of course, with a half-life of 5730 years, virtually all of the 14C that existed when the Earth was formed would have long ago decayed to the stable 14N, given the 4.5 billion year age of the Earth. However, 55 56 Chapter 2. Introduction to Kinetic Processes in Materials C is constantly being regenerated in the upper atmosphere by cosmic rays that generate neutrons by nuclear reactions that react with nitrogen in the atmosphere, 14 14 7 N + 01 n → 146 C + 11 H and forms 146 CO2, and the 14C in the atmosphere reaches a steady-state value that has been more or less constant over time (about 1 part per trillion of stable carbon, 1 part in 1012).* Corrections have been made by other techniques such as tree-ring dating—which gives the 146 C as a function of time because each tree ring counts as 1 year. Atomic bomb testing during the 1950s and 1960s almost doubled the concentration of carbon 14, but it now has dropped to close to its earlier—more constant—level. A living organism that is constantly in contact with the atmosphere and, using its biological processes to emit or absorb CO2, will maintain in its body this constant concentration of 14 C in equilibrium with the atmosphere. However, when the organism dies, it no longer exchanges CO2 with the atmosphere, and the 14C in its remains will start to decay. As a result, by measuring the 14C in something that previously had been alive, the time since its death can be determined from 14 6 C = e− kt 14 6 C 0 (2.15) where 146 C is the constant 14C concentration in the atmosphere and k = −ln(0.5/5730) = 1.21 × 10−4 0 years, as noted earlier. So if a mammoth tusk is found that has a carbon-14 ratio of 0.25, then from above, t = −ln(0.25/1.21 × 10−4) = 11,460 years. So the mammoth lived and died around 9500 BC. Today, mass spectrometry is also used to find the concentration of 14C, so a smaller amount of material can be used. For example, in 1988, radiocarbon dating was used to attempt to determine the age of the Shroud of Turin, the venerated and reputed burial cloth of Jesus, which many believe shows his face and body outline, shown in Figure 2.12. The analysis gave results that suggested that the Shroud was only about 690 years old, about the time when it first appeared on the scene in the early 1300s. It was dated from the flax used to make the cloth, and the same age was found independently by three different laboratories. The radiocarbon data suggest that the shroud was, in reality, a painting made in the early 1300s. However, these results have been disputed for a number of reasons including the possibility of repairs to the shroud over time and that the sampling was done on cloth added more recently as a repair. Another suggestion is that bacteria were present in the cloth in more recent times, and their presence led to a higher 14C content and a younger apparent age than the actual age. Several other suggestions have been made, as well, that could explain a higher initial 14C than is normally present in the atmosphere leading to an apparent younger age for the cloth (Wilson 1998; Turney 2006; Shroud of Turin). Clearly, rather than giving definitive results in this case, the radiocarbon dating of the Shroud probably increased the mystery and speculation surrounding its origin. For example, the image on the shroud is essentially a negative image! It is hard to explain how a fourteenth century painter could have made a painting that was the exact negative of the actual image as shown in Figure 2.13. That the image was a negative was not discovered until the late 1800s after the discovery of photography. Another example of recent radiocarbon dating was showing that the mummified human found in the snow and ice in the Alps in 1991—Ötzi, after the region where the body was found—died in 3300 BC. When the body was found, the discoverers thought it was someone who had died recently in a skiing or climbing accident. The artifacts found with the body, such as a 99.7% copper axe, have led some to speculate that he might have (a) (b) been involved with copper smelting and have given anthropologists a great deal of information about the inhabitants of Europe in a period for which no FIGURE 2.12 Photographs of the Shroud of Turin. (a) positive. (b) negative. Photo from Wikipedia history of the region exists (Ötzi the Iceman). Commons, public domain (Shroud of Turin_2). Original color image converted to grayscale and contrast-enhanced with Adobe Photoshop.® * This is an example of a steady-state concentration of an intermediate reaction product of two series reactions that will be discussed in Chapter 3. TiO2 dissolution rate (moles/cm2-h) 2.7 Importance of First-Order Reactions in Materials 2.5 × 10−7 2.0 × 10−7 1.5 × 10−7 1.0 × 10−7 5.0 × 10−8 0.0 0.0 0.2 0.4 0.6 0.8 1.0 1.2 1.4 1.6 HF concentration (moles/l) FIGURE 2.13 Linearized rate of TiO2 dissolution at 95°C in a [HCl] = 0.5 mole/L solution as a function of the [HF]. (Data from Bright and Readey 1987.) A mammoth tusk found on an island of the Southern California coast is undergoing radiocarbon dating to determine its age and whether or not it is, indeed, a mammoth tusk (Chang 2009). Finally, radiocarbon data were used to find the source of the “brown cloud” of pollution that covers much of South Asia. The question was as follows: Is the brown cloud due to burning fossil fuels or to burning forests and grasslands? If fossil fuels were the source, then the 14C content in the soot contributing to the brown cloud would be low. If the 14C content were near the normal atmospheric concentration, then the source would be the burning of forests and grasslands. The conclusion was the latter and so those concerned with improving the environment in the area now know which problem to address (Fountain 2009). Another example is the dating of some pages of the Quran, found in a British university library in 2015, to 568–645 about the time when Muhammad received the revelations for the Quran, between 610 and 632, the year he died (Bilefsky 2015). In spite of some controversy over these conclusions and their implications, many feel that this discovery demonstrates that the Quran has existed in its present form since the time of Muhammad. In summary, radiocarbon dating is a good example of first-order kinetics and shows how these kinetics can be applied to determine the age of carbon-containing materials to address a number of archaeological, anthropological, materials, and societal questions. 2.7 IMPORTANCE OF FIRST-ORDER REACTIONS IN MATERIALS First-order reactions are important in materials because many gas–solid and liquid–solid reactions are found to be first order. This is likely because the surface or interfacial reactions involve many series steps and it is only a single—perhaps final—first-order step involving one reactant species that determines the rate of reaction. This conclusion is drawn from many empirical results on surface reactions with solids. An example is the dissolution of TiO2, titanium dioxide—titania, in HF solutions, which is very similar to the dissolution of Al2O3 in HF solutions discussed in Section 2.12 (Bright and Readey 1987). The overall reaction is TiO2 (s) + 6HF(solution) TiF62 − (solution) + 2H + (solution) + 2H 2O(solution) and from the stoichiometry of the reaction, it would be impossible to predict the order of the reaction. Certainly, 6 HF molecules are not going to simultaneously converge at a single Ti4+ surface ion to produce the TiF62− ion. The probability of such a multimolecular event is just too low. However, as shown in Figure 2.13, the order of the reaction with respect to the [HF] is very close to 1.0 because the dissolution rate is essentially proportional to the HF concentration, [HF]. These approximate first-order kinetics suggest that the rate-controlling step may be the “squeezing” in of the last HF molecule at a titanium site on the surface to reduce the surface bond between the 57 Chapter 2. Introduction to Kinetic Processes in Materials TiO2 crystal surface Ligand “squeezing” in Attached ligands HF HF HF HF HF 58 Ti4+ ion FIGURE 2.14 Postulated possible mechanism for the first-order rate dependence on [HF] for the dissolution of TiO2 in 0.5 molar HCl solutions at 95°C. The figure shows an isolated Ti4+ ion at the surface of the dissolving TiO2 surrounded by several attached HF ligands (the exact nature of and number of the ligands is not known, possibly F−) and one final HF trying to “squeeze” into this coordination sphere that would provide the necessary bonding for the Ti4+ ligands (TiF62−?) to leave the surface and enter the solution. (After Bright and Readey 1987.) titanium ion—with its other surrounding ligands—to allow it to leave the surface and enter the solution. This is illustrated in Figure 2.14. 2.8 CHAPTER SUMMARY This chapter introduces several concepts about reaction kinetics. Is the reaction controlled by transport— diffusion—or an actual chemical reaction? Reactions can occur within single phases, homogeneous reactions, or more common in MSE, heterogeneous reactions involving more than one phase: the deposition of Si by CVD and the oxidation of a metal are examples. When discussing actual chemical reaction kinetics, the order of the reaction is important because knowing it can lead to understanding the actual atomistics of the chemical reactions taking place. The dissolution of TiO2 in HF is presented as a possible example of this. Zero-order reactions are the ones that depend neither on the concentrations of the reactants nor those of the products and are physically not very likely. First-order reactions are important because they occur frequently, particularly for heterogeneous reactions. In this case, the reaction rate is proportional to one of the reactants with the reaction rate constant, k, the proportionality constant. The reaction rate constant follows an Arrhenius equation (Svante Arrhenius), namely, it is exponentially temperature dependent—strongly temperature dependent—and the rate is largely defined by the value of the activation energy, Q. The concepts of fraction reacted, half-life, and relaxation time are introduced for first-order equations. Radioactive decay is used as an example of first-order reactions in radioisotope power sources and radiocarbon dating along with some nuclear chemistry associated with fissionable materials for nuclear reactors. The next chapter goes further into reaction kinetics discussing secondorder reactions, multistep reactions including serial and parallel reactions, and reactions that go to equilibrium. In reality, most reactions—even simple gas phase homogeneous reactions such as the formation of water vapor from hydrogen and oxygen—consist of multiple series and parallel reactions that preclude analytic solution and dictate the need for numerical computation of concentrations and reaction rates. EXERCISES 2.1 The reaction rate constant for a zero-order reaction for the decomposition of another liquid dissolved in water is given by k = k 0exp( − Q/RT) for the reaction A → B. a. Write the equation for the reaction rate for the decomposition of A. b. Give the units of k0 if the units of the reactant concentration [A] are millimol/cm3. Exercises 2.2 2.3 2.4 2.5 2.6 c. If Q = 30 kJ/mol and k0 = 10−2, calculate the reaction rate in millimol/liter at 25°F. d. Calculate how long it takes for the reaction to go to completion if [A]0, the reactant concentration at time zero, is one mole per liter. e. Neglecting any temperature effects on the density of water, which can be assumed to be 1.0 g/cm3, calculate the number of moles per cm3 of water in pure water. f. Assuming that the molar volumes of water and the reactant are the same, calculate the m/o, w/o, and v/o of A in water at 25°F at the start of the reaction if the molecular weight of the reactant is 60 g/mol. a. The reaction rate constant k (k = k 0exp( − Q/RT)) for a first-order reaction is 5.00 × 10−3 s−1 at 500°C and is 10.00 s−1 and 1000°C. Calculate the activation energy for this reaction. b. Calculate the preexponential term, k0, for the reaction rate constant and give its units. c. Calculate k at 750°C. d. Calculate the relaxation time for this reaction. e. Calculate the half-life of this reaction. f. Make a plot of log10(rate) versus 103/T (K−1) from 100°C to 1200°C. g. Calculate how long it takes (hours) at 750°C for the unreacted fraction to be 0.001. h. If the reaction is A → 2B, plot the concentrations of A and B versus time from time zero up to the time that was calculated in (g). A well-known generalization (for back of the envelope calculations) for biochemical reactions near room temperature (300 K) is that their rates double for every 10 K rise in temperature. a. Determine the activation energy (J/mol) for such reactions implied by this rule. b. Calculate the value of the activation energy in eV/molecule. a. The half-life for a first-order reaction is 1000 s. Calculate the reaction rate constant (s−1) for this reaction. b. Calculate the relaxation time (s) for this reaction. a. The half-life for a first-order reaction is 1200 s. Calculate the reaction rate constant (s−1) for this reaction. b. Calculate the relaxation time (s) for this reaction. c. Plot the fraction unreacted versus time for 0–10,000 s. Indicate the half-life and the relaxation time on your plot. 4 a. Plutonium-238, 238 94 Pu, spontaneously decays by alpha particle, 2 He, emission with a halflife of 86 years. The nuclear disintegration reaction is 238 94 b. c. d. e. f. g. h. Pu → 234 92 U + 42 He + 5.234 Mev. This disintegration rate is sufficiently fast to produce enough heat to be used as a power source in satellites. Calculate the first-order reaction rate constant for the nuclear disintegration of plutonium-238. Calculate the number of becquerels at time = 0 with one mole of pluonium-238. Calculate the number of curies at time zero in one mole of pure 238 94 Pu. Calculate the rate of energy generated in the plutonium-238 (watts) for one mole of plutonium-238 at time zero. Calculate how long (years) it will take for the rate of energy generation to drop to 10% of its initial value. If the 238 94 Pu were in the form of PuO2 rather than pure plutonium, calculate the number of curies in 5 cm3 of PuO2 at time zero if the density of PuO2 is 11.5 g/cm3. Calculate the number of watts that this 5 cm3 of 238 94 Pu-containing PuO2 generates. If this 5 cm 3 of PuO2 were perfectly insulated, calculate how long it takes (hours) for the 5 cm 3 of PuO2 to reach its melting point of 2390°C if its molar heat capacity is 75 J/mol K. 59 60 Chapter 2. Introduction to Kinetic Processes in Materials 2.7 A reaction obeys the following stoichiometric equation: A + B = Z. The rates of formation of Z at various concentrations of A and B are given in the following table. [A] (mol/L) 2.00 × 10−2 6.50 × 10−2 1.10 × 10−1 [B] (mol/L) 4.20 × 10−2 4.80 × 10−2 1.22 × 10−1 Rate (mol/L-s) 3.53 × 10−9 4.87 × 10−8 9.00 × 10−7 Determine the values of α, β, and k in the rate equation: rate = k [A]α[B]β. Give the units for k as well. You may use programs such as Excel and Mathematica, or by hand, to get the solution. Just clearly indicate what operations were performed, that is, copy that part of the Excel spreadsheet or the Mathematica page that shows the calculations. 2.8 In 2012, what were thought to be the bones of King Richard III of England were found under a parking lot in England and later confirmed by DNA evidence in 2014 that the bones were indeed his. The bones were dated by radiocarbon dating and confirmed that the date of death of the skeleton was 1485, the date of death of the king. Calculate the ratio of carbon-14 remaining in the bones. 2.9 If the number of disintegrations per minute per gram of carbon produced by pyrolyzing a piece of recently cut wood is 12.5 dis/min g, calculate the fraction of 14 C in carbon of age zero if the half-life of 14 C is 5730 years. (The wood is assumed to have an age of zero.) REFERENCES Bilefsky, D. 2015. Pieces of the Quran, Perhaps as Old as the Faith. New York Times, July 23. Brandes, E. A. and G. B. Brook, eds. 1992. Smithells Metals Reference Book, 7th ed. Oxford, UK: Butterworth-Heinemann. Bright, E. and D. W. Readey. 1987. Dissolution Kinetics of TiO2 in HF-HCl Solutions. J. Am. Ceram. Soc. 70(12): 900–907. Chang, A. 2009. Possible Mammoth Tusk Found on So Cal Island. San Diego Tribune, January 14. Fountain, H. 2009. Study Pinpoints The Main Source of Asia’s Brown Cloud. New York Times, January 27. Haynes, W. M. Editor-in-Chief. 2013. CRC Handbook of Chemistry and Physics, 94th ed. Boca Raton, FL: CRC Press. HSC Chemistry Software. http://www.hsc-chemistry.net/. Laidler, K. J. and J. H. Meiser. 1999. Physical Chemistry, 3rd ed. Boston, MA: Houghton Mifflin. Levin, E. M., C. R. Robbins, and H. F. McMurdie. 1964. Phase Diagrams for Ceramists. Columbus, OH: The American Ceramic Society. NIST-JANAF Thermochemical Tables. http://kinetics.nist.gov/janaf/. NIST Kinetics Database. http://kinetics.nist.gov/kinetics. Ötzi the Iceman. Wikipedia. http://en.wikipedia.org/wiki/%C3%96tzi_the_Iceman. Porter, D. A., K. E. Easterling, and M. Y. Sherif. 2009. Phase Transformations in Metals and Alloys, 3rd ed. Boca Raton, FL: Taylor & Francis Group. Radiocarbon Dating. Wikipedia. http://en.wikipedia.org/wiki/Radiocarbon_dating. Radioisotope Power Systems. http://solarsystem.nasa.gov/rps/types.cfm. Roine, A. 2002. Outokumpu HSC Chemistry for Windows, Ver. 5.11, Thermodynamic software program, Outokumpu Research Oy, Pori, Finland. Shroud of Turin. Wikipedia. http://en.wikipedia.org/wiki/Shroud_of_Turin. Shroud of Turin_2. Butko, Andrew. 2005. USPD photograph of PD piece of art. https://commons.wikimedia. org/wiki/File:Shroud_of_Turin_001.jpg. Svante Arrhenius. Wikipedia. http://en.wikipedia.org/wiki/Svante_Arrhenius. Taylor, R. E. 2000. Fifty Years of Radiocarbon Dating. Am. Sci. 88(1): 60–67. Turney, C. 2006. Bones, Rocks, and Stars. London: MacMillan. Willard Libby. Wikipedia. http://en.wikipedia.org/wiki/Willard_Libby. Wilson, I. 1998. The Blood and the Shroud. New York: Free Press. 3 Second-Order and Multistep Reactions 3.1 3.2 3.3 3.4 3.5 3.6 Introduction Second-Order Reactions 3.2.1 One Reactant 3.2.2 Two Reactants 3.2.3 Pseudo First-Order Reaction First-Order Reaction That Goes to Equilibrium and Not Completion Second Order ⇔ Second Order That Goes to Equilibrium 3.4.1 General 3.4.2 Equilibrium 3.4.3 Specific Example 3.4.4 The General Solution 3.4.5 Numerical Solution Parallel and Series Reactions 3.5.1 Introduction 3.5.2 Parallel Reactions 3.5.3 Series Reactions 3.5.3.1 Exact Solution 3.5.3.2 Steady-State Assumption 3.5.3.3 Example: Nuclear Decay Complexity of Real Reactions 3.6.1 Hydrogen Iodide 3.6.2 Chain Reactions 61 62 62 62 63 65 66 68 68 69 70 72 72 74 74 74 76 76 77 78 78 78 79 62 Chapter 3. Second-Order and Multistep Reactions 3.6.3 Chain Polymerization 3.6.3.1 Mechanism 3.6.3.2 Rate of Polymerization 3.6.4 Chain Branching Reactions 3.7 Summary Appendix Exercises References 3.1 79 79 80 81 81 82 91 93 INTRODUCTION This chapter introduces second-order reactions as examples of higher order reactions. Different initial concentrations of reactants in second-order reactions leads to quite complex results. In contrast, starting with equal initial concentrations greatly simplifies the results and the steps leading to them. This suggests that when trying to deduce the mechanism of the reaction from the kinetics, it is much easier if the initial concentrations are equal. This is also true when back reactions are considered. Reactions with back reactions go to equilibrium—the usual case for most reactions—and not to completion. Analytical solutions for first-order forward and back reactions are quite easily obtained. However, things become much more mathematically tedious when the forward or back reaction, or both, is a second-order reaction. Nevertheless, modeling a second-order equation that goes to equilibrium is useful largely because such solutions are rarely found elsewhere. The chapter then examines parallel reactions demonstrating that the faster or fastest step in parallel reactions determines the overall reaction rate and product concentrations. For series reactions, it is shown that the situation is the opposite in that the slower or slowest reaction step controls the overall reaction rate. These results are important and apply to diffusion controlled processes as well as reaction control. In addition, the steady-state approximation for two reactions in series has several important applications. Finally, most reactions depend on a combination of several series and parallel steps that are best solved by numerical techniques rather than attempting to obtain analytical expressions for the changes in concentrations with time and temperature. 3.2 3.2.1 SECOND-ORDER REACTIONS One Reactant Again, assume the simple reaction of A k → B but in this case, the reaction is second order with respect to [A]; that is, d [ B] d[A ] 2 =− = −k [A ] dt dt Slope = k this integrates to − 1/[A] 1 = − kt + C [A ] and if [A] = [A]0 when t = 0, then 1/[A]0 Time FIGURE 3.1 reaction. (3.1) 1/[A] versus time for a second-order 1 + [ A ]0 kt 1 1 = + kt = [ A ] [ A ]0 [ A ]0 which has the form y = mx + b, and is linear when plotted as 1/[A] versus temperature as is shown in Figure 3.1. Rearranging to obtain [A] explicitly, 3.2 Second-Order Reactions 1.0 k = 0.001 cm3/mole-s [B] Concentration (mol/cm3) 0.8 0.6 0.4 [A] 0.2 0.0 0 500 1000 1500 2000 2500 3000 Time (sec) FIGURE 3.2 Concentrations versus time for a second-order reaction of A → B that will eventually go to completion for k = 10 −3 cm3 mols. [A ] [ A ] = 1 + A 0 kt [ ]0 (3.2) as shown in Figure 3.2. If [B]0 = 0, then [B] is the amount of A reacted, so [A ] [ B] = [ A ]0 − [ A ] = [ A ]0 − 1 + A 0 kt [ ]0 or, [ A ] kt [ B] = 1 + A0 kt [ ]0 2 (3.3) also shown in Figure 3.2 with k = 10 −3 cm 3 mol s .* 3.2.2 twO Reactants Assume that there are two reactants, A and B reacting to give a product, C: A + B k →C (3.4) where C can be one or more products. Also assume that the reaction is first order with respect to both A and B resulting in overall second-order kinetics: d [A ] = − k [ A ][ B] dt (3.5) and is the case for the reaction of hydrogen and iodine to produce hydrogen iodide mentioned in Chapter 2†: H 2 (g) + I 2 (g) 2HI(g) and d [H2 ] = − k [ H 2 ][ I 2 ] . dt For this reaction, there is a relation between the stoichiometry of the reaction and the kinetics because one mole of hydrogen gas and one mole of iodine gas react to give two moles of hydrogen iodide gas, and the kinetics are first order with respect to each of the reactants. This is not * † Note that the units of k in this case are Units(k) = cm3/mol s or m3/mol s or L/mol s. However, some references (Laidler 1987) suggest that the kinetics for this reaction are more complex than simple second order. 63 64 Chapter 3. Second-Order and Multistep Reactions unexpected if a collision in the gas phase between a hydrogen molecule and an iodine molecule is necessary for the reaction to occur. This would be a bimolecular reaction and, most importantly, the collision between the hydrogen and iodine molecules to form HI would represent the mechanism of the reaction, which is a principal reason that reaction kinetics are studied: to determine the mechanism or model of the reaction rate to whatever level of detail desired, as a function of temperature and concentration or in more detail such as how the electron orbitals interact. However, a simple relation between the reaction stoichiometry, kinetics, and mechanism are not the usual case and most reactions may involve many steps that lead to more complex reaction kinetics. For example, the very similar reaction of hydrogen and bromine to produce hydrogen bromide does not follow simple second-order kinetics such as the formation of hydrogen iodide (Moore and Pearson 1981). Nevertheless, reaction kinetics are frequently studied to determine the molecular mechanism of the reaction but with the caveat (Moore and Pearson 1981, 3) “that the mechanism cannot be predicted from the overall stoichiometry. This point is emphatically reiterated in the case of gasphase formation of water from its elements: 2H2(g) + O2(g) → 2H2O(g). The reaction certainly does not involve simultaneous, trimolecular collisions of 2H2 with O2. As many as 40 elementary steps have been suggested for the mechanism, and about 15 steps are needed to account for the slow reaction under simplified conditions”. The formation of HBr, HCl, and H2O, all of which exhibit more complex reaction kinetics will be examined later. Back to the reaction in Equation 3.4, d [ A ] d [ B] d [C] = =− dt dt dt (3.6) where the concentrations of A and B can be expressed as [ A ] = [ A ]0 − ([ A ]0 − [ A ]) [ B] = [ B]0 − ([ B]0 − [ B]) ( = [ B]0 − [ A ]0 − [ A ] (3.7) ) [ B] = ([ B]0 − [ A ]0 ) + [ A ] because the amount of B produced must be the same as the amount of A reacted at any given time and the initial concentrations of A and B at time = 0 are [A]0 and [B]0, respectively. If the initial concentrations are the same, [ B]0 = [ A ]0 , then Equation 3.5 becomes Equation 3.1 and [ A ] = [ B] are given by Equation 3.2. If they are not equal, things become a little bit more complex but the equations can easily be integrated to give (Appendix A.1.1, where it is assumed that [ B]0 > [ A ]0 simply for convenience while doing the algebra) [A ] = ( [ B ] − [ A ] ) [ A ] e ([ ] ) − B 0 −[ A ]0 kt 0 0 0 [ B]0 − [ A ]0 e ([ ) − B]0 −[ A ]0 kt (3.8) and [ B] = ([ B]0 − [ A ]0 ) [ B]0 −([ B]0 −[ A ]0 ) kt [ B]0 − [ A ]0 e (3.9) 3.2 Concentrations 2.0 Second-Order Reactions [B]0 1.5 [B] 1.0 [A]0 [C] 0.5 0.0 [A] [C]0 0 10 20 30 40 50 Time (s) 60 70 80 FIGURE 3.3 Second-order reaction with two reactants A and B going to completion—all of A is reacted— to C. Note that there are no units on concentration in this and subsequent figures in this chapter because they depend either on the units of k or on the units of concentration chosen which need not be specified. and, of course, from Equation 3.6 [C] = [ A ]0 − [ A ] . (3.10) These three concentrations are plotted in Figure 3.3 for initial values of [B]0 = 2.0, [A]0 = 1.0, and [C]0 = 0 with k = 0.05. (Note: the Units(k) = Units([A]/s) so in Figure 3.3 [and subsequent figures] the “concentration” axis is whatever units of concentration chosen and that will determine the units of k. For example, in Equation 3.8 Units([A]) = mol/cm3, then Units(k) = cm3/mol s. If the Units([A]) = mol/m3, then Units(k) = m3/mol s, etc.) There are two extreme possibilities for this result: [ B]0 ≅ [ A ]0 , that is, starting concentrations of the two reactants are essentially the same, and Equations 3.8 and 3.9 give the expected result, Equation 3.2, as shown in Appendix A.1.2: [A ] ≅ 1 + [ A ]0 . [ A ]0 kt 3.2.3 PseudO FiRst-ORdeR ReactiOn The other possibility is that [ B]0 [ A ]0, that is, the starting concentration of B is much larger than that of A, and Equation 3.8 gives [ A ] ≅ [ A ]0 e−[B] kt 0 (3.11) which is referred to as a pseudo first-order reaction (Houston 2001). For example, if the HI reaction were being carried out with a great excess of hydrogen compared to the concentration of iodine, then the hydrogen concentration essentially does not change and leads to apparent first-order kinetics but with a modified reaction rate constant, k[B]0. When experimentally determining the reaction kinetics, the reaction rate constant, and the reaction mechanism, it clearly makes sense to start with the same initial concentrations of A and B to make the reaction kinetics simpler and easier to analyze. However, there may be constraints in an industrial process, in which A and B are—by necessity—not equal. In that case, the more complex kinetics of Equations 3.8 through 3.10 must be used, and the main reason that they are included here is to raise awareness of this possibility. 65 66 Chapter 3. Second-Order and Multistep Reactions 3.3 FIRST-ORDER REACTION THAT GOES TO EQUILIBRIUM AND NOT COMPLETION More often than not, a reaction will not go to completion, that is, [A] → 0, but will reach some equilibrium concentration.* A first-order reaction in which A → B that does not go to completion will eventually reach some concentration, [A]e, in equilibrium with a product concentration, [B]e, where the subscript e denotes the equilibrium concentrations. This implies that there is a back reaction of B → A, that could also be first order (but does not have to be), so 1 A k →B (3.12) 2 B k →A and the rate of reaction is the forward reaction plus the back reaction to give d[A ] dt , d [A ] = − k1 [ A ] + k 2 [ B ] . dt (3.13) Again, for the sake of simplicity, assume that at t = 0, [B]0 = 0 and [A] = [A]0 so that [B] = [A]0 − [A]. The rate of reaction Equation 3.13 becomes d [A ] = − k1 [ A ] + k 2 [ A ]0 − k 2 [ A ] dt = − ( k1 + k 2 ) [ A ] + k 2 [ A ]0 (3.14) k2 = − ( k1 + k 2 ) [ A ] − [ A ]0 . k k + 1 2 At equilibrium, the reaction rate must go to zero, so d [A ] = 0 = − k1 [ A ]e + k 2 [ B]e . dt (3.15) [ B]e = [ A ]0 − [ A ]e [ A ]e [ A ]e (3.16) Rearranging Equation 3.15 gives = k1 = Ke k2 because [ B] = [ A ]0 − [ A ], the amount of B is the amount of A reacted, and where Ke is the equilibrium constant for the reaction, which—of course—can be calculated from the thermodynamics for the reaction. Solving Equation 3.16 for [A]0, k 2 [ A ]0 − k 2 [ A ]e = k1 [ A ]e k 2 [ A ]0 = ( k1 + k 2 ) [ A ]e or [ A ]0 = * k1 + k 2 [ A ]e k2 Nuclear decay being an exception in that the reactions do go to completion; that is, the concentration of the reactant goes to zero. 3.3 First-Order Reaction That Goes to Equilibrium and Not Completion and substituting this for [A]0 in Equation 3.14 gives d [A ] = − k1 [ A ] + ( k1 + k 2 ) [ A ]e − k 2 [ A ] dt (3.17) d [A ] = − ( k1 + k 2 ) [ A ] − [ A ]e . dt ( ) Let x = [ A ] − [ A ]e, so that Equation 3.17 takes the form dx /x = − ( k1 + k 2 ) dt and integrating x 1 ∫ x dx = ln x − ln x 0 x0 x = ln − ( k1 + k 2 ) t x0 and noting that [A] = [A]0 when t = 0 gives [ A ] − [ A ]e [ A ]0 − [ A ]e = e − ( k1 + k 2 ) t (3.18) which is the rather nonsurprising result—after a lot of fun algebra—that the reaction stops when equilibrium is reached and reverts to the equation for a first-order reaction that goes to completion when [A]e = 0, Equation 2.5, [ A ] = [ A ]0 e − kt . Of course k1 = k2Ke from Equation 3.16 and k1+ k2 can be written as just k and the time dependence is again exponential, as shown in Figure 3.2. It is perhaps surprising that k should be a constant, that is, independent of concentration. What this means is that the original equation for the reaction rate must include the equilibrium concentration in the differential equation when the reaction goes to equilibrium (which it almost always does with the notable exception of nuclear decay) because the reaction must stop at equilibrium. As a result, the original first-order rate expression could have been written more generally as d [A ] = − k [ A ] − [ A ]e dt ( ) (3.19) and give the same result, Equation 3.18. In general, the concentration of B, [B], is the initial concentration of B, [B]0, plus the amount of A reacted to form B, [A]0 − [A], so [ B] = [ B]0 + ([ A ]0 − [ A ]) = [ B]0 − ([ A ] − [ A ]0 ) and makes the equilibrium concentration of B, [ B]e = [ B]0 + ([ A ]0 − [ A ]e ) or ( [ B] − [ B] ) = − ( [ A ] − [ A ] ) 0 e 0 e and [ B] − [ B]e = [ B]0 + ([ A ]0 − [ A ]) − [ B]0 − ([ A ]0 − [ A ]e ) [ B] − [ B]e = − ([ A ] − [ A ]e ) so the equivalent expression for [B] can be obtained simply by substituting these relations between [B] and [A] in Equation 3.18 to give 67 Chapter 3. Second-Order and Multistep Reactions [A]0 1.0 Concentration (arbitrary units) 68 0.8 [B]e [B] 0.6 [A] 0.4 [A]e 0.2 [B]0 0 FIGURE 3.4 k = 0.04 s−1 20 40 60 Time (s) 80 100 First-order reaction that goes to equilibrium—one that has a first-order back reaction. [ B] − [ B]e [ B]0 − [ B]e = e − kt . (3.20) Furthermore, Equation 3.13 can be written more generally as d [A ] = − k1 [ A ] − [ A ]e + k 2 [ B] − [ B]e dt ( ) ( ) ( ) ( ) = − k1 [ A ] − [ A ]e − k 2 [ A ] − [ A ]e ( = − ( k1 + k 2 ) [ A ] − [ A ]e (3.21) ) and Equation 3.19 is obtained as before. Also, Equation 3.21 shows immediately that k = k1 + k2. Figure 3.4 shows the concentrations as a function of time for a first-order reaction that goes to equilibrium. Equations 3.19 and 3.21 show that the rate of reaction, d[A]/dt is equal to the product of a kinetic factor, k, and a thermodynamic factor, ([A] − [A]e). The latter is a thermodynamic factor because it depends on the equilibrium value of [A], namely [A]e, that can be manipulated by the overall composition of the fluid phase while keeping k fixed. The reaction rate constant is, of course, exponentially temperature dependent. This product of a kinetic factor and a thermodynamic factor whose value determines the overall rate of a reaction or phase transformation will appear repeatedly in discussions of other kinetic processes. 3.4 SECOND ORDER ⇔ SECOND ORDER THAT GOES TO EQUILIBRIUM 3.4.1 GeneRal Whether the reaction is a second order forward and second order back, or first order forward and second order back, or second order forward and first order back, the results are all similar and the procedures used to get the solutions are essentially the same for all three cases. The reason for this is that the rates of reaction, dx/dt (x here is concentration to minimize symbol complexity), are all proportional to a second-order polynomial in x. From the results in Section 3.3.2, it is tempting to write for a second-order reaction, 3.4 2 d [A ] = − k [ A ] − [ A ]e . dt ( ) Second Order ⇔ Second Order That Goes to Equilibrium (3.22) Unfortunately, this is incorrect and solutions to second-order equations that go to equilibrium unfortunately are more complex. The detailed procedure carried out in Appendix A.2 works for second order ⇔ second order, second order ⇔ first order, and first order ⇔ second order because all involve the solution of quadratic equations. In Appendix A.2.4, the general solution for second order ⇔ second order is found. The reaction is assumed to be the simple reaction: AB or d [A ] 2 2 = − k1 [ A ] + k 2 [ B ] . dt (3.23) To minimize the notation, let [A] = x, and [A]0 = x0 and [B]0 = 0 so that Equation 3.23 becomes dx 2 = − k1x 2 + k 2 ( x 0 − x ) . dt (3.24) Now this is a relatively simple differential equation to solve because the variables are separable, all the “xs” on the left, and “ts” on the right, so that standard integration gives a solution without recourse to special differential equation solution techniques. 3.4.2 equilibRium At equilibrium, x = x e so Equation 3.24 becomes − k1x 2e + k 2 ( x 0 − x e ) = 0 2 or k1x 2e = k 2 ( x 0 − x e ) ± 2 k1 x 0 − x e . = k2 xe Note the ± sign in front of the term on the left that is necessary because the square root is being taken. This leads to two mathematically possible equilibrium values as will be seen. At this point, the initial concentration of A, x0, could be obtained and substituted into Equation 3.24 and eliminated as was done for the first-order reaction in Section 3.3. However, this does not help much to solve this problem. In any event, the equilibrium concentration can be obtained from xe ± k1 xe = x0 k2 k ± k1 x e 2 = x 0 k2 which leads to k2 x e = x 0 k 2 ± k1 (3.25) 69 70 Chapter 3. Second-Order and Multistep Reactions and the algebra is already getting messy and the differential equation, Equation 3.24, has yet to be solved. The general solution, involving much algebra, is left to the Appendix. 3.4.3 sPeciFic examPle To make things simpler, and hopefully more transparent, start with a specific case of k1 = 2, = k 2 1,= and x 0 1. So Equation 3.25 becomes k2 1.0 x e = x 0 = 1.0 ± k k 1.0 ± 2 2 1 which gives x e = 0.41421 and − 2.41421. Clearly, xe must be greater than zero so the first xe = 0.41421 must be the equilibrium value. (Note that if k2 > k1, then xe > x0, which is physically impossible if [B]0 = 0 as assumed.) The differential equation, Equation 3.24 with these numerical values, becomes, dx 2 = −2x 2 + (1 − x ) dt dx = −2x 2 + 1 − 2x + x 2 dt (3.26) dx = −x 2 − 2x + 1. dt This is easy to solve by finding the roots to the quadratic equation on the right and one of these roots will be the equilibrium concentration of A from which the equilibrium concentration of B can be calculated. So x=− or x= b ± b2 − 4ac 2a 2± 4+4 −2 x = −2.41421 and 0.41421. Not surprisingly, the roots of the quadratic equation are the equilibrium concentrations. As a result, Equation 3.26 can be written in terms of its factors: dx = ( 2.41421 + x ) ( 0.41421 − x ) . dt (3.27) Just as a check, multiplying these two factors gives 2.41421× 0.41421 − 2.41421x + 0.41421x − x 2 0.99999 − 2x − x 2 which is pretty close to 1 − 2x − x 2 ! The integration of Equation 3.27 is now straight forward. First, separate variables: dx = dt. ( 2.41421 + x ) ( 0.41421 − x ) (3.28) 3.4 Second Order ⇔ Second Order That Goes to Equilibrium Now separate the denominator into two terms that are easily integrated, the method of partial fractions, 1 A = + B ( 2.41421 + x ) ( 0.41421 − x ) ( 2.41421 + x ) ( 0.41421 − x ) multiplying both sides by the denominator of the left-hand side A ( 0.41421 − x ) + B ( 2.41421 + x ) = 1 and equate the left- and right-hand factors of x and the constant gives −Ax + Bx = 0 or A = B because there is no x-term on the right-hand side, and 0.41421A + 2.41421A = 2.82842A = 1 or = A 1= 2.82842 B. Equation 3.28 can now be written as dx + dx ( 2.41421 + x ) ( 0.41421 − x ) = 2.82842 dt and integrated to ln ( 2.41421 + x ) − ln ( 0.41421 − x ) = 2.82842t + C where C is just a constant of integration. Taking the exponent of both sides of the equation gives ( 2.41421 + x ) = C′e2.82842t ( 0.41421 − x ) where C′ is just another constant. When t = 0, x = x0, so C′ = ( 2.41421 + x 0 ) = ( 2.41421 + 1) = −5.8284 ( 0.41421 − x 0 ) ( 0.41421 − 1) and the solution becomes ( 2.41421 + x ) = −5.8284 × e2.82842t = D ( 0.41421 − x ) (3.29) where at any given time t the right-hand side of this equation is a constant D. It is now necessary to manipulate Equation 3.29 to get “x” explicitly. So, Equation 3.29 can be written as ( 2.41421 + x ) = D × ( 0.41421 − x ) 2.41421 + x = 0.41421× D − Dx x(1 + D) = 0.41421× D − 2.41421 x= 0.41421× D − 2.41421 1+ D x= 0.41421 − 2.41421 D 1 D +1 and replacing Equation 3.29 for D gives the sought for solution x= 0.41421 + 0.41421× e −2.82842 t 1 − 0.17157 × e −2.82842 t (3.30) 71 Chapter 3. Second-Order and Multistep Reactions 1.0 0.9 k1 = 2.0 k2 = 1.0 [A]0 = 1.0 0.8 [A] 0.7 Concentration 72 [B]e = 0.58579 0.6 0.5 0.4 0.3 [A]e = 0.41421 [B] 0.2 0.1 0.0 0.0 0.2 0.4 0.6 0.8 1.0 1.2 Time 1.4 1.6 1.8 2.0 FIGURE 3.5 Second-order reaction with a second-order back reaction A B with the specific values for the constants in the equation: [A]0 = 1.0, [B]0 = 0, k1 = 2.0, and k 2 = 1.0. The calculated points and the equilibrium concentrations are shown. when t = 0, x = 0.99999 which is pretty close to 1.0 and when t = ∞, x = xe = 0.41421. The concentration of B, [B], is just [ B] = x 0 − x and [B]e = 0.58579. Both [A] and [B] are plotted in Figure 3.5. 3.4.4 the GeneRal sOlutiOn Following exactly the same procedure as in Section 3.4.3 for the specific case, the general solution to Equation 3.24 is solved in Appendix A.2.4 and is x= x0 k 2 / 1− (( ( ){ k 2 + k1 1 + e )( k1 − k 2 / ( ) − 2 x 0 k 2 k1 t k1 + k 2 )) ( e } ) − 2 x 0 k 2 k1 t . (3.31) 3.4.5 numeRical sOlutiOn Given the amount of algebra and elementary calculus involved in obtaining the general solution to a relatively simple differential equation of importance to kinetics, what about higher order reactions and noninteger orders? In general, it is generally neither reasonable nor possible to solve such problems analytically—at least not in the time it might take—so numerical techniques are used. As simple example of one of these numerical procedures is the so-called Euler’s method (Celia and Gray 1992; Blanchard et al. 2012) that involves treating the derivative as a ratio of differences: dx dt = ∆x ∆t . This is an example of a finite difference approximation that can be used to solve both ordinary and partial differential equations under certain conditions (Celia and Gray 1992; Kee et al. 2003). It is a particularly useful technique because the solutions can frequently be obtained with simple spreadsheet calculations. For example, consider the specific differential equation given in Equation 3.26 dx = − x 2 − 2x + 1 dt (3.32) which required a fair amount of algebra and calculus to get the final result, Equation 3.30 with the initial condition that x = 1.0 at t = 0. Putting Equation 3.32 into difference form, 3.4 Second Order ⇔ Second Order That Goes to Equilibrium ∆x ( x t + ∆t − x t ) = = −x 2t − 2x t + 1 ∆t ∆t and rearranging gives ( ) x t + ∆t = x t + ∆t −x 2t − 2x t + 1 . (3.33) That is, for a uniform time-step, Δt, the value of x t +∆t at the next time-step, is just the value at the previous time-step, xt, plus Δt times the value of the differential equation at the previous time-step. For the plots of [A] and [B] in Figure 3.5 from Equation 3.30, a relatively large time-step of Δt = 0.05 s was used to calculate these curves. This is somewhat larger than desirable for the evaluation by Euler’s method but it will be used to illustrate the method. So, because x0 = 1.0, x1 at Δt is calculated by x1 = x 0 + ∆t ( −x 20 − 2x 0 + 1) x1 = 1.0 + 0.05( −1 − 2 + 1) x1 = 0.9 and x2 at t = 2Δt, x 2 = x1 + ∆t ( −x12 − 2x1 + 1) x 2 = 0.9 + 0.05( −(0.9)2 − 2(0.9) + 1) x 2 = 0.9 − 0.0805 x 2 = 0.8195 and so on. The values of x(t) at these two times calculated with the exact solution, Equation 3.30, are x1 = x(0.05) = 0.9092 and x2 = x(0.1) = 0.8342, less than 2% difference between the numerical and exact solution. This difference could be made considerably smaller with a smaller Δt. Figure 3.6 shows how the finite difference approximation can be easily and quickly calculated with a spreadsheet. The first column is just n increasing going down the column as far as desired; the second column is time, nΔt, where Δt is fixed (but does not have to be); and column three, x is calculated with Equation 3.33. A powerful feature of a spreadsheet solution is only the first row for n = 0 needs to be inserted and then simply copied vertically down to a desired end point. Also, Δt can be introduced as a separate constant and varied to get as close as possible to the analytical solution. Figure 3.7 gives plots of [A] dx = −x2 − 2x + 1 Differential equation dt 2 xn+1 = xn + Δt(−xn − 2xn + 1) Differential equation n Time x 0 0 x0 1 1Δt x1 2 .. . 2Δt .. . x2 .. . n nΔt n+1 .. . (n+1)Δt .. . 2 x1 = x0 + Δt(−x0 − 2x0 + 1) xn xn+1 ... 2 xn+1 = xn + Δt(−xn − 2xn + 1) Spreadsheet columns FIGURE 3.6 Spreadsheet layout for the numerical calculation of the concentrations as a function of time, for the specific reaction equation plotted in Figure 3.5, with Euler’s finite difference method of approximation. The values of xn from the difference equation are plotted in the x column. 73 Chapter 3. Second-Order and Multistep Reactions 1.1 1.0 0.9 Concentration 74 0.8 [A] exact 0.7 [A] Euler approximation 0.6 0.5 0.4 0.3 0.0 [A]e = 0.41421 0.2 0.4 0.6 0.8 1.0 1.2 1.4 1.6 1.8 2.0 Time FIGURE 3.7 The exact concentration [A] from Figure 3.5 plotted along with Euler’s method approximation of [A] with the time-step Δt = 0.05. The calculated points are shown for both curves. Although a smaller time-step would have made the approximation closer to the analytical solution, even with this relatively large time-step, the curves do not differ by more than 2% at any given time. for both the exact and a spreadsheet numerical solutions to Equation 3.32 with Δt = 0.5. The two solutions are pretty close and get closer at longer times because, in this case, the derivative is getting smaller. Clearly, the numerical solution is the easier and faster way to solve this relatively simple problem and numerical solutions become mandatory as the kinetics become more complex, as indeed they do, even for simple reactions. 3.5 3.5.1 PARALLEL AND SERIES REACTIONS intROductiOn Even more complex situations can be modeled such as parallel or series reactions, any order, with or without back reactions, with and without initial product concentrations, and so on, depending on the level of enthusiasm for doing algebra and solving ordinary differential equations! However, a brief look at simple first-order parallel and series reactions is useful for reasons other than just obtaining a solution. 3.5.2 PaRallel ReactiOns Consider first a parallel reaction such that A can react to form either B or C. As mentioned in Section 3.1, this leads to the important result that the faster of two parallel reactions will determine how quickly the reaction goes to completion and how much B and C are formed. For this parallel reaction, assume no back reactions and that the initial concentrations of B and C are both zero ([B]0 = [C]0 = 0) to avoid hiding the principles in the forest of the notation: 1 2 A k → B and A k → C so d [ B] d [C] = k1 [ A ] and = k 2 [ A ] so dt dt d [A ] d [ B] d [ C ] =− − = − ( k1 + k 2 ) [ A ] dt dt dt (3.34) 3.5 Parallel and Series Reactions and therefore [ A ] = [ A ]0 e−( k + k )t . 1 (3.35) 2 Substitution of Equation 3.35 in the rate expression for B gives d [ B] − k +k t = k1 [ A ] = k1 [ A ]0 e ( 1 2 ) dt and integrating ∫ [ B] 0 d [ B] = k1 [ A ]0 t ∫e − ( k1 + k 2 ) t 0 [ B] = k Similarly, dt to give { } k1 [ A ]0 1 − e−( k1 + k2 )t . 1 + k2 (3.36) d [C] − k +k t = k 2 [ A ] = k 2 [ A ]0 e ( 1 2 ) and is integrated to give dt [C] = k { k2 [ A ]0 1 − e−( k1 + k2 )t k + 1 2 } (3.37) which clearly shows that the faster reaction—the larger k—controls the rate of reaction and determines which product is preferentially created, as shown in Figure 3.8. This is a very general result: for parallel reactions the faster (fastest if more than two products) controls the overall rate of the reaction. For the k-values used to plot Figure 3.8, [C] is always about 20% of [B]. 1.0 [A]0 k1 = 0.02 k2 = 0.005 Concentration 0.8 [B] [A] 0.6 0.4 [C] 0.2 0.0 0 20 40 60 Time (s) 80 100 FIGURE 3.8 Concentrations as a function of time for parallel reactions that go to completion: A → B and A → C. For parallel reactions, the faster (fastest) of the rates, k1, determines the rate of the overall reaction and the relative amount of the major product, B. 75 Chapter 3. Second-Order and Multistep Reactions 3.5.3 seRies ReactiOns 3.5.3.1 Exact Solution 1 2 Consider a series reaction A k → B k → C in which the slower of the two reactions—the smaller of k1 and k2—determines the overall rate, or [C](t). The rates of reactions are given by d [A ] = − k1 [ A ] dt d [ B] = k1 [ A ] − k 2 [ B ] dt (3.38) d [C] = k 2 [ B] . dt The solutions to these three simultaneous ordinary differential equations are given in many physical chemistry texts without the mathematical details that require some techniques for solving differential equations (but given in Appendix A.3): [ A ] = [ A ]0 e− k t (3.39) 1 [ B] = [ A ]0 k1 k 2 − k1 [C] = [ A ]0 1 + k (e − k1t − e− k2 t ) (3.40) 1 k1e − k 2 t − k 2e − k1t . 2 − k1 ( ) (3.41) Figure 3.9 shows a case where k1 k 2 so A quickly forms B, which reacts more slowly to form C. Figure 3.10 shows the opposite case where k2 ≫ k1 so that hardly any B is present at any time because it quickly reacts to form C. In Appendix A.3.5, it is shown that it is the smaller of the two “ks”—the slower reaction—controls the overall reaction rate. Note that [C](t) does not depend on which of the two rates is the faster, which is obvious from Equation 3.41 because the reversal of k1 and k2 gives the same rate equation for [C]. For example, with k1 = 0.05 and k2 = 0.3 as in Figure 3.10, Equation 3.41 becomes 1.0 [A]0 [C] 0.8 Concentration 76 k1 = 0.3 s−1 [B] k2 = 0.05 s−1 0.6 0.4 [A] 0.2 0.0 0 20 40 60 80 100 Time (s) FIGURE 3.9 Series reaction in which the reaction of A to B, k1, is considerably faster than the reaction of B to C, k2. Because the rate of reaction of A to B is fast, A quickly reacts to form B and it is the slow reaction of B going to C that controls the reaction. As a result, the slower controls the rate of the overall reaction to C. 3.5 Parallel and Series Reactions 1.0 [A]0 [C] Concentration 0.8 k1 = 0.05 s−1 k2 = 0.3 s−1 0.6 0.4 [A] 0.2 0.0 [B] 0 20 40 60 Time (s) 80 100 FIGURE 3.10 Same series reaction as in Figure 3.9 only the reaction rates are reversed. Now B converts quickly to C and it is the slower rate of A reacting to B that controls the overall rate of reaction: the formation of C. Note also that the concentration of C, [C], as a function of time in both this figure and Figure 3.9 are the same because the slower reaction controls the overall rate, the concentration of C as a function of time. [C] = [ A ]0 1 + 0.3 − 0.05 ( 0.05e−0.3t − 0.3e−0.05t ) = [ A ]0 (1 + 4 ( 0.05e−0.3t − 0.3e−0.05t ) ) . 1 Reversing k1 and k2 so that k1 = 0.3 and k2 = 0.05, the equation becomes [C] = [ A ]0 1 + 0.05 − 0.3 ( 0.3e−0.05t − 0.05e−0.3t ) = [ A ]0 (1 + 4 ( 0.05e−0.3t − 0.3e−0.05t ) ) 1 which—not too surprisingly—is the same as the previous equation and [C](t) is the same in both Figures 3.9 and 3.10. However, [B](t) depends strongly on which is the faster reaction. In the limit of k2 ≫ k1, Equations 3.31 and 3.32 become respectively: [ B] ≅ [ A ]0 k1 e− k t = k1 1 k2 k2 [A ] [C] ≅ [ A ]0 (1 − e− k t ) . 1 (3.42) (3.43) These results clearly show that the rate of reaction that determines the concentrations of A, B, and C depend on the smaller reaction rate constant, k1: that is, for a series reaction, the slower (slowest) reaction controls the rate of the overall reaction. 3.5.3.2 Steady-State Assumption An approach to get an approximate solution to these series reaction equations, Equation 3.38, is to make the steady-state assumption for the concentration of B. It is extremely important to note that steady-state and equilibrium have two very different meanings in reactions even though the terms are often used—incorrectly—interchangeably. The term equilibrium means that the reaction has stopped. In contrast, steady-state implies that concentrations are no longer changing with time but the reaction is still taking place and may be a long way from equilibrium. The steady-state assumption is particularly useful for analyzing complex reactions having multiple series and parallel steps (Laidler 1987). That is, 77 78 Chapter 3. Second-Order and Multistep Reactions d [ B] = k1 [ A ] − k 2 [ B ] = 0 dt (3.44) this leads immediately to Equations 3.42 and 3.43 and is, of course, tantamount to the assumption that k 2 ≫ k1, for which, as Equation 3.42 shows, [B] does not vary rapidly with time because it depends on e − k1t and k1 is small. Of course, Equations 3.42 and 3.44 are mathematically inconsistent, but the result is a reasonable approximation if k 2 ≫ k1. 3.5.3.3 Example: Nuclear Decay In a nuclear reactor, the roughly 235 92 U enriched to 4% or 5% of the uranium present undergoes fission generating energy and several neutrons. Some of these neutrons are captured by the 96% 238 92 U to give 239 239 239 92 U, which decays to 93 Np and then to 94 Pu by the following reactions: 239 92 .5 min − U 23 → 239 93 Np + β + 1.28 MeV 239 93 .35 d − → 239 Np 2 94 Pu + β + 0.23 MeV 239 94 , 000 yr 4 Pu 24 → 235 92 U + 2 He + 5.23 MeV. (3.45) If a reactor is operating at a constant power level for a long period of time, typically several years, 239 then the amount of 239 92 U will stay at some small time-independent value as will the amount of 93 Np because of their relatively short half-lives. On the other hand, the amount of 239 94 Pu in the reactor core will continually increase. However, it too will reach a steady-state concentration because 239 94 Pu is also fissionable and can be used as fuel in nuclear power reactors, as it is in France. Nevertheless, it would 239 be expected that the relative steady-state concentrations of 239 92 U and 93 Np, which from Equations 239 3.44 and 3.45, would be 239 93 Np / 92 U = 2.35 d / 23.5 min = 720. 14 Of course, the concentration in the atmosphere of radioactive 6 C used for radiocarbon dating is a perfect example of a steady-state concentration between its formation by cosmic rays and its own nuclear decay. 3.6 COMPLEXITY OF REAL REACTIONS 3.6.1 hydROGen iOdide In all of the previous discussions, the kinetic expressions are for homogeneous reactions and are therefore most applicable to gases and liquids but they can be applied to heterogeneous reactions and solids as well. The objective has been to introduce some of the terminology and types of reactions that can take place and the effects of time and concentration on the reactions. The focus has been on homogeneous gas-phase reactions because they have been the most studied and they are—in principle—the simplest type of reaction. The questions are “How complex are real gas reactions?” and “Where can data be found on gas-phase reaction kinetics?” The answer to the second question is that the National Institute of Standards and Technology (NIST) of the U.S. Department of Commerce has an online database NIST, Kinetics Database (NIST 2013) of gas reaction kinetic parameters. These data show that the hydrogen iodide reaction is indeed a simple second-order reaction: d[H 2 ] = − k [ H 2 ][ I 2 ] dt (3.46) with the reaction rate constant given by k = Aexp(−EA/RT), which is the typical exponential temperature dependence of the reaction rate constant discussed in Chapter 4. In this case, the preexponential term k0 = A = 3.22 × 10−10 cm3/mol s which means that the concentrations would be expressed in 3.6 Complexity of Real Reactions mol/cm3. EA = Q, the activation energy in this case is EA = 171 kJ/mol.* However, the reality even for most gas-phase reactions is that they are not simple single-step reactions but consist of many serial and parallel steps. 3.6.2 chain ReactiOns Similar to the reaction for the production of HI, the formation of HCl can be written as H 2 (g) + Cl 2 (g) 2HCl(g). However, for this reaction the kinetics are more complex (Kee et al. 2003). In fact, the kinetics of this reaction represent a chain reaction. In a chain reaction, there is an initiation step, a chainpropagating step, and a termination step. For this reaction Initiation: Cl 2 Cl i + Cl i Propagation: Cl i + H 2 HCl + H i and Cl 2 + H i HCl + Cl i Termination: Cl i + Cl i Cl 2 and Cl i + H i HCl. Clearly, the propagation step leads to a continuation of the reaction by producing hydrogen and chlorine radicals (the species with the “dot”) to react with Cl2 and H2, respectively, to continue the reaction to HCl.† In principle, the differential equations for the concentrations of all of these species can be developed and, because the reaction rate constants for the reactions exist in the NIST Kinetics database, the equations for the concentrations of the various species could be solved as a function of time. However, rather than solving the equations analytically, it is easier to solve these simultaneous differential equations numerically. In fact, commercial software programs exist to perform complex gas-phase kinetic calculations. Such a program was developed at the Sandia Livermore Laboratory and is now available commercially (Kee et al. 2003; CHEMKIN). A similar series of reactions are involved in the formation of HBr by the reaction (Chang 2000) H 2 (g) + Br2 (g) 2HBr(g). 3.6.3 chain POlymeRizatiOn 3.6.3.1 Mechanism There are many different mechanisms for polymerization of monomers. In fact, a central feature of polymer science is the types of polymerization processes that can take place, how they differ for different polymers, the effects of temperature and concentration, and—most important—the role of various catalysts. The intention here is not to try to summarize all of this information that is best left to polymer chemistry. However, one mechanism that fits very nicely into the current discussion, and gives an example of one of the processes, radical chain polymerization that includes steps of initiation, propagation, and termination to form polymer chains. The process is covered in many polymer textbooks (Billmeyer 1984; Saunders 1988; Young and Lovell 1991; Elias 1997). * † “A” and “EA” are the symbols used in the NIST Database for the “k 0” and “Q” terms used here. The “dot” superscript represents a reactive radical, an atom or molecule with an unsatisfied electron bond—called free radicals in older literature. The literature is somewhat inconsistent in the designation of a radical. Sometimes the dot is placed directly on top of the symbol (Kee et al. 2003), sometimes to the side (Silbey and Alberty 2001), and sometimes it is not used at all (Laidler 1987; Houston 2001), but most frequently it is raised and to the right (or left of the atom with the unsatisfied bond) (Cowie 1991) as used here. 79 80 Chapter 3. Second-Order and Multistep Reactions O O O O O 2 C O 2 + 2 CO2 FIGURE 3.11 Benzoyl peroxide, a typical chain initiator for radical polymerization undergoing thermolysis— decomposition by heat—with the breaking of the oxygen–oxygen bond and release of CO2 to give two radicals, that can act as chain initiators, I •. Figure 3.11 shows a typical initiator material, benzoyl peroxide, that on heating, splits into two parts, gives off CO2, and provides two radicals, I•, that can act as chain initiation for polymerization. This radical reacts with a monomer molecule Initiation step: I • + CH 2 = CRH ⇒ I − CH 2 − C• RH Propagation step: I − CH 2 − C• RH + CH 2 = CRH ⇒ I − CH 2 − CRH − CH 2 − C• RH , etc. Termination step: ← − CH 2 − C• RH + C• RH − CH 2 − → ← − CH 2 − CRH − CRH − CH 2 − → In these equation, R = H, Cl, CH3, and so on and the single arrows indicate the extension of the polymer chain in both the positive and negative directions in the termination step. 3.6.3.2 Rate of Polymerization Initiation can be represented by two steps: I slow → nI· (3.47) · → IM i I· + M fast where M is the monomer molecule. Let RI be the rate of initiator formation R I = d[ I • ]/dt and kp the kp rate of chain propagation: M i + M → M i+1 so the rate of consumption of the monomer is − d [M] = k p M1i [ M ] + k p M i2 [ M ] + M ii [ M ] dt (3.48) − d [M] = k p [M] dt ∞ ∑ M = k [M] M • i p • i =1 where [ M• ] is the total concentration of all the radical species. The rate of termination is given by t M•i + M•j k → M i+ j where kt is the rate of termination so − [M • ] = 2k t [M • ]2 . dt (3.49) The 2 comes from the fact that two radical species are destroyed in a termination reaction. Steady1/ 2 state conditions are assumed; that is, d[ I • ]/dt = −(d[ M• ]/dt ) so R I = 2 k t [ M• ]2 or [ M• ] = ( R I /2 k t ) . Substituting this into Equation 3.48 and calling − d[M] dt = R p, the “rate of polymerization,” the result is k R p = 1/ 2 p 1/ 2 R1I / 2 [ M ] 2 k t (3.50) which indicates that the rate of monomer consumption is proportional to the monomer concentration with the proportionality consisting of the various rate constants. This is a first-order equation, at least in the specified steady state. 3.7 3.6.4 chain bRanchinG ReactiOns Many combustion reactions include chain branching reactions and can lead to explosive mixtures. For the very familiar simple reaction of the combustion of hydrogen with oxygen to form water vapor H 2 (g) + 1 2O2 (g) → H 2O(g) the reaction has a total of 19 identified separate steps including the following as examples (Li et al. 2004): Initiation: H 2 + O2 H i + HO2i Propagation: H 2 + O2 H i + HO2i i OH + H 2 H 2O + H i Branching: H i + O2 Oi + i OH Termination: HO2i + i OH H 2O + O2 the solution of which, of course, requires some sort of numerical solution (Kee et al. 2003) to obtain the rate of the reaction and/or the concentrations of the various possible gas species as a function of time and temperature. 3.7 SUMMARY In this chapter, second-order, primarily homogeneous reactions, as well as multistep reactions are considered. The focus remains on homogeneous reactions purely because the reactions are conceptually simpler and lead more readily to transparent solutions. Furthermore, in the materials world of today, what goes on in the gas or liquid phase is critical to many important commercial materials processes. The objectives of this chapter are several-fold. One is to demonstrate how rapidly reaction solutions can become complex strongly suggesting numerical rather than analytical solutions. A second objective is to demonstrate how some of these more complex reactions can be solved analytically with elementary calculus techniques. Another objective is to demonstrate the rate-controlling step in series and parallel reactions. The reactions investigated in this chapter include: simple second-order reactions; second-order reactions with different initial concentrations of reactants; reactions that go to equilibrium—those with back reactions; serial and parallel reactions; chain reactions; and branching reactions. It is demonstrated that the initial reaction rate for a first-order reaction that goes to equilibrium could be written as d [A ] = − k [ A ] − [ A ]e dt ( ) (3.51) where [A]e is the equilibrium concentration. Equation 3.51 shows the very general result that the reaction rate is the product of a kinetic factor, k, and a thermodynamic factor, ( [ A ] − [ A ]e ), and this is generally seen in the kinetics of other reactions. For second- and higher order reactions, even unpretentious looking reaction rates quickly become difficult to integrate analytically. As a result, numerical techniques are easy to implement and the simple case of Euler’s method applied to a second order ⇔ second order equation demonstrates the utility of a numerical solution to all but the simplest of reactions that go to equilibrium. Simple series and parallel reactions are then examined that show that the slowest step controls the overall rate of a series reaction while the fastest step controls the rate and product concentrations of parallel reactions. Finally, the potential complexity of ostensibly simple reactions, such as the reaction of hydrogen and chlorine to form HCl, and hydrogen and oxygen to form water vapor, are Summary 81 82 Chapter 3. Second-Order and Multistep Reactions examined. These examples demonstrate the need for numerical solution to the several parallel and series kinetic steps probable in real reactions to understand the effects of composition and ambient conditions on reaction rates and possible rate-controlling reaction steps. Up to this point, little has been said about the temperature dependence of the reaction rate constant. This is the subject of the next chapter. APPENDIX a.1 secOnd-ORdeR ReactiOn with diFFeRent initial cOncentRatiOns A.1.1 General Result In this case, assume that there are two reactants, A and B, reacting to give a product, C: (A.1) A + B k →C where C in this case can be one or more products. In addition, assume that the reaction is first order with respect to both A and B resulting in overall second-order kinetics: d [A ] = − k [ A ][ B] dt (A.2) and that the reaction goes to completion (either [A] and/or [B] goes to zero at t = ∞) the concentrations of A and B can be expressed as*: [ A ] = [ A ]0 − ([ A ]0 − [ A ]) [ B] = [ B]0 − ([ B]0 − [ B]) ( = [ B]0 − [ A ]0 − [ A ] ( (A.3) ) ) ∴ [ B] = [ B]0 − [ A ]0 + [ A ] because the amount of B reacted must be the same as the amount of A reacted at any given time and the initial concentrations of A and B at time = 0 are [A]0 and [B]0, respectively. So Equation A.2 becomes d [A ] = − k [ A ] [ B]0 − [ A ]0 + [ A ] dt ( ) or d [A ] = − kdt [ A ] [ B]0 − [ A ]0 + [ A ] ( (A.4) ) this can be integrated by the standard method of partial fractions (Edwards and Penney 1986). This means that constants D and E need to be found so that 1 D E = + . A [ A ] [ B]0 − [ A ]0 + [ A ] [ ] [ B]0 − [ A ]0 + [ A ] ( * ) To reduce the amount of algebra, assume that ([ B]0 − [ A ]0 ). ( ) Appendix Multiplying both sides of the equation by the denominator on the left-hand side of this equation gives 1 = D [ B]0 − [ A ]0 + D [ A ] + E [ A ] , and equating like powers of [A] on both sides of the equation: D [ A ] + E [ A ] = 0 so E = −D; because there is no term in x on the left and 1 = D [ B]0 − [ A ]0 so D = 1/ ([B]0 − [A ]0 ), Equation A.4 now becomes ( ( ) ) d [A ] − d [A ] = − kdt [ B ] − [ A ] − [ A ] 0 0 ( [ B] − [ A ] ) [ A ] ( [ B] − [ A ] ) ( 0 0 0 ( 0 ) ) multiplying both sides by [ B]0 − [ A ]0 and integrating from t = 0 to t gives [A ] ln [A ] 0 ( ( ) ) [ B] − [ A ] + [ A ] 0 0 = − k [ B] − [ A ] t . − ln 0 0 − + B A A [ ] [ ] [ ] 0 0 0 ( ) (A.5) This last equation essentially forces [B0] to be greater than [A0] because when [A]→0, ([ B0 ] − [ A 0 ]) would be negative and the loge of a negative number is not defined. Taking the exponent of both sides of the equation and moving a few things around, Equation A.5 becomes [ A ]0 e−([B] −[A] )kt = f t [A ] = () ([B]0 − [A ]0 ) + [A ] [B]0 0 0 so [ A ] = ([ B]0 − [ A ]0 ) f ( t ) + [ A ] f ( t ) or [ A ] − [ A ] f ( t ) = [ A ] (1 − f ( t ) ) = ([ B]0 − [ A ]0 ) f ( t ) and rearranging gives the final rather ugly result: [ B ] − [ A ] ) [ A ] e ([ ] ( [A ] = ) − B 0 −[ A ]0 kt 0 0 0 [ B]0 − [ A ]0 e ([ ) − B]0 −[ A ]0 kt (A.6) . Solving for [B], because [ B] = ([ B]0 − [ A ]0 ) + [ A ] [ B ] − [ A ] ) [ A ] e ([ ] [ ( [ B] = ( [ B] − [ A ] ) + ([ ] [ ] ) ) − B 0 − A ]0 kt 0 0 ( 0 0 0 [ B]0 − [ A ]0 e − B 0 − A 0 kt ) factoring out [ B]0 − [ A ]0 and getting a common denominator, this equation becomes [ B]0 . − ([ B] −[ A ] ) kt [ B]0 − [ A ]0 e [ B] = ([ B]0 − [ A ]0 ) ( 0 ) 0 When t = 0, [ B] = [ B]0 and when t = ∞, [ B] = [ B]0 − [ A ]0 as it should. (A.7) 83 84 Chapter 3. Second-Order and Multistep Reactions A.1.2 Initial Concentrations Equal From Equation A.6, when [ B]0 [ A ]0 , or the initial concentrations are about equal, then [A] is indeterminate, that is, [A] = 0/0. Therefore, to get a value for [A], the approximation is made that e x = 1 + x + ( x 2 / 2 !) + ≅ 1 + x, that is, only the first two terms in the infinite series expression for ex are used when x ≅ 0. Making this approximation, the right-hand side of Equation A.6 becomes ([B] − [A ] ) [A ] (1 − ([B] − [A ] ) kt ) [ B] − [ A ] (1 − ([ B] − [ A ] ) kt ) 0 0 0 = 0 0 0 0 0 ([B] − [A ] ) [A ] (1 − ([B] − [A ] ) kt ) ([B] − [A ] ) + [A ] (([B] − [A ] ) kt ) 0 0 0 ( 0 0 0 0 0 0 0 0 ) and canceling the [ B]0 − [ A ]0 term gives [A ] = [ A ]0 (1 − ([ B]0 − [ A ]0 ) kt ) 1 + [ A ]0 kt which—after all of this algebra—because [ B]0 − [ A ]0 ≅ 0 gives the result [A ] ≅ 1 + [ A ]0 [ A ]0 kt (A.8) and the result is the same as when [A] = [B], Equation 3.2, as it should. a.2 secOnd ORdeR ⇔ secOnd ORdeR A.2.1 Beginning The general procedure carried out here works for second order ⇔ second order, second order ⇔ first order, and first order ⇔ second order because all involve the solution of quadratic equations. The reaction is assumed to be the simple reaction AB or d [A ] 2 2 = − k1 [ A ] + k 2 [ B ] . dt (A.9) Again, to minimize the notation, let [A] = x, and [A]0 = x0 and [B]0 = 0 so that Equation A.9 becomes dx 2 = − k1x 2 + k 2 ( x 0 − x ) . dt (A.10) Now, this is a relatively simple differential equation to solve because the variables are separable— all the “xs” on the left and “ts” on the right—so that standard integrations give a solution without recourse to special differential equation solution techniques. As shown in this chapter, the equilibrium concentrations, xe (only one of which gives a solution), are given by Appendix k2 x e = x 0 . k 2 ± k1 (A.11) At this point, several options are available to proceed with the solution: (1) just solve Equation A.10 as is; (2) solve Equation A.11 for x0 and substitute it into Equation A.10 and solve; or (3) solve Equation A.11 for k 2 and substitute it into Equation A.10 and solve (Laidler 1987). Here the first approach is used to minimize the symbol complexity. The procedure used is exactly that for the specific case in Section 3.4.3 where specific numbers were used to simplify the system even further. The difference here is that the solution in terms of the parameters x0, k1, and k2 (and/or xe) is sought so that it can be applied to any such reaction. A.2.2 Finding Roots (Factors) As in Section 3.4.3, the two roots, x1 and x2, of the right-hand side of Equation A.10 are sought, namely, xi = − b ± b2 − 4ac . 2a Expanding Equation A.10, ( dx = − k1x 2 + k 2 x 20 − 2xx 0 + x 2 dt ) dx = − ( k1 − k 2 ) x 2 − 2k 2x 0 x + k 2x 02 dt 1 dx k = − 1 − 1 x 2 − 2x 0 x + x 20 k 2 dt k 2 1 dx = ax 2 + bx + c. k 2 dt So the roots of the right-hand side of the quadratic equation are xi = 2x 0 ± 4x 20 + 4 ( ( k1 / k 2 ) − 1) x 20 −2 ( ( k1 − k 2 ) /k 2 ) xi = − x0 (( (( k − k )/ ( 1 xi = ( ) ) )) k 2 ± k1 / k 2 x0 k 2 2 ( k 2 + k1 k2 k2 k 2 ± k1 )( ) k 2 − k1 ) . So the two roots are, as before, Equation A.11, ( /( ) k ) x1 = x 0 k 2 / k 2 + k1 x2 = x0 k 2 k2 − (A.12) 1 and x1 > 0 while x 2 < 0 if k1 > k 2. If the latter is not the case and [B]0 = 0, there is no reaction, and if [B]0 > 0, then the reverse reaction would occur, B → A. So k1 must always be greater than k2 if the 85 86 Chapter 3. Second-Order and Multistep Reactions initial concentration of B is assumed to be zero. As a result, x1 is the equilibrium point of interest physically because the concentrations must always be positive. A.2.3 Checking the Factoring So two factors for the right-hand side of the differential equation, Equation A.10 are ( −x 2 + x ) and ( x1 − x ). Is that all that is necessary? That is, if these factors are multiplied do they reproduce the right-hand side of Equation A.10? Checking this product, Product = ( −x 2 + x ) ( x1 − x) = −x 2x1 + x 2x + x1x − x 2 = −x 2x1 + ( x 2 + x1 ) x − x 2 = − = Product = ( x0 k 2 k 2 − k1 x0 k 2 ) ( ) k 2 + k1 + ( x0 k 2 k 2 − k1 + ) ( x0 k 2 k 2 + k1 ) x − x2 k + k1 + k 2 − k1 x 20 k 2 2 + x 0 k 2 2 x − x k1 − k 2 k k − 2 1 x k x 20 k 2 − 0 2 x − x2. k1 − k 2 k1 − k 2 To obtain the right-hand side of Equation A.10, this last equation must be multiplied by ( k1 − k 2 ) and divided by k 2. So the complete factoring of the right-hand side leads to the differential equation: 1 dy 1 = ( k1 − k 2 ) ( −x 2 + x ) ( x1 − x) k 2 dx k 2 1 k 2 cancels and the differential equation to be solved is now, dy = ( k1 − k 2 ) ( −x 2 + x ) ( x1 − x). dx A.2.4 (A.13) Solution of the Differential Equation Again, Equation A.13 is the equation to be integrated and follows the procedure used in this chapter. Separating variables dx = ( k1 − k 2 ) dt − x + x ( 2 ) ( x1 − x ) and letting, where A and B are now integration constants here, 1 = A + B ( −x 2 + x ) ( x1 − x ) ( −x 2 + x ) ( x1 − x ) and solving for A and B, Ax1 − Ax − Bx 2 + Bx = 1 so A = B and Ax1 − Bx 2 = 1 or A = B = 1 ( x1 − x 2 ). So, the equation that needs to be integrated is now dx + dx ( −x 2 + x ) ( x1 − x ) and integrating gives = ( x1 − x 2 ) ( k1 − k 2 ) dt Appendix ln ( x − x 2 ) − ln ( x1 − x ) = ( x1 − x 2 ) ( k1 − k 2 ) t + C ( x − x 2 ) = C′e( x −x )( k −k )t ( x1 − x ) 1 2 1 2 where C and C′ are both constants of integration. And when t = 0, x = x0 so C′ = ( x0 − x2 ) ( x1 − x 0 ) and the solution becomes ( x − x 2 ) = ( x 0 − x 2 ) e( x −x )( k −k )t = 1 D ( x1 − x ) ( x1 − x 0 ) 1 2 1 (A.14) 2 where D is a constant for a given time t. Equation A.14 needs to be solved for x so inverting Equation A.14 and multiplying by (x − x2) gives x1 − x = −x 2D + xD and solving for x x1 + x 2D . 1+ D x= (A.15) Substituting in the values of x1, x2, and D, the solution is finally obtained. But wait! The answer really is desired in terms of k1, k2, and x0, the real parameters of the problem. So it is worthwhile to see what the final equation looks like in terms of these parameters. Attacking the exponent first, k = − ( x1 − x 2 ) ( k1 − k 2 ) = − ( x0 k 2 k 2 + k1 ( k1 − k 2 ) k 2 − k1 x0 k 2 − ) ( ) k − k1 − k 2 − k1 k = x0 k 2 2 ( k1 − k 2 ) k1 − k 2 which reduces to the resultant reaction rate constant k, which has the appropriate units of cm 3/mol s: k = −2x 0 k 2 k1 . (A.16) Now for the factor in front of the exponent in D so ( x1 − x 0 ) = ( x0 − x2 ) = ( x k / ( k + k ) − x ) ( x − x k / ( k − k ) ) 0 2 0 (( (( 0 2 2 1 0 2 1 )( )/( )) k )) k 2 − k 2 − k1 / k 2 + k1 k 2 − k1 − k 2 k2 − 1 with the result ( x1 − x 0 ) = − ( x 0 − x 2 ) k1 − k 2 . k1 + k 2 (A.17) The other factor that needs to be calculated is ( x1 − x 0 ) × x = − 2 ( x0 − x2 ) k1 − k 2 × k1 + k 2 ( x0 k 2 k 2 − k1 ) 87 88 Chapter 3. Second-Order and Multistep Reactions which is ( x1 − x 0 ) × x = 2 ( x0 − x2 ) . x0 k 2 k1 + k 2 (A.18) Putting x1 and Equations A.16 through A.18 into A.15 gives the final result—the solution: x= x0 k 2 / ){ ( k 2 + k1 1 + e ( ( ) − 2 x 0 k 2 k1 t ) ( 1 − ( k1 − k 2 ) / ( k1 + k 2 ) e } ) − 2 x0 k 2 k1 t (A.19) which is a disagreeably messy solution, to say the least, for an apparent simple differential equation. A.2.5 Checking the Solution When t → ∞, only the first term in the numerator remains and it is x1 or the equilibrium composition, Equation A.12 which checks. When t = 0, x= = x0 k 2 / 1− (( ( ) k 2 + k1 {1 + 1} ) k ) k1 − k 2 ) / ( k1 + k 2 ) 2x 0 k 2 / ( k2 + 1 ( k 1 + k 2 − k1 + k 2 ) / ( k1 + k 2 ) x = x0 which also checks. The result can also be checked with the result of Equation 3.30 in which k1 = 2, k1 = 1, and x0 = 1. In this case, the exponent is k = −2x 0 k 2 k1 k = −2 (1) (1)( 2 ) k = −2.82842 which checks with Equation 3.30. The first factor in the numerator of Equation A.19 is simply x1 given by x1 = x1 = ( x0 k 2 k 2 + k1 ) 1 1 1+ 2 x1 = 0.41421 which also checks. So it is concluded that Equation A.19 is the general solution to Equation A.10. One last check could be made and that is when k 2 = 0, no back reaction, does Equation A.19 go to Equation A.8? This is left as an exercise. a.3 sOlutiOn FOR twO ReactiOns in seRies A.3.1 Introduction The problem is to find the solution for two first-order reactions in series; namely: 1 2 A k → B k →C (A.20) Appendix so the rate equations become d [A ] = − k1 [ A ] dt d [ B] = k1 [ A ] − k 2 [ B ] dt (A.21) d [C] = k 2 [ B] dt with the conservation of matter: [A]0 = [A] + [B] + [C] at any time t with [A]0 being the initial concentration of A and the initial concentrations of B and C at t = 0 are [B]0 = [C]0 = 0 to make the calculations more manageable. The solution to this series of equations is given in many physical chemistry texts but they do not give the details of the integration process and simply indicate that “... the following is obtained by integration ...” (Laidler and Meiser 1995; Silbey and Alberty 2001). The result is certainly not obvious but can easily be obtained although it requires some familiarity with ordinary differential equations. For completeness, and to satisfy the curiosity of those who are more conversant with ordinary differential equations, the details of the calculations are given. A.3.2 Concentration of A The solution to the first of the above equations for [A] is simply the solution for any first-order equation, [ A ] = [ A ]0 e− k t . 1 (A.22) A.3.3 Concentration of B The differential equation for [B]—the second equation above—now becomes d [ B] = k1 [ A ]0 e − k1t − k 2 [ B] dt (A.23) d [ B] + k 2 [ B] = k1 [ A ]0 e − k1t dt (A.24) which can be rewritten as which is a nonhomogeneous differential equation—the right-hand side of the equation is nonzero. The solution to such an equation is to first solve the homogeneous equation (make the right-hand side = 0) d [ B] + k 2 [ B] = 0 dt (A.25) and then add to the homogeneous solution a particular solution that satisfies the right-hand side of the equation, Equation A.24 in this case. The complete solution is the sum of the homogeneous and particular solutions (Kreyszig 1988). To simplify the notation, let [B] = y, so the homogeneous equation (subscript y) becomes dy h + k 2y h = 0 dt (A.26) where the subscript h refers to the homogeneous equation. This equation has been encountered several times already along with its solution. However, because more advanced differential equations are being solved here, the formal method for solution of such equations will be followed as a demonstration. The formal way to solve such an equation is by the method of characteristics because it is a linear differential equation with constant coefficients; that is, let y h = C1eλt, where C1 is just a constant of integration. Substituting this in the differential equation for yh, Equation A.26, 89 90 Chapter 3. Second-Order and Multistep Reactions C1λeλt + C1k 2eλt = 0 (A.27) which gives λ = −k2 and the solution, y h = C1e − k 2 t as expected. And the equation for d[B]/dt, Equation A.24, suggests a particular solution, y p, of the form: y p = C2e − k1t , where C2 is just another integration constant. Substituting y p for [B] in the differential equation gives y p′ + k 2 y p = k1[A ]0 e − k1t − k1C2e − k1t + k 2C2e − k1t = k1[A ]0 e − k1t . Obviously, e − k1t cancels in all the terms leaving C2(k2 − k1) = k1[A]0 that gives for y p: yp = k1 [ A ]0 k 2 − k1 e − k1t . (A.28) The complete solution is simply y = yh + y p, which is k1 [ A ]0 e − k1t [ B] = C1e− k t + 2 (A.29) k 2 − k1 At t = 0, B = 0 so that C1 = − k1 [ A ]0 /( k 2 − k1 ) and the solution for [B] is [ B] = [ A ]0 k1 k 2 − k1 (e − k1t ) − e− k2 t . (A.30) A.3.4 Concentration of C Because [C] = [A]0 − [A] − [B], inserting Equations A.22 and A.30 for [A] and [B], [ A ] k1 [C] = [ A ]0 − [ A ]0 e− k t − k −0 k ( e− k t − e− k t ) 1 1 2 2 1 (A.31) and rearranging [C] = [ A ]0 1 − k 2e − k1t + k1e − k1t − k1e − k1t + k1e − k 2 t k 2 − k1 gives for [C] [C] = [ A ]0 1 + k 1 k1e − k 2t − k 2e − k1t 2 − k1 ( ) (A.32) Equations A.22, A.30, and A.32 are the solutions to the differential equations Equation A.21. A.3.5 Slower Reaction Controls [C] If k2 ≫ k1 in Equation A.30, [B], and Equation A.32, [C], so that the reaction from B to C is much faster than the reaction from A to B, then the following approximation results from Equation A.30: k [ B] ≅ k 1 [ A ] 2 (A.33) which implies that, at any given time, the concentration of B will be much less than that of A, and [C] becomes from Equation A.32 [C] ≅ [ A ]0 (1 − e− k t ) = [A]0 − [ A ] . 1 (A.34) Exercises This implies that C comes almost directly from A and the rate depends on the smaller k, in this case, k1. The concentration of B is always small because it reacts very fast to form C so it is the slower step that controls the rate of reaction to form C from A; that is, the reaction of A going to B, which is the slower step. Conversely, if k1 ≫ k2, then from Equations A.30 and A.32 [ B] [ A ]0 e− k t (A.35) [C] [ A ]0 (1 − e− k t ) [ A ]0 − [ B] (A.36) 2 2 which imply that A goes to B very quickly, and it is now the reaction of B to C, or k 2—the slower series step—that controls the rate of formation of C. So as stated earlier, with series steps in a reaction process, it is the slower (or slowest step if there are more than two) that controls the rate of the overall reaction: in this case, A going to C. EXERCISES 3.1 a. The molecular weight of HI is 127.9 g/mol. Calculate the concentration of Hl in mol/cm3 at 800°C if its partial pressure is p(HI) = 1 atm. b. Calculate the number of HI molecules per cm3 at this temperature and pressure. c. If the Gibbs energy for the reaction: H2(g) + I2(g) = 2HI(g) at 800°C is ∆Gο = −26, 400 J / mol, calculate equilibrium partial pressures (atm) of HI, H2, and I2 at 800°C assuming that a closed container initially contained only H2 and I2 gases each at a partial pressure of 1 atm at 800°C. 3.2 a. From the NIST database, the reaction rate constant for the reaction H2(g) + I2(g) = HI(g) is given by k0 = 3.22 × 10−10 (cm3/molecule s) and Q = 171 (kJ/mol) and it is a secondorder reaction. Calculate the reaction rate constant (cm3/molecule s) at 800°C. b. Calculate the [H2]0 and [I2]0 in mol/cm3 at the starting pressure and temperature. c. For the reaction H2(g) + I2(g) = 2HI(g) at 800°C, H2 and I2 reach an equilibrium pressure calculated in Exercise 3.1 above. Calculate the [H2]e, [I2]e, and [HI]e in mol/cm3 at this temperature. d. Calculate and plot [H2] = [I2] and [HI] (on the same graph) at 800°C versus time (on a linear plot) until the [HI] = 0.90 [HI]e where “[]” is in mol/cm3. 3.3 A hypothetical second-order reaction that goes to completion with two reactants A and B going to C, that is, A + B → C d [C] = k [ A ][ B] dt with k = 10 −3 L mol ⋅ s , [ A ]0 = 0.1 mol L , [ B]0 = 0.5 mol L , [ C]0 = 0.1 mol L . Calculate and plot [A], [B], and [C] as a function of time from t = 0 to [A] = 0.001 mol/L all on the same plot. 3.4 For a simple reaction that goes to equilibrium A B by forward and backward first-order reactions, 1 A k →B 2 B k →A with k1 = 5 × 10 −3 s −1 and k 2 = 1 × 10 −3 s −1, if [ A ]0 = 1.0 mol L and [ B]0 = 0 : a. Calculate the equilibrium constant for this reaction. b. Calculate the equilibrium concentrations of A and B, [A]e and [B]e. c. On the same graph, plot [A] and [B] from t = 0 until [A] = 0.01[A]e. 91 92 Chapter 3. Second-Order and Multistep Reactions 3.5 Show that the general solution for a reaction A B that goes to equilibrium with both forward and back second-order reactions where x = [A] and [B]0 = 0, x= x0 k 2 / ( ){ k 2 + k1 1 + e ( ( ) − 2 x 0 k 2 k1 t ) ( 1 − ( k1 − k 2 ) / ( k1 + k 2 ) e } ) − 2 x0 k 2 k1 t goes to the simple solution for a second-order reaction with no back reaction—goes to completion, that is, x≅ x0 1 + x 0 k1t when k2 → 0. Hint: When k2 → 0 let e − y → 1 in the numerator and let e − y → 1 − y in the denominator. 3.6 A simple reaction A B that goes to equilibrium with both forward and back second-order reactions where x = [A], x0 = [A]0, and [B]0 = 0 gives the differential equation: d [A ] 2 2 = − k1 [ A ] + k 2 [ B ] dt dx 2 = − k1x 2 + k 2 ( x 0 − x ) dt a. Calculate the equilibrium concentrations of A and B in terms of [A]0 when the forward and back reactions have the same rate constant; that is, k= k= k. 1 2 b. Calculate the exact solution for x when k= k= k. 1 2 c. Use Euler’s method to approximate the solution if k = 3 × 10−2 mol/L-s, [A]0 = 1 mol/L, for n = 1 to n = 100 with a time-step of Δt = 1.0. d. Plot the results of parts b and c on the same graph with the parameters in part c. 3.7 A simple reaction A B that goes to equilibrium with a forward second-order reaction and a first-order back reaction, where x = [A], x0 = [A]0, and [B]0 = 0, gives the differential equation: d [A ] 2 = − k1 [ A ] + k 2 [ B ] dt dx = − k1x 2 + k 2 ( x 0 − x ) dt If = k1 2= , k 2 1, and x 0 = 1 a. Calculate the equilibrium concentrations of A and B. b. Derive an expression for x, the concentration of A, as a function of time for this specific set of conditions. c. Make a plot of [A] and [B] versus time on the same graph from t = 0 until [A] = 0.99 [A]e. 3.8 Derive the general solution for x from the differential equation in number 7 above; that is, dx = − k1x 2 + k 2 ( x 0 − x ) dt for a second-order forward reaction and a first-order back reaction. 1 2 3.9 For parallel first-order reactions of A k → B and A k → C, where k2 = 0.1 × k1, and −1 k1 = 0.01s plot the concentrations of the three species on the same graph as a function of References time up until [A] = 0.01[A]0 with [A]0 = 1 at t = 0 and the reactions go to completion; that is, no back reactions. 1 2 3.10 For a series reaction A k → B k → C, the equations for the concentrations of A, B, and C are [ A ] = [ A ]0 e− k t 1 [ B] = [ A ]0 k1 k 2 − k1 [C] = [ A ]0 1 + k 2 (e − k1t − e− k2 t ) 1 k1e − k 2t − k 2e − k1t − k1 ( ) a. Make two separate plots of [A], [B], and [C] versus time up to t = 10 4 s assuming that [A]0 = 1 and the initial concentrations of B and C are zero. In the first plot, k1 = 5 × 10 –4 s –1 and k2 = 5 × 10 –3 s –1 and in the second plot, the values of the constants are just reversed, k1 = 5 × 10−3 s –1 and k2 = 5 × 10 –4 s –1. b. Derive approximate expressions for these three equations if k 2 ≫ k1. c. Calculate the expressions for the three concentrations as a function of time if k1 = k2. REFERENCES Billmeyer, F. W. Jr. 1984. Textbook of Polymer Science, 2nd ed. New York: Wiley Interscience. Blanchard, P., R. L. Devaney, and G. R. Hall. 2012. Differential Equations, 4th ed. Boston, MA: Brooks/Cole (Cengage Learning). Celia, M. A. and W. G. Gray. 1992. Numerical Methods for Differential Equations. Englewood Cliffs, NJ: Prentice Hall. Chang, R. 2000. Physical Chemistry for the Chemical and Biological Sciences. Sausalito, CA: University Science Books. CHEMKIN. http://www.ca.sandia.gov/chemkin/. Program available from: Reaction Design, San Diego, CA. Cowie, J. M. G. 1991. Polymers: Chemistry & Physics of Modern Materials, 2nd ed. New York: Chapman and Hall. Edwards, C. H. and D. E. Penney. 1986. Calculus and Analytical Geometry, Englewood Cliffs, NJ: Prentice Hall. Elias, H.-G. 1997. An Introduction to Polymer Science. New York: VCH Publishers. Houston, P. L. 2001. Chemical Kinetics and Reaction Dynamics. Mineola, NY: Dover. Kee, R. J., M. E. Coltrin, and P. Glarsborg. 2003. Chemically Reacting Flow. Hoboken, NJ: Wiley. Kreyszig, E. 1988. Advanced Engineering Mathematics, 6th ed. New York: Wiley. Laidler, K. J. 1987. Chemical Kinetics, 3rd ed. New York: Harper and Row. Laidler, K. J. and J. H. Meiser. 1995. Physical Chemistry, 2nd ed. Boston, MA: Houghton Mifflin. Li, J., Z. Zhao, A. Kazakov, and F. L. Dryer. 2004. An Updated Comprehensive Kinetic Model of Hydrogen Combustion. Int. J. Chem. Kinetics. 36: 566–575. Moore, J. W. and R. G. Pearson. 1981. Kinetics and Mechanism. New York: Wiley. NIST. 2013. NIST Chemical Kinetics Database. Standard Reference Database 17, Version 7.0 (Web Version). Release 1.6.7. Data Version 2013.03. http://kinetics.nist.gov/kinetics/index.jsp. Saunders, K. J. 1988. Organic Polymer Chemsitry, 2nd ed. New York: Chapman and Hall. Silbey, R. J. and R. A. Alberty. 2001. Physical Chemistry, 3rd ed. New York: Wiley. Young, R. J. and P. A. Lovell. 1991. Introduction to Polymers, 2nd ed. London: Chapman and Hall. 93 4 Temperature Dependence of the Reaction Rate Constant 4.1 4.2 4.3 4.4 4.5 Introduction The Arrhenius Equation 4.2.1 Origins 4.2.1.1 Example: Calculating Q and k0 from Kinetic Reaction Rate Constants and Temperature The Hindenburg Disaster 4.3.1 Combustion of Hydrogen 4.3.2 Hydrogen and the Hindenburg 4.3.3 A Materials Failure? Controlled Combustion Reactions 4.4.1 Hydrogen–Oxygen Combustion 4.4.2 Combustion Synthesis Barometric Formula 4.5.1 Development 4.5.1.1 4.5.1.2 4.6 Example: Atmospheric Pressure in Denver Example: Atmospheric Pressure at the International Space Station 4.5.1.3 Example: The Thickness of Earth’s Atmosphere Boltzmann Distribution 95 96 96 96 97 98 98 98 99 100 100 101 102 102 103 104 104 104 96 Chapter 4. Temperature Dependence of the Reaction Rate Constant 4.7 The Activated State 4.7.1 Activation Energy 4.7.2 Role of a Catalyst 4.8 Summary Exercises References 4.1 106 106 107 109 109 110 INTRODUCTION The main purpose of this chapter is to demonstrate why the Arrhenius equation depends exponentially on temperature. This is not a first principles approach, but rather it is based on the barometric formula, the effect of altitude on atmospheric pressure, that assumes the equation of state of an ideal gas: PV = nRT. This result leads naturally to the Boltzmann distribution for the energy of atoms and molecules as a function of temperature. Because reaction rates depend exponentially on temperature, if a reaction is exothermic, releasing heat, then its rate can continually increase resulting in very high temperatures: combustion. Examples are given showing both the bad and useful effects of this exponential temperature dependence. Finally, a thermodynamic argument leading to an exponential temperature is also presented that leads to the concepts of an activated state, an activation energy, and how catalysts affect reaction rates. 4.2 THE ARRHENIUS EQUATION 4.2.1 Origins As was indicated earlier, reaction rate constants are exponential functions of temperature,* k = k 0exp(− Q/RT) or k = Aexp(− E A /RT), the so-called Arrhenius equation, named after Svante Arrhenius (Figure 4.1). Arrhenius was a Swedish chemist who received the 1903 Noble Prize in chemistry for his work on electrolytes (Worek 2008). However, he also did research on chemical kinetics. Van’t Hoff originally proposed the exponential temperature dependence of reaction rates in the late 1800s based on his equation proposed in 1884 for the temperature dependence of equilibrium constants, d ln K ∆H ° = or dT RT 2 d ln K ∆H° =− d1 T R (4.1) where: K is thermodynamic equilibrium constant ΔH° is the standard enthalpy for the reaction (J/mol) R is the gas constant (J/mol-K). As was seen in Chapter 3, when forward and back reactions with rate constants k1 and k2 go to equilibrium, the equilibrium constant is just the ratio of these two rate constants: K = k1/k2. Van’t Hoff realized that, if K is exponentially dependent on 1/T, the reaction rate constants must also have the same temperature dependence and therefore must be of the form FIGURE 4.1 Svante Arrhenius (1859–1927). (Photograph in the public domain because the copyright has expired, http://commons.wikimedia. org/wiki/File:Arrhenius2.jpg.) k = Ae * − EA RT More precisely, the rate constant is an exponential function of 1/T. 4.2 The Arrhenius Equation Temperature (°C) 527 393 298 Forward reaction rate (cm3 mole−1 s−1) 103 227 171 127 Slope = −Q/(2.303R) 101 10−1 10−3 10−5 10−7 1.0 1.2 1.4 1.6 1.8 2.0 2.2 2.4 2.6 1000/T (K−1) FIGURE 4.2 The reaction rate constant as a function of T for the reaction H2(g) + I2(g) ⇌ 2HI(g). (Data from the NIST Kinetics Database, http://kinetics.nist.gov/kinetics/index.jsp.) where: A is the constant, the preexponential term, the units of which depend on the order of the reaction EA is the activation energy (J/mol) (Laidler 1984). This is what might be termed a plausibility argument, in that what is known about the temperature dependence of the equilibrium constant, and the relationship between it and the reaction rate constants, makes the suggestion of the Arrhenius equation for the rate constants entirely reasonable and consistent with the known facts. Arrhenius’s subsequent contribution was that he felt that the temperature dependence of colliding atoms or molecules in gases and liquids was too small to give the observed values of activation energies. So he proposed an equilibrium between reactive molecules and the others based on the van’t Hoff equation (Laidler 1984). Of course, later experiments have shown that reaction rate constants do follow an Arrhenius equation and are indeed exponentially dependent on 1/T (there is often a mild temperature dependence of the preexponential term as well). Figure 4.2 shows the exponential temperature dependence for the second-order reaction rate constant (note the units for k) for the forward reaction of H 2 (g) + I 2 (g) 2HI(g). In this case (NIST 2013), ( ) k1 = 1.94 × 1014 cm 3mol −1s−1 e − 171kJ / mol RT Note that the reaction rate increases by about 11 orders of magnitude over a span of only about 400°C. By measuring the rate of a reaction as a function of temperature, the two important parameters of the rate equation, Q and k0, can be determined. 4.2.1.1 Example: Calculating Q and k0 from Kinetic Reaction Rate Constants and Temperature Given the following rate constants for some reaction at two different temperatures: k1 = 5.7 × 10 −5 s −1 at 25°C k 2 = 1.64 × 10 −4 s −1 at 40°C 97 98 Chapter 4. Temperature Dependence of the Reaction Rate Constant what are the values for Q and k0? By taking the ratio k1/k2, k0 is eliminated and Q can be obtained − Q Q Q 1 Q 1 − − − k1 e RT1 k Q 1 1 R = = e RT1 e RT2 = e T1 T2 so ln 1 = − − Q − k2 k R T1 T2 2 e RT2 Q=− R ln( k1 /k 2 ) −8.314 ln[(5.7 × 10 −5 ) /(1.64 × 10 −4 )] = = 54, 636 J /mol-K ( (1/T1 ) − (1/T2 ) ) ( (1/ 298) − (1/313) ) k0 can now be obtained from either of the two given rates because k = k 0exp(− Q/RT) , so k 0 = kexp(Q/RT) 54,636 k 0 = 5.7 × 10 −5 e 8.314 × 298 = 2.15 × 105 s−1 or −4 k 0 = 1.64 × 10 e 4.3 54,636 8.314 × 313 = 2.15 × 105 s−1. THE HINDENBURG DISASTER 4.3.1 COmbustiOn Of HydrOgen Because reaction rates are typically exponentially temperature dependent, once a reaction that has a large exothermic heat of reaction—essentially the thermodynamic enthalpy ΔHo—initiates, if this heat is not dissipated, it will continuously increase the temperature of the reactants and products, leading to an ever increasing reaction rate and temperature that can result in an explosion. This was the situation that befell the Hindenburg in May of 1937 when its hydrogen buoyancy gas ignited (Figure 4.3). This picture of the Hindenburg burning immediately comes to mind and generates concern when hydrogen is being considered as a motor vehicle fuel, possibly in a fuel cell. However, it should be noted that gasoline has almost three times the energy per unit volume than liquid hydrogen, so it is potentially more explosive. On the other hand, gasoline does not evaporate rapidly, whereas hydrogen–air mixtures are explosive between 5 and 95 v/o (volume percent) hydrogen. 4.3.2 HydrOgen and tHe Hindenburg Modern dirigibles or airships and balloons are filled with inert helium rather than the explosive hydrogen that destroyed not only the Hindenburg but the future of passenger travel by lighter than FIGURE 4.3 Hindenburg hydrogen-filled zeppelin accident, Lakehurst, New Jersey, May 6, 1937. (U.S. Navy photograph in the public domain, http://commons.wikimedia.org/wiki/File:Hindenburg burning.jpg.) 4.3 The Hindenburg Disaster air airship or dirigible.* Why was not the Hindenburg filled with helium? Helium was not discovered until 1868 when studies on the spectrum of the sun found it in the atmosphere of the sun as the product of the nuclear fusion reactions such as 3 1 H + 21 H ⇒ 42 He + 01 n + 17.6 MeV. (4.2) The new element was named “helium” after the Greek god of the sun, Helios (Emsley 2001). In reality, there is a lot of helium around because most of the visible matter in the universe consists of about 75% hydrogen and 25% helium created at the time of the Big Bang, 13.75 billion years ago when the universe was born. However, on the earth, helium is found only at about 8 ppb (parts per billion) in the earth’s crust where it occurs because of the alpha particle decay of some elements. Recall the decay of uranium 238 from Chapter 2: 238 92 9 .51×10 year U 4 → 23490Th + 42 He + 4.25 MeV Th → eventually to Pb. 234 90 (4.3) Helium had been detected in small amounts in uranium minerals in the late 1800s. In 1903, helium was found in significant quantities in natural gas wells in the United States and its potential for use in lighter than air airships was immediately recognized. But there is considerably more to the Hindenburg story (Provan 2011). Hydrogen was used to inflate gas balloons as early as the 1850s. Count von Zeppelin proposed a hydrogen-filled airship in 1895 and built one by 1900. These hydrogen-filled Zeppelins flew successfully for the next 40 years.† However, with the recent availability of much safer helium as a buoyancy gas, the Hindenburg was designed to use it. At that time (the 1930s), the United States was the world’s largest producer of natural gas—and helium as a by-product. Because of helium’s potential for military airship applications, its low abundance and high cost, and the virtual monopoly on its supply, the United States banned the export of helium in 1927. Germany thought that the United States would lift its ban and allow it to purchase helium for the Hindenburg class of commercial airships. However, the United States refused to lift the ban because Germany had used airships for propaganda purposes as well as the concern of many in the United States and other parts of the world—probably with good reason— that these airships were being used for mapping by the German military for use in the not too distant future. Without access to helium, the Hindenburg was redesigned and reconstructed to use hydrogen. After all, Germany had been using its airships for over 40 years without a major mishap and, besides, it was cheaper than helium and had more lifting ability so that more passengers could be carried making the venture more profitable (Provan 2011). 4.3.3 a materials failure? What caused the Hindenburg to crash and burn has been studied repeatedly for over 70 years (Provan 2011). Was it a gas leak? Was it a lightning strike? There were several thunderstorms in the Lakehurst New Jersey crash area on May 6, 1937, and the landing was delayed until the weather improved. No witness claims to have seen a lightning strike. Was it sabotage, perpetrated by a disgruntled employee or someone opposed to the National Socialist German Workers’ Party who then governed Germany? Was it a spark produced by a buildup of electrostatic charge on the covering of the airship? The external covering was a coating with a cellulose nitrate paint embedded with aluminum flakes to make it conductive and prevent charge buildup. Subsequent investigations have suggested that a spark ignited the very flammable paint, and its burning caused the rapid spread of * † The initiation of trans-oceanic airplane travel was really a more important factor in the demise of airship travel. Interestingly, it was the discovery of age-hardenable aluminum alloys, duralumin, around the turn of the century, with a high strength and light weight that allowed the construction of large passenger-carrying dirigibles such as the Hindenburg. This is another example of the enabling of a technology by materials. 99 100 Chapter 4. Temperature Dependence of the Reaction Rate Constant flames rather than burning of hydrogen. Was there an insufficient or a nonuniform distribution of the aluminum pigment to provide the necessary electrical conductivity to bleed off any charge accumulation? If so, then the loss of the Hindenburg could be attributed to a twofold materials failure: the conductive paint did not perform as expected and the polymer binder in the paint was too flammable to be used as the final encapsulation for such a large amount of highly combustible hydrogen.* 4.4 4.4.1 CONTROLLED COMBUSTION REACTIONS HydrOgen–Oxygen COmbustiOn The fact that hydrogen and oxygen react and generate high temperatures is used for combustion processes in gas torches and fuel for propulsion. Figure 4.4 shows the liftoff of the Columbia space shuttle launch on STS-1† in 1981 on the first shuttle mission. In 1992, on STS 50, the Columbia carried the U.S. Materials Laboratory experiments and two materials researchers, Dr. Bonnie Dunbar who was an astronaut and Dr. Eugene Trinh a mission specialist. The main engines of the space shuttle are fueled by liquid oxygen–liquid hydrogen fuel stored in the large main tank directly under the shuttle.‡ Hydrogen–oxygen flames are also used for cutting torches because the adiabatic flame temperature—all of the enthalpy in the reaction heats the products and is not lost to the surroundings—is about 4500°C (Butts 1943). Figure 4.5 is a temperature–enthalpy plot for the formation of water vapor from the reaction of hydrogen and oxygen: 1 H 2 (g) + O2 (g) → H 2O(g). 2 (4.4) The enthalpy change for each of the reactants and products in this figure is essentially H T = H 398 + CP (T − 398) if molar heat capacities are constant and no phase changes occur, as assumed in this figure. That is why the starting temperature was taken as 100°C to avoid the heat of vaporization of H2O for this graph. In reality, the heat capacities are not constant as discussed in Chapter 1, but close enough to being constant to demonstrate the principle involved. At all temperatures, the enthalpy for the reaction is about −250 kJ/mol of H2O, an exothermic reaction. If no heat is lost to FIGURE 4.4 The space shuttle Columbia taking off on STS-1 on April 12, 1981 on its initial flight. Its final flight, STS-107, ended in the destruction of the vehicle on re-entry. (NASA photograph in the public domain. Original color image converted to grayscale image, http://www.NASA.gov/centers/kennedy/ shuttleoperations/orbiters/columbia_info.html.) * † ‡ The zeppelins built both before and after the Hindenburg used a less flammable polymer binder. STS stands for “Space Transportation System” which the shuttle program was originally called. Each shuttle mission was given an STS designation more or less in sequence of launch date. Tragically, on its final mission, STS-107, the Columbia was destroyed and the crew lost on re-entering the earth’s atmosphere. 4.4 Controlled Combustion Reactions Enthalpy, ΔH° (kJ/mole) 300 200 Reactants: H2 + 1/2O2 ∆H° ≅ 250 kJ/mole 100 0 Nona diab −100 Product: H2O −200 −300 atic Adiabatic combustion temperature 1000 2000 3000 4000 Temperature (°C) 5000 6000 FIGURE 4.5 Enthalpy versus temperature plot for the reaction: H2 (g) + 1/2O2 (g) → H2O(g). This figure shows that if the reaction takes place at 100°C, then the adiabatic temperature is around 4800°C. the surroundings during the reaction,—adiabatic conditions—then the adiabatic combustion temperature is reached—the intersection of the horizontal dashed line in the figure with the product enthalpy. The higher the value of the reaction rate constant, the more likely combustion will be rapid and adiabatic. With the data used for this graph, if the combustion occurs at 100°C, an adiabatic temperature of about 4800°C is reached. As a result, the pressure generated by the high temperature gas is the driving force for the liquid fuel main engines on the space shuttle. The downward sloping line labeled “nonadiabatic” is what happens when some heat is lost to the surroundings by conduction, convection, and radiation, much more likely if the reaction rate is slow. In the example shown, the temperature reached would be about 3000°C, still hot enough to melt most metals. 4.4.2 COmbustiOn syntHesis The two rockets on either side of the shuttle that are producing the majority of the brightness and all of the smoke in Figure 4.4 are solid fuel boosters that make use of the reaction of powdered aluminum with a strong oxidizer, namely, ammonium perchlorate, 4Al(s) + 2NH4ClO4(s) → 2Al2O3(s) + 2H2O(g) + N2(g) + 2HCl(g) + H2(g) (4.5) generating a lot of expanding gas at high temperatures and pressures for propulsion because of the very high enthalpy and rapid rate of the reaction. The smoke primarily consists of (probably nanosize) particles of aluminum oxide. The formation of Al2O3 by this high temperature combustion process is an example of a materials synthesis process called combustion synthesis or self-propagating high temperature synthesis (SHS) that has been used to produce a wide variety of materials. However, producing them in the exhaust of the shuttle is probably not a cost-effective way of making materials! Interest in the process began in the old Soviet Union when solid fuel rocket scientists and engineers decided to apply their expertise to synthesizing materials after the end of the Cold War in the 1980s when rocket design became a less popular career choice. The principle of combustion synthesis is fairly straightforward. Figure 4.6 shows the enthalpy as a function of temperature for the reactants and products of a reaction to produce a high temperature and a high melting point material; in this case, Ti(s) + 2B(s) → TiB2 (s). In this figure, the enthalpy of melting is shown for both the products and reactants. If two solids are mixed, such as Ti and B powders, formed into a cylinder, and ignited at some point, then the enthalpy for the reaction will cause the temperature to become sufficiently high to continue the reaction. In this example, an adiabatic temperature above the melting points of both reactants 101 102 Chapter 4. Temperature Dependence of the Reaction Rate Constant 400 Bmp Enthalpy (kJ/mol) 300 Reactants: Ti phase change: α to β Ti and B 200 100 Timp TiB2 mp Adiabatic 0 −100 Product: TiB2 −200 −300 Adiabatic combustion temperature 0 500 1000 1500 2000 2500 Temperature (K) 3000 3500 FIGURE 4.6 Temperature–enthalpy plot for the formation of TiB2 by reacting titanium and boron mixtures. The adiabatic combustion temperature in this case is about 2900 K. is produced. However, the actual ignition temperature may be much higher than room temperature, producing an even higher adiabatic reaction temperature. This reaction zone is essentially a “flame” and the flame front will propagate from the point of ignition throughout the compacted mixed reactant powders. In many cases, the powders are formed into a cylinder and ignited at the top, and the flame front propagates down the length of the cylinder by heat transfer to the unreacted material completing the reaction throughout as shown in Figure 4.7. This is why the process is called SHS because the enthalpy from the reaction produces sufficiently high temperatures to produce a “self-propagating” flame front in the material as the reaction proceeds through the mixed reactants. The heat necessary to get the reaction started—increase the rate of reaction—can either be applied within a furnace, with a torch, or by some other heat source such as a spark. The combustion synthesis process has some advantages particularly if very high purity materials are needed. For example, SiC furnace parts that are used in silicon integrated circuit processing must be very pure. Starting with silicon and carbon of very high purity—electronic grade—SiC can be produced compared to the considerably less pure silicon carbide produced by the conventional Acheson process of reacting SiO2 and carbon in a carbonarc furnace to make abrasive and refractory materials where high purity is not essential. Ignition point Combustion reactions to make useful materials are not a new process. The thermite (themit) process was invented in the late 1800s and was/is used to weld steel railroad rails by the reaction of mixed powders of iron oxide and aluminum (Cary 1979): Fe2O3 ( s ) + 2 Al ( s ) → Al 2O3 ( s ) + Fe ( l ) Products Combustion zone (4.6) which liberates almost a million joules of heat per mole and an adiabatic flame temperature of 4273°C (Roine 2002), more than enough to form molten iron above its melting point of 1538°C, which then flows into a mold forming the weld. Flame propagation 4.5 Reactants FIGURE 4.7 Schematic drawing showing the process of combustion synthesis or SHS— self-propagating high temperature synthesis. 4.5.1 BAROMETRIC FORMULA develOpment A transparent approach to gain insights into the Arrhenius equation and why there is an exponential temperature dependence of reaction rates is to start with the barometric formula (Silbey and Alberty 2001). The barometric formula 4.5 gives the pressure at higher altitudes relative to the pressure at sea level—or whatever reference point is chosen and can be developed relatively simply. One of few things in the world that needs to be memorized is F = ma . So taking a slice of a column of atmosphere of cross-sectional area A extending from sea level upward, depicted in Figure 4.8, dm = ρ dV = ρ A dx where: ρ is the density of air dV is the small volume of air slice. A dF FIGURE 4.8 Schematic representation of cut through a column of air of area A and thickness dx extending from the surface of the earth out to infinity. The small slice of the column exerts a vertical downward force of dF. Therefore the pressure produced by this slice is dP = dF g ρ A dx =− = −g ρ dx A A (4.7) For an ideal gas, PV = nRT (one of the other things that is useful to memorize), so that ρ = MA n MA P = V RT where M A is the atomic or molecular weight of the gas species. A Combination of these equations gives dP M g = − A dx. P RT Integrating from sea level, P = P0 to some height above the earth, h, where the pressure is P P ∫ P0 h dP M g = − A dx P RT ∫ 0 leads to the barometric formula that gives the pressure as a function of altitude above sea level: P = P0e − M A gh RT = P0e m gh − A k BT (4.8) where mA is the atomic or molecular mass of species A (mA = MA/NA). Of course, Boltzmann’s constant, kB, is just equal to kB = R/NA = 8.314 J/mol/6.022 × 1023 atoms/mol = 1.381 × 10−23 J/atom. Actually, Equation 4.8 gives the pressure difference between two elevations separated by a distance, h. 4.5.1.1 Example: Atmospheric Pressure in Denver Denver is 5280 ft above sea level*, what is the pressure in Denver relative to sea level? If sea level pressure is 1 atm, then the pressure in Denver is P = 1× e − ( 28.84 × 10 −3 kg / mol )( 9.8 m/s2 )( 5280 ×12 × 2.54/100 m ) ( 8.314 J/mol − K )( 298 K ) = 0.833 atm and since 1 atm = 1013.2 millibar, P = 1013.2 × 0.833 = 844.9 millibar. * 103 dx dF = −g dm where g is the acceleration of gravity and m is the mass of the volume Adx and dF is negative because the force is downward. Now, Barometric Formula Denver is called the “mile-high city” and not the “1.6 km-high city.” Hence, the use of English units. 104 Chapter 4. Temperature Dependence of the Reaction Rate Constant The average molecular weight of air used for this calculation is given by M = 0.79 M( N 2 ) + 0.21 M(O2 ) = ( 0.79 × 28 ) + ( 0.21× 32 ) = 28.84 g /mol 4.5.1.2 Example: Atmospheric Pressure at the International Space Station The space station is about 220 miles high as it orbits the earth—high enough to miss most atmospheric friction but within the protection of the earth’s magnetic field to minimize radiation from solar mass ejection of energetic particles and cosmic rays. The pressure at this altitude is P = 1× e − ( 28.84 ×10 −3 kg / mol )( 9.8 m / s2 )( 220 mi ×1609 m / mi ) ( 8.314 J / mol − K )( 298 K ) = 3.79 × 10 −18 atm The actual pressure is 10−11 atm because there are temperature variations in the atmosphere as a function of altitude and the temperature is not a constant 298 K as assumed here. In any event, the International Space Station (ISS) operates in a pretty good vacuum. 4.5.1.3 Example: The Thickness of Earth’s Atmosphere Assume that the thickness of the atmosphere is that distance from sea level to where the atmospheric pressure drops to 0.01 atm or 1% of the sea level pressure. So h=− RT 8.314 × 300 × ln 0.01 4.06 × 10 4 m ln 0.01 = − = 4.06 × 10 4 m ∼ 25 mi −3 Mg 28.84 × 10 × 9.8 1609m / mi Now the radius of the earth is about 4000 mi, so that the thickness of the atmosphere is about 0.6% of the earth’s radius. You might remember Al Gore’s picture in An Inconvenient Truth (Gore 2006) showing the thickness of the atmosphere compared to the radius of the earth, and its thinness was striking. This is why! And it is thin! This was part of his argument about the effect of CO2 emissions on global warming. In reality, the “ocean of air” above us is really not so deep. Interestingly, Arrhenius, over 100 years ago, was worrying about the effect of atmospheric CO2 produced by industrial production on the earth’s temperature and predicted man-made global warming not greatly different from today’s more rigorous calculations (Arrhenius 1896). 4.6 BOLTZMANN DISTRIBUTION What is the relation between the Arrhenius equation and the barometric formula? Notice that M Agh or m Agh is the potential energy of the atoms at the higher elevation compared to the energy of the atoms at the lower elevation. As such, this is a Boltzmann distribution (Silbey and Alberty 2001). Again, since PV = nRT, the barometric formula could be rewritten as n = n 0e − E k BT = n 0e − Q RT (4.9) that is, the number of moles in some energy state E equals the number in the ground state n0, where E = 0, times an exponential factor that depends on energy difference between the two states relative to thermal energy, the Boltzmann factor. Both sides can be multiplied by Avogadro’s number to give the number of atoms or molecules in the two states, N and N0. So this expression could now be written as N ( E ) = N 0e − E RT (4.10) . If the total number of atoms or molecules available is NT, then ∞ ∫ ∞ ∫ N T = N ( E ) dE = N 0e 0 0 − E k BT dE = N 0 k BT (4.11) 4.6 Boltzmann Distribution which can be easily integrated by just letting x = E/kBT. So the fraction of atoms or molecules having energy E, f(E), is just N(E) 1 − k BT e = NT k BT E f (E) = (4.12) which is the Boltzmann distribution. This result could also be obtained by taking the fraction of molecules, f(E), having energies between E and E + dE written as f ( E) = (1/ N)(dN /dE) or E − 1 dN = A′e RT N dE f (E) = and can be integrated to get the value of A´: ∞ ∫ 0 ∞ ∞ E − dN = 1 = A′ e RT dE = A′RT e − x dx = N ∫ ∫ 0 0 ∞ − A′RT e − x = −A′RT e −∞ − e −0 = A′RT. 0 So A´ = 1/RT and f (E) = E dN ( E ) 1 − RT e dE = N RT (4.13) as before. Now, if molecules need a certain minimum energy to react, call it Q, then only those molecules or atoms with E ≥ Q will react, or the fraction of the molecules reacting will be ∞ E E − − 1 f (E ≥ Q) = e k BT dE = − e k BT k BT ∫ Q or f (E ≥ Q) = e − Q k BT ∞ Q (4.14) . Hence, the exponential dependence of the rate constants with temperature. Equation 4.14 is shown in Figure 4.9. f(E) Atoms or molecules with enough energy to react Q Energy, E ∞ FIGURE 4.9 Boltzmann distribution of energy showing that molecules with an energy greater than some minimum for reaction, Q, will react: shaded region. 105 106 Chapter 4. Temperature Dependence of the Reaction Rate Constant 4.7 4.7.1 THE ACTIVATED STATE aCtivatiOn energy An alternate way to justify the Arrhenius equation is to use a thermodynamic approach and assume that only certain atoms or molecules have energies in excess of the activation energy, EA, and that they are in some activated state. For example, for the reaction of H2 and I2 to form HI the hydrogen and iodine molecules will collide with each other in the gas phase, so there will be Z such collisions per second (Figure 4.10). However, only some of these molecules will have enough energy to react, namely, those in an activated state, H*2 , for example. Assuming a first-order reaction in hydrogen for simplicity, the reaction rate could be written as d [H2 ] = −Z H∗2 dt (4.15) where H*2 is the concentration of hydrogen molecules that have enough energy to react or the concentration of hydrogen molecules in the “activated state.” There is an equilibrium between the molecules in the activated state and those in a normal state, determined by an activation Gibbs energy, ΔG *, ΔG* = ΔH* − TΔS* and an equilibrium constant can be written for the reaction H 2 H*2 ∆G∗ ∆S∗ ∆H∗ H∗2 = K ∗ = e − RT = e R e − RT H 2 (4.16) so that the rate of reaction becomes ∆S∗ ∆H∗ − ∆S∗ − ∆H∗ − d H 2 = −Z H 2 e R e RT = − Ze R e RT [H 2 ] dt Q − = − k 0e RT H 2 = − k H 2 (4.17) which means that the activation energy, Q, is the activation enthalpy, ΔH*, and k 0 = Z exp(∆S∗ /R ) in k = k 0 exp(−Q/RT). The activation entropy, ΔS*, probably includes some orientation effects suggested in Figure 4.10, namely, the reacting molecules have to be oriented in a particular spatial relation, or close to it, in order to react. Two possible orientations are shown at the bottom of the figure. (a) Hydrogen, H2 Possible collision (b) configuration Iodine, I2 Another possible (c) collision configuration FIGURE 4.10 (a) Schematic representation of hydrogen and iodine molecules colliding in the gas phase to react to form 2 HI molecules. (b) Possible orientation configuration of the molecules when they collide. (c) Another possible orientation on collision. Note that the bonds between the atoms are represented by springs giving rise to the vibrational energy of the diatomic molecules. However, the distances between molecules and the lengths of the spring are greatly exaggerated. 4.7 Gibbs energy, G (kJ/mole) Activated state Reactants ΔG* Activation energy ΔG° Products Reaction coordinate/reaction extent FIGURE 4.11 Free energies as a function of the extent of the reaction from reactants to products. In order to react, the reactants must reach some activated state or activation free energy, ΔG*. However, it should be noted that all of these diatomic molecules are rapidly rotating and vibrating that makes the details of their interaction rather complex. Another way of representing this activated state is on a plot of the Gibbs energy as a function of the extent of the reaction or the reaction coordinate shown in Figure 4.11. ΔGo is the energy for the reaction, but for it to occur, molecules must be excited into the activated state having an energy ΔG* above the energy of the reactants. Therefore, there is an activation energy or activation barrier, ΔG*, that must be overcome for the reaction to proceed. 4.7.2 rOle Of a Catalyst It is usually stated that the role of a catalyst—something that speeds up(usually) the rate of a reaction but does not enter the reaction—is to lower the activation energy for reaction. For example, platinum is used to speed up the reaction between oxygen in hydrogen in a proton exchange membrane (PEM) fuel cell.* Platinum is also used as a catalyst to speed up the combination of oxygen ions diffusing through ionically conducting zirconia, ZrO2, to form oxygen gas in automobile oxygen sensors and, of course, it is used in large quantities as the oxidation catalyst in vehicle catalytic converters to oxidize CO and any unburned hydrocarbons in exhaust gases. However, catalysts usually play a more complex role than merely reducing the activation energy for a reaction. More generally, a catalyst provides an entirely different reaction pathway for a reaction to occur, most likely containing several different steps as shown schematically in Figure 4.12 (Haim 1989). As a result, to suggest that the primary role of a catalyst is to simply lower the activation energy for reaction is too simplistic. Although the intent is not to spend a lot of time on the atomistic or molecular details of reactions at surfaces or interfaces, one illustration is given for the simple case of what is thought to occur at the surface of platinum when it catalyzes the simple reaction of (Dickerson and Geis 1976; Friend 1993) H 2 (g) + D2 (g) 2HD(g) where D stands for deuterium or 2H. Figure 4.13 attempts to show the five steps envisioned to occur at the surface of the platinum. Note that because these are series steps, the slowest will control the overall rate. The steps are the following: (1) H2 and D2 adsorb onto the surface of the platinum. (2) The diatomic bonds in the H2 and D2 molecules are broken by the electronic attraction—and larger separation distance—of the electron orbitals of the platinum surface atoms. Eventually, most of the Pt sites on the surface are covered with single H or D atoms. When another molecule is absorbed to one of the few remaining empty sites, as in step 3, it can no longer be separated, but it is attracted to a neighboring H or D atom. The molecule can then exchange one of its atoms to the adsorbed * A PEM fuel cell is called either a polymer electrolyte membrane or proton exchange membrane fuel cell. The Activated State 107 Chapter 4. Temperature Dependence of the Reaction Rate Constant Without catalyst Gibbs energy, G (kJ/mole) 108 ΔG* with catalyst Reactants ΔG° Products With catalyst Reaction coordinate/reaction extent FIGURE 4.12 The effect of a catalyst on the reaction rate, activation energy, and activated state. The reality is that a catalyst frequently leads to a different pathway for the reaction that may show several steps, two in series are shown here, and not just lower the activation energy for the reaction. atom forming another molecule—on the average, an HD molecule. The HD molecule is shown on the platinum surface in step 4. Finally, the HD molecule desorbs from the surface as shown in step 5 releasing this site for further reaction. In reality, the H and D atoms are probably diffusing around on the surface, so that the locations of the open sites are constantly changing. Clearly, the electronic surface properties of the platinum are extremely important. There should be a sufficiently strong attraction between the Pt and the gas molecules to break the bond and separate the molecule into atoms, but not strong enough to form a permanent bond with either the diatomic molecule or a single atom at the surface. Understanding the details of the electronic structures of surfaces and their roles in catalysis is an active area of surface physics and chemistry research. It is very attractive to be able to tailor the electronic properties of an alloy or compound consisting of more readily available and cheaper materials than platinum or other noble metals. There have been instances in the past in which new catalyst compounds were thought to have been found only to have subsequent research show that the materials were contaminated with small platinum particles that were actually doing the catalysis. D H H D H D 1 1 H H 2 H H D 3 D H H D D 2 5 H D 4 FIGURE 4.13 Schematic representation of the reaction H2 (g) + D2 (g) 2HD(g) on the surface of a noble metal such platinum: adsorption of H2 and D2 on the surface (1), breaking of the molecular bond and separation of the atoms on the surface (2), the molecule interacts with a surface atom forming an HD molecule (3), HD molecule attached to the surface (4), and desorption of HD from the surface (5). Exercises Other good examples where catalysts provide more than just a decrease in activation energies are biological processes in which enzymes serve as catalysts. Take for example the oxidation of sucrose, sugar, C12H22O11. Sugar will burn in air being oxidized to C12H 22O11(s) + 12O2 (g) → 12CO2 (g) + 11H 2O(g) (4.18) and the large enthalpy for the reaction will sustain combustion just like any SHS reaction. In fact, a mixture of sugar and a good oxidizer such as potassium nitrate, KNO3, makes a nice solid fuel model rocket propellant. However, in the human body, enzymes take the sugar molecules apart slowly piece by piece generating the energy necessary for life. Clearly, the overall reaction pathways for combustion and biological oxidation of sugar are very different, and the enzymes do much more than just lower the activation energy of the reaction. Another example is the use of Ziegler–Natta catalysts (Claverie and Schaper 2013) on the polymerization of olefins, unsaturated hydrocarbon molecules with one or more carbon double bonds such as ethylene, H 2C=CH 2 . In this case, these catalysts—both homogeneous and heterogeneous—are designed to control, usually minimize, the branching of the polymer chain. As was seen in Chapter 3, radical polymerization is frequently used to make nominally linear polymers such as polyethylene, [CH 2CH 2 ]n. However, during polymerization, the radical may end up someplace along the chain, rather than at its end, forming a side branch and a branched polymer molecule. In contrast, Ziegler–Natta catalysts contain transition metal atoms, and the interaction of the monomers with the d-orbitals of these atoms adds additional monomers to the polymer molecule only at one site, essentially at the beginning of the molecule. As a result, these catalysts minimize branching. The lack of branching leads to better packing of the polymer molecules and a larger degree of crystallinity in polymers such as high density polyethylene, HDPE. These catalysts can also be designed to control the stereochemistry of the polymer chain, the tacticity, by determining how the various side groups arrange along the length of the polymer chain. Ziegler–Natta catalysts clearly demonstrate that the role of a catalyst is not merely to lower the activation energy for reaction but actually change the overall configuration of the polymer molecules. 4.8 SUMMARY The goal of this chapter has been to justify the exponential temperature dependence of reaction rate constants and how exothermic reaction rates can increase rapidly because of this strong temperature dependence. Strongly temperature exothermic rates can be taken advantage of in propulsion, welding torches, and the production of materials by combustion synthesis as examples. The first approach developed the barometric formula leading to the Boltzmann distribution for atoms and molecules as a function of temperature and the meaning of the activation energy. The thermodynamic approach to the activated state is presented, and the activation energy and the activated state are introduced. Finally, the role of catalysts in reaction kinetics is briefly discussed emphasizing that the role of catalysts is not merely to lower the activation energy for a reaction, but, more generally, achieve this by changing the paths or steps that take place in the catalyzed reaction compared to those in the absence of the catalyst. This chapter and the preceding two chapters have focused on homogeneous reactions to introduce the concepts of reaction kinetics. In the next chapter, heterogeneous reaction kinetics are introduced, specifically gas–solid reactions that play huge roles in many processes in materials science and engineering. EXERCISES 4.1 a. If k = 2.16 × 10−6 s−1 at 25°C and k = 5.35 × 10−2 s−1 at 100°C for a gas reaction, calculate the values of the preexponential factor and the activation energy. b. Make a plot of log10(rate) versus 1000/T over this temperature range. 109 110 Chapter 4. Temperature Dependence of the Reaction Rate Constant 4.2 Make a sketch showing the enthalpy versus temperature for both the products and reactants for a combustion reaction such as C2H 2 (g) + 3 / 2 O2 (g) H 2O(g) + 2 CO2 (g). Show a temperature at which combustion could initiate and the adiabatic combustion temperature. 4.3 a. The average heat capacities for various gases are CP(H2O) = 50 J/mol-K, CP(N2) = 33 J/mol-K, CP(CO2) = 55 J/mol-K. If the ΔH° at 30°C for the reaction H2(g) + 1/2 O2(g) → H2O(g) is −241.8 kJ/mol per mole of H2, calculate the adiabatic temperature for this reaction if ignition is at 30°C in pure oxygen. b. Do the same if the reaction occurs in air. 4.4 a. If the ΔH° at 30°C for the reaction CH4(g) + 2O2(g) → CO2 + 2H2O(g) is −802.5 kJ/mol per mole of CH4, calculate the adiabatic temperature for this reaction if ignition is at 30°C in pure oxygen. b. Do the same if the reaction occurs in air. 4.5 a. If the ΔH° at 30°C for the reaction C2H2(g) + 5/2O2(g) → 2CO2 + H2O(g) is −1256 kJ/ mol per mole of C2H2, calculate the adiabatic temperature for this reaction if ignition is at 30°C in pure oxygen. b. Do the same if the reaction occurs in air. 4.6 Calculate the air pressure (atmospheres) at the top of Mount Everest (29,029 ft). Do the same in millibar. 4.7 Calculate the number of atoms in an energy state 150 kJ/mol above the ground state having 6.022 × 1023 atoms at both 300K and 1300K. 4.8 Calculate the number of molecules that can react if the activation energy is 1 eV above the ground state containing 6.022 × 1023 molecules at both 300K and 1300K. 4.9 Calculate how many times a catalyst increases the reaction rate at both 300K and 1300K if the activation energy without a catalyst is 120 kJ/mole, while with a catalyst it is just one-half this value. The preexponential term is the same in both cases. REFERENCES Arrhenius, S. 1896. On the Influence of Carbonic Acid in the Air upon the Temperature of the Ground. Phil. Mag. J. Sci. 41(4): 237–276. Butts, A. 1943. Metallurgical Problems, 2nd ed. New York: McGraw-Hill. Cary, H. B. 1979. Modern Welding Technology. Englewood Cliffs, NJ: Prentice Hall. Claverie, J. P. and F. Schaper. 2013. Ziegler-Natta catalysis: 50 Years After the Nobel Prize. MRS Bull. 38(3): 213–218. (Note: the focus of the issue is Ziegler-Natta Catalysts). Dickerson, R. E. and I. Geis. 1976. Chemistry, Matter and the Universe: Integrated Approach to General Chemistry. New York: Benjamin-Cummings. Emsley, J. 2001. Nature’s Building Blocks. New York: Oxford. Friend, C. M. 1993. Catalysis on Surfaces. Scientific American. April: 74–79. Gore, A. 2006. An Inconvenient Truth. New York: Roble Books. Haim, A. 1989. Catalysis: New reaction Pathways, Not Just a Lowering of the Activation Energy. J. Chem. Ed. 66(11): 935–937. Laidler, K. J. 1984. The Development of the Arrhenius Equation. J. Chem. Ed. 61(6): 494–498. NIST. 2013. NIST Chemical Kinetics Database. Standard Reference Database 17, Version 7.0 (Web Version). Release 1.6.7. Data Version 2013.03. http://kinetics.nist.gov/kinetics/index.jsp. Provan, J. 2011. The Hindenburg. http://www.Amazon.com. Roine, A. 2002. Outokumpu HSC Chemistry for Windows, Ver. 5.11, thermodynamic software program, Outokumpu Research Oy, Pori, Finland. Silbey, R. J. and R. A. Alberty. 2001. Physical Chemistry, 3rd ed. New York: Wiley. Worek, M., ed. 2008. Nobel: A Century of Prize Winners. Buffalo, NY: Firefly Books. 5 Heterogeneous Reactions Gas–Solid Reactions 5.1 5.2 5.3 5.4 5.5 Introduction Gas Kinetics 5.2.1 Temperature and Speeds of Gas Molecules 5.2.2 Maxwell–Boltzmann Speed Distribution 5.2.3 Mean Molecular Speed 5.2.4 Flux of Gas Atoms Impinging on a Surface 5.2.5 Need for High Vacuum in Surface Studies 5.2.6 Condensation and Evaporation or Sublimation 5.2.6.1 The Model 5.2.6.2 Example: Sublimation of 1,4-Dichlorobenzene 5.2.7 Langmuir Adsorption Isotherm Gas–Solid Corrosion Reactions Gas–Solid Reactions in Materials Processing 5.4.1 Titanium Metal and TiO2 Pigments 5.4.2 Siemens Process 5.4.3 Optical Fibers 5.4.4 Halogen Bulbs Chemical Vapor Deposition of Silicon 5.5.1 Introduction 111 112 113 113 114 116 117 118 119 119 119 120 121 122 122 123 123 124 124 124 112 Chapter 5. Heterogeneous Reactions 5.5.2 Overview of Various Deposition Processes 5.5.2.1 Chemical Vapor Deposition 5.5.2.2 Epitaxy 5.5.2.3 Sputtering 5.5.3 The CVD of Silicon 5.5.3.1 Series Steps 5.5.3.2 Fluxes or Flux Densities 5.5.3.3 Possible Rate-Controlling Steps on the Surface 5.5.4 Deposition of Silicon from SiHCl3 5.5.4.1 Assumptions for the Model 5.5.4.2 Thermodynamics of the Reaction 5.5.4.3 Implications of Infinitely Fast Gas Diffusion 5.5.4.4 Deposition Rate Model 5.5.4.5 Deposition Rate Calculation 5.6 Active Gas Corrosion of Si in HCl and H2 5.7 Halogen Bulbs 5.8 Carbon–Carbon Composites 5.8.1 Introduction 5.8.2 Carbon–Carbon Composites on the Shuttle 5.8.3 CVD of Graphite: Pyrolytic Graphite 5.8.4 Fabrication of Carbon Fibers 5.8.5 Composite Fabrication 5.9 General Observations about Reaction-Controlled Growth 5.9.1 Kinetic and Thermodynamic Factors 5.9.2 Reaction Rate Constant and Accommodation Coefficient 5.9.2.1 Example: Condensation of Water Vapor to Ice 5.10 Summary Appendix Exercises References 5.1 124 124 125 126 127 127 127 127 128 128 128 129 130 131 132 132 135 135 135 135 136 137 138 138 139 140 141 141 146 148 INTRODUCTION In the previous chapters, the focus was on homogeneous reactions, with the exception for catalysts, and mainly on reactions in gases and liquids. In this chapter, the focus is gas–solid reaction kinetics, although many of the same principles apply to gas–liquid reactions. This is an area of great commercial importance in both the processing and performance of hard materials: metal, ceramics, composites, and electronic materials. It is also important in the processing and behavior of soft materials in a wide variety of environments. However, the focus is on hard materials because the various steps in the overall process are better understood with these materials. Moreover, these systems are 5.2 Gas Kinetics 113 engineered to give different characteristics depending on the requirements for the material or the environment it is being exposed to. In this chapter and several chapters to follow, the kinetic behavior of gas atoms and molecules are used extensively beginning with some kinetic theory of gases that apply directly to simple gas–solid or gas–liquid reactions such as condensation and sublimation that do not require any chemical reaction for the process to occur. The information obtained from these simple processes is useful when applied to chemical reactions such as the deposition of silicon from gas-phase reactants. The deposition of silicon from the gas phase is an excellent example of a gas–solid reaction of extreme importance in the fabrication of silicon integrated circuits, which, of course, have transformed the world we live in. A better example of materials enabling a system could not be found. The general concepts of heterogeneous reactions are illustrated by deposition from gaseous constituents. The major concepts to be encountered in this chapter are some aspects of the kinetic theory of gases, the factors important in gas–solid reactions, how gas–solid reactions are important in both deposition and corrosion processes, the wide variety of real processes to which these principles apply, and the interaction between kinetic and thermodynamic factors on solid growth kinetics. 5.2 5.2.1 GAS KINETICS TemperaTure and SpeedS of GaS moleculeS It is useful to begin by looking at the temperature dependence of the energies of atoms, ions, and molecules. Consider a box of with sides of equal length, L, with a monatomic gas atom having mass m and an x-component of velocity, v x, as shown in Figure 5.1. Assume that the walls of the box are impenetrable so the atom will hit a wall and rebound completely elastically in the negative x-direction. When it does so, the momentum change is ∆(mv) = 2 mv x—one for coming and one for going in the opposite direction with the same x-velocity. Therefore the force exerted by this single wall collision is simply = F ma = d(mv) dt (5.1) or ∆F = ∆(mv)/∆t where ∆t = time between collisions of this atom with this wall and is just the time it takes for the atom to travel to the back wall and return; that is, ∆t = 2L/v x. Therefore, the force per atom on the wall is ∆F = ∆( mv x ) 2mv x mv 2x = = . 2 L/v x ∆t L (5.2) If N is the total number of atoms in the box, then they all strike the wall in the time ∆t so the total force, F, is just N∆F and the pressure, P, is given by P = F/L2, so P= F N∆F Nmv 2x Nmv 2x = 2 = = L2 L L3 V (5.3) L m VX where V = L3 = volume of the box. Rearranging this, for an ideal gas N = PV Nmv == nRT = RT Nk BT NA 2 x Z (5.4) and therefore mv2x = k BT where NA is the Avogadro’s number and kB is the Boltzmann’s constant. The kinetic energy in the x-direction, KEx, for the atom is defined by Y X L L FIGURE 5.1 Model of a gas molecule moving in a cubic box of side L in the x-direction with a velocity v x used to calculate the translational kinetic energy of molecules. 114 Chapter 5. Heterogeneous Reactions z vz = KE x v vy vx 1 1 = mv 2x k BT. 2 2 (5.5) The velocity vector has three-components, one in each of the x, y, and z directions as shown in Figure 5.2. Therefore, y v2 = v2x + v2y + v2z x FIGURE 5.2 Schematic showing the x-, y-, and z-components of the velocity of a molecule that has a vector velocity v. and the total kinetic energy, KE, is given by the sum of the kinetic energies in each direction KE = 1 1 1 1 mv 2x + mv 2y + mv 2z = mv 2 2 2 2 2 1 1 1 3 KE = k BT + k BT + k BT = k BT. 2 2 2 2 (5.6) The second of these last two equations is a statement of the principle of equipartition of energy (Silbey and Alberty 2001) which essentially says that the microscopic modes—mechanisms—for absorbing energy will all have the same energy, 1/2 k BT, when things are in thermal equilibrium. For a monatomic gas, the only energy-absorbing modes are the translational energies in the three directions leading to KE = 3/2 kBT. This assumes that the temperature is not high enough to excite electrons into higher energy states, which does not happen at temperatures of normal interest.* From above, the RMS—root mean square—speed of gas molecules is defined as = v rms 3k BT = m 3k BT N A 3RT = m NA M (5.7) where M is the molecular or atomic weight. Take He gas as an example, M = 4 g/mol, at 300 K, v rms = = v rms = 3(8.314 J / mol ⋅ K)(300 K) = 1368 m / s 4.00 × 10 −3kg / mol 1368 m / s × 3600s / hour = 3060 mph 1609 m / mi 3060 mph = 4.02 Mach 761.2 mph / Mach where Mach 1 = 761.2 mph, the speed of sound at sea level. Even at room temperature, the speed of gas atoms is indeed very fast. 5.2.2 maxwell–BolTzmann Speed diSTriBuTion In most cases, the interest is in the average speed of the atoms and not in their RMS speed. This can be calculated from the Maxwell–Boltzmann speed distribution. In Chapter 4, it was shown * For example, at T = 1000 K: k BT = 1.38 × 10 –23 J/K × 1000 K = 1.38 × 10 –20 J = 1.28 × 10 –20 J/1.602 × 10 –19 J/eV = 0.08 eV which is considerably less than the several eV necessary for electron excitations. Note that at room temperature, T = 298 K, k BT ≅ 0.025 eV ≅ 1/40 eV. 5.2 Gas Kinetics that the distribution of energies for N T total atoms or molecules, or their fraction in a given energy state is E 1 dN 1 − k BT = e . N T dE k BT (5.8) This is an extension of the barometric formula that gives the number of molecules as a function of height above sea level, that is, their potential energy. The equivalence between the potential and kinetic energies of gas molecules is not surprising. For example, suppose an atom had a kinetic energy KE x = 1 / 2mv2z at sea level in the vertical direction, which is taken to be z. If it did not undergo any collisions with other gas molecules, then it would rise to a height where its initial kinetic energy would just reach its potential energy, its kinetic energy would go to zero, and then it would be accelerated back to earth ending with its initial kinetic energy. Therefore, the number of atoms at any given height, or potential energy, says something about the Maxwell distribution of the kinetic energy of atoms at sea level moving with a vertical velocity, v z; that is, mv 2z − 1 dN z = A′e 2 k BT N z dv z which considers molecules moving in the z-direction only, a Gaussian distribution (Figure 5.3) where A′ is just some constant (Moore 1955).* To evaluate the constant, A′, for molecules moving in the x-direction, this expression needs to be integrated; that is, ∞ ∞ ∫ A′ e − mv 2x 2 k BT dv x = ∫ dN −∞ −∞ Nx x − 1. (5.9) Let mv2x / 2 k BT = y 2 , or vx = (2 k BT /m ) y, and the integral becomes A′ 2 k BT m ∞ ∫e − y2 dy = 1. −∞ 2 ∞ Therefore, the key is evaluating the integral ∫−∞ e − y dy . How this is done is shown in Appendix A.2, and everyone needs to see this integration at least once in his or her career. In any event, from Appendix A.2 ∞ ∫ 2 e − y dy = π. (5.10) −∞ So A′ = * m 2πk BT Of course, in reality, no single molecule or atom travels very far (only about 0.1 μm at 1 bar and 300 K) before colliding with another gas atom or molecule, as will be seen when diffusion in gases is discussed later. Nevertheless, there is simply an energy exchange between atoms or molecules and there must have been some of them that had this energy at sea level and transfer their energy through multiple collisions to other atoms that made it to the higher potential energies. 1/Nx −x Vx FIGURE 5.3 One-dimensional Gaussian distribution of gas molecule speeds. dNx dvx +x 115 116 Chapter 5. Heterogeneous Reactions dV = 4πv2dv y and mv 2x v − dN x m = e 2 k BT dv x . Nx 2πk BT x This is only in one dimension and similar expressions exist for the other two directions (y and z) and what is of interest is the speed, v, which is v = v 2x + v 2y + v 2z , as shown in Figure 5.2. The fraction of molecules in three dimensions is just the product of the fractions in each direction, namely dv FIGURE 5.4 The volume element in spherical coordinates depending only on the radius, v, the molecular speed. dN dN x dN y dN z = N Nx Ny Nz m = 2πk BT 1 dN N dv v, speed (5.11) EA FIGURE 5.5 Maxwell–Boltzmann distribution for the molecular speed showing those molecules or atoms having energies above EA in the exponential tail of the distribution. 32 e − (5.12) m ( v2x + v 2y + v 2z ) 2 k BT dv x dv y dv z . Make the substitution for the speed, v, above, and change the volume element from dV = dv xdv ydvz to a spherical shell of radius v and thickness dv, so the volume element becomes dV= 4πv2dv = dv xdv ydvz, Figure 5.4, with the change in coordinate system shown in Appendix A.3. This gives the Maxwell–Boltzmann distribution for the speeds of gas atoms and molecules in thermal equilibrium: dN m = N 2πk BT 32 4πv 2 e − mv2 2 k BT dv (5.13) shown in Figure 5.5. The high speed tail end of this distribution, the shaded region in Figure 5.5, is essentially an exponential function. Note that Equation 5.13 could also be written in terms of the kinetic energy of the atom or molecule, ε = (1/ 2)mv2 as dN 2π = ε1 2e − εdε. N ( πk BT )3 2 5.2.3 mean molecular Speed By definition, the mean speed, v, is given by ∞ dN m v= v = N 2πk BT 0 ∫ 32 ∞ ∫ v4πv e 2 − mv2 2 k BT dv (5.14) 0 and substitution of z = mv2 / 2 k BT (or v = (2 k BT /m )z1 2) in the integral gives ∞ ∫ 0 v 4πv e 2 − mv 2 2 k BT ∞ ∫ = ∞ −z 2 3/ 2 1/ 2 1 2k T 2k T dv = 4π B z 3/ 2 B m 2 m 0 4 π 2 k BT 2 m z −(1/ 2) e − z dz 2 ∞ ∫ ze −z dz 0 ∫ 0 ze dz can be easily integrated by parts or found in most calculus books (Edwards and Penney 2002) 5.2 ∞ ∫ v 4πv e 2 − mv 2 2 k BT Gas Kinetics 117 2 dv = 0 ∞ 4 π 2 k BT −z −e ( z + 1) 0 2 m 2 = 4 π 2 k BT ( −0 + 1) 2 m so m v= 2πk BT 32 4 π 2 k BT 2 m 2 and gives the desired result for the mean speed, v= 8 k BT = π m 8 RT π M (5.15) which is about 7% smaller than the RMS speed, Equation 5.7. 5.2.4 flux of GaS aTomS impinGinG on a Surface The number of gas atoms that strike a solid or liquid surface per unit area, per unit time is a quantity of interest. Figure 5.6 shows how this can be approximated. Consider a column of gas of height h = vRMS that contains a number of gas atoms per unit volume, η, determined by the pressure. At any point in time, one-sixth of the gas atoms are moving in the −z direction and in 1 second all of these atoms in the column will strike the surface, so the approximate number of atoms striking the surface per unit area per unit time, I, the rate of impingement is (Hudson 1998) I≅ 1 ηv RMS . 6 (5.16) A better approximation would use the mean velocity, v, but this still is only an approximation. Equation 5.16 assumes that the atoms are only traveling in the three mutually perpendicular directions. The reality is the gas atoms can strike the area A from any direction. When this is taken into consideration, along with the mean velocity, the exact relation—as shown in Appendix A.4—is I= 1 η v. 4 (5.17) Substituting Equation 5.15 for v and η = N A P /RT gives I= I= A 1 N A P 8 RT 4 RT π M η NAP 2πRTM V 1/6 or as it normally found in the literature, I= P 2πmk BT (5.18) where Units(I) = atoms/m 2-s, Units(m) = kg/atom, and Units(P) = Pa. Not surprisingly, the impingement rate depends on the concentration of gas atoms, which is proportional to the pressure. FIGURE 5.6 A model to calculate the approximate number of gas molecules hitting a surface of area A per unit time with a mean speed v. Only 1/6 of the atoms per unit volume, η, are moving in the z-direction at any given time and only those strike the surface. 118 Chapter 5. Heterogeneous Reactions 5.2.5 need for HiGH Vacuum in Surface STudieS Take air with a mean molecular weight of M = 28.84 g mol (Chapter 4) or 28.84 × 10−3 kg/mol (M = 28.84 at a temperature of 25°C or 298 K at a pressure of 1 atm or 1.0132 × 105 Pa). Then, I= 1.0132 × 105 P = 2πmk BT 28.84 × 10 −3 2 ( 3.1416 ) 1.38 × 10 −23 ( 298 ) 23 × 6 . 022 10 ( ) (5.19) I = 2.88 × 1027 atoms m 2 ⋅ s = 2.88 × 1023 atoms cm 2 ⋅ s Suppose that an experimentalist wanted to study the surface properties of pure nickel, Ni, without any adsorbed oxygen impurities. If the atmosphere over the nickel were air, it might be expected that all of the oxygen molecules hitting the surface will react to form at least a monolayer—one atom thick—of nickel oxide, NiO, since it is stable in air at room temperature. The number of oxygen atoms impinging on the surface would simply be I O = 2I O2 = 2 × 0.21× 2.88 × 1023 atoms cm 2 ⋅ s =1.21× 1023 oxygen atoms cm 2 ⋅ s since air is 21% oxygen. For nickel, M = 58.693 g/mol and the density ρ = 8.90 g/cm3. So the number of Ni atoms per cm3 is ηNi = ( 8.90 ) 6.022 × 1023 ρ NA = M ( 58.693) ( ) ηNi = 9.13 × 1022 atoms cm 3 typical of most solids and liquids—something times 1022/cm3. The approximate number of nickel atoms per unit area is given by ( Ni /cm 2 ≅ η2Ni/ 3 = 9.13 × 1022 ) 2/3 Ni /cm 2 ≅ 2.03 × 1015 cm −2 . So the time it would take for the entire surface to be covered with a monolayer of NiO would simply be Ni / cm 2 2.03 × 1015 = = 1.68 × 10 −8 s ! IO 1.21 × 1023 About 10 ns, this means that the experimentalist must be pretty quick in carrying out the experiment if it is to be done on a surface essentially free of oxygen atoms! A more reasonable pace to perform such an experiment might be about 1 hour during which time, say, only 1% of the surface gets covered with oxygen. In that case, IO must be substantially reduced and can be estimated by IO = 15 Ni /cm 2 ( 0.01) 2.03 × 10 = time 3600 I O = 5.64 × 109 O cm 2 ⋅ s . Everything else being equal, this means that the pressure of air in the system would have to be reduced to about 5.64 × 109 /1.21 × 1023 ≅ 4.66 × 10 −14 atm. As seen in Chapter 4, the experiment might be best done on the outside of the International Space Station where the vacuum has about this value. However, modern vacuum systems can reach vacuums on the order of 10−11 torr* or in the * The quality of a vacuum is usually given in the units of torr = mm of mercury. One atmosphere = 760 torr. 5.2 Gas Kinetics order of 10−14 atm. Therefore, experiments on clean surfaces must be done in ultra-high vacuum on the order of 10−11 torr. 5.2.6 condenSaTion and eVaporaTion or SuBlimaTion 5.2.6.1 The Model Equation 5.18 also gives the rate of condensation or evaporation of atoms from the surface of a solid or liquid at equilibrium if the equilibrium pressure is pe, I= pe . 2πmk BT (5.20) If the solid or liquid is not in equilibrium with the gas that has a partial pressure p of the solid or liquid molecules or atoms in the gas phase, the Equation 5.20 needs to be modified to (Pound 1972), J′ = α ( p − pe ) (5.21) 2πmk BT where J′ is the atom flux density to—or away from—the solid or liquid surface depending on the relative values of p and pe: it p > pe, condensation will occur; if p < pe then evaporation or sublimation happens. Alpha, α, is called the accommodation coefficient or sticking coefficient (Adamson 1982) and is a positive quantity less than or equal to 1.0. If α ≠ 1.0 then the rate of condensation or evaporation is slower than if every atom or molecule that hit the surface stuck or remained there. Also, alpha less than one, implies that some kind of surface reaction must be occurring as well. An alpha of zero means that the atoms do not stick and just bounce off the surface. This situation will be explored in more detail later in this chapter. Also, the value of alpha may be different on evaporation than it is on condensation if the events are occurring far from equilibrium. However, for many substances, metals, inorganic compounds, and organics, α ≅ 1.0 when there is no chemical reaction but simply condensation or evaporation (sublimation) when near equilibrium (Pound 1972). 5.2.6.2 Example: Sublimation of 1,4-Dichlorobenzene Today, mothballs consist of 1,4-dichlorobenzene (Figure 5.7) that has a melting point of 53.5°C, a molecular weight of 147.00 g/mol, and a vapor pressure of pe = 3.27 × 10 −3 bar at 30°C (NIST Webbook). If there is no pressure of the compound in the gas phase, then dichlorobenzene will sublime. Assuming α = 1.0, then J′ becomes, J′ = ( )( ) 3.27 × 10 −3 bar 105 Pa/bar pe = 2πmk BT 2 ( 3.14.6 ) (147.00 × 10 −3 kg mol) / (6.022 × 1023 atoms mol) 1.38 × 10 −23 ( 303) ( )( ) J′ = 4.08 × 1024 molecules m 2 ⋅ s = 4.08 × 1020 molecules cm 2 ⋅ s and J= J′ 4.08 × 1020 = 6.78 × 10 −4 mol cm 2 ⋅ s . = N A 6.022 × 1023 Therefore, the dichlorobenzene is subliming as expected. Of practical interest is the rate of sublimation in terms of the thickness sublimed in a given amount of time. The density of dichlorobenzene ρ = 1.25 g/cm3 (Haynes 2013), so ( ) ρ g cm 3 1 J mol cm 2 ⋅ s = M ( g / mol ) A cm 2 ( ) ( ) ( dV cm 3 dt ( s ) ) Cl . (5.22) Cl FIGURE 5.7 The chemical structure of 1,4-dichlorobenzene. 119 120 Chapter 5. Heterogeneous Reactions For a sphere or radius a, V = (4 / 3)πa 3, dV /dt = 4πa 2 (da /dt ), and A = 4πa 2 so J= ρ da . M dt Therefore, the rate of evaporation, da/dt, is ( da M 147.02 6.78 × 10 −4 = J= dt ρ 1.25 ) da = 7.97 × 10 −2 cm s . dt This seems very fast compared to how long mothballs last, suggesting α ≠ 1.0, so there is some kind of surface reaction taking place and/or diffusion through the gas phase is rate controlling, the latter being more likely case. 5.2.7 lanGmuir adSorpTion iSoTHerm In Chapter 4, the role of catalysts in reactions was discussed: specifically, the adsorption of hydrogen and deuterium onto platinum and the catalytic role of the platinum surface in the exchange of hydrogen and deuterium atoms. A reasonable question to ask is, “What might determine the surface concentration of the adsorbed gases?” A simple way to approach this is through the equilibrium between the adsorbed gas and the atmosphere such as empty surface site, S + gas atom occupied surface site, S′; ∆Go (5.23) where ∆Go is the Gibbs energy of the adsorption reaction of the gas atoms (molecules) on the solid surface. An equilibrium constant for the reaction in Equation 5.23 can be written as [S′] = K = e− ∆RTG ° L [S ] P (5.24) where [S′] = θ, the fraction of occupied surface sites by the adsorbed gas, [S] = 1 – θ, the fraction of unoccupied surface sites, and P = pressure. So Equation 5.24 becomes θ = K LP 1− θ θ = K L P − θK L P θ (1 + K L P ) = K L P with the final result, the Langmuir isotherm (Adamson 1982; Hudson 1998): θ= K LP . 1 + K LP (5.25) If P = 1 bar and KL = 1 at 298 K, then θ = 0.5 or one-half of the sites are occupied and ∆G° ≅ 0. Now, ∆Go = ∆H o − T∆So and, of course, KL = e ∆S° R e − ∆H ° RT where ∆So is the entropy difference between the vibrations and translations of the atoms or molecules on the surface and the gas phase and ∆Ho is the enthalpy of adsorption. If the adsorbed atoms 5.3 Gas–Solid Corrosion Reactions 121 stick at one spot and do not translate on the surface, an estimate for the entropy change for water molecules adsorbing at 25°C and one bar is the entropy of sublimation of ice, ∆So298 ≅ −141.6 J mol ⋅ K (Roine 2002). In order to have K L = 1.0, ∆H° would have to be about −42, 200 Jmol. On the other hand, if there is 99% coverage (θ = 0.99), then ∆G o ≅ −11, 385 J mol or ∆H o ≅ −53, 568 J mol .* If θ ≅ 0.01, then ∆H o = −11, 435 J mol. All else being the same, as the pressure decreases, the fraction adsorbed decreases. Since the value of the bonding enthalpy, ∆Ho, determines what fraction of the surface is covered by an adsorbing gas, the boundary between physical adsorption and chemical adsorption or chemisorption becomes rather arbitrary and is around ∆H° = −10 k J mol: less negative for physical adsorption (Hudson 1998). 5.3 GAS–SOLID CORROSION REACTIONS Passive corrosion is the formation of a protective (usually oxide, but not always) layer that slows down the rate of further corrosion since this requires diffusion through the solid state, which is a slow process. For example, Figure 5.8 shows the passive oxidation of silicon to SiO2 that occurs at most oxygen pressures: Si(s) + O2 (g) → SiO2 (s). (5.26) Further oxidation occurs by either oxygen diffusing from the gas through the SiO2 to the Si–SiO2 interface or silicon diffusing from the Si–SiO2 interface to react with oxygen at the SiO2–gas interface. As a result, as the oxide layer gets thicker, the rate of oxidation becomes slower because of the greater distance the atoms (ions) must diffuse (to be discussed in greater detail in Chapters 10 and 14): the reason that it is called passive oxidation is that the rate decreases with time. In contrast is active corrosion. In this case, there is a gas–solid reaction with no formation of a protective solid layer, only gaseous products are formed with silicon at low oxygen pressures to form SiO, silicon monoxide gas,† as shown in Figure 5.9 and Equation 5.27 1 Si(s) + O2 (g) → SiO(g). 2 (5.27) This is called active corrosion because the rate of corrosion is constant—there is no protective layer developed to keep the solid from oxidizing or corroding further. Another example of active corrosion includes the oxidation of silicon carbide at low oxygen pressures SiC(s) + O2 (g) SiO(g) + CO(g). (5.28) Silicon carbide heating elements are frequently used in electric furnaces that operate up to about 1600°C. In an oxidizing atmosphere, a protective or passive oxide layer of SiO2 is formed on the SiC that slows oxidation. However, in reducing or very low oxygen pressure atmospheres, active gas corrosion will occur greatly reducing the life of the SiC heating elements. Therefore, such furnaces should never be used with reducing or low oxygen chemical potential atmospheres, to avoid frequent and expensive replacement of the heating elements. Oxygen Another example is the active oxidation of chromium metal in an oxidizing atmosphere with the production of CrO3 gas: 2Cr(s) + 3O2 (g) 2CrO3 (g). (5.29) An example that everyone is familiar with is the reaction of a hot tungsten filament in an incandescent bulb with air if the bulb is cracked or broken. The tungsten reacts to form WO3 gas that condenses on the cooler inside of the remaining bulb forming a white powder: * † See the discussion about catalysts and bonding in Chapter 4. SiO is a compound that exists only as a gas. On condensation it decomposes to solid SiO2 and Si. SiO2 O2 Si Silicon (Si) FIGURE 5.8 Model for the passive oxidation of silicon with the formation of a protective SiO2 layer through which either silicon or oxygen atoms must diffuse to continue the oxidation. 122 Chapter 5. Heterogeneous Reactions O2 SiO Surface reaction 2 Si + O2 = 2 SiO Silicon FIGURE 5.9 Active oxidation—gaseous corrosion—of silicon at low oxygen pressures with the formation of SiO gas and no SiO2 protective layer. 2W(s) + 3O2 (g) → 2WO3 (g) → 2WO3 ( s ) . (5.30) Finally, the chlorides of most metals are volatile and metals used in furnaces to incinerate dangerous chlorine-containing compounds can corrode: examples include the chemical weapon phosgene, COCl2, and PCBs—polychlorinated biphenyls (C12H10-xClx, where x = 1–10) once used as coolants in transformers. PCBs were banned in the 1970s because of their carcinogenic risk, but they still are found in older transformers and other electrical equipment. In addition, incinerators that burn PVC—polyvinylchloride—bags and other chlorinated polymers are subject to similar corrosion as are furnaces operating near sea water where NaCl in the atmosphere can be incorporated into the combustion gases. In each of these cases, the hot gases contain gaseous HCl or some other corrosive chlorine-containing gas. Most metals, nickel, for example, will undergo active gas corrosion to form volatile chlorides: Ni(s) + 2HCl(g) NiCl 2 (g) + H 2 (g). (5.31) Even the oxide refractory insulation in such furnaces is subject to similar active gas corrosion MgO(s) + 2HCl(g) MgCl2 (g) + H 2O(g). (5.32) In many cases, these active gas corrosion reactions are controlled by the surface reaction. As discussed Section 2.1.1 and shown again in Figure 5.9, in order for the active oxidation of silicon to occur, oxygen must: (1) be transported by diffusion through the gas to the solid surface (2) where it reacts with the silicon surface atoms and (3) the SiO product gas must diffuse away from the surface. Again, these are series steps and the slowest one controls the rate. In this chapter, the rates of surface reactions are considered to be slowest, and rate-controlling, and examined in detail. While active corrosion usually limits the lives of many components, the process can also be used to commercial advantage, as discussed in Section 5.4. 5.4 5.4.1 GAS–SOLID REACTIONS IN MATERIALS PROCESSING TiTanium meTal and Tio2 piGmenTS The Kroll process for making titanium consists of two important gas–solid reaction steps: TiO2 (s) + 4HCl(g) TiCl 4 (g) + 2H 2O(g) (5.33) TiCl 4 (g) + 2Mg(s) → MgCl 2 (s) + Ti(s). (5.34) TiO2 powders for paint pigments are made in extremely large quantities throughout the world by the reaction of TiCl4(g)—commonly referred to as tickle—produced by the reaction of TiO2 similar to the Kroll process with the subsequent re-oxidation of the TiCl4 to TiO2 (Equation 5.33 in reverse) 5.4 Gas–Solid Reactions In Materials Processing in a flame whose temperature is generated by the large enthalpy of oxidation of TiCl4 to TiO2. The Cl2 produced in the oxidation is recycled to produce more TiCl4 TiCl 4 (g) + O2 (g) TiO2 (g) + 2Cl 2 (g) (5.35) by essentially the reverse of this reaction, an active gas corrosion process. 5.4.2 SiemenS proceSS Another example of these reversible gas–solid processes is the Siemens process for making electronic grade silicon (EGS), which is close to 9-nines pure Si—only a few parts per billion (ppb) impurities— from metallurgical grade silicon (MGS)—about 98% pure 700 K → SiHCl3 (g) + H 2 (g). Si MGS (s) + 3HCl(g) ← (5.36) SiHCl3, trichlorosilane, is collected as a liquid that has a boiling point around 33°C allowing it to easily be distilled several times to obtain a very high purity final liquid. Multiple distillation is an important chemical engineering unit process. Because of the tremendous value added to pure trichlorosilane for electronic materials production, the cost of distillation is a minor part of the total cost of the final EGS. At higher temperatures, the reverse reaction takes place depositing high purity silicon 1300 K → Si EGS (s) + 3HCl(g) SiHCl3 (g, high purity) ← (5.37) either directly onto electronic devices or circuits or as polycrystalline material that is subsequently melted and grown into single crystals from the molten EGS. These crystals are then cut into wafers and processed into chips for electronic devices. 5.4.3 opTical fiBerS Another extremely important example of a gas–solid reaction is the production of optical fibers of high purity silica for fiber-optic applications, Figure 5.10. All of us are familiar with the green color of FIGURE 5.10 Silicon dioxide fibers for fiber optics applications. Original color photo changed to grayscale. Original photo attributed to BigRiz at Optical fiber, http://en.wikipedia.org/wiki/Fiber-optic. 123 124 Chapter 5. Heterogeneous Reactions window glass when viewed edge on. The greenish hue is caused by the presence of mainly iron ions dissolved in the glass that come from impurities in the starting SiO2 sand. These impurities absorb light, greatly reducing light transmission over long distances. As such, commercial, low cost glass would not be suitable as optical fibers now used in communications and many other devices, particularly in the medical field, because of the light loss over long path lengths. In order to achieve transparency over long distances—kilometers—very high purity SiO2 glass is required. To achieve this, semiconductor grade SiO2 (at least six-9s pure) is formed as a powder in the gas phase and deposited either inside or outside of a fused SiO2 tube by reacting SiCl4 with oxygen. SF6 gas is added to volatilize any residual impurities—for example, iron—as fluorides. Other oxides—GeO2 and P2O5—can be added in different radial concentrations to change the index of refraction across the radius of the fiber to ensure that light does not escape at the fiber surface. This porous SiO2 powder preform is then sintered to high density and drawn into fibers. This gas–solid deposition process requires the use of very high purity reagents—electronic grade—to produce the high purity SiO2 glass free of impurities that would limit its optical transmission. 5.4.4 HaloGen BulBS One final example used in certain high-intensity, tungsten-filament, halogen lamps where a halogen gas reacts to form a volatile halide and then undergoes the reverse reaction to deposit solid tungsten. For example, W(s) + I 2 (g) WI 2 (g) (5.38) where the reaction goes to the right at low—2500°C temperatures—and to the left at high— 2800°C—temperatures, which allows a bulb to operate at a higher filament temperature and higher light output. This process is discussed in more detail later. 5.5 CHEMICAL VAPOR DEPOSITION OF SILICON 5.5.1 inTroducTion An example of a gas–solid reaction that is surface reaction controlled is the deposition of silicon on a substrate from trichlorosilane, SiHCl3. This process is used to demonstrate the steps in developing a gas–solid surface reaction model since it is an important commercial process used for silicon integrated circuits and is well understood. The silane-related compounds that have been used in this process include the following (Haynes 2013). Silane Monochlorosilane Dichlorosilane Trichlorosilane Tetrachlorosilane (silicon tetrachloride) 5.5.2 SiH4 SiH3Cl SiH2Cl2 SiHCl3 SiCl4 Boiling point (°C) = −185 Boiling point (°C) = −30.4 Boiling point (°C) = 8.3 Boiling point (°C) = 33 Boiling point (°C) = 57.6 oVerView of VariouS depoSiTion proceSSeS Before discussing the details of silicon deposition, a brief summary of the different types of deposition processes and how they are used to produce a range of materials is presented. 5.5.2.1 Chemical Vapor Deposition Chemical vapor deposition (CVD) can be defined as the production of a solid from gas phase reactants. There are many variants in the CVD process used for the deposition of solids that include 5.5 Chemical Vapor Deposition of Silicon APCVD: atmospheric pressure CVD LPCVD: low-pressure CVD PECVD: plasma-enhanced CVD MOCVD: metal organic CVD In the latter case, compounds such as gallium arsenide, GaAs, are deposited for light-emitting diodes (LEDs) and vertical cavity surface-emitting lasers (VCSELs) by processes such as Ga ( CH 3 )3 (g) + AsH 3 (g) → GaAs(s) + 3CH 4 (g) (5.39) where the reactants are trimethyl gallium, Ga(CH)3, and arsine, AsH3, and are considered to be metal-organic compounds: hence, MOCVD. All of these are variants of essentially the same process except for PECVD, where the plasma generates ionic species and radicals that can speed up the reaction and give a very different reaction pathway. The reason for mentioning these variations on the CVD process is that they are frequently referred to in the materials literature only by their acronyms, so materials scientists and engineers need to be familiar with them. Another variant of the CVD process is chemical vapor infiltration—CVI—which is used, for example, to deposit graphite inside of a bundle of carbon fibers to form a carbon–carbon composite such as that used on the leading edge of the space shuttle, whose failure lead to the tragic destruction of the shuttle Columbia on re-entry. The process for making carbon–carbon composites is discussed in more detail later. In this example of silicon deposition, it is assumed that the surface reaction is controlling the deposition rate. In a real process, LPCVD is typically used to ensure this, since the rates of gas diffusion increase as the pressure decreases, making the surface reaction the slowest step in the sequence of the three series steps illustrated in Figure 5.11. This process is used to produce epitaxial layers of single crystal silicon on substrates of single crystal silicon—to change the additive or doping concentration—or on substrates of single crystal aluminum oxide, Al2O3—sapphire—to produce silicon on sapphire (SOS or SOI—silicon on insulator). The use of sapphire as a substrate is to electrically insulate or isolate the various electronic devices made on the silicon film since sapphire is a much better electrical insulator than silicon. 5.5.2.2 Epitaxy Epitaxy can be defined as the formation of a crystalline layer on a crystalline substrate in which there are definite crystallographic orientations between the crystal axes of the substrate and those of the layer. Homoepitaxy occurs when the layer is the same material as the substrate, that is, Si on Si. Heteroepitaxy occurs when they are different, that is, Si on Al2O3. SiHCl3 + H2 Gas 3HCl Reaction CVD silicon deposit Substrate FIGURE 5.11 Schematic description of the chemical vapor deposition, CVD, of silicon from trichlorosilane, SiHCl3, and hydrogen that shows the three series steps necessary for the deposition: (1) transport of the reactants to the surface; (2) the surface reaction; and (3) transport of the products, HCl, away from the surface. 125 126 Chapter 5. Heterogeneous Reactions 5.5.2.3 Sputtering Chemical vapor deposition is frequently used to deposit thin films—layers that are a micrometer thick or less. As such, CVD is very different than the other common process to deposit thin films, namely, sputtering, a form of physical vapor deposition (PVD). Sputtering and other PVD processes are briefly discussed here to contrast them with CVD. This is not to negate the importance of PVD processes because they are extremely important not only for forming electronic circuits but also are used for many other applications, including the partially reflective coatings on windows. There are other PVD processes for depositing thin films besides sputtering. These involve a source material at high temperature so that its vapor pressure is sufficiently high to produce a rather large flux of atoms to the substrate essentially as described by Equation 5.21 in an vacuum chamber similar to that shown in Figure 5.12. For example, aluminum and gold depositions are easily performed by heating the metals on a tungsten filament to temperatures high enough so the metals melt, wet the tungsten, and evaporate at a rate predicted by Equation 5.21. If the vacuum is sufficiently high, the atoms go directly from the filament and deposit on the target without any collisions with residual gas atoms in the vacuum deposition chamber. In contrast, sputtering can be defined as a process in which atoms, ions, or molecules are physically removed from a target material (composed of the same elements or compounds desired in the deposited layer) by bombardment with high energy ions or atoms and the target atoms deposit on a substrate. As such, the process is carried out in a vacuum with a high voltage between the target and substrate to give the bombarding atoms enough energy to remove atoms from the target. The sputtered atoms travel from the target and deposit on a substrate forming a thin film, as shown schematically in Figure 5.12. A vacuum is necessary so that the bombarding and sputtered atoms can travel far enough without colliding with other gas atoms before they reach the target or substrate. As shown in the sketch, argon ions are frequently used as the bombarding ions, and they are accelerated by the high voltage to gain enough energy to remove atoms—break the chemical bonds—from the target. This PVD process is usually slower than CVD and is typically limited to thin films. In contrast, CVD can be used to build up very thick layers such as the polycrystalline EGS silicon in the Siemens process that can reach tens of centimeters in thickness. It should also be noted that there are several variations of sputtering just as there are for CVD outlined above. For example, RF sputtering uses a radio frequency alternating field of about 14 MHz to prevent charge build-up on the target material and is particularly useful for sputtering insulators. Another variation is magnetron sputtering in which permanent magnets Si target Negative Several thousand volts Ar+ Low pressure Ar Si atom Si deposit Positive Substrate FIGURE 5.12 Schematic showing the formation of a thin-film of silicon by the process of DC sputtering. At low pressures and high voltages, argon atoms are ionized and accelerated at high energy to the silicon target where they physically eject silicon atoms from the surface. These atoms travel to, and condense on, the substrate material forming a silicon layer. 5.5 Chemical Vapor Deposition of Silicon are used to produce a magnetic field that focuses the sputtering ions onto the target to achieve higher sputtering rates. 5.5.3 THe cVd of Silicon Returning now to the details of silicon deposition by CVD, the modeling starts with the reaction of trichlorosilane with the hydrogen carrier gas, Equation 5.37. 5.5.3.1 Series Steps Again, for this reaction, there are three transport processes in series: ª ª ª Diffusional transport of the SiHCl3 to the Si surface The actual reaction at the surface Diffusional transport of the HCl and H2 product gases away from the surface These are series or sequential steps, and as was shown before, and again later, for this particular process, the slowest of series steps controls the overall rate of reaction. The transport of the gaseous reactants to and the products away from the surface are usually gaseous diffusion processes. Later, Chapters 8–12 are devoted to diffusion processes and CVD of silicon by diffusion control is covered in Chapter 10. 5.5.3.2 Fluxes or Flux Densities Since a surface reaction is being considered as the controlling step, it makes sense to consider the rate of reaction in terms of the rate per unit area of the surface. It is convenient to do this in terms of fluxes or flux densities, J, where the units of J are Units(J) = mol/cm2/s. For the reaction in question, the stoichiometry implies that the relation between the various fluxes is J(SiHCl3) to the surface = J(H2) to the surface = −J(Si) at the surface = −J/3(HCl) away from the surface. The 1/3 comes from the fact the there are three moles of HCl produced for every mole of SiHCl3 reacting and means that the flux of HCl away will be three times greater than the SiHCl3 flux to the surface. 5.5.3.3 Possible Rate-Controlling Steps on the Surface The actual surface reaction can consist of many possible molecular or atomistic series steps—similar to some of those presented for the H2 + D2 reaction on Pt presented in Chapter 4—which could include (among many other possibilities): ª ª ª ª ª ª ª ª ª Adsorption or sticking of the SiHCl3 molecules on the surface Adsorption of H2 molecules on the surface Splitting of the SiHCl3 and H2 into H, Si, and Cl atoms on the surface Migration (diffusion) of Si to the reaction site Reaction of Si at the reaction site Migration (diffusion) of H and Cl atoms to their reaction sites Reaction of H and Cl to form HCl somewhere on the surface Diffusion of HCl away from their reaction sites Desorption or removal of the HCl molecules from the surface As shown in Figure 5.13—a schematic illustration in which the atoms are depicted as cubes—the surface of a solid consists of partially complete atomic planes of atoms. The most likely site for surface reactions to take place is the kink site since atoms at this position have more unsatisfied bonds or fewer nearest neighbors than surface atoms on steps (ledges) or terraces. In principle, by changing the crystallographic orientation of the surface, the number of kink sites can be increased or decreased, thereby changing the rate of reaction since any surface will consist of low-surface energy planes. It is commonly observed that the rate of surface reactions on solids varies with crystallographic orientation and the variation of the number of kink sites with orientation can sometimes 127 128 Chapter 5. Heterogeneous Reactions Terrace Adatoms Kinks Step or ledge FIGURE 5.13 The classical picture of a surface where each cube in the drawing represents an atom. The important surface feature are named: terraces, steps or ledges, adatoms, and kinks, where the latter are the most likely spots for reactions to occur or atoms to stick. explain this effect. The adatom shown is basically unstable and will diffuse to a kink site, or the edge of a step or ledge, or perhaps leave the surface. Again, all of these atomistic steps are mainly in series since they must follow one another. For gas–solid reactions, the details of most such reactions are not known well enough to identify the slowest and singular rate-controlling step among these—and other—imaginable steps. Therefore, unless there is good experimental evidence to suggest otherwise, the assumption is made that the surface reaction rate is a simple first order reaction. 5.5.4 depoSiTion of Silicon from SiHcl3 5.5.4.1 Assumptions for the Model Any one of the silane compounds could be, and have been, used for the deposition of silicon by CVD. However, trichlorosilane is a liquid at room temperature and very near its boiling point, so it is easy to control its vapor pressure by slightly cooling the liquid and thereby controlling the pressure of SiHCl3 in the hydrogen carrier gas. In addition, its reaction rate covers a convenient range of temperatures for silicon deposition. To develop a model, several assumptions are made: (1) a surface reaction is the rate-controlling step—which implies that diffusion to and from the surface of the reactant and product gases is infinitely fast—that is, there are no concentration gradients in the gas phase; (2) the reaction goes to equilibrium; (3) a flowing reactor is used so that the pressure of SiHCl3 is constant in time; (4) the geometry is a flat surface (it could as easily be curved and the rate of deposition will be the same for a reaction-controlled process); (5) the HCl pressure in the gas is controlled to define the equilibrium pressure of SiHCl3; and (6) the surface reaction is first order. For gas–solid reactions, a first-order reaction is frequently observed and, if you had to guess, guessing a first-order reaction is probably correct.* This is the model for the reaction with these assumptions. How valid these assumptions are can only be determined by comparing model and experiment. If they do not compare favorably, then the model needs to be changed. However, it is just that, a model, and so there is freedom to assume whatever parameters are deemed necessary and important to model the real process. Most of science and engineering consists of trying to find better models of reality! 5.5.4.2 Thermodynamics of the Reaction Since the reaction is assumed to be first order, then the rate, expressed in terms of a flux, is * A first-order reaction is predicted by, and is consistent with, Equation 5.21. 5.5 ( J(SiHCl3 ) = − k [SiHCl3 ]0 − [SiHCl3 ]e =− Chemical Vapor Deposition of Silicon 129 ) k ( p0 (SiHCl3 ) − pe (SiHCl3 ) ) RT (5.40) which depends on the equilibrium pressure of the SiHCl3 at the surface. So this needs to be calculated. Assume a temperature of 1100°C and a p0(SiHCl3) = 0.1 bar, p(H2) = 1 bar as the carrier gas, and p(HCl) = 0.03 bar.* Note the similarity between Equations 5.40 and 5.21. These are very close to the values used in the actual CVD of silicon from SiHCl3. The overall reaction is SiHCl3 (g) + H 2 (g) Si(s) + 3HCl(g). (5.41) The Gibbs energy for this reaction at 1100°C is ∆Go = 43,280 J/mol (Roine 2002). Note that even though the free energy for the reaction is positive, it will still occur to some extent with these conditions. The equilibrium constant, Ke, is given by − Ke = e ∆G ° RT 43280 − 8.314 ×1373 =e = 2.26 × 10 −2 Therefore, a si p3HCl = Ke pSiHCl3 pH2 or pe ( SiHCl3 ) = (1.0 )( 0.03) = 1.19 × 10−3 bar. a si p3HCl = pH2 K e (1.0 ) 2.26 × 10 −2 3 ( ) Notice that even though the Gibbs energy for the reaction is positive, about 99% of the SiHCl3 is used up in the deposition ( p0 − pe = 0.1 − 0.001 = 0.099 ). The activity of Si is 1.0 since it is pure silicon and the total pressure in the system is slightly above one bar, which can be neglected. 5.5.4.3 Gas Implications of Infinitely Fast Gas Diffusion Since some of the SiHCl3 reacts, some HCl will be generated at the gas– solid surface. However, the assumption is that diffusion is infinitely fast compared to the rate of surface reaction. As a result, the hydrogen, HCl, and the SiHCl3 pressures must remain constant throughout the gas phase right up to the silicon surface—there can be no pressure gradient in the gas since the diffusion coefficient is assumed to be infinite (Figure 5.14). If just the opposite were true, that is, the surface reaction is infinitely faster than diffusion, then all of the surface pressures reach equilibrium and must be calculated from (p ( a Si p0HCl + 3x 0 SiHCl3 * )( −x p 0 H2 ) 3 −x ) = Ke (5.42) In reality, the pressure can probably be given in either atm or bar since all older thermodynamic data was based on a standard state of one atmosphere and much of the data has not been changed to a standard state of one bar. In reality, the thermodynamic data for most reactions are not known sufficiently accurately for the difference between one bar and one atmosphere to have a significant effect anyway. The NIST JANAF Tables, 3rd ed. (Chase et al. 1985) show the conversion factors used between the old and new definitions of the standard pressure state. p(H2) Silicon p(HCl) p(SiHCl3) pe(SiHCl3) Distance from surface FIGURE 5.14 Reactant and product gas pressures as a function of distance from the surface for the CVD of silicon from SiHCl3 and H2 with a surface reaction controlling the rate of deposition. Although some of the reactants are depleted and the HCl is increased in the reaction, their pressures or concentrations remain constant with distance since it is assumed that diffusion is infinitely fast and therefore there can be no pressure or concentration gradients in the gas phase. 130 Chapter 5. Heterogeneous Reactions where x is the pressure of SiHCl3 consumed (since this is an ideal gas, the pressure and the number of moles are proportional). This equation can easily solved numerically by iteration on a spreadsheet with the results: pe ( SiHCl3 ) = 7.13 × 10 −2 bar pe ( H 2 ) = 0.9713 bar pe ( HCl ) = 0.1161 bar. With diffusion control, only about 30% of the SiHCl3 reactant is consumed. This is fine in theory to calculate the two extremes, but for a real process, neither the diffusion flux nor the surface reaction will be infinitely faster than the other, and this leaves the pressures at the interface somewhat uncertain. The combined effects or reaction and diffusion on the concentrationdistance curves and surface concentrations are explored later in a model that takes into consideration both diffusion and reaction. Since HCl is a product of the reaction, adding HCl to the initial gas stream provides some control over the equilibrium pressures and the rate of deposition. For example, it is quite possible for the reaction to take place in the gas phase with the formation of small particles of silicon. In fact, silicon, silicon carbide, SiC, and silicon nitride, Si3N4, as well as other powders can be made in this way (Ring 1996). Putting HCl into the gas stream provides some control to prevent gas phase formation of silicon particles. Generating powders in the gas is desirable if the interest is in producing nanoparticles of high purity silicon, but it is not if the intent is to deposit a single crystal epitaxial layer of silicon. 5.5.4.4 Deposition Rate Model The flux of trichlorosilane to the surface determines the deposition rate, and this can be expressed as ( J(SiHCl3 ) = − k [SiHCl3 ]0 − [SiHCl3 ]e =− ) k ( p0 (SiHCl3 ) − pe (SiHCl3 ) ) RT where the [] represents concentration and the lower equation comes from [SiHCl3] = n/V = p/RT. Whether concentrations or pressures are used makes no difference. It just depends on what the value and units of k are. In this case, since the units of J are Units(J) = mol/cm2-s and the units of concentration are mol/cm3, so the units of k must be Units(k) = cm/s. And for this reaction, k = k0 e Q RT the values of k0 = 36.7 cm/s and Q = 67,200 J/mol can be calculated from data in the literature on the deposition of silicon (Campbell 1996, Wolf and Tauber 2000). It is necessary to relate the flux of SiHCl3 at the surface to the growing thickness of the silicon layer since this is really what is of interest, “How fast does the silicon layer grow?” This is simply a mass balance: the molar flux density of Si to the surface J that is producing the deposited silicon layer is VSi A Silicon − x FIGURE 5.15 Geometry of CVD silicon deposit used to calculate the rate of deposition, dx/dt. J(Si) = where: A is the area as shown in Figure 5.15 n is the moles of silicon. 1 dn A dt (5.43) 5.5 Chemical Vapor Deposition of Silicon Now, n= ρ VSi M where: ρ is the density of silicon = 2.33 g/cm3 M is the molecular weight of silicon = 28.09 g/mol VSi is the volume of the silicon layer Ax, where x = thickness. Note that M ρ = V = the molar volume of Si in cm3/mol. Making the mass balance—per unit area per unit time, as in Equation 5.22—and since Si is deposited as SiHCl3 is consumed, J(Si) = −J(SiHCl3 ) 1 ρ dV 1 ρ k dx = A = p0 ( SiHCl3 ) − pe ( SiHCl3 ) A M dt A M dt RT ( ) or dx Mk = ( p0 (SiHCl3 ) − pe (SiHCl3 ) ) dt ρRT (5.44) which is the rate of deposition, frequently reported, and can be integrated to give the thickness x of the deposited silicon layer as a function of time: x= Mk ( p0 (SiHCl3 ) − pe (SiHCl3 ) ) t. ρRT (5.45) The flux density of the silicon is opposite to the flux density of the trichlorosilane since it is increasing in thickness while the SiHCl3 is disappearing. This sign difference is also correct in a directional sense since the thickness is increasing in the positive vertical direction while the SiHCl3 is disappearing in the negative direction. 5.5.4.5 Deposition Rate Calculation To begin, collect all the parameters for the process in the above equations: T = 1373 K ρ = 2.33 g/cm3 M = 28.09 g/mol p0(SiHCl3) = 0.1 bar pe(SiHCl3) = 1.19 × 10−3 bar p(H2) = 1 bar k = k0e–(Q/RT) k0 = 36.7 cm/s Q = 67,200 J/mol R = 8.314 J/mol-K R = 83.14 cm3-bar/mol-k Chosen deposition temperature Density of silicon Molecular(atomic) weight of silicon Initial trichlorosilane pressure Equilibrium trichlorosilane pressure Hydrogen pressure, assumed constant Reaction rate constant Pre-exponential Activation energy To calculate k In the denominator of Equation 5.45 Calculating a value for k at 1373 K: k = k 0 exp(−Q /RT) = 36.7 exp[ −67, 200 /(8.314 × 1373)] = 0.102 cm /s so the rate of deposition dx/dt is ( ) dx 28.09 0.102 = 0.1 − 1.19 × 10 −3 = 1.06 × 10 −6 cm / s . dt 2.33 83.14 × 1373 (5.46) 131 132 Chapter 5. Heterogeneous Reactions Since the rate of deposition is constant, the layer thickness is just the product of the rate and time. Therefore, the time to grow a 10 μm layer would be x =t dx dt 10 × 10 −4 cm 1 × = 15.7 min. −6 1.06 × 10 cm /s 60 s / min (5.47) These rates and times are in the range of those that are actually used in industrial practice. 5.6 ACTIVE GAS CORROSION OF Si IN HCl AND H2 Notice in the above equation for the deposition rate, Equation 5.44, dx Mk = p0 ( SiHCl3 ) − pe ( SiHCl3 ) dt ρRT ( ) that if the p0(SiHCl3) were actually less than pe(SiHCl3), then the rate of deposition would be negative. That is, the silicon surface would be undergoing active gas corrosion or etching. As was shown earlier in Chapter 3, for a first-order reaction with a first order back reaction leading to equilibrium, the overall reaction rate constant is the same for both directions of the reaction: k = k1(forward) + k2(back) So the same value of k holds for corrosion and if the assumption is made that p0(SiHCl3) = 1 × 10−3 atm—less than the equilibrium pressure, then ( ) dx 28.09 0.102 = 0.001 − 1.19 × 10 −3 = − 2.05 × 10 −9 cm / s. dt 2.33 83.14 × 1373 (5.48) This demonstrates that exactly the same type of surface reaction kinetics apply to both active gas corrosion and CVD reactions. Which occurs depends on the concentrations of the reacting gas species and how fast either occurs depends on the value of the reaction rate constant for deposition or corrosion. 5.7 HALOGEN BULBS There are certain types of halogen lamps that use a combination of both active gas corrosion and CVD to allow operation at higher temperature and, therefore, a higher light output or brightness (halogen bulbs). These lamps contain a normal tungsten filament (Figure 5.16) that typically consists of a double 100 μm FIGURE 5.16 Tungsten filament from a burned-out bulb. The diameter of the tungsten wire is about 45 μm and consists of a double helix. 5.7 Halogen Bulbs W-sublimation Without halide Tthin Tthin > Tthick (a) With halide A (b) W + Cl2(g) = WCl2 gas corrosion Tthick CVD tungsten B WCl2 = W + Cl2(g) CVD of tungsten FIGURE 5.17 (a) how a tungsten filament can fail in an incandescent bulb due to evaporation of tungsten from the thinner and hotter part of the filament. (b) the active gas corrosion reaction of tungsten with a halide gas at lower temperatures and the reverse reaction, CVD of tungsten, at the higher temperatures or thinner part of the filament. This prevents thinning of the filament allowing it to be used at higher temperatures giving off more light. helix of tungsten wire about 45 μm in diameter and a small amount of halogen gas or substance that produces a gas such as I2, Br2, or Cl2, so that the following reversible reaction can take place: low T → WCl 2 (g). W(s) + Cl 2 (g) ← high T Regular incandescent bulbs eventually burn out because a hot spot forms at a thinner region in the filament as shown in Figure 5.17. At the high operating temperatures of these filaments—in the neighborhood of 2800°C—the bulbs burn out by sublimation of the hot tungsten onto the glass bulb causing darkening or dark areas on the inside of the bulb. As a filament region thins, it gets hotter because its electrical resistance goes up and sublimes tungsten at a faster rate, getting thinner, which in turn increases its electrical resistance and gets hotter until the thin region opens and the bulb fails (Figure 5.18). However, the tungsten filament in a halogen lamp (Figure 5.19) will Tungsten deposit 4 5 6 7 8 9 FIGURE 5.18 Burned-out incandescent bulb showing blackening of the inside of the bulb due to evaporation and deposition of tungsten on the inside of the glass envelope leading to eventual bulb failure. 133 Chapter 5. Heterogeneous Reactions 1 cm FIGURE 5.19 A small halogen bulb. interact with halogen-containing gases in the bulb to produce volatile tungsten halides as shown in Figure 5.20. This figure gives the equilibrium pressure of WCl2(g)—and those of Cl(g), WCl, and WCl3, the species with the highest vapor pressures—over tungsten in chlorine. The important point to note is that the WCl2(g) pressure is higher at lower temperatures than it is at high temperatures. This means that W can be transported from lower temperature regions via WCl2—active gas corrosion—and deposited at higher temperature regions—CVD—as shown in Figure 5.17, keeping the hot regions from getting thinner and preventing bulb burnout. As a result, such halogen bulbs are not only brighter but also have a longer life—taking advantage of the sublimation and deposition phenomena, which itself is determined by the thermodynamics and kinetics between the halogen gas and tungsten. These halogen bulbs are typically small, so that the glass bulb gets quite hot. As a result, the bulbs are made from amorphous SiO2 or fused quartz—SiO2 glass—that has a much higher glass transition temperature, about 1200°C—and softening temperature—than conventional soda-limesilica glass bulbs with glass transition temperatures around 500°C. However, because of the much higher operating temperature of the silica envelope, care must be taken not to contaminate the surface, particularly with the sodium from fingerprints. The sodium enhances devitrification— crystallization—of the silica, which appears as white powdery regions on the exterior of a bulb reducing light output and forming a potential source for cracking of the silica. 1 Cl 10−1 WCl2 10−2 Mole percent 134 10−3 Cl2 10−4 WCl 10−5 WCl3 10−6 10−7 2000 2200 2400 2600 Temperature (°C) 2800 3000 FIGURE 5.20 Calculated equilibrium gas pressures of the major tungsten-containing gases over tungsten in an inert atmosphere containing 1m/o Cl2 (Roine 2002). Note that major species, WCl2, has a higher pressure at lower temperatures. The operating temperature of such a bulb is in the neighborhood of 2500°C–2800°C. 5.8 Carbon–Carbon Composites 5.8 135 CARBON–CARBON COMPOSITES 5.8.1 inTroducTion The destruction of the space shuttle Columbia during its reentry into the atmosphere in 2003 (Figure 5.21) is believed to have been caused by fracture of the carbon–carbon composite on the leading edge of the wing by a piece of polymer foam falling from the fuel tank on lift-off (Columbia Accident Investigation Board 2003). Since carbon–carbon composites are complex materials that often involve the use of the chemical vapor infiltration, CVI, process to bind the carbon fibers together, it is appropriate to say a little about carbon–carbon composite processing. 5.8.2 carBon–carBon compoSiTeS on THe SHuTTle Carbon–carbon composites are used on the leading edges of the wings, fin, and nose of the shuttle—the black areas seen in Figure 5.21—because they are light weight and can withstand temperatures over 2000°C with no degradation in their mechanical properties. These composites are used in these locations because of the potential for aerodynamic heating on re-entry reaching temperatures on the order of 1600°C. Unfortunately, carbon–carbon composites are brittle. In previous shuttle flights, there was evidence that some of the carbon–carbon composite parts had undergone damage—chunks of the material removed by brittle failure from impacts with some type of foreign objects. The investigation into the accident determined that it was likely that insulating foam hitting the leading edge of the shuttle wing on lift-off ultimately lead to its destruction on reentry. As part of the accident investigation, pieces of foam were fired from an air gun at the likely failed composite parts with the result that large holes—over 1 ft in size—could be produced in these parts as Figure 5.22 demonstrates (Columbia Accident Investigation Board 2003). 5.8.3 cVd of GrapHiTe: pyrolyTic GrapHiTe Pyrolytic graphite can be made into free-standing parts or coatings several centimeters thick for a number of high-temperature applications. These components are produced by the CVD process with a reaction such as the decomposition of methane (Pierson 1999), CH 4 ( g ) temperature → C ( s ) + 2H 2 ( g ) . FIGURE 5.21 Columbia prior to its final launch of January 16, 2003. Note the black carbon– carbon composite leading edges of the wings. NASA Photograph, Kennedy Space Center (Columbia Accident Investigation Board 2003). Original color photograph transformed to grayscale. FIGURE 5.22 Large hole produced in one of the shuttle wing leading edge carbon–carbon composites by a piece of insulating foam fired from an air gun to mimic the piece of foam that hit the orbiter upon lift-off. NASA Photograph (Columbia Accident Investigation Board 2003). Original color photograph transformed to grayscale. (5.49) The actual reaction kinetics are presumably more complicated than suggested by Equation 5.49 with several intermediate parallel and series steps. Nevertheless, so called pyrolytic graphite, polycrystalline graphite, can be deposited by this overall reaction at temperatures of 1100°C and above over a range of total pressures from 10 −3 to 1.0 bar. The result is a columnar grain—long along the growth direction—structure as depicted in Figure 5.23. Presumably grains or crystallites having the best orientation for growth grow the fastest and produce the columnar structure. For pyrolytic graphite, the sheets of graphene (a sheet of hexagonally-arranged carbon atoms one atom thick in graphite) are lined up parallel to the substrate surface and so is the a-axis of the graphite structure while the c-axis is parallel to the growth direction or parallel to the long axes of the columnar grains. This leads to a strong anisotropy of many properties such as thermal conductivity due to the covalent bonding along the a-axis and van der Waals bonding in the c-direction. For example, Chapter 5. Heterogeneous Reactions CH4 = C(s) + 2 H2 Columnar grains a-axis c-axis Growth direction 136 Substrate FIGURE 5.23 Schematic microstructure of a pyrolytic graphite deposit depicting the columnar grain structure from the decomposition of methane. The c- and a-axes of the graphite crystals are shown. The columnar grains extend through the thickness of the deposited layer that may be as thick as several centimeters. Because of this strong preferred orientation, properties such as thermal conductivity along the a-axis may be as much as 100 times larger than that along the c-axis. the thermal conductivity along the a-axis of the structure is on the order of 100 W/m-k while in the c-direction it is on the order of 1 W/m-k. This anisotropy in properties can be utilized to optimize the performance of a part such as a rocket nozzle. This is the kind of carbon or graphite deposition that is used in CVI to infiltrate and bond together the carbon fibers in a carbon– carbon composite. 5.8.4 faBricaTion of carBon fiBerS By far, the majority of carbon fibers are used to reinforce polymers to form carbon-fiberreinforced-polymers, CFRPs. These composites are now used not only in military aircraft but also in civilian aircraft structural parts, as automotive parts, and as high-technology bicycle frames as well. They are produced by many manufacturers by largely proprietary processes. Nevertheless, there are several principles that are fairly common in making fibers. They are all made from carbonrich polymer resins, an example being polyacrylonitrile (PAN), as shown in Figure 5.24. The polymer is mixed with a solvent to form a viscous material that is drawn into fibers. This drawing process helps to align the polymer molecules and, what will become, the graphite rings parallel H H C H Polymerization C CN n C Acrylonitrile N Polyacrylonitrile (PAN) low T CN n PAN1 to PAN2 300°C, air N −H2O n N n 2000°C, argon −N2, graphite FIGURE 5.24 The formation of polyacrylonitrile (PAN) and its multistep thermal transformation to graphene sheets in carbon/graphite fibers. 5.8 Carbon–Carbon Composites to the long axis of the fiber. The solvent is then removed by extraction in another solvent or by evaporation. The polymer fiber is given a low temperature treatment in oxygen or air to remove hydrogen and finally a high temperature graphitization reaction in excess of 2000°C to remove the nitrogen from the structure and form graphene sheets whose a-axes lie parallel to the fiber axis. During heat treatment, tension is applied to the fiber to enhance the alignment of the graphite sheets along the fiber axis increasing the modulus of elasticity of the fiber (Buckley and Edie 1992). The finished fibers are about 8 µm in diameter, have elastic moduli of about 300 GPa (43 × 10 6 psi) and fracture strengths on the order of 3.1 GPa (443,000 psi) (Matthews and Rawlings 1994). Compare these values to those of mild carbon steel with an elastic modulus about 200 GPa (26 × 10 6 psi) and a tensile strength around 430 MPa (61,000 psi) (Ashby and Jones 1980). Carbon fibers are sold commercially in bundles or yarns or tows consisting of several thousand individual carbon fibers. 5.8.5 compoSiTe faBricaTion Carbon–carbon composites are made from woven carbon fibers yarns—as bundles or fabric—that are formed into the shape of the part to be made—the prepreg (Savage 1993). One process consists of infiltrating the porous fabric with a phenolic resin (or any number of carbon-rich resins)—a thermosetting resin produced by the reaction of formaldehyde, CH2O, and phenol, HOC6H5—cured and pyrolyzed (heated in a nonoxidizing atmosphere to drive all volatile gases leaving only carbon behind) to graphite at some elevated temperature in excess of 2000°C. The graphite forms a rigid bond between the fibers producing a solid piece. A variant is to use a CVD process to deposit the graphite in the interstices between the carbon fibers, such as in Equation 5.49 (Savage 1993): CH 4 ( g ) temperature → C ( s ) + 2 H 2 (g); ∆G o (1500°C ) = −103kJ / mol. This process is chemical vapor infiltration (CVI) and is a variation of the CVD process in which the conditions are controlled, so that surface reaction is the slower step and is rate controlling. This ensures that the reactant gas concentrations are essentially uniform throughout the fibrous part— since diffusion is relatively fast—and the deposition rate will be the same throughout the part. This also implies that low pressures are preferred since diffusion in gases varies inversely with the pressure as will be seen later. Figure 5.25 shows a schematic microstructure of a typical carbon–carbon composite infiltrated by CVI. Usually, several infiltrations by CVI are necessary as the surface reaction is still sufficiently fast to close the surface porosity and stop the reaction. As a result, the part must be cooled and the surface ground to remove the dense graphite layer exposing the porosity in the structure to allow additional CVI. Graphite fiber Braid or tow CVI layer Porosity 50 μm FIGURE 5.25 Schematic microstructure of a carbon–carbon composite showing three braids or tows of carbon fibers woven together in different directions showing: carbon fibers, CVI carbon layer, and residual porosity. 137 Chapter 5. Heterogeneous Reactions For the carbon–carbon composites used on the space shuttle, the outer surfaces of the parts are given a CVD coating of SiC by a similar reaction to close any remaining porosity and slow down the rate of oxidation of the carbon–carbon SiHCl3 ( g ) + CH 4 ( g ) SiC ( s ) + H 2 ( g ) + 3 HCl ( g ) ; DG o (1200°C ) = −100 kJ /mol. Here, diffusion control of the reaction is important, so that all of the reaction takes place at the surface and sealing it. Unfortunately, SiC has a larger thermal expansion coefficient than that of graphite, and the SiC layer cracks on cooling. The cracks are filled with TEOS—tetraethyl orthosilicate or tetraethoxysilane—Si(C2H5O)4, which reacts with water at room temperature to form SiO2 (glass) that seals the cracks at high temperatures.* When completed, a typical carbon–carbon composite still contains about 15 volume percent porosity (Buckley and Edie 1992). 5.9 5.9.1 GENERAL OBSERVATIONS ABOUT REACTION-CONTROLLED GROWTH KineTic and THermodynamic facTorS Looking again at the equation for the growth of silicon from SiHCl3 (Equation 5.44) dx Mk = p0 ( SiHCl3 ) − pe ( SiHCl3 ) dt ρRT ( ) it should be noted that—other than the constants—the rate of growth, dx/dt, is essentially a product of a kinetic factor, k, and a thermodynamic factor, [p0(SiHCl3) – pe(SiHCl3)]. The kinetic factor decreases exponentially with decreasing temperature while the thermodynamic factor increases linearly with the difference between the ambient pressure and the equilibrium pressure—which in many cases decreases with temperature—as sketched in Figure 5.26. Therefore, the product of these two factors frequently leads to a maximum in the growth rate at some temperature below the equilibrium temperature as evident in Figure 5.26. Equilibrium T, Te Overall rate Temperature 138 Kinetic factor ∝ exp(–Q/RT) Thermodynamic factor ∝ (Te − T) Growth rate FIGURE 5.26 Schematic of the growth rate as a function of temperature for a phase transition below the equilibrium temperature. The growth rate depends on two factors, a thermodynamic factor, proportional to ( T − Te ) and a kinetic factor that typically is proportional to exp( −Q / RT ) where Q is the activation energy. The product of the two factors leads to a maximum in the growth rate at some temperature below the equilibrium temperature. Similar plots could be made for growth rate versus composition or vapor pressure, etc. * TEOS is used in the semiconductor industry to produce SiO2 glass insulating layers by CVD on silicon microchips. 5.9 5.9.2 General Observations about Reaction-Controlled Growth reacTion raTe conSTanT and accommodaTion coefficienT If the rate of evaporation, sublimation, or condensation of a substance does not follow Equation 5.18 p 2πmk BT I= then an accommodation coefficient, α, is inserted to give Equation 5.21 J′ = α ( p − pe ) 2πmk BT where J′ is the atomic or molecular and Units(J′) = atoms/m2-s. Dividing Equation 5.21 by NA, gives the molar flux, J, with Units(J) = mol/m2-s J= α ( p − pe ) J′ = . NA 2πMRT (5.50) If α ≠ 1.0, then there must be some kind of surface reaction taking place, ( J = k A − A e ) (5.51) where: A is some gaseous species Ae is the equilibrium concentration for condensation, sublimation, or evaporation. As seen in Chapter 2 and as Equation 5.50 suggests, the surface reactions in Equation 5.51 are usually first order. In this equation, it is convenient to express concentrations in mol/cm3 so that Units(k) = cm/s. The question is, “What is the relationship between α and k?” Expressing Equation 5.51 in terms of pressures, it becomes J= k ( p − pe ) . RT (5.52) Equating Equations 5.50 and 5.52 gives the relationship between the accommodation coefficient, α, and the reaction rate constant, k, J= α ( p − pe ) 2πMRT = k ( p − pe ) . RT (5.53) If the units of pressure are Pa, the left-hand side of this equation has units of mol/m 2-s. If the units of k are Units(k) = cm/s, then the units of R must be Units(R) = (Pa-m3)/(mol-K) so the right-hand side must be divided by 100 cm/m, that is, Units ( J ) = ( cm s ) Pa 1 1 mol = . 8.314[Pa ⋅ m 3 / ( mol-K )] × K 100 cm m 100R m 2 ⋅ s So the relationship between α and k becomes α = 10 −2 2πM k. RT (5.54) This assumes that the pressure units in Equations 5.50 and 5.52 are the same and Units(p) = Pa. So if the units of p in Equation 5.52 are something other than pascals, then a different value of the gas constant in Equation 5.52 appropriate to the pressure units must be used. 139 Chapter 5. Heterogeneous Reactions 5.9.2.1 Example: Condensation of Water Vapor to Ice The growth of ice crystals in an atmosphere containing water vapor is important in environmental science and meteorology to understand cloud formation kinetics at high altitudes. Figure 5.27 shows some calculated data of growth of ice crystals from the gas phase as a function of temperature where the ambient H2O pressure is at equilibrium at −5°C, assuming surfacereaction limited growth (Equation 5.52). In this case, k = k0 e − Q RT with k 0 = 0.6 cm s and Q = 10 kJ mol arbitrarily chosen—and not necessarily the real values—in order to give a growth curve that clearly shows the product of the thermodynamic and kinetic factors illustrated in Figure 5.27. These data clearly indicate that a maximum in the rate occurs at about −25°C and, that above −5°C, the crystal actually sublimes since its vapor pressure is greater than that of the ambient H2O pressure. How realistic are these values for k0 and Q? There have been many determinations of the accommodation coefficient for condensation of water vapor on ice and ice sublimation and the approved value for these temperatures is α ≅ 0.7, although it is somewhat temperature dependent and wide variations in its value have been reported by different investigations (IUPAC Data Sheet 2009). In this case, taking the data at the maximum growth temperature, −25°C, where the calculated value of k is k = 4.70 × 10 −3 cm s , the calculation of the accommodation coefficient gives, α = 10 −2 α = 10 −2 2πM k RT ( 2π 18 × 10 −3 8.314 × 248 ) ( 4.70 × 10 ) −3 α = 3.48 × 10 −7 280 p(H2O) = 4.02 × 10−3 atm −20 Maximum rate Sublimation −40 220 −60 Temperature (°C) 240 0 Te = −5°C 260 Temperature (K) 140 200 −80 180 −100 −1 0 1 2 Growth rate (10−8 cm/s) FIGURE 5.27 A plot of growth rate of ice crystals as a function of temperature in an atmosphere containing water vapor at p (H2O ) = 4.02 × 10 −3 atm. In this plot, the activation energy for condensation was assumed to be Q = 10 kJ mole , which is much too large to give the generally accepted value for the condensation coefficient of α = 0.7 (International Union of Pure and Applied Chemistry 2009) but was used anyway to emphasize the concept of the growth rate being the product of both the thermodynamic and kinetic factors. Appendix 141 which is about a factor of 106 smaller than the literature value, suggesting that k really is much larger, k ≅ 2 × 106 cm s . It should be noted that small values of α in the order of α ≅ 6 × 10 −3 have been observed (Magee et al. 2006) and would imply k ≅ 1 cm s However, the goal here is not to accurately calculate the accommodation coefficient or the growth rate for ice but to demonstrate the general feature of growth involving the product of a kinetic factor and a thermodynamic factor. In order to do this, a larger activation energy is assumed. Such growth behavior as a function of temperature is typical of solids or liquids from the vapor or solids from liquids or solids from other solids. Growth of a second or new phase will be examined further when the topic of nucleation and growth is discussed. 5.10 SUMMARY In order to illustrate heterogeneous reactions, gas–solid reactions are chosen because of their importance in materials science and engineering. To understand the parameter dependence of these reactions, some gas kinetics and the interaction between gas atoms/molecules and a solid surface are described. The Langmuir isotherm is developed for the adsorption of gases onto solid (or liquid) surfaces. The importance of gas solid reactions in many industrial materials processes and applications is discussed. One area of particular importance in industrial practice is the process of CVD. The CVD process is contrasted with PVD and the important thin film deposition process of sputtering is described. The technologically important process of CVD of silicon is shown in detail with results that are close to those used in actual practice. The importance and analysis of active gas corrosion is also discussed. The example of halogen bulbs in which CVD and active gas corrosion occur simultaneously at different temperatures to enhance the lifetime and operating temperature of such lamps is presented. Some discussion about carbon–carbon composites and their fabrication is offered as another example of a gas–solid deposition process, chemical vapor infiltration, CVI. Finally, growth of a solid or a liquid from a gas depends on the product of a thermodynamic and a kinetic factor that typically lead to some maximum in the growth rate at some temperature (or other variable) below equilibrium conditions. These concepts reappear when discussing the process of phase transformations in Chapter 7. APPENDIX a.1 TranSforminG from carTeSian To polar coordinaTeS It is often useful to transform from Cartesian or x and y coordinates to polar coordinates, r and θ. For polar coordinates, this can be done by inspection, as indicated in Figure A.1. However, a general technique to transform from one set of coordinates to another is valuable. This is particularly true for situations where the transformation is not so obvious, such as spherical or other three-dimensional coordinates. To transfer from an area element, dA, in Cartesian coordinates to polar coordinates, the formal mathematical method is θ rd ∂ ( x, y ) dA = dxdy = drdθ ∂ ( r,θ ) dA′ = 2πrdr y (A.1) dr dθ dA r θ where x ∂x ∂ ( x, y ) ∂r = ∂ ( r,θ ) ∂y ∂r ∂x ∂θ =J ∂y ∂θ (A.2) FIGURE A.1 Polar coordinates (r, θ) showing two differential area elements dA = rdrdθ and the theta- integrated area of dA′ = 2πrdr. 142 Chapter 5. Heterogeneous Reactions where: J is the Jacobian matrix J is the absolute value of the Jacobian (Kreyszig 2011). For polar coordinates, x = r cos θ, y = r sin θ, and Equation A.2 becomes, ∂x ∂r ∂y ∂r ∂x ∂θ cos θ = ∂y sin θ ∂θ − r sin θ = r(cos2 θ + sin 2 θ) = r r cos θ so, in polar coordinates, dA becomes dA = rdrdθ. (A.3) Since θ is independent of r, the differential area element dA can be changed to dA′ by integrating θ over the range of interest, 0 to 2π, 2π dA′ = ∫ 2π ∫ rdrdθ = rdr dθ =2πrdr 0 0 which is now a circular ring of thickness dr and circumference 2πr as shown in Figure A.1 a.2 inTeGraTion of ∫−∞ e− x dx ∞ 2 2 +∞ − x Now ∫−∞ e dx is a definite integral and is just some number, call it I. Then I2 can be written as (this is the crucial step in the process) +∞ 2 +∞ ∞ ∞ − x2 + y2 2 I 2 = e− x dx e− y dx = e dxdy −∞ −∞ −∞ −∞ ∫ ∫ ∫∫ (A.4) where the last step is valid since x and y are independent dummy variables and the integration is over all space, −∞ ≤ x ≤ ∞ and −∞ ≤ y ≤∞. It is much more convenient to change to polar coordinates so that x2 + y2 = r2 and dA = dxdy = rdrdθ as shown in Figure A.1, and integrate over all space from 0 ≤ r ≤ ∞ and 0 ≤ θ ≤ 2π. ∞ ∞ I = 2 ∫∫ e ( − x2 + y2 )dxdy −∞ −∞ ∞ 2π I2 = ∫∫ ∞ ∫ 2 2 re − r dθdr = 2π re − r dr 0 0 0 ∞ 1 2 I 2 = 2π − e − r 2 0 1 I 2 = 2π − ( 0 − 1) = π. 2 Therefore, taking the square root, +∞ I= ∫ e−x dx = 2 −∞ ∞ 2 2 π. (A.5) In several situations, ∫ 0 e − x dx, is used. Now, e − x is a symmetrical or even function about the origin— 2 ∞ − x2 f(−x) = f(x)—as shown in Figure 5.3. And for an even function (Kreyszig 2011), ∫ −∞ e dx = 2∫ 0∞ e − x dx. Appendix This is easily shown to be the case since, ∞ ∫e ∞ 0 − x2 ∫e dx = −∞ − x2 ∫ 2 dx + e − x dx. −∞ (A.6) 0 In the first integral, make the substitution, y = −x so 0 ∫ ∞ 0 ∫ 2 ∞ ∫ 2 ∫ 2 2 e − x dx = − e − y dy = e − y dy = e − x dx. −∞ ∞ 0 0 since exchanging the limits of integration changes the sign (Edwards and Penney 2002) and x and y are dummy variables. Therefore, Equation A.6 becomes ∞ ∫ −∞ ∞ 2 ∞ ∫ ∫ 2 ∞ ∫ 2 2 e − x dx = e− x dx + e − x dx = 2 e − x dx 0 0 0 so ∞ ∫e − x2 dx = 0 a.3 π . 2 (A.7) cHanGinG coordinaTeS for SpHerical coordinaTeS Figure A.2 shows the volume element in spherical coordinates, dV = r 2 sin θ dr dθ dϕ (A.8) as can be seen graphically from the figure. However, again it can be obtained from the Jacobian for the spherical coordinates of Figure A.2 x = r sin θ cos ϕ y = r sin θ sin ϕ (A.9) z = r cos θ. z rd θ dφ r sin θ dr r sinθ θ r dθ y φ dφ x FIGURE A.2 Polar coordinates (r, θ, φ) and differential area, dA = r 2 sinθdθdϕ, and differential volume, dV = r 2 sinθdθdϕdr , elements. 143 144 Chapter 5. Heterogeneous Reactions In this case, the Jacobian is given by ∂x ∂r ∂y J= ∂r ∂z ∂r ∂x ∂θ ∂y ∂θ ∂z ∂θ ∂x ∂ϕ ∂y = r 2 sin θ ∂ϕ ∂z ∂ϕ (A.10) where the details of evaluating this Jacobian to get this result are left to the Exercises at the end of the chapter. So this means that the volume element, dV, transforms as dV = dx dy dz = r 2 sin θdr dθ dϕ (A.11) and since 0 ≤ θ ≤ π and 0 ≤ ϕ ≤ 2π and r, θ, and φ are independent of each other, a new volume element, dV, can be determined by integrating dV with respect to θ and φ π ∫ 2π ∫ dV = r 2dr sin θdθ dϕ 0 ( 0 ) dV = r 2dr − cos θ 0 ( 2π ) π dV = r 2dr ( − [ −1 − 1]) ( 2π ) or dV = 4πr 2dr. (A.12) a.4 exacT reSulT for GaS aTomS collidinG wiTH a Surface Figure 5.6 shows an approximate way to calculate the approximate number of gas atoms or molecules hitting a surface, per unit area, per second: Z= z θ v v cosθ y φ x FIGURE A.3 Column of gas atoms of speed v striking a surface at some angle θ. 1 η v. 6 This is only an approximation since this assumes that the atoms are only traveling in the three mutually perpendicular directions. The reality is the gas atoms can strike the area A from any direction. When this is taken into consideration, a slightly different value of Z is obtained. A more accurate calculation begins with a gas column again of length, v, but inclined from the vertical by an angle θ as shown in Figure A.3 (McQuarrie and Simon 1997). The volume of the column is still the height—in this case, v cos θ, even though its slant length is now v—times the area Vcolumn = A v cos θ. (A.13) That the volume of this column is still the height, v cos θ times the area, might not be readily obvious. But think of sliding a deck of cards at an angle, the volume of the deck is still the original height times the area of a card even though the distance along the slanted edge might be considerably longer than the original height. Appendix Now, the fraction of atoms moving along the axis of this tilted cylinder must be taken into account. It is assumed that atoms can be moving in any directions so the probability of them crossing the surface of a sphere is equally probable in any angular direction. So that the fraction of atoms in any direction at angles θ and φ is the small area of the sphere dA = ( r sin θdθ )( rdϕ ) (A.14) as shown in Figure A.2. The total area of the sphere is 4πr2 and therefore the fraction of the atoms moving in the direction of θ and φ is r 2 sin θdθdϕ sin θdθdϕ = . 4πr 2 4π dΩ = (A.15) Therefore, combination of these gives dZ = (number of atoms/vol) (volume of cylinder) (fraction of atoms traveling down the cylinder axis) or sin θdθdϕ dZ = ( η)( v cos θ ) 4π (A.16) and integrating with respect to θ and φ Z= = 2π π/ 2 0 0 1 ηv dφ sin θ cos θdθ 4π ∫ ∫ π/2 1 1 ηv ( 2π ) sin 2 θ 0 4π 2 with the final result Z= a.5 1 ηv. 4 (A.17) mean VerTical diSTance TraVeled Later, there will be a requirement to calculate the mean vertical distance an atom travels, z. The vertical distance an atom at an angle θ travels is simply v cos θ and is independent of φ. So if Equation A.16 is integrated with respect to φ only, then dZ(θ) is obtained which is the fraction of atoms coming from an angle θ. So dZ ( θ ) = 1 nv sin θ cos θdθ 2 and the mean vertical distance traveled is π/ 2 z= ∫ ( v cos θ) dZ ( θ) 0 Z (A.18) 145 146 Chapter 5. Heterogeneous Reactions which becomes on making the substitutions and integrating, π/ 2 z= ∫ ( v cos θ) dZ ( θ) 0 Z (1 2 ) nv 2 z= (1 4 ) nv π/ 2 ∫ cos θ sin θdθ 2 0 π/ 2 2 1 z = 2v − cos3 θ = − v ( 0 − 1) 0 3 3 to give the mean distance as z= 2 v. 3 (A.19) EXERCISES 5.1 Calculate the root-mean-square speed, the mean speed, and the most probable speed (the maximum in the Maxwell–Boltzmann distribution) for hydrogen molecules at 1000°C. 5.2 a. Calculate the number of hydrogen molecules/cm3 at 1000°C and 1 atm pressure. b. Calculate the approximate hydrogen impingement rate (molecules/cm 2-s) from I = (1/ 6)ηv rms under the same conditions as in a. c. Calculate the exact impingement rate (molecules/cm2-s) under the same conditions from I = p / 2πmk BT . 5.3 The number of atoms or molecules in a gas at a gas pressure p that attach themselves to a surface (or are evaporated or sublimed from), or any surface, is given by J′ = Zα where Units(J′) = atoms/cm2-s and α = sticking coefficient, which goes from zero to one depending on the surface reaction necessary for the atoms to stick. If there is no surface reaction, then α = 1.0 and J′ is J′ = Z = p 2πmk BT a. If J is the molar flux, mol/cm2-s show that: J = 10 −4 p / 2πMRT where Units(p) = Pa and Units(M) = kg/mol. b. From a. derive an expression for the rate of sublimation, dr/dt, (cm/s) of a graphite wire lamp filament (a long cylinder) at elevated temperatures where r is the wire radius. c. Calculate how long it would take (years) at 1800°C to completely sublime a graphite lamp filament 3 mils in diameter if the Gibbs energy for the reaction: C(s) = C(g) is ∆Go = 716,292 – 157 T(K) J/mol (Roine 2002) and the density of the graphite is ρ = 2.5 g/ cm3 and the molecular weight is M = 12.011 g/mol. 5.4 Given the following thermodynamic data at 1227°C (Roine 2002), calculate the water vapor partial pressure in a flowing hydrogen gas of 1 atm below which active gas corrosion of silicon occurs; that is, SiO(g) forms and SiO2(s) does not. Active corrosion: Si(s) + 1/2 O2(g) ⇒ SiO(g) Passive corrosion: Si(s) + O2(g) ⇒ SiO2(s) Exercises Compound SiO(g) SiO2(s) H2O(g) Gibbs Energy, ∆Go (J/mol) −227,501 −643,026 −164,419 5.5 a. Thin films of titanium nitride, TiN, (the gold coating seen on drill bits and other tools are either TiN or ZrN for wear resistance) can be deposited by CVD at 1000 K by the following reaction: 2TiCl4(g) + N2(g) + 4H2(g) = 2TiN(s) + 8HCl(g) With the following thermodynamic data (Roine 2002), calculate the equilibrium constant at 1000 K. ∆Go (J/mol) −642,872 −242,969 −100,805 Compound TiCl4(g) TiN(s) HCl(g) b. Calculate the equilibrium partial pressure of TiCl4 if the initial TiCl4 pressure is 0.01 atm and the pressure of N2 and H2 are held constant at 0.5 atm each. c. The reaction for the CVD of TiN (mol/cm2-s) is given by ( J TiCl4 = − k [ TiCl 4 ]0 − [ TiCl 4 ]e ) where the subscript 0 indicates the concentration (mol/cm3) in the gas and the subscript e indicates the equilibrium concentration. Derive a general expression for the rate of deposition (cm/s) for TiN in terms of the TiCl4 pressures in atmospheres. d. Calculate the reaction rate constant at 1000 K if k = k0 exp(–Q/RT) with k0 = 5.49 × 104 cm/s and Q = +120 kJ/mol. e. If the density and molecular weight of TiN are 5.22 g/cm3 and 61.89 g/mol, respectively, calculate how long (hr) it takes to deposit a layer of TiN 1 μm thick at 1000 K. 5.6 The following thermodynamic data at 1027°C are taken from an old database (Note units!). Compound FeCl2(g) HCl(g) ∆Go (cal/mol) −46,596 −24,534 a. Iron is undergoing active gas corrosion in an inert atmosphere containing 0.1 atm HCl by the following reaction: Fe(s) + 2 HCl(g) = FeCl2(g) + H2(g) Calculate the equilibrium constant at this temperature. b. Calculate the exact equilibrium pressures (atm) at 1027°C of all of the gas species. Assume that all of the hydrogen is generated by the reaction. c. If the first-order reaction rate constant for the active gas corrosion of iron by hydrogen chloride gas is given by k = k0exp(−Q/RT) with k0 = 0.1 cm/s and Q = 20 kJ/mol, calculate the value of the reaction rate constant at 1027°C. 147 148 Chapter 5. Heterogeneous Reactions d. Assuming the following first-order reaction for HCl with iron and a flowing gas atmosphere, derive an expression for the thickness of the iron reacted as a function of time in terms of the HCl pressures. ( J HCl = − k [ HCl ]0 − [ HCl ]e ) In the above, Units(J) = mols/cm2-s, 0 refers to the HCl concentration (mol/cm3) in the gas stream and e refers to the equilibrium concentration. e. If the density and atomic weight of iron are 7.86 g/cm3 and 55.85 g/g-atom respectively, calculate the rate of active gas corrosion (cm/s) at 1027°C under these conditions. f. Calculate the depth of corrosion (mils) of the iron in 1 day under these conditions. 5.7 A tungsten filament is reacting in a halogen lamp with the Cl2 in the lamp. There are several gaseous chlorides of tungsten produced, WCl2, WCl4, and WCl6. For this problem, it will be assumed that only WCl2 is produced. The following data are available: Melting point of W: Tmp = 3410°C Density of W: ρ(W) = 19.35 g/cm3 Molecular weight: M(W) = 183.85 g/mol Filament length: 40 in. Filament diameter: 3 mil (note: 1 mil = 0.001 in.) ∆G° (WCl2, 2500 K): −142,787 J/mol ∆G° (WCl2, 3000 K): −167,328 J/mol Bulb volume: 1 cm3 Initial Cl2 pressure: 10−2 atm and the reaction to consider is W(s) + Cl2(g) = WCl2(g) a. Calculate the exact pressures of Cl2 and WCl2 at equilibrium at both 2500 and 3000 K assuming that the Cl2 does not decompose. b. If the first-order reaction rate constant for active gas corrosion of tungsten by chlorine is given by k = k0exp(−Q/RT) with k0 = 0.1 cm/s and Q = 20 kJ/mol, where J = −k{[Cl2] – [Cl2]e}, calculate the values of the reaction rate constant at both 2500 and 3000 K. c. Calculate how long it takes for bulb to reach 99% of equilibrium if the temperature of the tungsten filament is rapidly raised from 2500 to 3000 K. Assume that the gas in the bulb is at a uniform temperature and that the cold SiO2 glass bulb wall has no effect. (This is not a good assumption. However, this is a model and any assumptions are acceptable. Whether they fit reality or not, is something that has to be examined.) Use the p(Cl2) at 2500 K and neglect any change in total pressure with T. d. Calculate the initial rate of deposition of W in units of in/s if the filament in part c. is suddenly heated to 3000 K. Assume that the reaction rate constant for the deposition of tungsten by chemical vapor deposition from WCl2 is the same as for the active gas corrosion of tungsten by chlorine. Neglect any change in total pressure on heating. 5.8 Show that the Jacobian for spherical coordinates, Equation A.10, is indeed equal to r 2 sin θ. REFERENCES Adamson, A. W. 1982. Physical Chemistry of Surfaces, 4th ed. New York: John Wiley & Sons. Ashby, M. F. and D. R. H. Jones. 1980. Engineering Materials: An Introduction to Their Properties and Applications. Oxford: Pergamon Press. Buckley, J. D. and D. D. Edie, eds. 1992. Carbon-Carbon Materials and Composites. NASA Reference Publication 1254. Washington, DC: National Aeronautics and Space Administration. References Campbell, S. A. 1996. The Science and Engineering of Microelectronic Fabrication. Oxford: Oxford University Press. Chase, M. W., Jr. et. al. 1985. JANAF Thermochemical Tables, Third Edition. J. of Physical and Chemical Reference Data. 14. Supplement No. 1. Columbia Accident Investigation Board. 2003. Columbia Accident Investigation Board, Report Volume 1. Washington, DC: National Aeronautics and Space Administration. Edwards, C. H. and D. E. Penney. 2002. Calculus, 6th ed. Englewood Cliffs, NJ: Prentice Hall. Halogen Lamp. Wikipedia Encyclopedia. http://en.wikipedia.org/wiki/Halogen_lamp. Haynes, W. M., editor-in-chief. 2013. Handbook of Chemistry and Physics, 94th ed. Boca Raton, FL: CRC Press. Hudson, J. B. 1998. Surface Science. New York: John Wiley & Sons. International Union of Pure and Applied Chemistry. 2009. IUPAC Task Group on Atmospheric Chemical Kinetic Data Evaluation-Data Sheet V.A1.6.HI6. http://iupac.pole-ether.fr/htdocs/datasheets/pdf/ H2O+ice_V.A1.6.pdf. Kreyszig, E. 2011. Advanced Engineering Mathematics, 10th ed. New York: John Wiley & Sons. Magee, N., A. M. Moyle, and D. Lamb. 2006. Experimental determination of the deposition coefficient of small cirrus-like ice crystals near −50°C. Geophys. Res. Lett. 33: L178l13. Matthews, F. L. and R. D. Rawlings. 1994. Composite Materials: Engineering and Science. London: Chapman and Hall. McQuarrie, D. A. and J. D. Simon. 1997. Physical Chemistry. Sausalito, CA: University Science Books. Moore, W. J. 1955. Physical Chemistry, 2nd ed. Englewood Cliffs, NJ: Prentice Hall. NIST Chemistry Webbook. http://webbook.nist.gov. Optical Fiber. Wikipedia Encyclopedia. http://en.wikipedia.org/wiki/Fiber-optic. Pierson, H. O. 1999. Handbook of Chemical Vapor Deposition, 2nd ed. Norwich, NY: Noyes Publications. Pound, G. M. 1972. Selected Values of Evaporation and Condensation Coefficients for Simple Substances. J. Phys. Chem. Ref. Data. 1(1): 135–146. Ring, T. A. 1996. Fundamentals of Ceramic Powder Processing and Synthesis. San Diego, CA: Academic Press. Roine, A. 2002. Outokumpu HSC Chemistry for Windows, Ver. 5.11, thermodynamic software program, Outokumpu Research Oy, Pori, Finland. Savage, G. 1993. Carbon-Carbon Composites. London: Chapman and Hall. Silbey, R. L. and R. A. Alberty. 2001. Physical Chemistry, 3rd ed. New York: John Wiley & Sons. Wolf, S. and R. N. Tauber. 2000. Silicon Processing for the VLSI Era, Volume 1-Process Technology, 2nd ed. Sunset Beach, CA: Lattice Press. 149 Section III Phase Transformations Chapter 6 Thermodynamics of Surfaces and Interfaces and Some Consequences 153 Chapter 7 Phase Transitions 195 151 6 Thermodynamics of Surfaces and Interfaces and Some Consequences 6.1 6.2 6.3 6.4 6.5 Introduction Surface Energy, Tension, and Stress 6.2.1 Surface Energy and Surface Tension 6.2.2 Surface Stress and Surface Tension Surface Tension in Materials 6.3.1 Importance 6.3.2 Values of Surface Tension 6.3.3 Surface Energies and Broken Bonds 6.3.3.1 Example: Copper 6.3.3.2 Example: Polymer 6.3.4 Anisotropy of Surface Tension and the Shape of Crystals 6.3.4.1 Introduction 6.3.4.2 Simple Cubic Crystal 6.3.4.3 A More Complex Crystal Surface Tension and Surface Curvature Curvature and Vapor Pressure 6.5.1 The Model 6.5.1.1 Example: Water Drop at 25°C 153 154 155 155 156 156 156 157 157 157 158 159 159 159 161 162 163 163 164 154 Chapter 6. Thermodynamics of Surfaces and Interfaces and Some Consequences 6.6 6.7 6.8 Curvature and Solubility Ostwald Ripening by Surface Reaction Control Freezing Point Depression of Small Particles 6.8.1 Application of the Clausius–Clapeyron Relation 6.8.1.1 Example: One-nm Water Drops 6.9 Specific Surface Area 6.10 Wetting 6.11 Interfacial Energies and Microstructure 6.12 Interfacial Energies and Surface Shape 6.13 Capillary Rise 6.13.1 The Model 6.13.1.1 Example: Liquid FeO at 1369°C 6.13.2 Mercury Porosimetry 6.13.3 Other Measurement Techniques 6.14 Surface Segregation and Surface Tension 6.14.1 Gibbs Adsorption Isotherm 6.14.1.1 Example: Water with Sodium Dodecylsulfate, C12H25OSO3Na, in Solution 6.14.2 Other Examples 6.14.2.1 Surface Segregation in Other Materials 6.14.2.2 Froth Flotation 6.14.2.3 Coupling Agents 6.15 Wetting of Microporous Surfaces 6.16 Chapter Summary Appendix Exercises References 6.1 165 166 169 169 170 170 171 173 174 175 175 176 176 176 177 177 178 179 179 179 180 181 184 185 189 192 INTRODUCTION The thermodynamics of surfaces and interfaces may seem to be out of place in a book on kinetics because this is a topic that would normally be covered in a book or course on thermodynamics. Yes (DeHoff 2006) and no (Gaskell 2008)! These are two very popular books used in thermodynamics courses in MSE: one covers surface properties and the other does not. Thermodynamics is a broad and difficult subject when encountered for the first time and surface phenomena may or may not be covered in a first thermodynamics course. Nevertheless, in the analysis of most kinetic processes, it is assumed that the thermodynamics of the system are known and usually the starting point for understanding the kinetics. Indeed, the thermodynamics of surfaces plays an important role as the driving force in many materials kinetic processes such as sintering, grain growth, nucleation, particle coarsening, and so on. The role of surface energies is critical in understanding these and other processes. Furthermore, as the size of a particle decreases, its surface-to-volume ratio increases and 6.2 Surface Energy, Tension, and Stress the surface energy has an even greater effect. This is particular true for processes that involve particles on the nanoscale. The thermodynamics and behavior of surfaces covers several phenomena and there are numerous books on surfaces and surface effects that cover virtually all of the topics discussed here, as well as many more (Adamson 1982; Adamson and Gast 1997; Miller and Neogi 1985; Hiemenz 1986; Hudson 1998; Evans and Wennerström 1999, to list but a few). The emphasis in this chapter is on those surface- and interface-related topics of solids and liquids that affect energies, vapor pressures, solubilities, and other properties that impact microstructural development and other kinetic processes important in materials science and engineering. 6.2 6.2.1 SURFACE ENERGY, TENSION, AND STRESS Surface energy and Surface TenSion Free surfaces of condensed phases—solids and liquids—have energies associated with them over and above the internal energy of the bulk material due to unsatisfied bonds at surfaces. Figure 6.1 depicts the situation for broken covalent bonds at the surface of silicon. In reality, this is oversimplified because the atoms or molecules at the surface adjust their positions—and bonding—to generate a lower energy structure—a process known as surface reconstruction. Investigation of such surface reconstructions is an active area of surface science research. Nevertheless, there still is a residual surface energy, γ. From Chapter 1, the differential of the Gibbs energy, dG, including a surface work term, γdA, for a two-component system is dG = SdT − VdP + µ1dn1 + µ 2dn 2 + γdA (6.1) so γ can be represented thermodynamically (macroscopically) as ∂G γ= ∂A T,p,ni (6.2) where G = Gibb’s energy and γ = surface energy (sometimes called the “Gibbs surface energy”). The units of surface energy are Units(γ) = J/m2 or J/cm2. Note that because 1 J = 1 Nm, the units of surface energy are also Units(γ) = N/m, or a force per unit length. As a result, γ is more commonly referred to as the surface tension and appears to be the preferred terminology over surface energy (IUPAC 2014) and is now used in most books describing surface phenomena. However, the terminology causes confusion because there is also a surface stress in solids that is indeed different as discussed below. This multiplicity of terms is best summarized by Adamson in his book on surfaces (Adamson 1982, 6; with similar wording in Adamson 1997, 5): Surface Broken bonds Si Si Si Si Si Si Si Si Si Si Si Si Si Si FIGURE 6.1 Broken or unsatisfied bonds at the surface of a solid or liquid are the source of surface energy, illustrated here with the surface of crystalline silicon. 155 156 Chapter 6. Thermodynamics of Surfaces and Interfaces and Some Consequences …so that the decision as whether surface tension or surface free energy is the more fundamental concept becomes somewhat a matter of individual taste. The two terms generally are used interchangeably in this book. The term surface tension is the earlier of the two; it goes back to early ideas that the surface of a liquid had some kind on contractile “skin.” More subtly, it can convey the erroneous impression that extending a liquid surface somehow stretches the molecules in it. In contrast, the term surface free energy implies only that work is required to form more surface, that is, to bring molecules from the interior of the phase into the surface regions. For this reason, and also because it ties more readily into conventional chemical thermodynamic language, this writer considers the surface free energy concept to be preferable if a choice must be made. Adamson’s point is a good one, because γ appears in Equation 6.1 as a thermodynamic work term, surface energy seems to be the less misleading term.* Here, it is assumed that surface energy and surface tension refer to the same excess energy at surfaces and both terms will be used depending on what is being discussed. For example, treating surface energy as a surface tension—as a force per unit length—permits the simple development of several useful relations between the energies of different surfaces and their microstructural effects more easily than with surface energies and surface areas. 6.2.2 Surface STreSS and Surface TenSion Adamson is not the only one concerned about the use of the term surface tension. Several other authors feel strongly that the term surface tension is confusing because there exists another surface term, surface stress, which is defined differently and can be the most important surface term is solids, particularly at low temperature (Cammarata 1994). Note that surface tension and surface stress are not the same for solids (Cammarata 1997). An actual surface stress, f, exists and can be smaller or larger than γ and occurs when a strain is applied to the bonds between the atoms at the surface of a solid: f = γ + (∂γ /∂ε), where ε is the strain. The rationale for this expression is developed in Appendix A.1. This equation applies to isotropic or highly symmetrical crystalline materials. More generally, surface stress and strain are second-rank tensors. Of course, in liquids, no strain in atomic bonds can exist at the surface because bulk atoms simply move into the surface to relieve the strain, so there really is no surface stress and, therefore, surface tension and surface energy are the same. This is also true for solids if the temperature is high enough so that atoms from the bulk can move into the surface to relieve the surface strain if sufficient time is allowed for diffusion to occur. Because much of the kinetics where surface tension plays a role in solids is at high temperatures, the latter situation is assumed in all further discussions on the effects of surface tension: that is, surface stress will not be considered. Nevertheless, it should be noted that for solids at low temperatures, many of the relations developed between γ and a given property should more appropriately be expressed in terms of f. Unfortunately, it is considerably more difficult to measure f and few experimental values are available, and theoretically calculated values must frequently be used (Cammarata 1994). 6.3 6.3.1 SURFACE TENSION IN MATERIALS imporTance Surface tension plays many important roles in materials science and engineering. One example is very familiar; namely, the formation of certain crystallographic bounding planes on crystals grown from the melt or from solution, such as the amethyst crystals—quartz with iron and water impurities that give the purple color—in Figure 6.2. These crystals slowly FIGURE 6.2 Centimeter-size quartz (amethyst) crystals grown from solution showing low surface energy faces. * As mentioned in Chapter 1, the IUPAC has also thrown out the “free” in free energy and now G is simply the “Gibbs energy” or the “Gibbs function” (IUPAC 2014). 6.3 Surface Tension in Materials grown from solution have crystal faces or facets that are usually those that have the lowest surface energies. In many metal-joining processes involving a liquid phase, there is the requirement for the liquid to wet the solid. These processes include the following: soldering—joining metals with a filler metal alloy that has a melting temperature less than about 450°C (lead-tin alloys are the most common solders); brazing—joining metals with a molten filler metal with a melting temperature above about 450°C (copper alloys are common); and welding—actual melting of the metals to be joined occurs at the joint with or without a filler metal. Surface tension is the driving force for sintering or densification of metal powders—powder metallurgy—as well as ceramic materials and polymers made from powders. Surface tension is also the driving force for coarsening or the growth of particles dispersed in gases, liquids, or solids—the process known as Ostwald ripening named after Wilhelm Ostwald, 1909 Nobel Prize in Chemistry (Laidler 1993; Ratke and Voorhees 2002). In addition, the surface or interfacial tension associated with grain boundaries in polycrystalline materials is responsible for the growth of these grains by diffusion at high temperatures. The relative interfacial energies between solids and liquids can also determine the distribution and shapes of these phases in the microstructures of multiphase materials and how the phases are distributed strongly influences the properties. Finally, surface tension plays a critical role in rates of phase transformations. 6.3.2 ValueS of Surface TenSion Values of surface tension are not always easy to find in the literature and exist in several disparate sources representing numerous scientific disciplines. Table 6.1 gives some values of surface tensions for a variety of solids and liquids gathered from several references. Note that for many solids at their melting points, the surface tensions of the liquids and the solids are similar, which is reasonable because the number of broken or unsatisfied chemical bonds at the surface is not too different between liquid and solid near the melting point. Also, note that surface tensions vary by about an order of magnitude from somewhere around 0.1 J/m 2 for polymers to about 1 J/m2 for high-melting metals and compounds. For back-of-the-envelope calculations, if one had to assume a value for surface tension for a metallic, ionic, or covalently bonded solid or liquid, a value of 500 mJ/m 2 would not be a bad guess: within a factor of 2 in most cases. For materials such as polymers whose surfaces represent unsatisfied van der Waals bonds, values on the order of 50 mJ/m 2 are reasonable. 6.3.3 Surface energieS and Broken BondS Surface energies essentially arise from unsatisfied bonds at the surface of solids and liquids. The details of the surface structure of solids can be complex because the atoms tend to move from their normal lattice sites and reconstruct the surface to minimize the surface tension or surface stress if given the opportunity for atomic movement. However, as shown in Table 6.1, the surface tensions of both solid and liquid copper and SiO2 glass and liquid SiO2 are not too different near the melting point, indicating that the detailed atomic structure at the surface does not have an overwhelming effect on the value of the surface tension, at least for these two materials. 6.3.3.1 Example: Copper The surface energy or surface tension of copper can be approximated by the number of broken bonds at the surface. The density of solid copper is ρ = 8.92 g/cm3 and its atomic weight is M = 63.55 g/mol, so the number of atoms per cm3 in solid copper, η(Cu), is η ( Cu ) = 8.92 ρ NA = × 6.022 × 1023 = 8.45 × 1022 cm −3 . 63.55 M 157 158 Chapter 6. Thermodynamics of Surfaces and Interfaces and Some Consequences TABLE 6.1 Values of Surface Tensions Material H2O Ethanol (C2H5OH) Acetone (CH3CH3CO) n-hexane Polyethylene Poly(ethylene oxide) Polytetrafluoroethylene Hg(l) Pb(l) Cu(s) Cu(l) Cu(l) Ag(s) Ag(l) Fe(l) Pt(l) Si(l) NaCl(100)(s) NaCl(l) NaCl(l) LiF(100)(s) LiF(l) CaF2(111)(s) SiO2(s,glass) SiO2(l) Al2O3(s) Al2O3(l) MgO(s) TiC(s) V2O5(l) B2O3(l) FeO(l) T (oC) 25 25 25 25 20 20 20 25 350 1080 1083 1120 750 961 1536 1769 1410 25 801 1000 25 1050 25 1100 1800 1850 2080 25 1100 1000 900 1420 Melting T (oC) 0 −117.3 −95.4 −95 139 66 330 −38.87 327 1083 “ “ 961 “ 1535 1769 1410 801 “ “ 845 “ 1423 1723 1723 2050 “ 2852 3140 690 450 1369 ɣ (mJ/m2) 72.8 22.3 23.7 18.4 35.7 42.9 23.9 498 468 1430 1285 1270 1140 903 1872 1800 865 300 114 98 340 229 450 295 307 905 700 1000 1190 86 80 585 Source 1, 2, 5 1, 5 1, 5 1, 5 4 4 4 3 3 2 3 2 2 3 3 3 3 2 2 3 2 3 2 6 7 2 2 2 2 3 2 2 Sources: 1. Chang (2000), liquids; 2. Kingery et al. (1976), nonmetals; 3. Brandes and Brook (1992), molten metals and molten salts; 4. Sperling (2006), polymers; 5. Haynes (2013), extensive lists of organic liquids and molten elements; 6. Parikh (1958); 7. Kingery (1959). The number of Cu atoms per square centimeter is roughly η2/3 = 1.93 × 1015 cm−2 or 1.93 × 1019 m−2. The number of broken bonds times about half of the single-bond energy gives a rough estimate of the surface tension. About half of the bond energy is used because fracture in a piece of copper creates two surfaces, in each of which the atoms have about half of the bond energy between copper atoms. For copper, if the bond strength is roughly 1 eV, then γ ≅ 1.93 × 1019 eV/m2 × 1.602 × 10−19 J/eV/2 ≅ 1.55 J/m2, which is probably fortuitously close to the measured values in Table 6.1; certainly close enough for a “back of the envelope” calculation. 6.3.3.2 Example: Polymer On the other hand, for polymers, there are really few broken chemical bonds at surfaces, just van der Waals forces, which have energies on the order of 0.1 eV/bond. Take, for example, polyethylene, (C2H4)n. In this case the density is ρ ≅ 0.9 g/cm3 and the molecular weight for a mer unit is 28 g/unit. Therefore, η ≅ (ρ/M ) N A ≅ (0.9/ 28) × 6.022 × 1023 = 1.93 × 1022 cm −3 . So, the number of 6.3 Surface Tension in Materials mer units at the surface is η2/3 ≅ (1.93 × 1022 ) ≅ 1.81× 1015 cm −2 = 1.81× 1019 m −2. Now if there are roughly four atoms (more than one anyway) in each mer on the surface, the total surface tension is γ ≅ ( 4 × 1.81× 1019 )(0.1)(1.602 × 10 −19 ) / 2 ≅ 58 mJ / m 2 . Here again, the rough, calculated value is again reasonably close to measured values! These two calculations are good demonstrations that the surface tension of solids and liquids—in which any surface strain can be relaxed by atoms moving to the surface—is due to unsatisfied chemical or physical bonds at the surface. 2/3 6.3.4 aniSoTropy of Surface TenSion and The Shape of crySTalS 6.3.4.1 Introduction Surface tensions in crystalline solids are not isotropic and usually vary with different crystal faces or planes. However, in many of the discussions that follow, to simplify things, the assumption is that the surface tension for both liquids and solids is isotropic. This assumption does not invalidate any of the basic results obtained. However, in real systems, surface tension anisotropy may introduce unwanted complexities in both measuring and interpreting surface effects. In the following few paragraphs, some simple—and rather old—ideas concerning surface tension anisotropy are presented mainly to demonstrate how anisotropy can affect the shapes of small crystals. What follows is entirely a thermodynamic approach that determines the shapes of crystals, particularly small ones in which the distance between the faces is sufficiently small to ensure that material transport processes are fast enough to move material around the crystal surfaces to ensure that all the faces are in chemical equilibrium. For larger crystals, the faces or facets that are observed may or may not be related to thermodynamics but could also be determined by the different growth rates—from gases, liquids, or solids—of different crystal faces. 6.3.4.2 Simple Cubic Crystal In Figure 5.13 of Chapter 5, the classical picture of the structure of the surface of a crystalline solid was schematically represented by the stacking of small cubes representing atoms that leads to steps, terraces, and kinks on the surface of a solid. Figure 6.3 again schematically shows the Area of single atom = d2 Single atom, unit cell (a) θ L H B (b) A FIGURE 6.3 (a) Simple cubic crystal showing all {100} surfaces. (b) Stacking of simple cubic planes to give a different surface at an angle θ with the horizontal used to develop a Wulff construction of surface energy versus angle. 159 160 Chapter 6. Thermodynamics of Surfaces and Interfaces and Some Consequences simple cubic packing of atoms with cubes representing the atoms of the solid. Only in this case, this representation is used to calculate the anisotropy of the surface tension. The surfaces of the simple cubic* crystal at the top of the figure have a number of broken bonds that determine their surface energies. Now if a new surface is constructed with these simple cubic crystal sheets stacked so that the terrace length is four unit cells and the ledge height is one unit cell, then this stacking represents a new surface at an angle θ relative to the (001) flat plane of the crystal, as shown in Figure 6.3. The angle θ is determined by tan θ = (ledge atoms /terrace atoms) = 1/ 4 = 14.04°. From the triangle, tan θ = (H/B) or H = B tan θ and B = L cos θ or L = B/ cos θ. The area of the plane defined by L and A is Area LA = LA = BA / cosθ. If Ω is the number of broken bonds on this area, then Ω= BA + HA BA + BA tan θ = d2 d2 Ω= BA (1 + tan θ ) d2 and if the energy per broken bond is ε, then the surface energy of the new surface at an angle θ is γ=ε γ= BA d 2 (1 + tan θ ) Ω =ε Area LA BA cos θ ε ( cos θ + sin θ ) d2 If γ(100) = ε /d 2, then γ ( θ ) = γ (100 ) ( cos θ + sin θ ) . This is plotted in Figure 6.4 and is known as the Wulff construction or Wulff plot (Wulff 1901). The length of a line from the center of the plot of γ(θ) to a plane tangent to γ(θ) is proportional to the surface energy of that plane. This was proposed in the original—very Tangents to γ plot long—paper by Wulff without proof. It has since been proven and the proof Z is readily available (DeHoff 2006). However, the proof is rather tedious and γ (θ) if the use of the Wulff construction was good enough for Wulff, it will be used here as well without proof. A small crystal assumes a shape giving it θ the lowest total surface energy. That is, the shape of the crystal in the Wulff γ (001) plot is the inner envelope of the tangents that intersect and are perpendicular to the four cusps in the plot. For the simple cubic crystal in Figure 6.4, X γ (100) Inner the inner envelope is the dashed square indicating that a small two-dimenenvelope sional crystal will form a square, whereas a three-dimensional crystal will of tangents form a cube because the Wulff plot will be the same in each coordinate plane: xy, xz, and yz. Therefore, the use of γ(100) is justified in the drawing rather than using just the two-dimensional version, γ(01). FIGURE 6.4 Wulff construction of surface energy versus angle for stacking of simple cubic planes to give surfaces with different surface energies as a function of angle (see Figure 6.3). The surface energy is plotted as the distance from the center of the plot; tangents are drawn to at each point; the inner envelop of tangents (dotted square) gives the crystal shape. * It should be noted that a simple cubic crystal does not require only one atom per cell. Perovskite crystals such as barium titanate, BaTiO3, are simple cubic but have only one formula unit (BaTiO3) per unit cell. 6.3 Surface Tension in Materials 6.3.4.3 A More Complex Crystal In Figure 6.5, Wulff plots are constructed with two values of the surface energy, γ(01) and γ(11). Two-dimensional crystals are considered first because they are easier to visualize and certainly easier to draw without any loss in generality. Figure 6.5a shows a 1 cm 2 area (in the plane of the page) small square crystal with γ(01) = 500 mJ/m2 (along the edges) and a total surface energy of 0.2 mJ.* Figure 6.5b shows a similar construction with γ(11) = 400 mJ/m2. In this case, a 1 cm 2 crystal has a total surface energy of 0.16 mJ. Putting Figure 6.5a and b together into Figure 6.5c gives a schematic plot of γ(θ), the Wulff construction, which shows that the cusps in γ(θ) on the {01} and {11} families of surfaces have the lowest values of γ and form the inner envelope of the tangents that generates the shaded area, the shape of the crystal. A 1 cm2 version of this crystal with the length of its faces drawn to scale is shown in Figure 6.5d and gives a total surface energy from the edges of 0.1579 mJ demonstrating that this crystal with the two different crystallographic faces does indeed give the lowest surface energy. Figure 6.5e shows a sketch of what the three-dimensional crystal would look like and, interestingly, Figure 6.5f shows some small crystals of NiO that have been equilibrated in an HCl atmosphere via vapor transport of NiCl2(g): NiO(s) + 2HCl(g) NiCl 2 (g) + H 2O(g) Surface (01) γ (11) = 400 mJ/m2 Total surface energy = 0.16 mJ 1 cm cm Total surface energy = 0.2 mJ 1 1 cm γ (11) (01) = 500 mJ/m2 1 cm (a) (b) γ (θ) γ (01) γ (01) γ (11) γ (11) 0.165 cm Total surface energy = 0.1579 mJ 0. 78 05 cm Inner envelope (c) (d) 5 μm (e) (f ) FIGURE 6.5 Cubic crystal with two surface energies that influence the shape: (a) γ(01) and (b) γ(11) in two dimensions; (c) the Wulff construction; (d) the two-dimensional crystal shape; (e) the three-dimensional crystal shape; and (f) NiO crystals showing similar shapes. (Photomicrograph courtesy of Steve Landin, CoorsTek, unpublished research, Colorado School of Mines, 1997.) * Note that the surface energy of the crystal face in the plane of the drawing is not being considered in this two-dimensional construction. This does not change the principles involved in the construction. The 0.2 mJ comes from summing γ(01) −3 2 2 4 2 2 around the four edges. Total = 4 × 500 × 10 J m × m 10 cm = 0.2 mJ cm or 0.2 mJ for the 1 cm2 crystal. 161 162 Chapter 6. Thermodynamics of Surfaces and Interfaces and Some Consequences (with permission of Steven Landin, CoorsTek, unpublished research). These crystals clearly show a surface shape similar to the theoretical one in Figure 6.5e. However, combinations of other planes such as the {111} family could give a similar shape. Without knowing the crystallographic orientation of a crystal relative to its faces, or the angles between the faces, whether they are actually {100} and {110} planes cannot be confirmed. Nevertheless, these crystals do show that the surface energy of NiO is anisotropic at the temperatures where these crystals were equilibrated, about 1100°C. 6.4 SURFACE TENSION AND SURFACE CURVATURE In many cases, the combination of surface curvature and surface tension provides the driving force—Gibbs energy difference—for microstructural changes. For example, Figure 6.6 shows a particle or drop that is sectioned through its center. If the surface tension is a force per unit length, then it produces a total downward force, F−z, around the perimeter of the cut equal to F− z = 2πrγ (6.3) The drop is not coming apart, so there must be an equal opposing force in the F+z direction ( ) F+ z = A∆P = πr 2 ∆P (6.4) where: A is the cross-sectional area of the drop ΔP is an internal pressure minus the ambient pressure external to the drop. Equating these two, the important result is obtained: ∆P = Z A r A γ (a) (b) Δp FIGURE 6.6 (a) A spherical particle or drop sliced through its center. (b) The necessary force balance that exists within the particle between an internal pressure, Δp, and the surface tension, γ, acting at the surface. r2 r3 r1 FIGURE 6.7 A more general solid shape that has more than one radius of curvature at each point: three (r1, r2, and r3) are shown. 2γ . r (6.5) This equation shows that there is an internal pressure—compression in this case—in the particle or drop produced by the surface tension and the radius. For example, if a particle of Al2O3 had a radius of 0.1 μm = 10−7 m at 1850°C with a surface tension of 900 mJ/m2, the pressure inside the particle would be ΔP ≅ 2 × 900 × 10−3 J/m2/10−7 m ≅ 180 × 105 N/m2 = 180 × 105 Pa ≅ 180 atm = 14.7 psi × 180 ≅ 2650 psi! This is a significant stress that can drive atom motion and shape change and is the driving force for many kinetic processes in materials. The important point is that by using surface tension as a force per unit length the influences of that surface tension can be expressed in terms of pressures and stresses that lead to shape and microstructural changes. Not all surfaces of interest are perfect spheres, however. There are more general shapes as shown in Figure 6.7 for which several radii of curvature can be defined. At the inner surface of the toroid in Figure 6.7 two radii of curvature exist: r1, which is the radius of the circular cross section, and r2, which is the radius from the center to the inner surface of the toroid. Similarly, at the outer surface of the toroid, the two radii are r1 and r3. The inverse of a radius of curvature to a surface is called the curvature, κ =1/r. Now, at every point on a surface, two mutually perpendicular radii of curvature, r1 and r2, or curvatures, κ1 and κ2, can be constructed so that one of the curvatures is the smallest and the other is the largest that can 6.5 r2 Curvature and Vapor Pressure r1 90° r1 (a) r1 r2 = ∞ (b) r2 r1 (c) FIGURE 6.8 (a) General curved surface showing principal radii of curvature, r1 and r2 in mutually perpendicular planes that are both perpendicular to the surface where they intersect. (b) Radii of curvature for a right circular cylinder. (c) Radii of curvature for a concave circular cylinder, right: r2 is the outer radius of curvature and is constant while r1 is the inner radius of curvature and varies along the height of the cylinder since it must remain perpendicular to r1 at a given point. be constructed at that point (Figure 6.8a). These are called the principal curvatures and a more general form of Equation 6.5 for ΔP becomes 1 1 ∆P = γ + = γ ( κ1 + κ2 ) = γ 2H r1 r2 (6.6) where H is called the mean curvature and H = (1/2)(κ1 + κ2) (Casey 1996; Green 2005; DeHoff 2006). Of course, for a sphere r1 = r2 = r. Two other examples are given in Figure 6.8. In the case of the right circular cylinder in Figure 6.8b, r2 = ∞ because the side of the cylinder is straight, so ΔP = γ/r1. This would be the situation inside of a round wire. Where the surface of the cylinder is concave (Figure 6.7c), the radius of curvature r2 is actually negative because the end of the radius arrow lies outside of the solid, so at the middle of the cylinder where one of radii as shown is r1 1 1 ∆P = γ − . r1 r2 (6.7) Also note that r1—because it has to be drawn perpendicular to the surface—will vary along the height of this convex cylinder constant, as shown by the two different r1 radii in contrast to the right circular cylinder, where r1 is constant. Such a geometry is important in modeling shape changes because it suggests that if the magnitude of r2 is less than that of r1, then there will be a negative pressure—a tension—at the surface trying to pull the surface out from the center of the cylinder. 6.5 CURVATURE AND VAPOR PRESSURE 6.5.1 The model Because the surface tension or energy generates an internal pressure in a particle or a small drop, its Gibbs energy will be different from that of a completely flat surface; that is, one where r = ∞. The chemical potential, μ, or the partial molar Gibbs energy, G, is given by dG = dµ = VdP − SdT (6.8) 163 164 Chapter 6. Thermodynamics of Surfaces and Interfaces and Some Consequences where V and S are the partial molar volume and entropy, respectively. At a constant temperature, dT = 0 and dG = VdP and can be integrated ∫ Gr Go dG = V ∫ Pr (6.9) dP. P∞ Here Go is the Gibbs energy of a flat surface where the ambient pressure is P∞ and the radius of curvature is infinity and G r is the free energy for a particle of radius r with an internal pressure Pr. This gives G r − G° = V ( Pr − P∞ ) = V 2γ . r (6.10) That is, the free energy of a particle or drop or radius r is greater than that of a flat surface. If the equilibrium vapor pressure of the material in the particle or drop—say water—over a flat surface is po (note: lower case p is being used here simply to distinguish vapor pressure from the applied pressure P), then, by definition of the thermodynamic activity a, p G r − G o = RT ln a = RT ln o p (6.11) where p is now the vapor pressure under an applied pressure P. Combining these last two equations gives the effect of surface tension, γ, and particle size, r, on the vapor pressure compared with the equilibrium vapor pressure over a flat surface: V p 2γ = RT ln o r p or 2γV p = poe rRT (6.12) this means that the vapor pressure over a particle of radius r is higher than that over a flat surface (note: sometimes 2γV RT = d p is referred to as the capillary length [Green 2005]). Furthermore, the smaller the particle size, r, or the larger the surface tension, γ, the greater the increase in vapor pressure. 6.5.1.1 Example: Water Drop at 25°C As an example, consider a drop of water that has a radius of say r = 0.1 μm at 25°C. The equilibrium vapor pressure of water at 25°C is (Haynes 2013) po = 23.8 mm Hg. Because 1 atm = 760 mm Hg, the equilibrium vapor pressure—100% humidity—is 23.8/760 = 3.13 × 10−2 atm × 1.013 × 105 Pa/ atm = 3.17 × 103 Pa. The molar volume of water is V = M(H 2O) / ρ(H 2O) = 18 (g/mol)/(1 g/cm3) = 18 cm3/mol = 18 × 10−6 m3/mol and from the Table 6.1, γ(H2O) = 72.8 × 10−3 J/m2. Let the exponent in Equation 6.12 be x, so ( ( )( −3 2 −6 3 2γV 2 72.8 × 10 J m 18 × 10 m mol = x= rRT 1× 10 −7 m ( 8.314 J mol ⋅ K )( 298K ) x = 1.05 × 10 −2 ) ) 6.6 Curvature and Solubility This is pretty small. Because e x = 1 + (x /1!) + (x 2 / 2!) + , for x small, e x ≅ 1 + x so that p ≅ 1.01 po or that the vapor pressure is only increased by 1%! This may seem small, but it is large enough to lead to significant changes of water vapor particle size distributions—a fog—with time.* 6.6 B B B B B B B Alpha CURVATURE AND SOLUBILITY FIGURE 6.9 Schematic showing isolated particles Figure 6.9 shows particles of B distributed in a continuous solution, α. of B in a continuous matrix of solution alpha. Alpha could either be a liquid or a solid solution. The question is: “How does curvature and surface tension affect the solubility of B in alpha?” Assume that alpha is a solid solution and the particles of B are solid as well. They do not have to be: the same argument would hold if they were liquids. The phase diagram sketched at the bottom of Figure 6.10 shows that the equilibrium solubility of B in alpha at some temperature Te is [B∞], where the subscript ∞ is used to indicate that this is the solubility for B over a flat surface—an infinite radius of curvature. The equilibrium between the solution and the solid B can be written as B → Bsolution, ∞ (6.13) with an equilibrium constant [ B∞ ] Ke = (6.14) aB . Gα G, Gibbs energy Gr(B) 2γ V r . G°(B) (a) Liquid α + liquid α T B + liquid Small particle solvus Te α+B A (b) [B∞] [B] x0 B [Br] FIGURE 6.10 (a) Gibbs energy-composition diagram showing the difference in solubility as a function of the particle size. (b) Schematic phase diagram of components A and B showing the solid solubility of B in alpha, XB, at some temperature Te and the effect of particle size on the solubility—the solvus curve, and its relationship to the energy-composition diagram. * x Note that e = e 1.05×10 −2 165 = 1.011 showing that the ex ≅ 1 + x approximation is more than satisfactory for this x. 166 Chapter 6. Thermodynamics of Surfaces and Interfaces and Some Consequences where B∞ = concentration of B in α over a flat surface of B and where aB = the thermodynamic activity of B. If it is pure B, as in Figure 6.10, then aB = 1.0 by definition of the standard state of P = 1 bar and T. This means that ∆G o = −RTe ln K e = −RTe ln [ B∞ ]. (6.15) One way to handle this for curved surfaces is as follows: for a curved surface, in this case spheres, the Gibbs energy of the spherical particle relative to the standard state, Go(B), is given by G B ( pure) = G oB ( pure) + 2γV + RT ln a B ( pure) r G B (sol) = G oB (sol) + RT ln [ Br ] so ∆G = ∆G o − [ Br ] 2γVB + RTe ln r aB = −RTe ln K e − 2γVB + RTe ln [ Br ] r ∆G = −RTe ln [ B∞ ] − 2γVB + RTe ln [ Br ] r where Br is the solubility for a particle of radius r. At equilibrium, ΔG = 0, so 2γVB [ Br ] = [ B∞ ] e rRT e (6.16) Here, VB is the molar volume of B and γ = γαB, or the interfacial energy between B and alpha. Equation 6.16 shows that the solubility of B increases as the particle radius decreases. [Br] and [B ∞] are both plotted on the bottom axis on the phase diagram. Because of the higher solubility of the small particles, the solvus curve is actually shifted to higher solubilities of B. This is just one example of how surface tension can have an effect on a phase diagram. The top part of Figure 6.10 is the Gibbs energy versus composition plot that shows the energy of the alpha phase as a function of composition and the energies of the large particles, Go(B) and the small particles Gr(B). The separation of these points is greatly exaggerated to emphasize the relation between the G versus [B] plot and the phase diagram. The tangents to the G α curve from the two values of G(B) for the large and small particles give the solubilities on the phase diagram as shown by the vertical dashed lines between the two drawings. The top drawing in Figure 6.10 shows the effect of particle size on solubility and solvus curve on the phase diagram. The bottom drawing graphicallys shows why this occurs with the Gibbs energy-composition diagram. Shifts in other phase boundary curves in phase diagrams also occur with small particles for similar reasons. 6.7 OSTWALD RIPENING BY SURFACE REACTION CONTROL Because the solubility of a particle depends on its radius, if there is a distribution of particle sizes of B as shown in Figure 6.9, this is an unstable configuration and the smaller particles will dissolve and the larger particles will grow. As a result, the average particle size will increase with time: particle coarsening or Ostwald ripening. For particles of B to grow, several series steps are required: the smaller ones must dissolve, B must diffuse to the larger particles and then B atoms must attach themselves 6.7 Ostwald Ripening by Surface Reaction Control to the larger particles. The three kinetic steps in series are (1) surface reaction-controlled dissolution of smaller particles; (2) solid-state or liquid diffusion of B; and (3) surface reaction-controlled growth of larger B particles. Diffusion control of the process will be examined later. For now, assume that growth of the larger particles by reaction at their surfaces controls the rate of particle growth, step 3. As shown earlier, the rate of growth—or shrinkage—of the particles can be obtained from the molar flux to—or from—the surface of the particles. With the assumption of spherical particles, where r = particle radius and a first-order reaction with reaction rate constant k (m/s): ( J = k [ B] r − [ B]r ) (6.17) where: r is the mean particle size of the distribution 3 B r is the concentration of B in the solution (mol/cm ) determined by the mean particle size Br is the equilibrium concentration of B (mol/cm3) at the surface of a particle or radius r. Equation 6.17 implies that particles with radii less than r will shrink and those with radii greater than r will grow. This will lead to an increase in the average particle radius, r, with time. All powders, particles, and precipitates show a range of particle size that can be described by some sort of particle size distribution. If the all of the particles are changing size, the distribution and the mean particle size are also changing. That makes modeling particle size changes with time a very difficult problem. This complex problem was solved over half a century ago, and the complicated part was developing the equation for the steady-state particle size distribution (Wagner 1961). Several other solutions with different particle size distributions based on volume constraints have been developed since then (Ratke and Voorhees 2002). The messy mathematical details of developing the appropriate particle size distribution will not be attempted here. Nonetheless, insight into the solution is realized by examining the behavior of a simple two-size distribution: one in which there are some very large particles all of the same radius and also some very small particles, again, all with the same smaller radius. An example of this might be fog particles over a lake where there is only one large particle, the lake with a radius of curvature of infinity. This is not an unreasonable distribution. If a composition, x0, in Figure 6.10 were cooled from the liquid phase, solid B would form when the temperature reached the liquid + B phase boundary. Because these B particles are growing from the liquid, they could be “large” because diffusion in the liquid is rapid. When the eutectic temperature is reached, all of the remaining liquid freezes to a eutectic mixture of alpha + B. If the rate of cooling were fast enough, these eutectic B particles could be much smaller than those formed earlier. As a result, a two-particle size distribution is produced. If this composition were reheated to some temperature below the eutectic temperature, then the small particles would dissolve and B would deposit on the large particles, increasing their size. Because the large B particles are much larger than the smaller particles, essentially then B r ≅ B∞ , so Equation 6.17 becomes ( ) J = k [ B]∞ − [ B]r . (6.18) Working on the left-hand side of the flux equation for the change in radius with time: J= ( ) 3 ρ dr ρ 1 dV ρ 1 d 4 3 πr = = dt M dt M A dt M 4πr 2 (6.19) so, combining Equations 6.18 and 6.19 ( dr Mk = B − B dt ρ ∞ r ) (6.20) 167 168 Chapter 6. Thermodynamics of Surfaces and Interfaces and Some Consequences where: M is the molecular weight of B (g/mol) ρ is the density of B (g/cm3) k is the first-order reaction rate constant (cm/s) [B]r is the concentration of B at the surface of a particle of radius r (mol/cm3) [B]∞ is the concentration of B over a flat surface. Now, M ρ = VB so that the rate of particle growth becomes ( dr = kVB [ B]∞ − [ B]r dt ) 2 γVB dr = VBk B ∞ − B ∞ e rRT dt = −VBk B ∞ 2 γVB ≅ VBk B ∞ 1 − 1 − rRT (6.21) 2γVB rRT and leads to r 2VB2 k [ B∞ ] γ dr =− dt RT (6.22) and is integrated to give r 2 − r02 = − 4VB2 k [ B]∞ γ RT t = −At (6.23) where r0 is the initial particle size at time = 0. This result basically says that the smaller particles will continue to get smaller and finally disappear. Wagner’s (1961) result for his particle size distribution is 2 2 8 VB k [ B]∞ γ r 2 − r02 = t = A′t RT 9 (6.24) where the mean particle size increases with time. The result for a two-size distribution, Equation 6.23, and that for a complex particle size distribution, Equation 6.24, have the same terms with two exceptions: in the complete solution, r2 is r 2 , the mean particle radius squared, and instead of the 4 in Equation 6.23, the more accurate solution in Equation 6.24 has this factor as (8/9)2. The exact solution takes into account a particular particle size distribution produced by the particle coarsening and that the rate of growth of a particle of a given radius depends on the difference between its solubility and that of the average particle size in the distribution, which changes with time. Determination of the particle size distribution produced by the coarsening makes model development much more complex. But notice that all the other parameters and predicted time dependence are exactly the same in Equations 6.23 and 6.24! The main point is that the particle size grows or shrinks roughly as the square root of time and is directly proportional to the thermodynamic solubility (over a flat surface), [B]∞, the interfacial energy, γ, and the reaction rate constant, k. In wet chemistry, Ostwald ripening or coarsening is used to “age” precipitates by waiting a while after precipitation before filtering to a get a larger particle size, making it easier to filter out the solid particles. This was one of the original observations examined by Ostwald. In addition, particle coarsening can occur via transport through the vapor phase because small particles have a higher vapor pressure— or reaction product pressure—than larger particles. For example, studies on the effect of atmospheres 6.8 Freezing Point Depression of Small Particles 20 m (a) (b) FIGURE 6.11 (a) Particle coarsening or Ostwald ripening of Fe2O3 powders in 10% HCl gas at 1200°C: top left, 10 min; top right, 30 min; bottom left, 100 min; bottom right, 300 min. The starting particle size was about 0.1 μm and exceeds 50 μm after 300 min. The flat surfaces are grain boundary fractures. (J. Lee photograph, Lee 1984) (b) Particle coarsening or Ostwald ripening of Al2O3 in pure HCl gas at 1500°C. Time increasing clockwise from 0 to 1084 min. (Photomicrograph by Marc Ritland, unpublished research, Colorado School of Mines, 1998.) on sintering have shown that Ostwald ripening occurs when the product gas pressures over solids are enhanced in a reactive atmosphere. Figure 6.11a shows this for iron oxide in HCl (Lee 1984) Fe2O3(s) + 6 HCl(g) = 2 FeCl3(g) + 3 H2O(g) whereas Figure 6.11b shows the same for Al2O3 (Marc Ritland, unpublished research) Al2O3(s) + 6 HCl(g) = 2 AlCl3(g) + 3 H2O(g). It is the equilibrium metal chloride pressures—FeCl3 and AlCl3—for these two materials that are enhanced by the curvature: a higher pressure over small particles compared with that over large particles. Note, particularly for the largest particle size, there are crystal faces or facets on the surfaces of the aluminum oxide grains, but the iron oxide grains are uniformly rounded except at the fracture surfaces, where particles were bonded together—grain boundaries. This shows that the surface tension of Al2O3 is still quite anisotropic at 1500°C, whereas that of Fe2O3 is isotropic at 1200°C. The anisotropy in surface tension would be expected to decrease with temperature simply because G = H − TS holds for surface energies as well. The main thing of interest about this coarsening is that no shrinkage or densification takes place while heating in the reactive HCl atmosphere. If the same starting compacted powders—with about 45% initial porosity—were held at the same temperatures and times in air, the resulting sintered powders would achieve densities on the order of 95% of the theoretical crystalline density—or only about 5% residual porosity by volume. The main reason that densification is significantly decreased in a reactive atmosphere is that the particles grow rapidly and reduce the surface tension, the driving force for sintering, which, of course, is the same driving force for particle growth. This process of sintering solids in a reactive atmosphere can be used to make porous materials of controlled porosity (amount: 0% to about 50% by volume) and pore size (proportional to the grain size) for filter applications. 6.8 FREEZING POINT DEPRESSION OF SMALL PARTICLES 6.8.1 applicaTion of The clauSiuS–clapeyron relaTion Figure 6.12 is the pressure–temperature phase diagram for H2O and shows that the melting point of ice decreases as the pressure increases. This is because ice has a lower density than water and over the range from 0°C to about −20°C, ice has about 9% greater volume than water as shown in Chapter 1. A variation of the Clausius–Clapeyron equation (Silbey and Alberty 2001) can be developed to 169 170 Chapter 6. Thermodynamics of Surfaces and Interfaces and Some Consequences show the effect of pressure on the melting point, and more specifically, the effects of surface tension on the melting point of small particles. For liquid and solid water, the differential partial molar Gibbs energies—differential chemical potentials—of each can be written as Liquid 1atmosphere Pressure dG L = VLdP − SLdT dG S = VSdP − SSdT Solid Gas 0 (6.25) where L refers to liquid water and S to ice—solid H2O—and the barred quantities are the partial molar values. At equilibrium along the line in Figure 6.12 between solid and liquid, the partial molar free energies are equal, so 100 VL dP − SL dT = VSdP − SSdT Temperature (°C) FIGURE 6.12 Schematic pressure–temperature diagram for H2O. (6.26) and rearranging ( VL − VS ) dP = ( SL − SS ) dT = ∆H fusion dT T where ΔH fusion is obviously the enthalpy or heat of fusion, and integrating ( VL −VS )∆P T = T0 e ∆H fusion (6.27) which for particles of radius r with a surface tension γ becomes ( VL −VS ) 2 γ T = T0 e ∆Hfusion 6.8.1.1 r . (6.28) Example: One-nm Water Drops Take a particle size of r = 1 nm = 1 × 10−9 m, γ(H2O) = 72.8 × 10−3 J/m2, and, from Chapter 1, VL = 18.08cm3/mol and VS = 19.65 cm 3 mol , so ( VL − VS ) ≅ (18.08 − 19.65 ) = −1.57 cm 3 mol × 10 −6 m 3 cm 3 ∆H fusion = ( 333.5 J / g )(18 g / mol ) = 6000 J / mol. Because T0 = 273 K, −1.57 × 10 −6 2 × 72.8 × 10 −3 T = 273 × exp = 263 K. 6000 1× 10 −9 In other words, the equilibrium freezing point of 1 nm radius drops is about −10°C. 6.9 SPECIFIC SURFACE AREA Because particle size is being discussed, this is an appropriate time to introduce the concept of the specific surface area = S. The units of S are m2/g or cm2/g and S is frequently used to give a measure of the average particle size of a powder. S is defined as the area per unit mass. So taking a sphere of diameter d, S= A A 6 πd 2 = = = m ρv ρ( πd 3 / 6) ρd (6.29) 6.10 Wetting Frequency where: m is the mass (g) A is the area (m2) v is the volume (m3) ρ is the density (g/m3) d is the particle diameter (m). 171 Mean For example, take Al2O3, with a density of ρ = 4.0 g cm 3 (Haynes 2013) with Particle size S = 200 m 2 g; then d = 6 ρS = 6 / 4.0 × 106 g m 3 × 200 m 2 g = 7.5 × 10 −9 m or 7.5 nm, roughly 50 atoms along an edge. The specific surface area, S, FIGURE 6.13 Typical particle size distribution, is only a rough estimate of the particle size because most powders will usually a log-normal distribution, showing the mean have a particle size distribution similar to that shown in Figure 6.13: one particle size. that is skewed to the smaller particle sizes typically and fits a lognormal distribution, that is, if plotted versus log10d, the distribution would look like a normal distribution symmetrical about µ = log10 d, where μ is the lognormal mean of the lognormal size distribution. Sometimes the specific surface area per mole, S (keeping the convention of barred quantities for molar quantities), is used rather than per gram. In this case ( S= ) A 6 A πd 2 M= M= M= V m d ρv ρ( πd 3 / 6) (6.30) where: M is the molecular weight V is the molar volume (m3/mol). For the alumina example above, with a molecular weight of M = 102 g/mol, S = 2.0 × 10 4 m 2 mol. 6.10 WETTING As seen above, treating surface tensions as if they were forces acting along the line of intersecting surfaces is a useful way of establishing relationships between surface tensions or surface energies and the shapes of condensed phases. The same can be said for the wetting of a liquid (or solid) on a solid (or liquid) surface. In Figure 6.14, a liquid drop in the shape of spherical cap is resting on a solid surface and the system is at equilibrium. Where the liquid surface meets the solid surface, a force balance can be established treating the relative surface—interfacial to be precise—energies as if they were forces acting along the curve of intersection of the surfaces. From Figure 6.14, this becomes γ SL + γ LV cos θ = γ SV or cos θ = γ SV − γ SL γ LV (6.31) Vapor Liquid γLV θ γSL γSV Solid FIGURE 6.14 A liquid drop on a solid surface with vapor, solid, and vapor in “equilibrium.” 172 Chapter 6. Thermodynamics of Surfaces and Interfaces and Some Consequences which says that the angle at the surface depends on the relative values of the three interfacial energies. This is Young’s equation. If θ < 90°, then the liquid wets the solid. If θ > 90°, the liquid is nonwetting. And if θ = 0, the liquid spreads on the surface or is spreading. So, the spreading coefficient, S (an unfortunate redundant symbol), can be defined as S = γ SV − ( γ LV + γ LS ) (6.32) and for S > 0, the liquid spreads or covers the surface of the solid. For S < 0, droplets form on the surface. This is obvious from the relative interfacial energies determining S. If the sum of the interfacial energies between the liquid and solid and liquid and vapor are less than that of the solid–vapor interface, then the total interfacial energy is lowered by spreading. As an example of partial wetting, take γSV = 1 J/m2, γLV = 0.3 J/m2, and γSL = 0.8 J/m2, so cos θ = 1.0 − 0.8 = 0.67 0.3 θ = 48° which would look very similar to the drop in Figure 6.14. Also, S = 1 − (0.8 + 0.3) = −0.1, which is less than zero, so droplets should form as they do. There is only one problem with this analysis. Clearly, in Figure 6.14, the vertical forces are not balanced! This has been pointed out by others (Hiemenz 1986; Hudson 1998) as one problem with Equation 6.31, among others, but it is used, nevertheless, to measure interfacial energies. On the other hand, if all three phases—gas, solid, and liquid—were in complete equilibrium, a situation much like that shown in Figure 6.15 might result. Here, some of the solid has dissolved in the liquid and redeposited to form the angle φ at the three-phase interface allowing equilibrium between the vertical surface forces as well as the horizontal. There are now two equations that must be solved, a modified equation 6.31, γ SL cos ϕ + γ LV cos θ = γ SV: horizontal (6.33) γ LV sin θ = γ SL sin ϕ : vertical. (6.34) and Given the three interfacial energies, the two equations can, in principle, be solved for the two angles: However, this might not be so straightforward and may require numerical iteration. Similarly, if both angles can be measured, then two of the interfacial energies can be calculated, and so on. The geometry in Figure 6.15 would be expected for two immiscible liquids such as a drop of oil floating on water and both the horizontal and vertical components would balance. Also, this equilibrium geometry could be envisioned for a water drop on the surface of a piece of sodium chloride, NaCl. The solid would dissolve in the drop until the liquid reached saturation and the equilibrium shape shown in Figure 6.15 would develop. However, complete equilibrium would never be reached for a water drop on SiO2 glass or on PTFE, polytetrafluoroethylene, Teflon® because the rate of dissolution would be too slow or thermodynamically not possible. Nevertheless, on the basis of Vapor Liquid γLV γSV θ φ γSL Solid FIGURE 6.15 Liquid drop on solid surface with true equilibrium between the solid, liquid, and gas. 6.11 Interfacial Energies and Microstructure 173 thermodynamic arguments, others (Adamson 1982; Miller and Neogi 1985; DeHoff 2006) conclude that Equation 6.31 is valid even if complete equilibrium is not reached, that is, the solid is essentially inert. In Appendix A.2, applying a composite of two approaches in the literature, a thermodynamic argument, it is shown that Young’s equation does hold for an inert solid surface. Because the Young equation has been used for over 200 years, it must give reasonably correct answers! 6.11 INTERFACIAL ENERGIES AND MICROSTRUCTURE Phase diagrams indicate whether two or more phases are in equilibrium but say nothing about how those phases are distributed in the microstructure of a solid (or a solid plus liquid or two liquids— maybe in microgravity of space to prevent convection). Figure 6.16 schematically depicts a second phase, β, dispersed in a solid phase, α (β could simply be a pore in a ceramic), with β shown at the grain boundary of α. Again, application of a force balance between the interfacial energies leads to γ αα = 2 γ αβ cos ϕ 2 (6.35) or cos ϕ γ αα = 2 2γ αβ where γαα is the grain boundary energy and φ is the dihedral angle—that is, it is bisected by the line of the grain boundary. If γαα/2γαβ = 0, the φ/2 = 90° or φ = 180° and beta forms spherical particles and there is no tendency for β to prefer grain boundaries. On the other hand, if γαα/2γαβ = 1.0, then β completely wets the grain boundaries of α, as shown in Figure 6.17. How the two phases are dispersed has a significant effect on properties. For example, assume that beta is copper and alpha is Al2O3. The electrical conductivity of copper is about σ ≅ 106 S/cm and that of Al2O3 about σ ≅ 10−12 S/cm, or about 18 orders of magnitude different! For the microstructure of Figure 6.17, continuous copper, the low-frequency* conductivity would be about σ ≅ 103 S/cm with only about 0.1 v/o Cu. For the microstructure of Figure 6.16, in which the copper is isolated in lenses at grain boundaries, the copper would have hardly any effect on the low-frequency conductivity and σ ≅ 10−12 S/cm, about that of the alumina. Clearly, the relative interfacial energies of phases have a significant effect on the microstructure of a material and its consequent properties. An industrial example where only a small amount of a grain boundary wetting phase has a significant impact on properties is the hot-shortness of steel. Hot-shortness refers to rolling of steel at elevated temperatures with cracking along the steel grain boundaries. The reason for this is sulfur impurities in the steel form molten FeS2 (melting point = 1172°C) that wets the grain boundaries with a continuous liquid film causing the grains to separate. To avoid this, manganese, Mn, is added to the steel, which preferentially forms MnS rather than FeS2 and has a melting point of 1530°C, above the rolling temperature of the steel so no liquid phase is formed during rolling and cracking does not occur. A corollary to the situation for the two-phase system in Figures 6.16 and 6.17 is a single-phase polycrystalline system where at three-grain junctions, as shown in Figure 6.18, the grain boundaries must form 120° angles. * High frequencies would give different results. Alpha γαβ γαα φ Grain boundary β γαβ Alpha FIGURE 6.16 Interfacial energy force balance on a second phase particle of beta, β, at a grain boundary in alpha, α. α α α β α FIGURE 6.17 Two phase microstructure of beta, β, completely wetting the grain boundaries of alpha, α, and forming a continuous phase. Grain boundaries α α γαα γαα φ = 120° γαα α FIGURE 6.18 Three-grain junction in a singlephase crystalline material. Interfacial energy balance requires 120° angles at the junctions. Chapter 6. Thermodynamics of Surfaces and Interfaces and Some Consequences 6.12 INTERFACIAL ENERGIES AND SURFACE SHAPE Chemical etchants are frequently used to delineate the details of the microstructures of metals. These etchants can either etch different crystallites or grains at different rates in different crystallographic directions or simply form an oxide layer of differing thickness in different crystallographic directions depending on the relative rate of the etchant–surface reaction kinetics. In either case, each grain or crystallite reflects differently in a microscope (optical or scanning electron microscope, SEM), so the microstructure is visible. For compounds such as ceramics, very strong acids at relatively high temperatures are needed to etch—dissolve—the crystallites. Also, of course, for oxides, oxidizing etchants will not work. Therefore, chemical etchants are not as useful for ceramic materials as for metals. However, the technique of thermal etching is far superior. In this case, the surface of the material is polished just as in the preparation of a surface for chemical etching. The sample is then heated at some elevated temperature, usually a few hundred degrees or more below the sintering or densification temperature where the atoms or ions can diffuse and cause shape changes and allow the surface tension forces to equilibrate as shown in Figure 6.19. In this case, at equilibrium γ SS = 2γ SV cos ϕ 2 or cos ϕ γ = SS 2 2γ SV (6.36) where γSS = grain boundary energy. Figure 6.20 shows an actual grain boundary groove formed on a thermally etched surface of MgO at 1200°C measured with an atomic force microscope (AFM). The AFM measures the vertical height on a surface by scanning a sharp point along the surface, which Polished surface γSV γGB After some time at elevated T (a) Grain boundary γSV φ (b) nm 0 75 FIGURE 6.19 The formation of a grain boundary groove at the surface of a polished polycrystalline solid. (a) Polished surface near a grain boundary. (b) Grain boundary-surface energy equilibration at elevated temperatures. −75 174 (a) (b) 0 μm 2.15 FIGURE 6.20 Grain boundary groove on polycrystalline MgO formed at 1200°C after 2 h in air imaged in an atomic force microscope (AFM). (a) Image produced by scanning and (b) shape across the grain boundary, average of the scans in the rectangle in the image on the left. Note that the groove shape is distorted by a 15:1 vertical to horizontal magnification. (Y. Yeo photograph; Yeo 2007.) 6.13 Capillary Rise measures the attractive force between the point and the surface. Note that the vertical magnification in Figure 6.20 is about 15 times that of the horizontal magnification. In reality, these grooves are rather shallow and their angles large. Assume that γSS ≅ 0.5 γSV. Then, cos (φ/2) = 0.25 and φ/2 = 75.6° or φ = 151.2°. A rather shallow groove. The “hump” at the side of the groove is caused by material moving away from the grain boundary by diffusion forming this characteristic groove shape. Figure 6.21 is again the thermally etched microstructure of the yttrium-iron-garnet magnetic oxide shown earlier, which also shows the “humps” or built-up regions in the vicinity of all of the grain boundaries. The “black” spots are pores, mainly at the grain boundaries; however, there is a single pore within a grain at the top center of the photograph. Note that the pore within the grain is essentially spherical, suggesting that the surface tension is isotropic at the temperatures at which this material was densified, about 1400°C. On the other hand, the pores at the grain boundaries are distorted into “football” shapes (upper right) by the equilibration of the surface and grain boundary energies (Figure 6.16). 6.13 10 μm FIGURE 6.21 Thermally etched polycrystalline garnet, Y3Fe5O12. Note the hills on the sides of the grain boundaries and the shapes of the pores both within the grain (top) and at grain boundaries. (D. W. Readey photograph.) Vapor θ r γLV CAPILLARY RISE Capillary tube 6.13.1 The model Figure 6.22 sketches the rise of a wetting liquid in a capillary tube of radius r. The force balance in this case is the upward pull of the surface tension of the liquid wetting the tube and the weight of the liquid in the capillary pulled up to a height h F+ z = F− z 2πrγ LV cos θ = πr 2ρgh rρgh = 2 cos θ 2γ 2γ cos θ F+ z = (area ) × ∆P = πr ∆P = πr = πr 2 = 2πrγ cos θ R r 2 Liquid FIGURE 6.22 Rise of a liquid in a small diameter capillary due to wetting. Vapor (6.38) and can be used to measure the surface tension of liquids and it is particularly useful for measuring the surface tensions of high-temperature liquids. The major difficulty is measuring the angle theta, θ. The above approach to the simple result in Equation 6.38 is unfortunately invalid, but it gives the correct answer anyway! The proper way to get to Equation 6.38 is to consider the pressure difference over the curved liquid surface and its balance with the amount of liquid raised by the pressure as shown in Figure 6.23. Because of the angle theta, θ, made by the intersection of the liquid with the surface of the capillary, the radius of curvature of the surface of the liquid, R, is actually negative (its center is outside of the curved liquid surface), so there is a negative pressure ΔP = −2γ/R pulling the liquid up balanced by the weight of the liquid pulling down. From the geometry of Figure 6.23, r = R cosθ, so, 2 h (6.37) where ρ = liquid density (g/cm3) and g = acceleration of gravity = 9.8 (m/s2). Rearranging this equation leads to γ LV 175 (6.39) θ r R θ R Capillary tube h Liquid FIGURE 6.23 Same as Figure 6.22 but with other geometrical features identified to use in the correct method for calculating capillary rise. 176 Chapter 6. Thermodynamics of Surfaces and Interfaces and Some Consequences which is exactly the same F+z obtained from Figure 6.22. Equation 6.39 leads immediately to Equations 6.37 and 6.38. 6.13.1.1 Example: Liquid FeO at 1369°C Molten FeO completely wets solid Al2O3 (melting point Al2O3 = 2050°C) at 1369°C, so θ = 0 and rises to a height of 4.18 cm in an alumina tube of r = 0.5 mm = 5 × 10−4 m. The density of molten FeO is ρ = 5.7 g/cm3 × (106 cm3/m3)/1000 g/kg = 5.7 × 103 kg/m3. Therefore, γ FeO ( )( ) ( 5 × 10 −4 5.7 × 103 ( 9.8 ) 4.18 × 10 −2 rρgh = = 2 2 ) γ FeO = 0.584 J m 2. 6.13.2 mercury poroSimeTry A very useful measurement technique based on the phenomenon of capillary rise is that of mercury porosimetry, which is used to measure pore size distributions in porous materials. In this case, mercury has a surface tension of γLV = 0.476 J/m2 and essentially does not wet nonmetals; so θ = 180°C and mercury must be forced into pores under positive pressure. From the value of the pressure, the pore size can be determined, and the volume of mercury forced into the porous body at a given pressure is the volume of pores of the size corresponding to this pressure. Suppose a porous rigid polymer has a pore diameter of 0.1 μm or r = 5 × 10−8 m. Therefore, ΔP = 2γ/r = 2 × 0.476/5 × 10−8 = 1.9 × 107 Pa = 19 MPa ≅ 2700 psi. If 0.1 cm3 of Hg were forced into the sample at this pressure in a total sample of 1 cm3, then the sample would have 10 v/o porosity of pore size 0.1 µm. By gradually changing the pressure and observing the volume of mercury forced into the sample as a function of pressure, the volume of porosity as a function of pore size can be obtained. Of course, this assumes that all of the porosity is open to the outer surfaces, so that the mercury can get to all of the porosity. If some of the porosity is closed porosity, mercury porosimetry will not detect it and additional techniques must be used to determine the amount of closed porosity. 6.13.3 oTher meaSuremenT TechniqueS There are many other techniques used to measure surface tension of both liquids and solids. Some examples are shown in Figure 6.24. The sessile drop technique relies on a liquid drop that does not wet the surface. From the density and the shape of the drop—d and h—the surface tension of the liquid Solid Liquid Solid h dm d Solid Sessile drop dS L Liquid dm 2r dL/dt Creep Pendant drop FIGURE 6.24 Other techniques used to measure surface energies that are particularly useful at high temperatures are shown. In the sessile and pendant drop techniques for liquids, the shapes are determined by the density and surface tension of the liquid and the latter is determined by comparing the shape to empirically determined shape parameters in the literature. For solids, the surface tension is balanced by the weight of the wire or fiber plus added weight when the creep rate is zero. From the weight of the fiber and added weight at zero creep, the surface tension can be calculated. 6.14 Surface Segregation and Surface Tension can be calculated from empirical shapes determined with liquids of known surface tension (Miller and Neogi 1985). This technique is particularly useful for making measurements at high temperatures (Humenik and Kingery 1954). A similar technique, the pendant drop, measures the dimensions of a suspended liquid drop as shown in Figure 6.24 and compares its shape to pendant drops of liquids of known surface tension (Adamson 1997). This technique is also particularly useful at high temperatures up to over 2000°C (Kingery 1959). Finally, a technique that is particularly useful for both inorganic glasses and amorphous polymers is zero creep, also shown in Figure 6.24. In this technique, thin strands or wires of different lengths of the material to be tested are suspended with or without weights and the creep rate is measured. The stress causing creep is the difference between the surface tension forces trying to distort the wire into a sphere making it deform in the upward direction and the downward weight of the wire itself (and added weights). When there is zero creep, these stresses just balance and the surface tension of the wire can be calculated. Again, this is a very useful technique for making hightemperature measurements on inorganic glasses and other solids (Udin et al. 1949; Parikh 1958). 6.14 SURFACE SEGREGATION AND SURFACE TENSION 6.14.1 giBBS adSorpTion iSoTherm The Gibbs adsorption isotherm in a two-component system in which the solvent is A and the solute is B is given by (Appendix A.3): dγ A = −Γ B,A dµ B = −Γ B,A dG B = −Γ B,A RTd ln a B = −Γ B,A RTd ln X B or dγ A = −Γ B,A RTd ln CB (6.40) where γA = the surface tension of A (J/m2), µ B = G B = the chemical potential or partial molar Gibbs energy of B (J/mol), aB = activity of B and aB = fBXB, fB = activity coefficient of B,* XB = mole fraction of B, and CB = the concentration of B = X B / Vso ln, where Vso ln = the molar volume of the solution of this composition. Note: because lnaB = lnfB + lnXB, d ln a B ≅ d ln X B ≅ d ln CB if the composition range is small so that fB and Vso ln are essentially constant, so the equation in the box is more or less valid. Now, Γ B, A is the excess surface concentration of B at the surface of the solution and Units(ΓB, A) = mol/m2. ΓB,A is the difference between the actual surface concentration of B minus the concentration that would be expected if the concentration of B were the same in the bulk and in the surface. As shown in Appendix A.2, the surface excess concentration of B in A, ΓB, A, can also be expressed as X Γ B, A = Γ B − B Γ A XA (6.41) where: ΓB is the actual surface concentration of B (mol/m2) ΓA is the surface concentration of A in pure A (mol/m2) X A and XB are the mole fractions of A and B, respectively, in the bulk solution. Now (XB/X A)ΓA is the surface concentration of B if it had the same surface concentration as the concentration in the bulk. So, if (X B/X A)ΓA has the same value as ΓB, then there is no surface excess of B—no segregation—and no effect of B on the surface tension. Therefore, Equation 6.40 states that the surface tension of the solution is lowered if the solute B segregates to the surface so that * Normally, the activity coefficient is given the symbol γ, but because this symbol is being used for the surface tension (energy), f will be used instead because it is only used briefly here. 177 178 Chapter 6. Thermodynamics of Surfaces and Interfaces and Some Consequences ΓB, A > 0. Atoms, ions, or molecules that segregate to the surface lower the surface tension and are called surfactants. Conversely, things that have a lower concentration in the surface than predicted from the bulk concentration, desegregate and raise the surface tension of A (Evans and Wennerström 1999). 6.14.1.1 Example: Water with Sodium Dodecylsulfate, C12H25OSO3Na, in Solution About 8 × 10−3 mol/L of Sodium dodecylsulfate (SDS) in solution will lower the surface tension of water considerably, about a factor of 2, to about 36 × 10−3 J/m2 (Evans and Wennerström 1999). First, calculate the surface concentration of water in pure water, 1 ρ 1g cm 3 = = = 5.56 × 10 −2 mol / cm 3 V M 18 g mol × 106 cm 3 m 3 = 55600 mol m 3 × 6.022e23 = 3.348 × 1028 molecules /m 3 which gives (3.348 × 10 ) = 28 Γ H 2O 6.022 × 10 2/3 23 = 1.725 × 10 −5 mol H 2O /m 2 for the number of moles at the surface of pure water. Another method is to calculate a monolayer thickness, d, at the surface of H2O. This is d= 1 = 3.103 × 10 −10 m. (3.348 × 1028 )1/3 So, Γ H 2O = ( d = 3.103 × 10 −10 m 55,600 mol /m 3 V ) = 1.725 × 10 −5 mol /m 2 which is the same. For 8 × 10−3 mol/L of SDS in the bulk (8 × 10−3 mol/L × 103 L/m3 = 8 mol/m3), the same calculation would give a surface concentration of 0 = 3.103 × 10 −10 m × 8 mol /m 3 ΓSDS = 2.482 × 10 −9 mol SDS /m 2 if there were no surface segregation. This can also be obtained from ( XB 8 1.725 × 10 −5 ΓA = XA 55600 ) = 2.482 × 10 −9 mol / m 2 because XB/XA = nB/nA as both the number of moles are divided by nA + nB, the total number of moles, to get the mole fractions. Calculating ΓSDS,H2O from the lowering of the surface tension of water: ΓSDS,H2O = − ∆γ H2O RT∆ ln CSDS ΓSDS,H2O = − 36 × 10 −3 (8.314 )( 300 ) ln 8 ×10−3 ΓSDS,H2O = 3.0 × 10 −6 mol m 2 ( ) 6.14 Surface Segregation and Surface Tension This value of the SDS surface concentration would be three orders of magnitude higher than that if the SDS were uniformly dispersed throughout the system. The excess surface concentration of SDS, 0 ΓSDS, H2 O = ΓSDS − ΓSDS ≅ ΓSDS , which is the surface concentration of SDS. Dividing this result by “d” gives the molar concentration at the surface [SDS] = ( ΓSDS mol / m 2 d( m ) ( 3.0 × 10 −6 10 −3 )× Hydrophobic tail 1 3 3 10 l / m 3 ) Hydrophilic head Air 3.103 × 10 −10 [SDS] = 9.7 mol / l about a factor of about 1000 higher than in the bulk! Clearly, the SDS segregates to the surface. 6.14.2 O O S Na+ oTher exampleS 6.14.2.1 Surface Segregation in Other Materials In the above example, SDS has a nonpolar, hydrophobic—water-hating— tail, C12H25, which would like to be at the surface and out of the water, the reason for its surface segregation, and the anionic hydrophilic—waterloving—head, −OSO3−, which would prefer to be solvated in the polar water (Figure 6.25). In contrast, sodium chloride, NaCl, in aqueous solution raises the water surface tension because the sodium and chlorine ions prefer the polar bulk of the water rather than to be near the air interface and desegregate (Evans and Wennerström 1999). Similar effects occur in other liquids. Oxygen and sulfur segregate to the surface of molten iron and lower its surface tension (Figure 6.26), whereas carbon does not segregate and has virtually no effect on γLV of iron (Kingery et al. 1976). Oxygen segregates to the surface of molten copper and silver and lowers their surface tensions as well. Finally, metals that are strong oxide formers, such as titanium, chromium, and zirconium, when added to molten metals such as Cu and Ni lower the interfacial energy, γSL , between these molten metals and solid oxides such as Al 2O3 and increase wetting of the oxide. In principle, the strong tendency for Ti, Cr, and Zr to form oxides causes them to segregate to the molten metal–solid oxide interface, thereby lowering the interfacial energy because they segregate to the interface. This concept is used to formulate metal–ceramic brazing alloys (Schwartz 1990). There are other examples. The segregation to the interface between molten copper and solid aluminum oxide by oxygen lowers the interfacial energy between the molten copper and the alumina, which allows the copper to wet the alumina (O’Brien and Chaklader 1974), This makes possible the fabrication of a near net shape Cu–alumina composite that has the mechanical properties and machinability of a steel but with a lower density and a much higher thermal conductivity. The former because of the alumina and the latter due to the presence of a continuous phase of copper: its microstructure is shown in Figure 6.27. 6.14.2.2 Froth Flotation Another important example where surface segregation plays an important role in materials processing is froth flotation, which is used to separate ores, particularly sulfides, from other minerals. The ore is ground into Surface − − − − − − − − − − − − − − Water solution FIGURE 6.25 Sodium dodecylsulfate (SDS) molecule and how the SDS molecules segregate to the surface of an aqueous solution so that the hydrophobic part of the molecule points out of the solution surface. Surface energy, γ [SDS] = O 179 log10XB FIGURE 6.26 The Gibbs adsorption isotherm shows the effect of segregation to the surface on the surface energy of A, γSV, as a function of the mole fraction of an additive B, XB. Typical of the behavior of oxygen and sulfur in liquid iron and oxygen in liquid copper as examples. (Kingery et al. 1976.) FIGURE 6.27 Backscatter SEM micrograph of a Cu–Al2O3 composite formed by the infiltration of molten copper into porous aluminum oxide. Cu is the light phase in this case and the Al2O3 the dark one. (S. Larpkiattaworn photograph; Larpkiattaworn, 1995.) Chapter 6. Thermodynamics of Surfaces and Interfaces and Some Consequences fine powder and dispersed in a water suspension containing sodium xanthate (Figure 6.28), which again is a surfactant that has an ionic head and a hydrophobic organic tail. The ionic sulfur head attaches itself to the sulfide powder particles and the organic tail points away from the surface as shown in Figure 6.29. Air is bubbled though the suspension, producing a “froth” of bubbles, and the hydrophobic tail of the xanthate ion segregates to the bubble surface and both the bubble and mineral rise to the surface of the suspension, separating the sulfides from the other minerals. The froth bubbles are collected and the sulfide mineral is washed from the xanthate solution, which can then be used again. S S− O Nonpolar Na+ Cation Anion − Representation FIGURE 6.28 Sodium ethyl xanthate molecule used for froth flotation of sulfide minerals. 6.14.2.3 Coupling Agents − − − − − − − − − − − − − − PbS − − FIGURE 6.29 Schematic representation of how xanthate ions attach themselves to sulfide ore particles allowing separation. Sodium ethyl xanthate specifically attaches to lead sulfide, PbS, particles allowing them to be separated from other sulfides. Another example of the tailoring of surfaces in materials science and engineering is the use of coupling agents (Plueddemann 1991) to bond silicate glass and other fibers (or other shapes) to polymers. In this case, silicon-containing compounds with organic tails—R—are used as shown in Figure 6.30. The CH3O– groups on the silane molecule, methacryloxypropyltrimethoxysilane here, react with the OH− ions on the surface of silicate glass to form Si–O–Si surface bonds with the formation of CH3OH, which goes into the solution. The OH is on the surface because of the reaction of the ambient atmospheric water vapor with the silicate surface: –Si–O–Si– + H2O → 2 –Si–OH. The organic tail of the silane now makes the inorganic surface of the silicate appear as a nonpolar polymer surface, allowing it to readily attach itself to another polymer or other nonpolar material. Such coupling agents are used in polymer–fiber glass composites and on the surface of silicon wafers to help bond the organic photoresist material to the native silicon dioxide on silicon. The photoresist is used to pattern the semiconductor device structures into the surface of silicon. O H3C O CH2 Coupling agent H2 C H2 C O CH3 Si C O CH3 H2 O CH3 Solution O H3C O CH2 H2 C HO Si HO Si HO Si Silicate glass Surface 180 C H2 H2 C Si O Si O Si O Si + 3 CH3OH FIGURE 6.30 Methacryloxypropyltrimethoxysilane is just one of many silane coupling agents (Plueddemann 1991). It is shown here to demonstrate how the methoxy groups react with the OH groups on the surface of the silicate forming chemical bonds and leaving the “organic” part of the molecule facing the solution, which makes it easier to bond the silicate glass to nonpolar materials such as polymers. 6.15 6.15 Wetting of Microporous Surfaces WETTING OF MICROPOROUS SURFACES In contrast to making surfaces more wettable, with the availability of nanoscale materials, there is an interest in using these small particles to create nonwettable surfaces (Yang et al. 2013). In the wetting equation, Equation 6.31 cos θ = γ SV − γ SL γ LV if the area of the surface the drop is covering (Figure 6.14) can be made larger than the geometric area of the bottom of the drop by roughening the surface producing a roughness factor, χ, where χ is simply (Wenzel 1936) χ = roughness factor = actual surface area geometric surface area then Equation 6.31 can be modified to cos θD = χ ( γ SV − γ SL ) γ LV (6.42) where θD is the contact angle on the rough surface to distinguish it from that on a smooth surface, θ. For example, assume that the liquid does not wet the solid and γ SV = 332 mJ m 2 , γ SL = 400 mJ m 2 , and γ LV = 200 mJ m 2, then cos θ = 332 − 400 = −0.34 200 θ = 110°. If the roughness factor were χ = 2 = 1.414, then cos θ = −0.481 and θ = 119°, as shown in Figure 6.31. If the roughness factor were χ = 2.08, then cos θ = −1 and θ = 180° or no wetting at all! Wenzel found indeed that the contact angle was greater on a rough surface compared with a smooth surface of the same material. Cassie and Baxter (1944) carried the analysis further to include porosity as well as roughness with the intent of minimizing wettability with a designed surface structure, which included both a higher surface area and porosity as shown in Figure 6.32. They were interested in waterproof Rough surface, 45° corrugations θ = 110° θD = 119° Liquid Liquid Smooth surface Rough surface FIGURE 6.31 The difference in wetting angle for a given liquid–solid system between a smooth and rough surface. The surface roughness increases the liquid–solid interfacial area and decreases the wetting angle as described in the text. 181 182 Chapter 6. Thermodynamics of Surfaces and Interfaces and Some Consequences Microporous lyophobic surface Liquid θ θD Solid FIGURE 6.32 The difference in wetting angle for a given liquid–solid system between a flat surface and one with roughness and porosity. With surface layers of nanoparticles with lyophobic coatings, so-called super lyophobic surfaces, can be made for a number of applications. Liquid A. γLS θ r φ θ . B Vapor Solid 2r γLV r γSV b 2b Solid FIGURE 6.33 Parallel rods of Cassie and Baxter (1944) used to model the apparent wetting angle, θD, for a real wetting angle of θ for a rough, microporous surface as shown at the top. The model is given in detail in the text. clothing, and Figure 6.33 shows the envisioned structure of parallel cylinders that simulates cloth fibers. Figure 6.33 also shows the details of the structure made of parallel cylinders of unit length perpendicular to the page with a radius r and a separation distance of 2b (the porosity). Let A LS be the area of the liquid–solid interface when a drop of liquid is placed on this composite surface. Likewise, let A LV be the area of the liquid–vapor interface in the pore area. The energy in forming a total area AD is given by E D A D = A LS ( γ LS − γ SV ) + A LV γ LV where ED is the energy per unit area. Now, as before, Equation 6.31, cos θ = γ SV − γ SL γ LV so E D A D = A LS ( − γ LV cos θ ) + A LV γ LV A A E D = γ LV LV − LS cos θ A A D D E D = γ LV ( f LV − f LS cos θ ) (6.43) 6.15 Wetting of Microporous Surfaces where: f LV is the fractional area of the liquid–vapor interface f LS is the fractional area of the liquid–solid interface. Now Equation 6.31 can be written as cos θ = −E γ LV because ( γ LS − γ LV ) is the energy, E, to form the unit area of the liquid–solid interface. Therefore, by analogy, for a drop sitting on a porous surface (Figure 6.32), a contact angle for a drop on the porous surface can be written as cos θD = − ED = f LS cos θ − f LV . γ LV (6.44) If the surface is just rough and not porous, f LV = 0, and the result is Wentzel’s equation for a rough surface (Equation 6.42). For the model in Figure 6.33, because the structure is one unit long perpendicular to the paper surface, a unit of area is A D = 1 × ( r + b ), so f LS = 1 ( r + b ) πr − πr θ 180° θ πr fLS = 1 − 180 . + r b (6.45) Also, f LV = 1 ( b + r − r cos ϕ ) . ( r + b) From the figure, cos ϕ = cos ( 90 − θ ) = cos ( 90 ) cos θ + sin ( 90 ) sin θ cos ϕ = 0 × cos θ + 1× sin θ cos ϕ = sin θ therefore, f LV = 1 ( b + r − r sin θ ) ( r + b) f LV = 1 − r sin θ. r+b Figure 6.34 shows how the wetting angle θD increases as a function of the ratio of ( r + b ) r with the wetting angle for a smooth interface, θ, as a parameter. Clearly, as the separation between the 183 Chapter 6. Thermodynamics of Surfaces and Interfaces and Some Consequences 200 180 160 140 180 160 120 140 θD (°) 184 120 100 100 80 80 60 60 θ (°) 40 58 20 0 1 2 3 4 5 r+b r FIGURE 6.34 The apparent wetting angle versus essentially the porosity for the parallel rod model of Figure 6.33 with the real wetting angle as a parameter. For wetting angles, the apparent wetting angle—the lyophobicity—increases as the amount of porosity increases. cylinders increases, the amount of porosity and the wetting angle increases. Therefore, it is the structure of the surface that is producing the lack of wettability. This is exactly the reason water “rolls off a duck’s back” (Cassie and Baxter 1944) and why water beads up on lotus leaves. It is also the driving force for the interest in making hydrophobic surfaces with nanoparticles because the structure can be designed and fabricated into many different mixtures of particles and porosities. Interestingly, more careful modeling and observation of the wettability of such surfaces leads to almost identical results as these two older studies described above (Wang et al. 2015). 6.16 CHAPTER SUMMARY Although this chapter is mainly concerned with the thermodynamics of surfaces, surface tension, and its consequences, many of the concepts presented are important in kinetics, particularly because of the increasing interest is small or “nanoparticles” and their intrinsic instability because of their large surface areas. Surface tensions arise due to broken or unsatisfied atomic bonds at surfaces. As a result, ionic, metallic, and covalently bonded materials have high surface tensions or surface energies, whereas materials with weaker intermolecular bonds, such as polymers, have lower surface tensions. For solids, in addition to the surface energy, there exists a surface stress as well, which may not be relaxed at low temperatures and needs to be considered when surface energy effects are important. Surface tensions can be related to surface curvature and lead to changes in vapor pressures, solubilities, reactivities, and other thermodynamic properties of condensed phases. This leads to particle coarsening in particulate systems because of the higher total energies of the surfaces of small particles relative to larger ones, the kinetic phenomenon known as Ostwald ripening. In addition, the relationships between the various interfacial energies determine wetting behavior and microstructures of multiphase materials. This phenomenon is useful in measuring surface energies and can be used to measure porosity in materials by mercury porosimetry because of the nonwetting behavior of mercury on many surfaces. Additives or impurities that segregate to the surface of a condensed phase, solid or liquid, lower the surface tension, as described by the Gibbs adsorption isotherm, and have several important commercial applications. Finally, by structuring the surface on a micro- or nanoscale, the wettability of the surface can be decreased, which is important in designing waterproof or hydrophobic coatings on a variety of surfaces. Appendix APPENDIX a.1 Surface STreSS The demonstration of the existence of a surface stress and its relation to the surface energy or the surface tension is presented in several places in the literature (Cammarata 1997; Hudson 1998). Figure A.1 illustrates the various quantities and steps involved in the derivation. As shown in the figure, consider a cube of dimension a. Then, if the cube is extended in the x-direction by an amount da, the work done, W0 (this should be a dW or ΔW, but differential and difference symbols are dropped for clarity), is W0 = Fda. (A.1) Now if the cube is cut in two at its midsection, the total forces acting on both the top and bottom are the bulk applied force F/2 plus the surface stress, which acts along the length of the cut a and perpendicular to the direction of a, is a second-rank tensor (like all stresses) and typically given the symbol fxx. Also, like the surface energy and surface tension, it too has units of N/m! This new work term, W′, is given by F W′ = 2 dA + 2f xx ada = W0 + 2f xx ada. 2 (A.2) Rearranging this equation and defining the strain in the x-direction, ε xx = da a , the surface stress is given by f xx = W′ − W0 1 W′ − W0 1 W′ − W0 = 2 = 2 . 2ada a 2da a a 2ε xx (A.3) The task is to find expressions for W′ and W0 in terms of the surface tension on the two faces of the cut and relate them to the surface stress. First consider the top sequence in the figure, designated (a), and leading to result WI. Here, the cube is first extended by the applied force and then cut. The surface energy term for each face on the cut is the product of the new surface tension of the extended cut, γ + ∆γ, and the extended surface, A + ∆A (note that Δs and differentials are being used more or less indiscriminately, but it makes no difference). So, the total work for sequence (a) is given by a a y a Stretch first W0 Wl Then split F/2 afxx F afxx x F/2 z a (a) (γ + dγ)(A + dA) da F/2 afxx F afxx F/2 γA (b) Split first Then stretch WII FIGURE A.1 Model (Hudson 1998; Cammarata 1997) used to show that the surface stress, f xx, is given by f xx = γ + (dγ/dεxx). (a) The cube is stretched first then split. (b) The cube is split first then stretched. The details of the model are described in Appendix A.1. 185 186 Chapter 6. Thermodynamics of Surfaces and Interfaces and Some Consequences WI = W0 + 2 ( γ + ∆γ ) ( A + ∆A ) ( WI = W0 + 2 ( γ + ∆γ ) a 2 + a∆a ) ( WI = W0 + 2 ( γ + ∆γ ) a 2 + a ( aε xx ) ) WI = W0 + 2a 2 ( γ + ∆γ ) (1 + ε xx ) this leads to WI ≅ W0 + 2a 2 γ + 2a 2∆γ + 2a 2 γε xx (A.4) ignoring the small ∆γε xx second-order product. In the second case, (b), the cube is cut first, giving two surface energy terms, a2γ, and then extended giving the work, W′. The resulting total work is WII WII = 2a 2 γ + W′. (A.5) If both processes are carried out reversibly, then the total work must be equal for the two processes: WI = WII . (A.6) Therefore, combining Equations A.4 and A.5 gives W0 + 2a 2 γ + 2a 2 ∆γ + 2a 2 γε xx = 2a 2 γ + W′ and can be rearranged to give W′ − W0 ∆γ dγ . =γ+ =γ+ 2a 2ε xx ε xx dε xx (A.7) Substitution of Equation A.7 into A.3 gives the desired result: f xx = γ + dγ dε xx (A.8) that is, the surface stress is equal to the surface energy or surface tension, γ, plus the change in γ with the surface strain. In liquids and solids at high temperatures, where atoms or molecules from the bulk can easily move into surface positions, the surface stress is the same as the surface tension or surface energy. Only in solids at low enough temperatures, where diffusion cannot relieve the surface strain, is the surface stress an important factor. a.2 a Thermodynamic argumenT for young’S equaTion and WeTTing Because the vertical component of the force balance in Equation 6.34 is not satisfied, that is, φ = 0, can the horizontal component, Young’s equation, Equation 6.31, be justified in other ways? A thermodynamic approach is most reasonable. What follows is a modified composite of two approaches in the literature used to show that Young’s equation holds (Miller and Neogi 1985; DeHoff 2006). For constant temperature, volume, and composition, for a liquid drop, L, on a flat solid surface, S, both in contact with the vapor, V (Figure 6.14), the differential Helmholtz energy, dF, can be written as (Miller and Neogi 1985): dF = γ SV dA SV + γ SLdA SL + γ LV dA LV . (A.9) Appendix Vapor New liquid-vapor surface Liquid dL θ θ a Solid da M N FIGURE A.2 Geometry used to obtain Young’s equation, Equation 6.31, by a thermodynamic argument. The triple interface at M is moved a distance da to point N. The change in area of each of the interfaces is determined and related to dASL and then the Helmholtz energy is minimized reproducing Young’s equation. Figure A.2 shows the relation between the differential areas of the interface and the liquid drop. Adopting a modified procedure that considers an arbitrary displacement of the three-phase interface from point M to point N (DeHoff 2006)* in two dimensions. In this case, only changes in the x-direction are important because the vertical components can not be in equilibrium if the liquid drop is sitting on a flat, inert solid surface. Consider da to be a vector da from point M to point N. Then, the dot prod uct of da with direction of the solid–vapor interfacial energy will give the x-component of the change in area of the solid–vapor interface when multiplied by some length along the three-phase interface, which, for simplicity, will be called Δρ. So, dA SV = −∆ρda , for example, because −da ⋅ i = −da cos ( 0 ) = −da where i is a unit vector in the x-direction and the dot product gives the horizontal or x-component (and only component) for A SV . The minus sign is necessary because the area is decreased between the solid and the vapor. Similarly, for the solid–liquid interface, −da ⋅ i = −da cos (180 ) = da () not terribly surprising: dA SL = ∆ρda = −dA SV . For the x-component of the change in liquid–vapor area, −da ⋅ dL = −da cos (180 − θ ) −da ⋅ dL = −da ( cos 180 × cos θ + sin 180 × sin θ ) if dL is a unit vector tangent to the liquid–vapor interface at points M and N and the double-angle formula can be found in many places in the literature. So, dA LV = ∆ρda cos θ = dA SL cos θ. (A.10) Substituting the values for the areas in Equation A.9 dF = − γ SV dA SL + γ SLdA SL + γ LV dA SL cos θ * DeHoff’s (2006) thermodynamic approach of calculating the change in entropy of the shift of the triple line between the phases to give changes in area of the phases reaches exactly the same conclusion as the force balance, Equation 6.33—with slight differences in sign and angle conventions. 187 188 Chapter 6. Thermodynamics of Surfaces and Interfaces and Some Consequences At equilibrium, the Helmholtz energy must be a minimum with respect to dASL, so ∂F = γ SL − γ SV + γ LV cos θ = 0 ∂A SL or Young’s equation is obtained, namely, cos θ = γ SV − γ SL . γ LV a.3 The giBBS adSorpTion iSoTherm Consider a liquid in equilibrium with its vapor and a “surface layer” in between both, in equilibrium with both, and where the properties—such as concentration—change continuously between the liquid and the vapor. If the liquid is a two-component system in which there is some solute, component 2, dissolved in the liquid of component 1. Then, the first law of thermodynamics for the liquid and vapor phases are dU vap = TdSvap − PdVvap + µ1dn1,vap + µ 2dn 2,vap dU liq = TdSliq − PdVliq + µ1dn1,liq + µ2dn 2,liq . (A.11) A similar equation for the interface region is obtained by substituting the surface work term, γdA, for the PdV term because the surface really has no volume, and this term is positive because it is work done on the surface “phase”: dU σ = TdSσ + γdA + µ1dn1,σ + µ 2dn 2,σ (A.12) where σ refers to the surface. Integrating either of Equations A.11 over the extensive variables, S, V, and ni, gives U liq = TSliq − PVliq + µ1n1, liq + µ 2 n 2, liq and taking the total differential dU liq = TdSliq + Sliq dT − PdVliq − Vliq dP + µ1dn1, liq + n1, liq du1 + µ2dn 2, liq + n 2, liq dµ 2 (A.13) and subtracting Equation A.11 from A.13 gives (see Chapter 1) 0 = Sliq dT − Vliq dP + n1,liq du1 + n 2,liq dµ 2 . (A.14) At constant temperature and pressure, Equation A.14 becomes the Gibbs–Duhem equation, 0 = X1du1 + X 2dµ2 (A.15) because X1or2 = n1or2/(n1 + n2). With the same procedure applied to the surface, Equation A.12, the following is obtained for the surface region: 0 = SσdT + Adγ + n1,σdu1 + n 2,σdµ2 . At constant temperature and dividing by the area, A, 0 = dγ + Γ1dµ1 + Γ 2dµ 2 (A.16) Exercises where the Γ = n/A = the surface concentrations with Units(Γ) = mol/m2. Substitution of Equation A.15, the Gibbs–Duhem equation, for du1, gives X dγ = −Γ 2,1dµ 2 = − Γ 2 − 2 Γ1 dµ 2 X1 (A.17) where Γ2,1 is the “excess surface concentration of component 2 in component 1.” That is, if the concentration in the surface is different from what would be expected from the bulk composition, the surface energy of the solution will either increase or decrease. Of course, if Γ 2 Γ1 = x 2 x1 , that is, the surface concentrations are in the same ratio or are the same as in the bulk, then there is no surface excess and dγ = 0. Now µ 2 = µ 02 + RT ln a 2 by definition. So, dµ 2 = RTd ln a 2 ≅ RTd ln X 2 ≅ RTd ln C2 particularly if the concentration, C2, is not very large. Therefore, the Gibbs adsorption isotherm becomes X dγ = −RT Γ 2,1d ln C2 = −RT Γ 2 − 2 Γ1 d ln C2 X1 (A.18) which states that if the solute, component number 2, segregates to the surface, Γ2,1 > 0, then the surface energy, γ, decreases. Conversely, if component two desegregates, Γ2,1 < 0, then the surface energy increases. EXERCISES 6.1 a. At 1200oC, for liquid copper, γLV = 1285 mJ/m2, for solid Al2O3 γSV = 900 mJ/m2, and for the interfacial free energy between liquid copper and solid Al2O3 at this temperature, γSL = 1200 mJ/m2. Calculate the wetting angle, θ (degrees), for a liquid copper drop on an alumina plate. b. Calculate the spreading coefficient for molten copper on solid alumina. c. Make a hand sketch of this drop on the alumina plate. 6.2 a. Addition of oxygen in solution in the copper increases the wetting of the molten copper on alumina. If 1 w/o copper changes interfacial energy to γSL = 900 mJ/m2, calculate the wetting angle (degrees) for this oxygen–copper alloy on alumina. b. Calculate the spreading coefficient for this oxygen–copper alloy on the solid alumina. c. Make a hand sketch of this drop on the alumina plate. 6.3 a. Finally, enough oxygen is added to the molten copper to make it react with the solid alumina, so that γSL = −600 J/m2. Calculate the spreading coefficient for this oxygen–copper alloy. b. Make a hand sketch of this drop on the alumina plate. 6.4 a. Small particles (0.1 μm in diameter at t = 0 seconds) of hematite, Fe2O3, are undergoing coarsening by gas transport through the vapor phase and a surface reaction in an HClcontaining atmosphere through the following reaction: Fe 2O3 ( s ) + 6 HCl ( g ) 2 FeCl3 ( g ) + 3 H 2O ( g ) If the Gibbs energy, ΔGo, for this reaction at 1200oC is ΔGo = 131,376 J/mole, calculate the equilibrium constant at this temperature. 189 190 Chapter 6. Thermodynamics of Surfaces and Interfaces and Some Consequences 6.5 6.6 6.7 6.8 b. The coarsening is taking place at 1200oC in argon gas containing 10 % HCl with a total pressure of 1 atm. All of the water in the gas is produced by the reaction. Calculate the equilibrium FeCl3 pressure at this temperature in this gas. c. Calculate the [FeCl3] in the gas phase in moles/m3 under these conditions. d. If the density of Fe2O3 is 5.24 g/cm3 and its molecular weight is 159.69 g/mole, calculate the molar volume of Fe2O3 in m3/mole. e. For the surface reaction rate constant k, k0 = 7.20 × 104 m/s and Q = 120,000 J/mole. Calculate the value of the surface reaction rate constant (m/s) at 1200oC. f. If particle coarsening is taking place by surface reaction control, calculate the average particle size (diameter in μm) of the Fe2O3 after a total reaction time of 3 h if the surface energy of Fe2O3 is 900 mJ/m2. Neglect the starting particle size if possible. g. If the initial particle size had been 0.1 μm in diameter, calculate the number of the initial particles that have been incorporated into a single coarsened particle after 3 h. The following data exist for Cu in the literature (Brandes and Brook 1992): melting point, Tmp = 1083oC; heat of fusion, ΔHm = 13.02 kJ/mole; density at 20oC, ρ = 8.96 g/cm3; density of the liquid at the melting point, ρ l = 8.00 g/cm3; linear thermal expansion coefficient, α L = 17.0 × 10−6 K−1; molecular weight, M = 63.55 g/mol; and the liquid surface energy at the melting point, γ = 1285 mJ/m2. a. Calculate the molar volume, V0 (m3/mol), of copper at 20oC. b. Assuming that the change in volume of the solid with heating to the melting point is given by ∆V = V0 3α L ∆T, calculate the molar volume of the solid at the melting point of copper (m3/mol). c. Calculate the molar volume of the liquid copper at the melting point (m3/mol). d. Calculate the melting temperature of 10 nm diameter copper particles. The following data exist for silicon (Si) in the literature (Brandes and Brook 1992): melting point, Tmp = 1410oC; heat of fusion, ΔHm = 50.66 kJ/mol; density at 20oC, ρ = 2.34 g/cm3; density of the liquid at the melting point, ρl = 2.51 g/cm3; linear thermal expansion coefficient, αL = 7.60 × 10−6 K−1; molecular weight, M = 28.09 g/mol; and the liquid surface energy at the melting point, γ = 865 mJ/m2. a. Calculate the molar volume, V0 (m3/mol), of silicon at 20oC. b. Assuming that the change in volume of the solid with heating to the melting point is given by ∆V = V0 3α L ∆T, calculate the molar volume of the solid at the melting point of silicon (m3/mol). c. Calculate the molar volume of the liquid silicon at the melting point (m3/mol). d. Calculate the melting temperature (oC) of 10 nm diameter silicon particles. A liquid silicate with surface tension of 500 mJ/m2 makes contact with a polycrystalline oxide with an angle of θ = 40 o on the surface of the oxide. If mixed with the oxide, it forms discrete liquid globules at three grain intersections with the average dihedral angle φ = 80o. If the interfacial tension of the oxide grain boundary is 900 mJ/m2, a. Sketch these two microstructures and show the interfacial energies acting as forces. b. Compute the solid–liquid surface energy. c. Compute the solid–vapor surface energy. d. Is this a reasonable value for the solid surface energy? Figure E.1 schematically depicts a typical snowflake about 1 mm in diameter. The hexagonal shape reflects the hexagonal symmetry of the ice crystal, and the dendritic (branched, treelike) structure reflects the details and anisotropy of the kinetics of the ice crystal growth process from the water vapor in the atmosphere after the snowflake had been nucleated in the center (probably by a dust particle) and not the anisotropy of the surface energy. The radius of curvature at the end of one of the hexagonal tips is about 10 μm. The vapor pressure of ice over a flat surface at 23oF is 3.01 mm of Hg (760 mm of Hg = 1 atm) and the density of ice at this temperature is 0.917 g/cc (Haynes 2013). Exercises FIGURE E.1 Schematic of a snowflake that shows the sharp points at the ends of each of its six arms. a. Calculate the molar volume of ice at 23oF. b. Convert 23oF into K. c. Calculate the percent increase of the vapor pressure of water at the end of one of the hexagonal tips at 23oF compared to a flat surface. d. What do the results of the calculation in (c) imply about the long-term stability of the shape of the snowflake assuming that the surface energy of ice is isotropic? 6.9 Ion implantation of helium in a particle accelerator deposits He interstitial atoms in a certain metal. If annealed, the helium atoms diffuse and form helium bubbles more or less uniformly throughout the metal thickness that cause the metal to swell and reduce its density to 0.95 of its original value (i.e., 5 volume percent porosity). When the porous metal is dissolved in acid, 2.26 cm3 at STP (standard temperature and pressure) of He is given off for each cubic centimeter of porous metal dissolved. Helium is quite insoluble in most metals, so assume that all the He given off was in bubbles and none was left in solid solution in the metal. Microscopic examination shows that the He bubbles are of a uniform size with a diameter of 0.5 micrometer. a. Calculate the He pressure in the bubbles. b. Calculate the surface energy of the metal. c. Is this a reasonable value? Why? d. How important is the assumption that all of the He evolved was in the bubbles? 6.10 The surface energy of poly(methyl methacrylate), PMMA, is γPMMA = 41.1 mJ/m2. (Sperling 2006). Water forms a contact angle, θ, of 71o on PMMA. a. Calculate the interfacial energy ( mJ/m2) between water and PMMA. b. 0.1 w/o sodium stearate, C18H35NaO2, a common surfactant, is added to the water and segregates to both the water–air and the water–PMMA interfaces and lowers both the interfacial energies by one-half when the concentration of sodium stearate goes from 0.01 to 0.1 w/o. Calculate the new contact angle in degrees. c. Calculate the bulk concentration of sodium stearate in mol/L. d. With the Gibbs adsorption isotherm, calculate the excess surface concentration of sodium stearate in mol/L. e. From (d), calculate the actual surface concentration of sodium stearate in mol/L. 6.11 Experimental data on interfacial properties of the Ni(liquid, m.p. = 1453 °C)-Al2O3(solid, m.p. = 2050oC) system at 1850o are the following (Kingery 1954): γLV(Ni) = 1480 mJ/m2; grain boundary groove dihedral angle for Al2O3 and air, φ = 151.8° (Figure 6.13); grain boundary groove dihedral angle for a grain boundary groove formed under liquid Ni, φNi = 166.4°; and the wetting angle of molten Ni on solid Al2O3, θ = 130°. From these data, calculate the following at 1850 °C: a. The alumina-Ni interfacial energy, γSL b. The alumina grain boundary energy, γGB c. The solid alumina surface energy, γSV 191 192 Chapter 6. Thermodynamics of Surfaces and Interfaces and Some Consequences rin h rout FIGURE E.2 A concave right circular cylinder with a constant external radius of curvature, rout, and an inner radius of curvature, rin, that varies along the height, h, of the cylinder. r 2,φ r1 φ r2,in r2 r2,out Center of toroid FIGURE E.3 Cross section through a toroid with a constant inner radius of curvature, r1, and an outer radius of curvature, r2φ , that varies with the angle from r2,in for φ = 0 to r2,out for φ = 180o. 6.12 Figure E.2 shows a concave circular cylinder with the following dimensions: h = 8 cm, rout = 6 cm is the radius of curvature of the vertical surface of the cylinder, and the diameter at the top = 5 cm. a. Calculate the inner radius of curvature at 0.5 cm intervals from the middle of the cylinder to the top (see Figure 6.8). b. Calculate the mean curvature at each of these points. 6.13 Figure E.3 sketches part of a toroid with an inner radius r1, the radius from the center of revolution of the toroid to the center of the circular part of the toroid, r2, the radius from the center of revolution to the inner surface of the toroid, r2,in, and the radius from the center of revolution of the toroid to the outer surface of the toroid, r2,out. Also is shown r2,φ = the second radius of curvature that must be normal to the surface. a. If r1 = 1cm and r2 = 10 cm, calculate r2,φ as a function of the angle φ for 0 ≤ ϕ ≤ π at 10o steps. b. From the results in (a), plot the mean curvature as a function of the angle φ for 0 ≤ ϕ ≤ π at 10o steps. c. From the results in (b), how would the shape of the toroid change if the temperature were high enough for atoms to move in response to the surface energy forces? REFERENCES Adamson, A. W. 1982. Physical Chemistry of surfaces, 4th ed. New York: Wiley. Adamson, A. and A. Gast. 1982. Physical Chemistry of surfaces, 7th ed. New York: Wiley-Interscience. Brandes, E. A. and G. B. Brook, eds. 1992. Smithells Metals Reference Book, 7th ed. Oxford: Butterworth-Heinemann. References Cammarata, R. C. 1994. Surface and interface stress in thin films. Progress in Surface Science. 46(1): 1–38. Cammarata, R. C. 1997. Surface and interface stress effects on interfacial and nanostructured materials. Materials Science and Engineering A237: 180–184. Casey, J. 1996. Exploring Curvature. Wiesbaden, Germany: Vieweg and Sohn. Cassie, A. B. D. and S. Baxter. 1994. Wettability of porous surfaces. Transactions of the Faraday Society. 40: 546–550. Chang, R. 2000. Physical Chemistry for the Chemical and Biological Sciences. Sausalito, CA: University Science Books. DeHoff, R. 2006. Thermodynamics in Materials Science, 2nd ed. Boca Raton, FL: CRC Press, Taylor & Francis. Evans, D. F. and H. Wennerström. 1999. The Colloidal Domain. New York: Wiley-VCH. Gaskell, D. R. 2008. Introduction to the Themrodynamics of Materials, 5th ed. New York: Taylor & Francis. Green, P. F. 2005. Kinetics, Transport, and Structure in Hard and Soft Material. Boca Raton, FL: Taylor & Francis. Haynes, W. M., editor-in-chief. 2013. CRC Handbook of Chemistry and Physics, 94th ed. Boca Raton, FL: CRC Press. Hiemenz, P. C. 1986. Principles of Colloid and Surface Chemistry, 2nd ed. New York: Marcell Dekker. Hudson, J. B. 1998. Surface Science. New York: Wiley. Humenik, M., Jr. and W. D. Kingery. 1954. Metal-ceramic interactions: III. Surface tension and wettability of metal-ceramic systems. Journal of the American Ceramic Society 37(1): 18–23. International Union of Pure and Applied Chemistry (IUPAC). 2014. Compendium of Chemical Terminology, Gold Book, Version 2.3.2. 2014-02-24. IUPAC. Kingery, W. D. 1954. Metal-ceramic interactions: IV. Absolute measurement of metal-ceramic interfacial energy and the interfacial adsorption of silicon from iron-silicon alloys. Journal of the American Ceramic Society 87(2): 42–45. Kingery, W. D. 1959. Surface tension of some liquid oxides and their temperature coefficients. Journal of the American Ceramic Society 45(1): 6–10. Kingery, W. D., H. K. Bowen, and D. R. Uhlmann. 1976. Introduction to Ceramics, 2nd ed. New York: Wiley. Laidler, K. J. 1993. The World of Physical Chemistry. New York: Oxford University Press. Larpkiattaworn, S. 1995. Oxidation Behavior of Al2O 3 -Cu Composites. MS Thesis. Colorado School of Mines. Golden, Colorado. Lee, J. 1984. Vapor Phase Sintering of Hematite in HCl. PhD Thesis. The Ohio State University, Columbus, OH. Miller, C. A. and P. Neogi. 1985. Interfacial Phenomena. New York: Marcell Dekker. O’Brien, T. E. and A. C. D. Chaklader. 1974. Effect of oxygen on the reaction between copper and sapphire. Journal of the American Ceramic Society 57(8): 329–332. Parikh, N. M. 1958. Effect of atmosphere on surface tension of glass. Journal of the American Ceramic Society 41(1): 18–22. Plueddemann, E. 1991. Silane Coupling Agents, 2nd ed. New York: Plenum Press. Ratke, L. and P. W. Voorhees. 2002. Growth and Coarsening. Berlin, Germany: Springer. Schwartz, M. M. 1990. Ceramic Joining. Materials Park, OH: ASM International. Shuttleworth, R. 1950. The surface tension of solids. Proceedings of the Physical Society A63: 444–457. Silbey, R. J. and R. A. Alberty. 2001. Physical Chemistry, 3rd ed. New York: Wiley. Sperling, L. H. 2006. Introduction to Physical Polymer Science, 4th ed. Hoboken, NJ: Wiley. Udin, H., A. J. Shaler, and J. Wulff. 1949. The surface tension of solid copper. Metal Transactions 1(2): 186–190. Wagner, C. 1961. Theorie der alterung von niederschlagen durch umlosen. Zeitschrift fur Elektrochemie 65(7–8): 581–591. Wang, Y., et. al. 2015. Evaluation of macroscale wetting equations on a microrough surface. Langmuir 31: 2342–2350. Wenzel, R. N. 1936. Resistance of solid surfaces to wetting by water. Industrial and Engineering Chemistry 28(8): 988–994. Wulff, G. 1901. Zur frage der geschwindigkeit des wachsthums und der auflösung der krystallflächen. Zeitschrift für Krystallographie und Mineralogie 34(5/6): 449–530. Yang, S., X. Jin, K. Liu, and L. Jiang. 2013. Nanoparticles assembly-induced special wettability for bio-inspired materials. Particuology 11: 361–370. Yeo, Y. 2007. Gas Corrosion of MgO Studied by Grain Boundary Grooving and Pore Smoothing. PhD. Thesis. Colorado School of Mines, Golden, Colorado. 193 7 Phase Transitions 7.1 7.2 7.3 7.4 7.5 7.6 7.7 7.8 Introduction Thermodynamics of Phase Transitions Rates of Phase Transformations Types of Phase Transformations Reconstructive Transformations 7.5.1 Silicates 7.5.2 Metals Transitions with Product Phases of Different Compositions 7.6.1 Nucleation and Growth Transitions 7.6.2 Spinodal Decomposition Nucleation and Growth 7.7.1 Introduction 7.7.2 Qualitative Description of Nucleation and Growth 7.7.3 Homogeneous and Heterogeneous Nucleation Homogeneous Nucleation 7.8.1 Critical Nucleus Size 7.8.2 Example of the Critical Nucleus Size for Water Condensation 7.8.3 Concentration of Critical Nuclei 7.8.4 Rate of Nucleation 7.8.4.1 Limitations 7.8.4.2 Nucleation of a Liquid or Solid from a Gas 195 197 197 199 202 202 202 203 205 205 205 206 206 207 208 208 208 210 211 212 212 212 196 Chapter 7. Phase Transitions 7.8.4.3 7.8.4.4 7.9 7.10 7.11 Nucleation of a Liquid from a Supersaturated Gas Example: Nucleation of Water Drops from Gas at Equilibrium at 300 K by Supersaturation 7.8.4.5 Example: Nucleation of Water Drops from Gas at Equilibrium at 300 K by Supercooling 7.8.5 Homogeneous Nucleation of Solids from Liquids and Solids from Solids 7.8.6 Overall Rate of Phase Transformation Heterogeneous Nucleation 7.9.1 Examples 7.9.2 Modeling Heterogeneous Nucleation Displacive Transformations 7.10.1 General Concepts 7.10.2 Zirconium Oxide 7.10.3 Barium Titanate 7.10.4 Martensite in Steels 7.10.5 Shape Memory Alloys Glass Transition 7.11.1 Introduction to the Glass Transition 7.11.2 Thermal Expansion 7.11.3 Short-Range and Long-Range Order 7.11.4 Viscosity 7.11.5 The Glass Transition Temperature, Tg 7.11.6 Viscoelastic Behavior 7.11.6.1 Material Differences 7.11.6.2 Some Viscoelastic Behavior 7.11.7 A Free Volume Approach to the Glass Transition 7.11.7.1 Free Volume 7.11.7.2 Free Volume and Tg 7.11.7.3 Volume Viscoelastic Behavior 7.11.7.4 Free Volume Relaxation 7.11.8 Glass Viscosity and Urban Legends 7.11.8.1 The Legends 7.11.8.2 Dispelling Legend One 7.11.8.3 Dispelling Legend Two 7.11.9 The Challenger Disaster and the Glass Transition 213 213 215 217 217 220 220 220 223 223 225 226 227 228 229 229 231 233 234 235 236 236 238 240 240 241 241 242 244 244 244 245 246 7.2 Thermodynamics of Phase Transitions 7.12 Particle Size and Phase Transitions 7.13 Chapter Summary Appendix Exercises References 7.1 247 248 249 250 252 INTRODUCTION One of the goals of this chapter is to describe and model the kinetics of different types of phase transformations including changes in state. The primary focus will be the types of phase changes or phase transitions that occur in solids. The largest number of phase transformations in all materials occur by a nucleation and growth process that is easy to understand and can be simply modeled in detail to predict the effects of times and temperatures on the extent of the phase transformation. Both homogeneous and heterogeneous nucleation are covered in this chapter. Heterogeneous nucleation is more import in real materials but homogeneous nucleation is easier to model and readily leads to the heterogeneous model. Spinodal decomposition is described qualitatively here relative to phase equilibria with the detailed kinetic model development relegated to Chapter 16. The other major type of phase transformation is the so-called diffusionless or displacive transitions that occur primarily in crystalline metals and ceramics. These are also referred to as martensitic transformations and have been studied extensively in metals primarily because of the hardening effect martensite has in steels. Here, the phenomenon will be discussed more qualitatively and described for several materials systems of technical importance. Finally, the glass transition is discussed, a topic of major importance in polymers, many inorganic elements and compounds, and some metals. A simple free-volume model for the glass transition is presented that makes a strong plausibility argument for many features of the glass transition. The chapter includes a description of the Challenger space shuttle accident whose proximate cause was the glass transition or brittle transition in the solid booster rocket polymer seals. Finally, particle size effects on phase transitions are discussed. 7.2 THERMODYNAMICS OF PHASE TRANSITIONS Frequently in kinetics of materials, the interest is in the rate of a transformation, or a phase change, of phase alpha, α, to a phase beta, β. These transformations or transitions include changes of state— solid, liquid, or gas—as well. Examples of phase transformations or phase transitions in single and multicomponent systems include ª ª ª ª ª ª Polymorphic (allotropic) transformation: structure 1 ⇒ structure 2; for example, white tin ⇒ gray tin Solidification; liquid ⇒ crystal; for example, freezing of copper Crystallization; glass ⇒ crystal; for example, crystallization of amorphous Si or polyethylene; devitrification (crystallization) of a silicate glass Condensation; gas ⇒ liquid; for example, rain Condensation; gas ⇒ solid; for example, snow Recrystallization; strained solid ⇒ strain-free solid; for example, rolled Cu 197 Chapter 7. Phase Transitions Gibbs energy, G 198 ª ª ΔGα−β Gelation: liquid ⇒ gel; for example, polymer plus liquid; cell walls Precipitation: liquid or solid ⇒ solid; for example, Fe3C in Fe-C alloys Gβ In general, for any of these phase transitions to occur, the Gibbs energy of the product phase(s) must be lower than that of the reactant phase(s) Gα as shown schematically in Figure 7.1. Figure 7.2 shows the Gibbs energy Temperature versus temperature for zinc liquid and zinc vapor and Figure 7.3 shows FIGURE 7.1 Gibbs energy for two phases undergoing the Gibbs energy versus temperature for liquid, solid, and gaseous H O 2 a phase transformation from α to β. Te is the equilibrium calculated from thermodynamic data (Roine 2002) as two examples for temperature. real materials. In both cases, the phase with the lowest Gibbs energy at a given temperature is the equilibrium state. Note that in both of these examples, ∆G = ∆G° since all of the phases are in their standard states—activity of the solid and liquid = 1.0 and pressure of the gas = 1 bar. If the Gibbs energy ∆G oα →β is negative, then the reaction is thermodynamically favorable. However, it may or may not take place depending on the details of the kinetics of the phase transition or phase transformation—as it is frequently referred to. If the reaction does take place, how fast it happens depends on the details of the kinetics of the phase transition. In this chapter, the rates of phase transformations controlled by a surface reaction are considered. Similar results hold for diffusion-controlled reactions modeled in Chapters 8 to 16. Diffusion control is the more important of the two processes for the high temperature transformations involving hard materials—metals, ceramics, and electronic materials—compared to polymers and some biomaterials, which are considered soft materials. The low temperature limitation of these materials frequently leads to a reaction controlling the rate of phase transition. Te −50 Zn(g) = Zn(l) −60 ΔG° Gibbs energy (kJ/mol) −70 −80 Zn(l) −90 −100 Zn(g) −110 Tbp = 907°C Lit = 907°C −120 750 800 850 950 1000 900 Temperature (°C) 1050 1100 1150 FIGURE 7.2 Gibbs energy versus temperature for zinc liquid and zinc vapor. (Data from Roine 2002.) Tbp is the boiling point at the intersection of the two lines and it is the value of the boiling point given in the literature, for example, Emsley (1998). 7.3 Rates of Phase Transformations −270 −280 H2O gas Gibbs energy (kJ/mol) −290 H2O(s,l) = H2O(g) ΔG° −300 Solid −310 Liquid −320 Gas −330 Tmp −340 −150 −100 −50 0 Tbp 50 100 Temperature (°C) 150 200 250 FIGURE 7.3 Gibbs energy versus temperature for liquid, solid, and gaseous H2O. The dashed lines are the extrapolation of the data for the liquid and solid states beyond their region of stability. Note that the phase with the lowest Gibbs energy at any temperature is the stable phase. (Data from Roine 2002) 7.3 RATES OF PHASE TRANSFORMATIONS The primary interest here is to develop an understanding of the rates of various phase transformations. However, it is impossible to cover all types of phase transitions completely. Only the nucleation and growth process is examined in detail since it can be controlled by both surface reactions, that have been examined earlier, and diffusion, and thus applies to a wide spectrum of materials and transitions. Furthermore, it is the most common type of transformation and has important technological implications. To put things in perspective, it is instructive to examine the iron–carbon system—steels—since the kinetics of phase transformations in this system have been studied exhaustively, not only to develop a better understanding of phase transitions or transformations but also, and perhaps more importantly, to produce heat treatment procedures that are used to optimize the properties of a given steel: very important to the industrial materials engineer. As emphasized earlier, materials science and engineering essentially began when the relationships between the chemistry, processing, microstructure, and properties of steel became the focus of the materials engineer. Boiler explosions and bridge collapses were a major impetus for achieving a better understanding of the mechanical properties of steel. By the early 1900s, a reasonably good understanding of these relationships had been developed. Furthermore, this system exhibits several phase transformations that are important commercially. The iron–carbon system up to Fe3C, cementite, is given in Figure 7.4 (Brandes and Brook 1992). Figure 7.5 gives the time–temperature–transformation (TTT) diagram for this steel (American Society for Metals 1973). This TTT diagram is for 1080 steel—which is almost the eutectoid composition in Figure 7.4—where the alloy is heated into the single-phase austenite region and then rapidly cooled into the two-phase ferrite + cementite field and held at a fixed temperature while the austenite Þ ferrite + cementite phase transformation occurs. This is an isothermal transformation diagram in that the data are taken by 199 Chapter 7. Phase Transitions 1300 1200 Liquid +δ Austenite, FCC, γ 1100 Liquid l + Fe3C 1000 Temperature (°C) 900 Austenite + cementite 800 α+γ 700 Ferrite, BCC, α Ferrite + cementite 600 500 0.77 w/o C 400 300 0 Cementite, Fe3C, 6.7 w/o C 4.32 w/o C 0.5 1.0 1.5 2.0 2.5 3.0 3.5 4.0 4.5 5.0 5.5 6.0 6.5 Weight percent carbon FIGURE 7.4 Part of the iron–carbon diagram after Brandes and Brook 1992. 800 700 Temperature (°C) 200 Austenite, A 727°C A 600 Ferrite, F + cementite, C 500 A+ F+ 400 300 Austenite, A C Start Finish 200 MS ∼Mf 1 10 102 103 104 105 106 Time/seconds FIGURE 7.5 Part of the isothermal transformation (TTT) of 1080 steel after American Society for Metals 1973. MS is the temperature at which martensite begins to form and Mf is the temperature at which martensite formation stops. cooling rapidly from above the As temperature 727°C (austenite, γ-iron-C alloy, face-centered cubic [FCC] lattice) to some temperature—say 650°C—and then holding at this temperature and observing when the presence of the ferrite (α-iron, body-centered cubic [BCC]) and cementite (Fe3C) first start to appear in the microstructure. This is the leftmost C-shaped curve in the diagram, which shows that this will occur in about 7 seconds at this temperature. The phase transformation continues and finishes at the intersection with the final curve in about 1 minute. The utility of the TTT diagram for steel is that it defines the time and temperature necessary to attain a certain microstructure, which in turn predicts the mechanical properties of the resulting heat-treated steel. Such diagrams are of great practical importance to the practicing industrial materials engineer. This transformation is a classic example of a nucleation and growth transformation in that at some point below the equilibrium temperature, TE = 727°C, at some locations in the austenite, the new phases will start to form. These locations are the nuclei—or the beginning sites for the new phase(s)—that then grow to completely transform the solid as shown schematically in Figure 7.6, for the more general case of alpha phase transforming completely to beta phase. 7.3 Rates of Phase Transformations β 201 β β α (a) α (b) (c) FIGURE 7.6 Schematic showing the stages in a nucleation and growth phase transition for the transformation of α to β for times (a) t ≅ 0, (b) 0 < t < ∞, and (c) t = ∞. Referring again to Figure 7.1, above an equilibrium temperature, TE , alpha is the stable phase and below TE , beta is the stable phase. So below TE in a transformation from α to β, there is a negative Gibbs energy change; that is, ΔG α-β = G(β) − G(α). Although the Gibbs energy of β is lower than that of α, the phase transformation does not occur instantly. Most phase transformations require a density or composition change and the generation of some phase interface surface energy all of which require either a diffusion process or a surface reaction or both (and sometimes heat transfer) that take time. In addition, the formation of a second phase, beta, requires that the new phase starts somewhere in the old phase, alpha. These particles of the new phase, perhaps very small containing only tens or hundreds of atoms, are the nuclei of the new phase. Even though the new phase is thermodynamically more stable, these nuclei have a surface or interfacial energy that needs to be overcome before they are stable and can grow. Once the stable nuclei of the second phase are formed, they grow by either a diffusion control or surface reaction control (Chapter 5), eventually transforming all of the original alpha to beta. As noted earlier, nucleation and growth is a major mechanism of phase transformations of interest in materials science and engineering. Figure 7.7 shows the nucleation and growth of silicon crystals in an amorphous thin film of silicon. Now, nucleation can be either homogeneous or heterogeneous. Homogeneous nucleation is the process where the small nuclei form spontaneously throughout the bulk of the material undergoing the phase change. In reality, homogeneous nucleation is hard to achieve in practice but it is easier to model. In contrast, heterogeneous nucleation is more common and it occurs when the new phase forms on particles of dust or another phase that allows the nucleus to lower its interfacial energy thereby allowing the nucleus to form more easily. Therefore, heterogeneous nucleation is the process where the small, stable particles of the new phase are formed at the interface with another phase (could be the free surface) that lowers the interfacial energy of the nuclei. An important example of heterogeneous nucleation is the process of cloud seeding with silver iodide, AgI, smoke particles that act as heterogeneous nuclei for ice formation, which will ultimately lead to rain (hopefully) during drought. Another classic and visual result of heterogeneous nucleation is the intentional production of crystalline glazes on ceramic art pieces where the heterogeneous nuclei are dust particles or small pieces of the kiln—furnace—insulation that fall onto the glaze surface serving as heterogeneous nucleation sites for crystals (Figure 7.8). The large round areas are the crystals of willemite, Zn 2SiO 4, that have grown out of the glaze. Notice the deeper coloration of the crystals com1 μm pared to the glass glaze. This is due to the optical absorption of electrons in the d-shells of transition metal ions, such as cobalt, that have FIGURE 7.7 Crystallization of an amorphous thin film of different optical absorption characteristics depending on their local silicon by a nucleation and growth phase transition. The electronic environments—number and proximity of anions—that are gray area is the glass and the white and black regions are different in the crystal and glass. crystals or grains of silicon. (Roy 2001) 202 Chapter 7. Phase Transitions In Chapter 5, growth processes controlled by surface reactions are analyzed. Now the process of nucleation is modeled and the two processes combined to demonstrate how nucleation and growth process controls the rate of phase transformation in materials. Nucleation and growth is not the only path by which phase transformations can occur. Another important one is spinodal decomposition that will be modeled in Chapter 16. 7.4 TYPES OF PHASE TRANSFORMATIONS There are several different terms that are used, sometimes loosely, to describe different phases that might be undergoing a phase transition or transformation. These include the following examples: FIGURE 7.8 Crystalline glaze vase from Taiwan on which large acicular crystals of zinc silicate, willemite, have grown from the glass by heterogeneous nucleation and growth. ª ª ª States of matter: Solid, liquid, and gas. Allotropes: Different forms (usually crystal structures) of an element: for example, tetragonal (white) and diamond cubic (gray) tin; BCC and FCC iron; O2 and O3 gas; amorphous and crystalline silicon. Polymorphs: Different crystal structures of the same compound or element: for example, white and gray tin (also allotropes); cubic, monoclinic, and tetragonal ZrO2. In general, there are two kinds of phase transitions in crystalline solids that involve only changes in crystal structure and not composition: (1) displacive or diffusionless transitions and (2) reconstructive or diffusion-controlled transitions. These can occur in both single and multicomponent systems. For both, the phase transition takes place by a nucleation and growth process. However, the growth or speed of the new phase interface in displacive or diffusionless transitions is roughly the speed of sound. As a result, the controlling kinetics are neither a surface reaction nor diffusion but perhaps the motion of dislocations. Furthermore, this rapid rate of transformation is difficult to study experimentally and results in a less than satisfactory understanding of the kinetic details of diffusionless transitions. Several important displacive transformations are presented later without any attempt to model their kinetics. 7.5 RECONSTRUCTIVE TRANSFORMATIONS 7.5.1 SilicateS In reconstructive transformations, atoms must diffuse to different positions in order for crystal structures to change. Figure 7.9 shows a schematic and purely hypothetical example for a silicate structure that goes from a ring arrangement of the SiO 4− 4 tetrahedra into a chain structure by a reconstructive transformation as well as a displacive transformation through a simple rotation of tetrahedra. Clearly, bonds must be broken and ions must diffuse to make the reconstructive structural change but not the displacive one. As a result, reconstructive transformations take time to occur and rapid cooling below the equilibrium temperature may prevent the transformation from taking place at all. The kinetics of these transformations is controlled by a nucleation and growth process. Figure 7.10 shows the various reconstructive and displacive phase transformations that occur for pure silica, SiO2 (Kingery et al. 1976).* In firing traditional ceramic porcelains that contain * There are references in the literature to several other displacive transformations in both tridymite and cristobalite but without unanimous agreement (Eitel 1954; Sosman 1965; Wells 1984). 7.5 Reconstructive Transformations Chain SiO−4 tetrahedron Reconstructive Ring e civ pla D is Ro tat ion s FIGURE 7.9 Schematic showing how displacive and reconstructive phase transformation take place in −4 silicates where the SiO 4 tetrahedral share corners. β-quartz hexagonal 870°C 573°C α-quartz trigonal β-tridymite hexagonal 1470°C 117°C α-tridymite triclinic β-cristobalite cubic 1705°C 270°C α-cristobalite cubic Molten SiO2 Tg ≅ 1200°C SiO2 glass FIGURE 7.10 Phase transformations in SiO2. The horizontal transformations are reconstructive while the vertical lines indicate displacive transformations. The glass transition temperature is included as well. (Eitel 1954, Wells 1984, Sosman 1965) silica as a filler material, depending on the firing temperature and time—a reconstructive phase transition is involved—since quartz, cristobalite, or tridymite (or some of each) is present in the final fired piece. All of these phases undergo displacive phase transitions on cooling with volume changes that can lead to internal cracking that either lowers the strength or actually causes cracking of the fired ceramic piece (or ware). 7.5.2 MetalS Titanium goes from a hexagonal crystal structure to BCC at about 900°C. And one of the classic examples, is that of white tin—tetragonal—going to gray tin—diamond cubic below room temperature with about a 21% increase in volume (Brandes and Brook 1992). Figure 7.11 shows the calculated Gibbs energies for white and gray tin predicting a phase transformation temperature of about 25°C although the actual observed temperature is considerably lower, about 13.2°C 203 Chapter 7. Phase Transitions −11 −12 Gibbs energy (kJ/mol) 204 Gray Sn: diamond cubic ΔG° White Sn: tetragonal ΔV = 21% −13 −14 −15 −16 TE = 25°C Tlit = 13.2°C −17 −50 −40 −30 −20 −10 0 10 20 30 40 50 Temperature (°C) FIGURE 7.11 Free energies of gray and white tin versus temperature. (Data from Roine 2002) White Gray FIGURE 7.12 White tin undergoing the very destructive phase transformation to gray tin—tin pest— at −40°C. (Frame from YouTube video: http://www.youtube.com/watch?v=sXB83Heh3_c uploaded by http://www.periodictable.ru.) (Roine 2002). The difference is probably caused by uncertainties in the thermodynamic data since it is very difficult to get bulk samples of gray tin to measure properties such as heat capacity necessary for accurate values of the Gibbs energy. Figure 7.12 shows how disruptive this transition can be at −40°C. It took about 20 hours for this roughly 1.5 in. long bar of white tin to completely transform—the markers are 1 cm. This loss in mechanical integrity is known as tin pest or tin plague and was observed to occur in tin buttons and on organ pipes in churches after a very cold winter in Russia in 1850 (Emsley 2001). Tin pest has been cited—perhaps apocryphally—as one of the determining factors in the defeat of Napoleon in the Russian winter of 1812. In June of 1812, Napoleon marched into Russia with an army of about 690,000. In September of that year he entered Moscow, which, shortly thereafter was burned to the ground by the Russians in what is known as a scorched earth policy, denying the enemy access to captured buildings, materiel, and food. Not having shelter, the French army left 7.6 Transitions with Product Phases of Different Compositions Moscow in October and started to return to France. Deprived of supplies, by December 14, 1812, the remaining 22,000 of Napoleon’s troops were forced out of Russian territory (French Invasion of Russia). Moscow can become bitterly cold in the winter and while records indicate that the winter of 1812 was not that cold during most of the retreat (the temperature did not go much below about 10°C), there were periods where the temperature dropped below 0°C. This led to one of the great stories in materials science that one of the factors that impacted Napoleon’s defeat in Russia was that his troops’ uniform buttons were made of white tin which underwent the white–gray transition leading to degradation and powdering of the tin. As a result, the French troops were supposedly too busy holding up their pants to reload their muskets and, as a result, lost the war! This serves as another example of the critical role that materials have played—and continue to play—in world history! This is a nice story, but not very likely to be true. It is suggested that any tin buttons made at that time were likely to have been impure and less likely to transform than pure tin (tin pest). Furthermore, the transformation takes place more rapidly the lower the temperature below the transformation temperature and during most of French army’s time in Russia, the temperature was not that low for long periods of time. Perhaps even more convincing is the evidence that the buttons on the French troops were actually made of bone and those of the officers were made of brass! (Emsley 2001). In contrast, there is strong evidence that Robert Scott’s expedition to the South Pole in 1910–1912 was a disaster partly because the cans of kerosene that were left behind for the return trip were found to be empty. These cans were soldered with tin and it has been suggested that tin pest caused the soldered joints to leak leaving no fuel to be used to provide heat for the expedition members who all subsequently froze (Emsley 2001; Tin Pest). 7.6 TRANSITIONS WITH PRODUCT PHASES OF DIFFERENT COMPOSITIONS 7.6.1 NucleatioN aNd Growth traNSitioNS Some phase transitions discussed above occur in multicomponent solids where there is no change of composition over large distances, only a change in structure. However, many phase transformations of interest in materials science and engineering are of the type where a single phase of a given composition decomposes into two or more other phases of quite different compositions. The decomposition of austenite to ferrite plus cementite in steels is a primary example of such a system. As a result, diffusion must be one of the series steps in the transformation in order to achieve the large changes in concentrations among the phases involved. Figure 7.13 schematically depicts a two component system with a complete solid solution, α, that decomposes to γ and β at the eutectoid temperature. If an alloy of composition x0 is rapidly cooled from the solid solution region at temperature T1 to a temperature T2 , precipitation of β can occur having a composition x β while α will equilibrate at composition x α . This will occur by a nucleation and growth process that involves diffusion and possibly a surface reaction. For hard materials, at high temperatures, diffusion is likely the rate-controlling step. However, for soft materials or at low temperatures, surface reaction may very well control the overall rate of decomposition. Nucleation and growth is described in detail shortly. 7.6.2 SpiNodal decoMpoSitioN In contrast to nucleation and growth, certain multicomponent phase transitions can occur by a process called spinodal decomposition in which there is no sharp interface developed by the new phases, although the process is controlled entirely by diffusion. Figure 7.14 schematically shows a system that can undergo spinodal decomposition. If an alloy of composition x0 is cooled from the γ solid solution range down to Te and held there to allow the reaction to take place, x 0 will decompose into the equilibrium compositions x1 and x 2 . This process takes place entirely by diffusion 205 Chapter 7. Phase Transitions Liquid, l Temperature (°C) α+ l T1 α β+α T2 α+γ β γ β+γ A xβ x0 xα m/oB B FIGURE 7.13 A schematic binary eutectoid system in which a complete solid solution, α, of composition X0 at T1 precipitates β of composition Xβ at T2 with accompanying change in α to Xα . Liquid Liquid + γ Temperature (°C) 206 γ Te γ1 + γ2 γ1 A x1 x0 m/oB γ2 x2 B FIGURE 7.14 Schematic phase diagram in which a solid solution alloy of composition X0 undergoes phase separation into new compositions X1 and X2 at temperature Te. with the concentration of B atoms increasing in γ2 and the concentration of A atoms increasing in γ2 but without the formation of an initial sharp interface between the two new phases. Since spinodal decomposition occurs entirely by diffusion in a thermodynamically nonideal system, a more complete analysis will be left to Chapter 16 after some discussion about diffusion in thermodynamically nonideal systems. 7.7 NUCLEATION AND GROWTH 7.7.1 iNtroductioN Since the nucleation and growth process of phase transformations can be controlled by a surface reaction, it is useful to model the process since all of the tools necessary for the development of the model have been discussed in Chapters 2, 4 and 6. It should be noted, however, that diffusion can also control the rate of a nucleation and growth process and so the process can be analyzed in terms of 7.7 Before going into the mathematical details of the nucleation and growth process, it is useful to examine qualitatively features of the transformation process that leads to TTT kinetics and diagrams, such as Figure 7.5, that have been developed extensively for steels. Figure 7.15 shows the rate of growth and the rate of nucleation as a function of temperature below the equilibrium temperature, Te, where the new phase(s) is the thermodynamically stable phase. Recalling the results from Chapter 5, the rate of growth is a product of a thermodynamic term that gets larger more or less linearly as the temperature decreases below Te. This term is multiplied by the kinetic factor that exponentially decreases with temperature because of the activation energy for the reaction. The product of the two gives the shape of the curve shown in Figure 7.15 with a maximum in the growth rate at some temperature below Te. As will be seen, similar considerations lead to a nucleation rate that also goes through a maximum at some temperature below Te—also the product of a thermodynamic term and a kinetic term. At Te, the nucleation rate must be zero since the thermodynamic driving force for the transformation must be sufficiently large to overcome the interfacial energy created with the formation of the new phase as well as any strain energy generated between the new phase and the matrix phase. The overall rate of the transformation is the product of the growth rate and the nucleation rate and leads to the curve shown in Figure 7.16, which also shows a maximum at some temperature below the equilibrium temperature, Te. By choosing three temperatures as shown, the overall percent of the transformation as a function of time can be calculated and these are shown in Figure 7.17. These S-shaped or sigmoidal curves of percent transformed as a function of time are characteristic of a nucleation and growth transformation. By choosing certain percent transformed at the various temperatures, the time for this percentage can be read from these curves and a TTT curve can be constructed as shown in Figure 7.18. Nucleation rate Rate FIGURE 7.15 Schematic drawing of the rates of growth and nucleation for a nucleation and growth phase transformation as a function of temperature below the equilibrium temperature Te where the new phase is stable. Te T1 T2 T3 Percent transformed r3 Rate r2 FIGURE 7.16 Schematic drawing of the overall rate of phase transformation as a function of temperature (product of the nucleation and growth rates of Figure 7.15) with three temperatures T1, T2, and T3 chosen to construct a time–temperature– transformation (TTT) diagram. 90 T3 Overall rate of transformation r1 100 T2 207 Growth rate Temperature (°C) 7.7.2 Qualitative deScriptioN of NucleatioN aNd Growth Te Temperature (°C) diffusion control as well. Diffusion control and reaction control essentially lead to similar results with minor changes in the meaning and values of some of the parameters of the process. Therefore, the nucleation and growth process is examined here assuming that surface reactions are the rate controlling steps. Nucleation and Growth T1 50 10 0 Time FIGURE 7.17 Percent transformed for the three temperatures of Figure 7.16: one above the maximum rate, T1; one at the maximum rate, T2; and one below the maximum rate, T3. Chapter 7. Phase Transitions Te Temperature (°C) 208 T1 Phase α α+β T2 Phase β 90% T3 10% Time FIGURE 7.18 TTT diagram drawn from the percent transformed versus time curves of Figure 7.17. 7.7.3 hoMoGeNeouS aNd heteroGeNeouS NucleatioN Nucleation and growth processes require the formation of a stable nucleus of the new phase that then grows to complete the phase transition. A nucleus is a stable small particle of the new phase consisting of only a small number of atoms or molecules—hundreds or so—whose Gibbs energy decreases when it grows. Homogeneous nucleation occurs when nuclei form throughout the bulk of the material because the interfacial and strain energies of the new phase are overcome by the Gibbs energy of the transformation. Heterogeneous nucleation occurs when the nuclei form at some surface or interface where the interfacial and strain energies of the nucleus are lower for a given size nucleus compared to what it would be if the nucleus were forming in the bulk of the material transforming. Hopefully, this distinction between homogeneous and heterogeneous nucleation will become clearer as these two processes are explored more fully below. In reality, homogeneous nucleation is very hard to achieve because of the usual presence of interfaces or impurity particles that can serve as sites for heterogeneous nucleation. However, homogeneous nucleation is somewhat easier to understand and it is modeled first. Going from homogeneous to heterogeneous nucleation is relatively straight forward and relies on the relationships between the relative interfacial energies discussed in Chapter 6. 7.8 HOMOGENEOUS NUCLEATION 7.8.1 critical NucleuS Size For a nucleus of new phase to form, not only must the volume Gibbs energy, ΔGV, be favorable for the formation of a new phase—ΔGV must be negative—but must be sufficiently large to overcome the new interfacial energy of the nucleus (and perhaps strain energy in a solid). Below the equilibrium temperature, Te (or above an equilibrium vapor pressure), where the energy to form the new phase is negative, atomic or molecular fluctuations within the transforming phase form embryos of the new phase where an embryo is a small cluster of atoms or molecules that form randomly and spontaneously throughout the bulk of the transforming phase. For a spherical embryo—another shape could be chosen but does not change the principles of the argument—of radius r, the Gibbs energy of the embryo is ΔGr is ∆G r = 4 3 πr ∆G V + 4πr 2 γ 3 (7.1) where the first term is the volume energy for the transformation for a spherical particle and is negative below some equilibrium temperature, Te, since ΔGV—the Gibbs energy per unit volume for the transformation to the new phase—is negative (∆G V = ∆G V where ΔG is the molar energy for the 7.8 Homogeneous Nucleation Surface free energy Nucleus free energy ΔGr* Total free energy Free energy increases with growth Free energy decreases with growth r*, critical nucleus Volume free energy Nucleus radius FIGURE 7.19 The energy of a nucleus, ΔGr, as a function of the nucleus radius, r, showing: the surface term increasing with r2, the volume term decreasing with r3, and the net energy with a maximum at the critical nucleus size, r*. transition and V is the molar volume of the nucleating phase). In solids, ΔGv may contain a strain energy term determined by any differences in molar volumes and the elastic properties of the parent or matrix phase and the nucleus. In what follows, the strain energy will assumed to be zero since its value depends strongly on the specific system and the goal here is to keep the final results as general as possible. The second term in Equation 7.1 is just the surface energy associated with a spherical nucleus of radius r. As shown in Figure 7.19, the volume energy term is negative and varies as r3 while the surface energy term is positive and varies with r2, where γ is the interfacial energy between the new and old phases. The resulting sum leads to a maximum in ΔGr at the critical nucleus size, r*. This critical nucleus size is very important for the following reasons. If the radius of the embryo is less than the critical nucleus size, r*, then any increase in the size of the embryo leads to a net positive Gibbs energy change, and the embryo is unstable, cannot exist, and will disappear. However, if the embryo has a radius greater than r*, then any increase in size leads to a net negative change in Gibbs energy so this embryo becomes a stable nucleus for the formation of the new phase. The critical nucleus size, r*, is obviously obtained by differentiating the above equation and setting it equal to zero: d∆G r = 0 = 4πr *2∆G V + 8πr *γ dr (7.2) and leads to a value for the critical nucleus size of r* = − 2γ ∆G V (7.3) (which looks similar to the effect of surface energy of the Gibbs energy of a spherical particle that was seen in Chapter 6) and, of course, r* is positive since ΔGV is negative. This makes intuitive sense in that high surface energies lead to a much larger critical nucleus size and, if the surface energy term is small, then the critical nucleus size is small. It follows that, the Gibbs energy for the critical nucleus, ΔG r* , is obtained by substituting Equation 7.3 into Equation 7.1: 209 210 Chapter 7. Phase Transitions ∆G r* = 4 3 πr *3∆G V + 4πr *2 γ 3 2 4 −2γ −2γ ∆G V + 4π π γ 3 ∆G V ∆G V = 4 8γ 3 4γ2 G =− π ∆ + 4 π γ V 3 ∆G 3V ∆G 2V ∆G r* = − πγ 3 32 πγ 3 + 16 2 3 ∆G V ∆G 2V with the result ∆G r* = γ3 16 π . 3 ∆G 2V (7.4) 7.8.2 exaMple of the critical NucleuS Size for water coNdeNSatioN Consider the case of water vapor condensing as a liquid at 300 K. The reaction is H2O(g) = H2O(l); ΔGo Now, ΔG = ΔGo + RT lnK, and in this case, K = a( H 2O) L /p ( H 2O ) = 1/p ( H 2O ) where a(H2O)l is the activity of the H2O and of course is 1.0 for the pure liquid. At equilibrium, ΔG = 0, and ∆G ° pe ( H 2O ) = pe = e RT or ∆G o = RT ln pe so ∆G = RT ln pe − RT ln p and p ∆G = −RT ln pe (7.5) and dividing by the molar volume, VH2O gives ΔG V. Putting in some numbers for water at 300 K (Haynes 2013) r* = − = 2γ 2γ 2γV =− = ∆G RT ln ( p/pe ) ∆G V V ( )( 2 72 × 10 −3 J/m 2 18 × 10 −6 m 3/mol (8.314J/mol ⋅ K )( 300K ) ln ( p/pe ) ) leads to r* = 1.04 × 10 −9 m ln ( p /pe ) (7.6) where p/pe = supersaturation, often given by the symbol S. If p = pe then the supersaturation = 1.0% or 100% humidity. Note that if the supersaturation is 1.0, then the critical nucleus is infinitely large! Table 7.1 gives the critical nucleus size and the number of H2O molecules comprising it as a function of the supersaturation. Supersaturation for homogeneous nucleation can reach values on the order of 4.0 (Silbey and Alberty 2001) and would suggest that a nucleus at this supersaturation would contain 59 H2O molecules and would be about 1.5 nm in diameter. 7.8 Homogeneous Nucleation TABLE 7.1 Supersaturation of Water Vapor and Critical Water Nucleus Size p/pe 1.0001 1.001 1.01 1.1 1.2 1.3 1.4 1.5 1.6 1.7 1.8 1.9 2 3 4 5 6 7 8 9 10 r*(m) 1.040 × 10−5 1.041 × 10−6 1.045 × 10−7 1.091 × 10−8 5.704 × 10−9 3.964 × 10−9 3.091 × 10−9 2.565 × 10−9 2.213 × 10−9 1.960 × 10−9 1.769 × 10−9 1.620 × 10−9 1.500 × 10−9 9.466 × 10−10 7.502 × 10−10 6.462 × 10−10 5.804 × 10−10 5.345 × 10−10 5.001 × 10−10 4.733 × 10−10 4.517 × 10−10 Molecules 1.58 × 1014 1.58 × 1011 1.60 × 108 1.82 × 105 2.60 × 104 8.73 × 103 4.14 × 103 2.36 × 103 1.52 × 103 1.06 × 103 776 596 473 119 59.2 37.8 27.4 21.4 17.5 14.9 12.9 7.8.3 coNceNtratioN of critical Nuclei A chemical equation can be written for the formation of a critical nucleus of n atoms of species A: nA A n : ΔG r* (7.7) where An is the critical nucleus. If the assumption is made that the concentrations of atoms and critical nuclei are small so that the activities of each are the same as their mole fractions (as will be seen, this is a good assumption), an equilibrium constant can be written as ∆G * r − XA n k BT = e X An where: X A n is the mole fraction of nuclei of size n X A is the mole fraction of atoms (or molecules) A. Note that Boltzmann’s constant, kB, is used in the exponent rather than R since ΔG r* is the actual energy for just a few atoms and nuclei and not moles of them. For the sake of simplicity, consider a gas and let ηA = number of gas atoms/m3—about 1025 at STP—standard temperature and pressure— (one bar and 298 K) then ηr* = number of critical nuclei per m3. Assuming ηr* ηA (as will be seen to be true) so that: X An = XA = ηr * η* r ηr* + ηA ηA ηA η A = 1. ηr* + ηA ηA 211 212 Chapter 7. Phase Transitions Therefore, ∆G * r − ηr * = K e = e k BT ηA or the concentration of critical nuclei, ηr* , is ηr* = ηA e − ∆G * r k BT . (7.8) 7.8.4 rate of NucleatioN 7.8.4.1 Limitations Modeling of the nucleation rate is a little more difficult and, although there have been many attempts at doing this accurately over the past 100 years, the results are still somewhat unsatisfactory in that the models frequently differ from experiment by large amounts. Furthermore, the values of experimental parameters such as the accommodation coefficient, α, discussed in Chapter 5, may vary considerably in the literature. Nevertheless, the main methodology of these approaches is illustrated to give nucleation rates that are reasonable if not precise. The fact that the model does not predict exact numerical results is not critical. It is the modeled behavior of the nucleation rate, and the concepts involved, as a function of the experimental parameters, such as the supersaturation or supercooling leading to the formation of a new phase, that is instructive and essentially correct. 7.8.4.2 Nucleation of a Liquid or Solid from a Gas A very important conceptual point is that a critical nucleus will grow and become a stable nucleation site with the addition of only a single atom or molecule since the addition of the single atom or molecule to the critical nucleus will lead to a lower Gibbs energy (Figure 7.19). Therefore, the nucleation rate depends on how fast gas atoms can attach themselves to critical nuclei to make them grow and generate the phase transformation. It should be noted that several different symbols are used for nucleation rate in the literature including I, J, and N, among others. For the sake of being different and not using the same letter or symbol for a number of entities, here the nucleation rate is given by Θ, capital theta. For the case of a gas forming liquid or solid nuclei, this process can be approximated by (Reed-Hill and Abbaschian 1992) Θ = J ′A r * η r * (7.9) where: Θ is the nucleation rate with Units(Θ) nuclei/m3-s J′ is the atomic or molecular flux. Units(J′) = atoms/m2-s and J′ = NAJ where J is the molar flux density, Units(J) = mol/m2-s that was modeled earlier for first order gas–solid (or liquid) surface controlled reactions; A r* = the area of the critical nucleus Units(A r* ) = m2; and ηr* = the number of critical nuclei per unit volume, Units(ηr* ) = m−3, Equation 7.8. As was as shown in Chapter 5 for condensation from a gas J′ = α ( p − pe ) 2πmk BT where: α is the accommodation or sticking coefficient p is the pressure of the condensing gas pe is the equilibrium pressure of the condensing gas. (7.10) 7.8 Homogeneous Nucleation If α < 1.0 , this implies some sort of surface reaction must occur for the atoms or molecules to stick to the surface as discussed in Chapter 5. 7.8.4.3 Nucleation of a Liquid from a Supersaturated Gas Putting everything together, the rate of nucleation is given by ∆G * ( p − pe ) − k rT *2 Θ= α 4πr ηe B 2πmk BT ( ) (7.11) Or Θ = Θ0e − ∆G * r k BT (7.12) where ( p − pe ) Θ0 = 2πmk T B *2 α 4πr η ( ) and, from above, r* = − 2γ ∆G V and ∆G r* = 16 γ3 π . 3 ∆G 2V 7.8.4.4 Example: Nucleation of Water Drops from Gas at Equilibrium at 300 K by Supersaturation The reaction to form water droplets from a supersaturated atmosphere is H2O(g) = H2O(l). As mentioned in Section 7.8.2, homogeneous nucleation is observed when the supersaturation, S, S = p pe is about 4. At 300 K, pe(300 K) = 3.53 × 10−2 bar (Roine 2002). From Chapter 6, γ(H2O) = 72 mJ/m2; and the molar volume, V = 18 cm 3 mol 1 106 m 3 cm 3 = 18 × 10 −6 m 3 mol. The value for the accommodation coefficient for water and water vapor is somewhat uncertain and varies by about an order of magnitude or more (Pound 1972; Davidovits et al. 2004). The most likely value is some place between 0.4 and 1.0, so for the sake of calculation, a value of α ≅ 0.7, is used here. Some additional assumptions are made that simplify the calculations and do not make a major difference in the final result. Making the calculation for ΔG V to calculate Θ0, a constant supersaturation of S = 4.0 is used so that: ( ∆G V = − ∆G V = − ) RT ln ( p pe ) V (8.314 )( 300 ) ln 4 18 × 10 −6 (7.13) ∆G V = −1.92 × 108 J m 3 and for the critical nucleus radius, r* = − r* = 2γ ∆G V ( 2 72 × 10 −3 ) 1.92 × 108 r * = 7.5 × 10 −10 m (7.14) 213 214 Chapter 7. Phase Transitions which, from Table 7.1, is about 60 water molecules. It should be noted that the increase in the equilibrium pressure of water over drops this small, Chapter 6, has been neglected as well. But here again, this will not make a major difference the result. The area of the critical nucleus is then ( A r* = 4πr *2 = 4 ( 3.1416 ) 7.5 × 10 −10 ) 2 (7.15) A r* = 7.07 × 10 −18 m 2 . The number of H2O molecules in the gas phase, η is given by η= η= N A peS RT (6.022 ×10 23 )( )( ) atoms mol 3.53 × 10 −2 bar 106 cm 3 m 3 ( 4 ) ( ) 83.14 cm ⋅ bar mol ⋅ K ( 300K ) 3 (7.16) η = 3.45 × 1024 H 2O molecules m 3 and the Gibbs energy for the critical nucleus, ∆G r* = 16 γ3 π 3 ∆G 2V ( ( 72 × 10 −3 J m 2 16 ∆G r* = ( 3.1416 ) 3 1.92 × 108 J m 3 ) ) 3 (7.17) 2 ∆G r* = 1.69 × 10 −19 J and, finally, the value of Θ0, ( p − pe ) Θ0 = αA r* η 2πmk BT ( 4 − 1) 3.53 ×10−3 bar 105 Pa bar Θ0 = −3 18 × 10 kg mol −23 2 ( 3.1416 ) 6.022 × 1023 atoms mol 1.38 × 10 J attom ⋅ K ( 300K ) ( )( ) ( ( )( ) × ( 0.7 ) 7.07 × 10 −18 m 2 3.45 × 1024 atoms m 3 (7.18) ) Θ0 = 1.137 × 1034 nuclei m 3 ⋅ s leading to a nucleation rate of Θ = Θ0e ( − ∆G * r k BT ) Θ = 1.137 × 1034 e −1.6×10−19 (1.38×10−23 )( 300 ) Θ = 2.12 × 1016 nuclei m 3 ⋅ s . (7.19) 7.8 Homogeneous Nucleation 14 Nucleation rate (1016 m−3s−1) 12 300 K 10 8 6 4 2 0 1.0 1.5 2.0 2.5 3.0 3.5 Supersaturation, S 4.0 4.5 FIGURE 7.20 Nucleation rate of water drops at 300 K as a function of the supersaturation. The nucleation rate as a function of supersaturation is shown in Figure 7.20 where ΔG V was calculated as a function of supersaturation, S, from, ∆G V = − RT ln ( p pe ) RT ln S =− . V V (7.20) Notice in Figure 7.20 how rapidly the rate of nucleation rises with supersaturation. Also note that the number of nuclei per unit volume is much smaller (≈8 orders of magnitude) than that of the gas atoms, η = 3.45 × 1024 m−3. Finally, even such low concentrations of nuclei, ≈ 1016 m−3 implies that they are roughly only 5 µm distant from each other! 7.8.4.5 Example: Nucleation of Water Drops from Gas at Equilibrium at 300 K by Supercooling The Gibbs energy for the reaction H2O(g) = H2O(l) can be written: ∆G = ∆H vap − T∆Svap (7.21) where subscript vap refers to the enthalpy and entropy of vaporization. Now, if the supercooling is not too large (so the enthalpy doesn’t change much over the temperature range) then this equation can be written: ∆G = ∆H vap − T = ∆H vap TE ∆H vap ( TE − T ) TE where TE − T is the degree of supercooling and leads to the volume Gibbs energy for the transformation: ∆G v = ∆H vap ( TE − T ) TE V (7.22) where going from the gas to the liquid ΔHvap is negative and, of course T < TE. For water that is at equilibrium at 300 K (i.e., the water vapor pressure at 300 K is the equilibrium pressure for water and water vapor, S = 1 at 300 K), this leads to a supercooling of about 25°C or down to about 275. Again, to simplify the equation, the factors in Θ0, and Θ0 itself, are calculated assuming this degree 215 Chapter 7. Phase Transitions of undercooling. The factors in Θ0 are calculated as before for a fixed supersaturation of S = 4, with the only exception was that ΔGV calculated from the supercooling from Equation 7.22 with ΔHvap = 45 kJ/mol (Haynes 2013) and α = 0.7 again at ΔT = 25 K, ∆G v = ∆G v = ∆H vap ( TE − T ) TE V ( 45, 000 ) (25) ( 300 18 × 10 −6 (7.23) ) ∆G v = 2.08 × 108 J m 3 . Calculation of r* as in Equation 7.14 gives r * = 6.92 × 10 −10 m and so from Equation 7.15 Ar* = 5.96 × 1018 m2. Likewise, from Equation 7.16 η = 8.63 × 1023 molecules m −3 which is a factor of four smaller than in the case of supersaturation that was estimated to be about four. However, for supercooling to about 275 K, the equilibrium water vapor at this temperature is pe ( H 2O) ≅ 7 × 10 −3 atm which is about 0.2 of the equilibrium pressure at 300 K. So for all practical purposes, p(300) − p ( 275 ) ≅ 0.8p(300) ≅ p(300) = 3.53 × 10 −2 atm in Θ0. These values give from Equation 7.18 Θ0 = 5.99 × 1032. nuclei/m3∙s. Note that Θ0 does not include its variation with temperature. The reality is that this can be ignored given all the other approximations in the calculations. For example, 3/ 2 the fractional difference in Θ0 between 300 and 275 K is roughly, ( 275 300 ) ≅ 0.9 or only about a 10% difference that is clearly negligible given the other uncertainties in the terms of Θ0, particularly the value of the accommodation coefficient, α. And finally, from Equation 7.17 ∆G r* = 1.45 × 10 −19 J which gives a nucleation rate at 275 K from Equation 7.19 of Θ = 1.52 × 1016 nuclei m 3 ⋅ s . The nucleation rate versus temperature is plotted in Figure 7.21 with the temperature plotted vertically to correspond to the earlier plots during the qualitative discussion of nucleation and growth processes. It should be noted that since the accommodation coefficient, α, is assumed constant, the nucleation rates in Figures 7.26 and 7.27 constantly increase. However, if the accommodation coefficient were strongly temperature dependent because of the nature of the surface reaction, that is, α = α 0 exp( − Q/RT), then the nucleation rate would go through a maximum as the temperature decreases as shown in Figure 7.15. 300 295 290 Temperature (K) 216 285 280 275 270 0 10 20 30 Nucleation rate (1016 nuclei m−3 s−1) FIGURE 7.21 Nucleation rate versus temperature for water that is in equilibrium with its vapor at 300 K. 7.8 Homogeneous Nucleation 7.8.5 hoMoGeNeouS NucleatioN of SolidS froM liQuidS aNd SolidS froM SolidS For the nucleation of solids from liquids or solids from solids everything is essentially the same as described above for gas condensation to liquids (or solids) with the major difference in the terms in, and the more difficult interpretation of, Θ0. Here, Θ0 is determined by something close to a diffusion process since the atoms neighboring the critical nucleus only have to move one interatomic distance. Nevertheless, Θ0 in these cases could be interpreted similar to the above gas for gases, Equation 7.11; for example, ∆G * r − 1 Θ = vη α 4πr *2 ηe k BT 4 ( ) (7.24) where η is now the number of atoms per unit volume in the solid or liquid and all the other terms are defined as above with the exception of the mean speed, v. The atom speed, v can be interpreted as the speed of an atom moving roughly one interatomic distance from the surrounding liquid or solid to the nucleating solid. This is kind of like a diffusion process as will be seen in Chapter 8 in that the speed could be written as v= −Q distance ≅ a fe RT time where: a is the jump distance, roughly equal to an interatomic distance f is the frequency or how often a neighboring atom tries to jump and is essentially equal to the atomic vibration frequency, f ≅ 1012 s −1 Q is some activation energy the atom must have to make the jump from the liquid/solid to the solid nucleus. So Equation 7.24 could be written, ∆G * Q r − 1 − Θ = aη fe RT α 4πr *2 ηe k BT 4 ( ) and aη ≅ η2 3 roughly the number of atoms per unit area surrounding the critical nucleus. As a result, for solid nucleation, Q 1 − Θ0 ≅ η2 3 fe RT α 4πr *2 η. 4 ( ) (7.25) If the nucleation is controlled by a surface reaction, α could also be exponentially temperature dependent as well; if diffusion-controlled, α ≅ 1.0. In either case, Θ0 will be exponentially temperature dependent and the nucleation rate will go through a maximum as shown in Figure 7.15 for the nucleation of solids. 7.8.6 overall rate of phaSe traNSforMatioN Before discussing heterogeneous nucleation it is useful to model the relationships between nucleation and growth rates and the resulting overall rate of phase transformation. As described later, the results are the same whether the nucleation is homogeneous or heterogeneous the only difference being the rate of nucleation in the final expression. Figure 7.22 schematically depicts an initial volume V of phase alpha, α, undergoing a phase transformation to phase beta, β. The resulting model holds regardless whether the transformation is gas to liquid or solid, liquid to solid, or solid to solid as long as the transition is a nucleation and growth process. 217 218 Chapter 7. Phase Transitions β V β β β β β β β β β α FIGURE 7.22 Schematic showing a volume V of phase α transforming to phase β by a nucleation and growth process. Referring to Figure 7.22, let nβ = the number of β particles in V so that dnβ = Θ Vαdτ where: Θ is the nucleation rate dτ is a small change in time. Now the volume of a single β particle, vβ, is simply vβ = 3 4 3 4 π a = π ( G ( t − τ)) 3 3 where: a is the particle radius G is the growth rate = da/dt = constant (surface reaction) t-τ is the time the particle has had to grow since it was nucleated at time = τ. Therefore, the total change in the volume of the new phase β is given by dVβ = vβdnβ = 4 3 πVαΘ G 3 ( t − τ ) dτ. 3 But Vα = V − Vβ so that dVβ dVβ d( Vβ /V ) df t = = = Vα V − Vβ 1 − ( Vβ /V ) 1 − f t where f t is the volume fraction transformed. Combining these last two equations gives the differential equation that needs to be solved: df t 4 3 = πΘ G 3 ( t − τ ) dτ. 1 − ft 3 This is integrated to give—assuming Θ and G are constant: − ln (1 − f t ) = 4 πΘ G 3 3 t ∫ ( t − τ) dτ. 0 3 7.8 Homogeneous Nucleation Let z = t − τ so z3 = (t − τ)3, dz = −dτ, and when τ = 0, z = t, and when τ = t, z = 0. Therefore, the equation becomes 4 ln (1 − f t ) = − πΘ G 3 3 4 = − πΘ G 3 3 ∫ 0 z 3 ( −dz ) t t ∫ z dz 3 0 1 ln (1 − f t ) = − πΘ G 3t 4 3 and leads to ft = 1 − e − 13 πΘ G3t 4 . (7.26) which gives the fraction reacted as a function of time with the nucleation and growth rates as parameters. This is known as the Johnson–Mehl–Avrami–Kolmogorov (JMAK) equation having been derived in different fields of science and engineering: Robert Mehl was a metallurgist and onetime head of the then Metallurgy Department at what is now Carnegie Mellon University. This leads to the S-shaped or sigmoidal curves discussed in Section 7.7.2 and shown in Figure 7.23. From these curves, as was shown earlier, TTT curves can be obtained for the phase transformation. Note that for small values of the exponent since e−y ≈ 1 − y, so 1 1 f t ≅ 1 − 1 − πΘ G 3t 4 πΘ G 3t 4 3 3 (7.27) or for short times or small fractions transformed, f t ∝ t4. 1.0 0.9 Nucleation rate, I = 1015 m−3 s−1 0.8 Growth rate, G = 2.5 × 10−8 ms−1 Fraction transformed 0.7 0.6 0.5 0.4 0.3 0.2 0.1 0.0 0 10 20 30 40 50 60 70 80 90 100 110 120 130 140 150 Time/sec FIGURE 7.23 Fraction transformed as a function of time calculated for the growth and nucleation rates indicated. 219 Chapter 7. Phase Transitions 7.9 HETEROGENEOUS NUCLEATION 7.9.1 exaMpleS Heterogeneous nucleation occurs much more readily and much more often than homogeneous nucleation. Obvious examples are the formation of dew and frost long before any fog or ice crystals form in the air. From the ice crystal or frost patterns that form on the surface of an automobile, for example, it is clear that the ice crystals are forming on dirt particles, wipe marks, and other artifacts on the surface. Another common example is the formation of CO2 bubbles on the surface of a glass of beer, champagne, or soda. The bubbles emanate from specific sites on the glass that are either small surface defects—cracks or flaws—in the glass or—hopefully not—dirt particles. Heterogeneous nucleation is used in cloud seeding in which silver iodide, AgI, smoke particles are used to nucleate raindrops during drought periods. AgI has the hexagonal wurtzite, ZnS, structure with each anion and cation surrounded by four nearest neighbors satisfying each atom’s four covalent bonds in ABAB packing. The wurtzite structure is analogous to the hexagonal diamond structure—that exists under special conditions—in which both Ag and I are replaced by a C atom covalently bonded to four other C atoms. This is similar to the crystal structure of hexagonal ice (ice I), the stable crystalline form at one bar pressure and zero centigrade. The idea is to have nuclei of ice form heterogeneously on the AgI particles which later grow to serve as nuclei for raindrops. The similar crystal structures of hexagonal ice and hexagonal AgI minimize the interfacial energy between the ice nucleus and AgI particle, enhancing the nucleation by a heteroepitaxy process. 7.9.2 ModeliNG heteroGeNeouS NucleatioN The analysis of heterogeneous nucleation is a straightforward extension of homogeneous nucleation but with a reduction in the overall interfacial energies since the nucleus forms on/at another surface, as shown schematically in Figure 7.24. This figure shows a partial wetting of the new phase on the heterogeneous nucleus surface. For the sake of concreteness, assume that the new phase is liquid and the heterogeneous nucleus is solid but this does not restrict the model to only this case: it could also be liquid on liquid, solid on solid, liquid or solid on a free surface, and so on. Now the Gibbs energy of the nucleating phase, ΔGhet, is ∆G het = VL ∆G V + A LV γ LV + A LS ( γ LS − γ SV ) (7.28) where V L = the volume of spherical liquid cap, and the Ai are the areas of interest and the interfacial energies are those discussed in Chapter 6. Also, from Chapter 6, equating the x-components of the surface energies: γ SV = γ LS + γ LV cos θ. From the geometry in Figure 7.30, A LS = πr 2 sin 2 θ Liquid drop r (1 − cosθ) Solid surface θ r sinθ r cosθ r 220 θ FIGURE 7.24 Spherical cap of the heterogeneously nucleating phase forming on the free surface of a solid heterogeneous nucleation site that shows partial wetting of the surface by the new phase. 7.9 Heterogeneous Nucleation and A LV = A cap = 2πr 2 (1 − cos θ ) VL = Vcap = π 3 r 2 − 3 cos θ + cos3 θ 3 ( ) which are taken from the literature (Lipschutz et al. 2012). (But could easily be obtained by integration of the surface area and volume of the spherical cap.) Putting in these areas and volumes into the equation for ΔGhet, Equation 7.28 ∆G het = π 3 r 2 − 3 cos θ + cos3 θ ∆G V + 2πr 2 (1 − cos θ ) γ LV + πr 2 sin 2 θ ( γ LS − γ SV ) . 3 ( ) (7.29) Notice that if θ = 180°, cosθ = −1, and sinθ = 0, there is no wetting, the spherical cap now becomes a spherical drop resting on the surface and the equation for ΔGhet becomes ∆G het = 4 3 πr ∆G V + 4πr 2 γ LV 3 which is the equation for a spherical drop used for homogeneous nucleation. This is, of course, what it should be since with θ = 180° there is no wetting and reduction of surface energy by the presence of the solid particle and only homogeneous nucleation will take place. Substitution of the relationships between the interfacial energies, gives ∆G het = π 3 r 2 − 3 cos θ + cos3 θ ∆G V + 2πr 2 (1 − cos θ ) γ LV + πr 2 sin 2 θ ( − γ LV coos θ ) . 3 ( ) The rest is just algebra. Combination of the last two terms gives 2πr 2 (1 − cos θ ) γ LV + πr 2 sin 2 θ ( − γ LV cos θ ) ( ) = πr 2 2 − 2 cos θ − cos θ sin 2 θ γ LV ( )) ( = πr 2 2 − 2 cos θ − cos θ 1 − cos2 θ γ LV ( = πr 2 γ LV 2 − 3 cos θ + cos3 θ ) and finally ( 2 − 3 cos θ + cos θ) 3 = 4πr 2 γ LV (7.30) 4 while the first term can be written as ( ) 2 − 3 cos θ + cos3 θ 4π 3 r ∆G V . 3 4 (7.31) Combining Equations 7.30 and 7.31 gives the final, and desired result: ( 3 2 − 3 cos θ + cos θ 4π ∆G het = r 3∆G V + 4πr 2 γ LV 4 3 ) . (7.32) 221 Chapter 7. Phase Transitions The first term is simply the Gibbs energy for the homogeneous nucleus and the second term depends on the extent of wetting, θ. Therefore, as Equation 7.32 shows, the energy for the heterogeneous nucleus is the same as for the homogeneous nucleus times a function of wetting angle: ∆G het = ∆G hom f ( θ ) where f ( θ) = ( 2 − 3 cos θ + cos θ) . 3 4 As a result, the previous discussion about the critical radius and the implications for nucleation rate and the overall rates of transformation follow the exact same procedure as for homogeneous nucleation. The only difference is now the dependence of the wetting angle, f(θ), which is just a number for a given system that varies between zero and one. Figure 7.25 shows how f(θ) varies with theta and Figure 7.26 shows how the resulting nucleation rate varies with supersaturation or supercooling. Of course, if θ → 0, f(θ) → 0 and there is no barrier to nucleation and it proceeds without any supersaturation or supercooling. On the other hand, if θ → 180°, f(θ) →1 and nucleation proceeds by homogeneous nucleation. Similar relations can be developed for other situations of heterogeneous nucleation such as a new phase forming at grain boundaries in a polycrystalline material. In this case, as was discussed in Chapter 6, the shape of the particle at the grain boundary is just two of the spherical caps shown in Figure 7.24 back to back. So the areas, volumes, and total interfacial energies are somewhat different but lead to exactly the same result: ∆G het = ∆G hom f ( θ ) the only difference being that, now ( 2 − 3 cos θ + cos θ) f ( θ) = 3 2 1.0 0.8 0.6 f(θ) 222 0.4 0.2 0.0 0 20 40 60 80 100 120 140 160 180 θ° FIGURE 7.25 f(θ) versus θ for a heterogeneous nucleus with a wetting angle of θ as in Figure 7.24. Nucleation rate m−3 s−1 7.10 Displacive Transformations Heterogeneous Homogeneous Supercooling or supersaturation FIGURE 7.26 Effect of heterogeneous nucleation on the nucleation rate. where θ is one-half of the dihedral angle, φ, as shown in Figure 6.16 of Chapter 6 and can only vary from 0° to 90° and at 90° there is no wetting of the grain boundary and homogeneous nucleation proceeds. In most real systems, there is at least partial wetting of the grain boundary by second phase particles and precipitation of a new phase in polycrystalline solids typically takes place more readily at grain boundaries. 7.10 DISPLACIVE TRANSFORMATIONS 7.10.1 GeNeral coNceptS In a typical displacive transformation, a crystalline solid transforms to a crystalline solid of exactly the same composition but with a different crystal structure simply by shifting atoms, ions, or molecules to a different position within a unit cell, distorting it, and changing the cell’s crystallography as shown schematically in Figure 7.27. Such a transformation does not require movement of atoms, ions, or molecules by diffusion and therefore cannot be prevented by cooling rapidly through the phase transition temperature since there is nothing to restrict the small atom or molecule motion within the unit cell. As a result, they are also called diffusionless transformations. In fact, displacive transformations are cooperative transformations—sometimes called military transformations—in that atoms in neighboring unit cells essentially all move together mutually reinforcing their tendency to move causing the interface between the transformed and untransformed phase moving as fast as the speed of sound (Balluffi et al. 2005). These transformations are also frequently referred to as martensitic transformations after the FCC to body-centered tetragonal (BCT) martensite transformation that occurs at low temperatures in steels that gives a very high hardness to steel.* One feature of diffusionless transitions is the twinning † that occurs in the transformed phase to minimize the strain energy developed due to the difference in crystallography and volume between the two phases: Figure 7.28 illustrates this. Figure 7.29 is a transmission electron micrograph (Chiang 1988) of a grain of BaTiO3 with 0.05 mole additive of (Bi2O3 + Nb2O5) that form a solid solution with the BaTiO3 and prevent the cubic to tetragonal phase change, discussed below. In this figure, the additives have diffused from the grain boundary into the BaTiO3 grain around its edges keeping it cubic at room temperature. However, the center of the grain is still almost pure BaTiO3 and has undergone the cubic to tetragonal phase transition with the attendant twinning. The other features in the micrograph are stacking faults (determined by changing the diffraction conditions in the microscope and observing the changes in contrast) that consist of a missing plane in a sequence ABC|BCABC… * † Martensite is named after the German metallurgist Adolf Martens, 1850–1914. One way to represent a twin is the plane stacking sequence in a cubic-close-packed structure. Instead of ABCABCABC… stacking it becomes ABC|BCABCABC|BCABC…where the vertical lines represent the twin boundaries. 223 224 Chapter 7. Phase Transitions Cubic Tetragonal Temperature Stress Tetragonal Monoclinic FIGURE 7.27 Schematic of diffusionless or displacive phase transformations: cubic ⇔ tetragonal ⇔ monoclinic structures. Grain in cubic Displacive material transformation: very large strain energy Twinning: minimizes strain energy FIGURE 7.28 Cubic material undergoing a displacive transformation. To minimize the strain energy associated with the transformation, the transformed grain forms twins. Stacking fault Twinned tetragonal BaTiO3 0.5 μm Grain boundary Cubic BaTiO3 FIGURE 7.29 Transmission electron micrograph of a core–shell structure grain in Bi2O3 plus Nb2O5-doped BaTiO3. The dopants are concentrated near the grain boundary and render the material cubic. The dopants have not had time to diffuse into the center of the grain leaving it essentially pure BaTiO3 allowing it to undergo the cubic-tetragonal phase transition with subsequent twinning. (Chiang 1988) 7.10 Displacive Transformations Because of the rapid propagation of the phase interphases in displacive transformations their kinetics are of limited interest from a practical point of view. Of far greater interest are the detailed crystallographic changes between the two phases, the resultant stresses developed in the two phases, how the transformation is nucleated, how the final microstructure develops, and how the properties—usually mechanical—are affected by the transformation. Most of these issues are outside of the main focus of this book. Nevertheless, some examples of displacive transformations are presented because of their technological importance. 7.10.2 zircoNiuM oxide Important examples of displacive polymorphic phase transformations include the transitions that occur in pure zirconium oxide, ZrO2: 1170° C 2370° C monoclinic tetragonal cubic Figure 7.30 shows the fluorite cubic structure of the high temperature cubic polymorph of ZrO2 in which the Zr+4 ion is surrounded by 8 oxygen ions. In reality, the Zr+4 ion is really too small to be in eightfold coordination by oxygen and it rattles around inside the eightfold oxygen cube. The radius of the Zr+4 ion is 87 pm and that of oxygen is 132 pm giving a cation/anion radius ratio of about 0.66 which is smaller than the minimum ratio of 0.732 necessary to stabilize eightfold coordination. Nevertheless, at the very high temperatures where the cubic phase is stable, there is enough thermal vibrational energy to keep the mean Zr+4 ion position centered in the oxygen cube. However, as the temperature is lowered, the zirconium ion would prefer to position itself closer to four oxygens on the face of the cube, hence the transformation to tetragonal zirconia. At still lower temperatures, a monoclinic structure is more stable in which the oxygen cube becomes even more distorted to attempt to satisfy the needs for the Zr+4 ion to have a lower coordination number than eight. The tetragonal to monoclinic transformation includes about a 3% increase in volume. Therefore, pure polycrystalline zirconia, sintered at some elevated temperature—say 1750°C—on cooling will essentially fall apart at this transition temperature due to this large volume change that causes cracking at grain boundaries and grain separation. Because ZrO2 has a high melting point—about 2680°C—it would make a good high temperature refractory for furnace insulation, and so on. Unfortunately, because of this low temperature phase transition, pure ZrO2 cannot be used as a thermal insulator. However, it was found almost a century ago that, by forming an alloy of ZrO2 with MgO, CaO, Y2O3, and others, the high temperature cubic phase could be stabilized to low temperatures and actually maintained all the way to room temperature. 4-fold coordination of O−2 Zr+4 O−2 8-fold coordination of Zr+4 Oxygen ions in neighboring cell FIGURE 7.30 The cubic structure of ZrO2, fluorite (CaF2), showing how the Zr+4 ions in the faces are eightfold coordinated by 8 oxygen ions, 4 within the cell and 4 in the neighboring cell. Note the eightfold site in the center of the fluorite cell is not occupied by a Zr+4 ion. The ions are drawn to scale. (Emsley 1998) 225 Chapter 7. Phase Transitions 3000 2800 Liquid 2600 2400 Temperature (°C) 226 Cubic + liquid 2200 Cubic 2000 1800 1600 1400 Cubic + tetragonal Cubic + MgO Partially stabilized 1400°C Tetragonal + MgO 1200 1140°C Monoclinic + MgO 1000 0 ZrO2 FIGURE 7.31 Fully stabilized 5 10 15 m/o MgO 20 25 MgO 30 Part of the MgO-ZrO2 phase diagram. (After Roth 1995) Figure 7.31 based on data in the literature (Roth 1995) shows that ZrO2 with about 12 m/o MgO fired—densified—at about 1750°C is entirely cubic. Hence, such solid solutions are called stabilized zirconia and if the material is 100% cubic it is called fully stabilized zirconia. The presence of these other elements in solid solution, Mg2+, if they are randomly distributed in the crystal lattice, gives the crystal a high degree of symmetry, a cubic structure. Therefore, in order to transform from the cubic—high symmetry—solid solutions, the added cations must diffuse into positions that give all the unit cells either tetragonal or monoclinic symmetry since in displacive transformations, unit cells transform together. Since moving the randomly dispersed cation alloying elements around is a diffusion process, it is possible to retain the cubic structure down to room temperature without transformation—hence, the existence of cubic zirconia gemstones. If the material is not fully stabilized by adding smaller amounts of alloying compounds—say 5 m/o MgO in Figure 7.31—and cooled under proper conditions to room temperature, a two-phase mixture of cubic and tetragonal zirconia is obtained. If the tetragonal grains or crystals are small enough, the tetragonal phase is inhibited from transforming to monoclinic by the surrounding cubic phase that prevents the tetragonal to monoclinic volume expansion. This material is called partially stabilized zirconia (PSZ) and it has a very high fracture strength for ceramics—on the order of 109 Pa. High strength occurs because crack propagation releases the compressive stress on the untransformed tetragonal zirconia allowing it to expand and transform to monoclinic, the expansion partially closes the crack, and increases the fracture resistance—fracture toughness—and strength. In order to achieve high strengths, the grain size of the tetragonal phase must be carefully controlled during firing and cooling. If the grain size is too large, it will simply transform on cooling providing no strengthening. If the tetragonal grain size is too small, cracks will not relieve enough stress to allow the transformation, also providing no strengthening (Green et al. 1989). 7.10.3 BariuM titaNate Another important set of displacive phase transformations are those in barium titanate, BaTiO3, which goes through the following series of transformations (Kingery et al. 1976): −90° C 0° C 130° C rhombohedral orthorhombic tetragonal cubic 7.10 Displacive Transformations 227 Note that the symmetry of the stable phase increases as the temperature increases similar to ZrO2 and is generally true for all solids. The high temperature cubic form has the perovskite crystal structure with the barium ions at the cube corners, the oxygen ions on the cube faces, and the Ti+4 ion in the center of the octahedron formed by the six oxygen ions on the cube faces, Figure 7.32. In this case, the size of the octahedron is determined by close packing of both the large oxygen and barium ions and the octahedron is a little too large for the Ti+4 ion to touch all the neighboring oxygen ions Ti+4 Ba+2 O−2 so it too rattles around inside the oxygen octahedron until the temperature becomes low enough for it to be bound closer to one or more of the oxy- FIGURE 7.32 The perovskite crystal structure of gen ions. As a result, cooling from elevated temperatures, the cubic phase barium titanate, BaTiO3. The ions are drawn to scale. transforms to tetragonal at 130°C simply due to a shift in the Ti+4 ion from (Emsley 1998) the center of its oxygen octahedron toward one of the cube faces distorting the crystal from cubic to tetragonal. This produces a built-in electric dipole that gives BaTiO3 its very large relative dielectric permittivity—6000—making it useful as a dielectric in capacitors. In addition, cooling through this transition temperature in an electric field, the materials are poled— aligning the electric dipoles—making the material piezoelectric—stress produces a voltage and an applied voltage produces a strain—enabling many applications including sonar and precise small voltage-controlled movements as required in the scanning tunneling microscope, STM. 7.10.4 MarteNSite iN SteelS ° ° 912 C 1394 C Pure iron goes through two phase transformations: BCC, α FCC,δ (Brandes FCC, γ and Brook 1992). Of course, a most important effect of carbon on the phase transformation of steels— iron containing carbon—is the displacive transformation to form martensite upon rapid cooling iron– carbon alloys from the cubic austenite* to prevent the diffusion-controlled decomposition of austenite to ferrite and Fe3C, cementite. “The way in which this transformation occurs, however, is a complex process and even today the transformation mechanism, at least in steels, is not properly understood” (Porter et al. 2009, 369). However, this much is known, the metastable FCC austenite undergoes a displacive transformation to BCT martensite that produces a large amount of strain in the steel that greatly increases the hardness: Figure 7.33 (Bain 1924). In principle, the FCC austenite could transform all the way to BCC ferrite via the Bain strain: 20% contraction along the c-axis of the BCT cell and 12% expansion along the a-directions. However, the presence of carbon in solid solution in octahedral interstitial site restricts the complete transformation to the BCC cubic phase. The result of the transformation is then a BCT phase whose lattice parameters depend on the carbon content of the alloy, Figure 7.34 (Krauss 1990; Reed-Hill and Abbaschian 1992). Note that 4 a/o carbon corresponds to only about one carbon atom per 12.5 BCT unit cells yet it has a very large influence on the transformation! The temperature below the eutectoid temperature in Figures 7.4 and 7.5 where martensite begins to form, the Ms temperature, also depends on the carbon content, decreasing as the carbon content increases implying that the Gibbs energy difference between the austenite and ferrite phase needs to get larger to overcome the strain energy produced in the transformation. Microscopically, the martensite forms randomly and in some cases consists of plates consisting of extremely small twins. As the temperature is lowered, more plates form until martensite formation stops. Usually, there is some retained austenite that does not transform and the amount increases with carbon content. In addition, the detailed microstructure of the martensite formed also depends on the carbon content of the steel. The details of the martensite transformation in steels has been studied extensively mainly with respect to crystallography, martensite nucleation, effect of carbon content and alloying elements, the effects on microstructure, all with a focus on optimizing the mechanical properties of steels for a large number of specific applications (Krauss 1990). For more details about the process—there are many—the literature should be consulted (Krauss 1990; Reed-Hill and Abbaschian 1992; Porter et al. 2009). * Named after the English metallurgist William Chandler Roberts-Austen, 1843–1902. Chapter 7. Phase Transitions FCC γ-iron, austenite BCT cell a0,γ a0,γ = 0.365 nm Bain strain c m .258 n a 0,γ = 0 a 7 nm a 0,α = 0.28 √2 FCC α-iron, ferrite BCT martensite cell Isolated BCT cell FIGURE 7.33 The Bain model of FCC austenite transforming to BCT martensite in steels, Fe-C alloys. In principle, pure iron should be able to transform from FCC to BCC by about a 20% negative strain in the z-direction and plus 12% in the x- and y-directions relative to the isolated BCT cell at the bottom left: the Bain strain. However, the presence of carbon in octahedral interstices in austenite only allows the transformation to proceed partially to BCT martensite at the bottom right. (Bain 1924) Weight percent carbon 0.22 0.44 0.66 0.89 1.12 1.35 1.59 1.84 0.305 Lattice parameter (nm) 228 BCT martensite 0.300 c-axis 0.295 Solid: experiment 0.290 a0(α) = 0.287 0.285 a-axis 0.280 0 1 2 3 4 5 6 Atomic percent carbon 7 8 FIGURE 7.34 The variation of the c- and a-axes of BCT martensite as a function of carbon content in steels. Note that they extrapolate to the lattice parameter of BCC iron, ferrite. (Data from Krauss 1989) Frequently, all displacive transformations are referred to as martensite or martensitic transformations (Buchanan and Park 1997) but others would restrict this terminology to displacive transformations in which strain energy plays a dominant role (diffusionless transformations). 7.10.5 Shape MeMory alloyS Shape memory alloys are important examples of displacive transformations. Important shape memory metals are the nitinol alloys of roughly 50 m/o Ni-50 m/o Ti or NiTi—hence the name since they were discovered at the U.S. Naval Ordinance Laboratory in Maryland. The crystal structure of NiTi is CsCl, four Ni at the corners of a cube and the Ti in the center, in its high temperature—T ≈ 60°C—austenitic phase and becomes tetragonal with about an 8% volume change going through the martensite transformation start temperature, Ms, near or slightly above room temperature (Brandes and Brook 1992). Again, like all materials that show a displacive transformation, the strain associated with the transformation in these materials is frequently accommodated in a 7.11 Cool below TE: Transformation, crytal structure, changes, twinning Anneal above TE: original crystal structure, twins and deformation gone Rectangular bar Plastic deformation by twin motion Deformed bar FIGURE 7.35 Schematic showing how the strain accompanying a displacive transformation can be minimized by twinning, and how the twinned material can be plastically deformed by twin reorientation. On reheating above TE, the twins and deformation go away and the deformed bar returns to its original shape: the shape memory effect. polycrystalline material by the formation of twins as sketched in Figure 7.35. Application of a stress changes the orientation of the twinned crystals producing plasticity or a strain. In these twinned materials, the plastic deformation is caused simply by movement of twin boundaries or reorientation of twins. Therefore, heating back into the austenite region, each crystal again becomes cubic and the strain introduced in the martensitic phase disappears and the material assumes its original shape. Hence, the name: shape memory alloys. On the other hand, if these materials are deformed slightly above the phase transformation temperature, then the stress can induce the phase transformation and a great deal of elastic strain—up to 10%—can be induced entirely by the alignment of the transformed crystals in the direction of the stress. On removal of the stress, the structure reverts to the cubic phase and the strain returns to zero. Such materials are called superelastic or pseudoelastic. Materials that exhibit displacive transformations are also classed under so-called ferroic materials. Ferroic crystals may be defined as crystals that possess two or more orientation states, or domains, and under a suitable driving force such as stress, electric field, or magnetic field the domain walls will move switching the crystal from one domain state to another. Materials that switch in an electric field are called ferroelectrics, those that switch under a stress are called ferroelastic, and those that switch under a magnetic field, not surprisingly, are called ferromagnetic. These properties and fields can be inter-related in interesting and complex ways depending on the symmetry of the crystals and the directional dependencies of their properties* (Newnham 2005). It should be noted that both ferroelectric and ferroelastic materials actually undergo phase transitions to different crystal structures and the domains—crystal regions with the same orientation of properties—are actually crystal twins. Most ferromagnetic materials do not undergo phase transitions and their domains merely consist of regions with different orientations of the aligned magnetic moments of the atoms or ions in the solid. 7.11 7.11.1 GLASS TRANSITION iNtroductioN to the GlaSS traNSitioN It is appropriate to say something about the glass transformation particularly since attempts to explain it have gone on for over 400 years. Morey (1938, 34) defined a glass as * If you enjoy linear algebra, then you will appreciate detailed investigations of the relationship between the structure, properties, and transformation of these materials. Glass Transition 229 Chapter 7. Phase Transitions A glass is an inorganic substance in a condition which is continuous with, and analogous to, the liquid state of that substance, but which, as the result of having been cooled from a fused condition, has attained so high a degree of viscosity as to be for all practical purposes, rigid. Well yes and no! This definition does not even include polymer glasses and most polymers are in the glassy rather than a crystalline state. What does “…analogous to, the liquid state…” mean? And glasses do not have to be made only from a fused or liquid state. They can be deposited from the vapor phase by some type of PVD process as was seen with the crystallization of amorphous silicon. During the last 100 years, the understanding of the structure and properties of materials has considerably improved, the glass transition has elicited numerous definitions and a wide variety of explanations, including whether or not it is a thermodynamic phase transformation or something different. For example, a first-order transition is the type of transition that most of this chapter is focused on; namely, there is a discontinuous change of the extensive thermodynamic variables U, V, H, and S at the transition temperature. On the other hand, the glass transition has often been referred to as a second-order transition, one in which derivative quantities such as thermal expansion and heat capacity are discontinuous but the extensive variables are continuous. There is some debate in the literature whether the glass transition is a true second-order transition: “…the glass-rubber transition is not a real thermodynamic phase transition, neither a first nor a second order transition… At the very best the Tg-transition may be seen as a quasi-second-order transition but certainly not as a first-order one” (Van Krevelen 1997, 130). Nevertheless, the IUPAC (International Union of Pure and Applied Chemistry) defines it as a second-order transition (McNaught and Wilkinson 2006, 360). One of the better literature definitions is (Glass transition 2016): Thus, the liquid-glass transition is not a transition between states of thermodynamic equilibrium. It is widely believed that the true equilibrium state is always crystalline. Glass is believed to exist in kinetically locked state, and its entropy, density, and so on, depend on the thermal history. Therefore, the glass transition is primarily a dynamic phenomenon. Glass transition temperature, Tg Glass Crystal Liq ui d Despite the variations in the definition, the glass transformation plays an extremely important role in materials technology even if its materials science is somewhat debatable. Metals (by rapid cooling), covalently bonded elements (Si, Ge, and chalcogenides: S, Se, Te), inorganic compounds (silicates, phosphates, borates, halides), and polymers, all show glass transitions (Varshneya 1994). Wherever you are, it doesn’t take much looking around to find something made with either an inorganic glass or a glassy polymer. Figure 7.36 shows the volume versus temperature for a material that when cooled from the liquid state can either crystallize at its melting point if cooled slowly or, if cooled sufficiently rapidly, Volume 230 Supercooled liquid Melting point, Tm Temperature FIGURE 7.36 Volume versus temperature for a material that forms a glass at the glass transition temperature, Tg, or becomes 100% crystalline at the melting point Tm. Note that volume expansion versus temperature for the glass and crystal are virtually the same but that for the liquid is much larger reflecting the additional motion of the atoms, ions, or molecules in the liquid state compared to the solid state. 7.11 Glass Transition 231 will form a glass instead. Note the discontinuity in the derivative of the volume, dV dT, the volume thermal expansion coefficient at the glass transition temperature. The terms slow and rapid depend on the material. For example, to crystallize a liquid silicate melt to prevent glass formation, the cooling rate might be measured in degrees Centigrade per hour or per day while for metallic glasses, cooling rates on the order of 106–108 °C/s are necessary. Polymers require cooling rates somewhat in between these extremes. If the cooling rate is sufficiently rapid, then the liquid can be supercooled below the melting point. Figure 7.36 illustrates two extremes where a material either crystallizes completely at the melting point or goes completely to a glass at the glass transition temperature. This is typically the behavior of silicate glasses. On the other hand, many polymers are partly crystalline and partly glass. As a result, the V-T curve on cooling can show behavior that is a combination of these two extremes. However, for purposes of distinguishing between crystallization and glass formation, Figure 7.36 is the most appropriate. 7.11.2 therMal expaNSioN As the glass transition can be defined in terms of a discontinuity in thermal expansion, it is worthwhile examining the fundamental processes producing expansion. In a monatomic gas, such as argon, only translational motion of the atoms is possible and they travel at speeds of several hundred m/s, about 1000 mph, as was seen in Chapter 5, and travel only about 0.1 μm before colliding with another atom. This is the basis for diffusion of atoms in gases as will be seen later in Chapter 9. Note that all of the thermal energy in the gas—the enthalpy—is in this translational motion and the value of the heat capacity reflects that heat added to a monatomic gas contributes only to higher translational speeds. Note that for one mole of an ideal gas, pV = RT, so the volume thermal expansion coefficient is just the inverse of the temperature, αg = d ( RT p ) ( R p ) dT = 1 1 dV = = V dT ( RT p ) dT ( RT p ) dT T (7.33) which is 3.33 × 10−3 K−1 at room temperature. This extra volume reflects the increasing translational velocity of the gas atoms. In contrast, in a solid, the atoms, molecules, or ions are fixed in position and merely vibrate on their lattice sites—at room temperature this vibration frequency, as is shown in Chapter 9 is on the order of 1013 Hz—as sketched in Figure 7.37 where the interatomic bonds essentially act like springs against which the atoms vibrate. The heat content or enthalpy of a solid is entirely contained in the kinetic and potential energy of these atomic vibrations. As the heat content and temperature is increased, the vibration amplitude increases giving rise to the thermal expansion of a solid as shown in Figure 7.38. The potential energy curves versus distance between atoms, ions, or molecules in solids are not perfectly symmetrical, so the average interatomic distance increases as the amplitude of vibrations or temperature increases. Figure 7.38 greatly exaggerates the effect of temperature on the average position of the atoms. Typically, the minimum in the potential energy versus distance curve, the equilibrium distance, is several electron volts negative, the bonding energy of the solid. The gas constant in eV/K is R 8.314 J mol ⋅ K = = 8.61 × 10 −5 eV K 23 N Ae 6.022 × 10 atom mol 1.602 × 10 −19 J eV ( )( ) so even at 1000°C the thermal energy is only about 0.11 eV above the minimum in the potential energy curve, hardly noticeable in Figure 7.38. The thermal expansion is related to the mean interatomic distance as a function of temperature, and therefore to the asymmetry of the potential energy curve with distance. The more symmetrical the bonding curves, such as those for covalently bonded materials, the smaller the expansion Z Y Atom X Vibrations FIGURE 7.37 Schematic showing an atom in a solid vibrating in three directions with the interatomic bonds depicted as springs. Each vibration contributes kBT to the heat capacity or 3kBT for each atom or ion. Repulsive Potential energy Chapter 7. Phase Transitions Interatomic distance, r 0 Attractive 232 T Vibrational amplitude Mean distance between atoms FIGURE 7.38 Potential energy versus interatomic distance in a solid. An asymmetric bonding curve exists for all types of bonding: ionic, covalent, and van der Waals. Because of the asymmetry, as the temperature (energy) increases the amplitude of the atomic vibration increases and its mean position—dashed curve— between the attractive and repulsive parts of the potential increases generating thermal expansion. The effect of temperature is greatly exaggerated in this drawing in that the minimum in the potential is several eV negative—the interatomic bond—and thermal energies are small, only on the order of a tenth of an eV for 1000°C. coefficient. Also, as the bond strength increases the deeper and more symmetrical the potential well becomes. Therefore, the melting point goes up and the thermal expansion coefficient decreases. For example, for the elements C (diamond), Si, and Ge all having the diamond cubic crystal structure with melting points of 4700 K (under pressure), 1687 K, and 1211 K, their thermal expansion coefficients are 1.18 × 10−6 K−1, 2.6 × 10−6 K−1, and 5.8 × 10−6 K−1, respectively (Haynes 2013). On the other hand, a more asymmetric bonding curve as in an ionic bond leads to higher expansion coefficients. For example, at 300 K, the linear thermal expansion coefficient of reasonably ionic MgO with a melting point of 3100 K, is about αl = 12 × 10−6 K−1 which makes the volume expansion coefficient, αV (see Appendix) αV = 1 dV 3α L = 36 × 10 −6 K −1 V dT about two orders of magnitude smaller than that of a gas. And—as mentioned in Section 5.2.1—each energy-absorbing mode of an atom contributes 1 2 k BT to the total energy of an atom. A vibration has both kinetic and potential energy each of which contribute 1 2 k BT for a total energy per vibration of kBT. But for each atom, there are three directions—or modes—of vibrations so the total energy contribution to a vibrating atom is 3kBT. For one Avogadro’s number of atoms, = E vib 3= N A k BT 3RT. So the heat capacity for a monatomic solid is simply, CP ≅ CV ≅ dE vib = 3R = 24.94 J mol ⋅ K . dT (7.34) This ignores quantum effects and the coupling of atoms that the Einstein and Debye theories of heat capacity take into account and that explain heat capacities at low temperatures. However, at high temperatures, Equation 7.34 is a good approximation. One thing to be careful about is that the molar heat capacity for metals is about 3R since there is only one Avogadro’s number of atoms per mole. However, for compounds as shown in Chapter 1, there are more atoms or ions than one NA per mole. For example, for NaCl, there are 2 NA per mole so its heat capacity is about 6R ≅ 50 J/mol-K. — Similarly, for Al2O3 there are 5 NA ions per mole so, C P ≅ 125 J/mol-K. 7.11 Liquid behavior is between that of a solid and a gas in many ways. As shown in Figure 7.36, on melting, for most solids,* there is an expansion in going from the solid to the liquid state—typically around 10 v/o (volume percent) or more. For example, for copper at its melting point of Tmp = 1083°C, the density of liquid copper is, ρ(Cu, l) = 8.00 g/cm3 while that of solid copper is ρ(Cu, s) = 8.96 g/cm3 (Haynes 2013). As a result, there is about 10% more volume in the liquid than in the solid and now the atoms can move with some translational velocity as well as vibrating back and forth against their interatomic bonds. Furthermore, in a polymer, there can be large and different sections of a polymer molecule that are free to move with increased volume without moving the entire molecule. Therefore, atoms or molecules in a liquid have both translational and vibrational motions that don’t exist in a crystalline solid, motions that contribute to heat capacity, enthalpy, and thermal expansion coefficient. For example, the heat of fusion at melting is essentially the energy necessary to give the atoms of the solid the translational energy that they have in a liquid. So the volume of a liquid is determined not only by the volumes of the atoms, ions, or molecules of the liquid but also by a certain amount of free volume that gives them extra freedom of movement compared to a crystalline solid. 7.11.3 Short-raNGe aNd loNG-raNGe order Because of the translational motion in a liquid, the atomic structure of a liquid is also somewhere between that of a solid and a gas. A solid has both short-range order and long-range order. For example, in solid Cu, which has an FCC lattice, each of the Cu atoms is surrounded by 12 nearest neighbor Cu atoms—all the same distance away—which is the short-range order. However, a copper crystal also has long-range order in that—if it is a perfect crystal—there is another Cu atom at one lattice parameter—cell edge—away, 10 lattice parameters away, or even a million lattice parameters away traveling along a cell edge in a <100> direction. In contrast, liquid Cu has only the same short-range order that exists in the Cu crystal; namely, each Cu is surrounded—on the average—by 12 nearest neighbor Cu atoms. However, there is no long-range order in that if one travels in any direction in the liquid, the chance of hitting the center of another Cu atom at 2, 10, or 100 interatomic distances away is highly unlikely. Furthermore, the atom positions are constantly changing in a liquid as well. Figure 7.39 gives an example of SiO2 that is made up of SiO 4− 4 tetrahedra bonded at corners to give a fairly open structure in crystals, liquids, and glasses and shows the difference between the ordered array of tetrahedra in a crystal compared to the disorder that exists in both liquids in glasses.† The hexagonal Crystal Glass Dangling oxygen bond SiO44− Tetrahedron (a) (b) FIGURE 7.39 Comparison between the ordered arrangement of (a) SiO 4− 4 tetrahedra in crystalline silicates (or PO3− 4 in phosphates) with (b) the more random arrangement of the tetrahedra in a silicate glass. Note that the short range order in both consists of four oxygen ions at fixed distances from the silicon ion but the uniform Si–Si distance and 180° angle in the crystal vary in the glass because of the random angular rotation of the tetrahedra around their corner bonds. * † Si and H2O being notable exceptions because of their directed covalent and hydrogen bonds, respectively. 3− This is actually a more accurate representation of phosphate crystals, liquids, and glasses in that the PO 4 tetrahedra sharing corners have only one unbonded corner oxygen to form sheets and chains. Glass Transition 233 234 Chapter 7. Phase Transitions array is presumed to extend infinitely in three dimensions with additional tetrahedra sharing the currently unshared corners. The short-range order in this case is that each silicon is surrounded by four oxygen ions and each oxygen by two silicon atoms at the same distance. Neighboring silicon–silicon distances in the crystal are all the same, but this distance varies in the liquid or glass because of the ability of the tetrahedra to rotate. Also, note the existence of a broken or dangling bond. In pure SiO2, at high temperatures, thermal energy generates a number of these broken bonds decreasing the continuity of the three-dimensional network of SiO 4− 4 tetrahedral and generating smaller groups of interconnected tetrahedra that constantly form and reform into different configurations. It is the breaking of the network into smaller groups that generates the higher thermal expansion in the liquid and decreases the viscosity—the ability of these groups to move past each other under stress.* Note in Figure 7.39, that idealized crystal structure consists of a three-dimensional array on interconnected hexagonal groupings of six tetrahedra. While in the glass or liquid state in Figure 7.39 there is a group of four and a group of eight interconnected tetrahedra. In order for this liquid or glass to crystallize, there must be bond breaking and rearrangement of these tetrahedra to form the ordered crystalline array. As the melting point is approached from above, the number of broken bonds decreases and the viscosity of the liquid continually increases. In polymers, short-range order exists within a chain segment. But if there is any rotational freedom around the bonds, then any long range order along the molecule length disappears to say nothing of the essentially independent orientation from one polymer molecule to each of its neighbors precluding long-range order. 7.11.4 viScoSity The viscosity of both glasses and liquids is critically important in flow behavior and the glass transition. Figure 7.40 shows how the viscosity of a liquid is defined—and frequently measured. This figure shows two parallel plates with a fluid of thickness y between them and a shear stress applied between the plates of τ† causing a gradient in the velocity of the liquid from v = 0 at the bottom, stationary plate, to a maximum value, v, at the top plate. The shear strain rate, γ , is defined as the gradient of the velocity with distance or, γ = dv dx dt ( dx y ) dγ = = = dy y dt dt (7.35) τ v Parallel plates y Fluid velocity v=0 x dγ dx/y γ = dv = dx/dt = = y y dt dt τ = μγ FIGURE 7.40 The shear motion of a moving plate relative to a stationary one with a fluid of thickness y in between showing how the viscosity of the fluid is defined by the shear strain rate, γ , and the shear stress, τ. * † In silicate glasses, sodium oxide, Na 2O, calcium oxide, CaO, and other oxides are added to break up the continuous threedimensional network of pure SiO2 as will be shown in Chapter 9. The symbol τ has already been used for the relaxation time in Chapter 2. Unfortunately, in the literature both the relaxation time and the shear stress are given this symbol. Hopefully, the contexts in which they appear will not make their use confusing. However, the relaxation time for stress relaxation will be used shortly and here a different notation for the relaxation time will be used to hopefully minimize confusion. 7.11 Glass Transition 235 and the viscosity, μ,* is defined as the resistance to flow, or τ = µγ . (7.36) The units of viscosity are Units(μ) = Pa-s. However, in the older literature the cgs version of viscosity is used and in the cgs system, Units(μ) = P for poise: 1 P = 0.1 Pa-S. Water, for example, has a viscosity of around one centipoise or μ = 10−3 Pa-s. The viscosity for forming inorganic glass objects, the working point (Varshneya 1994), is about 103 Pa-s around the same as viscous syrup and the viscosity for the injection molding of polymers is about 100 Pa-s (Morton-Jones 1989). 7.11.5 the GlaSS traNSitioN teMperature, tg Volume The formation of a glass takes place in the following way. As the temperature of a liquid is decreased, atomic and molecular translational—and some group migrational and rotational—motion is less energetic and becomes more difficult until, at the melting point in a simple monatomic material such as copper, the atoms can easily arrange themselves into the long-range ordered structure of the crystal since the atoms can move easily and do not need to go very far. In contrast, in polymers and inorganic materials the larger molecules and atomic groups in the liquid state require several coordinated motions and, perhaps, bond breaking and reforming to orient them properly to generate the long-range order of the crystal. This takes time and atomic or molecular translational and other motions—diffusion and/or viscous flow. If the material is cooled sufficiently below the normal melting temperature—a supercooled liquid—the temperature may become so low that these translational motions essentially stop and the lack of long-range order of the liquid is solidified in place at the glass transition temperature, Tg (Figure 7.41). Now the only thermal motions experienced by the atoms and molecules in the glass are the same thermal vibrations of the atoms that occur in the crystal. Therefore, the thermal expansion coefficient of the glass is essentially the same as the crystal and less than that of the liquid since there is no longer any translation or diffusional motion. As a result, the glass no longer flows like a liquid and becomes rigid and exhibits properties of a solid such as hardness, elastic modulus, and heat capacity in addition to the thermal expand ui liq sion coefficient. Figure 7.41 shows that the slopes of the volume d le versus temperature curves—the volume thermal expansion oo c r pe coefficients—of the crystal and the glass are essentially equal Su and both less than that of the liquid: αglass ≅ αcrystal < αliquid. Fast ht On reheating at Just rig Therefore, a good definition of a glass is: a material that just right rate Slow has the structure of a liquid—short range order but no long range order—and the properties of a solid—elastic modulus, hardness, thermal expansion coefficient, heat capacity, etc And Tg Tg Tg at the expense of being repetitious, that is why the volume verTemperature sus temperature plots for the crystalline solid and the glass are essentially the same, or parallel, in Figure 7.41 since the only FIGURE 7.41 Schematic showing how the cooling rate affects mechanism that produces volume expansion—thermal vibra- the glass transition temperature: the fastest cooling rate gives tions of atoms on stationary positions—is the same in both. Tg1 at the largest glass volume; the slowest cooling rate give While in the liquid state, in addition to thermal vibrations, the Tg3 and the smallest glass volume; and the middle cooling rate give Tg2 and the middle glass volume. Reheating all three glasses molecules in polymers and the large atomic groups in inorganic at the same rate as the middle cooling results in different behavcrystals have translational, rotational, and complex vibrational ior of each glass. The V-T curve of the glass heated and cooled motions that increase with temperature increasing the volume at the same rate, on reheating follows the cooling curve closely. However, the fastest cooled glass, at the slower reheating rate tries at a faster rate than atomic vibrations alone. 3 * The symbol η is frequently for viscosity and is the symbol recommended by the IUPAC (McNaught and Wilkinson, compilers 2006). However, here η is already being used as number per unit volume and μ is frequently used for viscosity. 2 1 to equilibrate its structure with the slower rate and, near the glass transition temperature, it actually shrinks to try to follow the V-T of the slower reheating rate. For the more slowly cooled glass, the opposite occurs: it tries to maintain its structure—volume—above the original Tg3. 236 Chapter 7. Phase Transitions Another important feature of the glass transition temperature is that it is not a material property like the melting point or the boiling point that are fundamentals of a first-order phase transition. In contrast, the glass transition temperature depends on the rate of cooling as shown in Figure 7.41: the faster the rate of cooling, the higher the glass transformation temperature but the glass transition temperature change with cooling rate is small. For all glass-forming materials, the glass transformation temperature occurs when the glass viscosity reaches about μ ≅ 1012 Pa-s. Figure 7.41 implies that glasses of identical composition, cooled at different rates with different glass transition temperatures, have different densities related to their volumes at the glass transition temperatures. Optical glasses used as lenses will have spatially different indices of refraction if cooled at different rates, which, of course is undesirable. As a result, such glasses are heated for long times just below the glass transition temperature and slowly cooled to insure uniform density. On the other hand, tempered (or toughened) glass, is a normal silicate glass that is rapidly cooled that puts the surface in compression when the entire part has cooled to room temperature increasing the strength of the glass (Jones 1956; Doyle 1979; Pfaender 1983; Varshneya 1994). Note also in Figure 7.41 when all three of the glasses are heated at the same rate as the intermediate cooling rate, the rapidly cooled glass shrinks as it reaches the glass transition temperature and actually gives it a negative thermal expansion in this region. At temperatures this close to the glass transition temperature, the glass has enough thermal energy for structural rearrangement and tries to have the same degree of order and volume as the glass cooled at that just right rate. In contrast, the glass cooled at the slowest rate, will actually try to maintain its greater degree of order until above its original glass transition temperature and then when its viscosity is low enough, it rapidly expands to give the supercooled liquid structure appropriate to the intermediate cooling rate. These changes and their rates are all functions of the glass viscosity as a function of temperature. Therefore, engineers in the glass industry working with silicate glasses have designated key viscosity points (Kingery et al. 1976; Varshneya 1994): Working point, where the glass is shaped Softening point, where the glass gets soft Annealing point, where cooling-induced stresses relax Strain point, below which nonuniform strain cannot form 103 Pa-s 106.65 Pa-s 1012.4 Pa-s 1013.5 Pa-s and the working range is the viscosity interval between the working point and the softening point. 7.11.6 viScoelaStic Behavior 7.11.6.1 Material Differences The intent here is not to discuss the many and varied mechanical properties of materials, but only those that relate to material behavior at temperatures near the glass transition temperature that lead to an improved understanding of Tg. Therefore, the focus is on glassy polymers and inorganic glassforming materials. Because of the different histories of development and processing requirements, particularly temperature, for these two classes of materials; testing procedures; and the properties measured are frequently different and difficult to compare. Furthermore, for many inorganic glasses, particularly oxides, the details of the various structural units in the melt and in the glass phase are not that well understood. The viscosity of inorganic glasses and the effects of additives, particularly in silicate glasses, is the primary property for the production of glass objects. A large volume of literature on the empirical effects of additives and temperature on viscosity has been developed over many years (Morey 1938) without a detailed understanding of the structural units in the glass that determine properties. In contrast, for polymers both their viscous and elastic (hence viscoelastic) behaviors are important for a number of reasons. It is important is to understand the effects of all the possible pre-determined structural variables of polymers such as chain length, chain composition, branching, cross-linking, chain and branch stiffness, chain and branch length, and so on, on the glass transition and mechanical properties (Scherer 1986; Ward and Hadley 1993; Sperling 2006). So for polymers, the structural elements in the glass are known and the major effort is to relate these 7.11 structural elements to properties such as viscosity as a function of temperature and the glass transition temperature. The glass transition temperature for many polymers is within roughly 100° of room temperature: high density polyethylene, −90°C; polypropylene, −18°C; poly(vinyl chloride), 87°C; and polycarbonate, 150°C (Callister and Rethwisch 2009). Even elastomers in which the polymer chains are cross-linked but can move freely past each other at room temperature can undergo a glass transition at low temperatures; for example, polybutadiene, Tg ≅ −90°C (Askeland and Phulé 2003). These low temperatures allow the use of in situ experimental techniques on polymers that are difficult to conduct at the high temperatures necessary for most inorganic glasses. One of these techniques involves the application of either a periodic stress or strain to the polymer and observation of its dynamic modulus and internal energy loss. Performing these experiments as a function of temperature and frequency can generate a great deal of information about the effects of chain structure on polymer melts and glasses. For example, polymers above their glass transformation temperatures exhibit several different regions for the shear modulus, G, as a function of temperature as shown in Figure 7.42. Most noncross-linked linear amorphous polymers exhibit a rubber-like region just above the glass transition temperature where inhibition to translational molecular motion is caused by a polymer chain that may be sufficiently tangled with other molecules that it takes time to untangle. For short times, this entanglement acts almost like a cross-linking covalent bond of the polymer molecules. As the temperature approaches the glass transition temperature from above, the polymer becomes stiffer or, more accurately, the greater is its elastic modulus. As a result, polymers exhibit both elastic and viscous behavior. For temperatures well above the glass transition temperature, thermal energy overcomes these tangles between the molecules and they flow or move past each other and the modulus drops rapidly as shown in Figure 7.42. As the chain length increases, the temperature where this drop occurs increases. This is in contrast to the real elastomers in which permanent cross-links retard flow at high temperatures (Figure 7.43). However, even for elastomers, it becomes more difficult for the molecules to move as the glass transition temperature is approached. This rubbery region above the glass transition temperature has only recently been observed for the first time in inorganic phosphate glasses that have individual chains of connected tetrahedra.* These experi3− ments on lithium metaphosphate glass, in the neighborhood of 200°C, based on LiPO3, in which PO 4 tetrahedra form long chains by bonding with other tetrahedra at two corners (not too dissimilar to the silicate tetrahedra sharing corners in Figures 7.9 and 7.39) with the Li+ ion forming ionic bonds between the chains. With substitutions of other larger monovalent and weaker bonding ions such 12 Cross-linked elastomer log10 G(Pa), log10μ (Pa-s) G 9 Leathery Rubbery 6 μ 3 Tg Linear polymer Temperature FIGURE 7.42 Temperature dependence of the shear modulus, G, and the viscosity, μ, for a linear polymer above the glass transition temperature emphasizing the rubbery region and contrasting it with a cross-linked elastomer. The temperature dependence of the viscosity roughly corresponds to µ = µ 0exp(Q/RT) with Q and μ0 chosen so that the magnitude of the viscosity change is about that expected over the temperature range of about 150°C. The viscosity probably varies in a more complex fashion than shown except near the glass transition temperature. * 3− Note that in a PO 4 tetrahedron, one of the oxygen atoms has a double bond to the phosphorus with the other three oxygen ions cancelling the remaining plus three charge on the phosphorus giving a net charge of minus three to the tetrahedron. Glass Transition 237 238 Chapter 7. Phase Transitions Entanglements Linear polymer Strain Stress Crosslinks Elastomer “Rubbery” behavior (a) (b) FIGURE 7.43 (a) Entanglements between polymer chains lead to rubbery behavior of linear polymers. (b) Real elastomers have covalently bonded cross-links between chains that allow molecules to slide past each other between the cross-links that limit the amount of sliding or elastic deformation. as Na+, K+, and Cs+ it is only the smaller Li+ ions that form the more distant pinning points between chains behaving similar to the tangles in linear polymers. As a result, recoverable elastic strains on the order of 30% are observed (Inaba et al. 2015). These results suggest that similar behavior might be found in metasilicate glasses based on the tetrahedral chain structure of metasilicate crystals such as MgSiO3, but at higher temperatures. Other candidates that might show similar behavior are the chalcogenide glasses, many of which consist of isolated chains of atoms. A potential implication of such a controlled chain structure in a silicate glass is that fibers based on such glasses might have higher strengths, all else being equal, due to the orientation of the chains during viscous drawing of the fibers. 7.11.6.2 Some Viscoelastic Behavior A common mechanical property test, particularly for metals, is the tensile test in which a metal sample is elongated at a constant applied tensile strain rate, ε a , and the stress and strain are measured and used to define the mechanical properties of the metal such as elastic modulus, yield stress, tensile stress, plastic strain, and fracture stress. Similar constant strain rate tests are also used for crystalline ceramics to determine the elastic modulus, the fracture stress, and the fracture toughness. In glasses, above the glass transition temperature, the main properties of interest are the shear modulus, G, Units(G) = Pa, and the viscosity, μ, Units(μ) = Pa-s, as shown in Figure 7.42.* Below Tg, the main properties of interest for glass are the shear modulus and the fracture strength. There are several ways to express the relationship between the properties of interest and the shear strain rate, γ = dγ dt (Scherer 1986; Ward and Hadley 1993). However, for a constant applied strain rate, γ applied , the type of test commonly used to determine the mechanical properties of metals and ceramics, general behavior can be obtained from the simple general relation, γ applied = γ elastic + γ plastic (7.37) where γ applied = γ = constant is the applied strain rate. Now, τ = Gγ elastic so γ elastic = (1/G )(dτ/dt ) where τ = shear stress defined in Figure 7.40 with Units(τ) = Pa. Finally, τ = µγ plastic . These substitutions into Equation 7.37, gives the following nonhomogeneous differential equation: γ = * 1 dτ τ + G dt µ (7.38) Finding viscosity versus temperature data for polymers is difficult and its behavior with temperature can be complex. The viscosity data in this figure were calculated with µ = µ 0exp(Q/RT) but with a much larger Q than would be expected for polymers in order to cover the range of viscosity values shown. 7.11 which is easy to solve by standard integrations when γ = constant. Rewriting this as dτ ( γ − τ µ ) = Gdt and integrating, −µ ln ( γ − τ µ ) = Gt + C where C is an integration constant. Rearranging and taking the exponent of both sides of this equation gives G γ − t − t − τ = C′ e µ = C′e t rel µ where C′ is another constant and t rel = µ G is the relaxation time and when t = 0, τ = 0, gives C′ = γ so the final solution is t − t rel τ = µγ 1 − e . (7.39) Figure 7.44 shows the stress–strain behavior near the glass transition of Figure 7.42 for a fixed value of G and different values of the viscosity. Figure 7.45 shows similar data but for both varying shear modulus and viscosity, which is a more realistic model near Tg. For both of these figures, the constant strain rate was 0.001 s−1, which is typical for a constant strain rate test and the resulting total strains are small (Askeland and Phulé 2003). This strain rate is much lower than typically used in forming polymeric and inorganic glasses where strain rates about 103 s−1 are more common and the viscosity and the shear modulus may vary with shear rate. Figure 7.46 shows a relaxation phenomenon typical of viscoelastic behavior. In this case, the applied strain rate was stopped at 15 s where the total stain is held at γ = 0.015 and the stress relaxes to zero with a relaxation time of trel = 4 seconds. Many of the mechanical properties of polymers above the glass transition temperature are performed not with a constant strain rate (or stress rate) but one that is periodic, that is, γ applied = A sin ωt , as a function of both temperature and frequency, ω. As a result, the solution to Equation 7.37 becomes more difficult (although not much more, but requires solution techniques beyond what are necessary here) but this technique provides detailed information about structural elements in the glass and their relaxations. This experimental technique is frequently referred to as the measurement of 10 μ = 10 GPa-s γ = 0.001s−1 μ = 6 GPa-s 1G 6 G= Stress (MPa) Pa 8 μ = 4 GPa-s 4 μ = 2 GPa-s 2 0 Relaxation time for μ = 10 GPa-s, 10 s 0.01 0.02 0.03 Strain FIGURE 7.44 Viscoelastic stress–strain behavior for a polymer with a fixed value of the shear modulus G = 1 GPa and four different viscosities that give rise to different relaxation times. The relaxation time of 10 seconds is shown for the material that has a viscosity of μ = 10 GPa-s. Glass Transition 239 Chapter 7. Phase Transitions 10 μ = 10 GPa-s, G = 8 GPa Stress 8 γ = 0.001s−1 μ = 6 GPa-s, G = 3 GPa 6 μ = 4 GPa-s, G = 1 GPa 4 μ = 2 GPa-s, G = 0.5 GPa 2 0 0.01 0.02 0.03 Strain FIGURE 7.45 This figure is similar to Figure 7.44 except in this case, each stress–strain curve has a different value of the shear modulus and viscosity, which is more realistic behavior particularly as the glass transition temperature is approached from higher temperatures. 0.4 γ = 0.001s−1 γ=0 μ = 4 GPa-s G = 1 GPa Relaxation time = 4 sec Str ain 0.3 Stress (MPa) 240 0.2 0.1 0 5 10 15 20 25 30 Time(s) FIGURE 7.46 Example of stress relaxation for a viscoelastic material in a constant strain rate test in which the applied strain rate was dropped to zero at 15 seconds. The figure shows the constant strain and the decreasing stress with time with a relaxation time of 4 seconds after the applied constant strain rate was stopped. internal friction and gives correlations between frequency and temperature that help to determine the structural features of the glass that produce a specific relaxation. One of the reasons that the technique has not been applied more frequently to inorganic glasses is that it is relatively easy experimentally near room temperature but becomes considerably more difficult as the temperature gets higher, particularly in excess of 500°C, where it would have the most interest for inorganic glasses, particularly silicates. 7.11.7 a free voluMe approach to the GlaSS traNSitioN 7.11.7.1 Free Volume A somewhat different approach to the glass transition involves a concept known as free volume. As was shown earlier, the increase in volume on melting of many metals is on the order of about 10%. For ionic compounds, this increase is about 20% (Kingery 1959). The volume change on melting of polymers is less certain but has been estimated between 2% and 10% (Sperling 2006). This free volume is associated with the increased degrees of freedom for the molecules, atoms, and ions in the liquid to perform translational and other larger modes of motion than in the solid state. As a result, the volume of a liquid can be given as V = Va + Vf 7.11 Glass Transition 241 where: Va is the volume of atoms, ions, and molecules Vf is the free volume. The volume thermal expansion of liquids is typically larger than that of solids, and so the free volume increases more rapidly with temperature than that required of vibrational motion in the solid state. 7.11.7.2 Free Volume and Tg As the temperature is decreased, the amount of free volume decreases because the extra motion of the molecules or atoms gets smaller. There are many, but not terribly different, approaches to relating the free volume to the glass transition temperature. In all cases, it is assumed that the changing configurations of the molecules cannot keep up with the rate of the decreasing temperature, β = dT dt ≅ ∆T ∆t for a constant rate, thereby freezing in an amount of free volume. Figure 7.47 shows the free volume of a liquid as a function of temperature with the free volume no longer changing at the glass transition temperature. As mentioned before, the glass transition is still not completely understood. However, a plausibility argument, developed by Varshneya, based on the free volume and modeled on the glass transition in inorganic glasses gives some valuable insight into the transition (Varshneya 1994). 7.11.7.3 Volume Viscoelastic Behavior In Section 7.11.6, it was shown that the shear strain rate could be expressed as γ applied = γ elastic + γ plastic that leads to the result t − τ = µγ 1 − e t rel (7.40) (7.41) where: t rel = µ G μ is the viscosity G is the shear modulus τ is the shear stress γ is the applied strain rate. A similar equation to Equation 7.40 can be written for the volume strain rates ξ i where ξ i = (1/Vi )(dVi /dt ) so ξ applied = ξ plastic + ξ elastic (7.42) Free volume ΔT V .V V e P = ηξ 1 − e − t t rel (7.43) where: t rel = µ K = µκ η is the volume viscosity ≅ μ K is the bulk modulus κ is the compressibility = 1/K P is the pressure ξ is the applied volume strain rate. The main point is that the volume viscous relaxation time is given by t rel = µκ where κ = (1/V )(dV /dP) = dξelastic /dP with Units(κ) = Pa−1. dT/dt = β V0 Ve with a similar result, . V 0 Tg Temperature FIGURE 7.47 Model for the relaxation of free volume as a function of temperature. The solid diagonal line and its dashed extension represent the equilibrium free volume of the liquid as a function of temperature. Above Tg, if the temperature is suddenly changed by an amount ΔT, the liquid will have time to relax to its equilibrium value Ve with the cooling rate, β. However, below Tg, there is insufficient time to relax and the volume does not change. By making ΔT sufficiently small, the glass transition temperature occurs at μ ≅ 1012 Pa-s, and the horizontal line is developed where no relaxation occurs and the free volume in the glass does not change with temperature. (After Varshneya 1994) 242 Chapter 7. Phase Transitions 7.11.7.4 Free Volume Relaxation Referring to Figure 7.47, suppose that at the V0 above Tg, the temperature were suddenly dropped by an amount ΔT where the new equilibrium free volume is Ve. The question is, Can the free volume relax fast enough to keep up with the constant rate of temperature decrease, β = dT dt = ∆T ∆t. This can be modeled with first order kinetics, dV dt =− V − Ve t rel (7.44) and integrated to give V − Ve = C′e − ∆t t rel (7.45) where Δt simply represents the time from t = 0 when the temperature was changed to current time, t. When t = 0, V = V0 so the solution is ∆t f unrel = ∆T − − V − Ve = e µκ = e µκβ V0 − Ve (7.46) where f unrel = the fractional unrelaxed free volume after an instantaneous temperature change of ΔT. If Equation 7.46 is 1.0 for a given set of parameters, then there is no relaxation and the liquid is now a glass. If Equation 7.46 is zero, then the liquid can completely relax. At the glass transition temperature, TG, it will be somewhere in between zero and one. Data in the literature used in this model for a soda–lime–silica (Na2O, CaO, SiO2) glass of unspecified composition are (Varshneya 1994): κ ≅ 10−11 Pa−1 and µ = 10 −43 exp ( 90, 000 T ) Pa ⋅ s. At a cooling rate of β = 10°C s the glass transition temperature of this glass is given to be about 710 K or about 412°C. Therefore, temperatures of 770, 730, 720, 710, and 680 K are chosen to calculate the relaxation with ΔT = 10 K. The results are given in Table 7.2. The results show that, at 770 K, the volume change can keep up with the rate of cooling, while at 680 K, there is no volume relaxation. Notably, at 710 K, the viscosity is μ ≅ 1012 Pa-s, the viscosity of the glass transition temperature. The reason that the relaxation rate changes so rapidly with temperature is because of the double exponential of the relaxation and the viscosity. From the table, it is clear that if the cooling rate, β, were decreased by a factor of 10 to 1°C/s the exponent in Equation 7.46 is increased by a factor of 10 and will decrease the transition temperature by around 10°. Conversely, an increase in rate by a factor of 10 will increase the glass transition temperature to a similar amount. To make the model more illustrative, Figure 7.48 shows the relative free volume of the glass described above as a function of the cooling rate. The calculations were performed in the following way. First, obviously the fraction relaxed, frel, f rel = 1 − f unrel , so from Equation 7.46, f rel = V0 − V V − V0 = = 1 − f unrel . V0 − Ve Ve − V0 (7.47) TABLE 7.2 Volume Relaxation of a Silicate Glass T(K) 770 730 720 710 680 T(°C) 472 432 422 412 382 μ(Pa-s) 5.78 × 107 3.49 × 1010 1.94 × 1011 1.13 × 1012 3.02 × 1014 ∆T µκβ 1.73 × 103 2.87 0.515 8.89 × 10−2 3.31 × 10−4 f 0.00 0.057 0.60 0.91 1.00 7.11 1.000 Relative free volume Cooling rate 0.998 100°C/s 10°C/s 0.996 μ ≅ 109 Pa-s 1°C/s μ ≅ 1012 Pa-s 0.994 640 660 680 700 720 740 Temperature (K) 760 780 FIGURE 7.48 Glass transition temperature as a function of cooling rate for the model shown in Figure 7.47 with a temperature change of ΔT = 2 K for each relaxation. The data points are not shown since they form essentially continuous curves. The details of the calculation are in the text. Note that the glass transition varies only about 40 K while the cooling rate varies by two orders of magnitude. The calculated viscosities for this glass over this temperature range are also shown. However, from Figure 7.47, on the free volume versus temperature curve it is obvious that Ve = V0 − V0 ∆T α f where the absolute value of ΔT is taken and αf, the thermal expansion coefficient of the free volume, (1/Vf )(dVf /dT). Therefore, Equation 7.47 can be written, V = V0 {1 − (1 − f unrel ) ∆T α f } . (7.48) The relaxation calculations were done at a |ΔT| = 2 K and the free volume, V(T), as a function of temperature was calculated from V ( T ) = V ( T + 2 ){1 − (1 − f unrel ) ∆T α f } (7.49) again, |ΔT| = 2 K and αf ≅ 10−4 since α f ≅ 3α V ≅ 3 ( 3α L ) and α L ≅ 10 × 10 −6 K −1 (Varshneya 1994). That is, the relaxation to a volume V(T) was taken as the relaxation at the volume 2 K higher. This expression was calculated as a function of temperature on a spreadsheet as a function of the cooling rate from 650 to 770 K and plotted in Figure 7.48. Since the actual free volume as a function of temperature requires more empirical data such as density as a function of temperature, relative free volumes were calculated with V(770 K) = 1.00. In contrast to most plots, the calculated data points are not shown in this figure since they essentially form a continuous curve for each of the three plots. Again, this simple plot of free volume versus temperature shows all of the characteristics of the glass transition temperature: a relatively sharp transition from an equilibrium free volume with falling temperature to one that is constant; the faster the cooling rate, the higher the transition temperature; and the glass transition occurs at µ ≅ 1012 Pa ⋅ s for reasonable cooling rates. This simple model of free volume relaxation shows clearly why a glass transition occurs, namely, the very strong double-exponential temperature dependence of the relaxation. Also, it predicts relatively small changes in the glass transition temperature with orders of magnitude changes in the cooling rate. Finally, it predicts that the glass transition temperature should occur at a viscosity of about 1012 Pa-s, which is experimentally found. Again, perhaps not all of the details of the glass transition are understood, but this simple plausibility model predicts the behavior of the glass transition extremely well! Glass Transition 243 244 Chapter 7. Phase Transitions It should be noted that 100°C/s is a rather rapid cooling rate for a glass. If this rate is applied to the surface of a cooling glass, because of the poor thermal conductivity of glasses, the interior of a piece is cooling more slowly. Therefore, the surface becomes rigid well before the interior that continues to shrink until it reaches the glass transition temperature at some lower temperature than the surface. This additional shrinkage of the interior puts the surface under compressive stress thereby increasing the glass strength. This is a commercial process called thermal tempering to distinguish it from chemical tempering where the composition of the glass is changed at its surface to put the surface under a compressive stress. 7.11.8 GlaSS viScoSity aNd urBaN leGeNdS 7.11.8.1 The Legends There is an urban legend that exists that suggests that glass—essentially window glass, soda–lime– silica glass, as above—is a supercooled liquid (sic) and therefore flows (very slowly) over long periods of time resulting in changes in thickness and optical properties of window panes! There are two observations that contributed to this legend. First, optical imperfections or striations that exist in old windowpanes are assumed to be flow marks due to the flow of the glass over time since it is just a very viscous liquid. The second version says that if the thickness of an old windowpane is measured, it will be thicker at the bottom than at the top because the glass has flowed over time under its own weight, as sketched in Figure 7.49 (Plumb 1989). Without spending much effort searching, several contradictory articles can be found in the printed literature and on the internet that refute both of these, imply that the data are insufficient to decide their truth, or simply lend some credibility to these legends. They neither attempt to demonstrate why the legends are true or not, nor do most give good definitions of a glass. These articles serve as good examples of why “…because something is in print or online implies that it must be correct…” is not always true and refute the validity of the often-heard comment, “I don’t need to know this stuff, I can just look it up!” 7.11.8.2 Dispelling Legend One In old buildings, glass windows have striations which are actually flow marks produced when the glass was poured. Years ago, flat glass for windowpanes was made by pouring the molten glass onto a flat iron or steel sheet to cool and solidify, or in more recent times, by passing it through cold rollers. As a result, the cooling and thickness was very nonuniform and flow marks remained on the surface of—and in—the glass. As a result, distortions are observed when looking through the glass that give the appearance of being caused by continuing flow. An extreme example of this is glass made in the United States during colonial times by just pouring the molten glass onto a cold iron plate as shown in Figure 7.50. This is a window in the Public House—an inn and restaurant—in Sturbridge, w Window glass Long time w Increase in thickness due to flow!! Shear stresses FIGURE 7.49 Sketch of the expected increase in thickness, right, of a window pane deforming under its own weight, w, which the text demonstrates to be unmeasurable. 7.11 FIGURE 7.50 Front door windowpane in the over 200-year-old Public House in Sturbridge Massachusetts. The pane was formed by pouring molten glass onto a cold iron plate producing the large variations in thickness and flow marks in the glass that result in severe optical distortion. The distorted image is that of a tree outside the window some 10 ft away. Massachusetts, that is over 200 years old. Such nonuniformities do not occur today because window glass is made by the float-glass process developed in 1959 (Doyle 1979) in which the molten and relatively low viscosity glass (μ ≅ 102 Pa-s), a viscosity similar to that of molasses, at about 1100°C, is poured onto a bath of molten tin where it reaches a uniform thickness and smoothness. The glass is slowly pulled along the molten tin bath with a gradually decreasing temperature until it exits the tin-bath furnace at about 600°C where the viscosity has now risen to about 1012 Pa-s (Doremus 1994, p. 100), near the glass transition temperature and the glass no longer flows and is of a uniform thickness and flatness. 7.11.8.3 Dispelling Legend Two A few rough calculations can quickly disprove this version of the myth. The viscosity of a soda– lime–silica glass (Na2O–CaO–SiO2)—window glass—is strongly temperature dependent, as is the viscosity of all silicate and other inorganic and organic glasses. Specifically, the viscosity of soda– lime–silica window glass can be approximated over a wide temperature range by an exponential function of temperature Q µ = µ0e RT where again μ0 = pre-exponential and Q = activation energy. Surprisingly, it is difficult to find data for Q and μ0 in the literature at low temperatures, so existing data need to be extrapolated to room temperature. With the viscosity data from Section 7.11.7.4, namely, µ = 10 −43 exp ( 90, 000 T ) Pa ⋅ s, at 298 K, room temperature, μ ≅ 1.5 × 1088!! As was seen in Section 7.11.4, the relaxation time for stress or strain provided by viscous flow is t rel = µ G. Now Young’s modulus for window glass is E ≅ 70 GPa (Kingery et al. 1976) and the shear modulus is given by G = E/2 (1 + ν ) (McClintock and Argon 1966) and ν = Poisson’s ration ≅ 0.25. So, G ≅ 28 GPa and the relaxation time would be, t rel = µ G = 1.5 × 1088 ≅ 5 × 1077 seconds !!!! 28 × 109 Now the age of the earth is about 4.5 billion years and there are 3 ≅ 107 s/year so the age of the earth is ≅ 1017 s; 60 orders of magnitude too small to produce any detectable strain! Glass Transition 245 246 Chapter 7. Phase Transitions This calculation assumes that the high temperature data can be extrapolated down to room temperature. This is undoubtedly not entirely correct and literature data suggest that the activation energy for viscosity below the glass transition is about one-half that above, or, at 298 K, room temperature, µ = 10 −43 exp ( 45, 000 T ) Pa ⋅ s and the viscosity at room temperature could be calculated from this based on the viscosity being 1012 Pa-s at the glass transition temperature of about 412°C. However, there are other data in the literature that suggest at room temperature the viscosity for window glass is about 1020 Pa-s (Jones 1956). In that case, the relaxation time is t rel = µ G = 1020 ≅ 3.6 × 109 seconds 28 × 109 or about 100 years. As was seen earlier, the relationship between viscosity, μ; shear stress, τ; and shear strain rate, γ , is τ = µ γ . This allows the following more precise calculation. For the sake of concreteness, take a windowpane 4 ft × 4 ft × 1/8 in. (these would be typical window dimensions in the United States) which has a total volume of 4.72 × 103 cm3. The density of this glass is ρ ≅ 2.3 g/cm3 so the weight of the window is (4.72 × 103 cm3)(2.3 g/cm3) = 1.08 × 104 g = 10.8 kg so that the total force at the bottom is 10.8 kg × 9.8 m2/s = 106.4 N. Now the bottom area is (12 in. ft × 4 ft × 2.54 cm in .)( 0.125 in. × 2.54 cm in .) = 38.70 cm 2 = 3.87 × 10−3 m 2. So the compressive stress at the bottom of the windowpane is σ = (106.4 N) ÷ (3.87 × 10−3 m2) = 2.79 × 104 Pa (~4 psi). The shear stresses will be on the same order of magnitude as the compressive stress, that is, τ ≅ σ/2 but at 45° to the plane of the window. Therefore, the strain rate can be calculated to be γ = dγ ∆x/x τ 2.79 × 10 4 Pa ≅ = ≅ = 2.7 × 10 −16 s−1 ∆t µ dt 1020 Pa ⋅ s where x = thickness of the glass = 0.125 in. = 3.175 × 10−3 m. Assume that the difference in thickness between the top and bottom could be measured to ± 1 μm = Δx (±1 mil = 0.001 in. = 25.4 μm would be more realistic). The time necessary then for this increase in thickness would be ∆t ≅ 1× 10 −6 m ∆x ≅ 1.2 × 1012 s. = − x γ 3.17 × 10 3 m 2.7 × 10 −16 s −1 ( )( ) (7.50) Again, since there are about 3 × 107 s/year this corresponds to about 40,000 years, far longer than most windowpanes have been around. This urban legend is clearly just that, a legend that has no basis in fact! In reality, variations in thickness of unused float glass produced today on the order of 140 µm are observed (Dorn et al. 2013). This implies that in order to observe a thickness difference between the top and bottom of a windowpane caused by flow and not a statistical variation, Δx would have to be at least 100 times larger in Equation 7.50 requiring something on the order four million years to be measureable! This is not an accurate model but certainly good enough for a back of the envelope calculation sufficiently plausible to send this myth to the dust-bin of history! 7.11.9 the challeNGer diSaSter aNd the GlaSS traNSitioN Figure 7.51 shows the liftoff of the shuttle Challenger on its last—and fatal—flight on January 28, 1986. The night of January 27–28, 1986, was an extremely cold night in Florida, freezing or below. The relevant conclusion of the Challenger Accident Report (The Presidential Commission on the Space shuttle Challenger Accident Report 1986) was that a hot gas leak occurred around an elastomer O-ring seal in one of the solid booster rockets and ultimately caused ignition of the main hydrogen and oxygen fuel tanks. There were several factors for the seal failure including poor design. However, the crash investigation team found that the temperature dependence of the elastic behavior of elastomer O-rings probably contributed to the seal failure as suggested by physicist and team 7.12 Particle Size and Phase Transitions FIGURE 7.51 The Challenger space shuttle launch on January 28, 1986, just moments before it was destroyed because of a hot gas leak in one of the O-ring seals in one of the solid booster rockets. Original NASA color photograph converted to grayscale. member, Richard Feynman. At these low temperatures, the fluorelastomer O-rings on the boosters either became brittle or lost some of their elasticity, entered the leathery region of Figure 7.42, and no longer provided a gas-tight seal. This allowed hot gases to leak and burn through eventually leading to ignition of the hydrogen and oxygen fuel tanks and complete destruction of the system. Data on the specific elastomer used for the solid booster O-rings could not be found other than they were fluoroelastomers. These are copolymers of polytetrafluoroethylene—or other fluorinated polymer— with another polymer and can have a glass transition temperature as high as −8°C (17.6°F) (Viton). Lacking modulus data as a function of temperature, it is a valid conjecture that this glass transition is high enough so that at the cold ambient temperatures that morning, near freezing, the elastomer probably became much less elastic contributing to the shuttle’s tragic destruction. 7.12 PARTICLE SIZE AND PHASE TRANSITIONS Research on surface energies of solids has shown that polymorphs that are unstable under normal conditions tend to have lower surface energies than the stable phases (Navrotsky 2011). For example, the surface energy of hematite, α-Fe2O3—corundum structure—has a surface energy of 1.9 J/m2. In contrast the metastable phase of large particles, maghemite, γ-Fe2O3—defect spinel structure—has a surface energy of 0.71 J/m2 (Navrotsky 2011). The implication of this is that a normally metastable phase may become the stable phase when the particle size is small since, at constant temperature, pressure, and composition, G = γS where γ is the surface energy and S is the specific surface area per mole, Units(S) = m2/mol (see Chapter 6, Section 6.9). Figure 7.52 schematically shows how this can occur. At large particle sizes, near S = 0, the stable phase is alpha, α; the next most stable is beta, β; and the least stable is delta, δ. As the specific surface area increases, because of the differences in surface energies—the slopes of the lines—around 20,000 m2/mol, beta is the stable phase and at specific surface areas in excess of about 25,000 m2/mol, the delta phase is stable. There are several implications of this. First, frequently the metastable phases result from the process used to attempt to make the stable phase of a material. For example, in the production of magnetic iron oxides such as spinels, iron oxide, Fe2O3, is often made by the decomposition of iron oxalate, Fe2(C2O4)3 247 Chapter 7. Phase Transitions Particle size (nm) 20 10 6.7 5 4 δ ∆G 248 δ-stable β β-stable α 0 α-stable 10 20 30 40 Specific surface area (1000 m2/mol) 50 FIGURE 7.52 Schematic drawing illustrating the effect of particle size on the stability of various polymorphs of a given material. With bulk or large particles the alpha phase is stable while with small particle sizes both the beta and delta phases are more stable because of their lower surface energies stabilizing small particles of these metastable phases. (Data from Navrotsky 2011) ° C Fe2 ( C2O 4 )3 100 → Fe2O3 + 3CO2 ( g ) + 3CO ( g ) and can be accomplished by combustion synthesis since the CO can be ignited to provide the heat for the reaction. The resulting Fe2O3 produced at this low temperature is small particle size γ-Fe2O3 long thought to be the result of the kinetics of decomposition rather than the thermodynamics. That is, it is thought that kinetically it is easier to form the gamma phase rather than the alpha phase at this low temperature. However, if the particle size is small enough, less than about 40 nm (S ≅ 5000 m 2 mol) then gamma is the stable phase because of its lower overall energy because its total surface energy is much lower than that of the alpha phase, hematite. (Navrotsky 2011). Similarly, hydrated surfaces of oxides have lower energies than those of oxides. As a result, the decomposition of goethite, α-FeOOH, to hematite occurs almost 100°C higher for 10 nm particles of goethite compared to bulk particles since it is the stable phase to higher temperatures because of its higher surface energy (Navrotsky 2011). Finally, because of this effect of particle size and relative energies of phases and their region of stability, the equilibrium phase boundaries as a function of p(O2) and temperature can be moved with small particle sizes, for example, 800 K 6Fe2O3 4Fe3O 4 + O2 ( g ) the equilibrium oxygen pressure at 800 K is p(O2) ≅ 10−16 bar for bulk particles (Roine 2002) while for 10 nm particles, p(O2) ≅ 10−12 bar. And the phase field for FeO, in T-p(O2) space for iron and oxygen, completely disappears for 10 nm particles! (Navrotsky et al. 2010). 7.13 CHAPTER SUMMARY This chapter covered many different topics, some in more detail, others in less. The thermodynamics of phase transformations is reviewed. Then the various types of phase transformations are presented focusing on the difference between displacive and reconstructive transformations. Reconstructive transformations in pure materials require the diffusive motion of atoms, ions, or molecules and, therefore, are dependent on time. As a result, most of these transformations occur through a nucleation and growth process that can be controlled by either a surface reaction or diffusion. Phase Appendix transformations between gases and solids and gases and liquids are emphasized since the interaction between a gas and a condensed phase interface is easiest to model. In order to do this, some kinetic theory of gases was introduced in order to calculate rates of condensation and growth. Then a model of homogeneous nucleation is introduced. The overall rate of phase transformation by a nucleation and growth process is calculated assuming that a surface reaction controlled the growth process. The model of homogeneous nucleation is then modified for heterogeneous nucleation based on the wetting behavior of a heterogeneous nucleus. The other important class of transformations but probably less well understood, displacive transformations, is illustrated in systems such as stabilized zirconia, BaTiO3, martensite in steels, and shape-memory alloys. However, the kinetics of such transformations are of less interest than their crystallography and resulting lattice strains since the transitions propagate at essentially the speed of sound. Finally, the glass transition is discussed because of its importance for both polymers and inorganic glasses and a definition of a glass is presented. A simple free-volume model is then presented that surprisingly lends significant insight into the glass transition: it is a relatively sharp transition because the relaxation of free volume depends on a double exponential with temperature! Then some calculations of viscoelastic behavior of inorganic glasses are made that help to dispel some urban legends about glass. Finally, a proximate reason for the space shuttle Challenger disaster may very well have been the glass transition in its booster rocket polymer O-ring seals. APPENDIX a.1 voluMe therMal expaNSioN coefficieNt The relation between the volume thermal expansion coefficient, αV, and the linear thermal expansion coefficient, αL, is given by α V ≅ 3α L and can be determined in the following way. The two expansion coefficients are defined as αL = 1 dL 1 ∆L ≅ L0 dt L0 ∆T αV = 1 dV 1 ∆V . ≅ V0 dt V0 ∆T Consider a cube of initial volume V0 and length L0 so V0 = L30 then with some temperature increase of ΔT L = L0 + ∆L = L0 + L0α L ∆T = L0 (1 + α L ∆T ) V = V0 + ∆V = V0 + V0α V ∆T = V0 (1 + α V ∆T ) but V = L3 so, L3 = L30 (1 + α L ∆T ) 3 ( L3 = L30 1 + 3α L ∆T + 3 ( α L ∆T ) + ( α L ∆T ) 2 3 ) V ≅ V0 (1 + 3α L ∆T ) since the squared and cubed terms are very small. Comparing the equations for V, it is clear that α V ≅ 3α L . 249 250 Chapter 7. Phase Transitions EXERCISES 7.1 The Gibbs energy, G, as a function of temperature for solid, liquid, and gaseous sodium chloride, follow closely the approximate expressions (Roine 2002): G ( solid ) = −430.86 − 0.1126 × T G(liquid ) = −361.87 − 0.1988 × T G(gas) = −244.35 − 0.2792 × T where Units(G) = kJ/mol and Units(T) = °C and the gas consists of NaCl molecules. a. Plot these three curves as a function of temperature between 0°C and 2000°C. b. Calculate the melting and boiling points of NaCl in °C from these data and compare them to literature values. Give the reference for the literature data. c. Calculate the Gibbs energy (J/mol) for condensation of NaCl vapor to solid NaCl at 500°C. d. Calculate the equilibrium NaCl vapor pressure at 500°C. 7.2 This problem uses some of the data from Exercise 7.1. a. The molecular weight and density of solid NaCl are 58.433 g/mol and 2.5 g/cm3, respectively, calculate the molar volume (m3/mol) (Haynes 2013). b. If solid NaCl is in contact with NaCl gas that is 10 4 times the equilibrium partial pressure at 500°C, calculate the Gibbs energy per unit volume (J/m3) to form a homogeneous nucleus. c. If the surface energy of solid NaCl from Chapter 6 is 300 mJ/m2, calculate the critical nucleus radius in meters. d. Calculate the number of NaCl molecules in this critical nucleus. e. Calculate the Gibbs energy of the critical nucleus, J. f. Calculate the number of NaCl molecules/m3 in the gas. g. Calculate the concentration of critical nuclei (m−3). h. If the sticking coefficient is unity, calculate the Θ0 in the expression for the nucleation rate. i. Calculate the nucleation rate for NaCl nuclei from the gas phase (m−3s−1) at 500°C with 104 times the equilibrium pressure of NaCl gas. 7.3 The major vapor species over solid and liquid selenium, Se, is Se2(g) so the sublimation or vaporization reaction is 2 Se(s, l) = Se2(g). The Gibbs energy, G, as a function of temperature for solid, liquid, and gaseous selenium follow closely the approximate expressions (Roine 2002): G ( 2Se, solid ) = −23.24 − 0.0970 × T kJ / 2 moles G(2Se, liquid ) = −6.20 − 0.1739 × T kJ / 2 moles G(Se2 , gas) = 72.74 − 0.2790 × T kJ / mol where Units(T) = °C. Note that the values of G for the solid and liquid are for two moles since two moles of each form one mole of Se2 gas. a. Plot these three curves as a function of temperature between 0°C and 1000°C. b. Calculate the melting and boiling points of Se in °C from these data and compare them to literature values. Give the reference for the literature data. c. Calculate the Gibbs energy (J/mol) for condensation of Se vapor to liquid Se at 500°C. d. Calculate the equilibrium Se vapor pressure at 500°C. Exercises 7.4 a. Given the data below (Brandes and Brook 1992) and the melting point of liquid selenium determined in Exercise 7.3, make a plot of volume versus temperature, from 0°C to 500°C for liquid and crystalline Se (see Figure 7.36). Linear thermal expansion coefficient of solid, α = 3.7 × 10−6 K−1 Solid density at 0°C, ρ(solid) = 4.79 g/cm3 Liquid density at the melting point, ρ(liq) = 3.989 g/cm3 Molecular weight of selenium, M = 78.96 g/mol Change in liquid density with temperature, dρ dT = −1.44 × 10 −3 g cm −3K −1 b. Calculate the volume expansion coefficient of the solid, K−1. c. Calculate the volume expansion coefficient of the liquid, K−1. 7.5 The TTT diagram for 1080 steel is Figure 7.5 and shows the times for 1% and 99% transformed. a. From the 99% transformed curve, make a table of the time for this amount of transformation and the rate of transformation (i.e., 99%/time) versus temperature from 700°C down to 300°C at 50°C intervals. b. From these data, plot the temperature vertically and the rate of transformation horizontally (%/s) and indicate the equilibrium temperature on your graph. 7.6 A silicate glass is crystallizing following the Johnson–Mehl–Avrami equation, where the 4 fraction crystallized is given by ftransformed = 1 − e − At . The following temperature and times are observed for 50% crystallization: 2 seconds at 600°C, 7 seconds at 500°C, 30 seconds at 700°C, 200 seconds at 750°C, 400 seconds at 300°C, and 300 seconds at 800°C. a. Calculate the value of “A” for each of these temperatures and times. b. Plot the Johnson–Mehl–Avrami equation for each of the values of “A” calculated in part “a.” all on the same plot of fraction transformed versus log10 (time in seconds). Plot at 0.001, 0.01, 0.1, 0.2...0.9, 0.99, and 0.999 transformed to show the shape of the curves. c. From these data make a table of 0.1, 0.5, and 0.9 transformed as a function of temperature and also include the rate of transformation (s−1) for 50% transformed by taking 50/ time(s). d. From the data, make a plot of temperature vertically and rate of transformation horizontally for the rate calculated for 50% crystallized. e. Make a TTT diagram for this crystallization by plotting the points for 0.1, 0.5, and 0.9 crystallized with a vertical temperature axis and a horizontal axis of log10 (time, seconds). 7.7 For a certain metal that undergoes a phase transformation from alpha to beta on cooling by a nucleation and growth process at 500°C, given the following data for the nucleation rate Θ (nuclei/m 3 -s) and the growth rate of G(m/s) as a function of temperature: T (oC) Θ(m−3s−1) G(m/s) 475 5.0 × 1011 2.0 × 10−8 400 1.0 × 1015 5.0 × 10−8 325 1.0 × 1016 1.00 × 10−10 a. On the same graph, calculate and plot the fraction transformed as a function of time (log10 [time, seconds] scale) from the Johnson–Mehl–Avrami equation for each of these temperatures with a minimum of 10 points on each curve. b. From the data and plots in “a” above, estimate the times for 5%, 50%, and 95% transformed and plot a TTT diagram for this transformation for 5%, 50%, and 95% transformed with temperature vertical and time horizontal (log10 [time, seconds] scale). Include and show the equilibrium temperature. 7.8 Glycerin (glycerol), C3H5(OH)3, has a melting point of 17.8°C but a fairly high viscosity at that temperature that allows it to be cooled to form a glass. The following data exist on the viscosity of glycerin (Haynes 2013): −42°C, μ = 6710 Pa-s; −25°C, μ = 262 Pa-s; −15.4°C, μ = 66.5 Pa-s; −4.2°C, μ = 14.9 Pa-s; 6°C, μ = 6.26 Pa-s; 15°C, μ = 2.33 Pa-s; and 25°C, μ = 0.954 Pa-s 251 252 Chapter 7. Phase Transitions a. Plot these data on a semilog plot versus 100/T (K−1) and determine Q and μ0 in for the µ = µ0exp(Q/RT) viscosity (use a least squares fit). b. Calculate the glass transition temperature, °C, for glycerin; that is, where μ ≅ 1012 Pa-s. 7.9 A soda–lime–silica window glass (0.15 w/o Na 2O, 0.15 w/o CaO, 0.70 w/o SiO2) has the following values of viscosity (log10μ(Pa-s)) and temperature (°C): 9.3, 600; 7.2, 700; 5.4, 800; 4.5, 900; 3.9, 1000; 2.9, 1100; 2.0 1200; 1.7, 1300; and 1.2, 1400 (several sources). a. Plot these data on a semilog plot versus 1000/T (K−1) and determine Q and μ0 in for µ = µ0exp(Q/RT) the viscosity (use a least-squares fit). b. Calculate the temperature at which the viscosity is 1012 Pa-s, °C, for this silicate glass. 7.10 From the data for viscosity calculated in 7.9, make a plot of the relative free volume from 50 K above to 50 K below the temperature at which μ ≅ 1012 Pa-s at a cooling rate of 0.1 K/s: a single plot like that if Figure 7.48 and use the same parameters as in Section 7.11.7 in the text. Take the free volume at the +50 K temperature to be 1.00. REFERENCES American Society for Metals. 1973. Atlas of Isothermal Transformation Diagrams. Metals Park, OH: American Society for Metals. Askeland, D. R. and P. P. Phulé. 2003. The Science and Engineering of Materials, 4th ed. Pacific Grove, CA: Brooks/Cole-Thomson Learning. Bain, E. C. 1924. The Nature of Martensite. Trans. AIME, Min. Metall. 70(Paper No. 1299-S): 1–11. Balluffi, R. W., S. M. Allen, and W. C. Carter. 2005. Kinetics of Materials. New York: Wiley. Brandes, E. A. and G. B. Brook. 1992. Smithells Metals Reference Book, 7th ed. Oxford: Butterworth-Heinemann. Buchanan, R. C. and T. Park. 1997. Materials Crystal Chemistry. New York: Marcel Dekker. Callister, W. D., Jr. and D. G. Rethwisch. 2009. Fundamentals of Materials Science and Engineering: An Integrated Approach, 3rd ed. New York: Wiley. Chiang, S.-K. 1988. Microstructure Development in Temperature-Stable BaTiO 3. PhD Dissertation. Columbus, OH: Ohio State University. Davidovits. P. et al. 2004. Mass Accommodation Coefficient of Water Vapor on Liquid Water. Geophys. Res. Lett. 31(L22111): 1–4. “Diffusionless transformation.” Wikipedia, The Free Encyclopedia, last modified May 5, 2016. https://en.wikipedia. org/w/index.php?title=Diffusionless_transformatin&oldid=718711113. (accessed July 13, 2016.) Doremus, R. H. 1994. Glass Science, 2nd ed. New York: Wiley, p. 100. Dorn, H. et al. 2013. Unusual Variation of Thickness Within a Pane of Annealed Float Glass. Can. Soc. Forensic Sci. J. 46(3): 166–169. Doyle, P. J., ed. 1979. Glass Making Today. Redhill, UK: Portcullis Press. Eitel, W. 1954. The Physical Chemistry of the Silicates. Chicago, IL: University of Chicago Press. Emsley, J. 1998. The Elements, 3rd ed. Oxford: Oxford University Press. Emsley, J. 2001. Nature’s Building Blocks. Oxford: Oxford University Press. “French invasion of Russia.” Wikipedia, The Free Encyclopedia, last modified June 24, 2016. https://en.wikipedia. org/w/index.php?title=French_invasion_of_Russa&oldid=726728034. (accessed July 13, 2016.) Glass Transition. Wikipedia Encyclopedia. http://en.wikipedia.org/wiki/Glass_transition. “Glass transition.” Wikipedia, The Free Encyclopedia, last modified July 7, 2016. https://en.wikipedia.org/w/ index.php?title=Glass_tansition*oldid=728786909. (accessed July 13, 2016.) Green, D. J., R. H. J. Hannink, and M. V. Swain. 1989. Transformation Toughening of Ceramics. Boca Raton, FL: CRC Press. Haynes, W. M. Editor-in-Chief. 2013. CRC Handbook of Chemistry and Physics, 94th ed. Boca Raton, FL: CRC Press. Inaba, S., H. Hosono, and S. Ito. 2015. Entropic shrinkage of an oxide glass. Nat. Mater. 14(March 15): 312–317. Jones, G. O. 1956. Glass. New York: Wiley. Kingery, W. D. 1959. Surface Tension of Some Liquid Oxides and Their Temperature Coefficients. J. Am. Ceram. Soc. 45(1): 6–10. Kingery, W. D., H. K. Bowen, and D. R. Uhlmann 1976. Introduction to Ceramics, 2nd ed. New York: Wiley. Krauss, G. 1990. Steels: Heat Treatment and Processing Principles. Metals Park, OH: ASM International. Lipschutz, S., M. Spiegel, and J. Liu. 2012. Schaum’s Outline of Mathematical Handbook of Formulas and tables, 4th ed. New York: McGraw-Hill. McClintock, F. A. and A. S. Argon, eds. 1966. Mechanical Behavior of Materials. Reading, MA: AddisonWesley Publishing. References McNaught, A. D. and A. Wilkinson, compilers. 2006. IUPAC. Compendium of Chemical Terminology, 2nd.ed. (the “Gold Book”). London: Blackwell. http://goldbook.iupac.org/G02641.html. Morey, G. W. 1938. The Properties of Glass. New York: Rheinhold Publishing. Morton-Jones, D. H. 1989. Polymer Processing. London: Chapman & Hall. Navrotsky, A. 2011. Nanoscale Effects on Thermodynamics and Phase Equilibria in Oxide Systems. ChemPhysChem. 12:2207–2215. Navrotsky, A. et al. 2010. Nanophase Transition Metal Oxides Show Large Thermodynamically Driven shifts in Oxidation-Reduction Equilibria. Science. 330:199–201. Newnham, R. E. 2005. Properties of Materials. Oxford: Oxford University Press. Pfaender, H. G. 1983. Schott Guide to Glass. New York: Van Nostrand Reinhold. Plumb, R. C. 1989. Antique Window Panes and the Flow of Supercooled Liquids. J. Chem. Ed. 66(12): 994–996. Porter, D. A., K. E. Easterling, and M. Y. Sherif. 2009. Phase Transformations in Metals and Alloys, 3rd ed. Boca Raton, FL: Taylor & Francis Group. Pound, G. M. 1972. Selected Values of Evaporation and Condensation Coefficients for Simple Substances. J. Phys. Chem. Ref. Data. 1: 135–145. Presidential Commission Report on Space Shuttle Challenger Accident. June 1986. http://science.ksc.nasa.gov/ shuttle/missions/51-l/docs/rogers-commission/table-of-contents.html. Reed-Hill, R. E. and R. Abbaschian. 1992. Physical Metallurgy Principles, 3rd ed. Boston, MA: PWS Kent. Roine, A. 2002. Outokumpu HSC Chemistry for Windows, Chemical Reaction and Equilibrium Software with Extensive Thermochemical Database, Version 5.1. Pori, Finland: Outokumpu Research Oy. Roth, R. S. 1995. Phase Equilibrium Diagrams, Phase Diagrams for Ceramists, Volume XI. Washington, DC: National Institute for Standards and Technology. Roy, B. 2006. Development of Copper Strontium Oxide and Recrystallization of Hot Wire Chemical Vapor Deposited Amorphous Silicon Films for Solar Cell Applications. PhD Thesis. Colorado School of Mines, Golden, CO. Scherer, G. W. 1986. Relaxation in Glass and Composites. New York: Wiley. Silbey, R. J. and R. A. Alberty. 2001. Physical Chemistry, 3rd ed. New York: Wiley. Sosman, R. B. 1965. The Phases of Silica. New Brunswick, NJ: Rutgers University Press. Sperling, L. H. 2006. Introduction to Physical Polymer Science, 4th ed. Hoboken, NJ: Wiley. “Tin pest.” Wikipedia, The Free Encyclopedia, last modified 13 May 2016. https://en.wikipedia.og/w/index. php?title=Tin_pest&oldid=720004224. (accessed July 13, 2016.) Van Krevelen, D. W. 1997. Properties of Polymers, 3rd ed. Amsterdam, the Netherlands: Elsevier B. V. Varshneya, A. K. 1994. Fundamentals of Inorganic Glasses. Boston, MA: Academic Press. Video frame from: www.periodictable.ru. (2009 May 2). Grey tin (tin pest) time-lapse video [Video file]. Retrieved from https://www.youtube.com/watch?v=FUoVemHuykM. Viton®. http://www.dupontelastomers.com. Ward, I. M. and D. W. Hadley. 1993. An Introduction to the Mechanical Properties of Solid Polymers. Chichester, England: Wiley. Wells, A. F. 1984. Structural Inorganic Chemistry, 5th ed. Oxford: Oxford University Press. 253 Section IV Diffusion with a Constant Diffusion Coefficient Chapter 8 Fundamentals of Diffusion Chapter 9 Atomistics of Diffusion Chapter 10 Steady-State Diffusion Chapter 11 Solutions to Fick’s Second Law Chapter 12 Diffusion with Finite Boundary Conditions 255 257 275 333 381 413 8 Fundamentals of Diffusion 8.1 8.2 8.3 8.4 Introduction The Process of Diffusion Fick’s First Law of Diffusion Values of Diffusion Coefficients 8.4.1 General 8.4.2 Diffusion in Gases 8.4.3 Diffusion in Solids 8.4.4 Diffusion in Liquids 8.5 Fick’s Second Law of Diffusion (Conservation of Matter) 8.6 Fick’s Second Law Redux 8.7 General Concepts on Solving Diffusion Problems 8.7.1 Infinite Boundary Conditions 8.7.2 Semi-Infinite Boundary Conditions 8.7.3 Finite Boundary Conditions 8.8 Chapter Summary Appendix Exercises References 8.1 257 258 259 260 260 261 262 263 264 265 266 266 267 267 269 269 271 273 INTRODUCTION The process of diffusion—atomic or molecular motion—is central to understanding the kinetics of many processes of interest to the materials scientist or engineer. In fact, the study of diffusion was initially stimulated more by its application to materials than any other field of science or engineering: for example, the heat treatment of steel. The purpose here is to introduce the microscopic mechanisms of diffusion in solids, liquids, and gases, and an elementary rationale given for the differences 257 Chapter 8. Fundamentals of Diffusion in diffusion behavior in various materials. The macroscopic differential equations that are used to describe these kinetic processes are also examined. For these, several diffusion geometries and conditions necessary in quantitatively modeling kinetic processes important to materials are presented, each of which requires a somewhat different mathematical treatment. This chapter serves as an introduction only, and both the microscopic and macroscopic aspects of diffusion are expanded in more detail in later chapters. Furthermore, the order in which the next four Chapters 9 through 12 are presented and studied is more a matter of individual choice than one of instructional necessity. 8.2 THE PROCESS OF DIFFUSION Again, diffusion can be defined as spontaneous intermingling or mixing of atoms, ions, molecules, or particles due to random thermal motion. This intermingling occurs in the solid, liquid, or gaseous state. Figure 8.1 schematically shows the macroscopic results of the microscopic or atomistic processes of diffusion. The diffusion process sketched in Figure 8.1 is pure nitrogen and oxygen of equal amounts initially separated by some kind of barrier, and at t = 0, this barrier is removed without introducing convection allowing the gas molecules to diffuse into each other. In this case of nitrogen and hydrogen, as in all diffusion processes, the kinetic energy of the molecules is determined by the temperature. Even at room temperature, gas molecules have rapid thermal motion—speeds on the order of thousands of miles per hour—and they travel only about 0.1 μm before colliding with another gas molecule. So they experience over a billion scattering collisions per second, which leads to their mixing or randomization. Referring to Figure 8.1, if these are ideal gases, an assumption that will always be made unless otherwise specified, then there is a thermodynamic driving force for the gases to intermingle, the molar ideal Gibbs energy of mixing: ∆G idm = −T∆Smid = RT( X1 ln X1 + X 2 ln X x ) (8.1) where X1 and X2 are the mole fractions of components 1 and 2: nitrogen and oxygen, respectively. Note that the ∆H id for ideal mixing is zero and is a good definition of an ideal solution. This is the thermodynamic equivalent of saying that the molecules are mixing by thermal motion: there is an increase in entropy on mixing. The individual molecules do not know anything about entropy but are mixing because of their random motion. Nevertheless, this can be a convenient way of describing the driving force for diffusion; namely, that the ideal Gibbs energy of mixing is negative. For the interdiffusion of one mole of nitrogen and one mole of oxygen, the ideal Gibbs energy of mixing at 300 K is ∆G idm (300 K ) = 8.314 × 300 × (ln 0.5) = −1729 J /mol. Not much, but enough. Before being allowed to diffuse, the gases are kept in separate chambers so that the concentration in each chamber is 100%. At time t = 0, they are allowed to begin diffusing into each other. When the two gases have completely mixed, t = ∞, and if there were one mole of each, then the final concentration of each is 50 m/o as shown in Figure 8.1. For times 0 ≤ t ≤ ∞, the concentration is a function of distance and time, C(x, t), as shown. For engineers, the interest is: (1) how long is close FIGURE 8.1 tion of time. N2 Distance, x t=0 J(N2) 0 J(O2) Distance, x 0<t<∞ 100 Percent O2 0 C(x, t) 100 Percent 100 Percent 258 50 0 Equilibrium J=0 Distance, x t=∞ Schematic diagram showing the mixing of nitrogen, N2 and oxygen, O2, by diffusion as a func- 8.3 Fick’s First Law of Diffusion enough to t = ∞ so the process can be considered complete and (2) what is the concentration as a function of time and distance, C(x, t). 8.3 FICK’S FIRST LAW OF DIFFUSION Adolf Fick, a German physiologist who was concerned about how fast sodium chloride solutions moved around in the human body, verified the following equation in about 1850, now known as Fick’s first law of diffusion (Cussler 1997; Narasimhan 2004) J = −D dC dx (8.2) where: J is the flux density D is the diffusion coefficient or the diffusivity dC/dx is the concentration gradient. One consistent set of units is Units(J) = mol/cm2 s, Units(D) = cm2/s, and Units(C) = mol/cm3 so Units(dC/dx) = mol/cm4 (or the comparable SI units such as Units(D) = m2/s).* Note that the flux is opposite to the concentration gradient, as is shown in Figure 8.1. Equation 8.2 is for one dimension but, in general, J is a vector and dC/dx is just one component of the gradient vector, ∇C, so, in general, D is a second rank tensor. That is, ∇C J = −D where ∂C ∂C ∂C k i+ j+ ∇C = ∂x1 ∂x 2 ∂x 3 and D11 D = D21 D31 D12 D22 D32 D13 D23 D33 so that J1 = −D11 ∂C ∂C ∂C − D12 −D ∂x1 ∂x 2 ∂x 2 with similar equations for the other two directions. However, in all following discussions, it will be assumed that D is scalar and isotropic; that is, it is the same in all directions. This is, of course, actually true and not just a mathematical simplification for gases, liquids, randomly oriented polycrystalline, and amorphous solids that do not have any crystallographic texture or preferred orientation. If considering diffusion in strongly anisotropic solids such as some single crystals, then it might be necessary to consider the varying components of the diffusion coefficient, but is not a concern here. In the above form, Fick’s first law applies only to thermodynamically ideal solutions† such as two gases, N2 and O2, or two liquids such as ethanol, C2H5OH, and water, or solids such as Cu and Ni, or Al2O3 and Cr2O3. How Fick’s first law changes for nonideal solutions, more typically the case for solids, is examined later. * † = J/cm 2 s = W/cm 2, T is the This is very similar Fourier’s law of heat flow, q = − kdT /dx, where q is the heat flux, Units(q) temperature, and k is the thermal conductivity, Units(k) = W/cm K or W/m K. One in which there is no enthalpy on mixing and the Gibbs energy of mixing is given by Equation 8.1. 259 260 Chapter 8. Fundamentals of Diffusion 8.4 VALUES OF DIFFUSION COEFFICIENTS 8.4.1 General Concentration, C When the atomistic mechanisms of diffusion are discussed later, the reasons for the following temperature and pressure dependences for diffusion coefficients in gases, solids, and liquids will become more apparent. However, for now, the interest is primarily in how and why the diffusion coefficients FIGURE 8.2 Random thermal motion of gas atoms or molecules that travel at high speeds and make in these three phases vary, particularly with temperature, and to get a betmany collision with other atoms/molecules per ter idea of the magnitudes for diffusion coefficients in the different states of second. The distance between collisions, λ, is called matter. Values for diffusion coefficients are found in a number of texts on the mean free path. diffusion and other publications (Cussler 1997). Whether the diffusion or atom motion is in gases, liquids, or solids, it is a random process. Figure 8.2 shows the motion of atoms or molecules λ λ in the gas phase. As was mentioned in Chapter 5, footnote to Section 5.2.2, gas atoms move with very high velocities but they do not travel very far—on the order of 0.1 μm—before colliding with another gas atom or J′ molecule, which alters their directions. The mean distance between the collisions is called the mean free path, λ, for atoms in a gas. Figure 8.2 η(−λ) η(0) η(+λ) shows how the gas atoms move randomly from collision to collision. From this simple picture of atoms or molecules moving at high FIGURE 8.3 Geometry used to calculate the diffusion coefficient in a gas. speeds in the gas phase with a distance between collisions of λ, a very general relationship that applies to diffusion in all states of matter can be easily obtained. Consider the three planes in Figure 8.3, a mean free path distance apart. Gas atoms at −λ traveling to the right will cross the plane at x = 0 before making a collision, and gas atoms at +λ traveling to the left will also cross the plane at x = 0 before making a collision and changing direction. Assume that there is a concentration gradient that decreases going from left to right as shown in Figure 8.4. If η = number of atoms or molecules/cm3 with η(−λ) the concentration at x = −λ and η(+λ) the concentration at x = λ, and J′ = atomic or molecular flux, Units(J′) = atoms/cm2 s, then as was seen in Chapter 5, the flux of atoms crossing a surface can be approximated by* C(−λ) C(x, t) C(0) C(+λ) −λ FIGURE 8.4 * +λ 0 Distance, x Concentration of gas atoms versus distance used to calculate the gas diffusion coefficient. In Chapter 5, it was shown that the correct values were J′ = ηv /4 and the mean distance was (2 / 3)λ from the plane of collision. Substitution of these two values into Equation 8.3 gives exactly the same result: the two errors in the approximation just cancel each other. 8.4 Values of Diffusion Coefficients J′ = I from left − I from right = 1 1 vη ( −λ ) − vη ( +λ ) 6 6 = 1 dη 1 dη λ − η+ v η− λ 6 dx 6 dx (8.3) 2 dη J′ = − vλ 6 dx with the final result 1 dη J′ = − vλ . 3 dx Dividing both sides by Avogadro’s number gives J = −(1/ 3) vλ(dC /dx) and comparing this to Fick’s first law shows that D= 1 vλ 3 (8.4) and is a very general result that can be applied to diffusion not only in gases, but also in solids and liquids. In fact, the difference in values between the diffusion coefficients in solids, liquids, and gases at any given temperature can be reasonably explained by this result. 8.4.2 Diffusion in Gases The diffusion coefficients for gases have very weak temperature dependences. As will be shown in Chapter 9, for gases, 3 D ≅ 10 −4 T2 cm 2 /s p (8.5) where: Units(p) = bar Units(T) = K Note: “≅” is used to denote “approximately equal to.” So for p = 1 bar at 300 K, D ≅ 0.5 cm2/s and at T = 1500 K, D ≅ 6 cm2/s. This only about an order of magnitude change over this temperature range that, compared to solids, is a very small change in D. Also, if you need a back of the envelope value for the diffusion coefficient of a gas, taking D ≅ 1 cm2/s would be within an order of magnitude for most gases at most temperatures. Gases have the largest diffusion coefficients because the diffusion or mixing occurs through collisions of gas atoms moving with high thermal velocities on the order of 500 m/s (1125 mph) and the atoms or molecules can move relatively large distances (relative to solids and liquids), in any direction, on the order of 0.1 μm at room temperature, mainly because of the low density of molecules in the gas. The mean free path for diffusion is, in part, determined by the number of atoms or molecules per cm3. For example, for a gas at room temperature T ≅ 300 K and at one bar (105 Pa) pressure, P, η= n P 105 NA = NA = 6.022 × 1023 V RT (8.314)(300) = 2.41 × 1025 m −3 = 2.41 × 1019 cm −3 261 262 Chapter 8. Fundamentals of Diffusion where: Units(η) = atoms/cm3 or molecules/L, and so on NA = Avogadro’s number. This is where the P term comes from in the denominator of Equation 8.5 and why T ends up in the numerator. The other T1/2 in the numerator comes from the gas mean speed, v = 8RT /πM . The molecules or atoms in a gas experience some 109 collisions per second, which produces rapid mixing and diffusion. If the gas velocity is 5 × 104 cm/s and the mean free path is λ = 3 × 10−5 cm, then D ≈ 0.5 cm/s from the general formula D = (1/ 3)vλ and is consistent with Equation 8.5. 8.4.3 Diffusion in soliDs The situation for solids is very different. In solids, the atoms are very densely packed; take for example copper, with a density of ρ = 8.92 g/cm3 and molecular weight of M = 63.55 g/mol*: η= 8.92 g /cm 3 ρ 6.022 × 1023 = 8.45 × 1022 cm −3 . NA = 63.55 g /mol M Note that in solids the atoms (ions, molecules) are tightly packed, almost like billiard balls, so it makes no difference what type of bonding there is between the atoms in a solid; the number of atoms (ions, molecules) per cm3 is going to be something × 1022 cm−3. The density of solids is some three orders of magnitude higher than the density of gases—in terms of the number of atoms per unit volume—which is one reason that diffusion coefficients in solids are much lower than in gases. For solids, the diffusion coefficient is strongly temperature dependent and follows an Arrhenius equation; namely, D = Do e − Q RT (8.6) where: Do is the pre-exponential, Units(Do) = cm2/s or m2/s, typically close to Do ≅ 10−3 cm2/s Q is the activation energy, Units(Q) = J/mol. For many solids, Q ≅ 100–200 kJ/mol, or more. For example, if Q = 200 kJ/mol, then at room temperature (300 K), −3 D (300 K ) = 10 e − 200,000 8.314 × 300 = 1.5 × 10 −38 cm 2/s. And at 1500 K, D (1500 K ) = 10 −3 e − 200 ,000 8.314 × 1500 = 1.08 × 10 −10 cm 2/s. This is a difference of 28 orders of magnitude over the same temperature range where the gas diffusion coefficient varied by only a factor of 10! Clearly, with such a small diffusion coefficient, there would be no evidence for any diffusion at room temperature. However, at 1500 K, the diffusion coefficient is large enough to see changes in microstructure in reasonable periods of time; 104 seconds, or about 3 hours. So this is a good back of the envelope value for the diffusion coefficient in a solid when property changes occur, D ≅ 10 −10 cm 2 /s. * Or g/g-atom: in either case it is the weight of one Avogadro’s number of the atomic or molecular species. In general, no distinction is made between the two: one “mole” of something is one Avogadro’s number, NA = 6.022 × 1023 molecules (or atoms)/mol). 8.4 Values of Diffusion Coefficients 263 There are two main mechanisms for diffusion in solids: Interstitial (1) interstitial mechanism (Figure 8.5) and (2) the vacancy mechanism (Figure 8.6). Other mechanisms have been postulated and some do occur but only in special cases and will not be considered here because they are not essential to understanding atomistic diffusion in most solids. The interstitial mechanism occurs for carbon and nitrogen in iron, hydrogen in platinum and palladium, oxygen in SiO2 FIGURE 8.5 Interstitial mechanism for diffusion in solids. The small glass, H2O and other gases in polymers. In fact, most diffu- circle represents the interstitial atom and the larger ones are the sion of engineering interest in solid polymers is essentially lattice atoms. interstitial diffusion. The vacancy mechanism is important in all close-packed solids and is the mechanism of diffusion of Cu in Cu; Fe in Fe; O2− in MgO; Si, B, and As in Si; Ga and As in GaAs, and so on. Typically, the activation energy for interstitial diffusion is less than that for vacancy diffusion because only the energy for the atom or ion to move or jump Vacancy from one interstitial site to another is necessary. In contrast, for the vacancy mechanism, the atom must jump, but to do that, a neighboring site must be vacant. The concentration of vacancies also depends exponentially on the temperature FIGURE 8.6 Vacancy mechanism for diffusion in solids. The “square” in the center represents the vacant site or vacancy. and, at a given temperature, there is an intrinsic concentration of vacancies that increases the randomness of the system, the entropy, even though it takes energy to create them. At the melting point of many solids, the fraction of lattice sites that are vacant—also the probability that a single site is vacant—is on the order of 10−4. As a result, the activation energy for vacancy diffusion is the sum of the energy for the atom to jump as well as the energy to form vacancies. This will be explored in some detail in Chapter 9. 8.4.4 Diffusion in liquiDs Liquids fall between solids and gases in that their diffusion coefficients have stronger temperature dependences than gases but much less so than solids. In fact, diffusion in liquids also follows an exponential temperature dependence, D = Doexp(−Q/RT) but the activation energies are on the order of 10–20 kJ/mol. For example, if Q = 10 kJ/mol, at 300 K, −3 D (300 K ) = 10 e − 10,000 8.314 × 300 = 1.8 × 10 −5 cm 2/s and at 1500 K, D (1500 K ) = 10 −3 e − 10,000 8.314 × 1500 = 4.5 × 10 −4 cm 2/s. This is only a factor of 40 different! This is a little larger than for gases but much smaller than the difference in the diffusion coefficients in a solid over the same temperature range. So a good choice for a back-of-the-envelope calculation would be D ≅ 10−5 – 10−4 cm2/s for most liquids. In liquids, the atoms have kinetic energies and velocities similar to the atoms in gases, on the order of 5 × 104 cm/s but they can only move roughly an interatomic distance (about 0.2 nm) before colliding with another atom or molecule. But they also need space to move. When a crystalline solid melts, it increases its volume about 10% or so: so-called free volume. As shown earlier, on melting, for most solids (Si and H2O being notable exceptions), there is an expansion in going from the solid to the liquid state—typically around 10 v/o (volume percent) or more. For example, for copper at its melting point of Tmp = 1083°C, the density of liquid copper is, ρ(Cu, L) = 8.00 g/cm3 (Brandes and Brook 1992) so that the number of atoms per cm3, η, is 264 Chapter 8. Fundamentals of Diffusion η(Cu, L) = 8.0 g /cc ρ 6.022 × 1023 atoms /mol = 7.58 × 1022 atoms /cm 3 NA = 63.55 g /mol M or about 10% less than calculated above for solid copper. Note that the number density is still on the order of 1022 atoms/cm3. This means that the vacancy concentration in a liquid is about 0.1 compared to 10−4 in the solid at the melting temperature. This factor alone contributes three orders of magnitude to the diffusion coefficient in the liquid compared to the solid at the melting point. As a result, there is about 10% more volume for a liquid atom to move around in. So, in any given direction, there is about a 10% chance the atom will have the extra volume in this direction. Thus, 1/3vλ ≈ 1/3 × (5 × 10 4) × (2 × 10−8) × 0.1 ≈ 3 × 10−5 cm2/s. This is a good approximation to the diffusion coefficients in liquids and explains the roughly five orders of magnitude difference in diffusion coefficients between solids and liquids. 8.5 FICK’S SECOND LAW OF DIFFUSION (CONSERVATION OF MATTER) Fick’s second law of diffusion—really the conservation of matter—is derived for the one-dimensional case in a relatively simple graphic way. The volume of the “box” in Figure 8.7 is V = Ah. The number of moles in the box, n, is simply: n = CAh, where C is the concentration in mol/cm3. So the change in the number of moles in the box with time, ∂n /∂t, is just the difference between the flux in the front and the flux out the back: ∂n ∂C = Ah = AJ( x) − AJ ( x + h) ∂t ∂t ∂C J( x + h) − J( x) = − . ∂t h where the partial derivative with respect to time is being used because the flux is given in terms of distance and the change in flux will be a partial derivative with respect to distance, x. The difference between flux out and flux in is what stays inside the box and increases the concentration. Taking the limit as h goes to zero, the right-hand side of this equation is the definition of the derivative of J; that is, lim h →0 J( x + h) − J( x) ∂J = h ∂x Therefore, ∂C ∂J ∂ ∂C =− = − −D ∂t ∂x ∂x ∂x n = number of moles in box A J(x + h) J(x) h x FIGURE 8.7 matter. x+h Schematic used for the derivation of Fick’s second law that is essentially the conservation of 8.6 Fick’s Second Law Redux and if D is a constant, not a function of x, then ∂C ∂ 2C =D 2 . ∂t ∂x (8.7) Equation 8.7 is the one-dimensional form of Fick’s second law that is an expression of the conservation of mass. This is very similar to Fourier’s law for non steady-state heat conduction, ∂T k ∂ 2 T = ∂t ρc ∂x 2 (8.8) where: T is the temperature k/ρc is the thermal diffusivity k is the thermal conductivity (Units(k) = W/cm K) ρ is the density (Units(ρ) = g/cm3) c is the mass heat capacity (Units(c) = J/g-K) so Units (k/ρc) = cm2/s: the same as the mass diffusivity. In many cases, solutions of C(x, t) of Fick’s second law as a function of time and temperature are needed to solve many macroscopic diffusion or mass flow problems. The same is true of T(x, t) in Fourier’s law to determine heat flow. Because these equations have the same form, they have the same solutions. As a result, solutions to these equations can be found in books on either heat or mass transfer (Carslaw and Jaeger 1959; Crank 1975; Glicksman 2000; Wilkerson 2000). 8.6 FICK’S SECOND LAW REDUX A more elegant derivation of Fick’s second law is as follows for those more mathematically passionate. Considering again the box in Figure 8.7—or any volume of arbitrary shape—the total number of moles in the box (volume), n, is simply: n( t ) = ∫ C( x, t )dV V so dn = dt ∫ ∂C dV V ∂t and J = −D∇C assuming that D is a scalar constant. Gauss’ divergence theorem is (Kreyszig 1988) ∫ J ⋅ dA = S ∫ ∇ ⋅ JdV V where dA represents the surface normal so that the integral of the flux parallel to the outwardpointing normal to the surface integrated over the surface is the divergence of the flux integrated over the volume. This becomes dn = dt ∫ ∂C dV = − V ∂t ∫ J ⋅ dA = −∫ S ∇ ⋅ JdV = V ∫ D∇ 2CdV V where ∇2 is the Laplacian operator. The negative sign is necessary because the flux is parallel to the surface normal that points out from the surface of the object. Therefore, ∫ ∂C dV = V ∂t ∫ D∇ 2CdV V 265 266 Chapter 8. Fundamentals of Diffusion or ∫ ∂C − D∇ 2C dV = 0 V ∂t or ∂C = D ∇ 2C ∂t So in three dimensions, Fick’s second law is ∂C = D∇ 2C ∂t (8.9) where ∂ 2C ∂ 2C ∂ 2C + + ∂x 2 ∂y 2 ∂z 2 (8.10) ∂ 2C 1 ∂C 1 ∂ ∂C + = r ∂r 2 r ∂r r ∂r ∂r (8.11) ∇ 2C = in Cartesian coordinates and ∇ 2C = in cylindrical or polar coordinates if there is no angular dependence (i.e., there is only circular symmetry and Equation 8.11 is developed in the Appendix). And in spherical coordinates (again no angular dependence; i.e., there is spherical symmetry and also developed in the Appendix) ∇ 2C = ∂ 2C 2 ∂C 1 ∂ 2 ∂C + = r . ∂r 2 r ∂r r 2 ∂r ∂r (8.12) In future problems where cylindrical, polar, or spherical coordinates are necessary, only the radial dependence on concentration is considered. Adding angular dependences only adds needless complications at this stage of demonstration of principles. 8.7 GENERAL CONCEPTS ON SOLVING DIFFUSION PROBLEMS Solutions to Fick’s second law are necessary and important in a large number of materials science and engineering problems when C(x, t) is required. The approach to solving Equation 8.7 depends on the type of boundary conditions (C(0, t) and C(L, t)) and the initial condition (t = 0 usually) that are necessary to solve a given diffusion problem. Because Fick’s second law has the second derivative with respect to distance and the first derivative with respect to time, two boundary conditions and one initial condition are necessary to solve a given diffusion problem. 8.7.1 infinite BounDary ConDitions For example, a piece of pure Cu and a piece of pure Ni—initial conditions: [Cu(0 ≤ x ≤ ∞, t = 0]* = 0 and [Ni(−∞ ≤ x ≤ 0, t = 0)] = 0—each 10 cm thick are placed in contact with each other at t = 0, as shown in Figure 8.8, and heated to a temperature (maybe around 1000°C) where the interdiffusion coefficient between them D ≅ 10−10 cm2/s. As will be seen in Chapters 11 and 12, a rough estimate of the interdiffusion distance, L, is 4Dt ≅ L2 so the extent of the interdiffusion in this diffusion couple after about 3 hours (∼104 seconds) is about L ≅ 20 μm around the original interface. * Here “[ ]” represents concentration. 8.7 General Concepts on Solving Diffusion Problems At the far ends of each piece (x = −10 cm ≅ −∞ and x = +10 cm ≅ ∞), the composition remains pure Cu and pure Ni, respectively. This is an example of a problem that has infinite boundary conditions in that the Ni and Cu do not have time to diffuse to the opposite ends of the diffusion couple so CCu(∞, t) = 0 and CNi(−∞, t) = 0 remain constant for all reasonable times. Applying the approximation 4Dt ≅ L2, it would take almost 10,000 years for the Cu and Ni to diffuse to the opposite ends of the 10 cm thick pieces at 1000°C! So infinite boundary conditions apply when measureable composition changes never occur at the far ends of diffusion couple. The equations describing the interdiffusion do give changes in concentration at the far ends of the couple but these are well below any measureable level and are simply due to the behavior of the mathematical functions. 8.7.2 semi-infinite BounDary ConDitions t=0 −∞ Cu Ni +∞ x L −∞ [Ni] [Cu] +∞ x t>0 FIGURE 8.8 Pieces of copper, Cu and nickel, Ni, interdiffusing into each other by solid-state diffusion. The size of the pieces is large compared to the distance the atoms of each diffuse, L, during the time allowed for the diffusion to take place. [Cu] is the concentration of copper and [Ni] that of nickel. This is an illustration of infinite boundary conditions. CS [C] t=0 +∞ As might be expected, semi-infinite boundary conditions 0 x are depicted in Figure 8.9 in which there is one end at L CS x = 0 and the other end of the diffusion field extends to +∞ [C(x, t)] [C] infinity. This example might represent a piece of pure iron, C(x, 0) = 0 (an initial condition), into which carbon is being 0 x t>0 diffused from the surface. The carbon activity (concentration) is fixed at the surface, C(0, t) = CS—a finite boundary FIGURE 8.9 Carbon diffusing from a surface concentration, CS, condition—by controlling the pressures of methane, CH4, fixed by the surrounding gas composition and thermodynamics, and hydrogen in the gas phase, for example. Then the total into a piece of iron whose thickness, is large compared “diffusion depth of diffusion L could be estimated by 4Dt ≅ L2 again. distance.” This is a case of semi-infinite boundary conditions. Again L, the depth of diffusion, would be on the order of micrometers for temperatures around 800°C and never reach very deep into the piece of iron. So C(∞, t) = 0 is the boundary condition at x = ∞. These are semi-infinite boundary conditions where one boundary condition is given at a fixed position (x = 0 in this case) and the other is fixed at x = ∞ (or −∞). 8.7.3 267 finite BounDary ConDitions Finite boundary conditions apply when the diffusion extends over the entire spatial region of interest during the time of diffusion. For example, Figure 8.10 represents a piece of relatively pure iron containing some carbon impurities being heat treated in hydrogen to remove the carbon by reaction with the hydrogen to form methane gas at both surfaces at x = 0 and at x = L with the initial conditions that C(x, 0) = C0 throughout the piece of iron. Assume that at t = 0, the hydrogen is introduced into the hot furnace and the carbon content at both surfaces drops immediately to zero (i.e., C(0, t) = C(L, t) = 0) and remain zero for all values of t as shown in the left sketch of Figure 8.10. These are the two finite boundary conditions in this case. As diffusion proceeds, the concentration profiles, C(x, t), change with time as shown in the middle sketch—actually approach sine curves—until finally at t = ∞, the concentration in the sheet has dropped to C(x, ∞) = 0 as shown in the right-hand sketch. The approximation 4Dt ≅ L2 can be used again to estimate how long it will take for the concentration to fall to zero: if L = 1 mm and D = 10 −8 cm 2/s, then t ≅ 2 × 105 seconds or about 70 hours, which is much less than t = ∞. Of course, this is only approximate and the partial differential equation really needs to be solved to determine when the carbon concentration has fallen to an acceptable level say, 0.01%, or whatever is necessary for the application of the carbon-free iron sheet: iron cores for special transformers is one application of carbon-free iron. 268 Chapter 8. Fundamentals of Diffusion C0 t1 C0 [C] [C] 0 t2 > t1 C0 [C] 0 L t=0 0 L 0<t<∞ L t=∞ FIGURE 8.10 Finite boundary conditions where the concentrations for all times are specified at x = 0 and at x = L. In this case, C(0, t) = C(L, t) = 0. The interdiffusion of nitrogen and oxygen, shown in Figure 8.1, is also a finite boundary condition problem. However, in this case, the boundary conditions are ∂[ N 2 ] ∂[ N 2 ] (0, t ) = ( L, t ) = 0. ∂x ∂x That is, the flux of nitrogen at both ends of the box is zero because J(N 2 ) = −D(∂[ N 2 ]/∂x). The same boundary conditions also apply for oxygen. These boundary conditions basically imply that neither the nitrogen nor the oxygen can leave the box of width L so that their fluxes at x = 0 and x = L are zero. These are derivative boundary conditions but still are finite boundary conditions. For finite boundary conditions, the solutions to Fick’s second law are of the form, C(x, t ) = f (x) + g(x, t ) where f(x) is a function of distance only and is either the equilibrium concentration or the steadystate concentration, and g(x, t) is called the transient part of the solution, where g(x, ∞) = 0, meaning that the transient disappears with time. In Figures 8.1 and 8.10, the transient terms are shown in the center sketches. In the right-hand sketch of both figures, the transient has gone to zero and only the equilibrium concentrations of C(x, ∞) = 0.5 remain in Figure 8.1 and C(x, ∞) = 0 in Figure 8.10. Note, that when equilibrium is reached, J = −D dC =0 dx which implies that dC/dx = 0. In contrast, however, in the steady state ∂C/∂t = 0, which means that ∂ 2C =0 ∂x 2 which can be integrated to give C(x). It is extremely important to note the difference between equilibrium and steady state! Steady state means that there is a concentration gradient and a resulting diffusion flux but the concentration does not change with time, ∂C/∂t = 0. While equilibrium implies that there is no concentration gradient or diffusion flux, so dC/dx = ∂C/∂x = 0. The difference between the two situations will become clearer when finite boundary condition diffusion problems are analyzed in Chapter 12. Appendix 8.8 269 CHAPTER SUMMARY The purpose of this chapter is to introduce concepts related to modeling diffusion at both the macroscopic and atomistic levels. Fick’s first law is introduced for ideal solutions, and the physical implications of the law are discussed for atoms moving in solids, liquids, and gases. The temperature dependences for diffusion coefficients in solids, liquids, and gases are qualitatively summarized as approximate values and are, in fact, very good estimates for diffusion coefficients lacking any other information. Chapter 9 models the atomistic mechanisms of diffusion in gases and solids in detail and justifies the form of the diffusion coefficients given in this chapter. The details of the diffusion in liquids are given in Chapter 13. Fick’s second law, conservation of mass, is derived for various coordinate systems. Solutions to Fick’s second law, C(x, t), that give the concentration as a function of time and distance, are typically obtained by the materials scientist of engineer with various mathematical techniques to solve the partial differential equation: ∂C /∂t = D ∂ 2C /∂x 2. These solutions depend strongly on the initial conditions and the type of boundary conditions for the model: infinite, semi-infinite, or finite boundary conditions that are defined in terms of the concentrations at the boundaries of the diffusion zone. Here, only the definitions of these terms are introduced, while Chapters 11 and 12 develop some exact and approximated methods of solving these equations. In between, in Chapter 10, steady-state solutions to the diffusion equations are modeled for a wide variety of materials applications in which diffusion plays an important role. APPENDIX A.1 fiCk’s seConD law in Polar or CylinDriCal CoorDinates The geometry for developing Fick’s second law in cylindrical coordinates is given in Figure A.1. Again, only the partial differential equation for change in the r direction will be considered because for the diffusion models here there is no interest in the angular dependence. In this case, the hollow cylinder has a height L, an inner radius of r, and an outer radius of “r + h” or a wall thickness of h that is considered to be very small. The volume of the cylinder is Vcyl ≅ 2πrLh because h is small. The total number of moles of whatever is diffusing, n, in the cylinder is n = VcylC ≅ 2πrLhC where C is the concentration: Units(C) = mol/cm3. So, ∂n ∂C = 2πrhL ∂t ∂t (A.1) Also, the change in the number of moles is the difference between the flux in and the flux out: ∂n = A( r ) J( r ) − A( r + h )J ( r + h ) ∂t ∂n = 2πrLJ( r ) − 2π( r + h)LJ( r + h) ∂t where: A(r) is the inner area of the cylinder A(r + h) is the outer area. n = moles in shell r+h J(r+h) (A.2) h r L FIGURE A.1 Geometry for deriving Fick’s second law in cylindrical coordinates. 270 Chapter 8. Fundamentals of Diffusion Equating Equations A.1 and A.2 gives ∂C ( r + h)J( r + h) − rJ( r ) = − ∂t h (A.3) ( r + h)J( r + h) − rJ( r ) ∂ = {rJr} lim h ∂r h →0 (A.4) r and where Equation A.4 is the definition of the derivative of rJ(r). Equating Equations A.3 and A.4 and substituting J = −D(∂C /∂r ) gives r ∂C ∂ ∂C = D r ∂t ∂r ∂r and the desired result of ∂C D ∂ ∂C = r . r ∂r ∂r ∂t a.2 (A.5) fiCk’s seConD law in sPheriCal CoorDinates Figure A.2 shows the geometry for the same derivation in spherical coordinates, again not worrying about angular dependence. In this case, the volume considered is a spherical shell of thickness h. Following the same procedure as above, n = VshellC ≅ 4πr 2 hC (A.6) ∂n ∂C = 4πr 2 h ∂t ∂t Again, the change in the number of moles is the difference between the flux in and the flux out: ∂n = A ( r ) J( r ) − A ( r + h )J ( r + h ) ∂t (A.7) ∂n = −4π ( r + h)2 J( r + h) − r 2 J( r ) ∂t { } and equating Equations A.6 and A.7 gives r2 ( r + h )2 J ( r + h ) − r 2 J ( r ) ∂C = − ∂t h (A.8) and in the limit as h → 0, Vshell = 4πr2h y n = moles in shell r x J(r) ( r + h ) 2 J ( r + h ) − r 2J ( r ) ∂ 2 r J( r) . = lim h ∂r h →0 { } (A.9) Equating Equations A.8 and A.9 and substituting J = −D(∂C /∂r ) gives J(r+h) r2 h ∂C ∂ ∂C = D r2 ∂t ∂r ∂r and the desired result of FIGURE A.2 Geometry for deriving Fick’s second law in spherical coordinates. ∂C D ∂ 2 ∂C = r . ∂t r 2 ∂r ∂r (A.10) Exercises EXERCISES 8.1 The experimentally measured diffusion coefficients as a function of temperature for hydrogen diffusion in SiO2 glass are given in the table below a. Plot of log10 D versus 1/T (K−1) T (°C) 100 200 300 400 500 600 700 800 900 1000 1100 1200 1300 1400 1500 Hydrogen Diffusion in SiO2 T (K) D (cm2/s) 373 8.10 × 10−10 473 9.99 × 10−9 573 3.22 × 10−8 673 2.58 × 10−7 773 3.20 × 10−7 873 1.50 × 10−6 973 4.21 × 10−6 1073 4.54 × 10−6 1173 6.85 × 10−6 1273 7.19 × 10−6 1373 1.30 × 10−5 1473 1.68 × 10−5 1573 3.32 × 10−5 1673 2.56 × 10−5 1773 2.85 × 10−5 b. From these data, calculate Q (kJ/mol) with a least squares fit to the data c. From these data, calculate D0 (cm2/s) 8.2 The temperature dependence of the diffusion coefficient for the p-type dopant aluminum in silicon single crystal is given by D = D0exp(− Q/RT), where D0 is the pre-exponential term of 0.5 cm2/s and Q is the activation energy of 289.5 kJ/mol. Plot on a semi-log scale the diffusion coefficient of Al in silicon, log10D(cm2/s), from 500°C to 1500°C versus 1/T (K−1) 8.3 a. The temperature dependence of the diffusion coefficient for He in polypropylene is given by D = D0exp(− Q/RT), where D0 is the pre-exponential term = 4.1 cm2/s and Q is the activation energy of 30.5 kJ/mol. Calculate the He diffusion coefficient (cm2/s) at both 30°C and 100°C b. Similarly, for the diffusion of H2O in polyethylene, D0 is the pre-exponential term of 0.028 cm2/s and Q is the activation energy of 24.3 kJ/mol. Calculate the H2O diffusion coefficient (cm2/s) at both 30°C and 100°C 8.4 Cobalt, melting point 1495°C, oxidizes under certain oxygen pressures to CoO, cobalt monoxide. Given below are the diffusion coefficients for cobalt and oxygen ions in CoO as a function of temperature Diffusion in Cobalt Oxide T (°C) 750 800 D(Co) cm2/s 4.54E−11 1.03E−10 D(O) cm2/s 2.07E−19 1.83E−18 850 900 950 1000 1050 1100 1150 1200 2.18E−10 4.31E−10 8.08E−10 1.44E−09 2.46E−09 4.04E−09 6.41E−09 9.85E−09 1.33E−17 8.13E−17 4.30E−16 2.00E−15 8.24E−15 3.07E−14 1.04E−13 3.26E−13 (Continued) 271 272 Chapter 8. Fundamentals of Diffusion Diffusion in Cobalt Oxide T (°C) 1250 1300 1350 1400 1450 D(Co) cm2/s 1.47E−08 2.14E−08 3.05E−08 4.25E−08 5.81E−08 D(O) cm2/s 9.46E−13 2.56E−12 6.54E−12 1.58E−11 3.61E−11 a. Plot the diffusion coefficients (all of the points in the above table) for both cobalt and oxygen on the same semi-log plot of log10D versus 103/T (K−1) b. From the plot in (a), calculate D0 (cm2/s) and Q (J/mol) for the diffusion of both cobalt and oxygen ions in CoO c. The diffusion of which of the two ions controls the rate of oxidation of cobalt and explain why 8.5 The experimentally measured diffusion coefficients as a function of temperature for oxygen interstitial diffusion in SiO2 are given in the table below Oxygen Diffusion in SiO2 T (°C) 500 600 700 800 900 1000 1100 1200 1300 1400 1500 T (K) 773 873 973 1073 1173 1273 1373 1473 1573 1673 1773 D (cm2/s) 5.5E−16 4.9E−14 1.2E−12 1.3E−11 8.6E−11 3.9E−10 1.3E−9 3.6E−9 8.6E−9 1.8E−8 3.4E−8 a. Plot log10D (cm2/s) on a semi-log plot versus 1/T (K−1) b. From these data, calculate D0 (cm2/s) and Q (kJ/mol). (Note: use a least squares fit to the data.) 8.6 The temperature dependence for the interstitial diffusion of carbon in iron is given by D = D0exp(− Q/RT) where D0 = 4 × 10−3 cm2/s and the activation energy Q = 80.1 kJ/mol. Plot log10D (cm2/s) for carbon in iron versus 1/T (K−1) from 0°C to 1500°C 8.7 The experimentally measured diffusion coefficients as a function of temperature for the diffusion of phosphorus in silicon are given in the table below Diffusion of P in Si Temperature (°C) 500 600 700 800 900 1000 1100 1200 1300 1400 D (cm2/s) 6.00E−24 2.10E−21 4.26E−19 2.75E−17 7.26E−16 2.21E−14 1.42E−13 9.50E−13 7.24E−12 3.15E−11 References a. Plot D (cm2/s) on a semi-log plot (or log10D) versus 1/T (K−1) b. From these data, calculate D0 (cm2/s) and Q (kJ/mol). (Note: use a least squares fit to the data.) 8.8 The experimentally measured diffusion coefficients as a function of temperature for Ni and Fe vacancy diffusion coefficients in NiO at low iron concentrations are given below. T (°C) 500 600 Ni in NiO Fe in NiO D (cm2/s) 1.41E−16 2.79E−17 3.80E−15 9.49E−16 700 5.21E−14 1.56E−14 800 4.39E−13 1.53E−13 900 2.57E−12 1.01E−12 1000 1100 1.14E−11 4.06E−11 4.97E−12 1.94E−11 1200 1.22E−10 6.29E−11 1300 3.19E−10 1.76E−10 1400 7.42E−10 4.33E−10 1500 1.57E−09 9.67E−10 a. Plot log10D (cm2/s) on a semi-log plot versus 1/T (K−1) for both Ni and Fe on the same plot b. From these data, calculate D0 (cm2/s) and Q (kJ/mol) for the diffusion of both Ni and Fe in NiO REFERENCES Brandes, E. A. and G. B. Brook. 1992. Smithells Metals Reference Book, 7th ed. Oxford, UK: ButterworthHeinemann, Ltd. Carslaw, H. S. and J. C. Jaeger. 1959. Conduction of Heat in Solids, 2nd ed. Oxford, UK: Oxford University Press. Crank, J. 1975. The Mathematics of Diffusion, 2nd ed. Oxford, UK: Clarendon Press. Cussler, E. L. 1997. Diffusion, Mass Transfer in Fluid Systems, 2nd ed. Cambridge, UK: Cambridge University Press. Glicksman, M. E. 2000. Diffusion in Solids. New York: Wiley. Kreyszig, E. 1988. Advanced Engineering Mathematics, 6th ed. New York: Wiley. Narasimhan, T. N. 2004. Fick’s insights on liquid diffusion, Eos. Trans. Am. Geophys. Union 85[47] November 2004: 499–501. Wilkerson, D. S. 2000. Mass Transport in Solids and Fluids. Cambridge, UK: Cambridge University Press. 273 9 Atomistics of Diffusion 9.1 9.2 9.3 9.4 Introduction Energy Absorption in Molecules and Solids Interstitial Diffusion in Solids 9.3.1 Atom Fluxes 9.3.2 Jump Frequency, Γ 9.3.3 Vibration Frequency, F 9.3.3.1 Example: Iron, Fe 9.3.3.2 Example: Copper, Cu 9.3.3.3 Quantized Vibrations 9.3.3.4 Velocity of Sound 9.3.4 Putting It All Together 9.3.5 Interstitial Jumps per Second, Velocity Vacancy Mechanism of Diffusion in Solids 9.4.1 Vacancy Diffusion 9.4.2 Vacancies in Elements (Metals, Ge, Si, etc.): Statistical Approach 9.4.3 Regular Solution Approach 9.4.4 Vacancy Concentrations 9.4.4.1 Fractions Not Concentrations 9.4.4.2 Example: Copper at Its Melting Point, 1083°C 9.4.4.3 Example: Silicon at Its Melting Point, 1410°C 275 277 278 279 279 280 281 281 282 282 282 283 283 284 284 284 286 286 286 287 288 276 Chapter 9. Atomistics of Diffusion 9.4.5 9.5 9.6 Vacancies, Quasichemical Approach: Point Defect Chemistry 9.4.5.1 In an Element 9.4.5.2 Very Small ∆GV 9.4.6 Charges of Point Defects in Compounds and Kröger–Vink Notation 9.4.6.1 Rationale 9.4.6.2 Kröger–Vink Notation 9.4.6.3 Charge Relative to the Perfect Crystal 9.4.7 Intrinsic Point Defects in Compounds 9.4.7.1 Intrinsic and Extrinsic Defects 9.4.7.2 Schottky Defects 9.4.7.3 Example: Vacancy Concentrations in NaCl at Its Melting Point 9.4.7.4 Schottky Defects in Al2O3 9.4.7.5 Example: Vacancy Concentrations in Al2O3 at Its Melting Point 9.4.7.6 Frenkel Defects 9.4.8 Back to the Vacancy Diffusion Coefficient 9.4.8.1 Example: Diffusion in Cu 9.4.8.2 Example: Diffusion in NaCl 9.4.8.3 Example: Diffusion in Al2O3 9.4.9 Additional Comments About Vacancy Diffusion 9.4.9.1 Vacancy Jumps and Vacancy Diffusion Coefficient 9.4.9.2 Sources and Sinks for Vacancies 9.4.10 Extrinsic Diffusion 9.4.11 Nonstoichiometry 9.4.11.1 General Concept 9.4.11.2 Example: Nonstoichiometry in Fe2O3 Other Diffusion Processes and Solids 9.5.1 Inorganic Glasses 9.5.2 Diffusion in Polymers 9.5.3 Diffusion in a Variety of Solids 9.5.4 Surface and Grain Boundary Diffusion Diffusion in Gases 9.6.1 The Diffusion Coefficient 288 288 289 290 290 291 291 292 292 292 295 295 296 297 298 299 299 299 302 302 302 302 305 305 306 307 307 308 309 310 311 311 9.1 Introduction 9.6.2 9.6.3 Mean Free Path in a Gas The Gas Diffusion Coefficient 9.6.3.1 Example 1: He and Ar Interdiffusion at 298 K 9.6.3.2 Example 2: H2O in N2 at 298 K and 1 bar 9.6.4 The Chapman–Enskog Equation 9.6.5 Knudsen Diffusion 9.7 Diffusion in Liquids 9.8 Chapter Summary Appendix Exercises References 9.1 312 313 314 314 314 316 317 318 319 328 330 INTRODUCTION In this chapter, simple atomistic models of the mechanisms of diffusion in solids, gases, and liquids are modeled and related to the macroscopic parameters: diffusion coefficients—or diffusivities. The mechanisms in solids and gases are relatively easy to model and give quantitative results consistent with experimentally measured values of diffusion coefficients. For gases, relatively straightforward models give calculated results within 10%–20% of measured values. For solids, it is demonstrated that a simple Arrhenius relationship holds for the diffusion coefficient D = D0e − Q RT (9.1) and plausible arguments about the temperature dependence are made without actually being able to calculate actual values of Q. This would require considerably more sophisticated modeling involving interatomic bonding and other parameters. Nevertheless, the approximate models give values of D0 that are reasonably close to those measured in systems where diffusion is well-characterized; that is, where the experimental data are pretty good. Liquids are harder to model and the atomistic concepts fall between those for solids and gases. The Stokes–Einstein model for liquids is readily modeled—except for the fluid dynamics part—and gives reasonable quantitative results for diffusion in liquids. This is discussed later in Chapter 13. However, a plausibility argument will be given in this chapter for the diffusion in liquids. The atomistic models presented here are relatively simple but include and illustrate all the important principles involved in atomic or molecular diffusive motion. More sophisticated models, of which there are many, take into consideration correlations with other experimental data that reflect more details about interatomic bonding, electronic structure, and molecular size and their interactions. These models have more precise agreement with experiment but without adding many new principles. These detailed models typically involve advanced mathematical and computational techniques and some physics above the level of this book and are good examples of the application of “computational materials science.” At this point in understanding diffusion processes, the simple models are all that are necessary to explain why diffusion coefficients are different for solids, liquids, and gases and how they vary with temperature, pressure, and composition. 277 278 Chapter 9. Atomistics of Diffusion 9.2 ENERGY ABSORPTION IN MOLECULES AND SOLIDS As discussed in Chapter 5, the kinetic energy in the x-direction, KEx, for a moving atom is simply = KE x 1 1 = mv 2x k BT. 2 2 (9.2) Again, the velocity vector has three components in the x, y, and z direction, so v2 = v2x + v2y + v2z and the total kinetic energy, KE, is given by KE = 1 1 1 1 mv 2 = mv 2x + mv 2y + mv 2z 2 2 2 2 1 1 1 3 = k BT + k BT + k BT = k BT. 2 2 2 2 (9.3) The second of these last two equations is a statement of the principle of equipartition of energy (Silbey and Alberty 2001), which essentially says that the microscopic modes for absorbing energy all have the same energy, (1/2)kBT, when in thermal equilibrium. For a monatomic gas, the only energy-absorbing modes are translational energies in the three directions leading to KE = (3/2)kBT in Equation 9.3 and the RMS—root mean square—speed, vrms, of gas molecules is = v rms 3k BT = m 3RT M (9.4) and the mean speed, v v= yz-plane rotation Vibration xy-plane rotation z Diatomic gas molecule z y x y x x, y, z vibrations Atom in solid FIGURE 9.1 Diatomic molecule showing both rotational and vibrational modes of energy absorption and an atom in a solid showing three vibrational modes. 8RT πM (9.5) where M is the molecular or atomic weight (kg/mol) (Chapter 5). For diatomic molecules such as H 2 , N2 , O2 , and so on, there are other mechanisms for absorbing energy as indicated in Figure 9.1. These molecules have two degrees of rotational freedom each of which contribute (1/2)k BT to the total energy of the molecule. In addition, the molecules can change their separation distance and vibrate very much like two masses at the ends of a spring—the chemical bond. For vibrations, or a moving mass on a spring, there are both kinetic energy of the motion and the potential energy of the stretched spring. As a result, the vibrational energy contribution is (1/2)k BT for each of these energy-absorbing modes or k BT total for each vibrational mode. These are also examples of the equipartition of energy among the various energy-absorbing modes. So, the total energy of a diatomic molecule would be as follows: energy = kinetic + rotational + vibrational = (3/2)k BT + 2 × (1/2)k BT + k BT = total of (7/2)k BT per molecule or (7/2) RT per mole of gas. For molecules with more atoms, the number of vibrational modes increases as the number of atoms increases. However, both the vibrational and rotational modes are quantized and the vibrational modes, in particular, do not contribute much at low temperatures, particular for light or strongly bonded atoms such as H 2 . 9.3 Interstitial Diffusion in Solids 279 The molar heat capacity at constant volume, CV, is given by (Chapter 1) ∂U ∂Q CV = = ∂T V ∂T V (9.6) so the molar heat capacity at constant volume for argon should be CV (Ar ) = (3/2)R = 12.47 J/K and that is what is used in databases (Haynes 2013). For Cl 2 at 1000 K, the experimental value is 29.325 J/K and very close to the theoretical value of (7/2)R is 29.099 J/K (Stull and Prophet 1971). For solids that are strongly bonded—ionic, metallic, or covalent—neglecting the small contributions that the electrons make to the heat capacity of metals, the only energy-absorbing motions are atomic or ionic vibrations in each of three directions that give rise to a total energy per vibrating atom or ion of 3kBT or a molar heat capacity of 3R = 24.94 J/K per Avogadro’s number of atoms or ions. The heat capacity of solids was discussed in Chapter 7. However this latter point is re-emphasized because it is something not always appreciated. As noted in Chapter 7, the heat capacity per mole for a compound such as Al2O3 depends on the number of atoms/ions in the chemical formula, in this case five. Therefore, the molar heat capacity of copper (with one atom per molecule) should be 24.94 J/K and is experimentally found to be 24.45 J/K at 300 K (Stull and Prophet 1971). However, Al2O3 contains 5NA ions per mole, so its molar heat capacity should be 5 × 24.94 = 124.7 J/K and is found to be 124.74 at 1000 K (Stull and Prophet 1971). These heat capacities of copper and alumina were chosen at a sufficiently high temperature, so quantum effects are no longer affecting heat capacity. A molar heat capacity at constant volume of 3R for metals is known as the law of Dulong and Petit in older literature (Darken and Gurry 1953). 9.3 9.3.1 INTERSTITIAL DIFFUSION IN SOLIDS Atom Fluxes Interstitial diffusion in solids can be simply modeled. In Figure 9.2 interstitial atoms are diffusing with a net flux to the right in a simple cubic lattice.* The spacing between the planes is a, the lattice parameter. Consider planes 1 and 2, where the interstitial atoms lie. As depicted in the figure, the interstitial atoms are vibrating both forward and backward in all three directions. The number of atoms per unit area in plane 1 is n1 (Units(n) = atoms/cm2) and the number interstitial atoms in plane 2 is n2. Then, the number flux density—J′, Units(J′) = atoms cm–2 s–1—of atoms moving from plane 1 → 2 is J1′→2 = n1Γ 6 (9.7) where Γ is the number of jumps from one interstitial site to another per second for an atom, the jump frequency, with Units(Γ) = s−1 and the 1/6 comes from the fact that the atom can jump in any of the six possible directions. Similarly, the flux of atoms going from 2 → 1 is 6 jump directions * Polonium is the only element that has a simple cubic lattice at room temperature (transforms to rhombohedral at 36°C) and atmospheric pressure; a radioactive element discovered and named by Madame Curie (Figure 9.3) (Emsley 1998). She was the first person—and one of the few—to be awarded two Nobel prizes in science, one in physics in 1903 with her husband Pierre and Antoine Becquerel for their discovery of radioactivity, which she named. She received a second Nobel Prize in chemistry in 1911 for her discovery of polonium and radium. She called the element polonium after Poland, where she was born Marja Sklodowska in 1867 (Quinn 1995). Sadly, both she and her daughter, Irène Joliot-Curie, died of leukemia caused by radiation, and in the case of Irène, it was thought to 210 be due to an explosion of a vial of polonium some 15 years earlier (Emsley 2001). Polonium 210, 84 Po, is highly radioactive with a half-life of 138 days (Emsley 1998) and has been suspected as being used in several political assassinations. It is also found in tobacco plants and was thought to be a possible cause of lung cancer from smoking. Interstitial z y x a 1 2 FIGURE 9.2 Model of interstitial atoms diffusing in a simple cubic crystal. 280 Chapter 9. Atomistics of Diffusion J′2→1 = n 2Γ 6 (9.8) and the net number flux moving from plane 1 to plane 2 is given by J′ = J1′→2 − J′2→1 = n1Γ n 2Γ Γ − = ( n1 − n 2 ) 6 6 6 (9.9) The concentrations, Units(C) = mol/cm3, are given by C1 = n1 /(aN A ) and C2 = n 2 /(aN A ), and because the spacing between the planes is very small, a, C2 = C1 + a(dC /dx). Putting in the values for the concentrations in Equation 9.9 gives J′ = FIGURE 9.3 A young Marie Curie. (Wikimedia Commons, Public Domain Photograph, https://commons.wikimedia. org/wiki/File:Marie_Curie_1903.jpg.) = Γ Γ ( n1 − n 2 ) = ( aN A C1 − aN A C2 ) , 6 6 ΓaN A ΓaN A dC ( C1 − C2 ) = C1 − C1 + a 6 6 dxx =− (9.10) Γ a 2 N A dC 6 dx Dividing Equation 9.10 by Avogadro’s number, NA, the molar flux density, J, is given by J= J′ Γ a 2 dC . =− NA 6 dx (9.11) Comparison of Equation 9.11 with Fick’s first law, J = −D(dC/dx), the diffusion coefficient, D, is given by D= Γa 2 6 (9.12) which is a general expression for the diffusion coefficient. In fact, this could be written as D= Γa 2 1 a 1 = (Γa ) = vλ 6 3 2 3 (9.13) as was seen earlier for the case of a gas, where v is the speed = Γa, because Units(Γa) = cm/s and a λ = a/2 the mean distance during a jump because λ = (1/ a) ∫ 0 x dx = a 2 /(2a ) = a / 2 . Again, this shows that Equation 9.13 is a very general relation that applies to diffusion in solids, liquids, and gases. 9.3.2 Jump Frequency, Γ G* What is the jump frequency, Γ? To jump from plane 1 to plane 2, an interstitial atom has to move between at least four atoms, where it does not fit as well as in the interstitial site. This takes a certain amount of energy, ΔG*, an activation energy as shown in Figure 9.4. Alternatively, as discussed in Section 4.7.1 during reaction rates, only a certain number of atoms, n* ΔG* 1 2 n n*; ∆G * on a given plane have enough energy to jump. And from the equilibrium constant for Equation 9.14, x FIGURE 9.4 Activation barrier ΔG* that must be overcome by an atom moving from plane 1 to plane 2 in a crystal lattice. (9.14) n* = ne − ∆G* RT . (9.15) Because this is the energy necessary to move, rename ΔG* = ΔGm, and ΔGm is the energy for motion of the interstitial atoms. 9.3 Interstitial Diffusion in Solids 281 The next part of the question that needs to be answered is as follows: “How often do the atoms jump over the barrier into the next interstitial site?” The answer to this is depends on how often they attempt to get over the barrier. The number of attempts per second is taken to be the vibrational frequency of the atoms on their sites in the crystal, f, the same vibrations that contribute to the heat capacity. This is reasonable because the atoms on plane 1 that move per second, Γ, is just the number of jump attempts per second, f, times the probability that an atom has enough energy to jump, exp(− ∆G m /RT). 9.3.3 VibrAtion Frequency, f Atoms vibrate on their lattice or interstitial sites as shown schematically in Figure 9.5. This leads to the differential equation for the vibrational motion: ma = F or m d 2x = −βx dt 2 (9.16) where β is the spring constant ((2β)/2, because one spring is compressed, whereas the other is extended), Units(β) = N/m. The solution to Equation 9.16 is either x = x0sin(ωx) or x = x0cos(ωx) (Appendix A.1), where the angular frequency ω = 2πf and f is the frequency, Units(f) = cycles/s = Hz. Substitution of either the sine or cosine solution into Equation 9.16 gives − mx 0ω2 sin(ωx) + β sin(ωx) = 0 (9.17) leading to ω2 = β/m, or, because f = ω/(2π), f= ω 1 β . = 2π 2π m (9.18) To estimate f, a value for β is needed. This can be approximated from an elastic constant, Young’s modulus, E: σ = εE, where σ is the stress (Units(σ) = Pa), ε the strain, and E the Young’s modulus (Units(E) = Pa). From Equation 9.16, F = βx and dividing both sides by a2, because x/a is the strain, ε, F βx β = = σ = ε = Eε a2 a a a or β = aE (9.19) where a is the interatomic separation. 9.3.3.1 Example: Iron, Fe For iron, η( Fe) = (ρ/M ) N A = (7.86 g/cm 3 / 55.847 g/mol) 6.022 ×1023 = 8.48×1022 cm −3 = 8.48 × 1028 m −3 is the number of iron atoms per m3. And an approximation to the interatomic spacing is given by a ≅ 1/ (η1/3 ( Fe)) = 1/ (8.48 × 1028 )1/ 3 = 2.28 × 10 −10 m. Young’s modulus for iron is E = 211.4 × 109 Pa (Brandes and Brook 1992), so β = aE = (2.28 × 10−10 m)(211.4 × 109 N/m2) = 48.12 N/m. The mass per atom of iron is M/NA = 55.847 × 10−3 kg/mol/(6.022 × 1023 atoms/ mol) = 9.27 × 10−26 kg/atom. Therefore, f= 1 β 1 48.12 N/m = = 3.6 × 1012 s−1 (Hz). 2π m 2π 9.27 × 10 −26 kg x β/2 Fixed a m 0 β/2 a Fixed FIGURE 9.5 An atom of mass “m” vibrates horizontally between its two nearest neighbors at a distance a with a spring constant on each side of β/2 and moved from its equilibrium position a distance x. The two adjacent atoms are assumed to not move. 282 Chapter 9. Atomistics of Diffusion 9.3.3.2 Example: Copper, Cu For copper, η(Cu) = (ρ /M)N A = (8.92 g/cm 3 / 63.546 g/mol) × 6.022 × 1023 = 8.44 × 1022 cm −3 == 88.44 .44 ×× 1028 m −3 28 –3 3 10 m is the number of copper atoms per m . Again, an approximation to the interatomic spacing can be given by a ≅ 1/ (η1/ 3 (Cu)) = 1 / (8.44 × 1028 )1/ 3 = 2.28 × 10 −10 m. Young’s modulus for copper is E = 129.8 × 109 Pa (Brandes and Brook 1992), so β = aE = (2.28 × 10−10 m)(129.8 × 109 N/m2) = 29.69 N/m. The mass per atom of copper is M/NA = 63.546 × 10−3 kg/mol/(6.022 × 1023 atoms/mol) = 1.055 × 10−25 kg/atom. Therefore, f= 1 β 1 29.69 N/m = = 2.53 × 1012 s −1 ( Hz ) 2π m 2π 10.55 × 10 −26 kg These two calculations suggest that the vibrational frequency is on the order of 3 × 1012 Hz. 9.3.3.3 Quantized Vibrations Another approach to approximating the vibrational frequency is from quantized vibrations. From above, the total energy for a vibrational mode is E x = (1/2)k BT + (1/2)k BT = k BT. Einstein quantized the atomic vibrations and assumed that all the vibration frequencies were the same—as Max Planck had quantized radiation waves—to successfully explain the fact that the heat capacity of solids approached zero as the absolute temperature approached zero. This leads to a quantized energy of vibration: E = hf = kBθE, where θE = Einstein temperature—determined experimentally—and h = 6.64 × 10−34 Js is Planck’s constant. Debye modified Einstein’s theory of heat capacity noting that the atoms could not vibrate independently, because they are coupled together by interatomic forces (springs), and there must be a series of vibration wavelengths or frequencies up to some maximum frequency, hfmax = kBθD, where θD is the Debye temperature, as sketched in Figure 9.6. The Debye theory models reality better than Einstein’s, and the Debye temperatures of a number of solids have been measured and are available (Gray 1972). So, the maximum vibrational frequencies of atoms in solids can be obtained from the Debye temperatures: θD(Fe) = 467 K, θD(Cu) = 343 K (Gray 1972), so f max ( Fe) = ( ) 1.38 × 10 −23 J/K ( 467 K ) k Bθ D = 9.74 × 1012 Hz = h 6.62 × 10 −34 Js and for copper z f max (Cu ) = x 9.3.3.4 ( ) 1.38 × 10 −23 J/K ( 343 K ) k Bθ D = 7.15 × 1012 Hz. = h 6.62 × 10 −34 Js Velocity of Sound The vibrational frequency can also be calculated from the velocity of sound in a solid, because (Appendix A.2): λmin FIGURE 9.6 A few vibration modes of coupled atoms used in the Debye model of heat capacity. The bottom mode has the smallest wavelength, λmin, or the highest frequency. v= E = λf ρ where: ρ is the density (kg/m3) λ is the wavelength = 2a (m) (Figure 9.6). (9.20) 9.3 Interstitial Diffusion in Solids Therefore, for iron 211.4 × 109 Pa = 1.14 × 1013 Hz 7.86 × 103 kg f= 1 2a 1 E = ρ 2 × 2.28 × 10 −10 m f= 1 2a 1 129.8 × 109 Pa E = = 8.37 × 1012 Hz. −10 ρ 2 × 2.28 × 10 m 8.92 × 103 kg and for copper On the basis of these three calculations (which in fact are really not independent), a good approximation for the vibrational frequency of atoms in strongly bonded solids would be on the order of f ≌ 1013 Hz. 9.3.4 putting it All together Combining Equations 9.12, 9.14, and 9.15, the expression for D becomes − 1 1 D = a 2Γ = a 2fe 6 6 ∆G m RT 1 = a 2fe 6 ∆Sm R e − ∆H m RT (9.21) where: ΔSm is the entropy for motion ΔHm is the enthalpy for motion. ΔSm is associated with the change in positions of the lattice atoms as the interstitial atom moves through and is not terribly easy to evaluate, but it is expected to be not very significant. For example, it is suggested that ΔSm ≌ R (Shewmon 1989), so e( ∆Sm / R ) ≅ e1 = 2.718. Therefore, for interstitial diffusion, D = D0e − Q RT where D0 ≅ 1 2 a fe 6 ∆Sm R 1 = (2.3 × 10 −8 cm )2 (1013 s −1 )(2.718) = 2.21× 10 −3 cm 2 /s 6 and Q = ΔHm. Table 9.1 gives some experimental data for interstitial diffusion in iron (Shewmon 1989). The agreement between experimental and calculated values of D0 are surprisingly good given the lack of details in the model. So, for interstitial diffusion, D ≅ 10 −3 exp(− ∆H m /RT) cm2/s, where ΔHm is the enthalpy of motion of the atoms, molecules, or ions, is a good approximation. Of course, ΔHm, will vary considerably depending on the material and the atoms or molecules moving because it depends on the crystal structure, the interstitial and lattice atom sizes, and the details of their atomic bonding. 9.3.5 interstitiAl Jumps per second, Velocity For interstitial motion of carbon in iron, from the data in Table 9.1, Γ, the jumps per second is given by Γ=fe − ∆H m RT ≅ 10 e 13 − 80,100 (8.314)(1000) = 6.54 × 108 s −1 at 1000 K. The speed is a Γ = 2.3 × 10−8 cm × 6.54 × 108 s−1 = 15.04 cm/s! This is pretty fast, yet still much slower than the speeds of atoms in a gas, which are on the order of 5 × 104 cm/s. Also, in the solid interstitials case, the mean free path, λ = a/2 ≌ 10−8 cm, is small, making D ≌ 1/3vλ on the order of D ≌ 10−8 to 10−7 cm2/s as expected. 283 284 Chapter 9. Atomistics of Diffusion TABLE 9.1 Interstitial Diffusion in Iron Interstitial Atom C N O Source: 9.4 9.4.1 D0 (cm2/s) 4 × 10−3 5 × 10−3 2 × 10−3 Q (kJ/mol) 80.1 76.8 86.0 D (1000 K) (cm2/s) 2.6 × 10−7 4.9 × 10−7 6.4 × 10−6 Shewmon, P., Diffusion in Solids, 2nd ed, The Minerals, Metals, and Materials Society, Warrendale, sPA, 1989. VACANCY MECHANISM OF DIFFUSION IN SOLIDS VAcAncy diFFusion The vacancy mechanism of diffusion is an important mechanism of atom movement in hightemperature, primarily crystalline, materials and less so in low-temperature materials such as polymers. This is primarily because atomic bonds must be broken to produce vacancies, which requires high temperatures not accessible to most solid polymers. The end of a polymer molecule might be considered a vacancy or the site of a missing atom. However, this does not lead directly to any useful insights into diffusion in polymers, as discussed later. In contrast, inorganic glasses can be treated much like their crystalline counterparts and the concept of a vacant site and other point defects* can be identified. In this case, the concepts of point defects do provide insight into diffusion as well as temperature and additive effects on viscosity and glass transition temperatures. This will also be explored briefly later. For now, the focus is on crystalline materials where high temperatures are necessary for diffusion to be an important factor in a material’s behavior. A vacancy or a vacant lattice site is one in which an atom or ion is missing, as shown again in Figure 9.7. It takes energy to create vacancies, but their presence increases the entropy because of mixing of the vacancies and atoms—the configurational entropy—in the crystal lattice and leads to a finite vacancy equilibrium concentration at any temperature. As will be more evident later, it is convenient to express the vacancy concentration in terms of the fraction of atomic or lattice sites vacant; that is, [V] = fraction of lattice sites vacant, so [ V] = ηV / (ηV + η), where ηV is the number of vacancies/cm3 and η the number of atoms/cm3, so that ηV + η = number of lattice sites/cm3 (or per cubic meter). Then [V] is also the probability that any single site is vacant. The model for the diffusion coefficient for vacancy diffusion is very similar to that for interstitial diffusion except that it must be multiplied by [V]; that is, the probability that the neighboring site into which an atom or ion is going to move is vacant; that is, − 1 1 D vacancy = a 2Γ[V ] = a 2fe 6 6 ∆G m RT 1 [V ] = a 2fe 6 ∆Sm R e − ∆H m RT [V ] (9.22) The problem then is to determine [V]. 9.4.2 Vacancy FIGURE 9.7 The vacancy mechanism of diffusion: an atom moves into the vacancy and the vacancy takes the atom’s place in the crystal lattice. VAcAncies in elements (metAls, ge, si, etc.): stAtisticAl ApproAch Vacant lattice sites (vacancies) and other point defects exist in crystals because they increase the entropy of the system. However, it takes energy to form them largely because of the unsatisfied chemical bonds that are created between the neighboring atoms or ions and the vacancy. The Gibbs energy of * Vacancies and interstitials are point defects, because they have zero dimension in contrast to dislocations that have one dimension, grain boundaries and other boundaries that have two dimensions, and pores and second phases that have three dimensions. 9.4 Vacancy Mechanism of Diffusion in Solids 285 a crystal with vacancies compared to one without—that is, a perfect crystal—G(n) with n = number of vacancies and N = number of atoms—(it is more convenient to use numbers per unit volume with no loss in generality)—is given by the following equation with the configurational entropy term of Boltzmann, S = kBlnW (Chiang et al. 1997): G( n) = n g V − T ∆Sm , config G( n) = n g V − k BT ln W (9.23) ( N + n )! G( n) = n g V − k BT ln N! n! where gV is the Gibbs energy to form a single vacancy and the entropy of mixing is given by (Chapter 1) ( N + n )! ∆Sm, config = k B ln W = k B ln N!n! (9.24) where W is just the number of ways that N atoms and n vacancies can be arranged on N + n total sites, or it is the number of possible physical arrangements of the system.* Stirling’s approximation is ln (n !) ≅ n ln n − n , Chapter 1. So, applying Stirling’s approximation in Equation 9.23, G(n) becomes, G(n) ≅ ng V − k BT[(N + n) ln(N + n) − (N + n) − N ln N + N − n ln n + n]. (9.25) Differentiating G(n) with respect to n to minimize the total Gibbs energy as a function of the number of vacancies present—the minimum in energy in Figure 9.8—results in ∂G = µ V = 0 = g V + ln( N + n) + 1 − ln( n − 1) ∂n p,T , N and rearranging gives N+n 0 = g V − k BT ln . n (9.26) gV − − n = e k BT = e [V ] = N+n ∆G V RT (9.27) where: g V = e V + pvV − TsV eV is the energy to form a single vacancy vV is the volume of a vacancy sV is the entropy associated with the formation of a single vacancy † ΔGV is the equivalent term for a mole of vacancies. * † Boltzmann’s gravestone has the inscription “S = k(lnW),” Chapter 1 (Lindley 2001). This entropy term relates mainly to the formation of new local lattice vibration frequencies in the neighborhood of a vacancy and the entropy associated with the introduction of these new modes. It is thought to be small and usually neglected. Ne t ng Note that minimizing the Gibbs energy of a crystal with vacancies is tantamount to setting the chemical potential of vacancies, µ V ,, in equilibrium at a given temperature and pressure to zero. The final result is G(n) 0 n Equilibrium −TΔS C FIGURE 9.8 Plot showing the increase in free energy, ng, with an increase in the number of vacancies, n, the decrease in free energy due to the entropy of mixing—the configurational entropy, ΔSC—and the resulting net energy that leads to a equilibrium concentration of vacancies at the minimum of the free energy. 286 Chapter 9. Atomistics of Diffusion Frequently in the literature, the approximation is made that (N + n) ≅ N, but there is no need or reason to do this. However, in calculations, the number of vacancies compared with the number of atoms or lattice sites is usually very small and can indeed be neglected. Nevertheless, it is important to note that Equation 9.27 is exactly correct and [ V] = n / (N + n) is the fraction of vacancies relative to the total of lattice sites, N + n, occupied by N atoms and n vacancies. This is emphasized because this fraction of vacancies, no units, is frequently confused in the literature with the actual concentration, number per cm3, of vacancies. This is incorrect! 9.4.3 regulAr solution ApproAch This same result can be obtained by finding the minimum in the energy for vacancies in a crystal with a regular solution (Reed-Hill and Abaaschian 1992), where for a regular solution (Darken and Gurry 1953) ∆G soln = n V ∆G V − T∆Sideal = n V ∆G V + RT( n V ln X V + n N ln X N ) where: ∆Gsoln is the total Gibbs energy of the solution ΔGV is the energy difference between the perfect crystal and one with a mole of vacancies not counting the entropy of mixing term nV is the moles of vacancies nN is the moles of atoms Xi is the mole fraction. If both the top and bottom of the two terms on the right-hand side of the equation are multiplied by Avogadro’s number, NA, ∆G′soln = n V ∆G V − T∆Sideal = ng V + k BT( n ln X V + N ln X N ) (9.28) with X V = n / (N + n), X N = N / (N + n). Substituting these values into Equation 9.28 gives Equation 9.25, which leads to the same result as before, Equation 9.27, upon differentiation. 9.4.4 VAcAncy concentrAtions 9.4.4.1 Fractions Not Concentrations Obviously, if both the numerator and denominator of the left-hand side of Equation 9.27 are divided by some volume, V, ηV = n/V and η = N/V will now be the number of vacancies and the number atoms per unit volume, respectively, and ηV + η the total number of lattice sites per unit volume. Because electrical conductivity, diffusion, and other properties depend on the number of vacancies per unit volume, the number of vacancies per cm3 or per m3 are logical choices. As a result, the “concentration” of vacancies, [V], is from above, gV [V ] = − − ηV = e k BT = e ηV + η ∆G V RT (9.29) where [V] is the fraction of lattice sites (bold added for emphasis) that are vacant: as such, it is unit less and not really a “concentration.” As mentioned in Section 9.4.1, equivalently, [V] is the probability that any given single site is vacant. Now ∆G V = ∆H V − T∆SV = ∆U V + P∆VV − T∆SV for a mole of vacancies and the entropy term is usually small as is the P∆V term and both can be ignored in calculating the concentration of vacancies. Of course, if there are pressure gradients that give rise to vacancy concentration gradients that lead to mass transport during sintering or creep, then the P∆V term is important. However, even then, the overall concentration of vacancies does not necessarily change very much. So, 9.4 Vacancy Mechanism of Diffusion in Solids ∆G V ≅ ∆H V ≅ ∆U V with values usually on the order of several electron volts (1 eV = 1.602 × 10−19 J ≌ 96,500 J/mol and kB = 1.38 × 10−23 J/atom/1.602 × 10−19 J/eV = 8.61 × 10−5 eV/atom) and even for large pressure values, for example, 700 mPa (100,000 psi) for a molar volume around 10 cm3/mol ≡ 10−5 m3/mol, P∆VV ≅ 700 × 106 × 10 −5 = 7000 J/mol 100 kJ/mol ≅ ∆U V and can be neglected. At atmospheric pressures, where P = 105 Pa, the P∆V term is on the order of 1 J/mol and certainly negligible in determining vacancy concentrations. Note that these energies are frequently given the subscript f to designate energy of formation; for example, ΔHf. Table 9.2 gives some values of the enthalpy of formation of vacancies in metals. 9.4.4.2 Example: Copper at Its Melting Point, 1083°C For Cu, ∆H V = 1.03 eV (Borg and Dienes 1988), so at its melting point of 1083°C [V] = exp(−1.03 × 96,500/(8.314 × (1083 + 273))) = 1.48 × 10−4 This implies that η ηV , so ηV + η ≅ η, which is the number of copper atoms per unit volume, which can be calculated from the molar volume, η= ρ 8.92 g/cm 3 × NA = × 6.022 × 1023 atoms/mol = 8.45 × 1022 atoms/cm 3 63.55 g/mol M which means that ηV = 1.48 × 10−4 × 8.45 × 1022 = 1.25 × 1019 vacancies/cm3. Note again that for all solids because the atoms and ions more or less pack like billiard balls, the concentration of atoms, ions, or (simple) molecules in most solids in something times 1022 cm−3. TABLE 9.2 Enthalpies of Vacancy Formation in Pure Metals and Elements Metal Al Ag Au Cu Fe Ni Pt Pd Pb Mo Nb Ta V W Fe Na Si Ge Lattice FCC FCC FCC FCC FCC FCC FCC FCC FCC BCC BCC BCC BCC BCC BCC BCC Diamond Diamond ΔHf (eV) 0.68, 0.87, 0.76 1.12, 0.99, 1.09 0.89, 0.87, 0.96 1.29, 1.03, 1.17 1.4 1.78 1.32, 1.49, 1.2 1.85 0.57, 0.5, 0.53 3.0, 2.3 2.65, 2.0 2.8 2.1 4.0, 3.3 1.6, 1.5 0.04,0.48,c 0.34 2.4 2.2 Melting T (°C) 660 961 1063 1083 1536 (910–1400) 1453 1552 1552 327 2620 2467 3015 1902 3400 T < 910 98 1410 937 References 1,2,3 1,2,3 1,2,3 1,2,3 1 1 1,2,3 1 1,2,3 1,2 1,2 1 1 1,2 1,2 2,5,5 4 4 References for the table: 1, Shewmon (1989); 2, Borg and Dienes (1988); 3, Henderson (1972); 4, Mayer and Lau (1990); 5, Catlow and Mackrodt (1982). Another reference gives the same data as Shewmon (1989) (Glicksman 2000). c = calculated. 287 288 Chapter 9. Atomistics of Diffusion 9.4.4.3 Example: Silicon at Its Melting Point, 1410°C For Si, ∆H V = 2.4 eV (Mayer and Lau 1990), at its melting point of 1410°C, [ V] = exp(−2.4 × 96,500/(8.314 × (1410 + 273))) = 6.48 × 10−8 and η= 2.32 g/cm 3 ρ × NA = × 6.022 × 1023 atoms/mol = 4.98 × 1022 atoms/cm 3 28.08 g/mol M so that ηV = 6.48 × 10−8 × 4.98 × 1022 = 3.22 × 1015 vacancies/cm3. Note that the energy to form a vacancy is considerably higher in silicon than in copper, indicating that the bonds between atoms in silicon are significantly stronger than those in copper, which is also reflected in the higher melting point of silicon. 9.4.5 VAcAncies, quAsichemicAl ApproAch: point deFect chemistry 9.4.5.1 In an Element All of the above discussion is fine and works well for simple monatomic systems such as Cu and Si, where there is only one crystal site to consider and the interaction between lattice and electronic defects does not have to be taken into consideration. However, when considering more complex materials, for example, Y3Fe5O12 with the possibility of additives in solid solution that can affect the concentration of vacancies (or interstitials) or introduce electronic defects, the statistical treatment becomes unwieldy and unattractive. The statistical approach can be used for more complex solids but becomes increasingly algebraically messy, impractical, and unnecessary particularly when electronic point defects such as electrons accompany the formation of lattice point defects, and/or impurity or atmosphere effects are introduced (Readey 1966a,b). In contrast, the quasichemical approach is very straightforward, simple, and absolutely correct! Furthermore, there is interest in the concentrations of all of the point defects—interstitials, vacancies, impurity atoms, electrons, and so on—present and their interactions and how they affect the properties of the material. Because the interest is only in equilibrium concentrations, some type of chemical equilibrium approach should be equivalent to the statistical method. Indeed, the exact same result, Equation 9.29, can be obtained by a simple quasichemical approach or writing a chemical equation for the formation of point defects, and then writing the equilibrium constant for the equation or reaction. For example, for the formation of vacancies in copper, a quasichemical equation is perfect crystal = null = 0 VCu; ∆G V (9.30) where ∆G V is the same as that given earlier—the energy necessary to form a mole of vacancies in a perfect crystal. As a result, the Gibbs energy is barred: ∆G V.* So, the “concentration” of vacancies— more precisely, the fraction of lattice sites vacant—is obtained from the equilibrium constant for this reaction, Equation 9.30: [VCu ] = K e = e − ∆G V RT . (9.31) Obviously, Equations 9.29 and 9.31 are the same with the caveat in the quasichemical approach that the vacancy concentrations, [VCu], must be defined as fraction of lattice sites that are vacant to be * However, to reduce the notation, in the following discussions and calculations on point defects, the bars are left off the molar quantities for defects and is more consistent with the literature. 9.4 Vacancy Mechanism of Diffusion in Solids consistent with the statistical approach. The left-hand side of Equation 9.30 is zero and is appropriate because the perfect crystal generates vacancies and there needs to be nothing on the left-hand side of the equation to balance it. It is a balanced equation because there is no mass or charge on either side!* However, the objection could be raised that “the lattice sites are not balanced, there are vacant sites on the right but none on the left.” True! Equation 9.30 might be better written as Cu Cu VCu + Cu surface ; ∆G V . (9.32) That is, a copper atom on a copper site in the crystal, CuCu, moves to the surface, Cusurface, leaving behind a vacant copper site, VCu, resulting in an equilibrium constant of − [VCu ][Cu surface ] = Ke = e [Cu Cu ] ∆G V RT (9.33) where: [VCu] is the fraction of copper sites vacant [CuCu] is the fraction of copper sites in the crystal occupied by a copper atom [Cusurface] is the fraction of surface sites occupied by copper. For most real situations where ΔGV ≌ 1 eV or greater, as it is for the majority of elements in Table 9.2, the vacancy site fraction is small as shown for copper and silicon. Because [VCu] + [CuCu] = 1, then [CuCu] ≌ 1 for small vacancy concentrations. Similarly, the fraction of surface sites does not change, they are all occupied, so [Cusurface] = 1 and Equation 9.33 becomes the same as Equation 9.31. However, if for some reason ∆G V were small, then Equation 9.33 would be necessary. Nevertheless, for real materials, the concentration of vacancies is small and Equations 9.30 and 9.31 are quite appropriate. 9.4.5.2 Very Small ∆GV For example, if, ∆G V were zero, then [VCu] = [CuCu] or ηV = ηCu, and [VCu] = [CuCu] = 1/2. Note that in Table 9.2, one of the values for the enthalpy of vacancy formation in sodium is 0.04 eV, which is very small. So, from Equation 9.33 [VNa ] [VNa ] = = Ke [ Na Na ] 1 − [VNa ] (9.34) because [V Na] is not small compared to 1.0 because ΔHf is so small. Rearranging Equation 9.34 gives [ VNa ] = K e / (1 + K e ) and at 300 K, − ∆Hf − (0.04)(96,500) e RT e (8.314)(300) Ke [VNa ] = = = ∆H ( 0.04 )( 96,500 ) ≅ 0.176! − f − 1+ Ke 1 + e RT 1 + e (8.314 )( 300 ) Such a high vacancy concentration should be easily measured by measuring the density of sodium and comparing to the theoretical or x-ray density of pure sodium. In fact, this is a technique that has been used to measure the vacancy concentration of solids if the vacancy concentration is high enough and the technique to measure the density is precise enough. The theoretical or x-ray density of a crystalline solid is given by ρ= * ∑ nA i i N A Vcell This is a good reason to call this a quasichemical approach. i 289 290 Chapter 9. Atomistics of Diffusion where: ni is the number of atoms of species i per unit cell Ai is the atomic weight of species i NA is the Avogadro’s number Vcell is the volume of the unit cell. Take for example sodium, which has a BCC unit cell of two sodium atoms per cell, an atomic weight of A = 22.99 g/mol, and a lattice parameter of a = 4.2906 × 10−8 cm (Gray 1972). Therefore, the theoretical or x-ray density of sodium is ρ (g/cm 3 ) = 2(22.99) = 0.9667 g/cm 3 . (6.022 × 1023 )( 4.2906 × 10 −8 )3 A literature value for the density of sodium is ρ = 0.9712 g/cm3 (Gray 1972). The calculated vacancy concentration is quite large and the calculation of the density must be modified because the number of atoms per unit cell is not 2.0 but 2.0 × (1 − [V Na]). So, the density with vacancies should be ρ (g/cm 3 ) = 2(1 − 0.176)(22.99) = 0.7965 g/cm 3 (6.022 × 1023 )( 4.2906 × 10 −8 )3 which is much smaller than the value for the observed density of sodium, which is very close to the x-ray value assuming that there were no vacant sodium sites in the crystal! What is the problem? A likely culprit is the value for the formation of vacancies in sodium, ΔHf = 0.04 eV, is just too small and probably was tabulated incorrectly in the literature.* It might be expected that the enthalpy for vacancy formation would scale with the melting point of a solid because both are determined by the strength of the interatomic bonds (Shewmon 1989). For BCC iron, ΔHV s(Fe) = 1.4 eV from Table 9.2. The melting point of iron is 1809 K, whereas that of sodium is 371 K. For iron, ΔHV/Tm = 7.74 × 10−4 eV/K. Multiplying this by the melting point of sodium gives ΔHV(Na) ≌ 0.287 eV, about a factor of 9 greater than the one literature value of 0.04 and closer to the other tabulated values. With this value of the enthalpy to form vacancies in sodium, the vacancy concentration at 300 K would be [VNa ] = e − ∆H f RT =e − ( 0.287 )( 96,500 ) ( 8.314 )( 300 ) ≅ 1.5 × 10 −5 which is too small to detect in the density and similar to vacancy concentrations in copper and silicon at their melting points. So from these data and calculations, it could be concluded that the value given in the literature ΔHf(Na) ≌ 0.04 eV is probably incorrect. In any event, this calculation for sodium is a good review of theoretical density calculations, the effect of vacancy concentrations on densities, and how large vacancy concentrations need to be handled, Equation 9.34. 9.4.6 chArges oF point deFects in compounds And Kröger–VinK notAtion 9.4.6.1 Rationale The quasichemical approach embodied in Equation 9.30 is particularly convenient for compounds such as very strongly ionically bonded solids.† In NaCl or MgO, creating just sodium (magnesium) or chlorine (oxygen) vacancies without the other is essentially impossible because of electrical charge imbalance. In compounds, whether ionically bonded or not, vacancies must be created on both anion and cation sites together—or all sublattices (ternary, etc. compounds)—for the crystal to remain electrically neutral * † Yes, this actually happens sometimes implying that “… just because it is published doesn’t mean it’s correct!” The approach also works perfectly well for metallic or covalently bonded compounds. To get completely correct results, all that needs to be done is to treat these compounds as if they were ionic and associate a formal charge to each element in the compound. Take GaAs for example. If gallium is taken to be Ga3+ and As3−, then point defect chemistry can easily and correctly be applied to point defects and dopants in gallium arsenide. 9.4 Vacancy Mechanism of Diffusion in Solids (also to maintain “cation” and “anion” site balance). In other words, an electrically neutral “molecule” or “formula unit”—NaCl or MgO—must be removed from the crystal. The key to developing point defect chemistry and defect concentrations in compounds is to have a suitable method to account for charge on the defects and balance these charges to determine the concentrations of defects. 9.4.6.2 Kröger–Vink Notation In the 1940s and 1950s, scientists at the Phillips-Eindhoven laboratory in Holland were developing phosphors for cathode ray tubes, CRTs. Phosphors are usually some inorganic compound that is “doped” (small additions) with one or more other compounds and emit light at a desired wavelength when irradiated with electrons, x-rays, or light. For example, a major breakthrough promoting the development of color television many years ago was the discovery of Eu2O3-doped YVO4 (YVO4:Eu), which gives off a bright red light under electron bombardment in a CRT. A bright red phosphor combined with existing green and blue phosphors allowed accurate color rendition on the TV screen. Because the additives and host lattice ions frequently have different charges—which is important in light emission—Kröger and Vink (1956) developed a convenient notation to consider the charge on the different ions in the phosphor that was far superior to all other notations in use at the time and is now quite universally accepted. Prior to this, each branch of engineering and science—or individual—had its own, different, notation for defects that made it difficult if not impossible for workers in different fields to understand the results of others working in a related field on similar materials. Unfortunately, although widely accepted*, the meaning of the K–V notation is still frequently misinterpreted even in many textbooks. As a result, some confusion still exists today on how to apply K–V notation and defect chemistry to calculate concentrations of point defects and their effect on properties such as diffusion and electrical conductivity. Being able to calculate the concentrations—in number per unit volume—is extremely important in predicting the influence of point defects on properties. 9.4.6.3 Charge Relative to the Perfect Crystal Figure 9.9 shows the essence of K–V notation that takes into consideration the charge on a point defect. Here vacancies in MgO are used as examples. If an Mg2+ ion is removed from a perfect crystal of MgO (rock-salt structure), the initially uncharged crystal must now have a net 2− charge. ′′ , where the V indicates a vacancy, As a result, the vacant magnesium site can be represented as VMg the subscript Mg indicates the lattice site, and the two apostrophes represent a 2− charge: each Magnesium ion vacancy: V″Mg Site in crystal Double apostrophe designates −2 charge MgO Mg¨i magnesium interstitial O−2 Mg+2 Oxygen ion vacancy: VÖ Double dot designates +2 charge Site in crystal FIGURE 9.9 Drawing of a magnesium oxide crystal showing vacancies and interstitials: a Schottky defect and a Frenkel defect and how the Kröger–Vink notation applies to these defects. * K–V notation is now the accepted point defect notation by the International Union of Pure and Applied Chemistry (Connelly et al. 2005). 291 292 Chapter 9. Atomistics of Diffusion apostrophe representing a single negative charge. This is more than just a “bookeeping” method to indicate charge because the vacant site really does have a net negative charge. Figure 9.9 shows the vacant Mg2+ site is surrounded by six O2− ions, four in the plane and one above and one below, whose charges are not balanced, giving the site a 2− charge relative to the perfect crystal. Similarly, a vacant oxygen site is designated by VOii, where the double-dot superscript represents a 2+ charge relative to the perfect lattice: each dot representing a single positive charge. Again, Figure 9.9 shows that the VOii really is surrounded by six cations whose charges are not satisfied giving the site a net positive charge. In fact, in crystals, the positively charged vacancy can capture an electron that will orbit the positive charge in stable energy states just as an electron has stable states around a hydrogen nucleus. Electron transitions between these stable states give rise to color absorption bands, and the trapped electron plus vacancy is known as an F-center (F-for “color” from the German word for color, Farben) (Shulman and Compton 1962). 9.4.7 intrinsic point deFects in compounds 9.4.7.1 Intrinsic and Extrinsic Defects Intrinsic point defects are those whose concentrations depend on the properties of the given crystal itself. As a result, any two very pure crystals of the same material at the same temperature and pressure will have the same point defect concentration: for example, copper, where [VCu ] = K e = exp(− ∆G V /RT), Equation 9.31, the vacancy site fraction depends only on the energy to form vacancies in copper, ΔGV, whose value depends on the strength of the atomic bonds in copper. On the contrary, in most compounds, impurities or additives can be present that can control the concentrations of point defects that vary with the additive concentration. Such defect concentrations that are controlled by something from “outside” the material and are called extrinsic defects. There are several types of intrinsic point defects in solids. But for now, the focus is on intrinsic Schottky and Frenkel defects that are considered here in some detail. 9.4.7.2 Schottky Defects Because vacancies in compounds are charged, cation and anion vacancies cannot be created independently: they can be only created in electrically neutral groups; that is, “formula groups” or “molecules” of vacancies. An electrically neutral “molecule” of vacancies is called a Schottky defect and the equilibrium constant is called the Schottky product named after Walter Schottky, who developed the concept while working at Siemens corporation in the 1920s and 1930s (Hoddeson et al. 1992). In NaCl, for example, a point defect equation for the formation of Schottky defect is given by ′ + VCli ; ∆G S . 0 VNa (9.35) where ∆GS is the Gibbs energy to form a Schottky defect (usually, a mole of Schottky defects). This is a perfectly valid quasichemical point defect equation in that three equation-balancing criteria are satisfied: (1) there is no mass on either side of the equation, mass is balanced; (2) there is no net charge on either side of the equation, charge is balanced; and (3) the number of sodium sites equals the number of chlorine sites on the right as required by the 1:1 stoichiometry of Na+ and Cl− ions in NaCl.* ∆GS is the energy to form the Schottky defect or vacancy pair. Writing the equilibrium constant for Equation 9.35 gives ′ ][VCl• ] = e [VNa * − ∆GS RT (9.36) Actually, the number sodium and chlorine sites are balanced because Equation 9.35 similar to Equation 9.32 would be i + − Na Na + Cl Cl NaCl surface + VN′ a + VCl , where there are both sodium and chlorine sites on both sides of the equation. Requiring a stoichiometric relationship between the number of cation and anion sites on the right-hand side of Equation 9.35 is equivalent to this more complete equation and is correct as long as the number of Schottky defects is small so that the − site fractions on the left-hand side are essentially 1: that is, [ Na +Na ] = [ Cl Cl ] ≅ 1. 9.4 Vacancy Mechanism of Diffusion in Solids ′ ] and [ VCli ] are the fraction of sodium sites vacant and fraction of chlorine sites vacant, where [ VNa respectively. This is where confusion often arises: these concentrations are site fractions and, therefore, have no units! This is what the statistical approach, Equation 9.29, gives. In the literature, these concentrations (site fractions) are frequently given units such as “mol/m3,” which is absolutely incorrect, they are fractions! Making this error, calculations of real concentrations (mol/m3) are usually incorrect and can be wrong by a factor of 2 or 3. On the other hand, when combining lattice or atomic point defects in equations with electronic defects such as electrons, treating these as “mol/ m3” or some other concentration units, can lead to errors of several orders of magnitude when calculating the actual defect concentrations per unit volume! Appendix A.4 expands on this. This incorrect usage occurs frequently in a rather large number of books and published papers that perpetuate and lend legitimacy to this error and make point defect chemistry more confusing than it ′ ] and [ VCli ] are the fraction of sodium sites need be. To emphasize this, it is worth repeating that [ VNa vacant and fraction of chlorine sites vacant, respectively, and therefore do not have units. If the number of NaCl Schottky defects per unit volume is ηVNaCl , then, obviously, ηVNa ′ = ηV i = ηVNaCl Cl are the number of sodium and chlorine vacancies per unit volume respectively. Because the concentrations of vacancies are usually small in strongly bonded solids—on the order of 10−4 at the melting point—as was the case for copper and silicon, the number of NaCl sites per cm3 is given approximately by * ηNaCl = (ρ /M)N A where ρ = density of NaCl = 2.165 (g/cm 3), M = molecular weight NaCl = 58.44 g/mol (Haynes 2013), so η(NaCl) = 2.165 ρ NA = × 6.022 × 1023 = 2.23 × 1022 cm −3 58.44 M and the number of sodium and chlorine lattice sites per cm3 is just ηNa = ηCl = η NaCl, which has the advantage of showing the charges on the vacancies because there is one site for each ion for each “molecule” of NaCl. So, ′ ]= [VNa ηV ( Na ) η (Cl) η ( NaCl) . = [VCl ] = V = [VNaCl ] = V η( Na ) η(Cl) η( NaCl) That is, for the Schottky product in NaCl, the site fraction of sodium and chlorine vacancies are ′ ] = [ VCli ], as they should be. equal: [ VNa Another approach, that is more general and applicable to all types of point defect equations, is to consider electrical neutrality more formally. That is, the number of positive charges per unit volume must be equal to the number of negative charges per unit volume. For a Schottky defect in NaCl, this means: Positive /cm 3 = Negative /cm 3 (9.37) ( z + )(e)ηVCl• = ( z − )(e)ηVNa ′ where: e is the electron charge, 1.602 × 10−19 C z+ and z− are the number of electron charges on the positively and negatively charged vacancies, respectively. * To enhance readability here and what follows, equivalent notation is used: for example, η(NaCl) = ηNaCl both mean the number of NaCl molecules cm−3. If the concentration of vacancies was not small, then as shown above for a metal, then the concentration of sodium vacancies, for example, is: [ V′ ] = Na η V ( Na ) η V ( Na ) + η Na ( Na ) and [ Na ] = Na η Na ( Na ) η V ( Na ) + η Na ( Na ) = {η V ( Na ) + η Na ( Na )} − η V ( Na ) η V ( Na ) + η Na ( Na ) and similarly for the fraction of chlorine sites occupied by chlorine and chlorine vacancies. = 1 − [ VNa′ ] 293 294 Chapter 9. Atomistics of Diffusion For NaCl, z+ = z− = 1 and so, ηVCli = ηVNa ′ (9.38) and dividing by ηNaCl ηVCli ηNaCl ηVCli ηCl = ηVNa ′ ηNaCl = ηVNa ′ ηNa (9.39) ′ ] [ VCli ] = [ VNa as before. Therefore, from the equilibrium constant, the Schottky product, Equation 9.36 becomes ′ ][VCl• ] = e [VNa − ∆GS RT ′ ]2 = [VCl• ]2 = e [VNa ′ ] = [VCl• ] = e [VNa − − ∆GS RT (9.40) ∆GS 2RT where ∆GS/2 is the average energy to form a vacancy. Table 9.3 gives some Schottky defect formation energies. TABLE 9.3 Schottky Defect Formation Energies in Compounds Compound NaBr NaCl KCl KBr CsI CsCl LiF LiCl LiI CaF2 BeO MgO CaO BaO MnO UO2 TiO2 Al2O3 MgAl2O4 Structure “ “ “ “ CsCl CsCl NaCl “ “ CaF2 Wurtzite, ZnS NaCl “ “ “ “ Rutile α-Al2O3 Spinel 𝚫HS (eV) 1.72, 1.68 2.3, 2.3, 2.3, 2.02 2.3, 2.3, 2.6, 2.3 2.4, 2.4, 2.53, 2.27c 1.9, 2.14 1.86 2.5, 2.5, 2.5, 2.68 2.12 1.34 5.5 6, 6 7.7, 6, 7.5c 6, 6 3.4 4.6 6.4 5.2 23, 25.7c 29.1c Melting T (°C) 747 801 771 734 632 646 848 610 469 1418 2578 2825 2613 1973 1842 2847 1843 2050 2105 References 2,6 1,2,3,5,6 1,2,3,5,6 1,2,6,7 1,6 3,6 1,2,3,5,6 5,6 5,6 3,4 3,4 3,4,7 3,4 3,7 3,7 3,4 3 3,7 3,7 References for the table: Crystal structures (Wells 1984); melting points (Haynes 2013); 1, Hayes and Stoneham (1985); 2, Henderson (1972); 3, Chiang et al. (1997); 4, Kingery et al. (1976); 5, Glicksman (2000); 6, Gray (1972); 7, Catlow and Mackrodt (1982). c = calculated. 9.4 Vacancy Mechanism of Diffusion in Solids To write an equation for the formation of both Na and Cl vacancies and the equilibrium constant as above assumes that the vacancies are not associated into a “molecule” of vacancies on neighboring lattice points. Quite the contrary, it assumes that they are dissociated and each cation and anion vacancy is free to mix randomly with the ions on the cation and anion lattices, respectively. In reality, the vacancies are charged and attract each and can associate. An equilibrium for this association can be written, but is not discussed here to keep things simple. 9.4.7.3 Example: Vacancy Concentrations in NaCl at Its Melting Point ∆GS ≅ ∆HS = 2.3 eV × 96,472 J/eV = 221,890 J/mol (Chiang et al. 1997). So, at the melting point of NaCl of T = 801°C = 1074 K, ′ ] = [VCli ] = e [VNa − 221,890 2( 8.314 )(1074 ) = 4.02 × 10 −6 roughly four vacancies for every million sites, which does not seem like very many. However, V(Na) = ′ ]η(NaCl) = 4.02 × 10−6 × 2.23 × 1022 cm−3 = 8.96 × 1016 cm−3, which now seems to be ηV(Cl) = [ VNa a reasonable number relative to the number of total sites. Note that for both copper and NaCl, the energy to form a single vacancy is on the order of 1 eV and their melting temperatures are not too different: Tm(Cu) = 1083°C and Tm(NaCl) = 801°C. 9.4.7.4 Schottky Defects in Al2O3 What about a more complex compound such as Al2O3? The same principles hold true in that an ′′′ and 3VOii, and the quasichemical electrically neutral “molecule” of vacancies must be formed, 2 VAl equation for the formation of the vacancies is ′′′ + 3VOii ; ∆G S 0 2VAl (9.41) with the Schottky product given by ′′′ ]2 [VO•• ]3 = e [VAl − ∆GS RT (9.42) where the ∆GS in this case is the energy to form 1 mole of “Al 2O3 ” vacancies. So, if ηV(Al 2O3) is the number of “Al 2O3 vacancies” per unit volume, then ηV(Al) = 2ηV(Al 2O3) and ηV(O) = 3ηV(Al 2O3) because there are 2Al and 3O per Al 2O3 “molecule.” Then, the number of Al 2O3 “molecule” sites per cm 3 is again, η(Al 2O3 ) = (ρ(Al 2O3 ) /M(Al 2O3 ))N A , where ρ is the density (g/cm 3) and M is the molecular weight (g/mol) of Al 2O3 . Here, η(Al) = 2η(Al 2O3) and η(O) = 3 η(Al 2O3), so ′′′ ] = [VAl ηV ( Al) 2ηv ( Al 2O3 ) ηv ( Al 2O3 ) = = η( Al) 2η( Al 2O3 ) η( Al 2O3 ) η (O) 3ηv ( Al 2O3 ) ηv ( Al 2O3 ) [VO ] = V = = η(O) 3η( Al 2O3 ) η( Al 2O3 ) (9.43) •• ′′′ ] = [ VOii ]; that is, the vacancy site fractions are equal in Al2O3 just as they were in NaCl. therefore, [ VAl Similarly, application of electrical neutrality in this case is (2e)ηVOii = (3e)ηVAl′′′ 295 296 Chapter 9. Atomistics of Diffusion and dividing by ηAl2O3 (2e)ηVOii ηAl2O3 = (3e)ηVAl′′′ ηAl2O3 (2e)ηVOii (3e)ηVAl′′′ = ηAl ηO 3 2 (6e)ηVOii ηO = (6e)ηVAl′′′ ηAl ′′′ ] [VOii ] = [VAl again as before for NaCl. This is true for all Schottky defects in binary compounds: The site fractions of the cation and anion vacancies are equal for Schottky defects. However, the numbers of vacancies per unit volume must be different to balance the charge difference, but their site fractions are the same. (Note: the charge has already been taken care of in the formula, e.g., Al2O3, so charge is counted twice and just cancels out.) So, the equilibrium constant in Equation 9.42 becomes ′′′ ]2 [VO•• ]3 = [VAl ′′′ ]5 = [VO•• ]5 = e [VAl ′′′ ] = [ VO•• ] = e [ VAl − ∆GS 5RT − ∆GS RT . (9.44) Again, the energy to form either aluminum or oxygen vacancies is the “average” energy per vacancy, ∆GS /5. 9.4.7.5 Example: Vacancy Concentrations in Al2O3 at Its Melting Point ∆GS ≅ ∆HS ≌ 22 eV × 96,472 J/eV = 2,122,400 J/mol. At the melting point of Al2O3 of T = 2050°C = 2323 K, ′′′ ] = [VOii ] = e [VAl − 2,122,400 5(8.314)(2323) = 2.85 × 10 −10 ′′′ ]η(Al) = Now, η(Al 2O3 ) = (ρ / M)N A = (4.00 /101.96) × 6.022 × 1023 = 2.36 × 1022 cm −3 , so ηV(Al) = [ VAl ii −10 22 −3 13 −3 ′′′ ] 2η(Al2O3) = 2.85 × 10 × 2 × 2.36 × 10 cm = 1.35 × 10 cm . For ηV(O) = [ VO ]η(O) = [ VOii ] [ VAl 3η(Al2O3) = 2.85 × 10−10 × 3 × 2.36 × 1022 cm−3 = 2.02 × 1013 cm−3 and the vacancy concentrations per cm3 are in a ratio of 2:3 as required by the formula for Al2O3. Note that the energy to form a single vacancy in aluminum oxide is in the neighborhood of about 4 eV, which is considerably larger than that for NaCl. This is not too surprising considering the higher charges on Al3+ and O2− ions compared with Na+ and Cl− produce stronger bonding as reflected in the melting points: 801°C for NaCl compared with 2050°C for Al2O3. However, from a practical point of view, the intrinsic vacancy site fraction at the melting point of alumina is only about 0.3 parts per billion! This means that to have a chance to observe intrinsic behavior in this material, the starting purity of the material must be greater than nine-9s pure*—semiconductorgrade material—otherwise, the impurities present are likely to influence the vacancy concentrations as will be discussed below. One final point about compounds. There are many important compounds that contain more than a single cation such as Y3Fe5O12, MgAl2O4, NiFe2O4, and so on. Again for such ternary * Nine-9s pure is 99.9999999% pure! 9.4 Vacancy Mechanism of Diffusion in Solids compounds, a Schottky defect is defined a “molecule” or formula unit of vacancies and a Schottky product can be written. Take MgAl2O4 for example: ′′ + 2VAl ′′′ + 4VOii ; ∆GS 0 VMg and ′′ ][ VAl ′′′ ]2 [ VO•• ]4 = K S = e [ VMg − ∆GS RT (9.45) as was the case for binary compounds. Just like binary compounds, the site fraction of vacancies are ′′′ ] = [ VOii ]. equal, that is, [ V′′] = [ VAl 9.4.7.6 Frenkel Defects Another type of intrinsic defect that is important in diffusion in solids is the Frenkel defect postulated by Jacob Frenkel in the 1920s while at the Leningrad Institute for Electrical Engineering in Russia (Hoddeson et al. 1992). A Frenkel defect is a vacancy and an intestinal pair. As such, they can occur in either elemental solids or compounds. It is difficult to force large lattice atoms or ions into small interstitial sites. However, they are particularly important in certain compounds that have either large interstitial sites such as the fluorite crystal structure or small ions such as the silver ion in the silver halides, where the interstitial silver plays an important role in the—rapidly becoming extinct—film photographic process. Figure 9.9 shows a magnesium Frenkel defect in MgO consisting of an interstitial magnesium ion and a vacant magnesium site. This Frenkel defect can be written as ′′ : ∆G F Mg Mg Mgiii + VMg (9.46) where ΔGF is the energy to form the Frenkel defect, the vacancy–interstitial pair, and the subscript i indicates an interstitial site. Again, for this point defect equation, mass and charge are balanced. To give a site balance, the equation would have to be written: ′′ : ∆G F Mg Mg + I Mgiii + VMg (9.47) where I is an interstitial site. But as was the case when the vacancy concentration was small, [I] ≌ 1 when the concentration of Frenkel defects is small; that is, very few interstitial sites are occupied, so Equation 9.46 works. Note that the MgMg has no charge relative to the perfect crystal in K-V notation, although it actually refers to a Mg2+ ion on a magnesium site. On the contrary, the Mg2+ on the interstitial site has a 2+ charge relative to the perfect crystal because the empty interstitial site has no charge. So, the equilibrium constant can be written as ∆G F − ′′ ] [Mg••i ][VMg ′′ ] [Mg••i ][VMg ′′ ] = K e = e RT ≅ = [Mg••i ][VMg 1 [Mg Mg ] (9.48) where [ Mgiii ] is the fraction of interstitial sites occupied. To continue to calculate the site fractions or the concentrations (number/cm3), information about the number of interstitial sites relative to the number of lattice sites is needed. This means that the specific interstitial site in the crystal that the magnesium goes into must be known. For example, MgO has the rock-salt structure with cubic close packing of oxygen ions. There are four oxygen sites per cell, all occupied with O2− ions and four octahedral cation sites per cell, all occupied with Mg2+ ions. The largest unoccupied site is the tetrahedral site inside the corners of the MgO unit cell, none of which are occupied in the perfect crystal. However, there are eight tetrahedral sites per cell. So, if the Mgiii goes into tetrahedral sites, the number of interstitial sites per unit volume is just twice the number of magnesium sites or ηi = 2ηMg. Electrical neutrality is now (2)(e)ηMgiii = (2)(e)ηVMg ′′ (9.49) 297 298 Chapter 9. Atomistics of Diffusion and cancelling and dividing each side by the number of magnesium sites per unit volume, ηMgiii = ηMg 2ηMgiii ηVMg ′′ ηMg = ηi ηVMg ′′ ηMg (9.50) ′′ ] 2[Mgiii ] = [VMg where the last equation states that the fraction of interstitial sites filled is half of the fraction of vacant lattice sites because there are twice as many interstitial sites per unit volume. Putting this result into Equation 9.48 gives 2 2 M iii = K e (9.51) ∆G 1 − 2RTF M iii = e 2 − ∆G F ′′ ] = 2 e 2RT . or equivalently, [ VMg Table 9.4 gives some literature values of the energy to form Frenkel defects in compounds. 9.4.8 bAcK to the VAcAncy diFFusion coeFFicient Substitution for the concentration of vacancies as the probability that a neighboring site is vacant, [V], in something like copper, from Equation 9.22 1 D = a 2f e 6 ∆Sm R 1 = a 2f e 6 ∆Sm R 1 = a 2f e 6 ∆Sm + ∆SV R = D0e − e e − ∆H m RT − ∆H m RT e [V ] e − ∆SV R e − ∆H V RT (9.52) ∆H m + ∆H V RT Q RT TABLE 9.4 Frenkel Defects in Compounds Compound AgCl AgBr ZnO Li2O MgF2 CaF2 Type Cation Cation Anion Cation Anion Anion Cation Structure NaCl NaCl ZnS Antifluorite TiO2, rutile CaF2 ΔHF (eV) 1.1, 1.4,c 1.44 1.13 2.51c 2.28,c 2.78 3.12c 2.5, 2.75,c 2.8 7 SrF2 BaF2 UO2 Anion Anion Anion Cation CaF2 CaF2 CaF2 Na2S Cation Antifluorite Melting T (°C) 455 430 1974 1438 1263 1418 References 1,2,3 3 2 2,3 2 1,2,3 1 2.38,c 2.5, 2.3 1.98,c 1.91, 1.86 5.1, 5.47c 9.5 1477 1368 2847 2,2,3 2,2,3 1,2 1 1.77 1172 3 References: Crystal structures (Wells 1984); melting points (Haynes 2013); 1, Kingery et al. (1976); 2, Catlow and Mackrodt (1982); 3 Gray (1972). c indicates a calculated value. 9.4 Vacancy Mechanism of Diffusion in Solids so D0 = (1 / 6)a 2f exp( −( ∆Sm + ∆SV )/R ) and Q = ΔHm + ΔHV for vacancy diffusion; that is, the activation energy for vacancy diffusion is the sum of the energy for atomic motion plus the energy to form vacancies. In the literature, ΔHV is typically called the enthalpy of formation and sometimes written as ΔHf and, similarly, ΔSV = ΔSf. Note, that for compounds, ΔHf is the average energy of defect formation, which was shown above to be ΔHS/2 for NaCl and ΔHS/5 for Al2O3, where ΔHS is the enthalpy to form the Schottky defect: the “molecule” of vacancies. In materials such as copper, iron, NaCl, Al2O3, and so on, vacancy diffusion is the main mechanism by which the atoms or ions in the crystals move about and diffuse. This is the process of selfdiffusion and the diffusion coefficient of copper in copper is the self-diffusion coefficient of copper and similarly, the diffusion coefficient of sodium in sodium chloride is the self-diffusion coefficient of sodium in sodium chloride, and so on. 9.4.8.1 Example : Diffusion in Cu Considering self-diffusion in copper, as calculated above, the vacancy concentration (site fraction) of copper at its melting point of 1083°C is 1.48 × 10−4 and the ΔHf = 1.03 eV = 1.03 × 96,472 = 99,366 J/mol. In Table 9.4, the activation energy for Cu diffusion in copper, Q = 210,900 J/mol. Therefore, ΔHm = Q – ΔHf = 210,900 − 99,366 = 111,534 J/mol. Also, from this table, D0 = 0.1 cm2/s, so the selfdiffusion coefficient of copper in copper at its melting point is D = D0e 9.4.8.2 − Q RT = 0.1× e − 210 ,900 ( 8.314 )(1356 ) = 7.51 × 10 −10 cm 2 /s Example: Diffusion in NaCl For self-diffusion in NaCl, as calculated above, the vacant sodium ion concentration in NaCl at its melting point of 801°C is 4.02 × 10−6 and ΔHS/2 = 221,890/2 = 110,945 J/mol. From Table 9.5 of diffusion coefficients in compounds, Q = 202,600 J/mol so ΔHm = Q – ΔHS/2 = 202,600 − 110,945 = 91,655 J/ mol. In this case, D0 = 18 cm2/s, so at its melting point, the self-diffusion coefficient of Na in NaCl is D = D0e − Q RT = 18.0 × e − 202,600 ( 8.314 )(1074 ) = 2.52 × 10 −9 cm 2 /s Also, in Table 9.5, for the diffusion of Cl in NaCl, Q = 199.7 kJ/mol so ΔHm = Q – ΔHS/2 = 88,755 J/mol. Here, D0 = 2.2 cm2/s, so at the melting point, the diffusion of Cl in NaCl is D = D0e − Q RT = 2.2 × e − 199,700 ( 8.314 )(1074 ) = 4.26 × 10 −10 cm 2 /s which is about a factor of 5 smaller than the diffusion coefficient for sodium at the same temperature. 9.4.8.3 Example: Diffusion in Al2O3 As a final example, consider diffusion in aluminum oxide, Al2O3. To emphasize the difference between the cation and anion diffusion coefficients, Figure 9.10 schematically shows the diffusion coefficients for aluminum and oxygen in aluminum oxide: the activation energies for the diffusion of the cation and anion are different and, typically, the diffusion coefficient for the anion is usually smaller because it is the larger ion and has more difficulty in moving. But for both, Q = ∆H m + (∆H S /n), where n is the number of atoms in the “molecule. For example, in aluminum oxide, Al2O3, the activation energies for diffusion of aluminum and oxygen are, respectively, Q(Al) = ∆H m (Al) + ∆H S 5 and Q(O) = ∆H m (O) + ∆HS . 5 299 300 Chapter 9. Atomistics of Diffusion TABLE 9.5 Diffusion Data Material Na Pb Ag H2O Do (cm2/s) Q (kJ/mol) 1.10 × 10−3 2.37 × 10−4 5.80 × 10−4 5.21 × 10−2 10.25 13.04 32.47 19.37 Tmp (°C) T (°C) D at T (cm2/s) Liquids 98 327 961 0 98 327 961 35 3.96 × 10−5 1.74 × 10−5 2.45 × 10−5 2.70 × 10−5 Liquid Liquid Liquid Liquid 1 1 1 3 Type Source Na Cu Ag Au Pt Mo Mo Zn in Cu Fe(fcc) Fe(bcc) C in fcc Fe C in bcc Fe N in fcc Fe 0.72 0.10 0.67 0.09 0.33 0.13 0.13 0.34 0.49 1.39 0.20 0.02 0.001 48.1 210.9 189.1 176.1 284.9 437.2 437.2 190.8 284.1 240.2 142.3 84.1 74.1 Metals 98 1083 961 1063 1552 2610 2610 1083 1538 1538 1538 1538 1538 98 1083 961 1063 1552 2610 1000 1000 1000 1000 1000 1000 1000 1.22 × 10−7 7.51 × 10−10 6.63 × 10−9 1.17 × 10−8 2.31 × 10−9 1.56 × 10−9 1.49 × 10−19 5.04 × 10−9 1.08 × 10−12 1.93 × 10−10 2.90 × 10−7 7.08 × 10−6 9.11 × 10−7 Vacancy Vacancy Vacancy Vacancy Vacancy Vacancy Vacancy Vacancy Vacancy Vacancy Interstitial Interstitial Interstitial 1 1 1 1 1 1 1 1 1 1 1 1 1 Si B in Si As in Si P in Si Al in Si Ge Ga in GaAs As in GaAs 1.50 × 103 0.76 12.00 3.85 0.50 18.50 2.90 × 108 0.70 484.3 333.8 390.7 353.1 289.4 296.2 578.8 308.7 Semiconductors 1414 1414 1414 1414 1414 937 1238 1238 1414 1414 1414 1414 1414 937 1238 1238 1.51 × 10−12 3.51 × 10−11 9.58 × 10−12 4.49 × 10−11 5.47 × 10−10 3.02 × 10−12 2.84 × 10−12 1.49 × 10−11 Vacancy Vacancy Vacancy Vacancy Vacancy Vacancy Vacancy Vacancy 2 2 2 2 2 2 2 2 Ag in AgBr Br in AgBr Na in NaCl Cl in NaCl Mg in MgO O in MgO Al in Al2O3 O in Al2O3 Ni in NiO O in NiO Ti in TiO2 O in TiO2 Cu in Cu2O O in Cu2O Na in Na2O·11Al2O3 57 3.00 × 104 18 2.2 0.25 4.3 × 10−5 28 2.90 × 103 4.40 × 10−4 6.20 × 10−4 6.20 × 10−2 2.00 × 10−3 4.36 × 10−2 6.50 × 10−3 2.71 × 10−4 2.71 × 10−4 6.20 × 10−2 93.6 186.2 202.6 199.7 330.54 343.5 477 636 184.9 240.6 256.9 252.04 151.04 164.43 16.5 16.5 138.3 Ceramics 432 432 801 801 2850 2850 2050 2050 1957 1957 1843 1843 1244 1244 2000 “ 2550 432 432 801 801 2850 2850 2050 2050 1957 1957 1843 1843 1244 1244 2000 300 1000 6.62 × 10−6 4.79 × 10−10 2.52 × 10−9 4.26 × 10 −10 7.40 × 10−07 7.73 × 10−11 5.26 × 10−10 1.45 × 10−11 2.31 × 10−8 1.67 × 10−9 2.49 × 10−8 1.06 × 10−9 2.56 × 10−7 1.31 × 10−8 1.13 × 10−4 8.49 × 10−6 1.31 × 10−7 Interstitial Vacancy Vacancy Vacancy Vacancy Vacancy Vacancy Vacancy Vacancy Vacancy Vacancy Vacancy Vacancy Vacancy Interstitial Interstitial Vacancy 6 6 6 6 6 6 6 6 6 6 6 6 6 6 7 6.9 5.65 × 10−4 125.4 43.03 1475 Tg 1475 Tg 1000 1000 Interstitial Interstitial 7 2 O in 0.15CaO–0.85ZrO2 Na in SiO2-glass H2 in SiO2-glass 4.93 × 10−5 9.69 × 10−6 7 (Continued ) 9.4 Vacancy Mechanism of Diffusion in Solids TABLE 9.5 (Continued) Diffusion Data Material O2 in SiO2-glass O in SiO2-glass He in polypropylene H2 in “ CO2 in polybutadiene H2 in “ N2 in “ O2 in “ CO2 in butyl rubber He in “ H2 in “ N2 in “ O2 in “ Polystyrene-self Poly(methyl methacrylate)-self Do (cm2/s) 2.70 × 10−4 1.20 × 10−4 Q (kJ/mol) 111.9 295 4.1 2.4 0.24 0.053 0.22 0.15 36 0.015 1.36 34 43 30.5 34.7 30.5 21.3 30.1 28.5 50.2 24.3 33.9 50.6 49.8 Tmp (°C) 1475 Tg 1475 Tg T (°C) 1000 1000 D at T (cm2/s) 6.91 × 10−9 9.42 × 10−17 Type Interstitial Vacancy Source 2 2 Polymers −18Tg −18Tg −85Tg −85Tg −85Tg −85Tg −73Tg −73Tg −73Tg −73Tg −73Tg 100Tg 105Tg 27 27 27 27 27 27 27 27 27 27 27 135 135 2.00 × 10−5 2.18 × 10−6 1.17 × 10−6 1.04 × 10−5 1.26 × 10−6 1.64 × 10−6 6.54 × 10−8 8.81 × 10−7 1.70 × 10−6 5.26 × 10−8 9.17 × 10−08 1.2 × 10−15 6.9 × 10−17 Interstitial Interstitial Interstitial Interstitial Interstitial Interstitial Interstitial Interstitial Interstitial Interstitial Interstitial Reptation Reptation 4 4 4 4 4 4 4 4 4 4 4 5 5 References for Table: Melting points (Haynes 2013); glass transition temperatures, Tg (Sperling 2006), (Callister and Rethwisch 2009). 1, Brandes and Brook (1992); 2, Mayer and Lau (1990); 3, Robinson and Stokes (2002); 4, Barrer (1941); 5, Sperling (2006); 6, Gray (1972); 7, Kinergy et al. (1976). Slopes = − Q 2.303R log10 D/m2s−1 D(Al) Q(Al) = ΔHm(Al)+ D(O) Q(O) = ΔHm(O)+ ΔHS 5 ΔHS 5 1000 /K T FIGURE 9.10 Representation of the intrinsic vacancy diffusion coefficients for aluminum and oxygen in aluminum oxide. The activation energy for diffusion consists of the activation energy for motion and the energy for formation of vacancies: in this case, the latter is the energy to form a Schottky defect divided by 5—the average energy of formation per vacancy. 301 302 Chapter 9. Atomistics of Diffusion 9.4.9 AdditionAl comments About VAcAncy diFFusion 9.4.9.1 Vacancy Jumps and Vacancy Diffusion Coefficient As was noted above, the model for the diffusion coefficient for a vacancy mechanism is not much different from that for the interstitial mechanism except that the expression for interstitial diffusion must be multiplied by the site fraction of vacancies, which is again, Equation 9.22: − 1 1 D = a 2Γ [ V ] = a 2f e 6 6 ∆G m RT 1 [ V ] = 6 a 2f e ∆Sm R e − ∆H m RT [V ] That means that the number of jumps per second for a vacancy, Γ, will be on the same order as that for interstitials, namely, about 108 jumps per second, and their speed will be similar to interstitials, on the order of cm/s. However, for the atoms in the lattice, for example, Cu, the number of jumps per second is about a factor of 10−4 jumps less—essentially that for vacancies times the site fraction of vacancies—and the speed will also be reduced by a similar amount. The above expression for vacancy diffusion, Equation 9.22, could be interpreted as 1 D = a 2Γ [ V ] = D V [ V ] 6 where DV is the diffusion coefficient for vacancies. This could be carried further D = DV [ V ] ≅ DV Atom moves to surface Surface ηV η where: ηV is the number of vacancies per cm3 η is the number of atoms per cm3, so that Vacancy Dη = D V ηV FIGURE 9.11 Depiction of a surface acting as a “source” (or sink) for vacancies. Other two-dimensional defects such as grain and interface boundaries can behave in a similar way to act as sources or sinks for vacancies. That is, the diffusion coefficient for atoms times the number of atoms per cm3 is equal to the vacancy diffusion coefficient times the number of vacancies per cm3. Extra atom half-plane Vacancy Atom moves Dislocation Dislocation moves-climb FIGURE 9.12 How a dislocation can act as a source or sink for vacancies. An atom leaves a lattice position and attaches itself to the end of an edge dislocation half plane leaving behind a vacancy in the lattice. The dislocation line moves downward, dislocation climb, and in doing so creates a vacancy; therefore, it is a vacancy source. Conversely, an atom can move from a dislocation filling a vacancy: again the dislocation “climbs” and a vacancy disappears, so the dislocation is acting as a vacancy sink. (9.53) 9.4.9.2 Sources and Sinks for Vacancies To equilibrate with changing temperatures, and so on, the concentration of vacancies needs to change. Vacancies can be created at vacancy sources and destroyed at vacancy sinks. As shown in Figure 9.11, the surface certainly can be a source or sink for vacancies but so can dislocations and grain boundaries—as these can be considered to be dislocation arrays—as sketched in Figure 9.12. Vacancies created or destroyed at the end of an edge dislocation gives rise to dislocation climb—important during creep— as opposed to dislocation glide, which is responsible for plastic deformation in crystalline solids. 9.4.10 extrinsic diFFusion In a discussion of vacancy diffusion, the vacancies are intrinsic vacancies and the resulting diffusion coefficients are intrinsic diffusion coefficients. These are intrinsic because they only depend on the temperature and the properties of the pure crystal—internal or intrinsic to the crystal; primarily, the type and strength of the interatomic bonding. On the contrary, something 9.4 Vacancy Mechanism of Diffusion in Solids that is both a benefit and a problem is that impurities or additives can alter the diffusion coefficient in compounds. This is a benefit if adding something increases or decreases a diffusion coefficient in a desired and controlled way. On the contrary, it is a major problem when trying to measure intrinsic diffusion coefficients in compounds where impurities—frequently at only the part per million (ppm) level—control the vacancy concentration (see the calculation for Al2O3 in Section 9.4.7.4). A classic example of extrinsic diffusion is the addition of CdCl2 to NaCl. For small concentrations, CdCl2 forms a solid solution with NaCl with Cd2+ ions going onto sodium sites and chlorine ions going onto chlorine sites. Consider the following quasichemical point defect equation for the dissolution of CdCl2 into NaCl. NaCl i X ′ ; ∆G sol CdCl2 Cd Na + 2 Cl Cl + VNa (9.54) where ΔGsol is the Gibbs energy for the reaction.* The equation has both backward and forward directions: forward = dissolution and backward = precipitation. The equilibrium constant for this X reaction can be written as (because [Cl Cl ] ≅ 1) ∆Gsol Cd iNa VNa ′ = K = e − RT e a CdCl2 (9.55) where a CdCl2 is the thermodynamic activity of CdCl2. A point defect equation such as Equation 9.54 must again have (1) mass balance (both sides of the equation must have the same mass: CdCl2 on both sides here), (2) charge balance (both sides must have the same charge: zero here), and (3) site balance (on the right-hand side of the equation, the number of cation and anion sites involved in the host lattice (NaCl) must be in the same ratio of anions and cations in the compound: 2 cation:2 anion in this case.† The Cd2+ replacing a Na+ ion has a net positive charge relative to the perfect crystal, hence the 1+ charge notation, which must be balanced by a negatively charged sodium ion vacancy, ′ .‡ The electrical neutrality requirement becomes VNa Positive charge/cm 3 = Negative charge/cm 3 (1)( e ) ( ηCd • Na ) = (1)( e ) ( η ′ VNa ) ′ , is created. so that for every cadmium ion, Cd2+, that goes into solid solution, a sodium vacancy, VNa If the concentration of vacancies created by the CdCl2 is much greater than the intrinsic concen′ ] is independent of temperature and depends only on the concentration of tration, then the [ VNa ′ ] ≅ [Cd iNa ] to maintain electrical neutrality. The vacancy CdCl2, [CdCl2], in solid solution, and [ VNa concentrations now depend on something other than the intrinsic properties of NaCl but depend on something from the outside, or extrinsic to the NaCl. Therefore, vacancy concentrations controlled by additives or impurities are called extrinsic vacancies or extrinsic point defects and the diffusion and diffusion coefficients that result are called extrinsic diffusion and extrinsic diffusion coefficients, respectively. Figure 9.13 schematically shows the results of a classic experiment on the effects of additives such as CdCl2 on the diffusion of sodium in sodium chloride showing both the intrinsic—Q = ΔHm + ΔHS/2—and the extrinsic region—Q = ΔHm—which depends on the level of CdCl2 additive, or doping. The extrinsic region exists at the lower temperatures where the extrinsic vacancy concentration is greater than the intrinsic vacancy concentration. At higher temperatures, because of the exponential temperature dependence of the intrinsic vacancy concentration, the * † ‡ A result of Equation 9.54 is that the formation of the solid solution of x-moles of CdCl 2 in NaCl can be written as xCdCl 2 + (1 − 2 x )NaCl = Na 1− 2 x Cd x Cl or Na1−2 x Cd x ( VNa ′ ) x Cl. NaCl i X ′ + 2 VCli Note that Equation 9.54 could also be written as CdCl 2 + 2 VNa Cd Na + VNa′ + 2Cl Cl. Cl− going on Cl− sites are electrically neutral and the neutrality is frequently designated with a superscript X, which is really not necessary. Also, it is useful, as shown in Equation 9.54 to indicate the host crystal—NaCl over the arrow. 303 Chapter 9. Atomistics of Diffusion Slope: − ΔHS+ΔHm 2.303 R Slope: − ΔHm log10D(Na+) 304 2.303 R Intrinsic Extrinsic [CdCl2] 1/T(K) FIGURE 9.13 Idealized plot of the diffusion of sodium in sodium chloride with additions of CdCl2 that create sodium ion vacancies giving rise to extrinsic diffusion at low temperatures. As the concentration of ′ ] and the sodium diffusion coefficient. CdCl2, [CdCl2], increases, so does the [VNa intrinsic vacancy concentration will exceed the extrinsic concentration and the slope of the log10D versus 1/T curve will increase at higher temperatures. Note that if the a CdCl2 = 1, then Equation 9.55 gives the solubility of CdCl2 in NaCl as a function of the temperature. It should also be noted, that a different, but perfectly valid, point defect reaction for the solution of CdCl2 into NaCl can be written as x CdCl2 NaCl → Cd •Na + Cl Cl + Cl′i ; ∆G sol (9.56) with the extra chlorine ion going into an interstitial position to balance the charge of the cadmium on the sodium site. The reality is that both reactions, Equations 9.54 and 9.56 will take place simultaneously, and both vacancies and interstitials will be produced. However, the important reaction is the one that takes place to a greater extent. In this case, it is very difficult to “squeeze” an extra chlorine ion into the NaCl unit cell. As a result, the ΔGsol for the reaction in Equation 9.56 will be much larger than for the formation of the sodium vacancies and the concentration of interstitials will be much less than the concentration of vacancies. However, for a real material, only an experiment would show which of the two reactions dominates. The diffusion data for CdCl2 in NaCl strongly suggests that the cadmium ion’s charge is compensated by the formation of sodium vacancies rather than chlorine interstitials. Extrinsic behavior in compounds is much more important than just academic interest. First, as was shown above for aluminum oxide at its melting point, the concentration of intrinsic vacancies is only a few tenths of a part per billion! To observe intrinsic diffusion in Al2O3 then the impurity concentration must be less than this or the material must be purer than nine-9s pure! This is about the purity of semiconductor-grade silicon, which has a considerably lower melting point and is much easier to purify. As a result, property measurements on Al2O3 that depend on point defect concentrations, such as diffusion, will almost always be measuring extrinsic rather than intrinsic behavior. On the contrary, in Chapter 7, it was shown that cubic ZrO2 could be made the stable phase down to room temperature by additives such as CaO and Y2O3 that can go into solid solution up to about 20 m/o (Figure 7.31). One of the reasons that these additives stabilize the cubic structure is, in addition to the additive cation, vacancies are created that also help make the phase transformation from cubic to tetragonal to monoclinic more difficult. For example, if Y2O3, yttrium oxide, is added to ZrO2, oxygen vacancies are created: ZrO 2 ′ + 3OOX + VOii . Y2O3 2YZr (9.57) 9.4 Vacancy Mechanism of Diffusion in Solids With some 10 or 20 m/o Y2O3 in solid solution, the vacant oxygen concentration is on the order of ηVOii ≅ 1021 cc −1, many orders of magnitude higher than the intrinsic vacancy concentration. So the oxygen vacancy diffusion coefficient is very high even at modest temperatures (Table 9.5). As will be seen later in Chapter 13, the oxygen ion electrical conductivity is directly proportional to the oxygen ion diffusion coefficient and such heavily doped ZrO2 has a high oxygen ion electrical conductivity at relatively low temperatures. As a result, it has been used as an oxygen sensor in automobiles for many years because of its high ionic conductivity. Similarly, it serves as the solid electrolyte in SOFCs, solid oxide fuel cells that are being considered for power generation, energy storage, and automobile propulsion. 9.4.11 nonstoichiometry 9.4.11.1 General Concept Most of the time, compounds in phase diagrams are shown as essentially vertical lines and do not show any solid solution between the end members as shown schematically in Figure 9.14. The main reason for this is that in compounds, solid solutions would require the formation of extrinsic point defects, which takes considerable energy and so the solubility is limited. As noted, Equation 9.56 represents the solubility of CdCl2 in NaCl if the activity of CdCl2, a CdCl2 = 1 (or some other constant value). However, as shown in the inset in Figure 9.14, particularly at higher temperatures for a general compound AB, the exact 1:1 stoichiometry of A:B does not hold and the stoichiometry of AB can vary between AB1−x to AB1+y, where x ≠ y in general. Now x and y are generally small, on the order of 10−6 or 10−4 (and may be much larger in some materials), but can have a significant effect on properties such as diffusion because the nonstoichiometry is taken care of by the creation of point defects, frequently vacancies. For an ionic compound with A2+ and B2−, AB i X 2A A + B(g) 2A A + BB + VA′′ ; ∆G R (9.58) where ΔGR is the energy for the reaction, mainly the energy to create a vacancy. The equilibrium constant for this reaction is 2 ∆G A iA VA′′ − R = K e = e RT p(B) (9.59) Tmp AB±x Liquid l + AB l + AB Temperature (°C) AB A + liq AB + liq AB + liq B + liq A + AB A B + AB AB B FIGURE 9.14 A–B phase diagram with a single compound AB that exhibits virtually no solid solubility of either excess A or B. However, as shown by magnified region in the insert, there is in reality a range of solid solubility AB ± x or nonstoichiometry that might be small—x 10 −4—but introduces defect concentrations greater than intrinsic concentrations that can control defect-dependent parameters such as the diffusion coefficient. 305 306 Chapter 9. Atomistics of Diffusion because A A ≅ 1 and BXB ≅ 1. If the gas pressure, p(B), the temperature, T, and the energy for the reaction, ΔGR, are known, then Equation 9.59 can be solved for the point defect concentrations, which may or may not be higher than the intrinsic concentrations. In fact, in a real material, intrinsic defects, impurities or additives, and nonstoichiometry all need to be considered together to determine the defect concentrations that will, in turn, determine the values of the material parameters such as the diffusion coefficient. 9.4.11.2 Example: Nonstoichiometry in Fe2O3 To make this more concrete, consider the loss of oxygen from Fe2O3 to make it nonstoichiometric, Fe 2O3−x, where the missing oxygen implies vacant oxygen sites, for example,* 1 2Fe Fe + OO 2Fe′Fe + VOii + O2 (g); ∆G R 2 (9.60) Equation 9.60 says that some Fe+3 ions (FeFe) are being reduced to Fe2+ ions (Fe′Fe ) with the loss of oxygen and the formation of oxygen vacancies. An equilibrium constant can be written for Equation 9.60, namely 2 ∆G Fe′Fe VOii p1O/22 − R RT (9.61) = = e K e 2 Fe Fe If the concentration of vacancies is small, then [ Fe Fe ] ≅ 1 and the electrical neutrality condition requires that ηFe′Fe = 2ηVOii and ηFe = 2ηFe2O3 and ηO = 3ηFe2O3 resulting in [ Fe′Fe ] = 3[ V ii ], so Equation 9.61 becomes 2 9 VO•• VO•• p1O/ 22 = K e = e − ∆G R RT and finally, 1 ∆G R − 1 3 V = pO−(21/ 6)e 3RT . 9 •• (9.62) Suppose ∆G R = 3 eV /mol ≅ 3 × 96, 500 J /eV = 289, 500 J /mol and pO2 = 10 −6 bar then at T = 1200°C 1 1 289,500 1 3 1 6 − VO•• = −6 e (3 × 8.314 × 1473) = 1.882 × 10 −3 9 10 For Fe2O3, the density is ρ = 5.24 g/cm3 and the molecular weight M = 159.69 g/mol. Therefore, ηFe2O3 = η = ρ 5.24 g /cm 3 NA = × 6.022 × 1023 mol −1 = 1.98 × 1022 cm −3 M 159.69 g /mol and ηO = 3η = 3 × 1.98 × 1022 = 5.93 × 1022 cm −3 and ηFe = 2η = 2 × 1.98 × 1022 = 3.95 × 1022 cm −3. So the number of vacant oxygen ions per cm3 is ( )( ) ηVO = VO•• ηO = 1.82 × 10 −3 5.93 × 1022 = 1.08 × 1020 cm −3 •• Now, for Fe 2O3−x, ii ηO 3 − x ηO − ηVOii 3 − 3 VO = = = ηFe 2 (2 / 3)ηO 2 * If the temperature is high enough, the electron is ionized off of the Fe′Fe , so Equation 9.60 could be written X ii O O VO + 2e′ + 1 2 O 2 ( g ); ∆G R . See Appendix A.9 for more details. 9.5 Other Diffusion Processes and Solids so x = 3[ VOii ] or the formula is Fe 2O3(1−[ VOii ]) not surprisingly. So for this example, the composition is Fe 2O3−0.0055 or Fe 2O2.99454 .* 9.5 9.5.1 OTHER DIFFUSION PROCESSES AND SOLIDS inorgAnic glAsses There are many different kinds of inorganic glasses such as chalcogenides, phosphates, borates, and silicates, but silicate glasses embody by far the greatest number of applications for these materials: just look out the window! All of these materials readily form glasses because of their very open structures with oxygen polyhedral sharing corners as seen in Chapter 7, for example Figure 7.39, which leads a very open glass or crystal structure. Again, to make the discussion more concrete, silicate glasses are examined. Crystalline SiO2 melts at 1705°C and has a glass transition temperature of about 1475 K. However, with such a high Tg, very high temperatures are needed to be able to get the pure silica glass viscosity low enough to work the glass and fabricate all the kinds of things that are made from glass. The viscosity decreases with temperature because oxygen–silicon–oxygen bonds are being broken by thermal energy decreasing the connectivity of the three-dimensional silica network. Fortunately, the silica network can be more easily broken up with the addition of additives such as Na2O and CaO and other alkali and alkaline earth oxides. This can be understood as the creation of extrinsic point defects: 2 2 Na 2O SiO → 4 Na ii + VSi′′′′ (9.63) where the sodium ions go into the large interstitial sites in the SiO 4− 4 tetrahedral network and are compensated by a vacant silicon site with a net charge of 4−. So, the four oxygens, which were associated with the tetrahedron that now has a silicon vacancy, are now dangling bonds or dangling oxygens because they are no longer joining two tetrahedra at their corners: the network is being broken up (Figure 9.15).† As a result, at a given temperature, SiO2, which has appreciable concentrations—10 wt.% Non-bridging oxygen ions O−2 Na+ Si+4 FIGURE 9.15 Schematic structure of a Na2O–SiO2 glass that shows the Na+ interstitial ions that electrically compensate for silicon vacancies that result in nonbridging oxygen ions. * This could also be obtained by the following solid solution reaction: 2 xFeO + (1 − x ) Fe 2 O 3 Fe 2 O 3 − x † since Fe′Fe is an Fe2+ ion on an Fe3+ site in the Fe2O3 crystal. Note that the extra electron on the Fe+2 ion can easily move to a neighboring Fe+3 ion, and so on, through the crystal giving an electrical current and electronic conductivity. This model of electronic conductivity is the so-called hopping electron or small polaron model of electronic conductivity in nonstoichiometric compounds. In reality, Figure 9.15 represents the structure of amorphous B2O3 better than it does SiO2 because boron is coordinated by three oxygen ions in a plane, whereas silicon is coordinated by four oxygen ions at the corners of a tetrahedron. 307 308 Chapter 9. Atomistics of Diffusion or more—of modifiers, alkali and alkaline earth oxides, has a much lower viscosity than pure silica glass, resulting in a much lower glass transition temperature—below 600°C. Also, because of the open structure, interstitial diffusion in silicate glasses would be expected and many gases diffuse in them as interstitials (Table 9.5). Similarly, the alkali ions such as Na+ are interstitials as well and have a large diffusion coefficient characteristic of interstitial diffusion. 9.5.2 diFFusion in polymers Figure 9.16 shows the two mechanisms by which diffusion can take place in polymers. The first is the familiar interstitial diffusion of gases through the relatively open structure of an amorphous polymer, either above or below the glass transition temperature. Therefore, it is very similar to interstitial diffusion in inorganic glasses but has the advantage that there is little interaction between the diffusing gas and the nonpolar polymer. As a result, interstitial diffusion is relatively fast and is very important commercially because polymers are used as gas separation membranes to separate different gases by their rates of diffusion (Kesting and Fritsche 1993; Mulder 1996). Such membranes are used to separate impurity gases (e.g., H2S) from methane pumped from natural gas wells and CO2 from biogas. In this application, the degree of separation really depends on the product of the gas diffusion coefficient D and its solubility in the polymer, S, that is, P = DS, where P is called the permeability and is the important parameter for this application. Gas permeation by diffusion will be discussed in more detail in Chapter 10. Although there are abundant data on the permeability of different polymers to different gases, the permeabilities are generally not separated into the solubility and diffusion coefficients (Mark 2007). As a result, interstitial diffusion coefficients for different gases in different polymers are not always readily obtainable but, with some searching, they can be found (Van Krevelen 1997). What about the self-diffusion of the polymer molecules? It is not easy for the individual polymer molecules to move when entangled with other polymer molecules in a polymer melt or solid. As schematically shown in Figure 9.16, the individual polymer molecules are restrained from moving transverse to their long axis because of the neighboring molecules. However, they can move along their length or long axis by the thermal generation and movement of small “defects” along their length. When a defect of length L has moved to the end of the molecule, the molecule has moved a distance L. This motion is very similar to the way in which reptiles move and, hence, is called reptation. This mechanism of diffusion has been analyzed by considering the motion of the polymer molecule of n-monomer units inside a “tube” in the polymer melt about 5 nm in diameter, roughly the amount of space between polymer molecules. Not too surprisingly, the result is similar to Equation 9.12; namely (Balluffi et al. 2005) 1. Interstitial gas 2. Polymer molecule diffusion path En lar reptation path g ed L Motion 5 nm Defect FIGURE 9.16 Diffusion in polymers showing (1) how small gas atoms can diffuse interstitially between the polymer molecules and (2) polymer diffusion along the length of the molecule by the process of reptation, where the polymer molecules move along their length inside a tubular volume by the motion of kink-like defects of length L. 9.5 D≅ 1 L f 6 n Other Diffusion Processes and Solids 2 (9.64) where: f is the frequency related to the defect motion L/n is a fractional length of the polymer chain similar to the jump distance in Equation 9.12. Equation 9.64 indicates that the diffusion coefficient is inversely proportional to the square of the length or molecular weight of the polymer chain. As a result, diffusion by reptation gets rather insignificant with large molecular weight polymers. Table 9.5 gives data for reptation diffusion for two polymers normalized to a molecular weight of 150,000 g/mol (Sperling 2006). Clearly, these diffusion coefficients at these low temperatures will not lead to any observable composition changes in reasonable periods of time and this process of reptation is not very important for composition changes and phase transitions. On the contrary, these small movements of polymer molecules can have important effects on dielectric and mechanical relaxation processes. 9.5.3 diFFusion in A VAriety oF solids Table 9.5 gives data for diffusion in a variety of solids collected from a number of sources. This compilation is not the result of an exhaustive search nor have the data been evaluated to present what appear to be best values of the parameters from available literature data. Rather, the information is presented to show how the discussion about diffusion mechanisms leads to actual diffusion coefficients and activation energies for different materials. First, the separation into the various material categories is somewhat artificial because, for example, “semiconductors” really refers to a property—electrical conductivity—that is, the conductivity is somewhere in between that of a good conductor and that of an insulator. Nevertheless, this method of classification of materials is rather common and various materials are recognized as being in one of these categories. A very good compilation on diffusion in solid and liquid metals is readily available and used as a source for data in this table (Brandes and Brook 1992). Similarly, there is a good compilation of diffusion data for semiconductors and liquids (and gases) (Haynes 2013). There are other sources for information on semiconductors as well as alkali halides and some oxides (Gray 1972). There is a continuing series of publications that provides current abstracts on diffusion data for ceramics without any compilation or evaluation of the data (Fisher 2011). An extension of this is the publication Defect and Diffusion Forum published by Trans Tech Publications (http:// www.ttp.net). Probably the most extensive publication of data on solids is in the Landolt-Börnstein Tables and Springer Materials published by Springer (http:\\www.materials.springer.com). As was shown for aluminum oxide, a material that has a high melting point, the energy to form intrinsic defects is also large so the concentration of defects at almost all temperatures is very small. As a result, measured diffusion coefficients can be influenced by small concentration of impurities, making it difficult to separate extrinsic and intrinsic behavior. Therefore, computational materials science techniques are frequently used to calculate defect formation energies and diffusion parameters (Catlow and Mackrodt 1982). These types of calculations have a long history (Mott and Gurney 1948), and, with the computational techniques and computing power available today, calculated parameters can be more reliable than those measured in experiments. Several of the parameters for the high-temperature materials in this table are actually calculated values. Table 9.5 shows that interstitial diffusion is typically on the order of D ≌ 10−6 cm2/s regardless of the material, but at different temperatures, of course. On the contrary, vacancy diffusion coefficients are on the order of D ≌ 10−10 – 10−12 cm2/s at the melting point, regardless of the material. Two unusual cases with high diffusion coefficients are that of oxygen in 15 w/o CaO in solid solution in ZrO2 and beta alumina, Na 2O ⋅ 11Al 2O3. Calcia-doped zirconia, Zr0.85Ca 0.15O1.85, was shown to have a very large concentration of oxygen ion vacancies and, therefore, is expected to have a high oxygen diffusion coefficient. Beta alumina has a hexagonal crystal structure with all of the sodium ions residing in planes perpendicular to the hexagonal axis with only about half of the possible sodium sites occupied. Therefore, the sodium ions can move very easily and the diffusion can be considered as either interstitial with a large interstitial concentration or as vacancy diffusion with about half 309 310 Chapter 9. Atomistics of Diffusion of the sites vacant. Both of these materials behave as solid electrolytes and are being considered for power generation and electrical energy storage. It is worth noting that the difference between interstitial and self-diffusion coefficients is best illustrated in a solid such as iron or steel. Because of its industrial importance in the heat treatment of steels, the diffusion coefficient of C, an interstitial, and the self-diffusion coefficients of iron are reasonably well characterized. From Table 9.5, at 1000°C, the diffusion coefficient of the interstitial carbon is 2.90 × 10−7 cm2/s, whereas that of iron via a vacancy mechanism is 1.93 × 10−10 cm2/s, the difference being mainly in the energy necessary to form vacancies. So the diffusion of carbon in iron is much faster than the diffusion of iron, and during the heat treatment of steel, it is the diffusion of carbon that controls the changes in composition and microstructure, which, in turn, determine the mechanical properties of the steel. 9.5.4 surFAce And grAin boundAry diFFusion Dislocations, grain boundaries, and surfaces are possible paths for rapid diffusion compared to diffusion through the crystal lattice or amorphous structure in a solid (Shewmon 1989). Dislocations and grain boundaries are likely paths for more rapid diffusion because the structure in and around them is distorted and atoms have more room to move from place to place. As a result, atoms or ions that move via a vacancy mechanism might find it easier to diffuse along these paths more so than interstitial atoms or ions. Diffusion along dislocations is called dislocation pipe diffusion or simply pipe diffusion. On surfaces, there is no hindrance to atom or ion motion normal to the surface, so, here too, more rapid diffusion might be expected. Such diffusion processes are difficult to model and perhaps even more difficult to unequivocally determine. One of the reasons for this can be analyzed with Figure 9.17, which models a single grain in a polycrystalline material surrounded, of course, by grain boundaries.* In this figure, assume that the material is copper and zinc is being diffused from the vapor into the copper via a vacancy mechanism. The zinc atoms may indeed move faster down the grain boundaries into the copper. How important this is to the overall composition as a function of distance and time into the bulk of the copper depends on the relative fluxes of zinc diffusing down the grain boundaries compared to the flux through the crystal. Consider the ratio of these total diffusion fluxes: Flux gb A gbJ gb ( πd δ 2 ) Dgb dC = = Flux g A gJ g πd 2 / 4 Dg dx ( ) (9.65) where: the subscript “gb” refers to the grain boundary and “g” to the grain A is the area D is the diffusion coefficient δ is the thickness of the grain boundary d is the grain size or diameter x is the direction perpendicular to the surface. δ d Grain boundaries FIGURE 9.17 An idealized circular grain of diameter “d” in a polycrystalline material with grain boundaries that have a width for diffusion of “δ.” The importance of grain boundary diffusion on the change of concentration normal to the surface depends on the ratio of δ:d—if small, not important, if large, it is. The grain boundary thickness, δ, is divided by 2 because only half of the material diffusing down it competes with the diffusion down the grain. Equation 9.65 becomes Flux gb 2δDgb . == Flux g dDg (9.66) Most of the parameters in Equation 9.66 are essentially constant in a given material with the exception of the grain size d. As a result, the amount of zinc diffused into a material along the grain boundaries relative to that in the grains * In a real polycrystalline material, the grain would not be circular but more like a hexagon if the grain boundary energies were isotropic and the edges of the grain would be straight and not curved. A circular grain is assumed to make the approximations easier. 9.6 Diffusion in Gases 311 will depend on the grain size. Assume that the grain boundary diffusion coefficient is about the same as for interstitials or Dgb ≌ 10−6 cm2/s; the width of grain boundary is slightly larger than the interatomic separation in the crystal, δ ≅ 3 × 10 −8 cm. From Table 9.5, the diffusion coefficient of zinc into copper at 1000°C is Dg ≌ 5 × 10−9 cm2s. With these values, Equation 9.66 becomes ( )( ) −8 10 −6 Flux gb 2 3 × 10 1.2 × 10 −5 = = . Flux g d d 5 × 10 −9 ( ) (9.67) For copper, a grain size of 10–100 μm (10−3 to 10−2 cm) or larger would be realistic for a typical polycrystalline copper. So the grain boundary contribution to diffusion would be only 0.1%–1% of that in the bulk and would have little effect on the zinc composition as a function of distance into the material. On the contrary, if this were nano-grain size copper, say d ≌ 10 nm ≌ 10−7 cm, then the grain boundary diffusion would dominate and determine the composition as a function of distance and time. A little more is said about grain boundary diffusion in Chapter 11 when measurement of diffusion coefficients is discussed. One final note about grain boundary diffusion is that care must be taken to clearly define what the “grain boundary” consists of: is it really an array of dislocations, a structural rearrangement at the interface of two grains to accommodate the difference in their relative crystallographic orientations, or more something more complex? For example, impurities in compounds really do not like to go into solid solution because vacancies or other kinds of extrinsic defects are created, for example, Equation 9.54, which takes energy so their solubility is limited. As a result, impurities would rather form a second phase, perhaps continuous at grain boundaries. For example, SiO2 is a common impurity in most polycrystalline oxides and it can react with the host oxide or other impurities to form a silicate glass that wets the grain boundaries. In such a material “grain boundary diffusion” may actually represent interstitial diffusion in a silicate glass that can be much faster than in the crystalline host. 9.6 9.6.1 DIFFUSION IN GASES the diFFusion coeFFicient In gases, gas atoms are moving at high velocities and collide with other atoms changing their paths and mix by these collisions (Figure 9.18). As was seen in Chapter 8, the diffusion coefficient for a gas can be written in the very general form: 1 D = vλ 3 (9.68) where: v is the molecular or atomic speed λ is the mean free path, or the distance between collisions. It was shown in Chapter 7 that the RMS speed of molecules in a gas is given by 3RT M = v v= rms a (9.69) and the mean speed by v= 8 RT π M where: R is the gas constant = 8.314 J/mol K T is the temperature, K M is the molecular weight, kg/mol. b c m (9.70) FIGURE 9.18 Schematic diagram showing a few collisions of atom of mass “m” colliding with three other gas molecules, at a, b, and c, that change the direction of the atom and produces “random thermal mixing,” diffusion, of the atoms. 312 Chapter 9. Atomistics of Diffusion In gas diffusion, the atoms are moving at high velocities and the distance they travel before a collision, the mean free path = λ, is determined by how far apart the atoms are in the gas phase—or on the number of atoms per unit volume. To model the diffusion coefficient in a gas, the mean free path must be determined. 2dAB dA dB vR r 9.6.2 FIGURE 9.19 Geometry used to calculate the number of collisions per unit time that a gas atom traveling at a relative velocity of vR and diameter dA makes with other gas atoms of diameter dB. If a B atom has its center within a distance of dAB of A, then it will collide with A, so the collision volume swept out by A per unit time is volume = πd2AB vR. meAn Free pAth in A gAs To calculate the mean free path of a gas atom, the corners of the circuitous path in Figure 9.18 can be neglected and the path straightened as shown in Figure 9.19, where a cylinder of gas of length vR is considered. To be completely general, it is convenient to consider the interdiffusion of two gases, A and B, so their relative speed, vR, needs to be considered. Their respective velocities are vectors, vR = vA + vB, but as shown in Figure 9.20, on the average, two atoms will collide on paths that are normal to each other so v R = v 2A + v 2B . − V R A − V A − V B B FIGURE 9.20 Relative gas atom velocities. On the average, the velocities of A and B will be perpendicular to each other in a collision, so vR2 = v 2A + vB2 . (9.71) For self-diffusion in the gas, A = B, the relative velocity is simply vR = 2 vA . So the distance an atom of A will move in one second relative to atoms of B, which it is going to collide with is the length of the column of gas in Figure 9.19, vR. Now all the B atoms that are at least halfway into that column will collide with A as shown in Figure 9.19. So, the collision distance and radius r of the column are simply r= dA + dB = d AB 2 (9.72) where: d A and dB are the “collision diameters”—essentially the atomic diameters—of atoms A and B, respectively d AB is simply the mean diameter of A and B. So, the number of collisions per second, Z, that an atom A makes with B atoms is simply the volume of the cylinder times the number of B atoms per unit volume, ηB, in the cylinder. That is Z = π d 2ABvR ηB (9.73) and for self-diffusion, vR = 2 vA , Z = πd 2AB 2 v A ηA . Finally, the mean free path, λ, is the distance traveled per second, vA, divided by the number of collisions per second, Z: λ= vA 1 = . Z 2 πd 2ABηA (9.74) As an example, consider oxygen at 1 bar pressure and 300 K. For oxygen, d O2 = 3.467 × 10 −8 cm (Geankoplis 1972), and η= N A P 6.022 × 1023 × 1 = = 2.41 × 1019 cm −3 RT (83.14)(300) 9.6 The mean speed of the oxygen molecules is v O2 = 8 RT 8(8.314)(300) = π M π(32 × 10 −3 ) = 4.46 × 10 2 m /s = 4.46 × 10 4 cm /s so that the number of collisions per second is ( Z = πd 2AB 2 v A ηA = π 2 3.467 × 10 −8 ) ( 4.46 ×10 ) ( 2.41×10 ) 2 4 19 Z = 5.74 × 109 collisions /s. Notice that this is about the same as the jumps per second for atoms in solids where the temperature is high enough for observable diffusion: for example, for C in iron, Γ ≌ 109 jumps/s at 1000°C. The mean free path for oxygen is λ= 1 ( 2 π 3.467 × 10 −8 ) ( 2.41×10 ) 2 19 λ = 7.77 × 10 −6 cm = 0.0777 × 10 −4 cm 0.1 µm which means that the jump—collision—distance in gases is almost 1000 times that of a solid. As a result, diffusion coefficients in gases are—because of the 104 faster speed and 103 greater jump distance—about 107 times higher than interstitial diffusion in solids or on the order 1 cm2/s. As will be seen, this is a good approximation. 9.6.3 the gAs diFFusion coeFFicient For interdiffusion between two gases A and B, again, D AB = (1/ 3)vR λ. So, v R = v 2A + v 2V 1 8 RT 8 RT 2 = + π MA π MB (9.75) 1 1 1 2 2 1 8 v R = RT + π MA MB and the mean free path is given by λ= = λ= 1 2 πd 2ABη 1 2 πd 2AB ( PN A /RT) (9.76) 1 RT 2 2 πN A d ABP Putting Equation 9.75 in for vR, Equation 9.76 for λ, and combining all the constants into the first factor: D AB 1 1 1 8 2 = vRλ = R 3 3 π 3 1 1 2 T2 1 + 2 πN A M A M B d 2ABP (R ) Diffusion in Gases 313 314 Chapter 9. Atomistics of Diffusion Evaluation of the constant term gives 1 1 8 2 R 3 π 83.14 6 10 2 π 6.022 × 1023 1 ( R ) = 1 8 8.314 2 2 πN A 3 π ( ) kg1/ 2 bar m 4 = 4.765 × 10 −29 1/ 2 3/ 2 mol K s if the Units(M A) and Units(MB) are kg/mol, Units(d AB) = m, Units(T) = K, and Units(P) = bar, then the Units(DAB) = m2/s. So, the final result is, 1/ 2 1 1 D AB = 4.765 × 10 −29 + MA MB T 3/ 2 2 m /s d 2ABP If the more convenient set of units is chosen: Units(Mi) = g/mol, Units(d AB) = 10−8 cm or Ångstroms, and Units(P) still bar, then multiplying the above by (103 g /kg)1/ 2 (1020 Α2 /m 2 )(10 4 cm 2/ m 2 ) to get a much more convenient set of units to work with 1 D AB 9.6.3.1 1 2 T 3/ 2 1 2 = 1.507 × 10 + 2 cm /s. M A M B d ABP −3 (9.77) Example 1: He and Ar Interdiffusion at 298 K d(Ar) = 3.542 × 10−8 cm, d(He) = 2.551 × 10−8 cm (Geankoplis 1972), M(Ar) = 39.9 g/mol, M(He) = 4.0 g/mol. Therefore, d AB = (3.542 + 2.551)/2 = 3.00 × 10−8 cm, so 1 D He−Ar 1 2 ( 298 ) 1 = 1.507 × 10 + 2 4.0 39.9 ( 3.00 ) (1) 3/ 2 −3 D He−Ar = 0.452 cm 2 /s which can be compared with a measured value of D = 0.729 cm2/s (Cussler 1997; Haynes 2013) and is different by less than a factor of 2. Note that the diffusion coefficient for helium and argon can be written as D He−Ar = 0.87 × 10 −4 T 3/ 2 P which is why the approximation for diffusion in gases is roughly D 10 −4 (T 3/ 2 /P ). 9.6.3.2 Example 2: H2O in N2 at 298 K and 1 bar d(H2O) = 2.641 and d(N2) = 3.798 (Geankoplis 1972), M(H2O) = 18.0, M(N2) = 28.01, so 1 D H 2O − N 2 1 2 ( 298 ) 1 = 1.507 × 10 + 2 28.01 18 ( 3.22 ) (1) 3/ 2 −3 which gives D H2O− N2 = 0.226 cm 2/ s compared to a measured valued of D = 0.242 cm2/s (Haynes 2013). 9.6.4 the chApmAn–ensKog equAtion The preceding derivation for the gas diffusion coefficient is based on what is known as the hard sphere model because it assumes that there is no interaction between gas atoms or molecules until they touch as shown in Figure 9.21a: the atoms or molecules essentially interact as billiard balls. In reality, gas atoms or molecules will, at a minimum, experience van der Walls attractive forces and electron cloud repulsive forces and are “squishier” than billiard balls and lead to a potential energy 9.6 Potential energy Potential energy Electron repulsion dAB 0 Van der Waals attraction 0 Distance Distance (a) (b) FIGURE 9.21 (a) Potential energy versus distance for a “hard sphere” model for atoms and molecules colliding in the gas phase. (b) Potential energy versus distance curve for a combined van der Waals attractive and a power dependence of the electron repulsion at small separation distances as an attempt to model gas collisions more precisely with a more realistic interatomic potential energy. versus distance curves that look more similar to that shown in Figure 9.21b. Taking into consideration such a potential energy curve leads to the so-called “Chapman–Enskog” equation for diffusion in gases (Geankoplis 1972; Cussler 1997; Bird et al. 2002), 1 D AB 1 2 T 3/ 2 1 2 = 1.86 × 10 + d 2 Ω p cm / s M M B AB AB A −3 (9.78) where ΩAB is the “collision integral” that accounts for the nonhard sphere interaction of the gas atoms, as do some of the d AB values that are used in the calculation of gas diffusivities. The values of ΩAB are generally between about 0.4 and 2.6 can be evaluated from data given in several references (Geankoplis 1972; Cussler 1997; Bird et al. 2002). Note that there is usually not much difference between the DAB calculated from the simple hard sphere model and that calculated with the Chapman–Enskog result. Diffusion coefficients calculated with Chapman–Enskog typically agree with measured gas diffusion coefficients to about 10%, which is good enough for “highway work.” Some of the d ABs that were used in the above calculations were those tabulated in the references for use in this equation. Also, note that for the case of DHe-Ar, Ω ≈ 0.5 (Geankoplis 1972), which if included in the above calculation, would make the calculated and measured diffusion coefficients much closer. Also, for the case on interdiffusion of H2O and N2, Ω ≈ 1.0 (Geankoplis 1972), so that the hard sphere calculation and the experimental values are much closer. The most important point is that the simple hard sphere model, Equation 9.77, gives all the correct temperature, pressure, collision diameter, and molecular weight dependencies that the more realistic—and more complex—model does. The main differences are in the initial constant and the inclusion of the collision integral. For calculation purposes, in future gas diffusion problems, the results of the simple hard sphere model will be completely satisfactory because the Chapman–Enskog equation only applies to nonpolar molecules. It does not strictly even apply to N2–H2O interdiffusion because it does not include dipolar effects of the H2O molecules: another model is necessary for this. This is a perfect example of, “How good do the models have to be to be useful?” With the simple billiard ball model, gas diffusivities can be computed quite accurately and can—and will—be used to quantitatively model reactions controlled by gaseous diffusion and the models compare pretty well with reality. Given the variety of other uncertainties in most models, improving the value of a gas diffusion coefficient by 10% will probably not have a significant effect of the predictability of the model. Is it important to be able to model gaseous diffusion coefficients more accurately? Yes, but the added complexity may not be important to understand, predict, and control an industrial process of interest. Compared with the uncertainty in the activation energies for defect formation and diffusion in solids that can be 10% or larger, the ability to accurately calculate gaseous diffusion Diffusion in Gases 315 316 Chapter 9. Atomistics of Diffusion coefficients even with the simple model, Equation 9.77, is much better than the ability to calculate solid diffusion coefficients. A difference of 10% in the activation energy can easily lead to a factor of 10 or more in the calculated diffusion coefficient. 9.6.5 Knudsen diFFusion One final point about gaseous diffusion worth mentioning is so-called Knudsen diffusion, which concerns diffusion of gases in porous media where the pore size is smaller than the mean free path in the gas phase. Knudsen diffusion is important in many applications in materials. For example, during the calcining of materials such as carbonates to give oxides, the evolving CO2 gas must diffuse through the porous outer layer of the oxide. As in all cases, the diffusion coefficient for Knudsen diffusion can also be written, D = (1/ 3)vλ. But in Knudsen diffusion, the mean free path is the distance that a gas atom or molecule can diffuse before it hits the wall of the pore as shown in Figure 9.22. In this case, the mean free path is essentially equal to the pore diameter, d, so that the Knudsen diffusion coefficient, DK becomes 1 D K = vd. 3 (9.79) At room temperature and one atmosphere the mean free path in a gas is on the order of 0.1 μm. This means that the pore size would have to be very small for pure Knudsen diffusion. Generally, it is more realistic to consider that both pore and gas collisions might be taking place simultaneously so that the total collision rate, Ztotal is given by Z total = Z gas + Z pore. Dividing the total number of collisions by the molecular speed, v, putting in the definition of the mean free path, λ, and finally dividing by 1/3v gives Z total Zgas Z pore = + v v v 1 1 1 = + λt λg d 1 1 1 = + (1/ 3) vλ t (1/ 3) vλ g (1/ 3) vd where the last equation is 1 1 1 = + D Dgas D K (9.80) which is nothing more than the reiteration of the principle that “when there are series steps, the slower or smaller one controls the rate.” Here, the smaller of the gas and Knudsen diffusion coefficients determines the overall value of D. As an example, take the case of N2 at STP diffusing in a porous material with 10-nm diameter pores. Here, Dgas is given by Atom path d, pore diameter Cylindrical pore FIGURE 9.22 Schematic drawing illustrating the principle of Knudsen diffusion that can occur with gases diffusing in porous material. In pure Knudsen diffusion, the mean distance between collisions of the atoms or molecules in the gas phase, the mean free path, is considerably greater than the diameter, d, of the pores. As a result, gas atoms strike the walls of the pore before they collide with other gas atoms and their mean free paths are now determined by the pore diameter. 9.7 1 D N2 2 2 ( 298 ) = 1.507 × 10 2 28.01 ( 3.798 ) (1) 3/ 2 −3 D N2 = 0.144 cm 2 /s v= 8 × 8.314 × 298 × 102 = 4.74 × 10 4 cm /s π × 28.01× 10 −3 8 RT = π M so ( )( ) 1 1 D K = vd = 4.74 × 10 4 10 × 10 −7 = 1.58 × 10 −2 cm 2 /s 3 3 and from Equation 9.80 D= 1.58 × 10 −2 × 0.144 DK D N2 = = 1.42 × 10 −2 cm 2 /s * DK + D N2 1.58 × 10 −2 + ( 0.144 ) ( ) D K = (1/ 3)vd = (d / 3) (8/π)(RT / M) demonstrates that the diffusion of a gas through a porous material depends inversely on M . So if a mixture of gases with different masses are passed through long small diameter tubes, those with the lighter mass will emerge first. This is the principle of uranium isotope separation by gaseous diffusion. 238UF6 and 235UF6 gases are prepared from the uranium oxide ore and separated by Knudsen diffusion through many miles of corrosion-resistant porous material with the lighter gas, 235UF6 coming out first. By repeated cycling, higher and higher enrichments can be obtained. Gaseous diffusion plants have been displaced by centrifuge facilities for the enrichment of uranium isotopes for a number of reasons, not the least of which, they can be made much smaller—and harder to detect—for a given output. 9.7 DIFFUSION IN LIQUIDS The atomistics of diffusion in liquids is between that for gases and solids but more similar to diffusion in gases, as might be expected, because at the critical temperature, the structure of the liquid and gas are indistinguishable. Therefore, the general equation for diffusion is applied to a liquid; namely, Equation 9.68 1 D = vλ 3 where: v is the molecular speed λ is the mean free path. The mean speed for gas molecules is given by Equation 9.70 v= 8 RT π M and the mean free path is roughly the distance between molecules in the liquid, λ≅ * 1 η1/ 3 Strictly speaking, for a 10-nm pore, the molecular diameter, on the order of 0.4 nm is a sizeable fraction of the pore diameter and this approximate calculation does not take this into consideration. Diffusion in Liquids 317 318 Chapter 9. Atomistics of Diffusion where η is the number of atoms or molecules per unit volume. However, much of the space between molecules is actually taken up by the volume of the molecules themselves. Therefore, a better approximation to λ is λ≅ 1 −d η1/3 where d is the diameter of the liquid molecule. Take water as an example, η= 1 ρ NA ≅ 6.022 × 1023 = 3.35 × 1022 cm −3 18 M ( ) and d H2O ≅ 0.276 nm is the diameter of the water molecule (Wells 1984), so λ≅ 1 1 − d H2O = 1/ 3 η 3.35 × 1022 ( ) 12 − 2.76 × 10 −8 cm = (3.10 − 2.76) × 10 −8 = 0.34 × 10 −8 cm and v= 8 8.314 × 300 × 100 cm /m = 5.94 × 10 4 cm /s. −3 π 18 × 10 Therefore, for water at 300 K, D ≅ (1/ 3)(5.94 × 10 4 cm /s)(0.34 × 10 −8 cm ) = 6.7 × 10 −5 cm 2 /s. The literature value for diffusion in water at 300 K is D ≌ 2.4 × 10−5 cm2/s (Robinson and Stokes 2002). This is less than a factor of 3 difference, so this is a pretty good plausibility argument. A better approach to the diffusion in liquids that can be applied more generally is given in Chapter 13. 9.8 CHAPTER SUMMARY This chapter covers the atomistics of diffusion in solids, gases, and an introduction to diffusion in liquids. The model of interstitial diffusion in solids is developed first showing the origin of D0 and Q in the diffusion coefficient D = D0 exp( −Q / RT). The preexponential term, D0, is shown to be D0 = (1/ 6)a 2f exp( − ∆Sm R ), where a is the jump distance ≌ the lattice parameter and ΔSm is the entropy for interstitial motion and usually involves the movement of neighboring atoms allowing the interstitial atom to move. For interstitial diffusion, the activation energy for diffusion, Q, includes only the energy for the interstitial to move, ΔHm. The jump frequency, f, is essentially the vibration frequency of atoms on their lattice sites and several approaches are used to show that f ≅ 1013 Hz . Vacancy diffusion is essentially the same as interstitial diffusion but multiplied by the site fraction of vacancies, [V], which is first determined in an elemental material by a statistical approach and found to be exponentially dependent on the energy to form a vacancy, ΔHf. Therefore, the activation energy for vacancy diffusion is Q = ∆H m + ∆H f and is much higher than the activation energy for interstitial diffusion leading to vacancy diffusion coefficients smaller than interstitial diffusion coefficients in a given material. A quasichemical approach or point defect chemistry is shown to give the same results as the statistical approach and is extremely useful when considering vacancies and interstitials in compounds. The Kröger–Vink notation for defects in compounds is used to balance charges on the crystal lattices. Schottky and Frenkel defects are introduced as intrinsic defects in compounds. Then extrinsic lattice defects produced by impurities, dopants, and atmospheric effects are shown as well as how the atmosphere can change the nonstoichiometry and point defect concentrations in compounds. A major point made, often repeated, that care must be used to distinguish the number of defects per unit volume, for example, the number of vacant oxygen ions per unit volume, ηVOii , and the fraction of oxygen sites that are vacant, [ VOii ], which has no units. It is the site fractions that must be used in chemical equilibria because they have no units and the equilibrium constant also has none. And because they are fractions, they have no charge. There is significant confusion in Appendix the literature about using these different terms in point defect chemistry and can lead to errors of many orders of magnitude in the calculated number of charged species per unit volume of interest in calculating properties. As stated before, literature must be viewed with a critical eye! Point defect chemistry is shown to apply to diffusion in glasses as well. Diffusion in polymers is briefly discussed where the main interest in these materials is interstitial diffusion. Finally, a few comments are made about grain boundary and surface diffusion. A rather simple model of atoms colliding is developed for diffusion in gases that gives quite precise values for gaseous diffusion coefficients. This model is applied to diffusion in porous media, Knudsen diffusion, and demonstrates that small pore sizes can limit the mean free path of gas atoms and molecules and determine the value of the diffusion coefficient. Finally, a plausibility argument is given for diffusion in liquids similar to the argument for diffusion in gases that predicts reasonable values for diffusion coefficients. An alternative approach that is more commonly used to model diffusion in liquids is left to Chapter 13. APPENDIX A.1 solution to x″ + ω2x = 0 For a mass m vibrating on a spring with a force constant, β, the equation of motion is F = ma = m d 2x = −βx dt 2 d 2x β d 2x + x = + ω2x dt 2 m dt 2 (A.1) where ω2 = β/m. Equation A.1 is a linear ordinary differential equation with constant coefficients and the standard method for solving such equations is to assume that the solutions are of the form x = e λt (Kreyszig 1988), which gives for the “characteristic equation,” λ 2eλt + ω2eλt = 0 λ 2 + ω2λ = 0 (λ − iw )(λ + iω) = 0 which has roots of λ = ±iω, where i = −1. The general solution is x = c1eiωt + c2e − iωt = c1 ( cos ωt + i sin ωt ) + c2 ( cos ωt − i sin ωt ) = ( c1 + c2 ) cos ωt + ( ic1 − ic2 ) sin ωt (A.2) x = A cos ωt + B sin ωt because e ix = cos x + i sin x (which is easily seen from the infinite series of the three functions). In other words, the solution to the mass on a spring equation is sinusoidal motion and whether it is a cosine or sine solution or a combination depends on the conditions at t = 0. The angular frequency is ω = β /m, rad/s, and the frequency, f, Hz (s−1) is given by f= 1 β ω . = 2π 2π m (A.3) 319 320 Chapter 9. Atomistics of Diffusion A.2 Y T ds dy θ + dθ θ T dx x X x + dx VibrAtions oF string The following derivation of the vibration of a string is covered in many books where different approximations are made (Pearson 1966; French 1971; Main 1984; Elmore and Heald 1985; Pain 1999) but all leading to the same result, the wave equation for a vibrating string. Figure A.1 shows a tiny part of vertically displaced string with arc length ds with mass per unit length, μ (kg/m) under a tension, T (Newton). Now from Figure A.1, the arc length is given by ( ds ) FIGURE A.1 Geometry to determine the transverse vibrations of a string. 2 ≅ ( dx ) + ( dy ) 2 2 (A.4) which can be manipulated in the following way ( ds ) 2 2 2 dy ≅ ( dx ) 1 + dx so 2 dy ds ≅ 1 + dx dx (A.5) which is the formula for arc length, ds. If the string is not displaced too far in the y direction so that slope dy/dx ≌ 0, then ds ≌ dx ≌ Δx so the mass of the string of length “ds” is dm = µds ≅ µ∆x . The forces in the x and y directions are Fx = T cos ( θ + ∆θ ) − T cos ( θ ) Fy = T sin ( θ + ∆θ ) − T sin ( θ ) . (A.6) For θ and Δθ very small, cos(θ) ≌ cos (θ + Δθ) ≌ 1 so Fx ≌ 0. Similarly, Fy ≅ T sin ( θ + ∆θ ) − T sin ( θ ) ≅ Tx ( θ + ∆θ ) − Tx ( θ ) ≅ T∆θ (A.7) Now tan θ = ∂y ∂x (A.8) so 1 1 ∂y ( tan θ ) = ∂x ∂x ∂x ∂θ ∆θ ∂ 2 y ≅ = sec θ ∂x ∆x ∂x 2 (A.9) 2 because sec θ = 1/cos θ ≌ 1 when θ is small as it is in this case and partial derivatives with respect to x are being used because the partial derivative with respect to t will be necessary for the acceleration. Therefore, Appendix (dm )a y = Fy ( µ∆x ) (A.10) ∂2y ∂2y θ = T ∆ = T ∆x ∂t 2 ∂x 2 where ay is the acceleration in the y direction (m/s2). Rearranging Equation A.10 gives the desired result: ∂2y 1 ∂2y = ∂t 2 v 2 ∂x 2 (A.11) where the wave velocity, v, is given by v = T /u m /s because Units(T/u) = (m/s)2. A.3 longitudinAl VibrAtions in A solid What follows is very similar to what was done above to develop Equation A.11 for the transverse vibrations of a string. The difference is that, here, longitudinal vibrations along the x-direction in Figure A.2 are considered. This results in the displacement of a section of the solid, Δx, by an amount w in the x-direction. As was true for the vibrating spring, many of the references cited in Appendix A.2 also derive the equation for longitudinal vibrations in a solid and, again, with a variety of different approximations all leading to the same result. In the case of longitudinal vibrations, the piece of solid of length Δx is not only being displaced an amount w, but it is also being stretched in the x-direction by an amount Δw by the opposing forces in the x-direction, Fneg and Fpos. Then the average strain over Δx is Δw/Δx and the average stress, σ, is given by σ = E(Δw/Δx) and at any particular point, σ = F /A = E(∂w /∂x), where A is the cross-sectional area of the bar. Now, σ( x + ∆x) = σ( x) + ∂σ ∆x ∂x (A.12) so Fneg = Aσ( x) = AE Fpos ∂w ∂x (A.13) ∂σ ∂w ∂ 2w = Aσ( x) + A ∆x = AE + AE 2 ∆x ∂x ∂x ∂x or Fnet = Fpos − Fneg = AE ∂ 2w ∆x. ∂x 2 (A.14) x The difference between the forces leads to the acceleration of the piece of material Δx long that has mass, m = AρΔx, where ρ is the density (kg/m3), that is, ma = ( Aρ∆x ) ∂ 2w ∂ 2w = Fnet = AE 2 ∆x 2 ∂t ∂x (A.15) x + Δx (a) and cancelling and rearranging gives the desired result: ∂ 2w ρ ∂ 2w 1 ∂ 2w = = 2 2 ∂x 2 E ∂t 2 v ∂t Δx Fpos Fneg (A.16) which is the wave equation for longitudinal waves in a solid with velocity v = E /ρ because Units(E/ρ) = Pa/(kg/m3) = (m/s)2. w (b) x+w Δw x + Δx + w + Δw FIGURE A.2 Geometry to determine the longitudinal vibrations of a rod. 321 322 Chapter 9. Atomistics of Diffusion A.4 electronic deFects A.4.1 Rationale An extensive review of point defect chemistry including electronic defects is available from many sources (Kröger 1964; Tilley 1987; Barsoum 1997; Chiang et al. 1997; Smyth 2000; Maier 2004), but each of these references uses a different but similar notation with frequent confusion between concentrations (numbers/cm3) and site fractions. In some cases, the notation [ VOii ] is defined as a site fraction in one place then, later, is defined as a concentration, number per cm3 that has been defined here as ηVOii . This is one of the reasons that η was defined as concentration with Units(η) = number/cm3. Although this leads to a slightly more complex notation, it does not lead to the confusion that exists in the literature. Another option used in the literature is, for example, that the Schottky defect is defined as ′′ VOii = K S = ηMgηOe VMg − ∆GS RT ii 3 ′′ ] = ηVMg and [ VMg ′′ and [ VO ] = ηVii are concentrations per cm . As long as this convention is used conO sistently, the resulting point defect equations should give the correct results sought: namely, the concentrations per cm3 as a function of temperature, partial pressures, and dopant concentrations. However, this gets a little messy with something like, say Fe2O3: ′′′ + 3VOii , 0 2VFe where the convention used here gives for the Schottky product 2 3 ′′′ VOii = K S = e VFe − ∆GS RT and the “[]” indicate site fraction. If “[]” is used as concentration then the equivalent equation would have to be: 2 3 ′′′ VOii = K S = η2Feη3Oe VFe Si Si Si Si − ∆GS RT = 108η5Fe2O3 e − ∆GS RT Confusing! Another variation is the use of the notation “VOii,” for both the vacant oxygen species in an equation and the number of vacant oxygen per unit volume! Finally, sometimes the “[ VOii ]” notation is used to represent a site fraction and then used in electrical neutrality expressions, which is clearly incorrect and will lead to incorrect answers: another example of “…just because it’s published does not mean it’s correct…” So when adopting material from these and similar resources, make sure that a consistent point defect chemistry is used and be aware that the literature must be used with caution and, perhaps, corrections. The addition of electronic defects into point defect chemistry is modElectric field eled to show how easy and consistent it is to include them and gives concentrations that are the same as given by a more solid state physics or statistical Si Si A approach. Furthermore, the confusion between concentrations and site fracḣ + − e′ tions described above can lead to large errors in calculated concentrations Si Si Si B that are important for electrical conductivity in particular. So it is important − e′ P Si to have a consistent model of electronic defects along with lattice defects to C + help decipher the confusion that exists in the literature. ḣ B Si Si FIGURE A.3 Schematic drawing of s silicon crystal showing (A) the generation of electron hole pairs by thermal energy; (B) phosphorus dopant acting as an electron donor; and (C) boron acting as an electron acceptor. A.4.2 Intrinsic Electronic Defects Figure A.3 uses a silicon crystal as an example with intrinsic electronic defects, free electrons and missing electrons in covalent bonds, holes, at point A, and extrinsic electronic point defects at points B and C introduced by the dopants phosphorus and boron. First, thermal energy may be sufficient to knock electrons out of bonds (covalent or ionic) leaving behind Appendix an empty electron site that has a charge of plus one relative to the perfect crystal, called a hole and designated h i in Kröger–Vink (K–V) notation. The electron of course is negative and designated e′. So, similar to the Schottky product, the ionization of a bond can be represented as 0 e′ + h i ; Eg (A.17) where Eg is the energy to form the electron–hole pair. As shown in the figure, under the influence of an electric field to the right, the electron will move to the left and contribute to electronic conductivity. Similarly, electrons in neighboring covalent bonds will move to the left and into the hole. This means that the hole moves to the right in the direction of the field, so it acts like a positively charged electron as far as electrical conductivity is concerned. This is why it is given a positive charge. An equilibrium constant can be written for Equation A.17; namely, e′ h • = K i = e − Eg RT (A.18) where [e′] is the fraction of electron energy states occupied [e′] = n /N C , where n is the number of electrons per cm3 and NC is the number of electron energy states per cm3. Similarly, [ h i ] = p/N V, where p is the number of holes per cm3 and N V is the number of hole energy states per cm3. For perfectly free electrons and holes—an empty box with just walls (there are no ions present to scatter electrons and the electrons do not collide)—NC = N V = 2.51 × 1019 cm−3, whereas in real materials that have atoms or ions, they are not the same but usually have not largely different values. These values for the density of states occur because the motion of both electrons and holes behave as waves that are quantized. The Heisenberg uncertainty principle states that the uncertainty in the position, Δx, times the uncertainty in the momentum, Δmv, is given by h 2π ∆x ∆( mv) = where h is the Planck’s constant = 6.626 × 10−34 Js. If the electron or hole is in a cubic piece of silicon that has a length = L, then Δx = L because the electron must be in the silicon, and each electron energy state must be separated by a momentum difference of (∆mv) = h / (2πL) or a kinetic energy difference of h2 1 ( ∆mv ) = 2 2 2 m 8π mL 2 ∆E = and limits the number of states per unit volume. Completing the calculation of the total number of states in three dimensions gives NC = 2.51 × 1019 cm−3 (Mayer and Lau 1990). So, Equation A.18 becomes n p N N C V E − RTg =e and electrical neutrality requires that n = p (always true for intrinsic material) and np = N C N V e − Eg RT so 1 n = p = ( N CN V ) 2 e − Eg 2 RT . For silicon, Eg = 1.1 eV so at room temperature, 300 K (Mayer and Lau 1990), (A.19) 323 324 Chapter 9. Atomistics of Diffusion n = p = 2.51× 1019 e − 1.1 × 96,500 2 × 8.314 × 300 = 1.44 × 1010 cm −3 and makes pure silicon a pretty good insulator at room temperature! A.4.3 Extrinsic Electronic Defects A.4.3.1 Phosphorous and Boron in Silicon Extrinsic electronic defects are produced by additives—dopants—or impurities in the crystal. For silicon, two common dopants are phosphorus, P, and boron, B. Phosphorous has five outer electrons and uses four of them to make four covalent bonds with neighboring silicon atoms in silicon as shown in Figure A.3. The fifth electron is loosely bound and easily ionized to give a free electron. Similarly, boron has only three outer electrons to make three covalent bonds with neighboring silicon atoms leaving one of the four bonds missing an electron, a hole. It too can be easily ionized to move through the crystal and contribute to electrical conductivity. Dopants that donate electrons to conduct are called donor dopants and those that generate holes are called acceptor dopants because they accept electrons from other covalent bonds to give electrical conductivity. To demonstrate the principles of extrinsic electronic defects, consider phosphorus as a dopant. The equation for the P atom to donate an electron is PSiX PSii + e′; E D where ED is the energy to ionize the electron. The equilibrium constant for this reaction is, E PSi• [ e′] − D = K D = e RT X PSi (A.20) and putting the expressions for the site fractions, ( η η) ( n N ( η η) • PSi X PSi C ) = (η )( n ) = K (η ) N • PSi X PSi D (A.21) C where η = ηSi is the number silicon sites per cm3. Now the total number of phosphorus donors per cm3 is the number of ionized and unionized: ηPSi = ηP X + ηPSii . The total electrical neutrality requires Si that ηPSii + p = n, but assuming that the hole concentration is going to be small and can be ignored, ηPSii ≅ n . Therefore, Equation A.21 becomes n2 = N CK D ηPSi − n giving the quadratic equation n 2 + nN C K D − N C K DηPSi = 0 the solution of which is n= n= − N CK D ± ( N CK D ) 2 + 4 N C K DηPSi 2 − N C K D + N C K D 1 + 4(ηPSi N C K D ) 2 Appendix The solutions to this quadratic equation at two extremes are as follows: first, if 4(ηPSi /(N C K D )) 1 then, 1 n ≅ ( N CηPSi ) 2 e − ED 2 RT (A.22) exactly the same as obtained from statistical approaches. Equation A.22 is essentially the case when ED is large. The second extreme is when 4(ηPSi /(N C K D )) 1, then the solution becomes* n= −N C K D + N C K D (1 + 2(ηPSi /(N C K D )) ) 2 (A.23) n ≅ ηPSi or all of the phosphorus atoms are ionized implying that ED is small. For phosphorus in silicon, ED = 0.045 eV (Mayer and Lau 1990) and for a total phosphorus concentration of ηPSi = 1016 cm −3 gives, 4 ηPSi 1016 =4 ≅ 10 −2 1 N CK D 2.51× 1019 ( exp( − 0.045 × 96, 500 8.314 × 300) ) so Equation A.23 should apply and all of the donors are ionized, n ≅ ηPSi = 1016 cm −3. To get a more accurate number, the quadratic equation would have to be solved. Figure A.4 shows the electron concentration as a function of the energy to ionize the donor, ED. This Figure clearly shows that all of the donor will be ionized up to about a value of ED ≌ 0.1 eV, regardless what the host material is.† Silicon doped with 1016 phosphorus atoms per cm3 would have an electronic conductivity about six orders of magnitude higher than intrinsic silicon where n = p = 1.44 × 1010 cm−3. Also, because np = 2.07 × 1020, p = 1.88 × 104! It is clear why the electrons, in this case, are called majority carriers and the holes minority carriers because there is a factor of 1012 difference in their concentrations! Boron, also with a small ionization energy of E A = 0.054 eV for holes (Mayer and Lau 1990), gives Electron concentration, n (cm−3) 1017 1016 1015 1014 1013 nD = 1016 cm−3 1012 1011 1010 0.001 0.010 0.100 Donor ionization energy, ED (eV) 1.000 FIGURE A.4 The effect of the donor ionization energy on the electron concentration for a donor concentration of 1016 donors/cm3. * † n (1 + x ) ≅ 1 + x /n for x small: that is, only the first two terms in the infinite series are important. Donors that are completely ionized and follow Equation A.23 are called shallow donors while those that have larger ionization energies and follow Equation A.22 are called deep donors. 325 326 Chapter 9. Atomistics of Diffusion similar results but for p-type material. It is this ability to dope silicon and other solids to change their electrical properties that have made this the “silicon age.” A.9.4.3.2 Electronic Doping of Compounds Fluorine-doped and indium-doped tin oxide (ITO) are used as transparent conducting oxides (TCOs) for a number of applications including transparent contacts for solar cells, heatable de-icing coating for aircraft windshields and other applications. For pure SnO2 , Eg ≌ 4 eV so the intrinsic electron and hole concentrations are quite small and visible light does not have sufficient energy to create an electron hole pair.* So, it is transparent in visible light and a pretty good insulator. However, it can be doped with fluorine to make a sufficiently good conductor for transparent contacts and de-icing. The doping of SnO2 with fluorine can be written as SnO2 X → SnSn SnF4 ← + 2FO• + 2e′ + F2 (g); ∆G D (A.24) where: FOi represents the F− ion on O−2 site and is a n-type dopant ∆GD is the energy to produce the four point defects: two fluorine on oxygen and two electrons. Also, their concentrations depend on the fluorine pressure.† But this raises a concern, because in Section 9.4.10, such dopants introduced lattice defects. In fact, the solid solution of SnF4 into SnO2 could be written with the formation of vacant tin sites: SnO2 X → SnSn "" ; ∆G V . SnF4 ← + 4FO• + VSn (A.25) This is also a valid point defect formation reaction. Both Equations A.24 and A.25 occur to some extent but which concentration, vacancies or holes, dominates depends on the relative values of the energies, ∆GD and ∆G V. Because fluorine-doped tin oxide is a good electronic conductor, the reaction in Equation A.24 must at least produce enough electrons for good conductivity. A.9.4.4 Kröger–Vink or Brouwer Diagrams There have been many studies of dopants on the electrical conductivity and defect chemistry of different compounds. However, very few of them cover the entire range of possible defect equilibria and not all of the results confirm these simple defect models. Therefore, rather than using data on real materials, a model of an imaginary oxide AO is doped with another oxide, B2O3 is developed. Note that this is not boron oxide but just some general oxide with a cation B3+. Assume that Schottky defects are the predominant lattice defects in AO. So, the complete point defect chemistry in AO is * † ‡ Schottky defect: 0 VA′′ + VOii ; K S Electron-hole pairs 0 e′ + h i ; K i Nonstoichiometry 1 OOX VOii + 2e′ + O2 (g); K R 2 Doping‡ X i B2O3 2BA + 2e′ + 2OO + AO 1 pO (g); K D 2 2 Light energy is given by E = hf = hc /λ ≅ (6.625 × 10 J s) ( 3 × 10 m /s ) / (1.602 × 10 J /eV ) × 10 µm /m = 1.24 eV µm. The lower limit of visible light is about 0.43 mm corresponding to an energy of 2.9 eV. So Eg must be greater than 2.9 eV, so that light is not absorbed by the production of electron–hole pairs. This equation really is the sum of two equations: one to put the SnF2 into solid solution and another to ionize the fluorine to produce the electrons. Only one of the possible doping reactions is necessary, the formation of vacancies will take care of itself. −34 8 −19 6 Appendix that lead to the following equations ηVA′′ ηVOii = η2K S np = N C N V K i (A.26) 1 ηVOii n 2 pO2 2 = ηN C2 K R 1 η2B⋅A n 2 pO2 2 = η2 N C2 a B2O3 K D where η = ηAO, along with the complete electrical neutrality equation, n + 2ηVA′′ = p + 2ηVO + ηBA . •• (A.27) • This gives five unknowns and five equations assuming temperature and oxygen pressure are constant, so the nonlinear equations could be solved simultaneously with perhaps more than a little effort. But of greater interest is to solve the equations for all of the concentrations as a function of oxygen pressure. This generates a Kröger–Vink diagram or the so-called Brouwer diagram, an approximation to the K–V diagram in which logarithm of all the concentrations are assumed to be linear with the oxygen pressure (Kröger 1964) that can be more easily constructed. To do this, it is first assumed that certain defects dominate in different regions of the diagram. Then the oxygen dependencies of all of the defects are calculated from Equations A.26 (Kröger 1964). This diagram for this system is shown in Figure A.5 with four different regions in the diagram and the concentrations determined from the set of equations in Equation A.26: Region 1: reduction, n ≅ 2ηVOii ∝ pO−12 6 so p,ηVA′′ and a B2O3 ∝ pO+12 6 Region 2: donor doping, n ≅ ηBiA = constant so p = constant also, and ηVOii ∝ pO−12 2 from KR and ηVA′′ and a B2O3 ∝ p1O22 Region 3: vacancy compensation,* 2ηVA′′ ≅ ηBiA = constant so ηVOii and a B2O3 are also constant and because n ∝ pO−12 4 and therefore, p ∝ pO+12 4 Region 4: oxidation, p ≅ ηVA′′ ∝ pO+12 6 as well as a B2O3 ∝ pO+12 6 while n and ηVOii ∝ pO−12 6 n = 2ηVO.. n = 2ηBA. 2ηV″A = ηBA. ηB A n ηVO.. log10η 2ηV″A = p . p ηV″A p n ηV″A ηVO.. Reduction Vacancy compensation Oxidation Slopes = ±1/2 Slopes = ±1/4 Slopes = ±1/6 Region 2 Region 3 Region 4 Donor doping aB2O3 Slopes = ±1/6 Region 1 log10 pO2 FIGURE A.5 Brouwer approximation to the Kröger–Vink diagram of a compound AO with a dopant B2O3 that gives the point defect concentrations as a function of oxygen pressure. Note that this represents compounds other than oxides such as GaAs, CdTe, and so on, where the pO2 is replaced by pAs2, pTe2, and so on. * When vacancies balance the charge on the dopant the dopant charge is compensated by the vacancy charge. When the dopant charge is balanced by the hole or electron charge it is called electronic compensation. 327 328 Chapter 9. Atomistics of Diffusion What the diagram shows is that, a given temperature, the point defect concentrations depend on both the oxygen pressure and the dopant concentration. Furthermore, the dopant will act as either an electron donor or produce vacancies depending on the partial pressure of oxygen. It should be noted that it is assumed that the concentration of B2O3 is well below its solubility, so that its activity varies with oxygen pressure. If the activity were to exceed 1.0, B2O3 would precipitate, more with increasing oxygen pressure, while the activity remains constant. As a result, the concentration of the dopant also changes with oxygen pressure. Needless to say, this complication makes the drawing of that diagram much more interesting! Three things are worthy of note. First, the entire range of oxygen pressures necessary to experimentally construct a complete K–V is usually not accessible. For example, low oxygen pressures can be achieved with H2O –H2 mixtures. For example, at 500°C, for H 2O:H 2 ≅ 10 −3 which is easily achievable, the pO2 ≅ 10 −34 bar (Roine 2002), whereas pressures greater that a few bar are hard to achieve. Similarly, CO2:CO gas mixtures can also achieve low oxygen pressures. Experimentally, this means that most data will be obtained toward the left hand, or reducing end of the K–V diagram. For example, for the AB diagram, this may only cover region 2, where B2O3 is acting as a donor dopant. Second, the concentrations of all of the point defect concentrations are rather compressed near the top of the diagram to get all of the other information into the graph. But, for example, if region 2 covered the experimental range of 10 −34 < pO2 < 1 bar then because of pO±12/ 2 pressure dependencies, the vacant oxygen and vacant cation concentrations vary by 1017 over this oxygen pressure range while the electron concentration remains constant! Third, the linear approximation is not valid near the transition from one region to another. In this case, the Equations A.26 and A.27 really do have to be solved simultaneously. EXERCISES 9.1 Would it be appropriate to say that [V] = mole fraction? Why or why not? 9.2 a. The density of silver, Ag, is 10.5 g/cm3 and its atomic weight is 107.87 g/g atom. Calculate the number of Ag lattice sites per cm3. b. Calculate the molar volume (cm3/mol) of Ag. c. The energy to form lattice vacancies in silver is ΔHf = 105 kJ/mol. Calculate the fraction of vacant lattice sites in Ag at its melting point of 961°C. d. Calculate the number of vacant Ag sites per cm3 at its melting point. e. For diffusion of silver in silver (silver “self-diffusion”), Do = 0.67 cm2/s and Q = 189.1 kJ/ mol. Calculate ΔHm (kJ/mol), the enthalpy for motion of Ag atoms in Ag in which the diffusion takes place by a vacancy mechanism. f. Calculate the diffusion coefficient of Ag in Ag at its melting point. 9.3 a. Suppose that sodium and chlorine vacancies attract each other and form nearest neighbor pairs according to the following equation: ( ) ′ + VCli VNa ′ VCli ; ∆G p ≅ ∆H p VNa where ΔGp ≌ ΔHp = −0.2 eV is the pairing energy. Note that it is negative because the vacancies attract each because of the charge difference. Neglecting possible entropy effects because the pairs can orient in different crystal directions, calculate the number of vacancy pairs/cm3 in NaCl at its melting point of 801°C. b. If the energy to form a Schottky defect in NaCl is 2.3 eV, calculate the concentration of paired and unpaired defects at 100°C intervals from 100°C to 800°C. Plot these data as log10[] versus T (°C). 9.4 Silicon replaced germanium, Ge, as the semiconductor material of choice about 50 years ago because it is easier to grow a good stable and insulating oxide, SiO2, on silicon while the oxide on Ge, GeO2, is not nearly as good. However, Ge has better semiconducting properties than silicon and there are some new devices in which the oxide on silicon has to be replaced with some other oxide. Therefore, Ge has the potential of making a “comeback” as a semiconductor material. Exercises a. The density of Ge is 5.35 g/cm3 and its atomic weight is 72.59 g/g atom. Calculate the number of Ge lattice sites per cm3. b. Calculate the molar volume (cm3/mol) of Ge. c. The energy to form lattice vacancies in germanium is ΔHf = 1.73 eV/vacancy. Calculate the fraction of vacant lattice sites in Ge at its melting point of 937°C. d. Calculate the number of vacant Ge sites per cm3 at its melting point. e. For diffusion of germanium in germanium (germanium “self-diffusion”), Do = 18.50 cm2/s and Q = 296.2 kJ/mol. Calculate ΔHm (in both kJ/mol and eV/atom), the enthalpy for motion of Ge atoms in Ge in which the diffusion takes place by a vacancy mechanism. f. Calculate the diffusion coefficient of Ge in Ge at its melting point. 9.5 a. The density of TiO2, rutile (titanium dioxide), is 4.26 g/cm3 and its molecular weight is 79.88 g/mol. Calculate the number of titanium and oxygen sites per cm3 in TiO2. b. Calculate the fraction of vacant oxygen ion sites at the melting point of TiO2, 1850°C, if the energy to form a Schottky defect is 5.2 eV per “molecule” of vacancies. c. Calculate the concentration of oxygen vacancies (cm−3) at the melting point of TiO2. 9.6 Show that the vacancy site fractions for a Schottky defect in MgAl2O4 are equal. 9.7 Show that Equation 9.62 follows from Equation 9.61. 9.8 An oxide compound, AO, undergoes nonstoichiometry at certain oxygen partial pressures by the reaction: 2A A + O O = 1 O2 (g) + VOii + 2A′A ; ∆G R = 4.0 eV 2 Of course, the A′A ion is an A 2+ ion reduced to an A+ ion in Kröger–Vink notation. Also, for a Schottky defect in AO: 0 = VA′′ + VO•• ; ∆GS = 2.1 eV. Because of three possible defects, the total electrical neutrality condition is 2ηVOii = 2ηVA′′ + ηA′A But because ηA = ηO , so 2[ VO•• ] = 2[ VA′′ ] + [A′A ]. This implies that two concentration ranges are possible, the stoichiometric range where [ VO•• ] ≅ [ VA′′ ] and the [A′A ] can be neglected and a nonstoichiometric range where 2[ VO•• ] ≅ [A′A ] and [ VA′′ ] can be neglected. a. Calculate the vacancy concentration in the stoichiometry range where [ VO•• ] ≅ [ VA′′ ] at 1000°C. b. Calculate [A′A ] in the stoichiometric range when pO2 = 10 4 bar at 1000°C. c. From parts (a) and (b), calculate the nonstoichiometry at pO2 = 10 4 bar at 1000°C; i.e. x in AO1−x. d. In the nonstoichiometry range, 2[ VO•• ] ≅ [A′A ], calculate [ VO•• ] and x at p(O2) = 10 –14 bar and 1000°C. e. Calculate all of the vacancy concentrations, x¸ and the oxygen pressure when 2[ VA′′ ] ≅ [A′A ]. 9.9 a. Calculate the RMS speeds (cm/s) of He and Ar gases at 1000°C. M(He) = 4.002 g/mol, M(Ar) = 39.948 g/mol. b. Calculate η (atoms/cm3) at 1000°C and 1 atmosphere pressure. c. Calculate the mean free path, λ (cm), at 1000°C and 1 atmosphere pressure if d(He) = 256 pm and d(Ar) = 348 pm. d. Calculate DHe-Ar (cm2/s) at 1000°C and 1 atmosphere pressure. 9.10 The general form for the gas diffusion coefficient is D = A(1/ M)1/ 2 (T 3/ 2 /d 2 p) where A is a constant, Units(M) = g/mol, Units(T) = K, Units(d) = Å (0.1 nm) and Units(p) = atm. Calculate the value of the “A” and give its units if Units(D) = cm2/s. 9.11 The mean speed of gas atoms is given by 329 330 Chapter 9. Atomistics of Diffusion v= 8RT πM where v is the speed and M is the molecular weight. a. Calculate the mean speed (cm/s) for hydrogen molecules at 1000°C. b. The mean free path, λ, for atoms in a gas is given by λ = 1/( 2 πd 2η) Where d is the molecular diameter, d = 282.7 pm and η is the number of molecules per unit volume. Calculate the number of hydrogen molecules per cm3 at 1-torr pressure and 1000°C. c. Calculate the mean free path (cm) for hydrogen at 1000°C and 1-torr pressure. d. The gas diffusion coefficient is given by D = (1/ 3)vλ. Calculate the gas diffusion coefficient (cm2/s) for hydrogen at 1000°C and p = 1 torr. 9.12 Assuming that Schottky defects are the only lattice defects, construct a K–V (Brouwer) diagram for the point defects (electrons, holes, and vacancies) in a pure compound AO with the following parameters: Eg = 3 eV, ∆G V = 3 eV , ∆G R = 3 eV, density = 5.0 g/cm3, and molecular weight of M = 80 g/mol. Use a range of oxygen pressures so that the diagram will extend from inside the reduction region to inside the oxidation region. Include the numerical values for the concentrations and pressures on the axes. REFERENCES Balluffi, R. W., S. M. Allen, and W. C. Carter. 2005. Kinetics of Materials. New York: John Wiley & Sons. Barrer, R. M. 1941. Diffusion in and Through Solids. New York: MacMillan. Barsoum, M. 1997. Fundamentals of Ceramics. New York: McGraw-Hill. Bird, R. B., W. E. Stewart, and E. N. Lightfoot. 2002. Transport Phenomena, 2nd ed. New York: John Wiley & Sons. Borg, R. J. and G. J. Dienes. 1988. Solid State Diffusion. New York: Academic Press. Brandes, E. A. and G. B. Brook. 1992. Smithells Metals Reference Book, 7th ed. Oxford, UK: ButterworthHeinemann, Ltd. Callister, W. D., Jr. and D. G. Rethwisch. 2009. Fundamentals of Materials Science and Engineering, 3rd ed. New York: John Wiley & Sons. Catlow, C. R. A. and W. C. Mackrodt. 1982. Computer Simulation of Solids. Berlin, Germany: Springer-Verlag. Chiang, Y.-M. C., D. Birnie, III, and W. D. Kingery. 1997. Physical Ceramics. New York: John Wiley & Sons. Connelly, N. G., T. Damhus, R. Hartshorn, and A. Hutton. 2005. IR-11.4 Point Defect (Kröger-Vink) Notation. Nomenclature of Inorganic Chemistry. Redbook of the International Union of Pure and Applied Chemistry. Cambridge: The Royal Society of Chemistry, 239–241. Cussler, E. L. 1997. Diffusion, 2nd ed. Cambridge, UK: Cambridge University Press. Darken, L. S. and R. W. Gurry. 1953. Physical Chemistry of Metals. New York: McGraw-Hill Book Company. Elmore, W. C. and M. A. Heald. 1985. Physics of Waves. New York: Dover Publications, Inc. Emsley, J. 1998. The Elements, 3rd ed. Oxford, UK: Oxford University Press. Emsley, J. 2001. Nature’s Building Blocks. Oxford, UK: Oxford University Press. Fisher, D. J., ed. 2011. Defects and Diffusion in Ceramics XII. Zurich, Switzerland: Trans Tech Publications. French, A. P. 1971. Vibrations and Waves. New York: W. W. Norton & Co. Geankoplis, C. J. 1972. Mass Transport Phenomena. Columbus, OH: Christie J. Geankoplis. Glicksman, M. E. 2000. Diffusion in Solids. New York: John Wiley & Sons. Gray, D. E., editor-in-chief. 1972. American Institute of Physics Handbook, 3rd ed. New York: McGraw-Hill. Hayes, W. and A. M. Stoneham. 1985. Defects and Defect Processes in Nonmetallic Solids. New York: John Wiley & Sons. Haynes, W. M., editor-in-chief. 2013. Handbook of Chemistry and Physics, 94th ed. Boca Raton, FL: CRC Press. Henderson, B. 1972. Crystalline Solids. New York: Crane, Russak & Co. Hoddeson, L., E. Braun, J. Teichmann, and S. Weart. 1992. Out of the Crystal Maze. New York: Oxford. Kesting, R. E. and A. K. Fritzsche. 1993. Polymeric Gas Separation Membranes. New York: John Wiley & Sons. Kingery, W. D., H. K. Bowen, and D. R. Uhlmann. 1976. Introduction to Ceramics, 2nd ed. New York: John Wiley & Sons. Kreyszig, E. 1988. Advanced Engineering Mathematics, 6th ed. New York: Wiley. Kröger, F. A. 1964. The Chemistry of Imperfect Crystals. Amsterdam, the Netherlands: North Holland Publishing Co. Kröger, F. A. and V. J. Vink. 1956. Relations between the concentrations of imperfections in crystalline solids. In Solid State Physics, Vol. 3. F. Seitz and D. Turnbull, eds. New York: Academic Press, 307–435. Lindley, D. 2001. Boltzmann’s Atom. New York: The Free Press. Maier, J. 2004. Physical Chemistry of Ionic Materials. Chichester, YK: John Wiley & Sons, Ltd. References Main, I. G. 1984. Vibrations and Waves in Physics, 2nd ed. Cambridge, UK: Cambridge University Press. Mark, J. E., ed. 2007. Physical Properties of Polymers Handbook, 2nd ed. New York: Springer Science and Business Media, LLC. Mayer, J. W. and S. S. Lau. 1990. Electronic Materials Science. New York: MacMillan. Mott, N. F. and R. W. Gurney. 1948. Electronic Processes in Ionic Solids. New York: Dover. Mulder, M. 1996. Basic Principles of Membrane Technology, 2nd ed. Dordrecht, the Netherlands: Kluwer Academic Publishers. Pain, H. J. 1999. The Physics of Waves and Vibrations, 5th ed. Chichester, UK: John Wiley & Sons, Ltd. Pearson, J. M. 1966. A Theory of Waves. Boston, MA: Allyn & Bacon, Inc. Quinn, S. 1995. Marie Curie. New York: Simon & Schuster. Readey, D. W. 1966a. Mass transport and sintering in impure ionic solids. Journal of the American Ceramic Society. 49(7): 366–369. Readey, D. W. 1966b. Chemical potentials and initial sintering in pure metals and ionic compounds. Journal of Applied Physics. 37: 2309–2312. Reed-Hill, R. E. and R. Abaaschian. 1992. Physical Metallurgy Principles, 3rd ed. Boston, MA: PWS Kent. Robinson, R. A. and R. H. Stokes. 2002. Electrolyte Solutions, 2nd ed. Mineola, NY: Dover. Roine, A. 2002. Outokumpu HSC Chemistry for Windows, Chemical Reaction and Equilibrium Software with Extensive Thermochemical Database, Version 5.1. Pori, Finland: Outokumpu Research Oy. Shewmon, P. 1989. Diffusion in Solids, 2nd ed. Warrendale, PA: The Minerals, Metals, and Materials Society. Shulman, J. H. and W. D. Compton. 1962. Color Centers in Solids. Oxford, UK: Pergamon Press. Silbey, R. J. and R. A. Alberty. 2001. Physical Chemistry, 3rd ed. New York: John Wiley & Sons. Smyth, D. M. 2000. The Defect Chemistry of Oxides. Oxford, UK: Oxford University Press. Sperling, L. H. 2006. Introduction to Polymer Physical Chemistry, 4th ed. New York: John Wiley & Sons. Stull, D. R. and H. Prophet. 1971. JANAF Thermochemical Tables, 2nd ed. NSRDS-NBS 37. Washington, DC: U.S. Government Printing Office. Tilley, R. J. D. 1987. Defect Crystal Chemistry. New York: Chapman & Hall. Van Krevelen, D. W. 1997. Properties of Polymers, 3rd ed. Amsterdam, the Netherlands: Elsevier B. V. Wells, A. F. 1984. Structural Inorganic Chemistry, 5th ed. Oxford, UK: Oxford University Press. 331